COMPOSITE MATERIALS DESIGN AND APPLICATIONS
© 2003 by CRC Press LLC
COMPOSITE MATERIALS DESIGN AND APPLICATIONS
Dani...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

COMPOSITE MATERIALS DESIGN AND APPLICATIONS

© 2003 by CRC Press LLC

COMPOSITE MATERIALS DESIGN AND APPLICATIONS

Daniel Gay Suong V. Hoa Stephen W. Tsai

CRC PR E S S Boca Raton London New York Washington, D.C.

© 2003 by CRC Press LLC

TX846 disclaimer Page iv Friday, November 8, 2002 8:38 AM

Library of Congress Cataloging-in-Publication Data Gay, Daniel, 1942[Matériaux composites. English] Composite materials / by Daniel Gay ; translated by Suong V. Hoa, Stephen W. Tsai. p. cm. Translation of: Matériaux composites. 4th ed. Includes bibliographical references and index. ISBN 1-58716-084-6 (alk. paper) 1. Composite materials. I. Title. TA418.9.C6 G39 2002 620.1′18—dc21

2002073794 CIP

This book contains information obtained from authentic and highly regarded sources. Reprinted material is quoted with permission, and sources are indicated. A wide variety of references are listed. Reasonable efforts have been made to publish reliable data and information, but the author and the publisher cannot assume responsibility for the validity of all materials or for the consequences of their use. Neither this book nor any part may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopying, microÞlming, and recording, or by any information storage or retrieval system, without prior permission in writing from the publisher. The consent of CRC Press LLC does not extend to copying for general distribution, for promotion, for creating new works, or for resale. SpeciÞc permission must be obtained in writing from CRC Press LLC for such copying. Direct all inquiries to CRC Press LLC, 2000 N.W. Corporate Blvd., Boca Raton, Florida 33431. Trademark Notice: Product or corporate names may be trademarks or registered trademarks, and are used only for identiÞcation and explanation, without intent to infringe.

Visit the CRC Press Web site at www.crcpress.com © 2003 by CRC Press LLC French editions published by Editions Hermès, Paris, 1997 No claim to original U.S. Government works International Standard Book Number 1-58716-084-6 Library of Congress Card Number 2002073794 Printed in the United States of America 1 2 3 4 5 6 7 8 9 0 Printed on acid-free paper

© 2003 by CRC Press LLC

TX846_Frame_FM Page v Thursday, July 11, 2002 5:38 PM

PREFACE The economic importance of composite materials is now well known. There are strong indications everywhere that this importance will be increasing in the future. Composite materials now occupy an established position in the aerospace industry. They are also used for many components in the automotive industry and civil infrastructures now have their reinforcements made of composite materials. There is a large range of manufacturing processes for the production of low-cost composites. There is a need by engineers working in composites for a practical source of reference for the design and application of composites. This book fills that need. In the educational sector, composite materials now are taught at many universities around the world. Usually the topic covered is laminate theory. Composites Design courses also exist in a few universities and institutes. The demand from students and also practitioners of composites for knowledge and training in design of composites is increasing. However a good design book has not been available. The content of these design courses concentrates mostly on analysis while applications still remain at the specimen level. This book, initially written by Daniel Gay in French, has been distributed widely in France and in French speaking countries. The authors are of the opinion that having the book in the English language would facilitate the training and dissemination of knowledge to the regions where composites are used the most. The book has been translated to English with modifications and updates. The book consists of four main parts, with increasing levels of complexity. Each part can be studied independently from the other parts. The first part presents an introduction to composite materials, the fabrication processes, the properties of a single ply, sandwich materials, conceptual design, assembly, and applications of composites in the aerospace and other areas. This part can be used by itself to form a part of a course on advanced materials and associated designs. The second part presents the mechanics of composite materials. This consists of discussion on elastic anisotropic properties, the directional dependence of different properties, and mechanical properties of thin laminates. This part can be used by itself to teach students and engineers on the mechanics of composite materials. The third part presents the orthotropic coefficients that may be conveniently used for design. The Hill–Tsai failure criterion, bending of composite beams, torsion of composite beams, and bending of thick composite plates. This part requires knowledge of strength of materials. Information presented here is more theoretical than in preceding parts. Its main objective is to contribute to a better interpretation of the behavior of composite components.

© 2003 by CRC Press LLC

TX846_Frame_FM Page vi Thursday, July 11, 2002 5:38 PM

The fourth part provides numerous (41) numerical examples on the use and design of composites. There are three levels of examples. Level 1 deals with the determination of mechanical properties of composite structures in different forms such as plates, tubes, or composite components made using different processes such as hand-lay-up or filament winding. Level 2 deals with thermoelastic properties of different laminates. Failure analysis is also carried out. Level 3 deals with bonding of cylinders made of composites, buckling of composite sandwich beams, flexural shear in sandwich beams, vibrations of composite This volume can be used to teach students at the first year graduate level as well as the final year undergraduate level. It is also useful for practical engineers who want to learn, on the job, the guidelines for the use of composites in their applications. The authors hope that this volume can make significant contribution to the training of future engineers who utilize composites. Suong V. Hoa Montreal, Quebec, Canada Daniel Gay Toulouse, France Stephen Tsai Stanford, California July 2002

© 2003 by CRC Press LLC

TX846_Frame_FM Page vii Thursday, July 11, 2002 5:38 PM

CONTENTS PART I: PRINCIPLES OF CONSTRUCTION 1

Composite Materials, Interest, and Properties 1.1 What Is Composite Material? 1.2 Fibers and Matrix 1.2.1 Fibers 1.2.2 Matrix Materials 1.3 What Can Be Made Using Composite Materials? 1.4 Typical Examples of Interest on the Use of Composite Materials 1.5 Examples on Replacing Conventional Solutions with Composites 1.6 Principal Physical Properties

2

Fabrication Processes 2.1 Molding Processes 2.1.1 Contact Molding 2.1.2 Compression Molding 2.1.3 Molding with Vacuum 2.1.4 Resin Injection Molding 2.1.5 Molding by Injection of Premixed 2.1.6 Molding by Foam Injection 2.1.7 Molding of Components of Revolution 2.2 Other Forming Processes 2.2.1 Sheet Forming 2.2.2 Profile Forming 2.2.3 Stamp Forming 2.2.4 Preforming by Three-Dimensional Assembly 2.2.5 Cutting of Fabric and Trimming of Laminates 2.3 Practical Hints on Manufacturing Processes 2.3.1 Acronyms 2.3.2 Cost Comparison

3

Ply Properties 3.1 Isotropy and Anisotropy 3.1.1 Isotropic Materials 3.1.2 Anisotropic Material 3.2 Characteristics of the Reinforcement–Matrix Mixture 3.2.1 Fiber Mass Fraction 3.2.2 Fiber Volume Fraction 3.2.3 Mass Density of a Ply 3.2.4 Ply Thickness

© 2003 by CRC Press LLC

TX846_Frame_FM Page viii Thursday, July 11, 2002 5:38 PM

3.3 Unidirectional Ply 3.3.1 Elastic Modulus 3.3.2 Ultimate Strength of a Ply 3.3.3 Examples 3.3.4 Examples of “High Performance” Unidirectional Plies 3.4 Woven Fabrics 3.4.1 Forms of Woven Fabric 3.4.2 Elastic Modulus of Fabric Layer 3.4.3 Examples of Balanced Fabrics/Epoxy 3.5 Mats and Reinforced Matrices 3.5.1 Mats 3.5.2 Summary Example of Glass/Epoxy Layers 3.5.3 Spherical Fillers 3.5.4 Other Reinforcements 3.6 Multidimensional Fabrics 3.7 Metal Matrix Composites 3.8 Tests

4

Sandwich Structures 4.1 What Is a Sandwich Structure? 4.2 Simplified Flexure 4.2.1 Stresses 4.2.2 Displacements 4.3 A Few Special Aspects 4.3.1 Comparison of Mass Based on Equivalent Flexural Rigidity (EI) 4.3.2 Buckling of Sandwich Structures 4.3.3 Other Types of Damage 4.4 Fabrication and Design Problems 4.4.1 Honeycomb: An Example of Core Material 4.4.2 Processing Aspects 4.4.3 Insertion of Attachment Pieces 4.4.4 Repair of Laminated Facings 4.5 Nondestructive Quality Control

5

Conception and Design 5.1 Design of a Composite Piece 5.1.1 Guidelines for Values for Predesign 5.2 The Laminate 5.2.1 Unidirectional Layers and Fabrics 5.2.2 Importance of Ply Orientation 5.2.3 Code to Represent a Laminate 5.2.4 Arrangement of Plies 5.3 Failure of Laminates 5.3.1 Damages 5.3.2 Most Frequently Used Criterion: Hill–Tsai Failure Criterion 5.4 Sizing of the Laminate 5.4.1 Modulus of Elasticity. Deformation of a Laminate 5.4.2 Case of Simple Loading 5.4.3 Case of Complex Loading—Approximate Orientation Distribution of a Laminate 5.4.4 Case of Complex Loading: Optimum Composition of a Laminate 5.4.5 Practical Remarks: Particularities of the Behavior of Laminates

© 2003 by CRC Press LLC

TX846_Frame_FM Page ix Thursday, July 11, 2002 5:38 PM

6

Joining and Assembly 6.1 Riveting and Bolting 6.1.1 Principal Modes of Failure in Bolted Joints for Composite Materials 6.1.2 Recommended Values 6.1.3 Riveting 6.1.4 Bolting 6.2 Bonding 6.2.1 Adhesives Used 6.2.2 Geometry of the Bonded Joints 6.2.3 Sizing of Bonded Surfaces 6.2.4 Examples of Bonding 6.3 Inserts

7

Composite Materials and Aerospace Construction 7.1 Aircraft 7.1.1 Composite Components in Aircraft 7.1.2 Characteristics of Composites 7.1.3 A Few Remarks 7.1.4 Specific Aspects of Structural Resistance 7.1.5 Large Carriers 7.1.6 Regional Jets 7.1.7 Light Aircraft 7.1.8 Fighter Aircraft 7.1.9 Architecture of Composite Parts in Aircraft 7.1.10 Elements of Braking 7.1.11 The Future 7.2 Helicopters 7.2.1 The Situation 7.2.2 Composite Zones 7.2.3 Blades 7.2.4 Yoke Rotor 7.2.5 Other Composite Working Components 7.3 Propeller Blades for Airplanes 7.4 Turbine Blades in Composites 7.5 Space Applications 7.5.1 Satellites 7.5.2 Pressure Vessels 7.5.3 Nozzles 7.5.4 Other Composite Components

8

Composite Materials for Other Applications 8.1 Composite Materials and the Manufacturing of Automobiles 8.1.1 Introduction 8.1.2 Evaluation and Evolution 8.1.3 Research and Development 8.2 Composites in Naval Construction 8.2.1 Competition 8.2.2 Ships 8.3 Sports and Recreation 8.3.1 Skis 8.3.2 Bicycles

© 2003 by CRC Press LLC

TX846_Frame_FM Page x Thursday, July 11, 2002 5:38 PM

8.4 Other 8.4.1 8.4.2 8.4.3 8.4.4 8.4.5 8.4.6

Applications Wind Turbines Compressed Gas Bottles Buggy Chassis Tubes for Off-Shore Installations Biomechanics Applications Telepherique Cabin

PART II: MECHANICAL BEHAVIOR OF LAMINATED MATERIALS 9

Anisotropic Elastic Media 9.1 Review of Notations 9.1.1 Continuum Mechanics 9.1.2 Number of Distinct ϕijk Terms 9.2 Orthotropic Materials 9.3 Transversely Isotropic Materials

10

Elastic Constants of Unidirectional Composites 10.1 10.2 10.3 10.4 10.5

11

Longitudinal Modulus E Poisson Coefficient Transverse Modulus Et Shear Modulus Gt Thermoelastic Properties 10.5.1 Isotropic Material: Recall 10.5.2 Case of Unidirectional Composite 10.5.3 Thermomechanical Behavior of a Unidirectional Layer

Elastic Constants of a Ply Along an Arbitrary Direction 11.1 Compliance Coefficients 11.2 Stiffness Coefficients 11.3 Case of Thermomechanical Loading 11.3.1 Compliance Coefficients 11.3.2 Stiffness Coefficients

12

Mechanical Behavior of Thin Laminated Plates 12.1 Laminate with Midplane Symmetry 12.1.1 Membrane Behavior 12.1.2 Apparent Moduli of the Laminate 12.1.3 Consequence: Practical Determination of a Laminate Subject to Membrane Loading 12.1.4 Flexure Behavior 12.1.5 Consequence: Practical Determination for a Laminate Subject to Flexure 12.1.6 Simplified Calculation for Flexure 12.1.7 Case of Thermomechanical Loading 12.2 Laminate without Midplane Symmetry 12.2.1 Coupled Membrane–Flexure Behavior 12.2.2 Case of Thermomechanical Loading

PART III: JUSTIFICATIONS, COMPOSITE BEAMS, AND THICK PLATES 13

Elastic Coefficients 13.1 Elastic Coefficients in an Orthotropic Material 13.2 Elastic Coefficients for a Transversely Isotropic Material 13.2.1 Rotation about an Orthotropic Transverse Axis 13.3 Case of a Ply

© 2003 by CRC Press LLC

TX846_Frame_FM Page xi Thursday, July 11, 2002 5:38 PM

14

The Hill–Tsai Failure Criterion 14.1 Isotropic Material: Von Mises Criterion 14.2 Orthotropic Material: Hill–Tsai Criterion 14.2.1 Preliminary Remarks 14.2.2 Case of a Transversely Isotropic Material 14.2.3 Case of a Unidirectional Ply Under In-Plane Loading 14.3 Variation of Resistance of a Unidirectional Ply with Respect to the Direction of Loading 14.3.1 Tension and Compression Resistance 14.3.2 Shear Strength

15

Composite Beams in Flexure 15.1 Flexure of Symmetric Beams with Isotropic Phases 15.1.1 Degrees of Freedom 15.1.2 Perfect Bonding between the Phases 15.1.3 Equilibrium Relations 15.1.4 Constitutive Relations 15.1.5 Technical Formulation 15.1.6 Energy Interpretation 15.1.7 Extension to the Dynamic Case 15.2 Case of Any Cross Section (Asymmetric)

16

Composite Beams in Torsion 16.1 Uniform Torsion 16.1.1 Torsional Degree of Freedom 16.1.2 Constitutive Relation 16.1.3 Determination of the Function Φ( y, z) 16.1.4 Energy Interpretation 16.2 Location of the Torsion Center

17

Flexure of Thick Composite Plates 17.1 Preliminary Remarks 17.1.1 Transverse Normal Stress σz 17.1.2 Transverse Shear Stresses τxz and τyz 17.1.3 Hypotheses 17.2 Displacement Field 17.3 Strains 17.4 Constitutive Relations 17.4.1 Membrane Equations 17.4.2 Bending Behavior 17.4.3 Transverse Shear Equation 17.5 Equilibrium Equations 17.5.1 Transverse Equilibrium 17.5.2 Equilibrium in Bending 17.6 Technical Formulation for Bending 17.6.1 Plane Stresses Due to Bending 17.6.2 Transverse Shear Stresses in Bending 17.6.3 Characterization of the Bending, Warping Increments ηx and ηy 17.6.4 Warping Functions 17.6.5 Consequences 17.6.6 Interpretation in Terms of Energy 17.7 Examples 17.7.1 Homogeneous Orthotropic Plate 17.7.2 Sandwich Plate

© 2003 by CRC Press LLC

TX846_Frame_FM Page xii Thursday, July 11, 2002 5:38 PM

PART IV: APPLICATIONS 18

Applications 18.1 Level 1 18.1.1 18.1.2 18.1.3 18.1.4 18.1.5 18.1.6 18.1.7 18.1.8 18.1.9 18.1.10 18.1.11 18.1.12 18.1.13 18.1.14 18.1.15 18.2 Level 2 18.2.1 18.2.2 18.2.3 18.2.4 18.2.5 18.2.6 18.2.7 18.2.8 18.2.9 18.2.10 18.2.11 18.2.12 18.2.13 18.2.14 18.2.15 18.2.16 18.2.17 18.3 Level 3 18.3.1 18.3.2 18.3.3 18.3.4 18.3.5 18.3.6 18.3.7 18.3.8 18.3.9

© 2003 by CRC Press LLC

Simply Supported Sandwich Beam Poisson Coefficient of a Unidirectional Layer Helicopter Blade Transmission Shaft for Trucks Flywheel in Carbon/Epoxy Wing Tip Made of Carbon/Epoxy Carbon Fiber Coated with Nickel Tube Made of Glass/Epoxy under Pressure Filament Wound Vessel, Winding Angle Filament Wound Reservoir, Taking the Heads into Account Determination of the Volume Fraction of Fibers by Pyrolysis Lever Arm Made of Carbon/PEEK Unidirectional and Short Fibers Telegraphic Mast in Glass/Resin Unidirectional Ply of HR Carbon Manipulator Arm of Space Shuttle Sandwich Beam: Simplified Calculation of the Shear Coefficient Procedure for Calculation of a Laminate Kevlar/Epoxy Laminates: Evolution of Stiffness Depending on the Direction of the Load Residual Thermal Stresses due to Curing of the Laminate Thermoelastic Behavior of a Tube Made of Filament-Wound Glass/Polyester Polymeric Tube Loaded by Thermal Load and Creep First Ply Fracture of a Laminate—Ultimate Rupture Optimum Laminate for Isotropic Stress State Laminate Made of Identical Layers of Balanced Fabric Wing Spar in Carbon/Epoxy Determination of the Elastic Characteristics of a Carbon/Epoxy Unidirectional Layer from Tensile Test Sailboat Shell in Glass/Polyester Determination of the In-Plane Shear Modulus of a Balanced Fabric Ply Quasi-Isotropic Laminate Orthotropic Plate in Pure Torsion Plate Made by Resin Transfer Molding (R.T.M.) Thermoelastic Behavior of a Balanced Fabric Ply Cylindrical Bonding Double Bonded Joint Composite Beam with Two Layers Buckling of a Sandwich Beam Shear Due to Bending in a Sandwich Beam Column Made of Stretched Polymer Cylindrical Bending of a Thick Orthotropic Plate under Uniform Loading Bending of a Sandwich Plate Bending Vibration of a Sandwich Beam

TX846_Frame_FM Page xiii Thursday, July 11, 2002 5:38 PM

APPENDICES, BIBLIOGRAPHY, AND INDEX Appendix 1 Stresses in the Plies of a Laminate of Carbon/Epoxy Loaded in Its Plane Characteristics of Each Ply

Appendix 2 Buckling of Orthotropic Structures Rectangular Panels Buckling of Orthotropic Tubes

Bibliography

© 2003 by CRC Press LLC

TX846_Frame_C01 Page 1 Monday, November 18, 2002 10:34 AM

PART I PRINCIPLES OF CONSTRUCTION

© 2003 by CRC Press LLC

TX846_Frame_C01 Page 3 Monday, November 18, 2002 10:34 AM

1 COMPOSITE MATERIALS, INTEREST, AND PROPERTIES 1.1 WHAT IS COMPOSITE MATERIAL? As the term indicates, composite material reveals a material that is different from common heterogeneous materials. Currently composite materials refers to materials having strong fibers—continuous or noncontinuous—surrounded by a weaker matrix material. The matrix serves to distribute the fibers and also to transmit the load to the fibers. Notes: Composite materials are not new. They have been used since antiquity. Wood and cob have been everyday composites. Composites have also been used to optimize the performance of some conventional weapons. For example: In the Mongolian arcs, the compressed parts are made of corn, and the stretched parts are made of wood and cow tendons glued together. Japanese swords or sabers have their blades made of steel and soft iron: the steel part is stratified like a sheet of paste, with orientation of defects 1 and impurities in the long direction (see Figure 1.1), then formed into a U shape into which the soft iron is placed. The sword then has good resistance for flexure and impact. One can see in this period the beginning of the distinction between the common composites used universally and the high performance composites. The composite material as obtained is Very heterogeneous. Very “anisotropic.” This notion of “anisotropy” will be illustrated later in Section 3.1 and also in Chapter 9. Simply put this means that the mechanical properties of the material depend on the direction.

1

15

In folding a sheet of steel over itself 15 times, one obtains 2

© 2003 by CRC Press LLC

= 32,768 layers.

TX846_Frame_C01 Page 4 Monday, November 18, 2002 10:34 AM

Figure 1.1 Effect of the Orientation of Impurities

1.2 FIBERS AND MATRIX The bonding between fibers and matrix is created during the manufacturing phase of the composite material. This has fundamental influence on the mechanical properties of the composite material.

1.2.1 Fibers Fibers consist of thousands of filaments, each filament having a diameter of between 5 and 15 micrometers, allowing them to be producible using textile 2 machines; for example, in the case of glass fiber, one can obtain two semiproducts as shown in Figure 1.2. These fibers are sold in the following forms: Short fibers, with lengths of a few centimeters or fractions of millimeters are felts, mats, and short fibers used in injection molding. Long fibers, which are cut during time of fabrication of the composite material, are used as is or woven. Principal fiber materials are

Glass Aramid or Kevlar‚ (very light) Carbon (high modulus or high strength) Boron (high modulus or high strength) Silicon carbide (high temperature resistant)

In forming fiber reinforcement, the assembly of fibers to make fiber forms for the fabrication of composite material can take the following forms:

2

One wants to have fibers as thin as possible because their rupture strength decreases as their diameter increases, and very small fiber diameters allow for effective radius of curvature in fiber bending to be on the order of half a millimeter. However, exception is made for boron fibers (diameter in the order of 100 microns), which are formed around a tungsten filament (diameter = 12 microns). Their minimum radius of curvature is 4 mm. Then, except for particular cases, weaving is not possible.

© 2003 by CRC Press LLC

TX846_Frame_C01 Page 5 Monday, November 18, 2002 10:34 AM

Figure 1.2 Different Fiber Forms

Unidimensional: unidirectional tows, yarns, or tapes Bidimensional: woven or nonwoven fabrics (felts or mats) Tridimensional: fabrics (sometimes called multidimensional fabrics) with fibers oriented along many directions (>2) Before the formation of the reinforcements, the fibers are subjected to a surface treatment to Decrease the abrasion action of fibers when passing through the forming machines. Improve the adhesion with the matrix material. Other types of reinforcements, full or empty spheres (microspheres) or powders (see Section 3.5.3), are also used.

1.2.1.1 Relative Importance of Different Fibers in Applications Figure 1.3 allows one to judge the relative importance in terms of the amount of fibers used in the fabrication of composites. One can immediately notice the industrial importance of fiber glass (produced in large quantities). Carbon and Kevlar fibers are reserved for high performance components. Following are a few notes on the fibers: Glass fiber: The filaments are obtained by pulling the glass (silicon + sodium carbonate and calcium carbonate; T > 1000∞C) through the small orifices of a plate made of platinum alloy. Kevlar fiber: This is an aramid fiber, yellowish color, made by DuPont de Nemours (USA). These are aromatic polyamides obtained by synthesis at -10∞C, then fibrillated and drawn to obtain high modulus of elasticity. Carbon fiber: Filaments of polyacrylonitrile or pitch (obtained from residues of the petroleum products) are oxidized at high temperatures (300∞C), then heated further to 1500∞C in a nitrogen atmosphere. Then only the hexagonal © 2003 by CRC Press LLC

TX846_Frame_C01 Page 6 Monday, November 18, 2002 10:34 AM

Figure 1.3 Relative Sale Volume of Different Fibers

Figure 1.4 Structure of Carbon Fiber

carbon chains, as shown in Figure 1.4, remain. Black and bright filaments are obtained. High modulus of elasticity is obtained by drawing at high temperature. Boron fiber: Tungsten filament (diameter 12 mm) serves to catalyze the reaction between boron chloride and hydrogen at 1200∞C. The boron fibers obtained have a diameter of about 100 mm (the growth speed is about 1 micron per second). Silicon carbide: The principle of fabrication is analogous to that of boron fiber: chemical vapor deposition (1200∞C) of methyl trichlorosilane mixed with hydrogen. The principal physical–mechanical properties of the fibers are indicated in Table 1.3. Note the very significant disparity of the prices per unit weight. © 2003 by CRC Press LLC

TX846_Frame_C01 Page 7 Monday, November 18, 2002 10:34 AM

1.2.2 Matrix Materials The matrix materials include the following: Polymeric matrix: thermoplastic resins (polypropylene, polyphenylene sulfone, polyamide, polyetheretherketone, etc.) and thermoset resins (polyesters, phenolics, melamines, silicones, polyurethanes, epoxies). Their principal physical properties are indicated in the Table 1.4. Mineral matrix: silicon carbide, carbon. They can be used at high temperatures (see Sections 2.2.4, 3.6, 7.1.10, 7.5). Metallic matrix: aluminum alloys, titanium alloys, oriented eutectics.

1.3 WHAT CAN BE MADE USING COMPOSITE MATERIALS? The range of applications is very large. A few examples are shown below. Electrical, Electronics Insulation for electrical construction Supports for circuit breakers Supports for printed circuits Armors, boxes, covers Antennas, radomes Tops of television towers Cable tracks Windmills Buildings and Public Works Housing cells Chimneys Concrete molds Various covers (domes, windows, etc.) Swimming pools Facade panels Profiles Partitions, doors, furniture, bathrooms Road Transports Body components Complete body Wheels, shields, radiator grills, Transmission shafts Suspension springs Bottles for compressed petroleum gas Chassis Suspension arms Casings Cabins, seats Highway tankers, isothermal trucks Trailers © 2003 by CRC Press LLC

TX846_Frame_C01 Page 8 Monday, November 18, 2002 10:34 AM

Rail transports: Fronts of power units Wagons Doors, seats, interior panels Ventilation housings Marine Transports: Hovercrafts Rescue crafts Patrol boats Trawlers Landing gears Anti-mine ships Racing boats Pleasure boats Canoes Cable transports: Telepherique cabins Telecabins Air transports All composite passenger aircrafts All composite gliders Many aircraft components: radomes, leading edges, ailerons, vertical stabilizers Helicopter blades, propellers Transmission shafts Aircraft brake discs Space Transports Rocket boosters Reservoirs Nozzles Shields for atmosphere reentrance General mechanical applications Gears Bearings Housings, casings Jack body Robot arms Fly wheels Weaving machine rods Pipes Components of drawing table Compressed gas bottles Tubes for offshore platforms Pneumatics for radial frames Sports and Recreation Tennis and squash rackets Fishing poles Skis © 2003 by CRC Press LLC

TX846_Frame_C01 Page 9 Monday, November 18, 2002 10:34 AM

Poles used in jumping Sails Surf boards, Roller skates Bows and arrows Javelins Protection helmets Bicycle frames Golf clubs Oars

1.4 TYPICAL EXAMPLES OF INTEREST ON THE USE OF COMPOSITE MATERIALS In the domain of commercial aircraft, one can compare the concerns of manufacturers with the principal characteristic properties of composite materials. The concerns of the manufacturers are performance and economy. The characteristics of composite components include the following: Weight saving leads to fuel saving, increase in payload, or increase in range which improves performances. Good fatigue resistance leads to enhanced life which involves saving in the long-term cost of the product. Good corrosion resistance means fewer requirements for inspection which results in saving on maintenance cost. Moreover, taking into account the cost of the composite solution as compared with the conventional solution, one can state that composites fit the demand of aircraft manufacturers.

1.5 EXAMPLES ON REPLACING CONVENTIONAL SOLUTIONS WITH COMPOSITES Table 1.1 shows a few significant cases illustrating the improvement on price and performance that can be obtained after replacement of a conventional solution with a composite solution.

1.6 PRINCIPAL PHYSICAL PROPERTIES Tables 1.2 through 1.5 take into account the properties of only individual components, reinforcements, or matrices. The characteristics of composite materials resulting from the combination of reinforcement and matrix depend on The proportions of reinforcements and matrix (see Section 3.2) The form of the reinforcement (see Section 3.2) The fabrication process © 2003 by CRC Press LLC

TX846_Frame_C01 Page 10 Monday, November 18, 2002 10:34 AM

Table 1.1 Properties of Commonly Used Resins Application 3

65 m reservoir for chemicals Smoke stack for chemical plant Nitric acid vapor washer Helicopter stabilizer Helicopter winch support Helicopter motor hub X–Y table for fabrication of integrated circuits Drum for drawing table Head of welding robot Weaving machine rod Aircraft floor

Price of Previous Construction

Stainless steel + installation: 1. Steel: 1. Stainless steel: 1. Light alloys + steel (16 kg): 1. Welded steel (16 kg): 1. (Mass: 1): 1. Cast aluminum: Rate of fabrication: 30 plates/hr Speed of drawing: 15 to 30 cm/sec Aluminum: Mass = 6 kg Aluminum: Rate = 250 shots/minute (Mass = 1): 1.

Price of Composite Construction

0.53 0.51 0.33 Carbon/epoxy (9 kg): 0.45 Carbon/epoxy (11 kg): 1.2 Carbon/Kevlar/epoxy (mass: 0.8): 0.4 Carbon/epoxy honeycomb sandwich: 55 plates/hr Kevlar/epoxy: 40 to 80 cm/sec Carbon/epoxy: Mass = 3 kg Carbon/epoxy: Rate = 350 shots/minute Carbon/Kevlar/epoxy (mass: 0.8): 1.7

These characteristics may be observed in Figure 1.5, which shows the tensile strength for different fiber fractions and different forms of reinforcement for the case of glass/resin composite, and Figure 1.6, which gives an interesting view on the specific resistance of the principal composites as a function of temperature. (The specific strength is defined as the strength divided by the density srupt/r.) Other remarkable properties of these materials include the following: Composite materials do not yield (their elastic limits correspond to the rupture limit; see Section 5.4.5). Composite materials are very fatigue resistant (see Section 5.1). Composite materials age subject to humidity (epoxy resin can absorb water by diffusion up to 6% of its mass; the composite of reinforcement/resin can absorb up to 2%) and heat. Composite materials do not corrode, except in the case of contact “aluminum with carbon fibers” in which case galvanic phenomenon creates rapid corrosion. Composite materials are not sensitive to the common chemicals used in engines: grease, oils, hydraulic liquids, paints and solvents, petroleum. However, paint thinners attack the epoxy resins. Composite materials have medium to low level impact resistance (inferior to that of metallic materials). Composite materials have excellent fire resistance as compared with the light alloys with identical thicknesses. However, the smokes emitted from the combustion of certain matrices can be toxic. © 2003 by CRC Press LLC

Density r 3 (kg/m )

Elastic Modulus E (MPa)

Shear Modulus G (MPa)

Poisson Ratio n

Steels

7800

205,000

79,000

0.3

Aluminum Alloy 2024 Titanium Alloy TA 6V Copper

2800

75,000

29,000

4400

105,000

8800

125,000

Nickel

8900

220,000

Beryllium

1840

294,000

Silicon

2200

95,000

Metals and Alloys

Tensile Strength sult (Mpa)

Elongation (%)

Coefficient of Thermal Expansion at -1 20∞C a (∞C ) -5

1.8 to 10

1.3 ¥ 10

0.3

400 to 1600 450

10

2.2 ¥ 10

40,300

0.3

1200

14

0.8 ¥ 10

48,000

0.3

200 to 500 500 to 850 200

0.05

-5

-5

-5

1.7 ¥ 10

-5

1.2 ¥ 10 5

Coefficient of Thermal Conductivity at 20∞C l(W/m∞C)

Heat Capacity c(J/kg˚C)

20 to 100

400 to 800

800

140

1000

350

17

540

700

380

390

650

70

500

900

150 (20˚C) 90 (800˚C) 1.4 (20˚C) 3 (1200˚C)

1750 (20˚C) 3000 (800˚C) 750 (20˚C) 1200(500˚C)

900

Useful Temperature Limit Tmax (˚C)

1300

TX846_Frame_C01 Page 11 Monday, November 18, 2002 10:34 AM

© 2003 by CRC Press LLC

Table 1.2 Properties of Commonly Used Metals and Alloys and Silicon

Tensile Fiber Modulus of Shear Diameter Density Elasticity Modulus Poisson Strength Elongation 3 Reinforcements d(mm) r(kg/m ) E(Mpa) G(Mpa) Ratio n sUlt (Mpa) E(%)

“R” glass, high performance “E” glass, common applications Kevlar 49 “HT” graphite, high strength “HM” graphite, high modulus Boron Aluminum Aluminum silicate Silicon carbide Polyethylene

Useful Coefficient of Coefficient Thermal of Thermal Heat Temperature Price Expansion Conductivity Capacity Limit Tmax 1993 -1 l(W/M∞C) c(J/kg˚C) a (∞C ) (∞C) ($/kg) -5

0.2

3200

4

0.3 ¥ 10

30,000

0.25

2500

3.5

0.5 ¥ 10

130,000 230,000

12,000 50,000

0.4 0.3

2900 3200

2.3 1.3

-0.2 ¥ 10 -5 0.02 ¥ 10

1800

390,000

20,000

0.35

2500

0.6

0.08 ¥ 10

100 20

2600 3700

400,000 380,000

3400 1400

0.8 0.4

0.4 ¥ 10

10

2600

200,000

3000

1.5

14

2550

200,000

2800

1.3

960

100,000

3000

10

2500

86,000

16

2600

74,000

12 7

1450 1750

6.5

-5

-5

-5

1

800

700

14

1

800

700

2

0.03 200 (20∞C) 60 (800∞C)

1400 800

>1500

70 70

200 (20∞C) 60 (800∞C)

800

>1500

140

900

500 >1000

500

50 (20∞C) 7 (800∞C)

1300

600

-5

-5

0.5 ¥ 10

150

TX846_Frame_C01 Page 12 Monday, November 18, 2002 10:34 AM

© 2003 by CRC Press LLC

Table 1.3 Properties of Commonly Used Reinforcements

Resins

Tensile Density Elastic Shear r Modulus Modulus Poisson Strength Elongation 3 (kg/m ) E(Mpa) G(Mpa) Ratio n sUlt (Mpa) E%

Coefficient of Thermal Expansion -1 a (∞C )

Thermosets

Epoxy

1200

4500

1600

0.4

130

Phenolic Polyester Polycarbonate Vinylester Silicone Urethane

1300 1200 1200 1150 1100 1100

1100 1400

0.4 0.4 0.35

70 80 60 75 35 30

Polyimide

1400

3000 4000 2400 3300 2200 700 to 7000 4000 to 19,000

0.5

1100

0.35

70

2 (100˚C) 6 (200˚C) 2.5 2.5 4

900

1200

1300

4000

1100 1350

2000 3000

1250 1300

3500 4000

0.4

0.35

1 8 6 5

¥ ¥ ¥ ¥

-5

10 -5 10 -5 10 -5 10

0.2

1000

90 to 200

0.3 0.2

1000 1400 1200

120 to 200 60 to 200 120 >100 100 to 350 100

100 1

Thermoplastics

Polypropylene (pp) Polyphenylene sulfone (pps) Polyamide (pa) Polyether sulfone (pes) Polyetherimide (pei) Polyether-etherketone (peek)

-5

11 ¥ 10

Coefficient Useful of Thermal Temperature Price Heat Conductivity Capacity Limit Tmax 1993 l (W/m∞C) C(J/kg∞C) (∞C) ($/kg)

-5

8 ¥ 10

0.2

-5

30

20 to 400

9 ¥ 10

65

100

5 ¥ 10

70 85

200 60

8 ¥ 10 -5 6 ¥ 10

105 90

60 50

6 ¥ 10 -5 5 ¥ 10

1000

250 to 300

330

70 to 140

-5

2.4 4 4

130 to 250

-5

-5

6 to 20

1200

0.2 0.3

170 180

6 25

200 140 to 250

20 96

TX846_Frame_C01 Page 13 Monday, November 18, 2002 10:34 AM

© 2003 by CRC Press LLC

Table 1.4 Properties of Commonly Used Resins

Cores

Balsa

Compressive Modulus Shear Strength Density of Elasticity Modulus Poisson Elongation 3 r(Kg/M ) E(Mpa) G(Mpa) Ratio n sUlt(Mpa) E%

100 to 190 30 to 70

Polyurethane foam Polystyrene 30 to 45 foam Honeycombs Impregnated carton Impregnated glass fabric Aluminum 15 to 130 Steel Nomex®

25 to 50

2000 to 6000 25 to 60

100 to 250

8 to 18 0.4

20 to 30

0.4

50 to 350 100 to 600 130 to 910 550 to 1250 10 to 40

Coefficient of Thermal Expansion -1 a(∞C )

Coefficient Useful of Thermal Temperature Price Heat Conductivity Capacity Limit 1993 Tmax (∞C) l(W/M∞C) C(J/Kg∞C) ($/Kg)

0.05

11 75

0.25 to 1.25

0.2 to 8

0.2 to 2.5

75

TX846_Frame_C01 Page 14 Monday, November 18, 2002 10:34 AM

© 2003 by CRC Press LLC

Table 1.5 Properties of Commonly Used Core Materials

TX846_Frame_C01 Page 15 Monday, November 18, 2002 10:34 AM

Figure 1.5 Tensile Strength of Glass/Resin Composites

Figure 1.6 Specific Strength of Different Composites

© 2003 by CRC Press LLC

TX846_Frame_C02 Page 17 Monday, November 18, 2002 10:40 AM

2 FABRICATION PROCESSES The mixture of reinforcement/resin does not really become a composite material until the last phase of the fabrication, that is, when the matrix is hardened. After this phase, it would be impossible to modify the material, as in the way one would like to modify the structure of a metal alloy using heat treatment, for example. In the case of polymer matrix composites, this has to be polymerized, for example, polyester resin. During the solidification process, it passes from the liquid state to the solid state by copolymerization with a monomer that is mixed with the resin. The phenomenon leads to hardening. This can be done using either a chemical (accelerator) or heat. The following pages will describe the principal processes for the formation of composite parts.

2.1 MOLDING PROCESSES The flow chart in Figure 2.1 shows the steps found in all molding processes. Forming by molding processes varies depending on the nature of the part, the number of parts, and the cost. The mold material can be made of metal, polymer, wood, or plaster.

2.1.1 Contact Molding Contact molding (see Figure 2.2) is open molding (there is only one mold, either male or female). The layers of fibers impregnated with resin (and accelerator) are placed on the mold. Compaction is done using a roller to squeeze out the air pockets. The duration for resin setting varies, depending on the amount of accelerator, from a few minutes to a few hours. One can also obtain parts of large dimensions at the rate of about 2 to 4 parts per day per mold.

2.1.2 Compression Molding With compression molding (see Figure 2.3), the countermold will close the mold after the impregnated reinforcements have been placed on the mold. The whole assembly is placed in a press that can apply a pressure of 1 to 2 bars. The polymerization takes place either at ambient temperature or higher. The process is good for average volume production: one can obtain several dozen parts a day (up to 200 with heating). This has application for automotive and aerospace parts. © 2003 by CRC Press LLC

TX846_Frame_C02 Page 18 Monday, November 18, 2002 10:40 AM

Figure 2.1 Steps in Molding Process

Figure 2.2 Contact Molding

Figure 2.3 Compression Molding © 2003 by CRC Press LLC

TX846_Frame_C02 Page 19 Monday, November 18, 2002 10:40 AM

Figure 2.4 Vacuum Molding

Figure 2.5 Electron Beam or X-ray Molding

2.1.3 Molding with Vacuum This process of molding with vacuum is still called depression molding or bag molding. As in the case of contact molding described previously, one uses an open mold on top of which the impregnated reinforcements are placed. In the case of sandwich materials, the cores are also used (see Chapter 4). One sheet of soft plastic is used for sealing (this is adhesively bonded to the perimeter of the mold). Vacuum is applied under the piece of plastic (see Figure 2.4). The piece is then compacted due to the action of atmospheric pressure, and the air bubbles are eliminated. Porous fabrics absorb excess resin. The whole material is polymerized by an oven or by an autoclave under pressure (7 bars in the case of carbon/epoxy to obtain better mechanical properties), or with heat, or with electron beam, or x-rays; see Figure 2.5). This process has applications for aircraft structures, with the rate of a few parts per day (2 to 4). © 2003 by CRC Press LLC

TX846_Frame_C02 Page 20 Monday, November 18, 2002 10:40 AM

Figure 2.6 Resin Injection Molding

Figure 2.7 Injection of Premixed

Figure 2.8 Injection of Thermoplastic Premixed

2.1.4

Resin Injection Molding

With resin injection molding (see Figure 2.6), the reinforcements (mats, fabrics) are put in place between the mold and countermold. The resin (polyester or phenolic) is injected. The mold pressure is low. This process can produce up to 30 pieces per day. The investment is less costly and has application in automobile bodies.

2.1.5

Molding by Injection of Premixed

The process of molding by injection of premixed allows automation of the fabrication cycle (rate of production up to 300 pieces per day). Thermoset resins: Can be used to make components of auto body. The schematic of the process is shown in Figure 2.7. Thermoplastic resins: Can be used to make mechanical components with high temperature resistance, as shown in Figure 2.8. © 2003 by CRC Press LLC

TX846_Frame_C02 Page 21 Monday, November 18, 2002 10:40 AM

Figure 2.9 Foam Injection

Figure 2.10 Centrifugal Molding

2.1.6 Molding by Foam Injection Molding by foam injection (see Figure 2.9) allows the processing of pieces of fairly large dimensions made of polyurethane foam reinforced with glass fibers. These pieces remain stable over time, with good surface conditions, and have satisfactory mechanical and thermal properties.

2.1.7 Molding of Components of Revolution The process of centrifugal molding (see Figure 2.10) is used for the fabrication of tubes. It allows homogeneous distribution of resin with good surface conditions, including the internal surface of the tube. The length of the tube depends on the length of the mold. Rate of production varies with the diameter and length of the tubes (up to 500 kg of composite per day). The process of filament winding (see Figure 2.11) can be integrated into a continuous chain of production and can fabricate tubes of long length. The rate of production can be up to 500 kg of composite per day. These can be used to make missile tubes, torpillas, containers, or tubes for transporting petroleum. For pieces which must revolve around their midpoint, winding can be done on a mandrel. This can then be removed and cured in an autoclave (see Figure 2.12). The fiber volume fraction is high (up to 85%). This process is used to fabricate components of high internal pressure, such as reservoirs and propulsion nozzles. © 2003 by CRC Press LLC

TX846_Frame_C02 Page 22 Monday, November 18, 2002 10:40 AM

Figure 2.11 Filament Winding

Figure 2.12 Filament Winding on Complex Mandrel

Figure 2.13 Sheet Forming

2.2 OTHER FORMING PROCESSES 2.2.1 Sheet Forming This procedure of sheet forming (see Figure 2.13) allows the production of plane or corrugated sheets by corrugation or ribs. © 2003 by CRC Press LLC

TX846_Frame_C02 Page 23 Monday, November 18, 2002 10:40 AM

Figure 2.14 Profile Forming

Figure 2.15 Stamp Forming

2.2.2. Profile Forming The piece shown in Figure 2.14 is made by pultrusion. This process makes possible the fabrication of continuous open or closed profiles. The fiber content is important for high mechanical properties. The rate of production varies between 0.5 and 3 m/ minute, depending on the nature of the profile.

2.2.3 Stamp Forming Stamp forming (see Figure 2.15) is only applicable to thermoplastic composites. One uses preformed plates, which are heated, stamped, and then cooled down.

2.2.4 Preforming by Three-Dimensional Assembly Example: Carbon/carbon: The carbon reinforcement is assembled by depositing the woven tows along several directions in space. Subsequently the empty space between the tows is filled by “impregnation.” The following two techniques are used: Impregnation using liquid: Pitch is used under a pressure of 1000 bars, followed by carbonization. Impregnation using gas: This involves chemical vapor deposition using a hot gaseous hydrocarbon atmosphere. Example: Silicon/silicon. The reinforcement is composed of filaments of silicon ceramics. The silicon matrix is deposited in the form of liquid solution of colloidal silicon, followed by drying under high pressure and high temperature (2000 bars, 2000∞C). The preforms are then machined. The phases of development © 2003 by CRC Press LLC

TX846_Frame_C02 Page 24 Monday, November 18, 2002 10:40 AM

of these composites, such as the densification (formation of the matrix) are long and delicate. These make the products very onerous. Applications include missile and launcher nozzles, brake disks, ablative tiles for reentry body of spacecraft into the atmosphere.

2.2.5 Cutting of Fabric and Trimming of Laminates Some components need a large number of fabric layers (many dozens, can be hundreds). For the small and medium series, it can be quite expensive to operate manually for following the form of a cut. respect the orientation specified by the design (see Chapter 5). minimizing waste. There is a tendency to produce a cut or a drape automatically with the following characteristics: a programmed movement of the cutting machine a rapid cutting machine, such as an orientable vibrating cutting knife or a laser beam with the diameter of about 0.2 mm and a cutting speed varying from 15 to 40 meters/minute, depending on the power of the laser and the thickness of the part. Example: With a draping machine MAD Forest-Line (FRA), the draping is done in two steps by means of two distinct installations: A cutting machine that produces a roller to which the cut pieces are attached (cassettes) A depositing machine which uses the cassette of cut pieces to perform the draping. The two operations are shown schematically in Figure 2.16.

2.3 PRACTICAL HINTS ON MANUFACTURING PROCESSES 2.3.1 Acronyms To describe the modes of fabricating the composite pieces, the professionals use many abbreviations. Each is detailed below, with reference to the paragraph number where the process is explained. B.M.C.: “Bulk Molding Compound.” Matrix: resins. Reinforcement: cut fibers; additional fillers (powder). Pressure: 5–10 MPa. Temperature: 120– 150∞C. Centrifugation: Matrix: resins. Reinforcement: cut fibers, mat, fabrics; see Section 2.1.7. © 2003 by CRC Press LLC

TX846_Frame_C02 Page 25 Monday, November 18, 2002 10:40 AM

Figure 2.16 Draping Process

Contact molding: Matrix: resins. Reinforcement: mat, fabrics; see Section 2.1.1. Filament winding: Matrix: resins. Reinforcement: continuous fibers; see Section 2.1.7. Compression molding: Matrix: resins. Reinforcement: fabrics or unidirectionals; see Section 2.1.2. Autoclave molding: Matrix: resins. Reinforcement: fabrics or unidirectionals; under pressure in an autoclave; see Section 2.1.3. Pultrusion: Matrix: resins. Reinforcement: mat, fabrics, continuous fibers; see Section 2.2.2. R-RIM: “Reinforced–Reaction Injection Molding” (there is expansion in the mold). Pressure: 0.5 MPa. Temperature: 50–60∞ C; see Section 2.1.6. S-RIM: “Structural Reaction Injection Molding” (components for structure, particularly in automobiles). Similar to R-RIM, injection of liquid thermoset resins consists of two highly reactive constituents. RTM: “Resin Transfer Molding.” Matrix: resins.. Reinforcement: Preforms of cut fibers or fabrics. Pressure: low (in vacuum or 0.1–0.3 MPa). Temperature: 80∞C. SMC: “Sheet Molding Compound.” Matrix: liquid resin with addition of magnesia. Reinforcement: mat, unidirectionals. Pressure: 5–10 MPa. Temperature: 120–150∞C. © 2003 by CRC Press LLC

TX846_Frame_C02 Page 26 Monday, November 18, 2002 10:40 AM

26 Composite Materials: Design and Applications

Figure 2.17 Cost Comparison for Different Processes

© 2003 by CRC Press LLC

TX846_Frame_C02 Page 27 Monday, November 18, 2002 10:40 AM

RTP: “Reinforced Thermoplastics.” Matrix: thermoplastic resins. Reinforcement: cut fibers. Pressure: 50 to 150 MPa. Temperature: 120–150∞C. RST: “Reinforced Stamped Thermoplastics.” Pressure: 15–20 MPa. Initial temperature: ª200∞C; see Section 2.2.3. ZMC: Matrix: resin. Reinforcement: cut fibers. Pressure: 30–50 MPa. Temperature: 120–150∞C. TMC: Similar to “SMC” but with higher amount of glass fibers (a few millimeters in thickness). XMC: Similar to “SMC” but with specific orientation of the fibers.

2.3.2 Cost Comparison The diagram in Figure 2.17 allows the comparison of the cost to fabricate composite products. One needs to note the important difference between the cost of composites produced in large volume and the cost of high performance composites.

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 29 Monday, November 18, 2002 12:05 PM

3 PLY PROPERTIES It is of fundamental importance for the designer to understand and to know precisely the geometric and mechanical characteristics of the “fiber + matrix” mixture which is the basic structure of the composite parts. The description of these characteristics is the object of this chapter.

3.1 ISOTROPY AND ANISOTROPY When one studies the mechanical behavior of elastic bodies under load (elasticity theory), one has to consider the following: An elastic body subjected to str esses deforms in a reversible manner. At each point within the body, one can identify the principal planes on which there are only normal stresses. The normal directions on these planes are called the principal stress directions. A small sphere of material surrounding a point of the body becomes an ellipsoid after loading. The spatial position of the ellipsoid relative to the principal stress directions enables us to characterize whether the material under study is isotr opic or anisotropic. Figure 3.1 illustrates this phenomenon. Figure 3.2 illustrates the deformation of an isotropic sample and an anisotropic sample. In the latter case, the oblique lines represent the preferred directions along which one would place the fibers of reinforcement. One can consider that a longitudinal loading applied to an isotropic plate would create an extension in the longitudinal direction and a contraction in the transverse direction. The same loading applied to an anisotropic plate creates an angular distortion, in addition to the longitudinal extension and transversal contraction. In the simple case of plane stress, one can obtain the elastic constants using stress–strain relations.

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 30 Monday, November 18, 2002 12:05 PM

Figure 3.1 Schematic of Deformation

Figure 3.2 Comparison between Deformation of an Isotropic and Anisotropic Plate

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 31 Monday, November 18, 2002 12:05 PM

Figure 3.3 Stress–Strain Behavior in an Isotropic Material

3.1.1 Isotropic Materials The following relations are valid for a material that is elastic and isotropic.

One can write the stress–strain relation (see Figure 3.3) in matrix form as

Ï ex Ô Ì ey Ô Ó g xy

1

1 n --- – --- 0 E E ¸ Ô n 1 ˝ = – --- --- 0 E E Ô ˛ 1 0 0 ---G

1

Ï sx ¸ Ô Ô Ì sy ˝ Ô Ô Ó t xy ˛

In these equations, ex,ey,gxy are also the small strains that are obtained in a classical manner from the displacements ux and uy as: ex = ∂ux /∂x; ey = ∂uy /∂ y; gxy = ∂ux /∂y + ∂uy /∂x.

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 32 Monday, November 18, 2002 12:05 PM

Figure 3.4 Deformation in an Anisotropic Material

There are three elastic constants: E, n, G. There exists a relation among them as: E G = -------------------2(1 + n ) The above relation shows that a material that is isotropic and elastic can be characterized by two independent elastic constants: E and n.

3.1.2 Anisotropic Material The matrix equation for anisotropic material (see Figure 3.4) is

Ï ex Ô Ì ey Ô Ó g xy

© 2003 by CRC Press LLC

1 ----Ex

¸ Ô n xy ˝ = – -----Ex Ô ˛ 0

n yx – -----Ey 1 ----Ey 0

0

Ï sx ¸ Ô Ô 0 Ì sy ˝ Ô Ô Ó t xy ˛ 1 -------G xy

TX846_Frame_C03 Page 33 Monday, November 18, 2002 12:05 PM

2

Note that the stress–strain matrix above is symmetric. The number of distinct elastic constants is five: Two moduli of elasticity: Ex and Ey, Two Poisson coefficients: nyx and nxy, and One shear modulus: Gxy. In fact there are only four independent elastic constants: Ex, Ey, Gxy, and nyx (or nxy). The fifth elastic constant can be obtained from the others using the symmetry relation: 3

E n xy = n yx -----x Ey

3.2 CHARACTERISTICS OF THE REINFORCEMENT–MATRIX MIXTURE We denote as ply the semi-product “reinforcement + resin” in a quasi-bidimen4 sional form. This can be A tape of unidirectional fiber + matrix, A fabric + matrix, or A mat + matrix. These are examined more below.

3.2.1 Fiber Mass Fraction Fiber mass fraction is defined as Mass of fibers M f = ----------------------------------Total mass In consequence, the mass of matrix is Mass of matrix M m = ------------------------------------Total mass with Mm = 1 – Mf

2 3 4

To know more about the development on this point, refer to Section 9.2 and Exercise 18.1.2. Refer to Section 13.2. Such condition exists in the commercial products. These are called preimpregnated or SMC (sheet molding compound). One can also find non-preformed mixtures of short fibers and resin. These are called premix or BMC (bulk molding compound).

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 34 Monday, November 18, 2002 12:05 PM

Table 3.1 Common Fiber Volume Fractions in Different Processes Molding Process

Fiber Volume Fraction

Contact Molding Compression Molding Filament Winding Vacuum Molding

30% 40% 60%–85% 50%–80%

3.2.2 Fiber Volume Fraction Fiber volume fraction is defined as Volume of fiber V f = ---------------------------------------Total volume As a result, the volume of matrix is given as Volume of matrix V m = --------------------------------------------Total volume 5

with

Vm = 1 – Vf Note that one can convert from mass fraction to volume fraction and vice versa. If rf and rm are the specific mass of the fiber and matrix, respectively, we have Mf --rf

V f = ----------------Mf Mm --- + ----r r f

Vf rf M f = -----------------------------Vf rf + Vm rm

m

Depending on the method of fabrication, the common fiber volume fractions are as shown in Table 3.1.

3.2.3 Mass Density of a Ply The mass density of a ply can be calculated as total mass r = -------------------------------total volume 5

In reality, the mixture of fiber/matrix also includes a small volume of voids, characterized by the porosity of the composite. One has then Vm + Vf + Vp = 1, in which Vp denotes the percentage of “volume of void/total volume.” Vp is usually much less than 1 (See Exercise 18.1.11).

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 35 Monday, November 18, 2002 12:05 PM

Table 3.2 Ply Thicknesses of Some Common Composites

E glass R glass Kevlar H.R. Carbon

Mf

H

34% 68% 65% 68%

0.125 mm 0.175 mm 0.13 mm 0.13 mm

The above equation can also be expanded as mass of fiber mass of matrix r = --------------------------------- + ------------------------------------total volume total volume volume of matrix volume of fiber = ---------------------------------------- r f + -------------------------------------------- r m total volume total volume or

r = r f V f + r mV m

3.2.4 Ply Thickness The ply thickness is defined as the number of grams of mass of fiber mof per 2 m of area. The ply thickness, denoted as h, is such that: m of 2 h ¥ 1 ( m ) = total volume = total volume ¥ ------------------------------------------fiber volume ¥ r f or m of h = --------Vf rf One can also express the thickness in terms of mass fraction of fibers rather than in terms of volume fraction. 1 1–M 1 h = m of ---- + ------ Ê ---------------fˆ rf rm Ë Mf ¯ Table 3.2 shows a few examples of ply thicknesses.

3.3 UNIDIRECTIONAL PLY 3.3.1 Elastic Modulus The mechanical characteristics of the fiber/matrix mixture can be obtained based on the characteristics of each of the constituents. In the literatur e, there are theoretical as well as semi-empirical relations. As such, the results from these relations may not always agree with experimental values. One of the reasons is

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 36 Monday, November 18, 2002 12:05 PM

Table 3.3 Fiber Elastic Modulus Kevlar

Carbon H.R.

Carbon H.M.

fiber longitudinal modulus in direction Ef (MPa)

74,000

130,000

230,000

390,000

fiber transverse modulus in t direction (MPa) Eft

74,000

5400

15,000

6000

fiber shear modulus (Mpa) Gft

30,000

12,000

50,000

20,000

fiber Poisson ratio vft

0.25

0.4

0.3

0.35

Ï Ô Ô Ô Ô Ô Ì Ô Ô Ô Ô Ô Ó

Glass E

Isotropic

Anisotropic

because the fibers themselves exhibit some degree of anisotropy. In Table 3.3, one can see small values of the elastic modulus in the transverse direction for 6 Kevlar and carbon fibers, whereas glass fiber is isotropic. With the definitions in the previous paragraph, one can use the following relations to characterize the unidirectional ply: Modulus of elasticity along the direction of the fiber El is given by

7

E = EfVf + EmVm or E = Ef Vf + Em ( 1 – Vf ) In practice, this modulus depends essentially on the longitudinal modulus of the fiber, Ef, because Em > E m .

Figure 3.12 Elastic Modulus of Glass/Epoxy Layers

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 46 Monday, November 18, 2002 12:05 PM

Figure 3.13 Tensile Strength of Glass/epoxy Layers

The composite (matrix + filler) is isotropic, with elastic properties E, G, n given by the following relations: Defining:

1 – n mˆ V f Em - 1 + 3 Ê -------------------------------K = -------------------------Ë 1 + n m¯ ( 1 – V f ) 3 (1 – 2 nm ) 9KG E ª ----------------3K + G Em 15 1 – n m ˆ V f - 1 + ------ Ê ----------------------------------G ª ----------------------2 (1 + nm ) 2 Ë 4 – 5 n m¯ ( 1 – V f ) 1 3K – 2G n ª --- ÊË --------------------ˆ¯ 2 3K + G

3.5.4 Other Reinforcements One may also use reinforcements in the form of crushed fibers, flakes (see Figure 3.15), or powders made of the following: Glass Graphite Metals

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 47 Monday, November 18, 2002 12:05 PM

Figure 3.14 Spherical Fillers

Figure 3.15 Form of Flakes

Figure 3.16 Mica Flakes Arrangement

Aluminum Mica (L ª 100 mm) Talc (L ª 10 mm) Immersed in a resin with stratified fibers, mica flakes have the arrangement as shown in the Figure 3.16. One can observe that the modulus of the resin is 13 increased as Ln ( 1 + u ) E = 1 – ------------------------- ¥ E mica V mica + E m V m ; u

13

L G m V mica - ¥ -----------u = -- ---------e E mica V m

For more details, see “Interaction Effects in Fiber Composites,” which is listed in the Bibliography at the end of the book.

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 48 Monday, November 18, 2002 12:05 PM

Figure 3.17 Cross Section with and without Mica

Figure 3.18 4D Architecture

The average properties of mica are Emica = 170,000 MPa and rmica = 2,800 kg/m . 3

Figure 3.17 shows the increase resistance against the microfracture of the resin.

3.6 MULTIDIMENSIONAL FABRICS An example of “4D” architecture of carbon reinforcement from the European society of propulsion (FRA) has the reinforcement assembled according to preestablished directions (see Figure 3.18). The fiber volume fraction is on the order 14 of 30%. The matrix comes to fill the voids between the fibers. The principal advantages of these types of composites are The supplementary connection (as compared with the bidimensional plies) makes the composites safe from delamination. The mechanical resistance is conserved—and even improved—at high temperatures (up to 3,000∞C for carbon/carbon). The coefficient of expansion remains small. They are resistant against thermal shock. 14

See Section 2.2.4.

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 49 Monday, November 18, 2002 12:05 PM

Table 3.7 Properties of Three-Dimensional Carbon/Carbon

Aerolor 41 3

Specific mass (kg/m ) Longitudinal tensile fracture strength (MPa) Longitudinal compressive fracture strength (MPa) Tensile strength in z direction (MPa) Compressive strength in z direction (MPa) Shear strength in z plane (MPa) Longitudinal elastic modulus E (MPa) Elastic modulus Ez (MPa) Shear modulus Gz (MPa) Shear modulus G (MPa) Poisson ratio uz Poisson ratio u Thermal expansion coefficient -1 a(∞C ) at 1000∞C at 2,500∞C Thermal expansion coefficient -1 az(∞C ) at 1000∞C at 2,500∞C Coefficient of thermal conductivity (W/m ¥ ∞C)

16

17

Septcarb 4

1700 to 2000 40 to 100 80 to 200

1500 to 2000 95 and increasing, up to 2000∞C 65

>10 80 to 200

3 120

20 to 40 30,000

10 16,000

-6

-6

0.7 ¥ 10 ; 3 ¥ 10 -6

-6

6 ¥ 10 ; 6 ¥ 10

5000 2200 5700 0.17 0.035 -6 -6 3 ¥ 10 ; 4 ¥ 10 -6

-6

7 ¥ 10 ; 9 ¥ 10

300

There is a high coefficient of thermal conductivity. They have small density. The silicon/silicon is transparent to radio-electric waves. Table 3.7 gives the characteristics of two composites made of tridimensional carbon/carbon. The mechanical properties are the same along all directions noted 15 16 17 by in the following figure. The composite is transversely isotropic.

15 16 17

This notion is shown in detail in Section 13.2. Product of the Aerolor company (FRA). Product of European company in propulsion (FRA).

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 50 Monday, November 18, 2002 12:05 PM

Figure 3.19 Layers of ARALL and GLARE

Figure 3.20 Sic Whisker

3.7 METAL MATRIX COMPOSITES There are a number of products in development or in experimental stage including: Matrices: aluminum, magnesium, titanium (see also Section 7.4) and Reinforcements (fibers): aramid, carbon, boron, silicon carbide (SiC) Example: ARALL (Aluminum Reinforced Aramid) and GLARE (Aluminum 18 Reinforced Glass). The essential advantage is better impact damage tolerance because of better resistance to failure due to thin metallic layers and resistance against the crack propagation from one layer to the other (see Figure 3.19). Example: Short silicon carbide fibers (whiskers)/aluminum. This is a socalled “incompatible” composite because the big difference between the thermomechanical properties of the constituents leads to high stress concentrations and debonding between the fibers and the matrix (see Figure 3.20). This has good applications at high temperatures. The diameter of the whisker is about 20 mm. Slenderness ratio L/∆ ª 5 and fiber volume fraction Vf ª 0.3. Example: Boron/aluminum. This is used in aerospace applications (see Section 7.5.4). The technique to obtain these materials is shown schematically in Figure 3.21. This composite can be used continuously at temperatures on the order of 300∞C, while maintaining notable mechanical properties (see Section 1.6 for the properties of boron).

18

®

AKZO Fibers/DELFT University (Holland). Structural Laminates Company/New Kensington (USA).

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 51 Monday, November 18, 2002 12:05 PM

Figure 3.21 Boron/Aluminum Composite

Some characteristics of unidirectional plies made of aluminum matrix (6061) include:

Fiber volume fraction Vf (%) 3 Specific mass (kg/m ) Longitudinal tensile strength (MPa) Longitudinal compressive strength (MPa) Longitudinal elastic modulus (MPa)

HR Carbon

Aluminum

Silicon Carbide

50 2300 800 600 200,000

50 3100 550 3100 190,000

50 2700 1400 3000 140,000

3.8 TESTS The relations cited on the previous pages for the calculation of the modulus and Poisson coefficients of the composites only allow obtaining an order of magnitude for the mechanical properties. Some of these relations are not quite accurate, particularly for the shear modulus. Also, these properties are very sensitive to the fabrication conditions. It is necessary for the design engineer to have the results provided by the suppliers of the reinforcement and the matrix materials or to better the results obtained by tests in the labs. Some of these tests have been standardized, for example, tensile tests, flexure tests, and impact tests. A tensile test (NF T 51–034, ASTM D 3039) on the specimen in Figure 3.22, instrumented with electrical strain gage, allows the measurement of the strength and the elongation to fracture. A delamination test (NF T 57–104) on a specimen which has a small span for bending (see Figure 3.23). It fails by delamination under the effect of interlaminar shear stress. One can obtain the interlaminar shear 19 strength. There are other tests, not yet standardized, that are very useful for the fabrication of high performance composites, for example, for control of the fiber volume fraction. In fact, during the phase of polymerization under pressure of a polymer matrix composite, the resin gets absorbed into an absorbing fabric, in variable quantity depending on the cycle of pressure and temperature. In consequence, 19

This is a simplified way that little reflects the complexity of the state of real stress due to the presence of very close concentrated loads.

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 52 Monday, November 18, 2002 12:05 PM

Figure 3.22 Tensile Test

Figure 3.23 Short Beam Shear Test

Figure 3.24 Variation In Stiffness During Curing

the fiber volume fraction Vf varies, and as a result, the dimensional characteristics of the piece (thickness) also vary. To deal with this problem, one may want to evaluate by test the optimal moment for the application of pr essure, by the measurement of the flexural rigidity of a specimen as a function of time of fabrication (see Figure 3.24).

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 53 Monday, November 18, 2002 12:07 PM

4 SANDWICH STRUCTURES Sandwich structures occupy a large proportion of composite materials design. They appear in almost all applications. Historically they were the first light and 1 high-performance structures. In the majority of cases, one has to design them for a specific purpose. Sandwich structures usually appear in industry as semifinished products. In this chapter we will discuss the principal properties of sandwich structures.

4.1 WHAT IS A SANDWICH STRUCTURE? A sandwich structure results from the assembly by bonding—or welding—of two thin facings or skins on a lighter core that is used to keep the two skins separated (see Figure 4.1). Their properties are astonishing. They have Very light weight. As a comparison, the mass per unit area of the dome 2 of the Saint Peter’s Basilica in Rome (45 meter diameter) is 2,600 kg/m , whereas the mass per surface area of the same dome made of steel/ 2 polyurethane foam sandwich (Hanover) is only 33 kg/m . Very high flexural rigidity. Separation of the surface skins increases flexural rigidity. Excellent thermal insulation characteristics. However, be careful: Sandwich materials are not dampening (no acoustic insulation). Fire resistance is not good for certain core types. The risk of buckling is greater than for classical structures. The facing materials are diverse, and the core materials are as light as possible. One can denote couples of compatible materials to for m the sandwich (see Figure 4.2). Be careful: Polyester resins attack polystyrene foams. 1

See Section 7.1.

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 54 Monday, November 18, 2002 12:07 PM

Figure 4.1 Sandwich Structure (10 £ Ec/Ep £ 100)

Figure 4.2 Constituents of Sandwich Materials

The assembly of the facings to the core is carried out using bonding adhesives. In some exceptional cases, the facings are welded to the core. The quality of the bond is fundamental for the performance and life duration of the piece. In practice we have 0.025 mm £ adhesive thickness £ 0.2 mm

4.2 SIMPLIFIED FLEXURE 4.2.1 Stresses Figure 4.3 shows in a simple manner the main stresses that arise due to the 2 application of bending on a sandwich beam. The beam is clamped at its left end, and a force T is applied at its right end. Isolating and magnifying one elementary segment of the beam, on a cross section, one can observe the shear stress resultant T and the moment resultant M. The shear stress resultant T causes shear stresses t and the moment resultant causes normal stresses s. 2

For more details on these stresses, see Chapters 15 and 17, and also Applications 18.3.5 and 18.3.8.

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 55 Monday, November 18, 2002 12:07 PM

Figure 4.3 Bending Representation

Figure 4.4 Stresses in Sandwich Structure

To evaluate t and s, one makes the following simplifications: The normal stresses are assumed to occur in the facings only, and they are uniform across the thickness of the facings. The shear stresses are assumed to occur in the core only, and they are 3 uniform in the core. One then obtains immediately the expressions for t and s for a beam of unit width and thin facings shown in Figure 4.4.

4.2.2 Displacements In the following example, the displacement D is determined for a sandwich beam subjected to bending as a consequence of Deformation due to normal stresses s and Deformation created by shear stresses t (see Figure 4.5). 3

See Section 17.7.2 and the Applications 18.2.1 and 18.3.5 for a better approach.

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 56 Monday, November 18, 2002 12:07 PM

Figure 4.5 Bending Deflection

To evaluate D, one can, among other methods, use the Castigliano theorem 4

2

1 k 1 M 2 W = --- ----------- dx + --- ------------T dx 2 · GSÒ 2 · EIÒ

Ú

elastic energy

Ú

contribution from bending

D

deflection

∂W = -------∂F

contribution from shear

energy load

5

where the following notations are used for a beam of unit width: M = Moment resultant T = Shear stress resultant Ep = Modulus of elasticity of the material of the facings Gc = Shear modulus of the core material ( ec + ep ) -; · EI Ò #E p e p ¥ 1 ¥ --------------------2 2

k/ · GS Ò = 1/G c ( e c + 2e p ) ¥ 1.

Example: A cantilever sandwich structure treated as a sandwich beam (see Figure 4.6). Elastic energy is shown by 1 W = --2

2 2 1 F ( – x) ------------------------ dx + --2 · EI Ò 0

Ú

2

k

dx Ú ------------F · GSÒ 2

0

3

k F W = ----- Ê -------------- + ------------ˆ 2 Ë 3 · EIÒ · GSÒ ¯ 4

5

See Equation 15.16 that allows one to treat this sandwich beam like a homogeneous beam. One can also use the classical strength of materials approach. See Application 18.2.1 or Chapter 15.

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 57 Monday, November 18, 2002 12:07 PM

Figure 4.6 Cantilever Beam

where · EI Ò = 475 ¥ 10 ; 2

· GSÒ ------------ = 650 ¥ 10 2 k

The end displacement D can be written as ∂W D = -------∂F Then for an applied load of 1 Newton D = 0.7 ¥ 10 Flexure

–2

mm/N + 1.54 ¥ 10

–2

mm/N

Shear

Remark: Part of the displacement D due to shear appears to be higher than that due to bending, whereas in the case of classical homogeneous beams, the shear displacement is very small and usually neglected. Thus, this is a specific property of sandwich structures that strongly influences the estimation of the bending displacements.

4.3 A FEW SPECIAL ASPECTS 4.3.1 Comparison of Mass Based on Equivalent Flexural Rigidity (EI) Figure 4.7 allows the comparison of different sandwich structures having the same flexural rigidity ·EI Ò. Following the discussion in the previous section, this accounts for only a part of the total flexural deformation. © 2003 by CRC Press LLC

TX846_Frame_C04 Page 58 Monday, November 18, 2002 12:07 PM

Figure 4.7 Comparison of Plates Having Similar Flexural Rigidity EI

Figure 4.8 Buckling of Sandwich Structure

4.3.2 Buckling of Sandwich Structures The compression resistance of all or part of a sandwich structure is limited by the so-called critical values of the applied load, above which the deformations become large and uncontrollable. This phenomenon is called buckling of the structure (see Figure 4.8). Depending on the type of loading, one can distinguish different types of buckling which can be global or local.

4.3.2.1 Global Buckling 6

Depending on the supports, the critical buckling load Fc is given by p · EI Ò F cr = K -------------------------------------2 2 · EI Ò + p -------------kK · GS Ò 2

6

See Application 18.3.4.

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 59 Monday, November 18, 2002 12:07 PM

Figure 4.9 Local Buckling of Facings

Figure 4.10 Damage by Local Buckling

4.3.2.2 Local Buckling of the Facings The facings are subject to buckling due to the low stiffness of the core. Depending on the type of loading, one can find the modes of deformation as shown in Figure 4.9. The critical compression stress is given in the equation below where nc is the Poisson coefficient of the core. 2 1/3

s cr = a ¥ (E p ¥ E c ) with

2 – 1 /3

a = 3 { 12 ( 3 – v c ) ( 1 + v c ) } 2

The critical load to cause local damage by local buckling of a facing and the types of damage are shown in Figure 4.10.

4.3.3 Other Types of Damage Local crushing: This is the crushing of the core material at the location of the load application (see figure below).

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 60 Monday, November 18, 2002 12:07 PM

Compression rupture: In this case (see figure below), note that the weak com7 pression resistance of Kevlar fibers leads to a compression strength about two times less than for sandwich panels made using glass fibers.

4.4 FABRICATION AND DESIGN PROBLEMS 4.4.1 Honeycomb: An Example of Core Material These well-known materials are made of hexagonal cells that are regularly spaced. Such geometry can be obtained using a technique that is relatively simple. Many thin sheets are partially bonded. Starting from stacked bonded sheets, they are expanded as shown in Figure 4.11. The honeycomb material can be metal (light alloy, steel) or nonmetal (carton impregnated with phenolic resin, polyamide sheets, or impregnated glass fabrics). Metallic honeycombs are less expensive and more resistant. Nonmetallic honeycombs are not sensitive to corrosion and are good thermal insulators. The following table shows the mechanical and geometric characteristics of a few current honeycombs, using the notations of Figure 4.11. Table 4.1 Properties of Some Honeycomb

Dia. (D): inscribed circle (mm) Thickness e (mm) 3 Specific mass (kg/m ) Shear strength txz rup (MPa) Shear modulus: Gxz (MPa) # 1.5 Gmat(e/D) Shear strength tyz rup (MPa) Shear modulus: Gyz (MPa) Compression strength: sz rup (MPa) a

Bonded Sheets of a Polyamide: Nomex

Light Alloy AG3

Light Alloy 2024

6; 8; 12

4

6

64 1.7 58

0.85 24 2.8

Nomex® is a product of Du Pont de Nemours.

7

See Section 3.3.3.

© 2003 by CRC Press LLC

0.05 80 3.2 520

2 250 4.4

0.04 46 1.5 280

0.9 140 2

TX846_Frame_C04 Page 61 Monday, November 18, 2002 12:07 PM

Figure 4.11 Honeycomb

Figure 4.12 Processing of Honeycomb

Figure 4.13 Deformation of Honeycomb

4.4.2

Processing Aspects

The processing of the honeycomb is done with a diamond disk (peripheral speed in the order of 30 m/s). The honeycomb is kept on the table of the machine by an aluminum sheet to which it is bonded. Below the aluminum sheet, a depression anchors it to the table (see Figure 4.12). One can also deform the honeycomb. It is important to constrain it carefully, because the deformation behavior is complex. For example, a piece of honeycomb 8 under cylindrical bending shows two curvatures as illustrated in Figure 4.13. 8

This phenomenon is due to the Poisson effect, particularly sensitive here (see Section 12.1.4).

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 62 Monday, November 18, 2002 12:07 PM

Figure 4.14 Over-Expansion of Honeycomb

Figure 4.15 Curvature of Honeycomb

Figure 4.16 Processing of a Sandwich Piece of a Structural Part

The processing can be facilitated using the method of overexpansion which modifies the configuration of the cells as shown in Figure 4.14. At limit of curvature, R is the radius of the contour, and e is the thickness of the sheets which consitute the honeycombs (see Figure 4.15). Nomex honeycombs (sheets of bonded polyamide) must be processed at high temperature. The schematic for the processing of a structural part of sandwich honeycomb is as in Figure 4.16. For moderate loadings (for example, bulkheads), it is possible to fold a sandwich panel following the schematic in Figure 4.17. © 2003 by CRC Press LLC

TX846_Frame_C04 Page 63 Monday, November 18, 2002 12:07 PM

Figure 4.17 Folding of Honeycomb

Figure 4.18 Incorporation of Inserts

4.4.3 Insertion of Attachment Pieces When it is necessary to transmit local loadings, depending on the intensity of these loads, it is convenient to distribute these over one or many inserts, as 9 indicated in Figure 4.18. The filling resin of epoxy type, shown in Figure 4.18, can be lightened by incorporation of phenolic microspheres with resulting density 3 for the lightened resin of 700 to 900 kg/m and crush strength # 35 MPa (see Figure 4.19).

4.4.4 Repair of Laminated Facings For sandwich materials of the type “honeycombs/laminates,” the repair of local damage is relatively easy. It consists of patching the plies of the laminate. The configuration of the repair zone appears as in Figure 4.20.

4.5 NONDESTRUCTIVE QUALITY CONTROL Apart from using the classical methods for controlling the surface defects, which allows the repair of external delaminations of laminated facings, using the following techniques allows the identification and repair of internal defects due to fabrication or due to damages in service. These defects can entail imper fect bonding, delaminations, and inclusions. Principal nondestructive detection methods are illustrated in Figure 4.21.

9

See Sections 6.2.4 and 6.3.

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 64 Monday, November 18, 2002 12:07 PM

Figure 4.19 Some Links for Sandwich Structures

Figure 4.20 Honeycomb Repair

When a composite structure (for example, a reservoir under pressure) is subjected to loading, many microcracks can occur within the piece. Microcracking in the resin, fiber fracture, and disbond between fiber and matrix can exist even within the admissible loading range. These ruptures create acoustic waves that propagate to the surface of the piece. They can be detected and analyzed using acoustic emission sensors (see Figure 4.22). The number of peaks as well as the duration and the amplitude of the signal can be used to indicate the integrity of the piece. In addition, the accumulated number of peaks may be used to predict the fracture of the piece (i.e., the change of slope of the curve in Figure 4.23). © 2003 by CRC Press LLC

TX846_Frame_C04 Page 65 Monday, November 18, 2002 12:07 PM

Figure 4.21 Principal Nondestructive Testing Methods

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 66 Monday, November 18, 2002 12:07 PM

Figure 4.21 (Continued).

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 67 Monday, November 18, 2002 12:07 PM

Figure 4.22 Acoustic Emission Technique

Figure 4.23 Plotting of AE Events

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 69 Monday, November 18, 2002 12:09 PM

5 CONCEPTION AND DESIGN A different paradigm: As every mechanical part, a composite part has to withstand loadings. In addition, the conception process has to extend over a range much larger than for a component made of “pre-established” material. In fact, For isotropic materials, the classical process of conception consists of selection of an existing material and then design of the piece. For a component made of composites, the designer “creates” the material based on the functional requirements. The designer chooses the reinforcement, the matrix, and the process for curing. Following that the designer must define the component architecture, i.e., the arrangement and dimensions of plies, the representation of these on the designs, etc. These subjects are covered in this chapter.

5.1 DESIGN OF A COMPOSITE PIECE The following characteristic properties always have to be kept in mind by the designer: Fiber orientation enables the optimization of the mechanical behavior along a specific direction. The material is elastic up to rupture. It cannot yield by local plastic deformation as can classical metallic materials. Fatigue resistance is excellent.

A Very Good Fatigue Resistance The specific fatigue resistance is expressed by the ratio (s/r), with r being the specific mass. For composite materials, this specific resistance is three times higher than for aluminum alloys and two times higher than that of high strength steel and titanium alloys because the fatigue resistance is equal to 90% of the static fracture strength for a composite, instead of 35% for aluminum alloys and 50% 1 for steels and titanium alloys (see Figure 5.1). 1

See Section 5.4.4.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 70 Monday, November 18, 2002 12:09 PM

Figure 5.1 Comparison of Fatigue Behavior Between Composite and Aluminum

The percent elongation is not the same as that for metals (attention should be paid to the metal/composite joints). Complex forms can be easily molded. It is possible to reduce the number of parts and to limit the amount of processing work. One must adapt the classical techniques of attachments and take into account their induced problems: fragility, delustering, fatigue, thermal stresses.

5.1.1 Guidelines for Values for Predesign Figure 5.2 shows a comparison between different materials, which can help in the choice of composite in the predesign phase. Figure 5.3 allows the comparison of principal specific properties of fibers which make up the plies. The specific modulus and specific strength are presented in the spirit of lightweight structural materials. The safety factors are defined to take care of uncertainties on

The The The The The

magnitude of mechanical characteristics of reinforcement and matrix stress concentrations imperfection of the hypotheses for calculation fabrication process aging of materials

The orders of magnitude of safety factors are as follows:

High volume composites: Static loading Intermittent loading over long term: Cyclic loading: Impact loading: High performance composites:

© 2003 by CRC Press LLC

short duration: long duration:

2 4 4 5 10 1.3 to 1.8

TX846_Frame_C05 Page 71 Monday, November 18, 2002 12:09 PM

Figure 5.2 Comparison of Characteristics of Different Materials

Figure 5.3 Specific Characteristics of Different Fibers

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 72 Monday, November 18, 2002 12:09 PM

Figure 5.4 Unidirectional Layer

5.2 THE LAMINATE Recall that laminates result in the superposition of many layers, or plies, or sheets, made of unidirectional layers, fabrics or mats, with proper orientations in each ply. This is the operation of hand-lay-up.

5.2.1 Unidirectional Layers and Fabrics Unidirectional layers are as shown in Figure 5.4. The advantages of unidirectional layers are: They have high rigidity (maximum number of fibers in one direction). The ply can be used to wrap over long distance. Then the load transmission of the fibers is continuous over large distance. They have less waste. The disadvantages of unidirectional layers are The time for wrapping is long. One cannot cover complex shapes using wrapping. Example: Carbon/epoxy unidirectionals: Width 300 or 1000 mm, preimpregnated with resin; usable over a few years when stored at cold temperature (–18∞C). Fabrics can be found in rolls in dry form or impregnated with resin (Figure 5.5). The advantages of fabrics are Reduced wrapping time Possibility to shape complex form using the deformation of the fabric Possibility to combine different types of fibers in the same fabric The disadvantages of fabrics are Lower modulus and strength than the case of unidirectionals Larger amount of waste material after cutting Requirement of joints when wrapping large parts

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 73 Monday, November 18, 2002 12:09 PM

Figure 5.5 A Fabric Layer

5.2.2 Importance of Ply Orientation One of the fundamental advantages of laminates is their ability to adapt and control the orientation of fibers so that the material can best resist loadings. It is therefore important to know how the plies contribute to the laminate resistance, taking into account their relative orientation with respect to the loading direction. Figures 5.6 through 5.9 show the favorable situations and those that should be avoided. Recall the Mohr circle:

cf. for example the stress state below and the associated Mohr circle

In Figure 5.7, the Mohr circle for stresses shows that the 45∞ fibers support the compression, s1 = -t (t is the arithmetic value of shear stress), while the resin supports the tension, s2 = t , with low fracture limit. The fibers in Figure 5.8 support the tension, s1 = t, whereas the resin supports the compression, s2 = -t. In Figure 5.9, one has deposited the fibers at 45∞ and –45∞. Taking into account the previous remarks, one observes that the 45∞ fibers can support the tension s1 = t, whereas the -45∞ fibers can support the compression, s2 = -t. The resin is less loaded than previously.

5.2.3 Code to Represent a Laminate 5.2.3.1 Normalized Orientation Considering the working mode of the plies as discussed in the previous section, the most frequently used orientations are represented as in Figure 5.10. The direction called “0∞” corresponds to either the main loading direction, a preferred direction of the piece under consideration, or the axis of the chosen coordinates. Note: One also finds in real applications plies with orientations ±30∞ and ±60∞.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 74 Monday, November 18, 2002 12:09 PM

Figure 5.6 Effect of Ply Orientation

Figure 5.7 Bad Design

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 75 Monday, November 18, 2002 12:09 PM

Figure 5.8 Mediocre Design

Figure 5.9 Good Design

Figure 5.10 Common Orientations

5.2.3.2 Middle Plane By definition the middle plane is the one that separates two half-thicknesses of the laminate. In Figure 5.11, the middle plane is the plane x–y. On this plane, z = 0.

5.2.3.3 Description of Plies The description of plies is done by beginning with the lowest ply on the side z < 0 and proceeding to the uppermost ply of the side z > 0. In so doing, Each ply is noted by its orientation. The successive plies are separated by a slash “/”.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 76 Monday, November 18, 2002 12:09 PM

Figure 5.11 Laminate and its Middle Plane x–y 2

One must avoid the grouping of too many plies of the same orientation. However, when this occurs, an index number is used to indicate the number of these identical plies.

5.2.3.4 Midplane Symmetry One notes that a laminate has midplane symmetry or is symmetric when the stacking of the plies on both sides starting from the middle plane is identical. Example:

Example:

2

This is to limit the interlaminar stresses (see Section 5.4.4 and Chapter 17). This precaution applies also to the fabrics (for example, no more than four consecutive fabric layers of carbon/ epoxy along one direction).

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 77 Monday, November 18, 2002 12:09 PM

Figure 5.12 Effect of Laminate Lay-up on Deformation

5.2.3.4.1 What Is the Need of Midplane Symmetry For the construction of laminated pieces, the successive impregnated plies are stacked at ambient temperature, then they are placed within an autoclave for curing. At high temperature, the extension of the whole laminate takes place without warping. However, during cooling, the plies have a tendency to contract differently depending on their orientations. From this, thermal residual stresses occur. When midplane symmetry is utilized, it imposes the symmetry on these stresses and prevents the deformations of the whole part, for example, warping as shown in Figure 5.12.

5.2.3.5 Particular Cases of Balanced Fabrics Some laminates are made partially or totally of layers of balanced fabric. One then needs to describe on the drawing the composition of the laminate. Example:

The previous laminate, made up of three layers of balanced fabric, has midplane symmetry. In effect, if one considers one woven fabric layer as equivalent to two 3 series of unidirectional layers crossed at 90∞, it also has midplane symmetry. 3

If this hypothesis is to be verified for a plain weave or a taffeta (see Section 3.4.1), and even for a ribbed twill, it becomes worse as long as the pitch of the weaving machine increases (pitch of the plain weave: 2; ribbed twill: 3; 4-harness satin: 4; 5-harness satin: 5; etc.). If one supposes that this pitch is increasing towards infinity, then the woven fabric becomes the superposition of two unidirectional layers crossed at 90∞. It then does not possess midplane symmetry any more. This property can be observed on a unique ply of 5-harness satin of carbon/epoxy as it is cured in an autoclave, which deforms (curved surface) on demolding (see Application 18.2.17).

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 78 Monday, November 18, 2002 12:09 PM

Figure 5.13 Laminate with Balanced Fabrics; Representation 1

As indicated in Section 3.4.2, one can consider the resulting laminate in two 4 different ways : (a) Each layer of fabric is replaced by two identical plies crossed at 90∞, each with thickness equal to half the thickness e of the fabric layer and each with known elastic properties. This representation is convenient for the determination of the elastic properties of the laminate. One then has the equivalencies shown in Figure 5.13. (b) Each layer of fabric is replaced by one anisotropic ply with thickness e for which one knows the elastic properties and failure strengths. This representation is useful for the determination of the rupture stress of the laminate. One then has the equivalencies shown in Figure 5.14.

5.2.3.6 Technological Minimum Generally one uses a minimum amount of plies (from 5 to 10%) for each direction: 5 0∞, 90∞, 45∞, -45∞. The minimum thickness of a laminate should be of the order of one millimeter, for example, eight unidirectional layers, or three to four layers of balanced fabric of carbon/epoxy.

5.2.4 Arrangement of Plies The proportion and the number of plies to place along each of the directions — 0∞, 90∞, 45∞, -45∞—take into account the mechanical loading that is applied to the laminate at the location under consideration. A current case consists of loading 4 5

See Exercises 18.2.9 and 18.2.10. Apart from space applications, where thicknesses are very small, the skins of sandwich plates are laminates which do not have separately midplane symmetry.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 79 Monday, November 18, 2002 12:09 PM

Figure 5.14 Laminate with Balanced Fabrics; Representation 2

Figure 5.15 Stresses and Stress Resultants 6

of the laminate in its plane. This is called membrane loading. The mechanical loadings can take the form of stresses (sx, sy, txy in Figure 5.15a) or stress resultants (Nx, Ny, Txy in Figure 5.15b). The stress resultants are the products of the stresses with the thickness h of the laminate. Generally, three criteria should be considered by the designer for the ply configuration: 1. Support the loading without deterioration of the laminate 2. Limit the deformation of the loaded piece 3. Minimize the weight of the material used These criteria do not always work together. For example, searching for minimum thickness might not be compatible with high rigidity. Searching for high rigidity 6

The laminate can also work in bending. This is studied in Chapters 12 and 17.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 80 Monday, November 18, 2002 12:09 PM

Figure 5.16 Example of Representation

might not be compatible with minimum weight. One will see in Section 5.4 guidelines for proportions values that allows a laminate with minimum laminate thickness to support specified mechanical loading without damage,. Once a laminate is defined (number of layers and orientations), one must respect the following conditions (without forgetting the technological minimum indicated at the end of the previous paragraph) as much as possible: 90∞ plies placed on the surface, then 45∞ and -45∞ plies, when the predominant stress resultant is oriented along the 0∞ direction No more than 4 consecutive plies along the same direction

5.2.4.1 Example of Representation The plies are progressively terminated to obtain a gradual change in thickness (maximum 2 plies for each 6 mm interval). The symbols for the composition of the laminate are shown on plan view (see Figure 5.16).

5.2.4.2 The Case of Sandwich Structure The description of the sandwich material is done as in Figure 5.17.

5.3 FAILURE OF LAMINATES 5.3.1 Damages Figure 5.18 shows schematically different types of failure leading to damage of a laminate. The main modes of damage, when the loads exceed the critical limits, are illustrated in Figure 5.19.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 81 Monday, November 18, 2002 12:09 PM

Figure 5.17 Description of a Sandwich Material

Figure 5.18 Different Modes of Failure

Figure 5.19 Modes of Damage

One cannot be satisfied with the classical maximum stress criterion Figure 5.20 shows a unidirectional laminate loaded successively in two different manners. In the two cases, the maximum normal stress has the same value denoted

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 82 Monday, November 18, 2002 12:09 PM

Figure 5.20 Stresses and Fiber Orientation

as s. In the loading case (a), the unidirectional specimen will rupture when

s > srupture along This is the maximum stress criterion. In the loading case (b), the maximum normal stress occurs in a direction that is different from that of the fibers (one can obtain this by tracing the Mohr’s circle as discussed previously). We have seen (Section 3.3.2) that the rupture resistance decreases. It is weaker than the situation of case (a). The unidirectional laminate therefore ruptures when

s < srupture along This phenomenon is more evident if the unidirectional laminate is loaded in a direction transverse to the fibers t. In this case, the laminate rupture resistance is that of the matrix, which is much less than that of the fibers. Taking into consideration the evolution of the rupture resistance with the loading direction, one can not use a simple maximum stress criterion as for the classical metallic materials.

5.3.2 Most Frequently Used Criterion: Hill–Tsai Failure Criterion

7

One can apply this criterion successively to each ply of the laminate, that is for each one of the orientations 0∞, 90∞, ±45∞ that have been considered. As has been discussed in Chapter 3, the axes of a unidirectional ply are denoted as for the direction along the fibers, and t for the transverse direction. The stresses are denoted as s in the fiber direction, st in the direction transverse to the fibers, and tt for the shear stress (see figure below). One denotes the Hill–Tsai number (see Figure 5.21) the number a such that If a < 1: no ply rupture occurs. If a ≥ 1: rupture occurs in the ply considered. Generally, this deterioration is due to the rupture of the resin. The mechanical properties of a broken ply become almost negligible, except for those along the fiber direction (modulus of elasticity and rupture resistance) 7

For more detailed study of this criterion, see Chapter 14.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 83 Monday, November 18, 2002 12:09 PM

Figure 5.21 Hill–Tsai Number

5.3.2.1 Notes Attention: The rupture resistance srupture does not have the same value in tension and in compression (see, for example, Section 3.3.3). It is therefore useful to place in the denominators of the previous Hill–Tsai expression the rupture resistance values corresponding to the mode of loading (tension or compression) that appear in the numerator. Using this criterion, when one detects the rupture of one of the plies (more precisely the rupture of the plies along one of the four orientations), this does not necessarily lead to the rupture of the whole laminate. In most cases, the degraded laminate continues to resist the applied stress resultants. In increasing these stress resultants, one can detect which orientation can produce new rupture. This may—or may not—lead to complete rupture of the laminate. If complete rupture does not occur, one can still increase 8 the admissible stress resultants. In this way one can use a multiplication factor on the initial critical loading to indicate the ratio between the first ply rupture and the ultimate rupture. As a consequence of the previous remark it appears possible to work with a laminate that is partially degraded. It is up to the designer to consider the finality of the application, to decide whether the partially degraded laminate can be used. One can make a parallel–in a gross way–with the situation of classical metallic alloys as represented in Figure 5.22.

5.3.2.2 How to Determine s, st, tt in Each Ply Consider for example the laminate shown in Figure 5.23, consisting of identical plies. The following characteristics are known:

8

See Exercise 18.2.7.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 84 Monday, November 18, 2002 12:09 PM

Figure 5.22 Comparison of Behavior until Failure Between Metal and Laminated Material

Figure 5.23 Average Stresses

the mechanical properties of the basic ply the proportions (percentages) of plies in each of the directions (0∞, 90∞, 45∞, -45∞) the global values of the applied stresses, here, for example, sx and txy One considers this case of loading as consisting of the superposition of two simple loading cases: sx only, and then txy only. For each of these cases of elementary loadings, one looks for the stresses s, st, tt in each ply. Manual calculation is 9 usually too long. It should be replaced by using a computer. Appendix 1 has tables for stress values for carbon/epoxy plies with 60% fiber volume fraction. Subsequently, one finds, always for each ply, the sum of the stresses s , st, and tt, respectively, due to each of the simple loadings sx and txy. It is then possible to calculate the Hill–Tsai number to verify the integrity of each of the plies. In the Application 18.1.6, there is an example to determine the thickness of a laminate subject to this type of combined loading.

9

The procedure for this calculation is described in Section 12.1.3.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 85 Monday, November 18, 2002 12:09 PM

5.4 SIZING OF THE LAMINATE 5.4.1 Modulus of Elasticity. Deformation of a Laminate For the varied proportions of plies in the 0∞, 90∞, ±45∞, the tables that follow allow the determination of the deformation of a laminated plate subject to the applied stresses. For this one uses a stress–strain relation similar to that described in Section 3.1 for an anisotropic plate, which is repeated below:

Ex, Ey, Gxy, nxy, nyx are the modulus of elasticity and Poisson ratios of the laminate, and ex, ey, gxy are normal and shear strains in the plane xy. Example: What are the elastic moduli and thermal expansion coefficients for a glass/epoxy laminate (Vf = 60%) with the following ply configuration?

10

Answer: Table 5.14 indicates the following values for this laminate: Ex = 33,100 MPa Ey = 17,190 MPa (this value is obtained by permuting the proportions of 0∞ and 90∞) nxy = 0.34 nyx = 0.17 Table 5.15) shows Gxy = 6,980 MPa. One then obtains the strains ex, ey, gxy, when the stresses are known, using the matrix relation mentioned above. -5 For the coefficient of thermal expansion, Table 5.14 shows: ax = 0.64 ¥ 10 -5 and ay = 1.21 ¥ 10 by permuting the proportions of 0∞ and 90∞.

10

Recall (Sections 3.1 and 3.2) that uxy/Ex = uyx/Ey .

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 86 Monday, November 18, 2002 12:09 PM

5.4.2 Case of Simple Loading The laminate is subjected to only one single stress: sx or sy or txy. Depending on the percentages of the plies in the four directions, one would like to know the order of magnitude of the stresses that can cause first ply failure in the laminate.

Tables 5.1 through 5.15 indicate the maximum stresses as well as the elastic characteristics and the coefficients of thermal expansion for the laminates having the following characteristics: Materials include carbon, Kevlar, glass/epoxy with Vf = 60% fiber volume fraction. All have identical plies (same unidirectionals, same thickness). The laminate is balanced (same number of 45∞ and -45∞ plies). The midplane symmetry is realized. The percentages of plies along the 4 directions 0∞, 90∞, ±45∞ vary in increments of 10%. Calculation of the maximum stresses sx max, sy max, txy max is done based on the Hill–Tsai 11 failure criterion. Example of how to use the tables:

Which maximum tensile stress along the 0∞ direction can be applied to a Kevlar/ epoxy laminate containing 60% fiber volume with the orientation distribution as shown in the above figure? Answer: Table 5.6 indicates the maximum stress in the 0∞ direction (or x). For the percentages given, one has:

sx max(tension) = 308 MPa 11

See Application 18.2.2.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 87 Monday, November 18, 2002 12:09 PM

Table 5.1 Carbon/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Maximum stress sx max (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

Example:

Which maximum compression stress along the 90∞direction (or y) can be applied to a carbon/epoxy laminate containing 60% fiber volume fraction with the orientation distribution as shown in the above figure?

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 88 Monday, November 18, 2002 12:09 PM

Table 5.2 Carbon/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Maximum stress symax (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

Answer: Table 5.2 shows the maximum stresses in the 90∞ direction. For this configuration, one has

symax = s13/67/10/10 = s10/60/15/15 + Ds = 744 + Ds 0∞

Denoting p and p one has

90∞

as the proportions of the plies along the 0∞ and 90∞ directions,

∂s ∂s 0∞ - ¥ Dp 90∞ D s = --------¥ Dp + ---------0∞ 90∞ ∂p ∂p

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 89 Monday, November 18, 2002 12:09 PM

Table 5.3 Carbon/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Maximum stress txymax (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

One obtains by linear interpolation: 3 7 D s = ( 747 – 744 ) ¥ ------ + ( 846 – 744 ) ¥ ------ = 72 MPa 10 10 Therefore,

sy max = 744 + 72 = 816 MPa Remark: The plates that show the maximum stresses are not usable for the balanced fabrics. In effect, the compression strength values of a layer of balanced

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 90 Monday, November 18, 2002 12:09 PM

Table 5.4 Carbon/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Modulus Ex (MPa), Poisson ratio uxy and coefficient of thermal expansion ax as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

fabric are smaller than what is obtained when one superimposes the unidirectional 12 plies crossed at 0∞ and 90∞ in equal quantities in these two directions.

5.4.3 Case of Complex Loading—Approximate Orientation Distribution of a Laminate When the normal and tangential loadings are applied simultaneously onto the laminate, the previous tables are not valid because they were established for the 12

Also see remarks in Section 3.4.2.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 91 Monday, November 18, 2002 12:09 PM

Table 5.5 Carbon/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Shear modulus Gxy (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

cases of simple stress states. However, one can still use them to effectively obtain 13 a first estimate of the proportions of plies along the four orientations. The principle is as follows: Consider the case of complex loading and replacing the stresses with the stress resultants Nx, Ny, Txy which were defined in Section 5.2.4. In general these stress resultants constitute the initial numerical data that are given by some previous studies. One then can assume that each one of the three stress resultants is associated with an appropriate orientation of the plies following the remarks made in Section 5.2.2. 13

Attention: What follows is for the determination of proportions, and not thicknesses.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 92 Monday, November 18, 2002 12:09 PM

Table 5.6 Kevlar/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Maximum stress sxmax (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞,-45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

Using this hypothesis, Nx, assumed to be supported by the 0∞ plies (or along x), requires a thickness ex for these plies such that: Nx e x = -----------------s rupture where s rupture is the rupture stress of a unidirectional ply in the long direction. In the same manner, Ny is supposed to be supported by the 90∞ plies (or along y), and requires a thickness for these plies of Ny e y = -----------------s rupture

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 93 Monday, November 18, 2002 12:09 PM

Table 5.7 Kevlar/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Maximum stress symax (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

Finally, Txy is assumed to be supported by the ±45∞ plies and requires a thickness for these plies of T xy e xy = ------------t rupture where trupture is the maximum stress that a ±45∞ laminate can support.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 94 Monday, November 18, 2002 12:09 PM

Table 5.8 Kevlar/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Maximum stress txy max (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

One then can retain for the complete laminate the proportions indicated below.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 95 Monday, November 18, 2002 12:09 PM

Table 5.9 Kevlar/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Longitudinal modulus Ex (MPa), Poisson ratio uxy and coefficient of thermal expansion ax as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

Example: Determine the composition of a laminate made up of unidirectional plies of carbon/epoxy (Vf = 60%) to support the stress resultants Nx = -800 N/mm, Ny = -900 N/mm, Txy = -300 N/mm. The compression strength s rupture is 1,130 MPa (see Section 3.3.3, or Table 5.1 for 100% of 0∞ plies). Then: 800 900 e x = ------------ = 0.71 mm; e y = ------------ = 0.8 mm 1130 1130

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 96 Monday, November 18, 2002 12:09 PM

Table 5.10 Kevlar/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Shear modulus Gxy (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

The optimum shear strength trupture is given in Table 5.3 for 100% ±45∞, then:

trupture = 397 MPa from which: 340 e xy = --------- = 0.86 mm 397

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 97 Monday, November 18, 2002 12:09 PM

Table 5.11 0.13 mm

Glass/Epoxy Laminate: Vf = 60%, Ply Thickness =

Maximum stress s x max (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

One obtains for the proportions at ex - = 0.3 0∞: --------------------------e x + e y + e xy ey - = 0.34 90∞: --------------------------e x + e y + e xy e xy - = 0.36 ± 45∞: --------------------------e x + e y + e xy

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 98 Monday, November 18, 2002 12:09 PM

Table 5.12 0.13 mm

Glass/Epoxy Laminate: Vf = 60%, Ply Thickness =

Maximum stress sy max (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

One can then retain for the composition of the laminate the following approximate values:

Remark: The thicknesses ex, ey, exy evaluated above only serve to determine the proportions. After that, they should not be kept. In effect each orientation really

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 99 Monday, November 18, 2002 12:09 PM

Table 5.13 0.13 mm

Glass/Epoxy Laminate: Vf = 60%, Ply Thickness =

Maximum stress txy max (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

supports a part of each stress resultant. For example, the 0∞ plies cover the major part of stress resultant Nx, but they also support a part of stress resultant Ny and a part of stress resultant Txy. This then results in a more unfavorable situation for each orientation as compared with what has been assumed previously. The minimum necessary thickness of the laminate will in fact be larger than the previous result (ex + ey + exy ), which therefore appears to be dangerously optimistic. The practical determination of the minimum thickness of the laminate is determined based on the Hill–Tsai failure criterion, as indicated at the end of Section 5.3.2, and explained in details in Application 18.1.6. Also, with the same stress resultants and proportions as in the previous example, one finds a minimum thickness of 2.64 mm (see Application 18.1.6, in Chapter 18), whereas the previous sum (ex + ey + exy) gives a thickness of 2.37 mm, 10% lower than the required minimum thickness (2.64 mm).

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 100 Monday, November 18, 2002 12:09 PM

Table 5.14 Glass/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Longitudinal modulus Ex (MPa), Poisson ratio uxy , and coefficient of thermal expansion a x as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

5.4.4 Case of Complex Loading: Optimum Composition of a Laminate Estimation of the proportions in the previous paragraph does not lead to an optimum laminate in general. An optimum laminate is the one with the smallest thickness among all laminates of different compositions that can support the given combined stress resultants Nx, Ny, Txy. 14 Tables 5.15 through 5.19, based on Hill-Tsai criterion, give the optimum compositions of laminates based on unidirectionals of carbon/epoxy for the various 14

See Section 5.3.2.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 101 Monday, November 18, 2002 12:09 PM

Table 5.15 0.13 mm

Glass/Epoxy Laminates. Vf = 60%. Ply Thickness =

Shear modulus Gxy as a function of percentages of plies in directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply, see Section 3.3.3).

stress resultants Nx, Ny, Txy. The indicated compositions correspond to laminates that are capable of supporting the specified stress resultants and at the same time keeping a minimum thickness. One can see this number, in millimeters, within the circles, when the arithmetic sum of the stress resultants is equal to 100 N/mm. Also represented in the tables are The direction along which the first ply failure will occur. The multiplication factor for the stress resultants in order to go from first ply failure to ultimate fracture of the laminate. The two compositions that are closest to the optimum composition, obtained by varying the indicated composition along the direction of the arrows.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 102 Monday, November 18, 2002 12:09 PM

First, the arrows in increasing solid line or decreasing solid line denote the increase or decrease of 5% in terms of the proportions marked. Next, the arrows in increasing broken line or decreasing broken line denote the increase or decrease of 5% in terms of the proportions marked. Example: Given the stress resultants: Nx = 720 N/mm;

Ny = 0;

Txy = 80 N/mm

one can then deduce values of the reduced stress resultants: N x = 720/ ( 720 + 80 ) = 0.9;

N y = 0;

Txy = 80/ ( 720 + 80 ) = 0.1

One then uses Table 5.16 (all stress resultants are positive), where one can obtain for these values of reduced stress resultants the following figure:

This can be interpreted as follows: Optimal composition of the laminate 70% of 0∞ plies (along x direction) 10% of 90∞ plies 10% of plies in 45∞, 10% of plies in –45∞ Critical thickness of the laminate: 0.156 mm when the arithmetic sum of the 3 stress resultants is equal to 100 N/mm. For this thickness, the first ply failure occurs in the 90∞ plies. However, one can continue to load this laminate until it reaches 1.33 times the critical load, as: Nx = 1.33 ¥ 720 = 957 N/mm;

Ny = 0

Txy = 1.33 ¥ 80 = 106 N/mm At this point, there is complete rupture of the laminate. Returning to our example, the arithmetic sum of the stress resultants is equal to 720 + 80 = 800 N/mm. Then, the thickness of the laminate has to be more than: 8 ¥ 0.156 = 1.25 mm Neighboring compositions: The second smallest thickness in the vicinity is obtained by modifying the indicated composition in the direction specified by the arrows in solid line, as

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 103 Monday, November 18, 2002 12:09 PM

Table 5.16 Optimum Composition of a Carbon/Epoxy Laminate

Vf = 0.6, 10% minimum in each direction of 0∞, 90∞, +45∞, -45∞. (Ply characteristics: see Appendix 1 or Section 3.3.3).

One then obtains (not shown on the plate) a thickness of 0.160 mm (increase of 2.5% relative to the previous value) and a multiplication factor for the loading equal to 1.35. Continuing in the direction of increasing thickness, the third smallest thickness in the immediate vicinity is obtained by modifying the indicated composition in the direction specified by the arrows in broken line, as:

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 104 Monday, November 18, 2002 12:09 PM

Table 5.17 Optimum Composition of a Carbon/Epoxy Laminate

Vf = 0.6, 10% minimum in each direction of 0∞, 90∞, +45∞, -45∞. (Ply characteristics: see Appendix 1 or Section 3.3.3).

One then obtains a thickness (not shown on the plate) of 0.165 mm (increase of 6%) and a multiplication factor of 1.3 for the load. Example: Given the stress resultants Nx = 600 N/mm; Ny = -300 N /mm; Txy = 100 N/mm The corresponding reduced stress resultants are N x = .6; N y = – .3 ; T xy = 0.1 N/mm One obtains from Table 5.18:

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 105 Monday, November 18, 2002 12:09 PM

Table 5.18 Optimum Composition of a Carbon/Epoxy Laminate

Vf = 0.6, 10% minimum in each direction of 0∞, 90∞, +45∞, -45∞. (Ply characteristics: see Appendix 1 or Section 3.3.3).

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 106 Monday, November 18, 2002 12:09 PM

Table 5.19 Optimum Composition of a Carbon/Epoxy Laminate

Vf = 0.6, 10% minimum in each direction of 0∞, 90∞, +45∞, -45∞. (Ply characteristics: see Appendix 1 or Section 3.3.3).

where Critical thickness is 10 ¥ 0.152 = 1.52 mm These are the 90∞ plies that fail first. Complete rupture of the laminate occurs when: Nx = 1.29 ¥ 600 = 774 N/mm Ny = 1.29 ¥ -300 = -387 N/mm Txy = 1.29 ¥ 100 = 129 N/mm

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 107 Monday, November 18, 2002 12:09 PM

The closest critical thicknesses (in increasing order) are obtained with the following successive compositions:

Remarks: A few loading cases can lead to several distinct optimum compositions, but with identical thicknesses. For example the reduced stress resultants: N x = N y = 0.5; T xy = 0 This is a case of isotropic loading, the Mohr circle is reduced to one point (see figure below).

Table 5.16 indicates

One obtains in this case a unique critical thickness of 0.161 mm (corresponding 15 to a sum Nx + Ny = 100 N/mm) independent of the proportion p. The isotropic composition (25%, 25%, 25%, 25%) in the directions 0∞, 90∞, +45∞, –45∞, which appears intuitive, can in fact be replaced by compositions that present the values of modulus of elasticity that are varied and adaptable to the designer in the 16 directions 0∞, 90∞ 45∞, or -45∞, or even a, a + p /2 with a certain a. 15 16

See Section 18.2.8. See Section 5.4.2, Table 5.4.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 108 Monday, November 18, 2002 12:09 PM

In some loading cases, one finds from the table only arrows in a solid line. For example, for the following reduced stress resultants: N x = 0.3;

N y = 0;

T xy = 0.7

one finds from Table 5.16 the following figure:

The three neighboring optimum compositions in increasing order are

(The thicknesses of 0.255 mm and 0.262 mm are not indicated on the plate). The third composition, characterized by an increase in thickness of 0.252 to 0.262 mm, or 6%, leads to an increase in modulus of elasticity in the x (0∞) by 36% (see Section 5.4.2, Table 5.4). One can note finally that for the majority of cases, the optimum compositions 17 indicated in Tables 5.16 to 5.19 are not easy to postulate using intuition.

5.4.5 Practical Remarks: Particularities of the Behavior of Laminates 18

The fabrics are able to cover the left surfaces due to pushing action in warp and fill directions. The radii of the mold must not be too small. This concerns particularly the inner radius Ri as shown in Figure 5.24. The graph gives an idea for the minimum value required for the inner and outer radii. The thickness of a polymerized ply is not more than 0.8 to 0.85 times that of a ply before polymerization. This value of the final thickness must also take into account a margin of uncertainty on the order of 15%. When one unidirectional sheet does not cover the whole surface required to constitute a ply, it is necessary to take precautions when cutting the different pieces of the sheet. A few examples of wrapping are given in Figure 5.25. The unidirectional sheets do not fit well into sharp corners in the fiber direction. The schematic in Figure 5.26 shows the dispositions to accommodate sudden changes in draping directions. 17 18

See Exercise 18.1.6. It is more difficult for the plain weave than for the satins, due to the mode of weaving (See Section 3.4.1).

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 109 Monday, November 18, 2002 12:09 PM

Figure 5.24 Minimum Required for Inner and Outer Radii of Mold

Figure 5.25 Recommended Arrangement for Cutting

Figure 5.26 Method to Lay up at Corner

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 110 Monday, November 18, 2002 12:09 PM

Figure 5.27 Corner Situations

Figure 5.28a Three Plies in Separate Positions

Delaminations: When the plies making up the laminate separate from each other, it is called delamination. Many causes are susceptible to provoke this deterioration: An impact that does not leave apparent traces on the surface and can lead to internal delaminations. A mode of loading leads to the disbond of the plies (tension over the interface) as shown in Figure 5.27. Shear stresses at the interfaces between different plies, very near the edges of the laminates, which one can make evident as follows (with a three-ply laminate): 1. Consider the three plies in Figure 5.28(a), separated. Under the effect of loading (right-hand-side figure), they are deformed independently and do not fit with each other when they are put together. 2. Now the plies constitute a balanced laminate. Under the same loading, they deform together, without distorsion, as shown in Figure 5.28(b). 3. This is because interlaminar stresses occur on the bonded faces. One can show that these stresses are located very close to the edges of the laminate, as illustrated in Figure 5.28(c).

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 111 Monday, November 18, 2002 12:09 PM

Figure 5.28b Three Plies, Together

Figure 5.28c Stresses at Free Edge

A complex state of stresses at the interface, due to local buckling, for example (see Figure 5.29). Practical as well as theoretical studies of these interlaminar stresses are difficult, and the phenomenon is still not well understood.

Why is Fatigue Resistance so Good? Paradox: Glass is a very brittle material (no plastic deformation). The resin is also often a brittle material. (for example, epoxy). However, the association of reinforcement/matrix constituted of these two materials opposes to the propagation of cracks and makes the resultant composite to endure fatigue remarkably. Explanation: When the cracks propagate, for example, in the unidirectional layer shown schematically in Figure 5.30 in the form of alternating of fibers and

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 112 Monday, November 18, 2002 12:09 PM

Figure 5.29 Delamination Due to Buckling at Interface

Figure 5.30 Crack Propagation in Composites

resin, the initial stress concentration at the end of the crack leads to failure in the resin. The fibers, then debonded, benefit from a relaxation of the stresses. There is no more stress concentrations as in a homogeneous material. Laminated tubes can be obtained by winding of filaments, rubans of unidi19 rectionals or fabrics. In a first approximation, one can estimate the strains and stresses in flexure and in torsion from the relations in Figure 5.31 in which Ex and Gxy are the moduli of elasticity in the tangent plane x,y. I and Io are respectively the quadratic moment of inertia and polar moment of inertia (Io = 2I). Y is the coordinate of a point in the section (in the undeformed position) in the X, Y, Z coordinates. r is the average radius of the tube.

19

For a complete study of the flexure and torsion of the composite beams, See Section 15 and 16.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 113 Monday, November 18, 2002 12:09 PM

Figure 5.31 Composite Tube Relations

© 2003 by CRC Press LLC

6 JOINING AND ASSEMBLY We have seen previously how to design a laminate to support loads. A second fundamental aspect of the design of a composite piece consists of the design for the attachment of the composite to the rest of the structure. Here we will examine the assembly problems involving riveting, bolting, and bonding: of a composite part to another composite part and of a composite part to a metallic part.

6.1 RIVETING AND BOLTING In all mechanical components, the introduction of holes gives stress concentration factors. Specifically in composite pieces, the introduction of holes (for molded-in holes or holes made by drilling) induces weakening of the fracture resistance in comparison with the region without holes by a factor of 40 to 60% in tension 15% in compression Example: Figure 6.1 presents the process of degradation before rupture of a glass/epoxy laminate containing a free hole, under uniaxial stress. Causes of hole degradation: Stress concentration factors: The equilibrium diagrams shown in Figure 6.2 demonstrate the increase in stress concentration in the case of a laminate. For the case of slight (and usually neglected) press-fit of the rivet, the stresses shown in these figures are:

s ¢M > s in a region where:

slocal rupture < slaminate rupture

© 2003 by CRC Press LLC

Figure 6.1 Cracks in a Laminate with Hole when Load Increases

Figure 6.2 Stress Concentration Factors

with the maximum stress s ¢M in the laminate given as: Ï E ¸ E sM¢ = s ¢ ¥ Ì 1 + 2 ÊË -----x – n xyˆ¯ + -------x- ˝ G E xy ˛ y Ó where

Ex and Ey are the moduli of elasticity in the 0∞ and 90∞ directions Gxy is the shear modulus nxy is the Poisson ratio

© 2003 by CRC Press LLC

Figure 6.3 Weakened Zones Due to Presence of Holes

Bearing due to lateral pressure: This is the contact pressure between the shaft of the assembly device (rivet or bolt) and the wall of the hole. When this pressure is excessive, it leads to mushrooming and delamination of the laminate. In consequence: The resistance of a hole occupied by the rivet or bolt is weaker than that of an empty hole: decrease on order of 40%). Fracture of fibers during the hole cutting process, or the misalignment of fibers if the hole is made before polymerization: Figure 6.3 illustrates the correlation between the weakened zones consecutive to rupture of fibers and the “overstressed” zones.

6.1.1 Principal Modes of Failure in Bolted Joints for Composite Materials These are represented in Figure 6.4.

6.1.2 Recommended Values Pitch, edge distance, thickness (see Figure 6.5) Orientation of plies: Recommendation for percentages of plies near the holes (see Figure 6.6). © 2003 by CRC Press LLC

Figure 6.4

Different Types of Bolt Joint Failures

Condition of nonbearing pressure: In Figure 6.7, F and T designate the normal and shear loads respectively, that are applied on the assembly over a width equal to one pitch distance. The equivalent bearing pressure which leads to the crushing of the wall of the hole of diameter Ø, is F/(Ø ¥ e). It must remain smaller than an admissible maximum, as: F ------ £ s carbon: s admissible bearing = 500 MPa f e admissible bearing pressure glass: t admissible bearing = 300 MPa © 2003 by CRC Press LLC

Figure 6.5 Recommended Pitch, Edge Distance, and Thickness

Figure 6.6 Recommended Orientation

Figure 6.7 Normal and Shear Loads on Assembly

Evaluation of the admissible stresses: The principle of calculation consists of magnifying the stresses that are given by elementary considerations, 1 by means of the empirical coefficients of magnification : 1

When one takes into account the aging of the piece, an additional 10% is applied to the maximum stresses.

© 2003 by CRC Press LLC

Due to the presence of the hole and Due to pressure of contact or bearing on the wall of the hole (rivet, bolt). With the notations of Figure 6.7, one has: F 1 F s magnified = --- ÊË --- + 0.2 ------ˆ¯ a S fe tension: a = 0.6 compression: a = 0.8 1 T t magnified = ------- --0.7 S One must also verify that these stresses are admissible (that is, they do not lead to the fracture of the ply) by using the method of verification of fracture described in Paragraph 5.3.2.

6.1.3 Riveting The relative specifics and recommendations for riveting the composite parts can be presented as follows: Do not hit the rivets as this can lead to poor resistance to impact of the laminates. Pay attention to the risk of “bolt lifting” of the bolt heads due to small thickness of the laminates. Note the necessity to assure the galvanic compatibility between the rivet and the laminates to be assembled. Riveting accompanied by bonding of the surfaces to be assembled provides a gain in the mechanical resistance on the order of 20 to 30%. On the other hand, the disassembly of the joint becomes impossible, and the weight is increased. Characteristics of rivets for composites are shown in Figure 6.8.

6.1.4 Bolting Examine a current example that requires a bolted joint. 2

Example: Junction of a panel by bolted joint (simple case) : Consider a sandwich panel fixed to a support component that is subjected to simple loadings that can be represented by a shear load and a bending moment (see Figure 6.9). One expects an attachment using bolt. As shown in the schematics of Figure 6.10, even if the bolt is not tightened, it is able to act to equilibrate the bending moment. However, action of the shear load will separate the facings. 2

A more complete case on the fixation of the panel is examined in the application in Paragraph 18.1.6.

© 2003 by CRC Press LLC

Figure 6.8 Different Types of Riveting

Figure 6.9 Junction of a Panel using Bolted Joint

© 2003 by CRC Press LLC

Figure 6.10 Local behavior without Bolt Tightening

Figure 6.11 Bolt tightening Reduces the Possibility of Damage

It is the tightening of the bolt that will lead to a distribution of contact pressure between the support component and the facings. The sum of the forces due to this contact pressure will balance out the shear load, while suppressing the risk of separating the facings (see Figure 6.11). The tightening of the bolt is therefore indispensable. However, the laminated facings being fragile cannot admit high contact pressures that are localized under the bolt head and under the nut. This leads to the insertion of metallic washers as shown in Figure 6.12. The bolting accompanied by bonding of the surfaces provides a gain in mechanical resistance on the order of 20 to 30%. On the other hand, the joint cannot be disassembled, and there is an increase in weight.

6.2 BONDING Remember briefly that this assembly technique consists of the adhesion by molecular attraction between two parties to be bonded and an adhesive that must be able to transfer the loads. One can cite the principal advantages of this mode of joining: © 2003 by CRC Press LLC

Figure 6.12 Configuration for Bolted Joints

Figure 6.13 Curing of Adhesive

distribution of stresses over an important surface possibility to optimize the geometry and dimensions of bonding light weight of the assembly insulation and sealing properties of adhesive

6.2.1 Adhesives Used The adhesives used include:

epoxies polyesters polyurethanes methacrylates

In all cases, the mechanism of curing is shown schematically in Figure 6.13. The adhesives are resistand simultaneously to high temperatures (>180∞C) humidity a number of chemical agents © 2003 by CRC Press LLC

Figure 6.14 Stresses in Bolted Joint

Figure 6.15 Fracture Modes in a Bonded Joint

The pieces to be assembled have to be surface treated. This consists of three steps: degreasing surface cleaning protection of cleaned surface The case of metal–laminate bond: The differences in physical properties of the constituents requires that the adhesive must compensate for the differences in thermal dilatations elongation under stress The schematic in Figure 6.14 indicates in an exaggerated manner the deformed configuration of a double bonded joint. This shows the role of the adhesive and the gradual transmission of the load from the central piece to the external support. Fracture of a bonded assembly can take dif ferent forms, as indicated in Figure 6.15.

6.2.2 Geometry of the Bonded Joints One must, as much as possible, envisage the joint geometries that allow the following specifications: the adhesive joint must work in shear in its plane tensile stresses in the joint must be avoided Consequently, the transmission of the loads will be dependent on the geometries, as shown in Figure 6.16. A double sided joint with increasing thickness is shown in Figure 6.17. Transmission of couples is shown in Figure 6.18. © 2003 by CRC Press LLC

Figure 6.16 Different Designs for Bonded Joints

Figure 6.17 Double Sided Lap Joint

6.2.3 Sizing of Bonded Surfaces The resistance of the adhesive is characterized by its shear strength trupture. This resistance varies with the process of bonding (cold bonding or hot bonding). For epoxy adhesive, one can cite the following values: Cold bonding: (Araldite): Adhesive thickness = 0.2 mm

trupture = 10 MPa at 20∞C = 3 MPa at 80∞C © 2003 by CRC Press LLC

Figure 6.18 Design for the Transmission of Couples

Figure 6.19 Curing Cycle of Epoxy Adhesive

Hot bonding: Polymerization temperature is between 120∞C and 180∞C:

t rupture = 15 to 30 MPa from 20∞C to 100∞C The diagram in Figure 6.19 shows, for example, the cycle of polymerization of an epoxy adhesive “REDUX 914.” Denoting ec for the thickness of the adhesive joint, one has for an order of magnitude: 0.1 mm £ ec £ 0.3 mm when the joints are very thick, one adds adhesive glass powder or cut fibers. © 2003 by CRC Press LLC

Figure 6.20 Scarf Joint

Figure 6.21 Configurations of Parallel Joint

Figure 6.22 Stresses in Adhesive

Scarf joint: This joint (see Figure 6.20) allows one to obtain a sufficient bonding surface, with weak tensile stress. Parallel joint: As illustrated in Section 6.2.2, there is bending in the bonded parts. The geometric configurations are varied (see Figure 6.21). When one isolates the bonded zone, the stress variation is shown in the figure on the right-hand side of Figure 6.22 (the bond width is assumed to be equal to unity) The stresses in the adhesive (Figure 6.22) consists essentially of a shear stress t and a normal stress called “peel stress” s. © 2003 by CRC Press LLC

Figure 6.23 Maximum Shear Stress

These stresses present maximum values sM and tM very close to the edges of the adhesive. These maxima can be approached by superposition of the partial maxima created by each of the resultants N, T, Mf, by means of the following expressions in which Ec is the modulus of the adhesive, and E1 and E2 are the moduli along the horizontal direction of the bonded parts 1 and 2. One can also write: Gc -; a 1 = -------------E1 e1 ec

Gc -; a 2 = -------------E2 e2 ec

12E c -; b 1 = -------------3 E1 e1 ec

12E c b 2 = -------------3 E2 e2 ec

Maximum shear stresses are illustrated in Figure 6.23 Maximum peel stress is shown in Figure 6.24.

Remarks: The resultants N, T, Mf are evaluated per unit width of the bond. When several resultants coexist, one obtains the total maximum shear stress by superposition of the partial maxima of shear stresses and the maximum peel stress by superposition of the partial maxima of peel stresses. When the lower piece is also subjected to the resultants, the previously obtained relations are usable, by means of permuting the indices 1 and 2, and by changing the sign of the second member © 2003 by CRC Press LLC

Figure 6.24 Maximum Peel Stress 3

Limits for the relations

a b 0.6 £ -----1 and -----1 £ 2 a2 b2 ( a1 + a2 ) ¥ ≥ 9 2

( b1 + b2 ) ¥ ≥ 4 ¥ 6 4

4

Example: For the simple lap joint below, one has (with the notations used previously)

e1 + e2 - + e cˆ N = F ; M f = F ¥ Ê -------------Ë 2 ¯

t M = t M( N ) + t M( M ) ; s M = s M( M ) f

f

This is valuable if a1, a2, b1, b2 respect the limits of utilization written above. Collar (see Figure 6.25) 4 Cylindrical sleeve (see Figure 6.26)

3

4

For more details, see Bibliography: “Elastic Analysis and Engineering Design Formulae for Bonded Joints.” For different thicknesses and different materials to be assembled, see Exercise 18.3.1.

© 2003 by CRC Press LLC

Figure 6.25 Shear Stresses in Simple Collar

Figure 6.26 Shear Stresses in Cylindrical Sleeve

Figure 6.27 Ply Orientation in Bonded Laminates

In a laminate, orientation of the plies that are in contact with the joint influences strongly the failure by fiber–resin decohesion. This can be easily understood through Figure 6.27. A tensile load in plies that are in contact with the adhesive requires that fiber orientation in these plies must be along the direction of the load. © 2003 by CRC Press LLC

Figure 6.28 An example of Laminate Bonding

Figure 6.29 Bonding of Sandwich Facings

6.2.4 Examples of Bonding Laminates One notes in Figure 6.28 the use of steps that gradually decrease the thickness of titanium piece. Note also that the design allows one to separate the str ess concentration effects localized at the beginning of each step. Sandwiches (see Figure 6.29) The bonding at the borders of sandwich panels must be done in a simple manner (especially for the preparation of the core) and with the best possible contact for the bonded parts, similar to the cases shown in Figure 6.30.

6.3 INSERTS It seems necessary to include in composite parts reinforcement pieces, or “inserts,” which may be used to attach to the surrounding structure. The inserts decrease the transmitted stresses to admissible values for the composite part. The case of sandwich pieces: One frequently finds the metallic inserts following the schematics in Figure 6.31. © 2003 by CRC Press LLC

Figure 6.30 Different Sandwich Facing Designs

Figure 6.31 Inserts in Sandwich Construction

The case of pieces under uniaxial loads: Tensile load (see Figure 6.32) Compression load (see Figure 6.33) Tension–compression load (see Figure 6.34) Arrangement that allows the increase of the bonded surfaces is shown in Figure 6.35.

© 2003 by CRC Press LLC

Figure 6.32 Composite Piece Under Tensile Load

Figure 6.33 Composite Piece under Compression Load

Figure 6.34 Composite Piece under Tension-compression Load

Figure 6.35 Arrangement to Increase Bond Surface

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 135 Monday, November 18, 2002 12:17 PM

7 COMPOSITE MATERIALS AND AEROSPACE CONSTRUCTION Aeronautical constructors have been looking for light weight and robustness from composites since the earlier times. As a brief history: In 1938, the Morane 406 plane (FRA) utilized sandwich panels with wood core covered with light alloy skins. In 1943, composites made of hemp fiber and phenolic resin were used on the Spitfire (U.K.) airplane. Glass/resin has been used since 1950, with honeycombs. This allows the construction of the fairings with complex forms. Boron/epoxy was introduced around 1960, with moderate development since that time. Carbon/epoxy has been used since 1970. Kevlar/epoxy has been used since 1972. Experiences have proved that the use of composites allows one to obtain weight reduction varying from 10% to 50%, with equal performance, together with a cost reduction of 10% to 20%, compared with making the same piece with conventional metallic materials.

7.1 AIRCRAFT 7.1.1 Composite Components in Aircraft Currently a large variety of composite components are used in aircrafts. Following the more or less important role that composites play to assure the integrity of the aircraft, one can cite the following: Primary structure components (integrity of which is vital for the aircraft): © 2003 by CRC Press LLC

TX846_Frame_C07 Page 136 Monday, November 18, 2002 12:17 PM

Wing box Empennage box Fuselage The control components: Ailerons Control components for direction and elevation High lift devices Spoilers Exterior components: Fairings “Karmans” Storage room doors Landing gear trap doors Radomes, front cauls Interior components: Floors Partitions, bulkheads Doors, etc. Example: The vertical stabilizer of the Tristar transporter (Lockheed Company, USA) With classical construction, it consists of 175 elements assembled by 40,000 rivets. With composite construction, it consists only with 18 elements assembled by 5,000 rivets.

7.1.2 Characteristics of Composites One can indicate the qualities and weak points of the principal composites used. These serve to justify their use in the corresponding components.

7.1.2.1 Glass/Epoxy, Kevlar/Epoxy These are used in fairings, storage room doors, landing gear trap doors, karmans, radomes, front cauls, leading edges, floors, and passenger compartments. Pluses: 1 High rupture strength Very good fatigue resistance Minuses: High elastic elongation Maximum operating temperature around 80∞C Nonconducting material 1

See Section 3.3.3.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 137 Monday, November 18, 2002 12:17 PM

7.1.2.2 Carbon/Epoxy This is used in wing box, horizontal stabilizers, fuselage, ailerons, wings, spoilers (air brakes) vertical stabilizers, traps, and struts. Pluses: High rupture resistance Very good fatigue strength Very good heat and electricity conductor High operating temperature (limited by the resin) No dilatation until 600∞C Smaller specific mass than that of glass/epoxy Minuses: More delicate fabrication Impact resistance two or three times less than that of glass/epoxy Material susceptible to lightning

7.1.2.3 Boron/Epoxy This is used for vertical stabilizer boxes and horizontal stabilizer boxes. Pluses: High rupture resistance High rigidity Very good compatibility with epoxy resins Good fatigue resistance Minuses: 2 Higher density than previous composites Delicate fabrication and forming High cost

7.1.2.4 Honeycombs Honeycombs are used for forming the core of components made of sandwich structures. Pluses: Low specific mass Very high specific modulus and specific strength Very good fatigue resistance Minuses: Susceptible to corrosion Difficult to detect defects

2

See Section 3.3.3.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 138 Monday, November 18, 2002 12:17 PM

7.1.3 A Few Remarks The construction using only glass fibers is less and less favored in comparison with a combination of Kevlar fi bers and carbon fibers for weight saving reasons:

If one would like to have maximum strength, use Kevlar. If one would like to have maximum rigidity, use carbon. Kevlar fibers possess excellent vibration damping resistance. Due to bird impacts, freezing rain, impact from other particles (sand, dirt), one usually avoids the use of composites in the leading edges without 3 metallic protection.

Carbon/epoxy composite is a good electrical conductor and susceptible to lightning, with the following consequences: Damages at the point of impact: delamination, burning of resin Risk of lightning in attachments (bolts) The necessity to conduct to the mass for the electrical circuits situated under the composite element Remedies consist of the following: Glass fabric in conjunction with a very thin sheet of aluminum (20 mm) The use of a protective aluminum film (aluminum flam spray) Temperature is an important parameter that limits the usage of epoxy resins. A few experimental components have been made of bismaleimide resins (ther4 mosets that soften at temperatures higher than 350 ∞C rather than 210 ∞C for epoxies). One other remedy would be to use a thermoplastic resin with high 5 temperature resistance such as poly-ether-ether-ketone “peek” that softens at 380∞C. Laminates made of carbon/peek are more expensive than products made of carbon/epoxy. However, they present good performance at higher operating temperatures (continuously at 130∞C and periodically at 160 ∞C) and have the following additional advantages: Superior impact resistance Negligible moisture absorption Very low smoke generation in case of fire

3

4

5

The impacts can create internal damages that are invisible from the outside. This can also happen on the wing panels (for example, drop of tools on the panels during fabrication or during maintenance work). The mechanical properties of the thermoset resins diminish when the temperature reaches the “glass transition temperature.” See Section 1.6 for the physical properties.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 139 Monday, November 18, 2002 12:17 PM

Figure 7.1 Temperature Cycle and Load Cycle for Components of an Aircraft

7.1.4 Specific Aspects of Structural Resistance One must apply to composite components the technique called fail safe in aerodynamics, which consists of foreseeing the mode of rupture (delamination, for example) and acting in such a manner that this does not lead to the destruction of the component during the period between inspections. Composite components are repairable. Methods of reparation are analogous to 6 those for laminates made of unidirectionals or fabrics. Considering the very important reduction of the number of rivets used as compared with the conventional construction, one obtains a smother surface, which can lead to better aerodynamic performance. One also considers that the attack of the environment and the cycles of fatigue over the years do not lead to significant deterioration of the composite pieces (shown in Figure 7.1 are two types of fatigue cycles for the components of aircraft structure). The failure aspect subject to a moderate impact is more problematic with the structures made of composite materials, because the energy absorbed by plastic deformation does not exist. For the cabins, one uses phenolic resins. These have good fire resistance, with low smoke emission. For the same reason, one prefers replacing Kevlar fibers with a combination of glass/carbon (lighter than glass alone and less expensive than carbon alone). It is possible to benefit from anisotropy of the laminates for the control 7 of dynamic and aeroelastic behavior of the wing structures.

7.1.5 Large Carriers The following examples give an idea on the evolution of use of composites in aircrafts over two decades: Example: Aerospatiale (FRA); Airbus Industry (EU) (Figure 7.2) Example: Boeing (USA) (Figure 7.3) 6 7

See Section 4.4.4. See Section 7.1.8.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 140 Monday, November 18, 2002 12:17 PM

Figure 7.2 Evolution of Mass of Composites in Aircraft

Figure 7.3 Use of Composite in Boeing Aircraft

How to evaluate the gains: In theory: For example, a study was made by Lockheed Company (USA) for the design of a large carrier having the following principal characteristics: payload 68 tons, range 8300 km. This study gives the following significant results: for an aircraft made using conventional metallic construction: total mass at take-off: 363 tons mass of the structure: 175 tons for an aircraft made using “maximum” composite construction: total mass at take-off: 245 tons mass of the structure: 96 tons. Such a difference can be explained by the cascading consequences that can be illustrated as in Figure 7.4. In practice: In reality, introduction of composites in the aircrafts is limited to certain parts of the structures. It is done case by case and in a progressive manner during the life of the aircraft (re-evaluation operation). One is then led to consider the different notions: © 2003 by CRC Press LLC

TX846_Frame_C07 Page 141 Monday, November 18, 2002 12:17 PM

Figure 7.4 Cascading Effect in Mass Reduction

Notion of the exchange rate is the cost for a kilogram saved when one substitutes a classical metallic piece with a piece made mainly with composite. For the substitution light alloy—carbon/epoxy—this cost is on the order of $160 (1984) per kilogram when the piece is calculated in terms of rigidity (similar deformation for the same load). It is amortized over a period of at least one year for the gain in “paying passenger.” Notion of gain in paying passenger is the gain in terms of the number of passengers, of freight, or in fuel cost; for example, for a large carrier: An aircraft of 150 tons, with 250 passengers consists of 60 tons of structure. A progressive introduction of 1600 kg of high performance composite materials leads to a gain of 16 more passengers along with their luggage. A reduction of 1 kg mass leads to the reduction of fuel consumption of around 120 liters per year. Why are the reductions of mass (average about 20%) not more spectacular? Consider the example of a vertical stabilizer. The distribution of mass of a composite vertical stabilizer can be presented as follows:

Facings in carbon/epoxy: 30% of total mass Honeycombs, adhesives: 35% of total mass Attachments: 25% of total mass Connections between carbon/epoxy components and attachments: overlayers of carbon/epoxy Allowance for the aging of the carbon/epoxy: overdimensions of the facings (the stresses are magnified about 10% more for a subsonic aircraft and 13% for a supersonic aircraft) In consequence, the global gain of mass in comparison with a classical metallic construction for the vertical stabilizer is not more than an order of about 15%. Example: European aircraft Airbus A-310–300 (Figure 7.5). © 2003 by CRC Press LLC

TX846_Frame_C07 Page 142 Monday, November 18, 2002 12:17 PM

Figure 7.5 Composite Components in an Airbus A-310

Total mass: 180 tons Mass of structure: 44.7 tons Mass of composites: 6.2 tons Mass of high performance composites: 1.1 tons Reduction of mass of structure: 1.4 tons Percentage of composites: 13.8% of mass of structure. A reduction of mass of the structure of 1 kg augments the range of the aircraft by 1 nautical mile.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 143 Monday, November 18, 2002 12:17 PM

Figure 7.6 Composite Components in an Airbus A-320

Example: European aircraft Airbus A-320 (Figure 7.6).

Total mass: 72 tons Empty mass: 40 tons Mass of structure: 21 tons Mass of composite materials: 4.5 tons, corresponding to a reduction of mass of the structure of 1.1 tons. The percent of composite mass is 21.5% of the mass of the structure. A few other characteristics: Length: 37.6 m; breadth: 34 m; 150 to 176 passengers transported from 3,500 to 5,500 km; maximum cruising speed: 868 km/h Example: European aircraft Airbus A-340 Total mass: 253.5 tons Mass of structure: 76 tons Mass of composites: 11 tons, corresponding to a reduction of structure mass of 3 tons Percentage of composites: 14.5% of the mass of the structure Example: Future supersonic aircraft ATSF (Figure 7.7), Aerospatiale (FRA) and British Aerospace (UK). Principal characteristics defined at the stage before the project Transport of 200 passengers over a distance of 12,000 km Cruising speed between Mach 2 (2,200 km/hr) and Mach 2.4 (2,600 km/hr) © 2003 by CRC Press LLC

TX846_Frame_C07 Page 144 Monday, November 18, 2002 12:17 PM

Figure 7.7 Composite Components in a Future Supersonic Aircraft

Economically viable for a single type of aircraft on the market (enlarged international cooperation)

7.1.6 Regional Jets Example: Regional transport aircraft ATR 72, ATR (FRA–ITA) (Figure 7.8): Total mass: 20 tons Percentage of composite materials more than 25% of the mass of the structure Transports 66 passengers over a distance of 2,600 kilometers Interior equipment: Facings of panels for portholes and ceiling, baggage compartment, bulkheads, toilets, storing armors in glass-carbon/phenolic resins/NOMEX honeycomb; decoration by a film of “TEDLAR” © 2003 by CRC Press LLC

TX846_Frame_C07 Page 145 Monday, November 18, 2002 12:17 PM

Figure 7.8 Composite Components in the Regional Transport Aircraft ATR 72

Figure 7.9 Business Aircraft Falcon 10

Example: Business aircraft Falcon 10 (Figure 7.9). Aircrafts (AMD–BA) (FRA). The principal wing box (primary structure) is constructed in ribbed panels of carbon/epoxy; it has been flying experimentally since 1985. Mass of wing box: 339 kg Reduction of mass in comparison with conventional metallic construction: 80 kg (20%) The connection between the wing and the fuselage and the attachment between the landing gears and the wing box are made using metallic pieces. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 146 Monday, November 18, 2002 12:17 PM

Figure 7.10 Propulsive Propeller Configuration

7.1.7

Light Aircraft

These are the aircrafts for tourism and for the gliders. The new generation of these aircrafts is characterized by A large utilization of composites A renewal in aerodynamic solutions Remarks: In addition to the problems to be resolved by the manufacturers (small manufacturers for the most part), comes the preparation of the dossiers of certification including composite primary structures. The useful reduction of masses, the range of flight, and the cruising speed, due to the utilization of composites, are amplified more clearly in these types of aircrafts. Example: Back propeller aircraft. The principle of this is illustrated in Figure 7.10, with the advantages and drawbacks. The modification of the mass distribution, due to the displacement of the motor, requires a propeller shaft (foreseen to be in carbon/epoxy) and a wing shifted to the back. One can propose the “all composite” solution as follows: The solution “long shaft.” Sup’air airplane Centrair (FRA); Figure 7.11 The solution of shifted wing and additional duck wing: Beech Starship aircraft (USA); Figure 7.12: Eight to ten passengers: 650 km/hr with low fuel consumption Structure in carbon/epoxy Mass of the wings: 800 kg (reduction of 35% in comparison with a metallic solution) Mass of fuselage (structure): 240 kg Mass of the composite: about 70% of the mass of the structure © 2003 by CRC Press LLC

TX846_Frame_C07 Page 147 Monday, November 18, 2002 12:17 PM

Figure 7.11 An All-composite Airplane

Figure 7.12 Beech Starship Aircraft

Example: The modern glider planes. These are made entirely of composites. Figure 7.13 shows a plane made of glass/epoxy: Two-seater glider plane: Marianne Centrair (FRA): Mass: 440 kg © 2003 by CRC Press LLC

TX846_Frame_C07 Page 148 Monday, November 18, 2002 12:17 PM

Figure 7.13 The Marianne Centrair Airplane

Wings: 2 parts bonded Fuselage: 2 parts bonded

7.1.8 Fighter Aircraft For this type of aircraft, there is a progressive replacement of metallic elements by composite elements. Beyond specific characteristics already mentioned previously for the large aircrafts, here the composite components have to assure the necessary rigidity for the wing box to conserve the ability of command in a domain of flight larger than for the case of large civil aircrafts. For the flight with electrical commands, the use of composites allows for an evolution of the aerodynamic design for better maneuverability. In the near future, 25 to 40% of the structure of the fighter aircrafts will be made of composite materials. Example: European airplane Alphajet (Figure 7.14). Example: Airplane Mirage 2000 A.M.D.–B.A. (FRA; Figure 7.15). Mass of composite materials: 65 kg (On this aircraft there are boron/epoxy composite components.) Characteristics of boron: The diameter of the fiber varies between 0.1 mm and 0.2 mm depending on the demand of the customer. The radius of curvature, in fact, cannot be less than 4 or 5 mm. One finds for the sheets: width is 1 m, 80 filaments/cm, length: 3.5 m. 8 for the fabrics: patented process; the warp direction consists of textile filaments, the fill direction consists of boron filaments. Example: Airplane F-18 Hornet, M.D. Douglas/Northrop (USA; Figure 7.16). Example: Airplane X-29 Grumman (USA; Figure 7.17). Example: Airplane Rafale A.M.D.–B.A. (FRA; Figure 7.18). Note that on this airplane there is a very large usage of high performance composites (carbon/ epoxy and Kevlar/epoxy). Mass of composite materials is 1,110 kg, leading to a 9 25% reduction in the mass of the structure. Figure 7.18 shows the main components using composites. 8 9

Patent Avions M. Dassault-Bréguet Aviation/Brochier. This is to compare with the number for Mirage 2000 airplane presented previously.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 149 Monday, November 18, 2002 12:17 PM

Figure 7.14 Alphajet Plane

Figure 7.15 Mirage Airplane

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 150 Monday, November 18, 2002 12:17 PM

Figure 7.16 F-18 Hornet Airplane

Figure 7.17 X-29 Grumman Airplane

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 151 Monday, November 18, 2002 12:17 PM

Figure 7.18 Rafale Airplane

7.1.9 Architecture of Composite Parts in Aircraft 7.1.9.1 Sandwich Design Sandwich with transverse honeycomb: Following the nature of the component, one uses two methods of fabrication: Multisteps in which the facings of the sandwich piece are polymerized separately and then are placed on the core having an adhesive film. After that the assembly is polymerized following the method represented in 10 Section 4.4.2, where eventually polymerization is done in an autoclave. Monostep in which, after the honeycomb core is formed, the facings are placed directly on this core. The assembly is polymerized using the same method as for the multistep method. Example: Wing box (Figure 7.19). 10

See also Section 2.1.3.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 152 Monday, November 18, 2002 12:17 PM

Figure 7.19 Wing Box

Figure 7.20 Horizontal Empennage of a Fighting Aircraft

The honeycomb core assures the rigidity of the component. However, the mass of the piece depends on the thickness of the core. Example: Horizontal empennage of a fighting aircraft (Figure 7.20). Remarks: One avoids drilling holes in boron/epoxy pieces as much as possible. This operation is onerous and requires ultrasonic technique with diamond tools. There is a problem with corrosion of metallic honeycomb. The corrosion is due to the progressive condensation of water in the cavities. This is combined with the mechanical and thermal stresses (fatigue) in the structure. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 153 Monday, November 18, 2002 12:17 PM

Figure 7.21 Sandwich Construction for Panels

Figure 7.22 High Lift Devices Flap

Remedies include Covering the honeycomb core surface with a resin film Introducing an inorganic inhibitor at the potential points of attack to prevent the reaction with water Sandwich construction for panels: When the thickness of the piece becomes large (on the order of 150 mm), the facings are stiffened separately by using a honeycomb core, following the arrangements shown in Figure 7.21. When the piece is of large size (long), the requirement of “nondeformation” can require the interposition of intermediate “ribs.” Each component (facings, ribs) is polymerized in the assembled state, following the technique of monostep described above. Example: High lift devices flap (Figure 7.22) Sandwich for the reinforcement of spars and ribs: One can increase the rigidity in flexure and in torsion by introducing honeycombs, as represented in Figure 7.23. Stiffened panels: Currently one can find the ribbed panels in metallic construction. The ribs can be added, or monolithic, meaning that they are formed as part of the same piece when the panel is made. One observes in parallel here with the same technique in ribbed panels in composites. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 154 Monday, November 18, 2002 12:17 PM

Figure 7.23 Sandwich for Spars and Ribs

Figure 7.24 Stiffeners Form

Figure 7.25 Wing Box

Added stiffeners: The composite stiffeners can have the forms shown in Figure 7.24. Example: Wing box (Figure 7.25). Monolithic stiffeners: These are cured at the same time with the facings. These can support higher loads than the previous case, but with higher cost. The mode of fabrication is shown schematically in Figure 7.26 for the so-called “omega” ribs. One uses cores, which are made partly by thermoexpandable silicone. One also uses hollow silicone cores stiffened by compressed air, or cores that melt at temperature on the order of 170∞C, which is slightly higher than the polymerization temperature of the piece. Example: Flanged plates (Figure 7.27) Example: Stabilizer panel (European aircraft Airbus A-300; see Figure 7.28). The carbon/epoxy ribs are obtained by combining the autoclave pressure and 11 the thermal dilatation of detachable metallic light alloy modules. The steps of the process are shown schematically in Figure 7.28: 11

See Section 1.6 for the coefficients of thermal expansion as compared between light alloy and carbon.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 155 Monday, November 18, 2002 12:17 PM

Figure 7.26 Monolithic Stiffeners

Figure 7.27 Flanged Plate

Example: Wing tip (Airplane ATR 72, ATR (FRA-ITA). This is a primary wing piece (its failure will bring about the failure of the airplane). It consists of two carbon/epoxy panels with monolithic ribs, two spars in carbon/epoxy, and 18 metallic flanges in light alloy folded sheets, as shown schematically in Figure 7.29. Mass of box: 260 kg (reduction of 65 kg as compared with a metallic solution). Remarks: Lightning protection of such a structure requires specific precautions such as: Incorporation of a conducting fabric made of bronze wires on all external surfaces Installation of lightening conductors along the spars Protection of the connections Example: Air brakes (European airplane Airbus A-320; Figure 7.30).

7.1.10

Elements of Braking

Different from the brakes for ground vehicles, the brakes for aircrafts are characterized by successively distinct phases of isolated operations over time. These repeat themselves in almost identical conditions from one landing to the next. These are © 2003 by CRC Press LLC

TX846_Frame_C07 Page 156 Monday, November 18, 2002 12:17 PM

Figure 7.28 Stabilizer Panel

Figure 7.29 Wing Tip on ATR 72 Airplane

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 157 Monday, November 18, 2002 12:17 PM

Figure 7.30 Air Brakes on Airbus A-320

“heat absorption” brakes, which are activated for only a few seconds (about 20 seconds). The subsequent cooling of these brakes happens progressively afterwards. The heat coming from the transformation of kinetic energy is stored in the components participating in the friction phenomenon, which serve as “heat sinks.” These components must have the following characteristics: Being able to create a high braking moment which remains stable as the temperature increases Being able to support a very important “thermal shock,” on the order of 6 10 joules per kg mass of the component Being refractory and retaining a good dimensional stability Being able to retain their mechanical properties at high temperature Having as low mass as possible The corresponding brakes are of “disk” type. The materials that can be used to make these friction disks are compared in Figure 7.31. One can see the interest in using three-dimensional composite materials in carbon/carbon, which have the following characteristics: Their dynamic friction coefficient is stable with respect to the temperature, varying from 0.25 to 0.3. They resist thermal shock and are refractory until 1600∞C. 12 They retain their mechanical properties at high temperature. 3 They are light weight (specific mass of 1900 kg/m ). Example: Disk brakes in carbon/carbon (Figure 7.32) “Aerolor” (FRA). Example: Supersonic transport aircraft Concorde (FRA-U.K.). The gain in paying passenger due to this type of brakes represents six passengers and their luggage, or 600 kg. 12

See order of magnitude of the mechanical properties in Section 3.6.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 158 Monday, November 18, 2002 12:17 PM

Figure 7.31 Airbrake Materials

Such types of brakes can also be developed for rapid trains, as well as for racing cars and motorcycles.

7.1.11 The Future One can cite as the principal objectives for the airplane manufacturers: Obtain with composite materials a minimum mass reduction of 20% as compared with the metallic solution using the new light alloys aluminum/ lithium. This implies the improvement in the performance of fibers and matrices. Improvement on the manufacturing process. The graph in Figure 7.33 shows that significant efforts remain to be done to reduce the labor cost in the manufacturing of high performance composite components. Apart from improvement such as automatic draping or electron beam curing or by x-ray, other more classical techniques described in Chapter 2 have actually been adapted for the fabrication of aircrafts or their components. One can mention RTM process (see Section 2.3.1), for example, tail cone of airplane Airbus A-321. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 159 Monday, November 18, 2002 12:17 PM

Figure 7.32 Disk Brakes in Carbon/carbon

Figure 7.33 Different Costs in Composite Solution © 2003 by CRC Press LLC

TX846_Frame_C07 Page 160 Monday, November 18, 2002 12:17 PM

Figure 7.34 Evolution of Percent of Composite Materials in Aircraft Structure

Figure 7.35 Relative Mass of Principal Materials Used in Aircraft Structures

High pressure injection (see Section 2.1.5) with short fibers or with particles. Thermoforming (see Sections 2.3.1 and 2.2.3) for the small pieces. Compression molding (see Sections 2.3.1 and 2.1.2). One can see in Figure 7.34 that about 20% of the mass of the structure of civil aircrafts should integrate composite materials. Figure 7.35 shows the evolution foreseen for the relative mass of the principal materials used for aircraft structures.

7.2 HELICOPTERS 7.2.1 The Situation This category of aircraft is less advanced than the airplanes in terms of technological evolution towards “perfection” as shown in the graph in Figure 7.36. In fact, taking into account the possibilities of specific mass reduction for this type of aircraft, one can see in the graph in Figure 7.37 the increasing trend in the strong integration of composites, with higher percentages as compared with the case of airplanes. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 161 Monday, November 18, 2002 12:17 PM

Figure 7.36 Degree of Technological Evolution

Figure 7.37 Evolution of Composites Mass on Helicopters

Example: Evolution of the mass of composite materials on the helicopters of Aerospatiale (FRA). In comparison with conventional metallic construction, one can mention the following mass reduction:\. 15% on the secondary structures Up to 50% in the working pieces, such as the elements of transmission of power and control

7.2.2 Composite Zones Figure 7.38 shows the composite components in a helicopter.

7.2.3 Blades The blades are the essential elements of the aircraft. They consist principally of the following: An envelope or a box that assures an aerodynamic profile and a stiffener for torsion (the blade does not twist under aerodynamic forces, at least for the actual generation of aircrafts). © 2003 by CRC Press LLC

TX846_Frame_C07 Page 162 Monday, November 18, 2002 12:17 PM

Figure 7.38 Composite Components in a Helicopter

A spar which resists the centrifugal tension on the blade as well as the flexure caused by the lift and drag loads. It is made of glass/epoxy (“R” glass, more resistant and less sensitive to aging by humidity). A rear edge that stiffens the blade in flexure in the direction of the drag. A filler material (foam or honeycomb) that prevents the deformation of the profile. Figure 7.39 shows the different parts of the blade.

7.2.3.1 Advantages The list of advantages obtained with this type of design is impressive: The blade is molded (molding by assembly of two half shells under pressure). This solution allows one to obtain an optimized profile (variable chord and thickness, nonsymmetric profile, nonlinear twist). The stiffeners for fluttering and for torsion can be controlled thanks to judicious usage of composite materials.

7.2.3.2 Consequences The payload is augmented. The mass reduction attains 400 kg for the aircraft Superpuma Aesrospatiale (FRA). The cruising speed is increased for the same power. The gain is 32 km/h at 1500 m altitude as compared with a previous helicopter. The cost of fabrication is reduced by 50% in comparison with conventional metallic solution. The cost of operation is reduced. The life of the blade is practically unlimited. None of the load in the range of flight of the aircraft can lead to the fatigue damage. It is quasiindestructible, even when testing the specimens. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 163 Monday, November 18, 2002 12:17 PM

Figure 7.39 Helicopter Blade 13

Increased security: the blade has the fail safe character. An impact (projectile, collision) causes a local deterioration which does not lead to the fall of the aircraft. 14 The blade is repairable with a relatively simple process. The blade is not sensitive to corrosion. Remarks: The blade as conceived can be ultralight. However, light weight cannot be below a value that assures a minimum inertia that is indispensable for the good operation of the rotor.

7.2.4 Yoke Rotor This is the mechanical assembly that allows The rotation of the blades The small amplitude angular displacements of the blades during rotation

13 14

See Section 7.1.4. See Section 4.4.4.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 164 Monday, November 18, 2002 12:17 PM

Pitch control, that is, the control of the aerodynamic incidence of the profiles of the blades To assure all these functions, the previous classical metallic rotors were very complex. They consisted of many pieces —in particular the ball bearings —and numerous points of lubrication. In fact, the maintenance was very costly. The modern rotors—first developed by Aerospatiale (FRA)—substitute for these classical articulations the degrees of freedom starting from the elastic deformation: Composites made of metal/elastomer Laminates Example: The yoke “Starflex” Aerospatiale (FRA). As its name indicates, this yoke has the form of a star with flexible arms (see Figure 7.40) obtained by draping a large amount of balanced glass/epoxy fabric and molding under heat and pressure. The different degrees of freedom necessary for the operation as cited above are made possible by the capabilities as shown in Figure 7.41:

Figure 7.40 The Starflex Yoke

Figure 7.41 Details of the Starflex Yoke System © 2003 by CRC Press LLC

TX846_Frame_C07 Page 165 Monday, November 18, 2002 12:17 PM

The elastic arm assures angular displacement called “lift fluttering.” The elastic ball and socket allows for the rotation noted as pitch on the figure. This translates into a variation in the incidence of the profile. The elastomer bearing allows for fluttering of the blade in the plane of the figure, called “drag fluttering.” Consequences include the following: A spectacular decrease in the number of components. (One goes from 377 pieces for a classical metallic solution with 30 bearings to 70 pieces for a composite solution without any bearings.) There is a corresponding mass reduction of 40 kg. There is a reduced cost of fabrication. The maintenance is reduced in considerable proportion, lowering significantly the hourly cost of the flight. There is increased security (more viability of the mechanical assembly).

7.2.4.1 Evolution of the Yoke Rotors Example: The yoke “Triflex” Aerospatiale (FRA). The elastic deformation of the arms (see Figure 7.42) is sufficient to assure the displacements in lift, drag, and the variable incidence (pitch). The liaison arm/yoke and arm/joints of the blades are delicate works.

Figure 7.42 Triflex Yoke © 2003 by CRC Press LLC

TX846_Frame_C07 Page 166 Monday, November 18, 2002 12:17 PM

Figure 7.43 Spheriflex Yoke

Figure 7.44 Pitch Lever

Example: The yoke “Spheriflex” Aerospatiale (FRA). This is so called because only the elastic ball-and-socket allows the various angular displacements: flapping and pitching. The foot of the blade is modified as a consequence (see Figure 7.43). The number of components becomes extremely reduced, with a minimum volume (less than the volume of the previous solutions).

7.2.5 Other Composite Working Components Most of these are made of carbon/epoxy. The parts already in service or in development include

The rotor mast The plate for the cyclical control of the pitch The struts for the control of the pitch The levers for the pitch (see Figure 7.44) where the composite design leads to a reduction of mass of 45% as compared with the metallic solution 15 Lever winch gallows The stabilizer 15

See Section 1.5.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 167 Monday, November 18, 2002 12:17 PM

Example: Aircraft Dauphin Aerospatiale (FRA). Stabilizer in light alloy

231 parts 5900 rivets Mass = 1 Global cost = 1

Stabilizer in carbon/epoxy

88 parts 0 rivets Mass = 0.78 Global cost = 0.66

In the case of the military helicopters: Utilization of composite materials reduces the “radar signature” of the helicopter. The damages by the projectiles on the blades, yokes, and command struts evolve more slowly in the composite parts and allow the aircraft to be able to return to its base (except for the case of a projectile shell break with a diameter larger than 20 mm). 16 The “crash” resistance is less for a composite structure as compared with conventional structure.

7.3 PROPELLER BLADES FOR AIRPLANES The design using composites for the propeller blades for airplanes is analogous to that for the helicopter blades. They consist essentially of a torsion box of composite with a spar made of metal or composites. Example: Propeller blade Hamilton Standard (USA) for the motor “14 SF” for 17 the airplane ATR 42 (Figure 7.45). Example: Propeller blade Ratier-Figeac (FRA) for the motor of the plane TRANSALL (FRA–GER). The adoption of a spar in unidirectional glass and a torsion box in carbon leads to a particular weight reduction, when the diameters of the rotors become important, as indicated in Figure 7.46, which has the following characteristics: Diameter of the 4-bladed rotor: 5.5 m Mass of a composite blade: 51 kg Mass reduction as compared with a metallic blade: 53 kg (mass of a metallic blade: 104 kg) Total mass reduction (2 ¥ 4 blades): 430 kg The centrifugal inertia force at the foot of the blade decreases from 105,000 daN to 30,000 daN. This is taken up by the glass fibers in the spar which are bonded to a steel piece having the form of a tulip and addition of circumferential hoop winding of rovings to allow for the “fail safe” design. If there is bonding rupture, the blade is retained on its base by the hoop windings. The construction of the Ratier-Figeac propeller blade is shown schematically in Figure 7.47. 16 17

See Section 7.1.4. See Section 7.1.6.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 168 Monday, November 18, 2002 12:17 PM

Figure 7.45 Propeller Blade, Hamilton Standard

Figure 7.46 Mass Saving in Using Composites for Blades

Example: Airplane with rocking rotors XV-15 BELL (USA; Figure 7.48), propellers Dowty Rotol Ltd. (U.K.), which has the following characteristics:

Rotor diameter: 7.6 m Chord at foot of blade: 0.5 m Mass of composites: 70% of the mass of the structure. Wing: stiffened panels in carbon/epoxy.

The new generation of the propellers (called “rapid” or “transonic”) is destined to propel commercial airplanes with a speed close to that obtained with the jets (Mach 0.8 to 0.85, or more than 850 km/h). Interest in such propellers rests in a propulsion efficiency higher than that of modern jets (with double flux) at high speeds, as shown in Figure 7.49. For good aerodynamic and acoustic behavior, the propellers are characterized by low thickness, a large “chord” and a strong curvature which gives them the form of an oriental saber. The complexity of the geometry combined with important speeds of rotation (more than 4000 revolutions per minute) requires the composite construction. Example: Propeller “Propfan” Hamilton Standard (USA; Figure 7.50). Made of two rotors in “counter-rotation,” this is designed to propel the middle range airplanes. The method of fabrication is the same as the more classical propellers mentioned above: a spar made with light metal alloy forged and machined. A filling foam is molded around the spar to give the form of the torsion box in glass/epoxy. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 169 Monday, November 18, 2002 12:17 PM

Figure 7.47 Ratier-Figeac Propeller Blade

Figure 7.48 Rocking Rotor in Bell XV-15 Plane © 2003 by CRC Press LLC

TX846_Frame_C07 Page 170 Monday, November 18, 2002 12:17 PM

Figure 7.49 Propulsion Efficiency of Propellers

Figure 7.50 Profan Propeller

Example: Transonic propeller “Charme” ONERA (FRA; Figure 7.51). The number of blades is high (12) to reduce the load in each blade. The blades are made of carbon/epoxy bonded to the titanium foot of the blades.

7.4 TURBINE BLADES IN COMPOSITES Research to increase the efficiency of aeronautical motors leads to the increase of Air compression ratios, which reach the values on the order of 45. Temperatures of the gases in the turbines. The fixed or mobile blades in the release stages have to operate with a gas temperature on the order of 1500∞C. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 171 Monday, November 18, 2002 12:17 PM

Figure 7.51 The Transonic Propeller “Charme”

Among the materials experimented with in view of increasing the operating temperature are the “oriented eutectics.” These are composed of two distinct phases: A superalloy phase with nickel base A carbon phase The solidification of this alloy is directed with a solidification front (interface between the liquid and the solid). The carbon phase is developed in the form of fibers with diameters on the order of microns and of infinite length, and parallel to the direction of displacement of the solidification front. One then obtains a unidirectional composite metal/metal. The advantages and disadvantages of these types of materials can be summarized as follows: Pluses: It is possible to obtain directly, using solidification, pieces with the form of the turbine blades. There can be a gain of 30∞C on the maximum operating temperature of actual blades. Minuses: The growing speed of the composite is low: 2 cm/hour. The proportion of fibers is low (5% to 10%) and cannot be controlled because it is constrained by the composition of the eutectic. The material is sensitive to thermal fatigue due to the run–stop operating cycles of the turbine. Fracture resistance at temperatures above 900∞C is weaker than that for super alloys in actual service.

7.5 SPACE APPLICATIONS There is no doubt that for launchers, space shuttles, and satellites the reduction of mass is most critical. Each kilogram reduction on the launcher for the European rocket Ariane E.S.A. (EU) gives a gain in payload of 30,000 US dollars. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 172 Monday, November 18, 2002 12:17 PM

7.5.1 Satellites The structural part of the satellites is essentially constituted of an assembly of tubes and plates. Principally the structure has to Resist average and fluctuating accelerations of the launch, counted as number 2 of times the acceleration of gravity (g = 9.81 m/sec ), up to 5 ¥ g continuously and 5 ¥ g maximum amplitude in sinusoidal fluctuation, for frequencies up to 40 Hz. (In order to avoid resonance, the structure has to be very rigid. It is the rigidity that appears like the factor that controls the dimensions.) Be quasi-insensitive to temperature variations (such as in the case of precision optical instruments: telescope, high-resolution camera). Here, carbon is used for the tubular structure (very low coefficient of expansion, on the -7 18 order of 10 ). The primary structures of satellites can include sandwich plates, with the following characteristics: 19

Light alloy honeycomb cores (not Nomex because of gas emission in space). Facings (skins) made of laminates, without mirror symmetry for maximum lightness. The thickness of the skin is on the order of 0.1 mm. When 20 demolding, they are very deformed. These are then bonded onto the aluminum core. One then obtains a sandwich plate that is globally balanced. Example: Camera V.H.R. (Visible high-resolution) SPOT (FRA), which is the upper part of the satellite shown in Figure 7.52. In the case of the spatial structures, among the foreseen solutions for the construction of tubular space stations, one can experiment on tubes made of extruded carbon with junctions of half-shell made of carbon.

7.5.2 Pressure Vessels The pressure vessels contain the combustibles, fuel or “powder,” for the propulsion. These can be made by winding impregnated unidirectional ribbons over a mandrel with a particular form. The mandrel must be resistant to shrinkage after 21 polymerization and should be designed to be extractable (see Figure 7.53). The efficiency of a filament-wound pressure vessel is defined as: p ( burst pressure ) efficiency ratio = ------------------------------------------------r g ( specific weight ) ( meters ) and has the units of length, for example: Efficiency of glass/epoxy: 25 km. Efficiency of Kevlar/epoxy: 35 km. which explains the predominant use of Kevlar/epoxy in these applications. 18 19 20 21

See See See See

Section Section Section Section

1.6. 1.6. 5.2.3. 2.1.7.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 173 Monday, November 18, 2002 12:17 PM

Figure 7.52 Camera V.H.R Spot

Figure 7.53 Filament-wound Pressure Vessel © 2003 by CRC Press LLC

TX846_Frame_C07 Page 174 Monday, November 18, 2002 12:17 PM

Figure 7.54 Filament Winding for Mono-block Part

Figure 7.55 Evolution of the Structure of Nozzles

For some applications, the principle of filament winding allows one to obtain vessels and tubes at the same winding session (see Figure 7.54).

7.5.3 Nozzles The propulsion nozzles of solid propergol (powder) have operating temperatures up to 3000∞C during several dozens of seconds, with pressures varying between 22 a few bars and several dozens of bars. The material making up the internal liner disappears progressively by decomposition, melting, vaporization, and sublimation. This is the phenomenon of ablation. The materials that can play such a role have to possess A strong resistance to ablation at a high operating temperature A low specific mass A strong resistance to mechanical and thermal shock Figure 7.55 shows the evolution of the structure of these nozzles until the advent of the three-dimensional carbon/epoxy composite materials with the mechanical characteristics indicated in Section 3.6. 22

1 bar = 0.1 MPa.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 175 Monday, November 18, 2002 12:17 PM

Figure 7.56 Sepcarb Material for Propulsion Nozzles

Figure 7.57 Nozzles in Rosette Form

Example: Material “Sepcarb” European company for propulsion (FRA; 23 6 Figure 7.56). The quantity of heat before ablation can reach 84 ¥ 10 joules per kilogram of material. For example the motor for peak operation of the European launcher Ariane, with the divergent nozzle made of carbon/epoxy, has the following characteristics: A mass reduction of 50% in comparison with previous nozzle constructions A gain of the launch force of 10% thanks to higher elongation Example: Divergent nozzle with “rosette” layering. Figure 7.57 shows the difference in constitution of this type of nozzle and a nozzle with classical concentric stratification, with a few orders of dimensional amplitude. To compare with the concentric stratification, this design: allows more convenient machining (more precise work of the lathe tool). is more resistant to delamination. 23

See Section 3.6.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 176 Monday, November 18, 2002 12:17 PM

7.5.4 Other Composite Components 7.5.4.1 For Thermal Protection One can distinguish two modes on entrance into the atmosphere during the return of the space vehicles: Rapid entrance with strong incidence: This is the case of the ballistic missiles and manned capsules. The heat flux is very high (on the order 2 of 10,000 kW/m ) with relatively short time of entrance. One can use, depending on the particular case: 24 Heat sinks in carbon/carbon or in beryllium (for case of the ballistic missiles). Ablative materials (see above for the case of the nozzles) for the manned capsules. Slow entrance with weak incidence: This is the case of hypersonic planes or “space shuttles.” The duration of the entrance is on the order of 2000 seconds. The heat fluxes are weaker but can attain hundreds of kilowatts per square meters of the structure at the beginning of the entrance (80 km altitude), for example: 2 500 kW/m at the leading edge 2 100 to 200 kW/m on the under part The entrance temperatures reach 1700∞C, or 2000∞C at the nose of the shuttle. There are several types of thermal protection, depending on the zones of the equipment and the reutilization of the facing: 25

Heat sinks associated with insulation Reflective thermal barrier (lining of the vehicle reflects the heat flux it receives) Ablative facing (The transformation of the facing by fusion, vaporization, sublimation, chemical decomposition absorbs the heat, and the vaporized gases cool the remaining layer, decreasing also the convective thermal flux.) The areal masses of these devices are related to the limiting admissible temperatures of the structure immediately below (see Figure 7.58). Example: NASA space shuttle (USA), which has an empty mass of 70 tons. Depending on the zones, one uses the linings made of composites of carbon/ carbon or silicon/silicon and pieces of structure (horizontal members, cross members) in boron/aluminum. The useful temperature of the latter is 300∞C for continuous use and up to 600∞C for peak applications. 26 The under part is protected by composite “tiles” in silicon/silicon ceramic that constitutes a reflective thermal barrier. The tiles are separated from the structure of light alloy or laminated boron/aluminum by a sandwich of felt and nonflammable 24 25 26

See Section 7.1.10. See Section 3.7. See Sections 2.2.4 and 3.6.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 177 Monday, November 18, 2002 12:17 PM

Figure 7.58 Areal Mass for Thermal Protection

nylon/silicon/“NOMEX” honeycomb. There are about 30,000 tiles. Their installation is shown in Figure 7.59. Example: Space shuttle Hermes (EU), which has an empty mass of 8.5 tons. The tiles are replaced by thousands of pieces made of carbon/carbon, silicon/ silicon (see Figure 7.60). The pieces have to be reused for thirty landings.

7.5.4.2 For Energy Storage On board satellites and space stations, systems using the composite flywheels for the supply of electric power and for the control of attitude provide a mass reduction of 25% as compared with conventional storage methods using batteries and gyroscopic means (specific power on the order of 5 kW per kilogram of the device). In addition, in the Strategic Defense Initiative program (USA), the devices of flywheels can deliver high levels of specific powers on the order of 100 kW per kilogram of the device. The peripheral speeds can attain 1400 m/sec (filament-wound flywheels in carbon), and the speeds of rotation from 40,000 to 60,000 rpm. Example: Development of an energy storage module (USA; Figure 7.61). 3

Total mass: 200 kg (occupied volume: 0.15 m ) Specific energy: 230 kJ/kg (total energy # 46,000 kJ) Peripheric speed: 1100 m/sec Figure 7.62 shows different solutions for the construction of carbon/epoxy flywheels. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 178 Monday, November 18, 2002 12:17 PM

Figure 7.59 NASA Space Shuttle

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 179 Monday, November 18, 2002 12:17 PM

Figure 7.60 Space Shuttle Hermes

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 180 Monday, November 18, 2002 12:17 PM

Figure 7.61 Flywheel Energy Storage

Figure 7.62 Different Flywheel Designs

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 181 Monday, November 18, 2002 12:22 PM

8 COMPOSITE MATERIALS FOR OTHER APPLICATIONS We have given in Chapter 1 an idea on the diversity of the products which can 1 be made using composite materials. In this chapter we examine a few of these products, which form a good part in the evolution of these materials, excluding the aerospace sector presented in the previous chapter.

8.1 COMPOSITE MATERIALS AND THE MANUFACTURING OF AUTOMOBILES 8.1.1 Introduction Composite materials have been introduced progressively in automobiles, following polymer materials, a few of which have been used as matrices. It is interesting to examine the relative masses of different materials which are used in the construction of automobiles. This is shown in the graph in Figure 8.1. Even though the relative mass of polymer-based materials appears low, one needs to take into account that the specific mass of steel is about 4 times greater than that of polymers. This explains the higher percentage in terms of volume for the polymers. Among the polymers, the relative distribution can be shown as in Figure 8.2. The materials called “plastics” include those so-called “reinforced plastics” for composite pieces that do not have very high performance. The graph in Figure 8.3 gives an idea for the distribution by zone of the “plastic” pieces in an automobile and also shows the evolution in time. One can see the increasing importance of high-performance parts.

8.1.2 Evaluation and Evolution A few dates on the introduction of composite parts (fibers + matrix) include: The antiques as shown in Figure 8.4 1968: wheel rims in glass/epoxy in automobile S.M.Citroen (FRA) 1970: shock absorber shield made of glass/polyester in automobile R5 Renault (FRA) 1

See Section 1.3.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 182 Monday, November 18, 2002 12:22 PM

Figure 8.1 Use of Different Materials in Automobiles

Figure 8.2 Mass Distribution Among Polymer Materials

Consequences of the introduction of composite pieces in automobiles are now well-known. They allow a number of advantages. One can find several common points with aeronautic construction. There are also disadvantages that are more specific to automobiles. Advantages include Lightening of the vehicles: A reduction of mass of 1 kg induces a final reduction of 1.5 kg, taking into account the consecutive lightening of the mechanical components.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 183 Monday, November 18, 2002 12:22 PM

Figure 8.3 Distribution of “Plastic” Components in an Automobile

Figure 8.4 Composite Pieces in Antique Cars

Cost reduction: This is due to the reduction of the number of pieces required for a certain component and to noise reduction and isolation. The better corrosion resistance of the composite pieces. Significant disadvantages are It is difficult, for fabrication in large volume, to obtain as good a surface finish as that of painted sheet metals. For the car body, the painting process and the treatment of the surfaces require high temperature exposure.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 184 Monday, November 18, 2002 12:22 PM

How to Evaluate the Gains: In theory: These are the experimental vehicles; Ford, Peugeot (1979). As compared with the metallic pieces, composite parts have obtained mass reduction of 20% to 30% on the pieces for the body. 40% to 60% on the mechanical pieces Example: Ford vehicle, which has a mass in metallic construction of 617 kg and a mass in composite construction of 300 kg for a global gain of 52%. It is convenient to consider this case as “technological prowess” far from the priority of economic constraints. In practice: Over the past years, an increasing number of pieces made of glass fibers/organic matrices have been introduced. The following list contains pieces that are in actual service or in development. Components for the body Motor cap Hood cover Hatchback door Fenders Roofs Opening roof Doors Shock absorber Interior components Seat frames Side panel and central consoles Holders Components under the hood Headlight supports Oil tanks Direction columns Cover for cylinder heads Cover for distributor Transmission shafts Motor and gearbox parts Components for the structure Chassis parts Leaf springs Floor elements Figure 8.5 shows the importance of the volumes actually occupied by the composites in an automobile. Example: Automobile BX Citroen (FRA)1983 with a total mass of 885 kg. Many of the molded pieces made of glass/resin composites as shown in Figure 8.6 are now commonly used by the automobile manufacturers. We note in particular the two elements below, the importance and large volume production of which (rate of production of more than 1000 pieces per day), indicate a significant penetration of composites in the manufacturing of automobiles.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 185 Monday, November 18, 2002 12:22 PM

Figure 8.5 Composite Pieces in an Automobile

The hood is made of glass/polyester molded at high temperature in a press 2 (20,000 kN) with the deposition of a gel coat during molding to assure the quality of the surface. The following comparison is eloquent: 2

See Section 2.1.1.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 186 Monday, November 18, 2002 12:22 PM

Figure 8.6

Composite Pieces in BX Citroen

Figure 8.7 Automobile Alpine V6, Renault

Conventional metallic construction (GS Citroen): 7 elements Composite construction: 1 element Mass gain: 7.8 kg or 46%. The rear window frame is made of injection molded glass/polyester (23,000 kN press). The mechanical characteristics obtained with this method (fracture resistance, modulus, impact resistance) are in the vicinity of those obtained by compression molding. One obtains a single piece that can support the rear glass piece, the aerodynamic details, the hinges, and the lower part of the trunk. The advantages over the classical construction are great: Classical construction (GS Citroen): 27 elements Composite construction: 7 elements Mass reduction: 1.7 kg or 16% Example: Automobile Alpine V6 Turbo, Renault (FRA), 1986 (Figure 8.7). The entire body in glass/polyester composites is not obtained by molding according to

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 187 Monday, November 18, 2002 12:22 PM

3

the technique used for the previous model A 310 (contact molding). It is made by bonding around fifty elements in glass/polyester on a tubular chassis. The panels are made by molding using a press at low pressure and temperature (6 minutes at 45∞C). 4 Contouring is done using a high-speed water jet. Structural bonding is done on a frame at 60 ∞C. Robots control it. The classical mechanical nuts and bolts are replaced by 15 kg of adhesives. Significant advantages include the following: There is reduction in fabrication time: 80 hours versus 120 hours for the construction of the previous model A 310. Excellent fatigue resistance is realized: (mileage > 300,000 km). There is good filter for noise from mechanical sources. The flexibility in the method of fabrication: The tooling in the press is interchangeable in order to produce small series of different pieces on the same press. This process is well adapted to a low rate of fabrication (10 cars per day). Mass reduction—as compared with the technique used in the previous model, which itself was using composites—is 100 kg. 3 For a cylinder size of 2500 cm (power of 147 kW or 240 CV), it is one of the most rapid series of vehicles ever produced in France previously (250 km/h) with a remarkable ratio of quality/price as compared with other competing European vehicles (Germany in particular). Example: Racing car “F.1” Ferrari (ITA) (Figure 8.8). This car body is a sandwich made of NOMEX honeycomb/carbon/epoxy. In addition, a crossing tube made of carbon/epoxy transmits to the chassis aerodynamic effects that act on the rear flap. This is attached to the chassis by light alloy parts, bonded to the composite part with structural araldite epoxy adhesive. There is weight reduction compared with previous metallic solution, and one also sees very good fatigue resistance, which is important in regard to mechanical vibrations.

8.1.3 Research and Development A number of working pieces—traditionally made of metallic alloys—of road vehicles have been designed and constructed in composite materials, and they have actually been tested and commercialized:

8.1.3.1 Chassis Components Research and Development work has been concerned with the spars, floors, front structures, rear structures, and also the complete structure. Principal advantage: Reduction in the number of parts and thus in the cost. Secondary advantage: Mass reduction (beams for truck chassis in Kevlar/ carbon/epoxy lead to a mass reduction of 38%—46 kg versus 74 kg for metal). 3 4

See Section 2.1.1. See Section 2.2.5.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 188 Monday, November 18, 2002 12:22 PM

Figure 8.8 Ferrari F.1 Racing Car

Figure 8.9 Front Face of 405 Peugeot

The problems involved are numerous: How to assemble the pieces. What will be the mechanical behavior when subjected to strong impacts? How is the rate of production to be augmented? The actual fabrication methods are too slow (decrease in the cycle time by using automation). Example: The superior cross beam or “front face” of the automobile 405 Peugeot (FRA). This component (see Figure 8.9) is subjected to repeated load cycles in tension, flexure, and torsion. It also supports several dozens of

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 189 Monday, November 18, 2002 12:22 PM

Figure 8.10 Comparison Between Metallic and Composite Springs

components and equipment that form the front face of the vehicle. Characteristics include: Part molded in glass/polyester (Vf = 42%) 5 Fabrication process: SMC : Press 15,000 N Rate of production: 1200 pieces/day Machining/drilling (70 holes); installation of inserts (30) and components made by laser, numerical machining, and robots

8.1.3.2 Suspension Components Springs: One of the principal characteristics of the unidirectionals (namely 6 glass/resin) is their capacity to accumulate elastic energy. Herein lies the interest in making composite springs. In theory, a glass/resin spring is capable of storing 5 to 7 times more elastic energy than a steel spring of the same mass. Other advantages include: The composite springs are “nonbreakable.” Damage only translates into a minor modification of the behavior of the component. It is possible to integrate many functions in one particular system, leading to a reduction in the number of parts, an optimal occupation of space, and an improvement in road behavior. The mass reduction is important (see Figure 8.10) The disadvantages: It is difficult to adapt the product to the requirements of the production. It is not sufficient to demonstrate the technical feasibility; one must optimize the three-criteria product-process-production rate (rates of production of 5 6

S.M.C. process: See Section 2.1.3 and 3.2. See Section 3.3.2, comparison of load-elongation diagrams for a metal and a unidirectional.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 190 Monday, November 18, 2002 12:22 PM

Figure 8.11 Leaf Spring

Figure 8.12 Combination of Functions

several thousands of parts per day in the automotive industry, to be made using a few processes, i.e., filament winding, compression molding, pultrusion, and 7 pultrusion-forming). The current development and commercialization efforts deal with leaf springs and torsion beam springs. Example: Single leaf spring (see Figure 8.11). A spring made of many metallic leaves is replaced by a single leaf spring made of composite in glass/epoxy. Many vehicles are sold with this type of spring, for example, Rover –GB; Nissan–JAP; General Motors–USA; Renault–FRA). Example: Multifunctional system (Bertin–FRA). This prototype for the front suspension of the automobile combines the different functions of spring, rolling return, and wheel guide (see Figure 8.12). Example: Stabilizing system. This is used for the connection between an automobile and a caravan (Bertin/Tunesi–FRA). The combined functions are shown schematically in Figure 8.13. The mass is divided by 4.5 in comparison with an “all metal” solution. Example: The automobile suspension triangle has two parts (FRA) that are bonded to make a box (see Figure 8.14).

8.1.3.3 Mechanical Pieces Motor: The parts shown schematically in Figure 8.15 are in the experimental stage or in service in thermal motors. For pieces that have to operate at high temperatures, one should use the high temperature material system

7

See Chapter 2.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 191 Monday, November 18, 2002 12:22 PM

Figure 8.13 Stabilizing System

Figure 8.14 Composite Suspension Triangle 8

glass/polyamide (up to 300∞C). One can also mention the pump blades and the synchronizers in speed boxes made of glass/polyamide. 9 Composite transmission shafts : These are used in Competition vehicles (rallies), allowing high speed of rotation with low inertia Small and large trucks Figure 8.16 shows how the low mass density associated with high rigidity in flexure allows the elimination of the intermediate bearing (this induces also a supplementary reduction in mass and cost). 8

9

The polyamide resin is said to be “thermally stable;” that is, it can maintain its mechanical properties at high temperatures (up to 500∞C for one hour). See Application 18.1.4.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 192 Monday, November 18, 2002 12:22 PM

Figure 8.15 Composite Mechanical Components

Figure 8.16 Composite Shafts

For the transmission shafts equipped with supports, one obtains the following advantages: Reduction of mass of 30% to 60% in comparison with the transmission shafts with universal cardan joints

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 193 Monday, November 18, 2002 12:22 PM

Figure 8.17 Composite-metal Shaft Bonding

Reduction in mechanical vibrations Decrease in acoustic vibration level (in particular the “peak”) Good resistance against chemical agents Very good fatigue resistance

Lateral transmission shafts are used for vehicles with front drive. They are used to eliminate the homokinetic joints that are actually used. They are made of a weak matrix material and wound fibers that allow the freedom of flexure for the transmission shaft.

8.2 COMPOSITES IN NAVAL CONSTRUCTION 8.2.1 Competition 8.2.1.2 Multishell Sail Boats In the past years there has been a spectacular development in the sailboat competition, with significant research activities on the improvement of the qualities of the boats, and the design of sail boats called “multishells” with large dimensions, made of high performance composites, characterized by Low mass leading to reduced “water drafts” 10 New and more performing “riggings” Resistance against intense fatigue loadings, namely for the joint mechanisms between the shells Example: Catamaran Elf Aquitaine (FRA) 1983 (see Figure 8.18). This is a large boat (20 m) in high performance composite materials. It has the following principal characteristics: A mast-sail constituted of two half-shells in carbon/epoxy, 24 meters long Connecting arms for shells with “x” shape that work in flexure to take up the difference in pitching between the two shells

10

There is a record speed of 34 knots with a class C catamaran (7.6 m in length).

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 194 Monday, November 18, 2002 12:22 PM

Figure 8.18 Elf Aquitaine Catamaran

A total fully equipped mass of 5.3 tons, corresponding to a mass reduction of 50% as compared with a construction in light alloy Example: Competition skiff WM (FRA) 1995 (see Figure 8.19). Example: Surf board 1995 (see Figure 8.20).

8.2.2 Ships In the defense domain, there are composite boats of large dimensions (>50 m): escort-patrollers are expected to be 90 m in length. Example: Anti-mine ocean liner BAMO (FRA). The Catamaran shell is 52 m in length, 15 m in width, and molded in 8 parts. It has 250 tons of glass/polyester composites in monolithic and sandwich construction with balsa core for the bridges and walls (see Figure 8.21).

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 195 Monday, November 18, 2002 12:22 PM

Figure 8.19 Competition Skiff

Figure 8.20 Surf Board

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 196 Monday, November 18, 2002 12:22 PM

Figure 8.21 Anti-mine Ocean Liner

8.3 SPORTS AND RECREATION 8.3.1 Skis Initially made of monolithic wood, the ski has evolved toward composite solutions in which each phase — each in itself a composite material — fulfills a determined function. Figure 8.22 illustrates a transverse cross section of a ski of a previous generation: steel for the elasticity of the element, wood to dampen the vibration, interspersed aluminum for its better adherence to wood. Among the essential mechanical characteristics, the manufacturer has to master the following:

Flexibility in flexure Ski stiffness in torsion (for turning) Elastic limit Fracture limit

One must also note the large diversities of the quality of The snow and the slopes (operating conditions) The skiers (different levels) Taking into account the above specifications requires the manufacturers to provide a large variety of skis. The principal components include The structure is the part of the ski that assures the essential functions as mentioned previously. It may require a piece—or an assembly of several pieces—along the longitudinal direction of the ski, and the cross section

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 197 Monday, November 18, 2002 12:22 PM

Figure 8.22 Cross Section of an Antique Ski

Figure 8.23 Different Ski Cross Section Forms

Figure 8.24 Section of Ski Dynastar

area may take the form shown in Figure 8.23. In fact, other elements can be added to these requirements, which will allow one to control separately stiffness in flexure and stiffness in torsion. The ratio of these two stiffnesses will determine the behavior of the ski, particularly during turning. For this, one uses mainly the following materials: Glass/epoxy Carbon/epoxy Kevlar/epoxy Honeycombs Zicral (AU 2 ZN) Steel alloy Example: Skis Dynastar (FRA): The real appearance of a section is complex, as shown in Figure 8.24, on which one can recognize the “omega,” the box, and the sandwich structures described previously. The filling contributes little to the mechanical characteristics of the whole structure (10% to 15%), but it constitutes the big part in the total volume

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 198 Monday, November 18, 2002 12:22 PM

Figure 8.25 Composite Bicycle

(70 to 80%). Its specific mass has to be as small as possible. The filling can be of Wood, which is sensitive to humidity, with scatter in mechanical characteristics and specific mass depending on the lots Polyurethane foam, with weak mechanical characteristics Acrylic foam, which is very onerous The covers and the edges are in glass/phenol or in glass/granix. The upper edges are in zicral, the lower edges are in steel. The synthetic inner soles have high specific mass.

8.3.2 Bicycles Initially reserved only for competition, numerous variations with frames and wheels made of carbon/epoxy can now be found (see Figure 8.25).

8.4 OTHER APPLICATIONS 8.4.1 Wind Turbines The renewed interest in wind turbines has been caused by the use of composites in the fabrication of the blades. These can be of large dimensions (lengths exceeding 24 meters). Example: Figure 8.26 gives an idea of the size of a wind turbine that develops a maximum power of 33 kW. The blades in glass/epoxy are made here by vacuum 11 forming using two half-shells assemblies by epoxy adhesive bonding. The blades can also be done by filament winding, a process well suited for the construction of torsion box (Figure 8.27). Nevertheless, for longer lengths, the

11

See Section 2.1.3.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 199 Monday, November 18, 2002 12:22 PM

Figure 8.26 Wind Turbines

Figure 8.27 Filament Winding for Wind Turbine

flexure of the blade varies during winding (difference in flexural rigidity in one neutral plane from the other). One can mention also the composite propeller blades for the cooling blowers, 12 which borrow the technology of the aircraft propellers, which have a speed of rotation larger than for the wind turbines. 12

See Section 7.3.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 200 Monday, November 18, 2002 12:22 PM

Figure 8.28 Composite Gas Bottles

8.4.2 Compressed Gas Bottles These are made using filament-wound glass/epoxy or Kevlar/epoxy (see Figure 8.28) reinforcing a thin envelope in light alloy which is used for sealing purposes. The pressure can reach 350 bars in operating conditions (rupture at more than 1,000 bars). The ratio (gas volume/bottle mass) is multiplied by 4 in comparison with the steel solution. Applications include Very light breathing apparatus (for scuba diving) Reservoirs for gaseous fuels Accessories for missiles

8.4.3 Buggy Chassis These are made using glass/epoxy. They are very resilient and can help reduce noise. They are very light with a reduced number of pieces in comparison with the metallic solution. They also offer very good fatigue endurance, as has already 13 been described above for glass/epoxy. Other advantages include the possibility of integration of the “spring” function in the structure of the chassis and increase in the “critical” speed from which a proper mode of vibration can develop in the suspension (see Figure 8.29).

8.4.4 Tubes for Off-Shore Installations These are used in deep waters. The weight of the metallic tubes —or risers— increases proportionally with the depth and can attain high values (one third of the limit stress for a depth of 1000 m). This gives rise to interest in using tubes made of glass/carbon/resin, which are three to four times lighter than tubes made of steel. Example: Production tubes for a cable-held platform. The platform is held with cables toward the bottom (see Figure 8.30). A large number of production 13

See Section 5.4.4.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 201 Monday, November 18, 2002 12:22 PM

Figure 8.29 M.B.B. Buggy

Figure 8.30 Riser Tubes

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 202 Monday, November 18, 2002 12:22 PM

tubes connect the underwater bottom to the platform. They are subjected to the static and dynamic loadings (due to underwater currents) as: Tension Flexure Circumferential extension and contraction due to external and internal pressures Characteristics: Safety factor as compared with complete rupture: 2 to 3. The micro cracks in the resin require internal and external sealings using elastomers.

8.4.5 Biomechanics Applications The carbon/carbon composites (see Section 3.6) have the rare properties of not provoking fibrous outgrowth when in contact with the blood stream; they are socalled thrombo resistant. In addition, the following qualities also favor their implantation in the human body:

Chemical resistance and inertness Mechanical and fatigue resistance Controllable flexibility due to the nature of composite materials Low specific mass Transparency to different rays Possible sterilization at very high temperatures

The principal applications (to be expanded) for the moment are

Hip and knee implants (in development) Osteosynthesis plates Dental implants Implant apparatus

8.4.6 Telepherique Cabin A substitution using composites on the classical solution for the telepherique cars made of metals gives, at equal mass, a notable augmentation of the useful payload. Example: Company Ingenex/telepherique of Argentieres (FRA): Increasing capacity while keeping existing installations, that is cables—pylons—motorization. Previous metallic telepherique: useful payload 45 passengers New composite telepherique, carbon/Kevlar/epoxy (Figure 8.31): useful load 70 passengers (with the same mass as the previous construction) Augmentation of capacity: 55%

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 203 Monday, November 18, 2002 12:22 PM

Cost comparison: renewal of all installation with the metallic solution ($11 million) Renewal of two telepherique cabins with the composite solution ($1.1 million): cost divided by 10

Figure 8.31 Telepherique Cabin

© 2003 by CRC Press LLC

TX846_Frame_C09 Page 205 Monday, November 18, 2002 12:24 PM

PART II MECHANICAL BEHAVIOR OF LAMINATED MATERIALS We have introduced in the previous part the anisotropic properties of composite 1 materials from a qualitative point of view, and we have indicated the characteristic elastic constants for the behavior of an anisotropic layer in its plane. We have also mentioned the relations that allow one to predict the mechanical behavior of a fiber/matrix combination from the properties of the individual 2 3 constituents. In Chapter 5, we have also given the elements necessary for the sizing of the laminates made of carbon/epoxy, Kevlar/epoxy, and glass/epoxy, in terms of strength and deformation. This second part is dedicated to the justification and application of these properties and results. It requires a detailed study of the behavior of anisotropic composite layers and of the stacking that makes up the laminate. It is useful to note that the basics of the mechanics of continuous media—namely, the state of stress and strain at a point—already described in great details in many texts on mechanics of materials, are supposed to be known.

1 2 3

See Section 3.1. See Section 3.3.1. See Section 5.2/5.3.

© 2003 by CRC Press LLC

TX846_Frame_C09 Page 207 Monday, November 18, 2002 12:24 PM

9 ANISOTROPIC ELASTIC MEDIA 9.1 REVIEW OF NOTATIONS 9.1.1 Continuum Mechanics We consider the following classical notions and notations of the mechanics of continuous media: State of stress at a point: This is defined by a second order tensor with the symbol Â. The 3 by 3 matrix associated with this tensor is symmetric. In this matrix, there are six distinct terms, which are denoted as sij:

s11 ; s22 ; s33 ; s23 ; s13 ; s12 State of strain at a point: This is defined as a second order tensor e. The 3 by 3 matrix for this tensor is symmetric. It consists of six distinct terms denoted as eij:

e11; e22; e33; e23; e13; e12 Linear elastic medium: The strains are linear and homogeneous functions of the stresses. The corresponding relations are:

e ij = j ijk ¥ s k

1

Homogeneous medium: In this case, the matrix terms jijkl characterizing the elastic behavior of the medium are not point functions. They are the same at all points in the considered medium.

1

For example:

e11 = j1111 s11 + j1112 s12 + j1113 s13 + j1121 s21 + j1122 s22 + j1123 s23 + j1131 s31 + j1132 s32 + j1133 s33.

© 2003 by CRC Press LLC

TX846_Frame_C09 Page 208 Monday, November 18, 2002 12:24 PM

9.1.2 Number of Distinct jijk Terms The above stress–strain relation can be written in matrix form as:

Due to the symmetry of the stresses ( s k = s k ), the corresponding coefficients are the same, i.e., j ijk = j ijk . Due to the symmetry of the strains (eij = eji), the corresponding coefficients are the same, i.e., j ijk = j jik . In other words, the knowledge of only the coefficients of the 6 ¥ 6 matrix written above is required. In addition, application of the theorem of virtual work on the stresses 2 shows that the coefficients jijk are symmetric, meaning: j ijk = j kij . Therefore, the 6 ¥ 6 matrix mentioned previously is symmetric. The number of distinct coefficients is: 6(6 + 1 ) -------------------- = 21 coefficients 2 2

Consider two simple stress states: • State No. 1: One single stress, (sk)1, which causes the strain: (eij)1 = jijk (sk)1 • State No. 2: One single stress, (spq)2, which causes the strain: (emn)2 = jmnpq (spq)2 One can write that the work of the stress in state No. 1 on the strain in state No. 2 is equal to the work of the stress in state No. 2 on the strain in state No. 1, as: ( s k ) 1 ¥ ( e k ) 2 = ( s pq ) 2 ¥ ( e pq ) 1 which means: ( s k ) 1 ¥ j kpq ¥ ( s pq ) 2 = ( s pq ) 2 ¥ j pqk ¥ ( s k ) 1 from which one has:

© 2003 by CRC Press LLC

jkpq = jpqk

TX846_Frame_C09 Page 209 Monday, November 18, 2002 12:24 PM

In summary: stress reciprocity: j ijk = j ijk strain definition: j ijk = j jik

(9.1)

symmetry: j ijk = j kij There remain 21 distinct coefficients j ijk The previous stress–strain relation can then be written as: Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

e 11 e 22 e 33 e 23 e 13 e 12

¸ j 1111 Ô Ô j 2211 Ô Ô j 3311 ˝ = j 2311 Ô Ô j 1311 Ô Ô j 1211 ˛

j 1122 j 2222 j 3322 j 2322 j 1322 j 1222

j 1133 j 2233 j 3333 j 2333 j 1333 j 1233

2 j 1123 2 j 2223 2 j 3323 2 j 2323 2 j 1323 2 j 1223

2 j 1113 2 j 2213 2 j 3313 2 j 2313 2 j 1313 2 j 1213

2 j 1112 2 j 2212 2 j 3312 2 j 2312 2 j 1312 2 j 1212

Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

s 11 s 22 s 33 s 23 s 13 s 12

¸ Ô Ô Ô Ô ˝ Ô Ô Ô Ô ˛

The matrix above does not have the general symmetry as in the general form (9 ¥ 9) presented previously. (Note the coefficients 2 in this matrix). One can get around this inconvenience by doubling the terms e23, e13, e12, introducing the shear strains:

g 23 = 2 e 23 ;

g 13 = 2 e 13 ;

g 12 = 2 e 12

from which the stress–strain behavior can then be written in a symmetric form as:

Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

e 11 e 22 e 33 2 e 23 2 e 13 2 e 12

¸ j 1111 j 1122 j 1133 Ô Ô j 2211 j 2222 j 2233 Ô Ô j 3311 j 3322 j 3333 = ˝ 2 j 2311 2 j 2322 2 j 2333 Ô g 23 Ô g 2 j 1311 2 j 1322 2 j 1333 Ô 13 Ô g 12 2 j 1211 2 j 1222 2 j 1233 ˛

2 j 1123 2 j 2223 2 j 3323 4 j 2323 4 j 1323 4 j 1223

2 j 1113 2 j 2213 2 j 3313 4 j 2313 4 j 1313 4 j 1213

2 j 1112 2 j 2212 2 j 3312 4 j 2312 4 j 1312 4 j 1212

Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

s 11 s 22 s 33 s 23 s 13 s 12

¸ Ô Ô Ô Ô ˝ Ô Ô Ô Ô ˛

(9.2)

9.2 ORTHOTROPIC MATERIALS Definition: An orthotropic material is a homogeneous linear elastic material having two planes of symmetry at every point in terms of mechanical properties, these two planes being perpendicular to each other.

© 2003 by CRC Press LLC

TX846_Frame_C09 Page 210 Monday, November 18, 2002 12:24 PM

3

Then one can show that the number of independent elastic constants is nine. The constitutive relation expressed in the so-called “orthotropic” axes, defined by three axes constructed on the two orthogonal planes and their intersection line, can be written in the following form, called the engineering notation because it utilizes the elastic modulus and Poisson ratios:

Ï Ô Ô Ô Ô Ô Ô Ô Ô Ì Ô Ô Ô Ô Ô Ô Ô Ô Ó

¸ e 11 Ô Ô Ô e 22 Ô Ô Ô Ô e 33 Ô ˝ Ô g 23 Ô Ô Ô g 13 Ô Ô Ô g 12 Ô ˛

n 21 n 31 – ------ – -----E2 E3 n 12 n 32 1 – ------ ----- – -----E2 E1 E3 n 13 n 23 1 – ------ – ------ ----E3 E1 E2 1 ----E1

0

0

0

0

0

0

0

0

0

Ï 0 Ô Ô Ô 0 0 0 Ô Ô Ô 0 0 0 ÔÔ Ì Ô 1 0 Ô -------- 0 G 23 Ô Ô 1 0 ------- 0 Ô Ô G 13 1 Ô 0 0 -------- Ô G 12 Ó 0

0

s 11 ¸ Ô Ô Ô s 22 Ô Ô Ô s 33 Ô Ô ˝ Ô s 23 Ô Ô Ô s 13 Ô Ô Ô Ô s 12 ˛

(9.3)

where E1, E2, E3 are the longitudinal elastic moduli. G23, G13, G12 are the shear moduli. n12, n13, n23, n21, n31, n32 are the Poisson ratios. In addition, the symmetry of the stress–strain matrix above leads to the following relations:

n 21 n 12 ------ = ------; E2 E1

n 31 n 13 ------ = ------; E3 E1

n 32 n 23 ------ = ------E3 E2

(9.4)

9.3 TRANSVERSELY ISOTROPIC MATERIALS Definition: A transversely isotropic material is a homogeneous linear elastic material such that any plane including a preferred axis, is a plane of mechanical symmetry. 4 One can show that the constitutive relation has five independent elastic constants. For the fiber/matrix composite shown in Figure 9.1 the preferred axis is . The fibers are distributed uniformly in the direction along . All directions perpendicular to the fibers characterize the transverse direction t. 3 4

Proof is shown in Section 13.1. Proof is shown in Section 13.2.

© 2003 by CRC Press LLC

TX846_Frame_C09 Page 211 Monday, November 18, 2002 12:24 PM

Figure 9.1 Transversely Isotropic Unidirectional

The engineering stress–strain relation has the form: Ï Ô Ô Ô Ô Ô Ô Ô Ô Ì Ô Ô Ô Ô Ô Ô Ô Ô Ó

Ï n n 1 e ¸ ----- – -----t- – -----t0 0 0 Ô Ô E E E t t Ô Ô Ô Ô n n 1 e tt Ô – -----t- ---– ----t 0 0 0 Ô Et E Et Ô Ô Ô Ô n t nt 1 Ô e t¢t¢ Ô --0 0 0 – ----– --Ô Ô E E E t t ˝ = Ì Ô Ô 2 ( 1 + nt ) g tt¢ Ô --------------------- 0 0 0 0 0 Ô Et Ô Ô Ô Ô 1 0 0 0 0 g t¢ Ô ------- 0 Ô G t Ô Ô Ô 1 Ô 0 0 0 0 0 ------- Ô g t Ô G t Ó ˛

s ¸ Ô Ô Ô s tt Ô Ô Ô s t¢t¢ Ô Ô ˝ Ô t tt¢ Ô Ô Ô t t¢ Ô Ô Ô Ô t t ˛

(9.5)

Remarks: The independent elastic constants are

Young modulus along the direction: E. Young modulus along any transverse direction t: Et. Shear modulus in the plane , t: Gt. Poisson coefficients: nt and nt.

The symmetry of the coefficients of the constitutive relation leads to

n n ------t = -----t- E Et One may also note that the shear modulus in the plane t, t¢ can be written as: Et --------------------2 (1 + nt ) This equation is classic for isotropic materials.

© 2003 by CRC Press LLC

TX846_Frame_C10 Page 213 Monday, November 18, 2002 12:25 PM

10 ELASTIC CONSTANTS OF UNIDIRECTIONAL COMPOSITES In this chapter we examine a distinct combination of two materials (matrix and fiber), with simple geometry and loading conditions, in order to estimate the elastic properties of the equivalent material, i.e., of the composite.

10.1 LONGITUDINAL MODULUS E The two materials are shown schematically in Figure 10.1 where m stands for matrix. f stands for fiber. Hypothesis: The two materials are bonded together. More precisely, one makes the following assumptions: Both the matrix m and the fiber f have the same longitudinal strain el. The interface between the two materials allows the z normal strains in the two materials to be different.

ez π ez m

f

The state of stresses resulting from a force F can therefore be written as:

s 0 0 SÆ 0 0 0 m 0 0 0 m

s 0 0 SÆ 0 0 0 f 0 0 0 f

and the corresponding state of strains:

e 0 0 e Æ 0 et 0 m 0 0 ez m

© 2003 by CRC Press LLC

e 0 0 e Æ 0 et 0 f 0 0 ez f

TX846_Frame_C10 Page 214 Monday, November 18, 2002 12:25 PM

Figure 10.1 Longitudinal Modulus E

Each material is assumed to be linear elastic and isotropic, with the following stress–strain relation: 1+n n e = ------------ S – --- trace ( S )I E E

(10.1)

in which e represents the strain tensor, S represents the stress tensor, and I the unity tensor. E and n are the elastic constants of the considered material. For the composite (m + f ), one uses Equation 9.5 with restriction to the plane l,t. It reduces to:

Ï e ¸ Ô Ô Ì et ˝ = Ô Ô Ó g t ˛

1 ----E

n – -----tEt

n – -----tE

1 ---Et

0

0

0

Ï s ¸ Ô Ô 0 Ì st ˝ Ô Ô 1 Ó t t ˛

------G t

The stress s(m+f ) can be written as (see Figure 10.1 above): em ef F F - + s --------------s = --- = ------------------------------ = s --------------( em + ef ) ¥ 1 em + ef em + ef S m + f

m

f 1

which can be written in terms of the volume fractions of the fiber and the matrix as

s m + f

1

See Section 3.2.2.

© 2003 by CRC Press LLC

=

s Vm + s Vf m

f

TX846_Frame_C10 Page 215 Monday, November 18, 2002 12:25 PM

Expressing the stresses in terms of the strains for each material yields E e = Em e Vm + Ef e Vf then: E = Em Vm + Ef Vf

(10.2)

Note: Among the real phenomena that are not taken into account in the expression of El is the lack of perfect straightness of the fibers in the matrix. Also, the modulus El depends on the sign of the stress (tension or compression). In rigorous consideration, the material is “bimodulus.” Example: Unidirectional layers with 60% fiber volume fraction (Vf = 0.60) with epoxy matrix:

E tension (MPa) E compression (MPa)

Kevlar

“HR” Carbon

“HM” Carbon

85,000 80,300

134,000 134,000

180,000 160,000

10.2 POISSON COEFFICIENT Considering again the loading defined in the previous paragraph, the transverse strain for the matrix m and fiber f can be written as:

n e t = – --- s = – ne E and for the composite (m + f ):

n = -----t- ¥ s E m + f m + f et

= – n t e

The strain in the transverse direction can also be written as:

et m + f

et

m + f

De D ( em + ef ) De m - V m + --------f V f - = --------= -----------------------em + ef em ef = et Vm + et Vf m

f

Because e has the same value in m and f: – n t e = – n m e V m - n f e V f

n t = n m V m + n f V f © 2003 by CRC Press LLC

(10.3)

TX846_Frame_C10 Page 216 Monday, November 18, 2002 12:25 PM

10.3 TRANSVERSE MODULUS Et To evaluate the modulus along the transverse direction E, the two materials are shown in the Figure 10.2. In addition, one uses the following simplifications: Hypothesis: At the interface between the two materials, assume the following: Freedom of movement in the l direction allows for different strains in the two materials:

e π e m

f

Freedom of movement in the z direction allows for different strains in the two materials:

ez π ez m

f

Then, the state of stress created by a load F (see Figure 10.2), can be reduced for each material to the following: 0 0 0 S Æ 0 st 0 0 0 0

Figure 10.2 Transverse Modulus Et © 2003 by CRC Press LLC

TX846_Frame_C10 Page 217 Monday, November 18, 2002 12:25 PM

The strains can be written as:

e 0 0 e Æ 0 et 0 0 0 ez m or f Then for the composite (m + f ), one has 1 e t = ---- s t Et On the other hand, using direct calculation leads to (see Figure 10.2) D ( em + ef ) - = et Vm + et Vf e t = -----------------------em + ef m f then: 1 1 1 ---- s = ------ s t V m + ---- s t V f Et t Em Ef

Vm Vf 1 ---- = ------ + ----Em Ef Et

or

1 E t = E m ----------------------------------Em -V ( 1 – V f ) + ----E f

(10.4)

f

Remarks: Due to the above simplifications that allow the possibility for relative sliding along the l and z directions at the interface, the transverse modulus Et above may not be accurate. One finds in the technical literature many more complex formulae giving Et. However, none can provide guaranteed good result. Taking into consideration the load applied (see Figure 10.2),: the modulus Ef that appears in Equation 10.4 is the modulus of elasticity of the fiber in a direction that is perpendicular to the fiber axis. This modulus can be very different from the modulus along the axis of the fiber, due to the 2 anisotropy that exists in fibers. 2

This point was discussed in Paragraph 3.3.1.

© 2003 by CRC Press LLC

TX846_Frame_C10 Page 218 Monday, November 18, 2002 12:25 PM

10.4 SHEAR MODULUS Gt Load application that can be used to evaluate the shear modulus Gt is shown schematically in the Figure 10.3, both with the angular deformations that are produced. The state of stress, identical for both the matrix and fiber material, can be written as: 0 t t 0 S Æ t t 0 0 0 0 0 The corresponding strains can be written as: 0 e t 0 e Æ e t 0 0 m or f 0 0 0 Using the constitutive equation, one has

t t 1+n e t = ------------ t t = -----2G E then:

t t g t = ----G Also, from Figure 10.3, one has

g t m + f

Figure 10.3 Shear modulus Gt © 2003 by CRC Press LLC

( e m + e f ) = g t e m + g t e f m

f

TX846_Frame_C10 Page 219 Monday, November 18, 2002 12:25 PM

which can be rewritten as: = g t V m + g t V f m + f m f

g t

t t t t t t ------ = ------ V m + -----V G t Gm Gf f V V 1 ------- = ------m- + -----f Gm Gf G t 1 G t = G m ----------------------------------Gm - Vf ( 1 – V f ) + -----G

3

(10.5)

f

10.5 THERMOELASTIC PROPERTIES 10.5.1 Isotropic Material: Recall When the influence of temperature is taken into consideration, Hooke’s law for the case of no temperature influence: 1+n n e = ------------ S – --- trace ( S )I E E is replaced by the Hooke–Duhamel law: 1+n n e = ------------ S – --- trace ( S ) I + a DT I E E where

10.5.2

(10.6)

e = Strain tensor S = Stress tensor I = Unity tensor E, n = Elastic constants for the considered material 4 a = Coefficient of thermal expansion DT = Change in temperature with respect to a reference temperature at which the stresses and strains are nil

Case of Unidirectional Composite

The coefficient of thermal expansion of the matrix is usually much larger (more 4 than ten times) than that of the fiber. In Figure 10.4, one can imagine that even in the absence of mechanical loading, a change in temperature DT will produce a 3 4

A few values of the shear modulus Gf are shown in Section 3.3.1. See Section 1.6, “Principal Physical Properties.”

© 2003 by CRC Press LLC

TX846_Frame_C10 Page 220 Monday, November 18, 2002 12:25 PM

Figure 10.4 Unidirectional Composite

longitudinal strain in the composite. This longitudinal strain has a value that is intermediate between the strain of the fiber alone and that of the matrix alone. Then, in the composite one finds internal stresses along the direction l (along the direction t, the fiber and matrix can expand differently). One then has: For the stresses:

s 0 0 SÆ 0 0 0 m 0 0 0 m

s 0 0 SÆ 0 0 0 f 0 0 0 f

For the strains:

e 0 0 e Æ 0 et 0 m 0 0 ez m

e 0 0 e Æ 0 et 0 f 0 0 ez f

10.5.2.1 Coefficient of Thermal Expansion along the Direction l One has for the fiber and the matrix, respectively:

s s e = ------ m + a m DT = e = ----- f + a f DT Em Ef f m The external equilibrium can be written as (see Figure 10.4):

s ¥ em + s ¥ ef = 0 m f © 2003 by CRC Press LLC

TX846_Frame_C10 Page 221 Monday, November 18, 2002 12:25 PM

where, taking into account the equality of the strains: em 1 s ------ m + a m DT = – s ¥ ----¥ ---- + a f DT Em ef Ef m ( a f – a m )DT ( a f – a m )DT ----------------------------= s = ----------------------------em Vm 1 1 1 1 ------ + ----- ¥ --------- + ------ ¥ ---ef Vf Em Em Ef Ef m V represents the volume fraction. The longitudinal strain can then be written as: ( a f E f V f + a m E m V m ) ( DT ) e = e = -----------------------------------------------------------------Ef Vf + Em Vm m f It is also the longitudinal strain that is created only by the effect of temperature:

e

= a DT

m + f where a is the longitudinal coefficient of thermal expansion. One can then equate the above expressions to obtain:

af Ef Vf + am Em Vm a = -----------------------------------------------Ef Vf + Em Vm

(10.7)

10.5.2.2 Coefficient of Thermal Expansion along the Transverse Direction t The global thermal strain can be written as (see Figure 10.4): ef D ( em + ef ) em - = e t --------------- + e t --------------= -----------------------em + ef em + ef em + ef m + f m f

et

then:

et m + f

= et ¥ Vm + et ¥ Vf m

f 5

Using the Hooke and Duhamel law (Equation 10.6) :

n Vm - s + a m DTˆ V m + Ê – ----f s + a f DTˆ V f = Ê – -----Ë Em ¯ Ë Ef ¯ m m + f f et

5

For the Poisson coefficients of common fibers, see Section 3.3.1.

© 2003 by CRC Press LLC

TX846_Frame_C10 Page 222 Monday, November 18, 2002 12:25 PM

Using the expressions for stresses obtained before, one obtains:

et m + f

Ï ¸ ( nf Em – nm Ef ) = Ì ( a m V m + a f V f ) + ---------------------------------V m Vf ( a f – a m ) ˝DT E V + E V m m f f Ó ˛

The quantity between the brackets represent the coefficient of thermal expansion along the transverse direction t, at, which can be written as: ( nf Em – nm Ef ) - ¥ ( af – am ) a t = a m V m + a f V f + --------------------------------E Em ------ + ------fV V f

(10.8)

m

10.5.3 Thermomechanical Behavior of a Unidirectional Layer Under the combined effect of the stresses and temperature, the global thermomechanical strains of a unidirectional layer can be obtained using the following relation: 1 -----

E Ï e ¸ Ô Ô v Ì e t ˝ = – -----tE Ô Ô Ó g t ˛ 0

n

t – ----E t

1 ---Et

0

0

Ï a ¸ Ï s ¸ Ô Ô Ô Ô 0 Ì s t ˝ + DT Ì a t ˝ Ô Ô Ô Ô Ó0˛ 1 Ó t t ˛

(10.9)

------G t

in which the coefficients E, Et, vt, Gt, a and at have the values given by the Equations 10.2 to 10.8, respectively.

© 2003 by CRC Press LLC

TX846_Frame_C11 Page 223 Monday, November 18, 2002 12:26 PM

11 ELASTIC CONSTANTS OF A PLY ALONG AN ARBITRARY DIRECTION To study the behavior of a laminate made up of many plies with different orientations, it is necessary to know the behavior of each of the plies in directions that are different from the principal material directions of the ply. We propose to determine the elastic constants for this ply behavior using relatively simple calculations.

11.1 COMPLIANCE COEFFICIENTS 1

The ply is already defined in Chapter 3. Let , t and z be the orthotropic axes 2 of a ply shown in the Figure 11.1. For a thin laminate made up by a superposition of many plies, we assume that the stresses szz are zero. It is then possible, for an orthotropic material, to write the stress–strain relation in the plane ,t starting from Equation 9.3 or 9.5 in the form: n

l t - – -----Ï e ¸ Ï ---Et Ô Ô Ô E Ô Ô Ô nt l ---Ì e t ˝ = Ì – -----Et E Ô Ô Ô Ô Ô Ô 0 0 Ó g t ˛ Ó

0 ¸Ï s ¸ ÔÔ Ô ÔÔ Ô 0 ˝Ì s t ˝ ÔÔ Ô l Ô -------- ÔÔ G t ˛Ó t t ˛

(11.1)

Problem: How can one transform this relation expressed in the coordinates ,t into a relation expressed in coordinates x,y inclined at an angle of q with the ,t 3 coordinates (see Figure 11.1). First recall the following: 1 2 3

See Section 3.2. The orthotropic axes 1,2,3 in Equation 9.3 are now called l,t,z, respectively. What follows is treated more globally and completely in Section 13.2.2.

© 2003 by CRC Press LLC

TX846_Frame_C11 Page 224 Monday, November 18, 2002 12:26 PM

Figure 11.1 Orthotropic Axes and Arbitrary Direction in the Plane of a Ply

Recall 1: The stress s acting on a surface with a normal vector n is given by { σ } = [ σ ij ] { n }

(11.2) column matrix of stress components σ

stress matrix

column matrix of direction cosines n

Recall 2: The coordinates of the same vector V in axes x,y as well as ,t, such that ( x . ) = cos q, are V = V + Vt t = Vx x + Vy y with the relation: Ï V x ¸ Ï c s ¸Ï V ¸ Ì ˝ = Ì ˝Ì ˝ Ó V y ˛ Ó – s c ˛Ó V t ˛

Ê c = cos q ˆ Ë c = sin q ¯

(11.3)

In axes ,t the stress acting on the surface with a normal x can be expressed as follows, using Equation 11.2 above: Ïc ¸ { s /x } ,t = [ s ij ] ,t { x } ,t = [ s ij ] ,t Ì ˝ Ós ˛ where {s/x} is the stress vector and [sij] is the stress matrix and in axes x,y, following Equation 11.3:

{ s /x } x,y =

© 2003 by CRC Press LLC

Ïc ¸ [ s ij ] ,t Ì ˝ –s c Ós ˛ c

s

TX846_Frame_C11 Page 225 Monday, November 18, 2002 12:26 PM

In a similar manner, the stresses acting on the surface with the normal y are written in the x,y axes as:

{ s /y } x,y =

Ï –s ¸ [ s ij ] ,t Ì ˝ c Óc˛

c

s

–s

Therefore, the matrix of stresses in the x,y axes is: c

{ s ij } x,y = [ s /x , s /y ] =

s

–s c

[ s ij ] ,t

c –s s

c

in setting:

c

[P] =

s

–s c

and observing that the matrix [P] is orthogonal ( [P] = [P] ), one has –1

t

4

[ s ij ] , t = [ P ] [ s ij ] x, y [ P ] t

t

where [P] is the transpose of matrix [P]. This expression can be developed to become

s t t s x t xy c s = c –s s c t xy s y – s c t t s t One can also rearrange the equation to be Ï s ¸ Ô Ô Ì st ˝ = Ô Ô Ó t t ˛

2

s

2

2

c s

sc

c

2

– sc

Ï sx ¸ Ô Ô 2cs Ì sy ˝ Ô Ô 2 2 ( c – s ) Ó t xy ˛ – 2cs

Then: [ s ] ,t = [ T ] [ s ] x,y 4

One has: sx,y = Ps,t P; st P = Psxy; Ps,t = sx,y P; s,t = Psx,yP.

© 2003 by CRC Press LLC

t

t

t

t

(11.4)

TX846_Frame_C11 Page 226 Monday, November 18, 2002 12:26 PM

5

with

c [T ] =

s

2

s

2

2

– 2sc

2

2sc

c

sc

(c – s ) 2

– sc

2

In a similar manner, the strain components can be transformed as: 2 2 Ï ex ¸ c s Ô Ô 2 Ì ey ˝ = s c2 Ô Ô – cs cs Ó e xy ˛

Ï e ¸ Ô Ô – 2cs Ì e t ˝ Ô 2 2 Ô ( c – s ) Ó e t ˛ 2cs

or: 2 Ï ex ¸ s c Ô Ô 2 2 s Ì ey ˝ = c Ô Ô Ó g xy ˛ – 2cs 2cs 2

Ï e ¸ Ô Ô Ì et ˝ – cs Ô Ô 2 2 ( c – s ) Ó g t ˛ cs

Ïe ¸ Ïe ¸ Ì ˝ = [T ¢]Ì ˝ Ó g ˛x,y Ó g ˛,t

then: with:

c [T ¢] =

s

2

2

s

2

cs

2

– cs

c

– 2cs 2cs

(c – s ) 2

2

The stress–strain Equation 11.1 can then be expressed in the axes x,y since we have written:

Ïe ¸ Ïe ¸ Ïe ¸ Ì ˝ = [T ¢]Ì ˝ ; Ì ˝ = Ó g ˛x,y Ó g ˛,t Ó g ˛,t

1 ----E

– n t ---------Et

– n t ---------E

1 ---Et

0

5

0

0 0 { s } ,t ; { s } ,t = [ T ] { s } x,y 1 -------G t

This [T ] matrix is readily established if one knows the relation that allows one to express the components of a tensor in one system in terms of the components of the same tensor in m m m another system. Here this relation is: s IJ = cos I cos J smn with cos I = cos(m,I ); see Section 13.1.

© 2003 by CRC Press LLC

TX846_Frame_C11 Page 227 Monday, November 18, 2002 12:26 PM

where after substitution: n t -------E t

1 ----E

n

[ T ¢ ] – ------t E

0

1 ---Et

0

Ï sx ¸ Ô Ô Ô Ô 0 [ T ] Ì sy ˝ Ô Ô Ô Ô 1 -------Ó t xy ˛ G t 0

Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

Ï ex ¸ Ô Ô Ô Ô Ì ey ˝ = Ô Ô Ô Ô Ó g xy ˛

new matrix of elastic coefficients in x,y axes

When all calculations are performed, one obtains the following constitutive relation, written in the coordinates x,y that make an angle q with the axes ,t. The elastic moduli and Poisson coefficients appear in these relations. One can also see the 6 existence of the coupling coefficients h and m, which demonstrates that a normal 7 stress can produce a distortion. Ï ex ¸ Ô Ô Ô Ô Ì ey ˝ = Ô Ô Ô Ô Ó g xy ˛

yx – ------E y

h xy -------G xy

xy – ------E x

1 --Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

n

1 --Ex

n

Ï sx ¸ Ô Ô Ô Ô Ì sy ˝ Ô Ô Ô Ô Ó t xy ˛

with: 1 E x ( q ) = ---------------------------------------------------------4 4 n tˆ 2 2 1 c s ----- + ---- + c s Ê -------- – 2 -----Et Et ¯ E Ë Gt 1 E y ( q ) = ---------------------------------------------------------4 4 n tˆ 2 2 1 s c ----- + ----- + c s Ê -------- – 2 -----Et Et ¯ E Ë Gt

(11.5)

1 -2 G xy ( q ) = ----------------------------------------------------------------------n tˆ ( c 2 – s 2 ) 2 2Ê 1 1 ------------------------------4c s E + E + 2 E + G Ë t t¯ t

6

7

n yx ------(q) Ey

=

n t 4 -----(c Et

h xy -------(q) G xy

Ï c2 s2 n t 2 2 1 ˆ¸ - – ---- + ( c – s ) Ê -----– ---------= – 2cs Ì ---E Et Ë Et 2Gt¯ ˝ Ó ˛

m xy -------(q) G xy

Ï s2 c2 n t 2 2 1 ˆ¸ - – ----- – ( c – s ) Ê -----– ---------= – 2cs Ì ---E Et Ë Et 2Gt¯ ˝ Ó ˛

4 2 2 1 1 1 - + ---- – ------ˆ + s ) – c s Ê ---Ë E Et Gt¯

Recall that the matrix of elastic coefficients is symmetric, meaning in particular: hxy /Gxy = hx /Ex and mxy /Gxy = my /Ey. See example described in Section 3.1.

© 2003 by CRC Press LLC

TX846_Frame_C11 Page 228 Monday, November 18, 2002 12:26 PM

11.2 STIFFNESS COEFFICIENTS When one inverts Equation 11.1 written in the coordinate axes l,t of a ply, one obtains n E

------------------Ï s ¸ ( 1 – n t n tl ) Ô Ô n t E t Ô Ô Ì s t ˝ = (-------------------1 – n t n t ) Ô Ô Ô Ô 0 Ó t t ˛

E

0 Ï e ¸ Ô Ô Ô Ô 0 Ì et ˝ Ô Ô Ô Ô G t Ó g t ˛

t --------------------

( 1 – n t n t ) Et -------------------( 1 – n t n t )

0

where the “stiffness” coefficients appear, as opposed to the Equation 11.1 where the “compliance” coefficients appear. To simplify the writing, one can denote Ï sl ¸ E Ô Ô Ì s t ˝ = n t E t Ô Ô 0 Ó t t ˛

0 Ï e ¸ Ô Ô 0 Ì et ˝ Ô Ô G t Ó g t ˛

n t E Et 0

(11.6)

An identical procedure can be followed to arrive at the stress–strain relation: c s

2

2

– cs

s

2

c

2

Ï s ¸ Ô Ô – 2cs Ì s t ˝: Ô Ô 2 2 ( c – s ) Ó t t ˛ 2cs

cs

Ï Ô Ô Ô Ì Ô Ô Ô Ó

Ï sx ¸ Ô Ô Ì sy ˝ = Ô Ô Ó t xy ˛

[ T1 ] (11.7) 2

s

2

2

c

2

c s

2cs

– 2c s

–c s cs (c – s ) 2

2

Ï ex ¸ Ô Ô Ì ey ˝ Ô Ô Ó g xy ˛

Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

Ï e ¸ Ô Ô Ì et ˝ = Ô Ô Ó g t ˛

[ T 1¢ ] Recall that axes x,y are derived from the axes ,t by a rotation q about the third axis z. Substituting Equations 11.7 into 11.6, one obtains Ï sx ¸ E Ô Ô Ì s y ˝ = [ T 1 ] n t E t Ô Ô 0 Ó t xy ˛

n t E Et 0

Ï ex ¸ Ô Ô 0 [ T 1¢ ] Ì e y ˝ Ô Ô G t Ó g xy ˛ 0

which can be rewritten as: Ï sx ¸ E 11 E 12 E 13 Ô Ô Ì s y ˝ = E 21 E 22 E 23 Ô Ô Ó t xy ˛ E 31 E 32 E 33

© 2003 by CRC Press LLC

Ï ex ¸ Ô Ô Ì ey ˝ Ô Ô Ó g xy ˛

TX846_Frame_C11 Page 229 Monday, November 18, 2002 12:26 PM

Once the calculations are performed, one obtains the following expressions for the stiffness coefficients E ij , where c = cosq and s = sinq.

Ï sx ¸ E 11 E 12 E 13 Ô Ô s = Ì y˝ E 21 E 22 E 23 Ô Ô t Ó xy ˛ E 31 E 32 E 33

Ï ex ¸ Ô Ô Ì ey ˝ Ô Ô Ó g xy ˛

with: E 11 ( q ) = c E + s E t + 2c s ( n t E + 2G t ) 4

4

2 2

E 22 ( q ) = s E + c E t + 2c s ( n t E + 2G t ) 4

4

2 2

2 2

E 33 ( q ) = c s ( E + E t – 2 n t E ) + ( c – s ) G t 2 2

2

(11.8)

E 12 ( q ) = c s ( E + Et – 4G t ) + ( c + s ) n t E 2 2

4

4

E 13 ( q ) = – cs { c E – s E t – ( c – s ) ( n t E + 2G t ) } 2

2

2

2

E 23 ( q ) = – cs { s E – c E t + ( c – s ) ( n t E + 2G t ) } 2

2

2

2

expressions in which: E = E / ( 1 – n t n t ) : E t = E t / ( 1 – n t n t ) The rate of variation of stiffness coefficients E ij as functions of the angle q is repre sented in Figure 11.2 for a ply characterized by moduli E and Et with very different 8 values, for example the case of unidirectional layers of fiber/resin.

11.3 CASE OF THERMOMECHANICAL LOADING 11.3.1 Compliance Coefficients 9

When considering the temperature variations, one must substitute the stress–strain Equation 11.1 with Equation 10.9: Ï e ¸ Ô Ô Ô Ô Ì et ˝ = Ô Ô Ô Ô Ó g t ˛ 8 9

1 ----E

n

n

t – -----E t

t – -----E

1 ---Et

0

0

0 Ï s ¸ Ï a ¸ Ô Ô Ô Ô Ô Ô Ô Ô 0 Ì s t ˝ + DT Ì a t ˝ Ô Ô Ô Ô Ô Ô Ô 1 Ô -------Ó0˛ G t Ó t t ˛

See characteristics of the fiber/resin unidirectionals in Paragraph 3.3.3. See Section 10.5.

© 2003 by CRC Press LLC

TX846_Frame_C11 Page 230 Monday, November 18, 2002 12:26 PM

Figure 11.2 Variation of Stiffness Coefficients for a Misaligned Ply

in which a and a t are the coefficients of thermal expansion of the unidirectional layer along the longitudinal direction and transverse direction t, respectively. Following the same procedure as in Section 11.1 with the same notations, one can write

Ïe ¸ Ïe ¸ Ì ˝ = [ T ¢ ] Ì ˝ ; { s } ,t = [ T ] { s } x,y Ó g ˛x,y Ó g ˛,t

© 2003 by CRC Press LLC

TX846_Frame_C11 Page 231 Monday, November 18, 2002 12:26 PM

Then, upon substituting, Ï ex ¸ Ô Ô Ô Ô Ì ey ˝ = [ T ¢ ] Ô Ô Ô Ô Ó g xy ˛

1 ----E

n

n

t – -----E

0

t

t – -----E

1 ---Et

0

0

0

1 -------G t

Ï a ¸ Ï sx ¸ Ô Ô Ô Ô Ô Ô Ô Ô [ T ] Ì s y ˝ + DT [ T ¢ ] Ì a t ˝ Ô Ô Ô Ô Ô Ô Ô Ô Ó0˛ Ó t xy ˛

One finds again in the first part of the second term a matrix of compliance coefficients, the terms of which are described in details in Equation 11.5. The second part of the second term is written as: 2

s

2

2

c

2

– 2 cs

2cs

c DT

s

Ï a ¸ Ï c a + s at ¸ Ô Ô Ô Ô – c s Ì a t ˝ = DT Ì s 2 a + c 2 a t ˝ Ô Ô Ô Ô 2 2 Ó 2cs ( a t – a ) ˛ (c – s ) Ó 0 ˛ 2

cs

2

Therefore, the thermomechanical relation for a unidirectional layer written in the axes x.y, different from the ,t coordinates, can be summarized as follows:

h xy -------G xy

n

1 yx ----- – ------Ï ex ¸ Ex Ey Ô Ô Ô Ô n xy 1 ----Ì e y ˝ = – ------Ey Ex Ô Ô hx my Ô Ô ---------Ó g xy ˛ Ex Ey

m xy -------G xy 1 -------G xy

Ï sx ¸ Ô Ô Ô Ô Ì s y ˝ + DT Ô Ô Ô Ô Ó t xy ˛

Ï ax ¸ Ô Ô Ô Ô Ì ay ˝ Ô Ô Ô Ô Ó a xy ˛

E x , E y ,G xy , n xy , n yx , h xy , m xy are given by the relations [11.5]

ax = c a + s at 2

2

ay = s a + c at 2

2

a xy = 2cs ( a t – a ) c = cos q ; s = sin q

© 2003 by CRC Press LLC

(11.9)

TX846_Frame_C11 Page 232 Monday, November 18, 2002 12:26 PM

11.3.2 Stiffness Coefficients Inverting Equation 10.9 gives

E

n E

t -------------------- -------------------- 0 Ï s ¸ ( 1 – n t n t ) ( 1 – n t n t ) Ô Ô Ô Ô n t E t Et - -------------------- 0 Ì s t ˝ = -------------------( 1 – n t n t ) ( 1 – n t n t ) Ô Ô Ô Ô Ó t t ˛ G t 0 0

Ï e ¸ Ô Ô Ô Ô Ì e t ˝º Ô Ô Ô Ô Ó g t ˛ n E

E

t Ï --------------------------------------- ¸ Ô ( 1 – nt nt ) a + ( 1 – nt nt ) a t Ô Ô Ô º – DT Ì nt Et Et ˝ --------------------------------------a + a l t Ô ( 1 – nt nt ) ( 1 – n t n t ) Ô Ô Ô 0 Ó ˛

Following the procedure of Section 11.2, with the same notations, one can write: Ïe ¸ Ïe ¸ { s } x,y = [ T l ] { s } ,t ; Ì ˝ = [ T 1¢ ] Ì ˝ Ó g ˛,t Ó g ˛x,y where after substitution: Ï E a + n t E a t ¸ Ï sx ¸ Ï ex ¸ E n t E 0 Ô Ô Ô Ô Ô Ô Ì s y ˝ = [ T l ] n t E t Et 0 [ T 1¢ ] Ì e y ˝ – DT [ T l ] Ì n t E t a + E t a t ˝ Ô Ô Ô Ô Ô Ô 0 0 0 G t Ó ˛ Ó t xy ˛ Ó g xy ˛ One finds again, in the first part of the second term, the matrix detailed in Equation 11.8. The second part of the second term can be developed as follows:

c – DT

s

2

2

– cs

s

2

c

2

cs

2cs Ï E a + n t E a t ¸ Ô Ô – 2c s Ì n t E t a + E t a t ˝ = º Ô Ô 2 2 0 ˛ (c – s ) Ó Ï c E ( a + n t a t ) + s E t ( n t a + a t ) ¸ Ô Ô º – DT Ì s 2 E ( a + n t a t ) + c 2 E t ( n t a + a t ) ˝ Ô Ô Ó cs [ E t ( n t a + a t ) – E ( a + n t a t ) ] ˛ 2

© 2003 by CRC Press LLC

2

TX846_Frame_C11 Page 233 Monday, November 18, 2002 12:26 PM

Therefore, the thermomechanical behavior of a unidirectional layer in the coordinate axes x,y can be written in the following form, in terms of the properties in the ,t coordinates.

Ï sx ¸ E 11 E 12 E 13 Ô Ô Ì s y ˝ = E 21 E 22 E 23 Ô Ô Ó t xy ˛ E 31 E 32 E 33

Ï ex ¸ Ô Ô Ì e y ˝ – DT Ô Ô Ó g xy ˛

Ï a E1 ¸ Ô Ô Ì a E2 ˝ Ô Ô Ó a E3 ˛

E 11 E 22 E 33 E 12 E 13 E 23 are given by the relations [11.8]

a E 1 = c E ( a + n t a t ) + s E t ( n t a + a t ) 2

2

a E 2 = s E ( a + n t a t ) + c E t ( n t a + a t ) 2

2

a E 3 = cs [ E t ( n t a + a t ) – E ( a + n t a t ) ] c = cos q ; s = sin q E = E / ( 1 – n t n t ) E t = E t / ( 1 – n t n t )

© 2003 by CRC Press LLC

(11.10)

TX846_Frame_C12 Page 235 Monday, November 18, 2002 12:27 PM

12 MECHANICAL BEHAVIOR OF THIN LAMINATED PLATES 1

The definition of a laminate was given in Chapter 5. In the same chapter the practical calculation methods for the laminate was also described. We propose here to justify these methods, meaning to study the behavior of the laminate when it is subjected to a combination of loadings. This study is necessary if one wants 2 to have correct design with strains or stresses within their admissible values.

12.1 LAMINATE WITH MIDPLANE SYMMETRY 12.1.1

Membrane Behavior 3

We consider in the following a laminate with midplane symmetry. The total thickness of the laminate is denoted as h. It consists of n plies. Ply number k has a thickness denoted as ek (see Figure 12.1). Plane x, y is the plane of symmetry.

12.1.1.1 Loadings The laminate is subjected to loadings in its plane. The stress resultants are denoted as Nx, Ny, Txy = Tyx. These are the membrane stress resultants.They are defined as: Nx: Stress resultant in the x direction over a unit width along the y direction. th

Nx =

Ú

n ply

h/2 – h/2

s x dz =

Â

( sx )k ¥ ek

(12.1)

st

k=1 ply

Ny: Stress resultant along the y direction over a unit width along the x direction. th

Ny =

1 2 3

Ú

h/2 – h/2

n ply

s y dz =

Â

( sy )k ¥ ek

(12.2)

st

k=1 ply

See Section 5.2. The problem of buckling of the laminates is not the scope of this chapter. See Appendix 2. See Section 5.2.3.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 236 Monday, November 18, 2002 12:27 PM

Figure 12.1 Definition of Laminate and Membrane Loading

Txy (or Tyx ): Membrane shear stress resultant over a unit width along the y direction (or respectively along the x direction): th

T xy =

Ú

n ply

h/2 – h/2

Â

t xy dz =

( t xy ) k ¥ e k

(12.3)

st

k=1 ply

12.1.1.2 Displacement Field The elastic displacement at each point of the laminate is assumed to be two dimensional, in the x, y plane of the laminate. It has the components: uo , vo. The nonzero strains can be written as:

e ox = ∂ u 0 / ∂ x e oy = ∂ v 0 / ∂ y g oxy = ∂ u 0 / ∂ y + ∂ v 0 / ∂ x It was shown in the previous chapter (Equation 11.8) that one can express, in a given coordinate system, the stresses in a ply as functions of the strains. Then the stress resultant Nx defined in Equation 12.1 can be written as follows: th

n ply

Nx =

Â

k

k

k

{ E 11 e ox + E 12 e oy + E 13 g oxy }e k

st

k=1 ply

then: N x = A 11 e ox + A 12 e oy + A 13 g oxy © 2003 by CRC Press LLC

TX846_Frame_C12 Page 237 Monday, November 18, 2002 12:27 PM

with: th

th

n ply

A 11 =

Â

th

n ply

Â

k 11 k

E e ; A 12 =

st

n ply k 12 k

E e ; A 13 =

st

k=1 ply

Â

k

E 13 e k

st

k=1 ply

k=1 ply

In an analogous manner, one obtains for the Equation 12.2: N y = A 21 e ox + A 22 e oy + A 23 g oxy with: th

n ply

Â

A 2j =

k

E 2j e k

st

k=1 ply

and for the shear stress resultant Txy one can write, starting from Equation 12.3: T xy = A 31 e ox + A 32 e oy + A 33 g oxy with: th

n ply

Â

A 3j =

k

E 3j e k

st

k=1 ply

Therefore, it is possible to express the stress resultants in the following matrix form: Ï Nx ¸ A 11 A 12 A 13 Ô Ô N = Ì y˝ A 21 A 22 A 23 Ô Ô T A 31 A 32 A 33 Ó xy ˛ with:

Ï e ox ¸ Ô Ô Ì e oy ˝ Ô Ô Ó g oxy ˛

4

(12.4)

th

n ply

A ij =

Â

k

E ij e k = A ji

st

k=1 ply

Remarks: One observes from the above expressions that coefficients Aij are independent of the stacking order of the plies. One can also see that the normal stress resultants Nx or Ny create angular distortions. This coupling will disappear if the laminate is balanced. This means that apart from the midplane symmetry, there are as many and identical plies that make with the x axis an angle +q as those that make 4

The developments of E ij are given in Equation 11.8.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 238 Monday, November 18, 2002 12:27 PM

with the x axis an angle -q. In effect, the coefficients E 13 and E 23 are 6 antisymmetric in q and, therefore, cancel each other out for the pairs of plies at ±q when one calculates the terms A13 and A23. The result is then: 5

A 13 = A 23 = 0 and the stress–strain relation for the laminate is reduced to Ï Nx ¸ A 11 A 12 0 Ô Ô N = Ì y˝ A 12 A 22 0 Ô Ô 0 0 A 33 Ó T xy ˛

Ï e ox ¸ Ô Ô Ì e oy ˝ Ô Ô Ó g oxy ˛

(12.5)

It is possible to substitute the stress resultants Nx, Ny, Txy with the global average stresses (which are fictitious):

s ox = N x /h s oy = N y /h

(12.6)

t oxy = T xy /h One then deduces from Equation 12.4 the average membrane stress–strain behavior of a laminate as: Ï s ox ¸ A 11 A 12 A 13 Ô Ô 1 -s = Ì oy ˝ h A 21 A 22 A 23 Ô Ô t A 31 A 32 A 33 Ó oxy ˛

Ï e ox ¸ Ô Ô Ì e oy ˝ Ô Ô Ó g oxy ˛

(12.7)

One can also note that according to Equation 12.4 the terms of the matrix 1 ---[A] above can be written as: h th

1 --- ¥ A ij = h

n ply

Â st

e k E ij ¥ ----k h

k=1 ply

Then the ratios ek /h can be rearranged to obtain the proportions of plies having the same orientation. In case where these proportions have already been fixed—and therefore their numerical values are known—it becomes possible to calculate the terms --h1-Aij without knowing the thickness. For example, if the selected orientak tions are 0∞, 90∞, +45∞, -45∞, and by denoting p (%) as the percentages of the plies along the different orientations, one has: 1 --- ¥ A ij = E ij0∞ ¥ p 0∞ + E ij90∞ ¥ p 90∞ + E ij+45∞ ¥ p +45∞ + E ij-45∞ ¥ p -45∞ h 5 6

See Figure 12.1 and figure in the Equation 11.8. The expressions developed for E ij are given in Equation 11.8.

© 2003 by CRC Press LLC

(12.8)

TX846_Frame_C12 Page 239 Monday, November 18, 2002 12:27 PM

Figure 12.2 Practical Determination of a Laminate Subject to Membrane Loading

12.1.2 Apparent Moduli of the Laminate Inversion of Equation 12.7 above allows one to obtain what can be called as apparent moduli and coupling coefficients associated with the membrane behavior in the plane x,y. These coefficients appear in the following relation: Ï e ox ¸ Ï s ox ¸ Ô Ô Ô Ô Ô Ô Ô –1 Ô Ì e oy ˝ = h [ A ] Ì s oy ˝ = Ô Ô Ô Ô Ô Ô Ô Ô Ó g oxy ˛ Ó t oxy ˛

1 ----Ex

yx –n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï s ox ¸ Ô Ô Ô Ô Ì s oy ˝ Ô Ô Ô Ô Ó t oxy ˛

(12.9)

12.1.3 Consequence: Practical Determination of a Laminate Subject to Membrane Loading Given: The stress resultants are given and denoted as: Nx, Ny, Txy. Using the values of these stress resultants, one can estimate the ply 7 proportions in the four orientations. Assume in Figure 12.2 that the plies are identical (same material and same thickness). The problem is to determine The apparent elastic moduli of the laminate and the associated coupling coefficients, in order to estimate strains under loading The minimum thickness for the laminate in order to avoid rupture of one of the plies in the laminate

7

See Section 5.4.3.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 240 Monday, November 18, 2002 12:27 PM

12.1.3.1 Principle of Calculation Apparent moduli of the laminate: The matrix --h1-[A] evaluated using Equation 12.8 can be inverted, and one obtains Equation 12.9 as: Ï e ox ¸ Ô Ô Ô Ô Ì e oy ˝ = Ô Ô Ô Ô Ó g oxy ˛

1 ----Ex

yx –n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï s ox ¸ Ô Ô Ô Ô Ì s oy ˝ Ô Ô Ô Ô Ó t oxy ˛

We have already determined the apparent moduli and the coupling coefficients of the laminate. Nonrupture of the laminate: Let s, st, and tt be the stresses in the orthotropic axes , t of one of the plies making up the laminate that is subjected to the loadings Nx, Ny, Txy. Let h be the thickness of the laminate (unknown at the moment) so that the rupture limit of the ply using the Hill–Tsai failure criterion is just reached. 8 One then has for this ply :

s s t s s t t t -----2 + -----2 – ---------- = 1 + ----2 2 s st s t t 2

2

2

rupture rupture rupture rupture

Multiplying the two parts of this equation with the square of thickness h: ( s h ) ( s t h ) ( s h ) ( s t h ) ( t t h ) --------------- + -------------- – --------------------------- = h2 - + --------------2 2 2 2 s st t t s 2

rupture

2

rupture

2

rupture

(12.10)

rupture

To obtain the values (s h), (sth), (tt h), one has to multiply with h the global stresses sox, soy, toxy that are applied on the laminate, to become (soxh), (soy h), (toxy h) which are the known stress resultants: N x = ( s ox h ); N y = ( s oy h ); T xy = ( t oxy h ) Then, for a ply, the calculation of the Hill–Tsai criterion can be done by substituting for the unknown global stresses the known stress resultants Nx, Ny, Txy. This leads to the calculation of the thickness h so that the ply under consideration does not fracture. In this way, each ply number k leads to a laminate thickness value denoted as hk. The final thickness to be retained will the one with the highest value. 8

For the Hill–Tsai failure criterion, see Section 5.2.3 and detailed explanation in Chapter 14.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 241 Monday, November 18, 2002 12:27 PM

12.1.3.2 Calculation Procedure 1. Complete calculation: The ply proportions are given, the matrix --h1- [A] of the Equation 12.7 is known, and then—after inversion—we obtain the 9 elastic moduli of the laminate (Equation 12.9). Multiplying 12.9 with the thickness h (unknown) of the laminate: 1 ----Ï h e ox ¸ Ex Ô Ô Ô Ô xy Ì h e oy ˝ = –n------Ex Ô Ô Ô Ô hx -----Ó h g oxy ˛ E

yx –n------Ey

h xy -------G xy

1 ----Ey

m xy -------G xy

my

1 -------G xy

----

Ey

x

Ï Nx ¸ Ô Ô Ô Ô Ì Ny ˝ Ô Ô Ô Ô Ó T xy ˛

Then introducing a multiplication factor of h for the stresses in the ply—or the group of plies—corresponding to the orientation k (see Equation 11.8): E 11 Ï h sx ¸ Ô Ô Ì h s y ˝ = E 21 Ô Ô E 31 Ó h t xy ˛ ply n∞k

E 12 E 22 E 32

E 13 Ï h e ox ¸ Ô Ô E 23 Ì h e oy ˝ Ô Ô E 33 Ó h g oxy ˛

ply n∞k

laminate

and in the orthotropic coordinates of the ply (see Equation 11.4): 2 2 Ï h s ¸ s – 2cs c Ô Ô 2 2 h s = Ì t˝ c 2cs s Ô Ô 2 2 h t Ó t ˛ sc – sc ( c – s )

Ï h sx ¸ Ô Ô Ì h sy ˝ Ô Ô Ó h t xy ˛

ply n∞k

ply n∞k

ply n∞k

c = cos q ; s = sin q

Saturation of the Hill–Tsai criterion leads then to Equation 12.10 where the above known stress resultants values appear in the numerator as: ( h s ) ( h s t ) ( h s ) ( h s t ) ( h t t ) --------------- + -------------- – --------------------------- = h2 ¥ 1 - + ------------2 2 2 2 s st t t s 2

rupture

2

2

rupture

rupture

rupture

After having written an analogous expression for each orientation k of the plies, one retains for the final value of the laminate thickness, the maximum value found for h. 9

One can read directly these moduli in Tables 5.1 to 5.15 of Section 5.4.2 for balanced laminates of carbon, Kevlar, and glass/epoxy with Vf = 60% fiber volume fraction.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 242 Monday, November 18, 2002 12:27 PM

(2) Simplified calculation: One can write more rapidly the Equation 12.10 if one knows at the beginning for each orientation the stresses due to a global uniaxial state of unit stress applied on the laminate: first s ¢ox = 1 (for example, 1 MPa), then s ¢¢oy = 1 MPa, then t ¢¢¢ oxy = 1 MPa. Assume first that the state of stress is given as: ¢ = 1 ( MPa ) s ox

s ox ¢ = 0 t ¢oxy = 0 Inverting the Equation 12.9 leads to Ï e o¢ x Ô Ô Ì e o¢ y Ô Ô ¢ Ó g oxy

¸ Ô Ô ˝ = Ô Ô ˛

1 ----Ex

yx –n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï 1 MPa ¸ Ô Ô Ô Ô Ì 0 ˝ Ô Ô Ô Ô Ó 0 ˛

which can be considered as “unitary strains” of the laminate. These allow the calculation of the stresses in each ply by means of Equations 11.8 and then 11.4, successively, as: Ï s ¢x Ô Ì s ¢y Ô Ó t x¢ y

E 11 ¸ Ô ˝ = E 21 Ô E 31 ˛

ply n∞k

E 12 E 22 E 32

E 13 Ï e o¢ x Ô E 23 Ì e o¢ y Ô E 33 Ó g o¢ xy

ply n∞k

¸ Ô ˝ Ô ˛

laminate

and in the orthotropic coordinates of the ply (Equation 11.4): Ï s ¢ Ô Ì s ¢t Ô Ó t ¢ t

2 2 ¸ s – 2cs c Ô 2 2 = ˝ c 2cs s Ô 2 2 ˛ sc – sc ( c – s )

ply n∞k

ply n∞k

Ï s ¢x Ô Ì s ¢y Ô Ó t ¢x y

¸ Ô ˝ Ô ˛

c = cos q s = sin q

ply n∞k

Consider then the state of stresses:

s ox ≤ = 0 s oy ≤ = 1 ( MPa ) ≤ = 0 t oxy Following the same procedure, one can calculate s ¢¢ , s ¢¢t , and t ¢¢t in the orthotropic axes of each ply for a global stress on the laminate that is reduced to s ¢¢oy = 1 MPa. © 2003 by CRC Press LLC

TX846_Frame_C12 Page 243 Monday, November 18, 2002 12:27 PM

Finally consider the state of stresses: ¢¢¢ = 0 s ox ¢¢¢ = 0 s oy ¢¢¢ = 1 ( MPa ) t oxy Following the same procedure, one obtains s ¢¢ , s ¢¢t , and t ¢¢t in the orthotropic axes of each ply for a global stress applied on the laminate, and that is reduced ¢¢ = 1 MPa.10 to t oxy 11 It is then easy to determine by simple rule of proportion (or multiplication) the quantities (s h), (sth), and (tt h) in each ply, corresponding to loadings that are no longer unitary, but equal successively to N x = ( s ox h ) then: N y = ( s oy h ) then: T xy = ( t oxy h ) Subsequently, the principle of superposition allows one to determine (sh)total (sth)total and (tth)total when one applies simultaneously Nx, Ny, and Txy. From these it is possible to write the modified Hill–Tsai expression in the form of Equation 12.10, which will provide the thickness for the laminate needed to avoid the fracture of the ply under consideration. If hk is the laminate thickness obtained from the ply number k, after having gone over all the plies, one will retain for the final thickness h the thickness of highest value found as: h = sup {hk}

12

Remark: The principle of calculation is conserved when the plies have different thicknesses with any orientations. It then becomes indispensable to program the procedure, or to use existing computer programs. Then one can propose a complete composition for the laminate and verify that the solution is satisfactory regarding the criterion mentioned previously (deformation and fracture). This is 10

11

This calculation can be easily programmed on a computer: cf. Application 18.2.2 “Program for Calculation of a Laminate.” One will find in Appendix 1 at the end of the book the values s, st, tt obtained for the particular case of a carbon/epoxy laminate with ply orientations of 0∞, 90∞, +45∞, -45∞. These values are given in Plates 1 to 12. For example, one has the following:

s ox ¢ = 1 MPa Æ s ¢ , s t¢, t t¢ s ox ( MPa ) then: 12

Æ s , s t , t t

s ox s s ox s ¢ -------- = ----- fi s = s ¢ ¥ -------, - ¥ Nx and h s = -----1 1 ¢ ¢ s ox s

This method to determine the thickness is illustrated by an example: See Application 18.1.6.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 244 Monday, November 18, 2002 12:27 PM

Figure 12.3 Bending of the Laminate

facilitated by using the user friendly aspect of the program, allowing rapid return of the solution.

12.1.4

Flexure Behavior

In the previous paragraph, we have limited discussion to loadings consisting of Nx, Ny, and Txy applying in the midplane of the laminate. We will now examine the cases that can cause deformation outside of the plane of the laminate. The laminate considered is—as before—supposed to have midplane symmetry.

12.1.4.1 Displacement Fields Hypothesis: Assume that a line perpendicular to the midplane of laminate before deformation (see Figure 12.3) remains perpendicular to the midplane surface after deformation. Consequence: If one denotes as before uo and vo the components of the displacement in the midplane and wo as the displacement out of the plane (see Figure 12.3), the displacement of any point at a position z in the laminate (in the nondeformed configuration) can be written as

∂ w0 Ï u = u o – z -------Ô ∂x Ô w0 Ì v = v – z ∂-------o Ô ∂y Ô Ów = w o

(12.11)

One can then deduce the nonzero strains: 2 Ï ∂ w0 Ô e x = e ox – z ----------2 Ô ∂x Ô 2 Ô ∂ w0 Ì e y = e oy – z ----------2 Ô ∂y Ô 2 Ô ∂ w0 Ô g xy = g oxy – z ¥ 2 ------------∂x∂y Ó

© 2003 by CRC Press LLC

(12.12)

TX846_Frame_C12 Page 245 Monday, November 18, 2002 12:27 PM

Figure 12.4 Moment Resultants

12.1.4.2 Loadings In addition to the membrane stress resultants Nx, Ny, Txy in the previous paragraphs, one can add the moment resultants along the x and y directions (see Figure 12.4). As in the case of the membrane stress resultants, the moment resultants serve to synthesize the cohesive forces that appear by sectioning, following classical method that is common for all structures (beams, plates, etc.). One can interpret 13 these as the unit moments of the cohesive forces. They are written as: My: Moment resultant along the y axis, due to the stresses sx, over a unit width along the y direction. My =

Ú

h/2 – h /2

s x z dz

(12.13)

Mx: Moment resultant along the x direction, due to the stress sy, over a unit width along the x direction. Mx = –

Ú

h/2 – h /2

s y z dz

(12.14)

Mxy: (or –Myx): Twisting moment along the x axis (or y axis), due to the shear stress txy over a unit width along the y direction (or x direction): M xy = – 13

Ú

h/2 – h /2

t xy z dz

(12.15)

The expression of My can be written in integral form as:

Ú–h /2 sx z dz

My =

Ú–h /2 zz Ÿ sx xdz

Mx =

Ú–h /2 zz Ÿ sy ydz

. x = – Ú–h /2 s y z dz

M xy =

Ú–h /2 zz Ÿ txy ydz

. x = – Ú–h /2 t xy z dz

h/2

.y =

h/2

also: h/2

h/2

Finally:

© 2003 by CRC Press LLC

h/2

h/2

TX846_Frame_C12 Page 246 Monday, November 18, 2002 12:27 PM

Taking Equation 11.8 into consideration, which allows one to express, in a certain coordinate system, the stresses in a ply as functions of strains, the moment resultant My (Equation 12.13) can be written as: th

n ply

Ï

Â ÌÓ Ú

My =

zk z k-1

st

k=1 ply

¸ ( E 11k e x + E 12k e y + E 13k g xy )z dz ˝ ˛

which, when using Equation 12.12 becomes th

n ply

My =

Ï Ì Ó

Ï kÊ ∂ w oˆ º 2 ∂ w oˆ - + E 12k Ê z e oy – z 2 ----------E z e ox – z ----------z k-1 Ì 11 Ë 2 ¯ 2 Ë ∂x ∂y ¯ Ó 2

Â Ú st

k=1 ply

zk

2

¸ ∂ w oˆ ¸ º + E 13k Ê z g oxy – z 2 2 -----------dz ˝ Ë ∂ x ∂ y¯ ˝˛ ˛ 2

Due to midplane symmetry, every integral of the form:

Ú

zk z k-1

E lj z dz

in the above expression is accompanied by an integral of the form:

Ú

– z k-1 –zk

E lj z dz

that is opposite in sign. Integrals of this type disappear and there remains th

n ply

My =

Â st

k=1 ply

Ï k ( z k – z k-1 ) ∂ w o k ( z k – z k-1 ) ∂ w o … ------------------------- ----------------------------------- ----------- + E 12 – Ì E 11 2 2 3 3 ∂x ∂y Ó 3

3

3

2

3

2

k ( z k – z k-1 ) ∂ w o ¸ … + E 13 ------------------------- 2 ------------- ˝ 3 ∂x∂y ˛ 3

3

which can be written as: 2 2 ∂ w ∂ wo ∂ wo – M y = -C 11 ----------C ----------- – C 13 2 ------------o12 2 2 ∂ x∂y ∂x ∂y 2

with th

n ply

C 1j =

Â st

k=1 ply

© 2003 by CRC Press LLC

( z k – z k-1 ) E 1jk -----------------------3 3

3

2

TX846_Frame_C12 Page 247 Monday, November 18, 2002 12:27 PM

Proceeding in an analogous manner with Mx and Mxy (Equations 12.14 and 12.15), one obtains the following matrix form: Ï ∂ w ¸ C 13 Ô – ------------2o- Ô ∂x Ô Ô Ô ∂ 2w Ô C 23 Ì – -------------o- ˝ Ô ∂ y2 Ô Ô Ô C 33 Ô ∂ 2 wo Ô Ó – 2 -----------∂x∂y ˛ 2

C 11 Ï My ¸ Ô Ô Ô Ô Ì – M x ˝ = C 21 Ô Ô Ô Ô C 31 Ó – M xy ˛

C 12 C 22 C 32

(12.16)

with : th

n ply

C ij =

Â st

( z k – z k-1 ) E ijk -----------------------3 3

3

k=1 ply

Remarks: One can observe that in Equation 12.16 the coefficients Cij depend on the stacking sequence of the plies. Does a laminated plate bend under membrane loadings? Using the displacement field due to flexure to express, for example, the stress resultant Nx (Equation 12.11), one has th

n ply

Nx =

Ï Ì Ó

Ï kÊ ∂ w oˆ ∂ w oˆ … k Ê - + E 12 E e – z ----------e oy – z ----------z k – 1 Ì 11 Ë ox 2 ¯ 2 Ë ∂x ∂y ¯ Ó 2

Â Ú st

k=1 ply

zk

2

¸ ∂ w ¸ k Ê … + E 13 g – z ¥ 2 ------------o-ˆ¯ ˝ dz ˝ Ë oxy ∂x∂y ˛ ˛ 2

Making use of the remark mentioned above, the midplane symmetry causes the disappearance of integrals of the type:

Ú

zk z k-1

E ljk z dz

As a consequence, one finds again the Equation 12.4 as: N 1 = A 11 e ox + A 12 e oy + A 13 g oxy As a result of the midplane symmetry, the membrane behavior is independent of the flexural behavior. Even in the case of balanced laminate (as many plies oriented at angle q as the number of plies oriented at an angle -q), terms C13 and C23 in Equation 12.16 are not zero. This modifies the deformed bending configuration compared with the isotropic case (see Figure 12.5). © 2003 by CRC Press LLC

TX846_Frame_C12 Page 248 Monday, November 18, 2002 12:27 PM

Figure 12.5 Bending Configurations of a Plate

The terms C13 and C23 disappear only in the following cases: The plies are oriented uniquely in the 0∞ and 90∞. Then the product 14 cosq ¥ sinq is zero and : k k E 13 = E 23 = 0

"k

The laminate [0/90/45/-45] is constituted mainly with balanced fabric layers (in each fabric layer, the fibers along the warp and fill directions 15 are, by first approximation at the same z location), or mats layers. The stresses in the different plies are obtained from the Equations 11.8. For example, in the ply number k, one has: k k k s x = E 11 e x + E 12 e y + E 13 g xy

and taking into consideration Equations 12.12 for the strains: k k k k ∂ wo º ----------s x = [ E 11 e ox + E 12 e oy + E 13 g oxy ] – z E 11 2 ∂x 2

∂ w k ∂ wo k º + E 12 ----------- + E 13 ¥ 2 ------------o2 ∂ x∂y ∂y 2

2

one can resume by:

s x = s xmembrane + s xflexure Along the thickness of the laminate, the stress sx can be considered as the sum of two parts: a constant part and a linearly varying part, as seen in Figure 12.6. One can also observe analogous forms for the stresses sy and txy .

14 15

See Equations 11.8 See Section 5.2.3.5, Particular Cases of Balanced Fabrics.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 249 Monday, November 18, 2002 12:27 PM

Figure 12.6 Total Normal Stress in a Laminate

12.1.5 Consequence: Practical Determination for a Laminate Subject to Flexure Given: The moment resultants are known. Using these resultants, one is led to estimate proportions of plies along 16 the four orientations (or more, eventually) and to predict the stacking sequence. Principle for the calculation: Nonrupture of laminate: Following a procedure analogous to that described in Section 12.1.3, it is possible to calculate the stresses s, st, tt along the orthotropic axes of each of the plies. This allows the control of their integrity using the Hill–Tsai failure criterion. This requires the use of a computer program which can allow the adjustment of the composition of the laminate. Flexure deformation: The determination of the deformed configuration of the laminate under flexure poses the same problem as with the isotropic plates: outside of a few cases of academic interest, it is necessary to use 17 a computer program based on the finite element method.

12.1.6 Simplified Calculation for Flexure It is possible, for a first estimate, to perform simplified calculations by considering that 2 ∂ wo ----------the moment M is related uniquely to the curvature and the moment Mx to the y 2 2 ∂x wo curvature ∂-----------. One then can determine experimentally: 2 ∂y

1. The apparent failure stresses in flexure An experiment on a sample can provide the value for the moment at failure, denoted by Mrupture on Figure 12.7 (per unit width of the sample). Analogy with 16 17

See Section 5.2. These elements are constituted on the basis presented above and can include the effects which were not taken into account previously: in particular, the transverse shear stresses in flexure due to the transverse shear stress resultants (consult this subject in Chapter 17).

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 250 Monday, November 18, 2002 12:27 PM

Figure 12.7 Bending Failure

Figure 12.8 Homogeneous and Laminated Beams

the flexure of beams leads to: M rupture ¥ h/2 6 then: s rupture = M rupture ¥ -----2 s rupture = ------------------------------3 h /12 h 2. Apparent flexure moduli These are obtained starting from the comparison of relations between the “composite” and “homogeneous.” One recalls on Figure 12.8(a) the relation between the moment and curvature for a homogeneous beam with unit width, obtained 18 by integration of the local behavior : 3 s M h ¥ 1 d wo - = – ------f e x = -----x Æ -------------- ¥ ----------2 E 12 E dx 2

If one notes that Equation 12.16, recalled as: Ï My ¸ Ï –∂ wo / ∂ x ¸ Ô Ô Ô Ô 2 2 Ì –Mx ˝ = [ C ] Ì –∂ wo / ∂ y ˝ Ô Ô Ô Ô Ó – M xy ˛ Ó – 2 ¥ ∂ 2 w / ∂ x dy ˛ 2

2

o

18

∂u

dw o

2

d wo

sx

- = – z ----- which can be integrated into Recall that e x = ------ with u = –z ---------- ; then z ----------2 ∂x dx E dx the thickness.

© 2003 by CRC Press LLC

2

TX846_Frame_C12 Page 251 Monday, November 18, 2002 12:27 PM

can be inverted, and noting:

[C]

-1

1/EI 11

1/EI 12

1/EI 13

= 1/EI 21

1/EI 22

1/EI 23

1/EI 31

1/EI 32

1/EI 33

one obtains:

∂ wo –1 1 1 ----------- = --------- ¥ M y + --------- ¥ M x + --------- ¥ M xy 2 ∂x EI 11 EI 12 EI 13 2

The identification of the behavior noted in Figure 12.8(a), on the one hand, with only the first term of the moment My in the equation in Figure 12.8(b), on the other hand, that is: h ¥1 EI 11 ∫ E -------------12 3

leads to an approximate equation of an equivalent modulus E that one can interpret as the flexure modulus along the x direction of the homogeneous material: 12 E flexure = -----3- ¥ EI 11 h ( along x ) Note: When the plies of the laminate are oriented uniquely along the 0∞ and 90∞ directions, or when the laminate [0/90/45/–45] is constituted uniquely of balanced fabrics and of mats, excluding the unidirectional layers, then one has in the matrix [C]: C 13 = C 23 = 0 then: 2

EI 11

C 12 = C 11 – ------C 22

12.1.7 Case of Thermomechanical Loading 12.1.7.1 Membrane Behavior When one considers variation in temperature, which is assumed to be identical in all plies of the laminate, the stresses are given by the modified Equations 11.10. Following the procedure of Section 12.2, with the same hypotheses and notations, the stress resultant Nx (Equation 12.1) becomes th

th

n ply

Nx =

Â st

k=1 ply

n ply

{E

k 11

e ox + E

k 12

e oy + E

k 13

g oxy }e k – DT

Â st

k=1 ply

then: N x = A 11 e ox + A 12 e oy + A 13 g oxy – DT · a EhÒ x © 2003 by CRC Press LLC

a E1 ¥ ek k

TX846_Frame_C12 Page 252 Monday, November 18, 2002 12:27 PM

with: th

th

n ply

A 1j =

Â

n ply

E

k 1j

e k ; · a EhÒ x =

st

Â

a E1 ek k

st

k=1 ply

k=1 ply

Following the same procedure for Ny and Txy, the stress resultants are expressed as: Ï Nx ¸ A 11 A 12 A 13 Ô Ô N = Ì y˝ A 21 A 22 A 23 Ô Ô A 31 A 32 A 33 Ó T xy ˛

Ï e ox ¸ Ï · a EhÒ x ¸ Ô Ô Ô Ô Ì e oy ˝ – DT Ì · a EhÒ y ˝ Ô Ô Ô Ô Ó g oxy ˛ Ó · a EhÒ xy ˛

with : th

n ply

A ij =

Â

E ijk ¥ e k = A ji

cf. [ 11.8 ]

st

k=1 ply

¸ Ô · a EhÒ x = a E ¥ ek Ô Ô st k=1 ply Ô th Ô n ply Ô k · a EhÒ y = a E2 ¥ ek ˝ Ô st k=1 ply Ô th Ô n ply Ô k · a EhÒ xy = a E3 ¥ ek Ô Ô st k=1 ply ˛ th

(12.17)

n ply

Â

k 1

Â

cf. [ 11.10 ]

Â

Inversion of the above relation allows one to show the apparent moduli of the laminate (see Paragraph 12.1.2) and thermal membrane strains: Ï e ox ¸ Ï s ox ¸ Ï · a EhÒ x ¸ Ô Ô Ô Ô –1 Ô –1 Ô Ì e oy ˝ = h [ A ] Ì s oy ˝ + DT [ A ] Ì · a EhÒ y ˝ Ô Ô Ô Ô Ô Ô Ó g oxy ˛ Ó t oxy ˛ Ó · a EhÒ xy ˛ or with Equation 12.9: Ï e ox ¸ Ô Ô Ô Ô Ì e oy ˝ = Ô Ô Ô Ô Ó g oxy ˛ © 2003 by CRC Press LLC

1 ----Ex

yx –n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï s ox ¸ Ï · a EhÒ x ¸ Ô Ô Ô Ô Ô Ô Ô –1 Ô Ì s oy ˝ + DT [ A ] Ì · a EhÒ y ˝ Ô Ô Ô Ô Ô Ô Ô Ô Ó t oxy ˛ Ó · a EhÒ xy ˛

TX846_Frame_C12 Page 253 Monday, November 18, 2002 12:27 PM

which can be rewritten as: Ï e ox ¸ Ï s ox ¸ Ï --1- · a EhÒ ¸ x Ô Ô Ô Ô Ô Ôh Ô Ô Ô Ô –1 Ô –1 Ô 1 Ì e oy ˝ = h [ A ] Ì s oy ˝ + DT ¥ h [ A ] Ì --h- · a EhÒ y ˝ Ô Ô Ô Ô Ô Ô Ô Ô Ô Ô Ô --1- · a EhÒ Ô xy ˛ Ó g oxy ˛ Ó t oxy ˛ Óh

Remarks: Evaluation of terms (1/h)·aEhÒx, (1/h)·aEhÒy, and (1/h)·aEhÒxy only requires the knowledge of the proportions of plies along the different orientations 19 and not their thicknesses. -1 The matrix h[A] , already mentioned in Section 12.1.2, contains the global moduli of the laminate. One can then write (see Equation 12.9): Ï e ox ¸ Ô Ô Ô Ô Ì e oy ˝ = Ô Ô Ô Ô Ó g oxy ˛

1 ----Ex

yx –n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï s ox ¸ Ô Ô Ô Ô Ì s oy ˝ + DT Ô Ô Ô Ô Ó t oxy ˛

1 ----Ex

yx n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï --1- · a EhÒ ¸ x Ô Ôh Ô1 Ô Ì --h- · a EhÒ y ˝ Ô Ô Ô --1- · a EhÒ Ô xy ˛ Óh

The last term of the above equation allows one to show the global expansion coefficients of the laminate, which are denoted as aox, aoy, and aoxy, as below: Ï a ox ¸ Ô Ô Ô Ô Ì a oy ˝ = Ô Ô Ô Ô Ó a oxy ˛

1 ----Ex

yx –n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï --1- · a EhÒ ¸ x Ô Ôh Ô1 Ô Ì --h- · a EhÒ y ˝ Ô Ô Ô --1- · a EhÒ Ô xy ˛ Óh

(12.18)

In summary, the membrane thermomechanical behavior of a laminate with midplane symmetry can be written as: Ï e ox ¸ Ô Ô Ô Ô Ì e oy ˝ = Ô Ô Ô Ô Ó g oxy ˛

19

1 ----Ex

yx –n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï s ox ¸ Ô Ô Ô Ô Ì s oy ˝ + DT Ô Ô Ô Ô Ó t oxy ˛

Ï a ox ¸ Ô Ô Ô Ô Ì a oy ˝ Ô Ô Ô Ô Ó a oxy ˛

See Application18.2 “Residual Thermal Stresses due to Curing of the Laminate.”

© 2003 by CRC Press LLC

(12.19)

TX846_Frame_C12 Page 254 Monday, November 18, 2002 12:27 PM

This is an equation in which aox, aoy, and aoxy are given by Equations 12.17 and 20 12.18.

12.1.7.2 Flexure Behavior Following the procedure in Section 12.14 with the same notations, the moment resultant My (Equation 12.13) becomes, using the modified Equations 11.10: th

n ply

My =

Ï

Â ÌÓ Ú

zk zk – 1

st

k=1 ply

¸ k k ( E 11 e x + E 12 e y + E 13 g xy )z dz ˝ ˛ th

n ply

– DT

Â ÊË Ú

zk zk – 1

st

k a E 1 ¥ z dzˆ¯

k=1 ply

The plate is assumed to have midplane symmetry, then each integral of the form – z k-1 Úzk-1 a E1 z dz is associated with another integral such that Ú–zk a E1 z dz is equal and opposite in sign. There remains the following expression, with the notations of Section 12.1.4: zk

∂ w0 ∂ w0 ∂ w - – C 12 ----------- – C 13 ¥ 2 ------------0M y = – C 11 ----------2 2 ∂ x∂y ∂x ∂y 2

2

2

Due to the midplane symmetry, the behavior in flexure 12.16 is not modified when the laminate is subjected to thermomechanical loading.

Remark: In the preceding discussion, it is assumed that the temperature field is uniform across the thickness of the laminate.

12.2 LAMINATE WITHOUT MIDPLANE SYMMETRY 12.2.1 Coupled Membrane–Flexure Behavior If one considers again the calculations of Section 12.1.4 without midplane symmetry, one can see the presence of new integrals as: 2

zk

2

k k z k – z k-1ˆ E ij z dz = E ij Ê ------------------Ë 2 ¯ z k-1

Ú

for the ply k. When the summation over all plies is taken, these integrals lead to nonzero terms with the form: th

n ply

B ij =

Â st

2

2

k z k – z k-1ˆ E ij Ê ------------------Ë 2 ¯

k=1 ply 20

One indicates in Tables 5.4, 5.9, and 5.14 of Section 5.4 the values of expansion coefficients of the laminates made of carbon, Kevlar, and glass/epoxy with Vf = 60% fiber volume fraction.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 255 Monday, November 18, 2002 12:27 PM

Then one has for the development of My (see Section 12.1.4):

∂ w0 ∂ w0 ∂ w - – C 12 ----------- – C 13 ¥ 2 ------------0- + B 11 e ox + B 12 e oy + B 13 g oxy M y = – C 11 ----------2 2 ∂ x∂y ∂x ∂y 2

2

2

In this expression appears the coupling between bending and membrane behavior. In a similar manner, the stress resultant Nx which was developed in Section 12.1.4 is rewritten as: 2 ∂ w0 ∂ w ∂ w0 - – B 13 ¥ 2 ------------0- – B 12 ----------N x = A 11 e ox + A 12 e oy + A 13 g oxy – B 11 ----------2 2 ∂ x∂y ∂y ∂x 2

2

where one can find the coupling as mentioned previously. Developing along the same manner the resultants Mx, Mxy, Ny, and Txy, one can regroup the obtained relations. Therefore, the global relation for the behavior can be written as: Ï Nx ¸ Ô Ô Ô Ny Ô Ô Ô Ô T xy Ô Ì ˝ = Ô My Ô Ô –M Ô x Ô Ô Ô –M Ô Ó xy ˛

A

B

B

C

e ox Ï ¸ Ô Ô e oy Ô Ô Ô Ô g oxy Ô Ô Ì –∂ 2 w / ∂ x2 ˝ 0 Ô Ô Ô 2 2 Ô Ô –∂ w0 / ∂ y Ô Ô Ô 2 Ó –2 ∂ w0 / ∂ x ∂ y ˛

(12.20)

with : th

th

n ply

n ply

Â

A ij =

E e k ; B ij =

st

st

k=1 ply

2

2

k z k – z k-1ˆ E ij Ê ------------------Ë 2 ¯

k=1 ply

th

n ply

C ij =

Â

k ij

Â st

3

3

k z k – z k-1ˆ E ij Ê ------------------Ë 3 ¯

k=1 ply

12.2.2 Case of Thermomechanical Loading Using the expression developed for moment resultant My as shown in Section 12.1.7.2, one can find the following form of integrals for each ply k: zk

2

2

z k – z k-1ˆ a E ¥ z dz = a E ÊË ------------------2 ¯ z k-1

Ú

k 1

k 1

after summing over all plies of the laminate, it appears a nonzero term of the form: th

n ply

· a Eh Ò x = 2

Â st

k=1 ply

© 2003 by CRC Press LLC

2

2

k z k – z k-1ˆ a E 1 ÊË ------------------2 ¯

TX846_Frame_C12 Page 256 Monday, November 18, 2002 12:27 PM

A similar development for other resultants lead to the following relation for thermomechanical behavior: Ï Nx ¸ Ô Ô Ô Ny Ô Ô Ô Ô T xy Ô Ì ˝ = Ô My Ô Ô –M Ô x Ô Ô Ô –M Ô Ó xy ˛

A

B

B

C

A ij =

with:

Â

e ox Ï · a EhÒ x ¸ Ï ¸ Ô Ô Ô Ô e oy Ô · a EhÒ y Ô Ô Ô Ô Ô Ô Ô g oxy Ô · a EhÒ xy Ô Ô Ô ˝ Ì – ∂ 2 w / ∂ x 2 ˝ – DT Ì 2 0 Ô · a Eh Ò x Ô Ô Ô Ô Ô Ô 2 2 Ô 2 Ô · a Eh Ò y Ô Ô –∂ w0 / ∂ y Ô Ô Ô Ô Ô 2 2 Ó · a Eh Ò xy ˛ Ó –2 ∂ w0 / ∂ x ∂ y ˛ k

E ij e k ;

B ij =

k

Â k

C ij =

2

2

k z k – z k-1ˆ E ij Ê ------------------Ë 2 ¯ 3 k

(12.21)

3 k-1

-ˆ Â E ÊË ------------------3 ¯ k ij

z –z

k

· a EhÒ x =

Â aE

k 1

ek ;

· a EhÒ y =

k

· a Eh Ò x = 2

Â k

Â aE

k 2

ek ;

· a EhÒ xy =

k

k ( z k – z k-1 ) -; a E 1 -----------------------2 2

k 3

k

2

· a Eh Ò y = 2

Â k

· a Eh Ò xy = 2

k ( z k – z k-1 ) -; a E 2 -----------------------2

Â k

© 2003 by CRC Press LLC

Â aE

2

2

k ( z k – z k-1 ) a E 3 -----------------------2 2

2

ek

TX846_Frame_C13 Page 257 Monday, November 18, 2002 12:29 PM

PART III JUSTIFICATIONS, COMPOSITE BEAMS, AND THICK PLATES We regroup in Part III elements that are less utilized than those in the previous parts. Nevertheless they are of fundamental interest for a better understanding of the principles for calculation of composite components. In the first two chapters, we focused on anisotropic properties and fracture strength of orthotropic materials, and then more particularly on transversely isotropic ones. The following two chapters allow us to consider that composite components in the form of beams can be “homogenized.” This means that their study is analogous to the study of homogeneous beams that are common in the literature. Finally, the last chapter in this part describes with a similar procedure the behavior of thick composite plates subject to transverse loadings.

© 2003 by CRC Press LLC

TX846_Frame_C13 Page 259 Monday, November 18, 2002 12:29 PM

13 ELASTIC COEFFICIENTS The definition of a linear elastic anisotropic medium was given in Chapter 9. We have also given, without justification, the behavior relations characterizing the particular case of orthotropic materials. Now we propose to examine more closely the elastic constants which appear in stress–strain relations for these materials. In the case of transversely isotropic materials, we will study also the manner in which the constants evolve.

13.1 ELASTIC COEFFICIENTS IN AN ORTHOTROPIC MATERIAL Recall: Consider the relation for elastic behavior written in Paragraph 9.1.1 in the form:

e mn = j mnpq ¥ s pq Recall that the components jmnpq of a tensor expressed in the coordinate system 1,2,3 are written as FIJKL in a coordinate system I,II,II using the relation: F IJKL = cos I cos J cos K cos L j mnpq m

n

p

q

(13.1)

in which: cos I = cos ( m, I ) m

1

By definition, for mechanical behavior, an orthotropic medium has at any point two orthogonal planes of symmetry. Consider here two coordinate systems 1,2,3 and I,II,III, constructed on these planes and their intersection. One plane can be obtained from the other by a 180∞ rotation about the 3 axis as shown in Figure 13.1. One can deduce

[ cos I ] = m

1

See Section 9.2.

© 2003 by CRC Press LLC

–1 0 0 0 –1 0 0 0 1

TX846_Frame_C13 Page 260 Monday, November 18, 2002 12:29 PM

Figure 13.1 Orthotropic Medium

Application of Relation 13.1 above leads to = j 1 1 1 1 ; F I I II II

FI I I I

= j 1 1 2 2 ; F I I III III

= j1 1 3 3

F II II II II = j 2 2 2 2 ; F II II III III = j 2 2 3 3 ; F III III III III = j 3 3 3 3 F II III II III = j 2 3 2 3 ; F I III I III = j 1 3 1 3 ; F I II I II

= j1 2 1 2

and: F I I II III = – j 1 1 2 3 ; However, because the mechanical properties in the coordinates 1,2,3 and I,II,III are identical, one has F I I II III = j 1 1 2 3 from this: F I I II III = j 1 1 2 3 = – j 1 1 2 3 = 0 In an analogous manner:

j II II II III = 0; F III III II III = 0 F I I I III = 0; F II II I III = 0; F III III I III = 0 F II III I II = 0; F I III I II = 0 finally: F I I I II

= j 1 1 1 2 ; F II II I II = j 2 2 1 2 ; F III III I II = j 3 3 12

F II III I III = j 2 3 1 3 © 2003 by CRC Press LLC

TX846_Frame_C13 Page 261 Monday, November 18, 2002 12:29 PM

Until now, we have taken into account the symmetry with respect to plane 1,3. Consider now the coordinates 1,2,3 and I’, II’, III’ (see Figure 13.1), which can be obtained from each other by a 180∞ rotation about the 2 axis (symmetry with respect to plane 1,2). One has [ cos I ] = m

–1 0 0

0 0 1 0 0 –1

The same procedure as above will lead to F I¢I¢I¢II¢

= – j 1 1 1 2 = j 1 1 1 2 = 0; F II¢II¢I¢II¢ = – j 2 2 1 2 = j 2 2 1 2 = 0

F III¢III¢I¢II¢ = – j 3 3 1 2 = j 3 3 1 2 = 0; F II¢III¢I¢III¢ = – j 2 3 1 3 = j 2 3 1 3 = 0 Considering the symmetry of the coefficients jmnpq indicated in Relation 9.1, we have written here the only nonzero terms. For the mechanical behavior, one obtains by simplification of Equation 9.2:

2

Ï e 11 ¸ j1 1 1 1 j1 1 2 2 j1 1 3 3 0 0 0 Ô Ô Ô e 22 Ô j2 2 1 1 j2 2 2 2 j2 2 3 3 0 0 0 Ô Ô Ô e 33 Ô j3 3 1 1 j3 3 2 2 j3 3 3 3 0 0 0 Ì ˝ = g 0 0 0 0 0 4 j2 3 2 3 Ô 23 Ô Ôg Ô 0 0 0 0 0 4 j1 3 1 3 Ô 13 Ô Ôg Ô j 0 0 0 0 0 4 1 2 12 Ó 12 ˛

Ï s 11 ¸ Ô Ô Ô s 22 Ô Ô Ô Ô s 33 Ô Ì ˝ Ô t 23 Ô Ôt Ô Ô 13 Ô Ôt Ô Ó 12 ˛

(13.2)

There remain then only nine distinct elastic coefficients, which can be written in the form of Young’s moduli and Poisson ratios as: Ïe ¸ Ô 11 Ô Ô Ô Ô e 22 Ô Ô Ô Ô Ô Ô e 33 Ô Ì ˝ = Ôg Ô Ô 23 Ô Ô Ô Ô g 13 Ô Ô Ô Ôg Ô Ó 12 ˛

2

1 – n 21 – n 31 ----- --------- ---------E3 E1 E2 – n 12 1 ---------- ----E1 E2

– n 32 ---------E3

– n 13 – n 23 ---------- ---------E1 E2

1 ----E3

0

0

0

0

0

0

0

0

0

0 0 0 ÏÔ s 11 ¸Ô Ô Ô 0 0 0 Ô s 22 Ô Ô Ô Ô Ô 0 0 0 Ô s 33 Ô Ì ˝ 1 -------- 0 0 Ô t 23 Ô G 23 Ô Ô Ô Ô 1 - 0 Ô t 13 Ô 0 ------G 13 Ô Ô 1 Ô - t 12 Ô 0 0 ------˛ G Ó 12

Recall the symmetry relations: jijkl = jijlk; jijkl = jjikl; jijkl = jklij.

© 2003 by CRC Press LLC

(13.3)

TX846_Frame_C13 Page 262 Monday, November 18, 2002 12:29 PM

Figure 13.2 Transversely Isotropic Material

13.2 ELASTIC COEFFICIENTS FOR A TRANSVERSELY ISOTROPIC MATERIAL 3

Recall: By definition, a transversely isotropic material (Figure 13.2) is such that any plane including a preferred axis is a plane of mechanical symmetry. We have already noted that this is a particular case of orthotropic materials. Therefore, the 4 only nonzero elastic constants are shown in Figure 13.2. The preferred direction is axis 1 in Figure 13.2. Considering that the coordinates 1,2,3 and I,II,III can be obtained from each other by a rotation of q. One then has 1 0 0 m [ cos I ] = 0 c – s with c = cos q s = sin q 0 s c From the definition of material, the matrix of elastic coefficients has to remain invariant in this rotation. The Relation 13.1 allows one to write • FI I I I = j1 1 1 1 • F I I II II = j 1 1 2 2 c + j 1 1 3 3 s = j 1 1 2 2 2

3 4

2

See Section 9.3. Using the symmetries in Equation 9.1 and also using the discussion of the previous paragraph.

© 2003 by CRC Press LLC

TX846_Frame_C13 Page 263 Monday, November 18, 2002 12:29 PM

then:

j1 1 2 2 ( c – 1 ) + j1 1 3 3 s = 0 2

2

j1 1 2 2 = j1 1 3 3 4 2 2 2 2 2 2 • F II II II II = j 2 2 2 2 c + j 2 2 3 3 s c + j 2 3 2 3 s c + j 2 3 3 2 s c º

º + j3 2 2 3 s2 c2 + j3 2 3 2 s2 c2 + j3 3 2 2 s2 c2 + j3 3 3 3 s4 and: F II II II II = j 2 2 2 2 Then, taking into account the symmetries, we obtain the relation:

j 2 2 2 2 ( c – 1 ) + j 3 3 3 3 s + 2s c ( j 2 2 3 3 + 2 j 2 3 2 3 ) = 0 4

4

2 2

(a)

4 2 2 2 2 2 2 • F III III III III = j 2 2 2 2 s + j 2 2 3 3 s c + j 2 3 2 3 s c + j 2 3 3 2 s c º

º + j3 2 3 2 s2 c2 + j3 2 3 2 s2 c2 + j3 3 2 2 s2 c2 + j3 3 3 3 s4 and: F III III III III = j 3 3 3 3 then taking in account symmetry, we have:

j 2 2 2 2 s + j 3 3 3 3 ( c – 1 ) + 2s c ( j 2 2 3 3 + 2 j 2 3 2 3 ) = 0 4

4

2 2

(b)

Examining member by member the difference of relations shown in (a) and (b) above, one obtains:

j2 2 2 2 = j3 3 3 3 Replacing in (a):

j 2 2 2 2 ( c + s – 1 ) + 2s c ( j 2 2 3 3 + 2 j 2 3 2 3 ) = 0 4

4

2 2

– 2 s c j 2 2 2 2 + 2s c ( j 2 2 3 3 + 2 j 2 3 2 3 ) = 0 2 2

2 2

2 j2 3 2 3 = j2 2 2 2 – j2 2 3 3 • F I III I III = j 1 2 1 2 s + j 1 3 1 3 c = j 1 3 1 3 2

© 2003 by CRC Press LLC

2

TX846_Frame_C13 Page 264 Monday, November 18, 2002 12:29 PM

then

j1 2 1 2 s + j1 3 1 3 ( c – 1 ) = 0 2

2

j1 2 1 2 = j1 3 1 3 We have written four relations for the nine coefficients; there remain five distinct elastic coefficients. Equation 13.2 is reduced to Ï e 11 ¸ j1 1 1 1 j1 1 2 2 j1 1 2 2 0 0 0 Ô Ô Ô e 22 Ô j2 2 1 1 j2 2 2 2 j2 2 3 3 0 0 0 Ô Ô e Ô 33 Ô j2 2 1 1 j3 3 2 2 j2 2 2 2 0 0 0 Ì ˝ = 0 0 0 0 0 2 ( j2 2 2 2 – j2 2 3 3 ) Ô g 23 Ô Ôg Ô 0 0 0 0 0 4 j1 2 1 2 Ô 13 Ô Ôg Ô 0 0 0 0 0 4 j1 2 1 2 Ó 12 ˛

Ï s 11 ¸ Ô Ô Ô s 22 Ô Ô Ô Ô s 33 Ô Ì ˝ (13.4) Ô t 23 Ô Ôt Ô Ô 13 Ô Ôt Ô Ó 12 ˛

or in the form of Young’s moduli and Poisson ratios: Ï e 11 ¸ Ô Ô Ô Ô Ô e 22 Ô Ô Ô Ôe Ô Ô 33 Ô Ì ˝ = Ô g 23 Ô Ô Ô Ô Ô Ô g 13 Ô Ô Ô Ôg Ô Ó 12 ˛

13.2.1

1 ----E1

– n 21 ---------E2

– n 21 ---------E2

0

0

– n 12 ---------E1

1 ----E2

–n -----E2

0

0

– n 12 ---------E1

–n -----E2

1 ----E2

0

0 0

0

0

0

2(1 + n) -------------------E2

0

0

0

0

1 -------G 12

0

0

0

0

0

0 ÏÔ s 11 ¸Ô Ô Ô 0 Ô s 22 Ô Ô Ô Ô Ô 0 Ô s 33 Ô Ì ˝ 0 Ô t 23 Ô Ô Ô Ô Ô 0 Ô t 13 Ô Ô Ô 1 -------- Ô t 12 Ô ˛ G Ó

(13.5)

12

Rotation about an Orthotropic Transverse Axis

13.2.1.1 Problem How can one transform the elastic coefficients of the previous constitutive equation 5 when writing them in coordinate axes x,y,z other than the orthotropic axes ,t,z ? The coordinate axes x,y,z are obtained from the orthotropic axes by a rotation q about the z axis, as shown in Figure 13.3. Recall Relation 13.1, which allows the calculation of components FIJKL in the coordinate axes x,y,z as functions of the components jmnpq in the coordinate axes ,t,z to be: F IJKL = cos I cos J cos K cos L ¥ j mnpq m

( axes x, y, z ) 5

n

p

q

( axes , t, z )

The orthotropic axes 1,2,3 of Equation 13.5 are therefore denoted as ,t,z.

© 2003 by CRC Press LLC

TX846_Frame_C13 Page 265 Monday, November 18, 2002 12:29 PM

Figure 13.3 Rotation above an Orthotropic Transverse Axis

with (see Figure 13.3):

[cos I ] = m

cos ( , x ) cos ( t, x ) cos ( z, x )

cos ( , y ) cos ( t, y ) cos ( z, y )

c –s 0 cos ( , z ) = s c 0 cos ( t, z ) 0 0 1 cos ( z, z )

Noting that the only nonzero coefficients jmnpq are those that appear in Equation 13.4, one obtains: • FI I I I = c j1 1 1 1 + c s j1 1 2 2 + c s j1 2 1 2 + c s j1 2 2 1 º 4

2 2

2 2

2 2

º + c2 s2 j2 1 1 2 + c2 s2 j2 1 2 1 + c2 s2 j2 2 1 1 + s4 j2 2 2 2 • F I I I I = c j 1 1 1 1 + s j 2 2 2 2 + 2c s ( j 1 1 2 2 + 2 j 1 2 1 2 ) 4

4

2 2

Expressing this coefficient as a function of the “technical” constants which appear in Equation 13.5, one obtains: 4 4 n s c 2 2 1 F I I I I = ----- + ---- + s c Ê ------- – 2 -----t-ˆ Ë E Et Et ¯ G t

• F I I II II = c s j 1 1 1 1 + c j 1 1 2 2 – c s j 1 2 1 2 – c s j 1 2 2 1 º 2 2

4

2 2

2 2

º – s2 c2 j2 1 1 2 – s2 c2 j2 1 2 1 + s4 j2 2 1 1 + s2 c2 j2 2 2 2 • F I I II II = ( c + s ) j 1 1 2 2 + c s ( j 1 1 1 1 + j 2 2 2 2 – 4c s j 1 2 1 2 ) 4

4

2 2

2 2

or in the “technical” form:

n 1 1 4 4 2 2 1 F I I II II = – -----t- ( c + s ) + c s Ê ----- + ---- – -------ˆ Ë E E t G t¯ Et • F I I III III = c j 1 1 3 3 + s j 2 2 3 3 and as 2

2

j1 1 3 3 = j1 1 2 26

F I I III III = c j 1 1 2 2 + s j 2 2 3 3 2

6

2

Because this is a transversely isotropic material; see Equations 9.2 and 13.4.

© 2003 by CRC Press LLC

TX846_Frame_C13 Page 266 Monday, November 18, 2002 12:29 PM

or in the “technical” form: 2n 2n F I I III III = – Ê c -----t- + s ----ˆ Ë Et E t¯

• F I I II III = 0 • F I I I III = 0 • F I I I II = – c s j 1 1 1 1 + c s j 1 1 2 2 + c s j 1 2 1 2 – cs j 1 2 2 1 + sc j 2 1 1 2 º 3

3

3

3

3

… – s3 c j2 1 2 1 – s3 c j2 2 1 1 + s3 c j2 2 2 2 F I I I II = – sc { c j 1 1 1 1 – s j 2 2 2 2 – ( c – s ) ( j 1 1 2 2 + 2 j 1 2 1 2 ) } 2

2

2

2

or in the “technical” form: Ï c2 s2 n 1 ¸ 2 2 F I I I II = – cs Ì ----- – ---- + ( c – s ) Ê -----t- – -----------ˆ ˝ Ë E t 2G t¯ ˛ Ó E Et • F II II II II = s j 1 1 1 1 + s c j 1 1 2 2 + s c j 1 2 1 2 + s c j 1 2 2 1 º 4

2 2

2 2

2 2

º + s c j2 1 1 2 + s c j2 1 2 1 + s c j2 2 1 1 + c j2 2 2 2 2 2

2 2

2 2

4

F II II II II = s j 1 1 1 1 + c j 2 2 2 2 + s c ( 4 j 1 2 1 2 + 2 j 1 1 2 2 ) 4

4

2 2

or in “technical” form: 4 4 n c s 2 2 1 F II II II II = ----- + ---- + s c Ê ------- – 2 -----t-ˆ Ë G t E Et Et ¯

• F II II III III = s j 1 1 3 3 + c j 2 2 3 3 and as j 1 1 3 3 = j 1 1 2 2 7 2

2

F II II III III = s j 1 1 2 2 + c j 2 2 3 3 2

2

or in “technical” form: 2n 2n F II II III III = – Ê s -----t- + c ----ˆ Ë Et E t¯

• F II II II III = 0 • F II II I III = 0 • F II II I II = – s c j 1 1 1 1 + s c j 1 1 2 2 – sc j 1 2 1 2 + s c j 1 2 2 1 º 3

3

3

3

… ( – sc 3 j 2 1 1 2 + s 3 c j 2 1 2 1 – sc 3 j 2 2 1 1 + c 3 s j 2 2 2 2 ) F II II I II = – sc { s j 1 1 1 1 + c j 2 2 2 2 + ( c – s ) ( j 1 1 2 2 + 2 j 1 2 1 2 ) } 2

7

See Equations 9.2 and 13.4.

© 2003 by CRC Press LLC

2

2

2

TX846_Frame_C13 Page 267 Monday, November 18, 2002 12:29 PM

or in “technical” form: Ï s2 c2 n 1 ¸ 2 2 F II II I II = – cs Ì ----- – ---- – ( c – s ) Ê -----t- – -----------ˆ ˝ Ë ¯ E E E 2G t t t ˛ Ó • F III III III III = j 3 3 3 3 in “technical” form: 1 F III III III III = ---Et • F III III II III = 0 • F III III I III = 0 • F III III I II = – sc j 3 3 1 1 + sc j 3 3 2 2 and as j 3 3 1 1 = j 1 1 2 2 8 F III III I II = – sc j 1 1 2 2 + sc j 2 2 3 3 in “technical” form:

n – n tˆ F III III I II = – sc Ê --------------Ë Et ¯ • F II III II III = s j 1 3 1 3 + c j 2 3 2 3 2

2

8

we know that for a transversely isotropic material, one has:

j1 3 1 3 = j1 2 1 2

and

2 j2 3 2 3 = j2 2 2 2 – j2 2 3 3

then: 2 2 j2 2 2 2 – j2 2 3 3 ˆ F II III II III = s j 1 2 1 2 + c Ê ---------------------------------Ë ¯ 2

in “technical” form: c (1 + n) s F II III II III = ----------- + ---------------------4G t 2E t 2

2

• F II III I III = – sc j 1 3 13 + sc j 2 3 2 3 is still:

8

1 F II III I III = – sc Ê j 2 1 2 1 – --- ( j 2 2 22 – j 2 2 3 3 )ˆ Ë ¯ 2 8

See Equations 9.2 and 13.4.

© 2003 by CRC Press LLC

TX846_Frame_C13 Page 268 Monday, November 18, 2002 12:29 PM

or in “technical” form: 1 (1 + n) F II III I III = – sc Ê ----------- – -----------------ˆ Ë 4G t 2E t ¯ • F III II I II = 0 • F I III I III = c j 1 3 1 3 + s j 2 3 2 3 is still: 2

2

2 2 ( j2 2 2 2 – j2 2 3 3 ) F I III I III = c j 1 2 12 + s ------------------------------------2

or in “technical” form: c 2(1 + n) F I III I III = ----------- + s ----------------4G t 2E t 2

• F I III I II = 0 • F I II I II = s c j 1 1 1 1 – s c j 1 1 2 2 + c j 1 2 1 2 – s c j 1 2 2 1 º 2 2

2 2

4

2 2

º – s2 c2 j2 1 1 2 + s4 j2 1 2 1 – s2 c2 j2 2 1 1 + s2 c2 j2 2 2 2 2 2

F I II I II = s c ( j 1 1 1 1 + j 2 2 2 2 – 2 j 1 1 2 2 ) + ( c – s ) j 1 2 1 2 2 2

2

or in “technical” form:

n ¸ 1 2 2Ï 1 2 2 2 1 F I II I II = s c Ì ----- + ---- + 2 -----t- ˝ + ( c – s ) ----------Et ˛ 4G t Ó E Et All the nonzero coefficients F IJKL found above allow one to write the constitutive 9 relation in the form : Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

e xx e yy e zz g yz g xz g xy

¸ F I I II II F I I III III 0 0 2F I I I II FI I I I Ô Ô F II II I I F II II II II F II II III III 0 0 2F II II I II Ô Ô F III III I I F III III II II F III III III III 0 0 2F III III I II ˝ = 0 0 0 4F II III II III 4F II III I III 0 Ô Ô 0 0 0 0 4F I III II III 4F I III I III Ô Ô 0 0 4F I II I II 2F I II I I 2F I II II II 2F I II III III ˛

Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

s xx s yy s zz t yz t xz t xy

¸ Ô Ô Ô Ô ˝ Ô Ô Ô Ô ˛

(13.6) 9

This is deduced from the general Equation 9.2.

© 2003 by CRC Press LLC

TX846_Frame_C13 Page 269 Monday, November 18, 2002 12:29 PM

13.2.1.2 Technical Form In analogy with the technical form of Equation 13.5, which was written in orthotropic axes, one can write the constitutive equation in terms of equivalent moduli and Poisson coefficients, as: Ï Ô Ô Ô Ô Ô Ô Ì Ô Ô Ô Ô Ô Ô Ó

e xx ¸ Ô Ô e yy Ô Ô e zz ÔÔ ˝ = g yz Ô Ô Ô g xz Ô Ô Ô g xy ˛

1 ----Ex – n xy ---------Ex

– n yx – n zx ---------- ---------Ey Ez

0

0

– n zy ---------Ez

0

0

1 ----Ez

0

0

1 ----Ey

– n xz – n yz ---------- ---------Ex Ey

0

0

0

1 -------G yz

x xz ------G xz

0

0

0

x yz ------G yz

1 -------G xz

hx ----Ex

my ----Ey

z ----zEz

0

0

h xy ------G xy

Ï Ô m xy Ô -------- Ô G xy Ô z xy Ô ------G xy Ô Ì 0 Ô Ô Ô 0 Ô Ô 1 Ô -------- Ó G xy

s xx ¸ Ô Ô s yy Ô Ô Ô s zz Ô ˝ t yz Ô Ô Ô t xz Ô Ô Ô t xy ˛

(13.7)

In this equation, there are coupling terms characterized by the coefficients hxy , mxy , zxy , and xxy , which are not similar to the Poisson coefficients. The values of elastic constants in Relation 13.7 are deduced immediately from the technical forms obtained above for the coefficients FIJKL. These constants are detailed below. One obtains subsequently the elastic modulus and Poisson coefficients in the x,y,z coordinates.

n c s 1 1 ----- = ----- + ---- + s 2 c 2 Ê ------- – 2 -----t-ˆ Ë Ex E Et Et ¯ G t 4

4

4 4 n s c 1 1 ----- = ----- + ---- + s 2 c 2 Ê ------- – 2 -----t-ˆ Ë G t Ey E Et Et ¯

1 1 ----- = ---Et Ez

1 E x ( q ) = --------------------------------------------------------4 4 ➡ 2 n tˆ c s 2 2 1 ----- + ---- + s c Ê ------– ---------Ë G t E t ¯ E Et ➡

➡

n n yx 4 4 – ------ = – -----t- ( c + s ) º Et Ey 1 1 1 º + c 2 s 2 Ê ---- + ---- – -------ˆ Ë E E t G t¯

➡

1 E y ( q ) = --------------------------------------------------------4 4 s c 2 n tˆ 2 2Ê 1 ----- + ----- + s c ------- – ---------Ë G t E t ¯ E Et E z ( q ) = E t ( "q )

n yx n ------ ( q ) = -----t- ( c 4 + s 4 ) º Ey Et 1 1 1 º – c 2 s 2 Ê ---- + ---- – -------ˆ Ë E E t G t¯

n zx 2n 2n – ------ = – Ê c -----t- + s ----ˆ Ë Et E t¯ Ez

➡

n zy 2n 2n – ------ = – Ê s -----t- + c ----ˆ Ë E E t¯ Ez t

➡

2(1 + n ) s 1 -------- = c 2 -------------------- + ------G t Et G yz

2 ➡ G yz ( q ) = ---------------------------s 2 2(1 + n)

2

© 2003 by CRC Press LLC

n zx ( q ) = c n t + s n 2

2

n zy ( q ) = s n t + c n 2

2

1

c -------------------Et

+ -----G t

TX846_Frame_C13 Page 270 Monday, November 18, 2002 12:29 PM

1 2(1 + n ) c -------- = s 2 -------------------- + ------G t G xz Et 2

1

2 ➡ G xz ( q ) = ------------------------c 2 2(1 + n) s -------------------- + ------Et G t

2 2 2 1 n 1 1 1 (c – s ) -------- = 4c 2 s 2 Ê ----- + ---- + 2 -----t-ˆ + ---------------------- ➡ G xy ( q ) = ---------------------------------------------------------------------2 2 2 n 2 2 1 (c – s ) 1 Ë E Et G xy Et ¯ G t - + 2 -----t-ˆ + ---------------------4c s Ê E----+ --Et ¯ G t Ë Et

Ï c2 s2 h xy ------- = – 2cs Ì ----- – ---- º G xy Ó E Et

Ï s2 c2 m xy ------- = – 2cs Ì ----- – ---- º G xy Ó E Et

;

n t 1 ¸ º + ( c – s ) Ê ----- – -----------ˆ Ë E t 2G t¯ ˝ ˛ 2

n t 1 ¸ º – ( c 2 – s 2 ) Ê ----- – -----------ˆ Ë E t 2G t¯ ˝ ˛

2

z xy ( n – n t ) ------- = – 2cs ------------------Et G xy

z xz 1 2(1 + n ) ------- = – cs Ê ------- – --------------------ˆ Ë G t G xz Et ¯

;

(13.8)

13.3 CASE OF A PLY One can observe from Equation 13.7 that the stress–strain relations in the plane x,y appear decoupled in the case when szz = 0. We suppose that this applies for the plies making a thin laminate. Each ply will be characterized in its plane by 10 the following relations which are extracted from relations 13.5 and 13.7: In the orthotropic axes ,t: Ï e ¸ Ô Ô Ô Ô Ì et ˝ = Ô Ô Ô Ô Óg t ˛

1 ----E

– n t --------Et

– n t --------E

1 ---Et

0

0

0 ÏÔs ¸Ô Ô Ô 0 Ì st ˝ Ô Ô 1 Ô Ô ------- t G t Ó t ˛

(13.9)

In the x,y axes, making an angle q with the orthotropic axes:

10

The orthotropic axes of Equation 13.5 are denoted as l,t,z for a ply (see Section 3.3.1).

© 2003 by CRC Press LLC

TX846_Frame_C13 Page 271 Monday, November 18, 2002 12:29 PM

Ï e xx ¸ Ô Ô Ôe Ô Ì yy ˝ = Ô Ô Ôg Ô Ó xy ˛

1 ----Ex

yx – -----E

h xy ------G xy

– n xy ---------Ex

1 ----Ey

m xy ------G xy

hx ----Ex

my ----Ey

1 -------G xy

n

y

Ï s xx ¸ Ô Ô Ôs Ô Ì yy ˝ Ô Ô Ôt Ô Ó xy ˛

For the constants, the values were shown in detail in 13.8.

© 2003 by CRC Press LLC

(13.10)

TX846_Frame_C14 Page 273 Monday, November 18, 2002 12:30 PM

14 THE HILL–TSAI FAILURE CRITERION

There are many failure criteria for orthotropic materials. The most commonly used 1 for design calculations is the so-called “Hill-Tsai” criterion. This criterion can be interpreted as analogous to the Von Mises criterion which is applicable to isotropic material in elastic deformation. We will review at the beginning the principal aspects of the Von Mises criterion.

14.1 ISOTROPIC MATERIAL: VON MISES CRITERION The material is elastic and isotropic. In Figure 14.1, one denotes by I,II,III the principal directions of the stress tensor S for a given point. The corresponding matrix is

sI 0 0 0 s II 0 0 0 s III The general form of the deformation energy dW for an elementary volume dV surrounding the point considered can be written as: 1 dW total = --2

ÂÂs i

ij

e ij dV

j

which can be reduced to 1 dW total = --- ( s I e I + s II e II + s III e III ) dV 2 1

See failure of composite materials in Section 5.3.2.

© 2003 by CRC Press LLC

TX846_Frame_C14 Page 274 Monday, November 18, 2002 12:30 PM

Figure 14.1 Principal Directions for the Stress Tensor

eI eII eIII are the principal strains that one can express as functions of stresses using the constitutive Equation 10.1 as: 1+n n e = ------------ S – --- trace ( S )I E E This leads to: 1Ï1 + n 2 n 2 2 2¸ Ê dW --------- ˆ = --- Ì ------------ ( s I + s II + s III ) – --- ( s I + s II + s III ) ˝ Ë dV ¯ total E 2Ó E ˛ (Note that (dW/dV) represents energy per unit volume). The total elastic deformation above is due to the dilatation and distortion of the material. The Von Mises criterion postulates that the material resists to a state of isotropic (or spherical) stress, but will plastify when the distortion energy per unit volume reaches a critical value. One notes that: dW dW Ê dW --------- ˆ = Ê --------- ˆ – Ê --------- ˆ Ë dV ¯ total Ë dV ¯ spherical stress Ë dV ¯ distorsion The isotropic portion of the stress state here is written as: a state of isotropic dilatation (Equation 10.1):

s I + s II + s III --------------------------------. 3

1 + n s I + s II + s IIIˆ n - – --- ( s I + s II + s III ) e = ------------ ÊË ------------------------------¯ E 3 E then: ¸ s I + s II + s IIIˆ 1Ï Ê dW - ¥ e˝ --------- ˆ = --- Ì 3 ¥ Ê ------------------------------Ë ¯ Ë dV ¯ spherical stress 3 2Ó ˛ ¸ 1 Ï 1 + n ( s I + s II + s III ) n Ê dW - – --- ( s I + s II + s III ) 2 ˝ --------- ˆ = --- Ì ------------ -------------------------------------Ë dV ¯ spherical stress 3 E 2Ó E ˛ 2

© 2003 by CRC Press LLC

It creates

TX846_Frame_C14 Page 275 Monday, November 18, 2002 12:30 PM

One obtains then by replacing: 1Ï1 + n 2 n 2 2 2 Ê dW --------- ˆ = --- Ì ------------ ( s I + s II + s III ) – --- ( s I + s II + s III ) º Ë dV ¯ distorsion E 2Ó E ¸ 1 + n ( s I + s II + s III ) n º – ----------- --------------------------------------- + --- ( s I + s II + s III ) 2 ˝ 3 E E ˛ 2

2 ( s I + s II + s III ) ¸ 1 Ï 2 dW 2 2 -˝ then: Ê --------- ˆ = ------- Ì ( s I + s II + s III ) – -------------------------------------Ë dV ¯ distorsion 4G Ó 3 ˛

(14.1)

One can rewrite as following the quantity in brackets: 2 2 --- { s I + s 2II + s 2III – s I s II – s II s III – s III s I } 3 2 --- { ( s I + s II + s III ) 2 – 3 ( s I s II + s II s III + s III s I ) } 3 1 2 Ê dW --------- ˆ = ------- { ( s I + s II + s III ) º Ë dV ¯ distorsion 6G º – 3 ( s I s II + s II s III + s III s I ) }

(14.2)

Remarks: If one denotes as n the direction making the same angle with each of the principal directions (following Figure 14.1), one observes on the face with the normal n, a stress s such that: s = S(n) that is: Ï sI / 3 ¸ Ô Ô {s } = Ì s II / 3 ˝ Ô Ô Ó s III / 3 ˛ which can be decomposed as: A normal stress: sn = s ◊ n

s I + s II + s III s n = -----------------------------3

then:

The above consists of the average or isotropic part of the stress tensor.

2

A shear stress:

t = 2

s – sn 2

2

Recall the expression sI + sII + sIII that constitutes the first scalar invariant of the stress tensor.

© 2003 by CRC Press LLC

TX846_Frame_C14 Page 276 Monday, November 18, 2002 12:30 PM

then:

s I + s II + s IIIˆ 2 ¸ 1Ï 2 2 2 2 - ˝ t = --- Ì s I + s II + s III – ÊË ------------------------------¯ 3 3Ó ˛ which can be compared with Equation 14.1. Thus, 1 3 2 Ê dW --------- ˆ = ------- Ê --- t ˆ Ë dV ¯ distorsion 2G Ë 2 ¯ The shear stress t also appears as the shear characteristic of the distortion energy. One recognizes in Equation 14.2 the presence of the first and second scalar invariants of the stress tensor independent of the coordinate system. In coordinate axes other than the principal directions, the second invariant can be written as: ( s 11 s 22 – t 12 ) + ( s 22 s 33 – t 23 ) + ( s 33 s 11 – t 31 ) 2

2

2

One then has for any coordinate system: 1 2 Ê dW --------- ˆ = ------- { ( s 11 + s 22 + s 33 ) º Ë dV ¯ distorsion 6G º – 3 ( ( s 11 s 22 – t 212 ) + ( s 22 s 33 – t 223 ) + ( s 33 s 11 – t 231 ) ) } then: 1 2 2 Ê dW --------- ˆ = ---------- { ( s 11 – s 22 ) + ( s 22 – s 33 ) º Ë dV ¯ distorsion 12G º + ( s 33 – s 11 ) 2 + 6 ( t 212 + t 223 + t 231 ) } The elastic domain (where the distortion energy is below a certain critical value) can then be characterized by the condition: 2 2 2 a { ( s 11 – s 22 ) + ( s 22 – s 33 ) + ( s 33 – s 11 ) º

º + 6 ( t 212 + t 223 + t 231 ) } < 1

(14.3)

To determine the constant, a uniaxial test is sufficient; in effect if one denotes by se the elastic limit obtained from a tension–compression test, one has: a ¥ 2 se = 1 2

then: a = 1/2 s e

2

© 2003 by CRC Press LLC

TX846_Frame_C14 Page 277 Monday, November 18, 2002 12:30 PM

Figure 14.2 Principal Axes for an Orthotropic Ply

14.2 ORTHOTROPIC MATERIAL: HILL–TSAI CRITERION 14.2.1 Preliminary Remarks A parallel with the Von Mises criterion can be seen with the following remarks: For an orthotropic material, the principal directions for the stresses do not coincide with the orthotropic directions, unlike the isotropic case. A uniaxial test is not enough to determine all the terms of the equation for the criterion because the mechanical behavior changes with the direction of loading. For the fiber/resin composites, the elastic limit corresponds with the rupture limit. The rupture strengths are very different when loading is applied along the l direction or along the t direction. The rupture strengths are different in tension as compared with in compression. One can then write in the orthotropic coordinates ,t,z — shown in Figure 14.2 — an expression similar to Equation 14.3, as: a ( s – s t ) + b ( s t – s z ) + c ( s z – s ) + d t z + e t tz + f t t £ 1 2

2

2

2

2

2

(14.4)

14.2.2 Case of a Transversely Isotropic Material In the following, we will limit ourselves, for the purpose of simplification, to the 3 case of a transversely isotropic material. The constants a, b, c, d, e, f in Equation 14.4 above will be determined using the results of the following tests: Test along the longitudinal direction : 1 a + c = ------2s rupture 3

For an orthotropic material, the procedure is identical.

© 2003 by CRC Press LLC

TX846_Frame_C14 Page 278 Monday, November 18, 2002 12:30 PM

Test along the transverse direction t: 1 a + b = ------2 s t rupture Test along the transverse direction z: due to transverse isotropy:

1 b + c = ------2 s t rupture then:

1 a = c = ---------22 s rupture 1 1 – ---------2 b = ------2 s t rupture 2 s

rupture

Shear tests:

1 t t Æ f = -----2t t rupture

1 t tz Æ e = -----2t tz rupture 1 t Æ d = -----2t t rupture

z

due to transverse isotropy. Replacing in Equation 14.4:

1 ---------2 2 s

{ ( s – st ) + ( s – sz ) } º 2

2

rupture

t tz 1 1 1 ˆ 2 º – Ê ---------------------- ( t 2t + t 2z ) + -------------------£1 - – ------------------ ( s t – s z ) + ------------------2 2 2 Ë 2 s2 ¯ t t rupture t tz rupture s t rupture rupture 2

© 2003 by CRC Press LLC

TX846_Frame_C14 Page 279 Monday, November 18, 2002 12:30 PM

4

and in developing :

s st + sz s 2 1 ------------------- + ------------------ – ------------------- – ------------------ ˆº - ( s t + s z ) + s z s t Ê ------------------2 2 2 2 Ë s2 ¯ s rupture s t rupture s rupture s rupture t rupture 2

2

2

t tz t + t z º + t-------------------- £1 + ------------------2 2 t t rupture t tz rupture 2

2

2

(14.5)

Remark: For the case of a “three-dimensional” orthotropic material, an analogous reasoning to the previous presentation leads to a more general criterion, which can be written as:

s st sz 1 1 1 ˆ ------------- + ------------- – ------------+ -----------s st º + -----------– Ê ------------2 2 2 2 2 2 Ë s rupt. s t rupt. s z rupt. s rupt. s t rupt. s z rupt.¯ 2

2

2

1 1 1 1 1 ˆ 1 ˆ º – Ê ------------ + ------------– ------------s t s z – ÊË ------------+ ------------– ------------ sz s º 2 2 2 2 2 Ë s2 ¯ ¯ s s s s s t rupt. z rupt. z rupt. rupt. rupt. t rupt.

tt t tz tz º + ------------- + ------------- + --------------£1 2 2 2 t t rupt. t tz rupt. t z rupt. 2

2

2

14.2.3 Case of a Unidirectional Ply Under In-Plane Loading When the stress state is plane-stress, in the plane defined by the axes ,t (see Figure 14.2), one has

s z = t z = t tz = 0 Equation 14.5 is simplified, and one obtains what is called “the Hill–Tsai criterion” for a ply subject to stresses within its plane:

s st s st tt ------------------ + ----------------- – ------------------ + ------------------ 0) and Equations 14.7, s rupture will be the limit stress in compression, and st rupture the limit stress in tension for 0∞ £ q £ 90∞.

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 283 Monday, November 18, 2002 12:30 PM

15 COMPOSITE BEAMS IN FLEXURE Due to their slenderness, a number of composite elements (mechanical components or structural pieces) can be considered as beams. A few typical examples are shown schematically in Figure 15.1. The study of the behavior under loading of these elements (evaluation of stresses and displacements) becomes a very complex problem when one gets into three-dimensional aspects. In this chapter, we propose a monodimensional approach to the problem in an original method. It consists of the definition of displacements corresponding to the traditional stress and moment resultants for the applied loads. This leads to a homogenized formulation for the flexure—and for torsion. This means that the equilibrium and behavior relations are formally identical to those that characterize the behavior of classical homogeneous beams. Utilization of these relations for the calculation of stresses and displacements then leads to expressions that are analogous to the common beams. We will limit ourselves to the composite beams with constant characteristics (geometry, materials) in any cross section, made of different materials—which we call phases —that are assumed to be perfectly bonded to each other. To clarify the procedure and for better simplicity in the calculations, we will limit ourselves in this chapter to the case of composite beams with isotropic phases. The extension to the transversely isotropic materials is immediate. When the phases are orthotropic, with eventually orthotropic directions that are changing from one point to another in the section, the study will be analogous, with a 1 much more involved formulation.

15.1 FLEXURE OF SYMMETRIC BEAMS WITH ISOTROPIC PHASES In the following, D symbolizes the domain occupied by the cross section, in the y,z plane. The external frontier is denoted as ∂D. One distinguishes also (see Figure 15.2) the internal frontiers which limit the phases, denoted by lij for two contiguous phases i and j. The area of the phase i is denoted as Si; its moduli of elasticity are denoted by Ei and Gi. The elastic displacement at any point of the beam has the components: ux (x, y,z); uy (x,y,z); uz (x,y,z). The beam is bending in the plane of symmetry x,y under external loads which are also symmetric with respect to this plane. 1

The only restrictive condition lies in the fact that one of the orthotropic directions is supposed to remain parallel to the longitudinal axis of the beam.

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 284 Monday, November 18, 2002 12:30 PM

Figure 15.1 Composite Beams

Figure 15.2 Composite Beam, with Plane of Symmetry

15.1.1 Degrees of Freedom 15.1.1.1 Equivalent Stiffness One writes in condensed form the following integrals taken over the total cross 2 section : · ESÒ =

Ú

=

E i dS or

D

ÂE S

i i

i

number of phases

· EI zÒ =

Ú

ÂE I

=

2

E i y dS or

D

i zi

i

number of phases

· GSÒ =

Ú

D

G i dS or

=

ÂG S

i i

i

number of phases

2

Izi is the quadratic moment of the Phase i with respect with z axis.

© 2003 by CRC Press LLC

(15.1)

TX846_Frame_C15 Page 285 Monday, November 18, 2002 12:30 PM

15.1.1.2 Longitudinal Displacement By definition, longitudinal displacement is denoted by u(x) and written as: 1 u ( x ) = -----------· ESÒ

Ú

D

E i u x ( x, y, z )dS

which consists of a mean displacement u(x) and an incremental displacement Dux as: u x ( x, y, z ) = u ( x ) + Du x ( x, y, z ) where one notes that:

Ú

D

E i Du x dS = 0

(15.2)

15.1.1.3 Rotations of the Sections By definition, this is the fictitious rotation—or equivalent—given by the following expression: –1 q z ( x ) = ------------· EI zÒ

Ú

E i u x ( x, y, z ) ¥ y dS

Ú

E i y dS +

D

Or, with the above: –1 Ï q z ( x ) = ------------- Ì u ( x ) · EI zÒ Ó

D

¸ E i Du x ( x, y, z )y dS ˝ D ˛

Ú

15.1.1.4 Elastic Center Origin 0 of the coordinate y is chosen such that the following integral is zero:

Ú

D

E i y dS = 0

We call elastic center the corresponding point 0 that is located as in the expression above. Then Dux takes the form: Du x ( x, y, z ) = – y q z ( x ) + h x ( x, y, z ) 3

with :

Ú

D

E i h x y dS

and

Ú

D

E i h x dS = 0

(*)

The displacement ux (x,y,z) can then take the form: u x ( x, y, z ) = u ( x ) – y q z ( x ) + h x ( x, y, z ). 3

In what follows, the second property is the consequence of Equation 15.2.

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 286 Monday, November 18, 2002 12:30 PM

15.1.1.5 Transverse Displacement along y Direction By definition, this is v(x) that is given by the following expression: 1 v ( x ) = -----------· GSÒ

Ú

D

G i u y ( x, y, z )dS

It follows from this definition that: u y ( x, y, z ) = v ( x ) + h y ( x, y, z ) where one notes that:

Ú

G i h y dS = 0.

D

15.1.1.6 Transverse Displacement along z Direction By definition, this is w(x) given by 1 w ( x ) = -----------· GSÒ

Ú

D

G i u z ( x, y, z )dS

It follows from this definition and from the existence of the plane of symmetry x,y of the beam a zero average transverse displacement, as: w(x) = 0. u z ( x, y, z ) = 0 + h z ( x, y, z ),

with

Ú

D

G i h z dS = 0.

In summary, we obtain the following elastic displacement field: Ê u x = u ( x ) – y q z ( x ) + h x ( x, y, z ) Á u = v(x ) + h y ( x, y, z ) Á y Ë uz = h z ( x, y, z )

(15.3)

The origin of the axes is the elastic center such that:

Ú

D

E i y dS = 0

(15.4)

The three-dimensional incremental displacements hx, hy, hz with respect to the unidimensional approximation u, v, qz verify the following:

Ú E h dS = Ú Ú G h dS = 0 Ú G h dS = 0 i

x

D

D

i

y

i

z

D

D

© 2003 by CRC Press LLC

E i y h x dS = 0 (15.5)

TX846_Frame_C15 Page 287 Monday, November 18, 2002 12:30 PM

Remarks: hx represents the longitudinal distortion of a cross section, that is, the quantity that this section displaces out of the plane which characterizes it if it moves truly as a rigid plane body. hy and hz represent the displacements that characterize the variations of the form of the cross section in its initial plane.

15.1.2 Perfect Bonding between the Phases 15.1.2.1 Displacements The bonding is assumed to be perfect. Then the displacements are continuous when crossing through the interface between two phases in contact. For two phases in contact i and j, one has: ux i

= ux j

uy i

= uy j

uz i

= uz j

15.1.2.2 Strains For the phases i and j in Figure 15.3, in the plane of an elemental interface with a normal vector of n, the relations between the strain tensors e are: x ◊ e(x) i = x ◊ e(x) j t ◊ e(x) i = t ◊ e(x) j t ◊ e( t ) i = t ◊ e( t ) j which can also be written as:

e xx = e xx i j – e xy n z + e xz n y = – e xy n z + e xz n y i

i

j

j

e yy n – 2 e yz n y n z + e zz n = e yy n – 2 e yz n y n z + e zz n y 2 z

i © 2003 by CRC Press LLC

2 y

i

i

2 z

j

2

j

j

TX846_Frame_C15 Page 288 Monday, November 18, 2002 12:30 PM

Figure 15.3 Interface between Two Phases

15.1.2.3 Stresses The stress vector s = S ( n ), where S represents the stress tensor, remains continuous across an element of the interface with normal n as:

t xy n y + t xz n z = t xy n y + t xz n z i

i

j

j

s yy n y + t yz n z = s yy n y + t yz n z i i j j t yz n y + s zz n z = t yz n y + s zz n z i

i

j

(15.6)

j

15.1.3 Equilibrium Relations Starting from the local equilibrium, in the absence of body forces, we have

∂s ij --------- = 0 ∂ xj By integrating over the cross section: d -----dx

Ú

D

s xx dS +

∂ t xzˆ xy Ê ∂t --------- + --------- dS = 0 Ë ∂y ∂z ¯ D

Ú

where the normal stress resultant Nx appears as: Nx =

Ú

D

s xx dS .

Then, transforming the second integral to an integral over the frontier ∂D of D : 4

dN ---------x + dx 4

∂t xy

∂t xz

Ú

∂D

( t xy n y + t xz n z )dG = 0

- + ------ )dS = Ú ∂ D ( t xy n y + t xz n z )d G is made possible due to the contiNote that equality Ú D ( -----∂y ∂z nuity of the expression (txy ny + txz nz) across the interfaces between the different phases (see Equation 15.6).

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 289 Monday, November 18, 2002 12:30 PM

in which ny and nz are the cosines of the outward normal n , and d G represents element of frontier ∂D. If one assumes the absence of shear stresses applied over the lateral surface of the beam, then txy ny + txz nz = 0 along the external frontier ∂D. Then for longitudinal equilibrium we have5 dN ---------x = 0 dx d -----dx

Ú

D

t xy dS +

∂t yzˆ yy Ê ∂s ---------- dS = 0 + --------Ë ∂y ∂z ¯ D

Ú

where one recognizes the shear stress resultant: Ty =

Ú

D

t xy dS.

Then transforming the second integral into an integral over the external frontier 6 ∂D of the domain D of the cross section :

∂T --------y + ∂x

Ú

( s yy n y + t yz n z )d G = 0

∂D

if one remarks that:

Ú

∂D

(s yy n y + t yz n z )d G =

Ú

∂D

y ◊ S ( n )d G = y ◊

Ú

∂D

s dG = p y ( N/m )

which is the transverse density of loading on the lateral surface of the beam, transverse equilibrium can be written as: dT y --------- + p y = 0 dx d -----dx

5

Ú

D

– y s xx dS +

∂t xy ∂ t xzˆ - + ---------- dS = 0 – y Ê --------Ë ∂y ∂z ¯ D

Ú

We have neglected the body forces which appear in the local equation of equilibrium in the form of a function fx. If these exist (inertia forces, centrifugal forces, or vibration inertia, for dN - + p x = 0 in which p x = Ú D f x dS represents the example), one obtains for the equilibrium: -----dx longitudinal load density. ∂s ∂t - ) dS = Ú ∂D ( s yy n y + t yz n z )d G is made possible due to the Note that the equality Ú D ( ------+ -----∂y ∂z x

6

yy

yz

continuity of the expression (syy ny + tyz nz ) across the frontier lines between different phases (see Equation 15.6).

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 290 Monday, November 18, 2002 12:30 PM

where appears the moment resultant: Mz =

Ú

D

– y s xx dS.

7

Then transforming the second integral : dM ----------z + dx

Ú

∂D

– y ( t xy n y + t xz n z ) dG +

Ú

D

t xy dS = 0

where one notes that:

Ú

∂D

– y ( t xy n y + t xz n z ) dG =

Ú

∂D

– yx ◊ S ( n )dG º =

Ú

∂D

– y ( s ◊ x ) dG = m z ( mN/m )

which can be called a density moment on the beam. Then one obtains the equilibrium relation: dM ----------z + T y + m z = 0 dx The case where a density moment could exist in statics is practically nil, we therefore assume that mz = 0. In summary, one obtains for the equations of equilibrium: dN ---------x = 0 dx dT y --------- + p y = 0 dx dM ----------z + T y = 0 dx

(15.7)

15.1.4 Constitutive Relations Taking into account the isotropic nature of the different phases, the constitutive relation can be written in tensor form for Phase i as: 1 + ni ni – ----tr ( S )I e = -------------S Ei Ei

7

( I = unity tensor)

Analogous note for the continuity of the expression (txy ny + txz nz) across the lines of internal interfaces (Equation 15.6).

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 291 Monday, November 18, 2002 12:30 PM

One deduces, in integrating over the domain occupied by the cross section of the beam:

Ú

D

Ú

e xx E i dS =

D

s xx dS –

Ú

D

n i ( s yy + s zz )dS

Taking into account the form of the displacements in Equation 15.3, one can write

Ú

D

e xx E i dS =

∂u dq ---------x E i dS = – ---------z ∂ x dx D

Ú

∂ E i dS + -----x ∂ D

du yE i dS + ------dx D

Ú

Ú

Ú

D

E i h x dS

which leads, with the notation in Equation 15.1, to the relation: du N x = · ESÒ ------- + dx

Ú

D

Ú

– y e xx E i dS =

D

Ú

D

– y s xx dS +

n i ( s yy + s zz )dS

Ú

D

(15.8)

n i y( s yy + s zz ) dS

Taking into account the form of the displacements in Equation 15.3 one can write dq – y e xx E i dS = ---------z dx D

du 2 E i y dS – ------dx D

Ú

Ú

∂ E i y dS – -----∂x D

Ú

Ú

E i y h x dS

D

This leads, with the notation in Equation 15.1, to the relation: dq M z = · EI zÒ ---------z – dx

Ú

D

Ú

D

n i y ( s yy + s zz ) dS

2 e xy G i dS =

Ú

D

t xy dS

(15.9)

Taking into account the form of the displacements in Equation 15.3, one can write

Ú

D

2 e xy G i dS =

u x ∂u yˆ Ê ∂-------- + -------- G i dS = – q z Ë ∂x ¯ D ∂y

Ú

º+

∂h dv G i ---------x dS + -----∂y dx D

Ú

G i dS º

D

∂ G i dS + -----∂x D

Ú

Ú

Ú

D

h y G i dS

which gives with the notation in Equation 15.1, the relation: dv T y = · GSÒ Ê ------ – q zˆ + Ë dx ¯ © 2003 by CRC Press LLC

∂h Gi ---------x dS ∂y D

Ú

(15.10)

TX846_Frame_C15 Page 292 Monday, November 18, 2002 12:30 PM

15.1.5 Technical Formulation 15.1.5.1 Simplifications We extend to the composite beams the simplifications made for the homogeneous beams as: 1. syy and szz ---------z (Equation 15.9) and N x # < ES > ------- (Equation 15.8): dx dx Mz Nx - y + E i ----------s xx = – E i -----------· EI zÒ · ESÒ bending

(15.11)

extension

Remark: The continuity (exx )i = (e xx )j at the interface between the Phases i and j leads to 10

( s xx ) i ( s xx ) -------------- = --------------j Ei Ej

8

9

10

This hypothesis is better verified by the fact that the Poisson coefficients of the different phases have similar values. This hypothesis is known in the literature for the homogeneous beams as the generalized “Navier–Bernoulli” hypothesis. See Section 15.1.2.

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 293 Monday, November 18, 2002 12:30 PM

Figure 15.4 Normal and Bending Stresses

which shows the discontinuity of normal stresses due to the difference in the longitudinal moduli, as illustrated in Figure 15.4.

15.1.5.3 Shear Stress Expression 15.1.5.3.1 Characterization of Warping Starting from the local equilibrium described by the relation:

∂s ij --------- = 0 ∂ xj we study the flexure shear stress in the plane of the cross section, noted as:

t = t xy y + t xy z Taking into consideration Equations 15.11 and 15.7, and the simplification 2, at the beginning of Section 15.1.5.1, one can write E i dN x E i dM z ∂t xy ∂ t xz Ei ∂s xx ---------- + ---------- = – ---------- ----------y – ----------- --------- = – ------------ = ------------T ¥ y ∂y ∂z · EI zÒ dx · ESÒ dx ∂x · EI zÒ y and with the displacement field in Equation 15.3:

∂h ∂h Ei -¥y G i Ê ----------2-x + ----------2-xˆ = – T y -----------Ë ∂y ¯ · EI zÒ ∂z 2

2

Putting hx in the form: Ty ¥ g ( y,z ) h x = -----------·GS Ò © 2003 by CRC Press LLC

(15.12)

TX846_Frame_C15 Page 294 Monday, November 18, 2002 12:30 PM

leads to E · GSÒ 2 — g = – -----i ------------- ¥ y G i · EI zÒ

(15.13)

and Equation 15.10 becomes dv T y = · GSÒ Ê ------ – q zˆ + Ë dx ¯ 1 T y Ê1 – -----------Ë · GSÒ

Ty ∂ g ------ dS G i -----------· GS Ò ∂y D

Ú

∂g dv G i ------ dSˆ = · GSÒ Ê ------ – q zˆ ¯ Ë ¯ ∂ y dx D

Ú

or: · GSÒ dv T y = ------------ Ê ------ – q zˆ ¯ k Ë dx

(15.14)

In the above relation appears a k coefficient which is analogous to the shear coefficient for homogeneous beams.

15.1.5.3.2 External Limit Condition We have supposed that the lateral surface of the beam is free from shear. This gives, along the external contour ∂D of the cross section, the relation:

t ◊ n = t xy n y + t xz n z = 0, and, with the displacement field in Equation 15.3 and the simplifications described above: dv Ê -----– q zˆ n y + grad h x ◊ n = 0 Ë dx ¯ Introducing the function g(y,z) (Equation 15.12) and with 15.14, one obtains

∂g grad g ◊ n = ------- = – kn y ∂n Substituting the function g(y,z) with the function go (y,z) such that: g o ( y,z ) = g ( y,z ) + k ¥ y © 2003 by CRC Press LLC

(15.15)

TX846_Frame_C15 Page 295 Monday, November 18, 2002 12:30 PM

one verifies that go is solution of the problem: E · GSÒ Ï — 2 g o = – -----i ------------ ¥ y in domain D G i · EI zÒ Ô Ì go Ô ∂------Ó ∂ n- = 0 on the boundary ∂ D We denote go(y,z) as the longitudinal warping function for the cross section.

15.1.5.3.3 Conditions at the Interfaces The continuity conditions already described in Section 15.1.2 lead for the warping function, at the interface between two phases i and j, g oi = g oj

t xyi n y + t xzi n z = t xyj n y + t xzj n z then:

∂g ∂g G i --------oi- = G j --------oj∂n ∂n

15.1.5.3.4 Uniqueness of the Solution This is given by Equation 15.5 which is interpreted here as:

Ú

D

E i g o dS = 0

15.1.5.3.5 Form of the Shear Stresses One can easily verify the following expressions: Ty ∂ go -------t xy = G i -----------· GSÒ ∂ y Ty ∂ go -------t xz = G i -----------· GSÒ ∂ z then again: Ty t = G i ------------grad go · GSÒ

15.1.5.3.6 Shear Coefficient for the Section The shear coefficient for the section is obtained starting from the Equation 15.5:

Ú

D

© 2003 by CRC Press LLC

E i h x dS = 0

TX846_Frame_C15 Page 296 Monday, November 18, 2002 12:30 PM

This necessitates the knowledge of the warping function go. Then the above relation can be rewritten as: Ty E i -----------( g – k ¥ y ) ¥ y dS = 0 · GS Ò o D

Ú which leads to:

1 k = ------------· EI zÒ

Ú

E i g o ydS

D

In summary, in the absence of body forces (inertia forces for example), the bending of a composite beam in its plane of symmetry can be characterized by a homogenized formulation — equivalent to a classical homogeneous beam solution—in the following manner:

• Elastic center 0: it is such that

Ú

D

E i ydS = 0

• Equivalent stiffnesses: (15.16) · ESÒ =

ÂE S ; i i

i

· EI zÒ =

ÂE I

i zi

i

;

· GSÒ ------------ = k

Â i

1 G i S i ¥ --k

• Equilibrium relations: (stress resultants calculated at elastic center) dT dN x --------- = 0; --------y + p y = 0; dx dx • Constitutive relations: du N x = · ESÒ ------- ; dx

© 2003 by CRC Press LLC

dM ----------z + T y = 0 dx

· GSÒ dv T y = ------------ Ê ------ – q zˆ ; ¯ k Ë dx

dq M z = · EI zÒ ---------z dx

TX846_Frame_C15 Page 297 Monday, November 18, 2002 12:30 PM

(Contd.)

Stresses: Mz Nx - y + E i ----------s xx = – E i -----------· EI zÒ · ESÒ

normal stresses

Ty ∂ go -------- ¸ t xy = G i -----------· GSÒ ∂ y Ô Gi gradg o ˝ t = ------------T · GS Ò y Ty ∂ go Ô t xz = G i ------------ -------- ˛ · GSÒ ∂ z

shear stresses

• longitudinal warping function go(y, z): it is the solution to the problem Ï ∂ 2g ∂ 2g Ô ----------o + ----------o = Ô ∂ y2 ∂ z2 Ì ∂ go Ô -------- = Ô ∂n Ó

E · GSÒ – -----i ------------- y in domain D of the section. G i · EI zÒ

(15.16)

0 on the boundary ∂ D

with internal continuity: ¸ Ô ∂ g oi ∂ g oj ˝ along internal boundaries ij G i --------- = G j --------- Ô ∂n ∂n ˛ g oi = g oj

and the uniqueness condition:

Ú

D

E i g o dS = 0

Shear coefficient k: it is given by the formula: 1 k = ------------· EI zÒ

Ú

E i g o y dS

D

15.1.6 Energy Interpretation 15.1.6.1 Energy Due to Normal Stresses sxx Denoting by dWs as the deformation energy of an elementary portion of a beam with length dx due to the application of normal stresses sxx, one has Ï1 1 dW s = --- s xx e xx dV = Ì --2 Ó2

Ú

© 2003 by CRC Press LLC

s xx ¸ -------- dS ˝dx D Ei ˛

Ú

2

TX846_Frame_C15 Page 298 Monday, November 18, 2002 12:30 PM

Taking into account Equation 15.11 for the normal stresses: dW 1 ----------s- = --dx 2 1 = --2

2 Ei Ei 1 - M z y + ----------- N x dS ---- – -----------· EI zÒ · ESÒ D Ei

Ú

2

Mz 2 1 -2 y dS + --E i -------------2 D · EI zÒ

Ú

2

Nx -2 dS º E i ------------D · ESÒ

Ú

Mz Nx -y dS E i -----------------------· EI zÒ · ESÒ D

Ú

º+

(the above expression simplifies due to the definition of the elastic center 0 in 15.16); therefore: 2

2

dW 1 Mz 1 Nx ----------s- = --- ------------ + --- ----------dx 2 · EI zÒ 2 · ESÒ

15.1.6.2 Energy Due to Shear Stresses t Denoting dWt as the deformation energy of an elementary portion of a beam with length dx due to the application of shear stresses t , one has: 1 dW t = --2

1Ï 2 ( t xy e xy + t xz e xz )dV = --- Ì 2Ó D

Ú

¸ 1 2 2 ----- ( t xy + t xz )dS ˝ dx G D i ˛

Ú

then, taking into account the form of the shear stresses in 15.16: dW 1 -----------t = --dx 2

T y Ï Ê ∂ g oˆ 2 Ê ∂ g oˆ 2 ¸ -2 Ì -------- + -------- ˝ dS G i -------------D · GSÒ Ó Ë ∂ y ¯ Ë ∂ y ¯ ˛ 2

Ú

2

dW t 1 Ty ----------- = --- -------------dx 2 · GSÒ 2

Ï∂ ¸ ∂g ∂g ∂ 2 G i Ì ------ Ê g o --------oˆ + ------ Ê g o --------oˆ – g o ◊ — g o ˝ dS Ë ¯ Ë ¯ ∂y ∂z ∂z D Ó ∂y ˛

Ú

11

with the value from 15.16 of the Laplacian of the warping function go : dW t 1 Ty Ï ----------- = --- -------------dx 2 · GSÒ 2 ÌÓ 2

11

∂ go

E · GSÒ Gi g o -----i ------------- ydS + G D i · EI zÒ

Ú

∂ go

∂ go

¸ ∂g G i g o --------o dG ˝ ∂ n ∂D ˛

Ú

∂ The equality Ú D G i { ∂---∂-y ( g o ----is made possible due the continuity of ) + ∂---z- ( g o ----) } dS = Ú ∂D G i g o -----dG ∂n ∂y ∂y g the quantities G i g o ∂----at the interfaces lij (See Section 15.1.5.3.3, “Conditions at the Interfaces”). o

∂n

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 299 Monday, November 18, 2002 12:30 PM

One knows in the above the expression of the shear coefficient k for the section (see 15.16). Then: 2

dW t 1 Ty ----------- = --- k -----------dx 2 · GSÒ In summary, the strain energy density can be written as: 2

2

2

1 Mz 1 Ty dW 1 N x - + --- k -------------------- = --- ------------ + --- -----------dx 2 · ESÒ 2 · EI zÒ 2 · GSÒ

(15.17)

Remarks: Note the analogy between this expression and that for the strain energy of a classical homogeneous beam, which should be written here as: 2

2

2

dW 1N 1M 1 T --------- = --- -----x- + --- ------z- + --- k ------ydx 2 ES 2 EI z 2 GS As a practical consequence of this homogenization, it becomes possible to determine the equivalent characteristics which are necessary for the entry of data into a computer program utilizing finite elements of classical homogeneous beams. The problem then comes to the numerical evaluation of the following values: Equivalent moduli: Eequivalent, Gequivalent, (or nequivalent) Geometric characteristics: Sequivalent, Iz

, and k

equivalent

By taking Sequivalent = S (real area of the cross section), one can easily verify that: E

· ESÒ · GSÒ G = ------------ ; = -----------equivalent S S · EI zÒ 1 · ESÒ n = -----------------; = --- ------------ – 1 equivalent E 2 · GSÒ

equivalent

Iz

equivalent

equivalent

15.1.7 Extension to the Dynamic Case The equilibrium relations of Section 15.1.3. were written in the absence of body forces. In vibratory motions, these body forces exist in the form of inertia forces. One then has

∂s ij --------- – r ü i = 0 ∂ xj © 2003 by CRC Press LLC

TX846_Frame_C15 Page 300 Monday, November 18, 2002 12:30 PM

Following the main steps of the calculations in Section 15.1.3, for a beam under 12 free vibration, one obtains: 2 ∂ Nx ∂ --------- = -------2 ∂x ∂t

Ú

r i u x dS

D

which leads, with Equation 15.3, to the following expression: 2 ∂ Nx ∂q ∂u --------- = · r S Ò --------2- – y G · r S Ò ---------2-z ∂x ∂t ∂t 2

in which we denote ·r S Ò =

Ú

D

r i dS

y G ·r S Ò =

and

Ú

D

r i y dS.

yG appears here as the ordinate of the mass center (center of gravity) of the section. One has neglected the secondary coupling due to hx: 2 ∂T ∂ --------y = -------2 ∂x ∂t

Ú

r i u y dS

D

with Equation 15.3 and neglecting the secondary coupling due to hx: 2 ∂T ∂v --------y = · r SÒ -------2∂x ∂t 2 ∂ Mz ∂ ---------- + T y = -------2 ∂x ∂t

Ú

D

– y r i u x dS

with Equation 15.3, posing · r I zÒ = Ú D r i y dS , and neglecting the secondary coupling due to hx: 2

2 ∂ Mz ∂q ∂u ---------- + T y = · r I zÒ ---------2-z – yG · r SÒ --------2∂x ∂t ∂t 2

The above relations are to be joined with the constitutive relations in 15.16. However one must note these constitutive relations were written in the absence of body forces. Nevertheless, we will consider them to be valid, with the condition that the concerned frequencies are not too high. Generally this case corresponds to the mechanical frequencies, and one denotes this as the “quasi static” domain. 12

One removes all the forces and moments on the beam except inertial forces and moments.

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 301 Monday, November 18, 2002 12:30 PM

In summary, in dynamic regime, one has to replace the equilibrium relations and the constitutive behavior which appear in 15.16 with the following relations: • Governing equations (stress resultants calculated at elastic center): 2 ∂ Nx ∂q ∂u --------- = · r S Ò --------2- – y G · r S Ò ---------2-z ∂x ∂t ∂t 2

2 ∂ Tx ∂v -------- = ·r S Ò -------2∂x ∂t

(15.18)

2 ∂ Mz ∂q ∂u ---------- + T y = · r I z Ò ---------2-z – y G · r S Ò --------2∂x ∂t ∂t 2

with · r SÒ =

Âr S ; i i

Âr I

· r I zÒ =

i zi

i

;

y G · r SÒ =

i

Ú

D

r i y dS

• Constitutive relations:

∂u N x = · ESÒ ------; ∂x

· GSÒ ∂ v T y = ------------ Ê ------ – q zˆ ; ¯ k Ë ∂x

∂q M z = · EI zÒ --------z ∂x

Remark: We note in the above relations a nonclassical coupling between the longitudinal oscillations u(x,t) and flexural oscillations. This coupling disappears 13 if the elastic center is mixed with the center of gravity.

15.2 CASE OF ANY CROSS SECTION (ASYMMETRIC) Now, the cross section of the beam does not present any particular symmetry (see Figure 15.5). One can consider for this general case the procedure adopted in the previous paragraph for beams with symmetry. One notes the supplementary equivalent stiffness: ·EI y Ò =

Ú

D

E i z dS = 2

Â EI

i yi i number of phases

It also appears an equivalent rotation qy(x) defined by the expression: 1 q y ( x ) = ------------· EI y Ò

Ú

D

E i u x ( x, y,z ) ¥ z dS

Then, from the definitions of qy, u, and qz (Section 15.1.1): 1 q y ( x ) = ------------· EI y Ò 13

See Chapter 18, Application 18.3.9.

© 2003 by CRC Press LLC

Ú

D

E i { u – y q z + h ox } ¥ z dS

TX846_Frame_C15 Page 302 Monday, November 18, 2002 12:30 PM

Figure 15.5 Composite Beam with any Cross Section

this expression simplifies if one chooses the origin of the coordinate z such that:

Ú

D

E i z dS = 0;

Ú

D

E i yz dS = 0

These relations, joined with the condition already established in the previous paragraph: Ú D E i y ds = 0 , allow one to define the position of the elastic center 0 of the section, as well as the orientation of the axes y and z that we will call the principal axes of the section. Then, in summary: elastic center:

Ú E y dS = 0 Ú E z dS = 0 Ú E yz dS = 0 i

D

i

D

principal axes:

i

D

One can then rewrite the contribution hox to the longitudinal displacement ux , which appeared above, in the form:

h ox ( x, y, z ) = z ¥ q y + h x ( x, y, z ) and one verifies that, by definition of the degree of freedom q y:

Ú

D

E i h x z dS = 0

The displacement ux (x, y, z) then takes the form: u x ( x, y, z ) = u ( x ) – y q z ( x ) + z q y ( x ) + h x ( x, y, z ) In addition, due to the disappearance of symmetry in the section, the transverse displacement w(x) (Section 15.1.1.6) is not zero. © 2003 by CRC Press LLC

TX846_Frame_C15 Page 303 Monday, November 18, 2002 12:30 PM

We then obtain for the elastic displacement field: ux = u (x ) – y qz + z qy + hx uy = v (x ) + hy uz = w ( x ) + hz The three-dimensional incremental displacements hx, hy,hz verify (see Section 15.1.1.6):

Ú

D

Ú

E i h x dS =

D

E i h x y dS =

Ú Ú

D

D

Ú

D

E i h x z dS = 0

G i h y dS = 0 G i h z dS = 0

Starting from the above and following the same procedure as in the previous paragraph, successively for the bending in the plane x,y, with identical results, then in the plane x,z, we obtain results summarized in the following relations:

• degree of freedom: u(x ) v ( x ); q y ( x )

along x: along y:

along z: w ( x ); q z ( x ) • elastic center: it is such that:

Ú

D

Ú

E i ydS =

D

E i z dS = 0

• principal axes: they are such that:

Ú

D

E i yz dS = 0

• equivalent stiffnesses: · ESÒ =

ÂE S

i i

i

· EI zÒ =

ÂE I

i zi

;

· EI yÒ =

i

· GSÒ ------------ = ky

© 2003 by CRC Press LLC

i yi

i

Â G S ¥ ----; k 1

i i

i

ÂE I

y

· GSÒ ------------ = kz

Â G S ¥ ----k1

i i

i

z

(Continued)

TX846_Frame_C15 Page 304 Monday, November 18, 2002 12:30 PM

(Contd.) • equilibrium relations: (stress resultants calculated at elastic center) dN ---------x = 0 dx dT dT y --------- + p y = 0; ---------z + p z = 0 dx dx dM z dM ---------- + T y = 0; ----------y – T z = 0 dx dx • constitutive relations: du N x = · ESÒ ------dx · GSÒ dv T y = ------------ Ê ------ – q zˆ ; ¯ k y Ë dx dq M z = · EI zÒ ---------z ; dx • normal stresses:

· GSÒ dw T z = ------------ Ê ------- + q yˆ ¯ k z Ë dx

14

(15.19)

dq M y = · EI yÒ --------y dx

Mz My Nx - y + E i ------------ z + E i ----------s xx = – E i -----------· EI zÒ · EI yÒ · ESÒ • shear stresses: Gi Ê ∂ go ∂h T y -------- + T z --------oˆ t xy = -----------Ë · GSÒ ∂y ∂y ¯ Gi Ê ∂ go ∂h T y -------- + T z --------oˆ t xz = -----------Ë · GSÒ ∂z ∂z ¯ then Gi t = ------------ ( T y grad g o + T z grad h o ) (Continued) · GSÒ

14

Remark: As already mentioned in Section 15.1.6 for a beam with a plane of symmetry, it is possible to evaluate the equivalent characteristics that one has to introduce in data form in order to utilize computer programs for the calculation by 14

· GSÒ dv

- ( ---- – q z ) it comes to a form such as: In fact, in place of the constitutive relation Ty = -------k y dx dv --- – q z ) where appears a coupling coefficient kyz. This means that a unique k y Ty + k yz Tz = · GSÒ ( dz shear resultant Tz leads to flexure in the x,y plane. This secondary effect has been neglected · GSÒ dw - + q y ). - ( ---here. Analogous remark yields for the constitutive relation T z = -------dx k z

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 305 Monday, November 18, 2002 12:30 PM

• Longitudinal warping functions: function go(y,z): It is the solution to the problem Ï ∂2 g ∂2 g E i · GSÒ Ô ----------o + ----------o = – ---- ------------- y in domain D of the section G i · EI zÒ Ô ∂ y2 ∂ z2 Ì ∂ go Ô -------- = 0 on the boundary ∂D Ô ∂n Ó with internal continuity: ¸ Ô ∂ g oi ∂ g oj ˝along internal boundaries ij G i --------- = G j --------- Ô ∂n ∂n ˛ g oi = g oj

and the uniqueness condition:

Ú

D

E i g o dS = 0

function ho(y,z): It is the solution to the problem : Ï ∂2 h ∂2 h E i · GSÒ Ô ----------o + ----------o = – ---- ------------- z in domain D of the section 2 G Ô ∂ y2 i · EI yÒ ∂z Ì ∂ ho Ô -------- = 0 on the boundary ∂D Ô ∂n Ó with internal continuity: ¸ Ô ∂ h oi ∂ h oj ˝along internal boundaries ij G i ---------- = G j ---------- Ô ∂n ∂n ˛ h oi = h oj

and the uniqueness condition:

Ú

D

E i h o dS = 0

• Shear coefficients coefficient k y : it is given by the formula: coefficient k z : it is given by the formula:

1 k y = ------------· EI zÒ

Ú

E i g o y dS

1 k z = ------------· EI yÒ

Ú

E i h o z dS

D

D

• Strain energy 2

2

2

2

2

Ty Tz 1 Mz 1 My 1 1 dW 1 N x - + --- ------------ + --- k y -------------------- = --- ------------ + --- -----------+ --- k z -----------dx 2 · ESÒ 2 · EI zÒ 2 · EI zÒ 2 · GSÒ 2 · GSÒ

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 306 Monday, November 18, 2002 12:30 PM

15

finite elements for the classical beams. The characteristics Eequivalent, Gequivalent, Iz equivalent, Iy equivalent, can be obtained right away. On the contrary, the calculation of the shear coefficients ky and kz is not direct. At first it is necessary to know the values of the functions go and ho, solutions in the domain occupied by the cross section of Poisson type problem, as one can take note in the preceding table. The nature of these problems makes it possible for each of the functions go and ho to write an equivalent functional which allows the calculation of the function considered by means of discretization of the cross section using finite elements.

15

It is convenient to note that a computer program based on elements of homogeneous beams cannot provide correct values for the stresses in a cross section, because these stresses are of particular formulation for composite beams (see 15.16).

© 2003 by CRC Press LLC

TX846_Frame_C16 Page 307 Monday, November 18, 2002 12:32 PM

16 COMPOSITE BEAMS IN TORSION As in the previous chapter, we consider here the composite beams made of isotropic phases. Extension to transversely isotropic phases is straightforward. The study of orthotropic phases with one principal direction parallel to the axis of the beam, the other two principal directions in the plane of a cross section, does not present fundamental difficulties.

16.1 UNIFORM TORSION We will keep the conventions and notations of the previous chapter. On Figure 16.1, 0 is the elastic center, x, y, and z are the principal axes. The beam is slender and uniformly twisted, this means that every cross section is subjected to a pure and constant torsion moment, along the x axis, denoted as Mx. Then, under the application of this moment, each line in the beam, initially parallel to the x axis, becomes a helicoid curve, including (in the absence of symmetry in the cross section) the line which, initially, was coinciding with the elastic x axis itself. The only line which remains rectilinear is cutting the plane of all sections at a point which will be called torsion center and denoted as C, with coordinates yC and zC in the principal axes (see Figure 16.1).

16.1.1 Torsional Degree of Freedom By definition, this is the rotation of each section about the x axis, denoted as qx. The torsional moment Mx being constant, the angle qx evolves along the x axis in such a manner that, for any pair of cross sections spaced with a distance dx, one can observe a same increment of rotation dqx; then: 1

d qx --------- = constant dx 1

Here it is not necessary to define the rotation qx by means of an integral of displacements, as in the previous chapter relating to flexure. In effect, we will see in the following that the displacement field associated with this pure rotation of the sections leads to the exact solution of the problem in the elastic domain (at least for the case of uniform warping).

© 2003 by CRC Press LLC

TX846_Frame_C16 Page 308 Monday, November 18, 2002 12:32 PM

Figure 16.1 Elastic Center (O), Torsion Center (C), and Principal Axes

From this it comes that the angle of rotation of the sections varies linearly along the longitudinal axis x. As a consequence, we assume a priori the components of the displacement field ux, uy, uz, to be written as: dq u x = ---------x ¥ j ( y, z ) dx uy = –( z – z c ) qx

(16.1)

uz = ( y – y c ) qx where the function denoted as j (y, z) is characteristic of the cross section shape and of the materials that constitute the section. This is called the warping function for torsion.

16.1.2 Constitutive Relation With the displacement field in Equation 16.1 the only nonzero strains are written as: d q ∂j g xy = ---------x ÊË ------ – ( z – z c )ˆ¯ dx ∂y d q ∂j g xz = ---------x ÊË ------ + ( y – y c )ˆ¯ dx ∂z The only nonzero stresses are then the shear stresses txy and txz. The torsional moment can be deduced by integration over the domain of the straight section as: Mx =

dq ( y t xz – z t xy ) dS = ---------x dx D

Ú

Ï Gi Ì y D Ó

Ú

∂j Ê ----- – y cˆ º Ë ∂z ¯

¸ ∂j º – z Ê ----- + z cˆ + y 2 + z 2 ˝ dS Ë∂ y ¯ ˛ © 2003 by CRC Press LLC

TX846_Frame_C16 Page 309 Monday, November 18, 2002 12:32 PM

Substituting to the function j (y, z) the function F(y,z) such that: F ( y, z ) = j ( y, z ) + yz c – zy c

(16.2)

it becomes: dq M x = ---------x ¥ dx

∂F ∂F 2 2 G i Ê y -------- – z -------- + y + z ˆ dS Ë ¯ ∂ z ∂ y D

Ú

In this expression, it is possible to define an equivalent stiffness in torsion with the form: · GJ Ò =

Ú

D

∂F ∂F 2 2 G i Ê y -------- – z -------- + y + z ˆ dS Ë ∂z ¯ ∂y

(16.3)

One obtains then for the constitutive relation:

∂q M x = · GJ Ò --------x ∂x

16.1.3 Determination of the Function F(y,z) 16.1.3.1 Local Equilibrium Local equilibrium is written as:

∂t xy ∂t xz --------- + --------- = 0 ∂y ∂z then with the displacement field in Equation 16.1: 2

— j =0 and with form 16.2 of the function F: 2

— F =0

16.1.3.2 Conditions at the External Boundary The lateral surface being free of stresses, one can write along the external boundary ∂D:

t . n = 0. With the displacement field in Equation 16.1: Ï ∂f ¸ Ï ∂f ¸ - – ( z – z c ) ˝n y + Ì ------ + ( y – y c ) ˝ n z = 0 Ì ----Ó ∂y ˛ Ó ∂z ˛ © 2003 by CRC Press LLC

TX846_Frame_C16 Page 310 Monday, November 18, 2002 12:32 PM

then again:

∂F ∂F -------n y + -------n z = zn y – yn z ∂y ∂z

16.1.3.3 Conditions at the Internal Boundaries The continuity conditions of Section 15.1.2 are verified for uy and uz. At an interfacial line lij between two phases i and j, the continuity of ux leads to Fi = Fj The continuity relations in Equation 15.6 lead to the continuity of (txy ny + txz nz) when crossing the lines lij, that produces the continuity of

∂F ∂F G i Ê ---------i – zˆ n y + G i Ê ---------i + yˆ n z Ë ∂z ¯ Ë ∂y ¯

16.1.3.4 Uniqueness of the Function F If one superimposes torsion and bending, by using the degrees of freedom for flexure defined in the previous chapter, the displacement component ux becomes: dq u x = u – y q z + z q y + ---------x j + h x dx The longitudinal displacement u(x) has to respond to its definition (Section 15.1.1), meaning 1 u = -----------· ESÒ

Ú

E i u x dS

D

1 Ï u = ------------ Ì u · ESÒ Ó

Ú

E i dS – q z

Ú

q º+d ---------x dx

E i j dS +

D

Ú

D

D

E i y dS + q y

Ú

E i z dS º

D

¸ E i h x dS ˝ D ˛

Ú

This requires that:

Ú

D

E i j dS = 0

Then, taking into account the form in Equation 16.2 of F and the properties of the elastic center:

Ú

D

© 2003 by CRC Press LLC

E i F dS = 0

TX846_Frame_C16 Page 311 Monday, November 18, 2002 12:32 PM

In summary, the function F(y,z) is the solution of the problem: Ï —2 F = 0 Ô Ì ∂F - = zn y – yn z Ô ------Ó ∂n

in domain D of the section on the external boundary ∂D

with the internal continuity: Fi = Fj

¸ Ô along the internal ∂ Fi ∂ Fj ˝ Ê ˆ Ê ˆ G i --------- – ( zn y + yn z ) = G j --------- – ( zn y + yn z ) Ô boundaries ij Ë ∂n ¯ Ë ∂n ¯ ˛ and the condition of uniqueness:

Ú

D

E i F dS = 0

16.1.4 Energy Interpretation The strain energy of an elementary segment of a beam with thickness dx is written as: Ï1 1 dW = --- 2 ( t xy e xy + t xz e xz ) dV = Ì --2 Ó2

Ú

¸ 2 2 G i ( g xy + g xz ) dS ˝ dx D ˛

Ú

then, taking into account the displacement field in Equation 16.1: dW 1 dq --------- = --- Ê ---------xˆ dx 2 Ë dx ¯

2

2 2 Ï ∂F ¸ ∂F G i Ì Ê ------- – zˆ + Ê ------- + yˆ ˝ dS ¯ Ë ¯ Ë ∂z D Ó ∂y ˛

Ú

2

which can be rewritten as : 2 dW 1 dq Ï --------- = --- Ê ---------xˆ Ì dx 2 Ë dx ¯ Ó

º+

2

Ï ∂F ∂F 2 2¸ G i Ì y ------- – z ------- + y + z ˝ dS – ∂y D Ó ∂z ˛

Ú

Ú G F— F dSº 2

i

D

Ï ∂F ¸ ¸ ∂F G i F Ì Ê ------- – zˆ n y + Ê ------- + yˆ n z ˝ d G ˝ Ë ¯ Ë ¯ ∂z ∂D Ó ∂y ˛ ˛

Ú

In effect, one has, for example: 2 2 ¸ Fˆ ∂F ∂F ∂F ∂ F ∂ Ï ∂F Ê ∂------ – z ------- = ------- Ê ------- – zˆ = ------ Ì F Ê ------- – zˆ ˝ – F --------2Ë ∂y ¯ ¯ ¯ ∂y Ó Ë ∂y ∂y ∂y Ë ∂y ∂y ˛

© 2003 by CRC Press LLC

TX846_Frame_C16 Page 312 Monday, November 18, 2002 12:32 PM

where we note the presence of the stiffness in torsion ·GJ Ò defined by Equation 16.3. Thus, dq 2 dW 1 --------- = --- · GJ Ò Ê ---------xˆ Ë dx ¯ dx 2

2

1 Mx or = --- -----------2 · GJ Ò

16.2 LOCATION OF THE TORSION CENTER Consider the cantilever beam that is clamped at its left end as shown schematically in Figure 16.2, and more particularly the segment limited by the cross sections denoted by D0 and D1. In the section D1,0 is the elastic center and C is the torsion center the position of which we wish to determine. With this objective, we will apply on the cross section D1 the two following successive loadings: Loading No. 1: One applies on the torsion center C of the cross section D1 a force F situated in the plane of the section. Loading No. 2: One applies on the same cross section D1 a torsional moment denoted as Mx (see Figure 16.2). When one applies these two loads successively, the final state is independent of the order of the application. As a consequence for the external forces acting on the isolated segment (D0 D1), the work corresponding to loading No. 1 on the displacements created by loading No. 2 is equal to the work corresponding to loading No. 2 on the displacements created by loading No. 1. This can be written in the following form: W

(loading 1¥ displacement 2)

=W

(loading 2¥ displacement 1)

Now we evaluate these works: a) W (loading 1 ¥ displacement 2) On D0: F creates the bending moments Mz and My, thus a normal stress distribution given in the principal axes by Equation 15.17 as: Mz My - ¥ y + E i ------------¥z ( s xx ) 1 = – E i -----------· EI zÒ · EI yÒ

Figure 16.2 Cantilever Beam with Two Successive Loadings © 2003 by CRC Press LLC

TX846_Frame_C16 Page 313 Monday, November 18, 2002 12:32 PM

Then, taking into account the displacement field in Equation 16.1, the work done on D0 is

Ú

D

( s xx ) 1 ¥ ( u x ) 2 dS =

Ï ¸ dq Mz My - ¥ y + E i ------------ ¥ z ˝ ---------x j dS Ì – E i -----------· EI Ò · EI Ò DÓ z y ˛ dx

Ú

dq = ---------x dx

Ï ¸ Mz My - ¥ y + E i ------------ ¥ z ˝( F – yz c + zy c )dS Ì – E i -----------· EI zÒ · EI yÒ DÓ ˛

Ú

On D1: The torsion center C does not move in the plane of the cross section during torsion. The work done by the force F in the displacement field of torsion is nil. b) W (loading 2 ¥ displacement 1) Force F as applied to the torsion center C does not lead to the rotation of the cross sections around the longitudinal axis x. From this the torsional moment Mx does not work on the bending displacement field due to F . The equality of the two works is then written as: dq ---------x dx

Ï ¸ Mz My - ¥ y + E i ------------ ¥ z ˝( F – yz c + zy c )dS = 0 Ì – E i -----------· EI zÒ · EI yÒ DÓ ˛

Ú

then: Mz -----------· EI zÒ

Ú

D

( E i y F – E i y z c + E i yzy c )dS º

My º + -----------· EI yÒ

2

Ú

D

( E i z F + E i z y c – E i yzz c ) ds = 0 2

This relation has to be verified when the force applied at C varies in magnitude and direction in the plane of the section. One can deduce fr om there that the relation is valid no matter what the values of Mz and My are. Both the above integrals are then nil. One extracts from this property the coordinates of the torsion center: 1 y c = – ------------· EI yÒ

Ú

1 z c = ------------· EI zÒ

D

D

Ú

E i z F dS

E i y F dS

In summary, the uniform torsion of a cylindrical composite beam made of perfectly bonded isotropic phases can be characterized by a homogenized © 2003 by CRC Press LLC

TX846_Frame_C16 Page 314 Monday, November 18, 2002 12:32 PM

formulation — equivalent to that of a classical homogeneous beam — in the following manner:

• degree of freedom: about x axis: q x • elastic center 0: it is such that

ÚD Ei y dS

• principal axes: they are such that

=

ÚD Ei z dS

ÚD Ei yz dS

= 0

= 0

• equivalent stiffnesses: · EI z Ò =

Â Ei Izi

;

· EI yÒ =

Â Ei Iyi i

i

∂F ∂F 2 2 · GJ Ò = Ú G i Ê y -------- – z -------- + y + z ˆ dS Ë ∂z ¯ ∂y D • torsion center: coordinates in principal axes: 1 y c = – ------------- Ú E i z F dS · EI yÒ D 1 z c = -------------- Ú E i y F dS · EI z Ò D dM • equilibrium relation: ----------x = 0 dx

( M x = constant )

dq • constitutive relation: M x = · GJ Ò ---------x dx d qx ∂ F • shear stresses t xy = G i --------- ÊË -------- – zˆ¯ dx ∂y dq ∂ F t xz = G i ---------x ÊË -------- + yˆ¯ dx ∂z • function F(y, z): it is the solution to the problem: Ï ∂2 F ∂2 F Ô --------- + --------- = 0 in domain D of the section. Ô ∂ y2 ∂ z2 Ì Ô ∂F = zn y – yn z on the external boundary ∂D. Ô ------∂n Ó with internal continuity: Fi = Fj

¸ Ô along internal ∂ Fi ∂ Fj ˝ Ê ˆ Ê ˆ G i --------- – zn y + yn z = G j --------- – zn y + yn z Ô boundaries ij Ë ∂n ¯ Ë ∂n ¯ ˛ and the uniqueness condition: Ú E i F dS = 0 D

• strain energy density 2

1 Mx dW --------- = --- -----------2 · GJ Ò dx

© 2003 by CRC Press LLC

(16.4)

TX846_Frame_C16 Page 315 Monday, November 18, 2002 12:32 PM

Remarks: A finite element computer program for the classical homogeneous beams 3 is usable with the condition that the equivalent rigidity in torsion ·GJ Ò can be available. This requires the numerical calculation of the function 4 F. The latter is the solution of a Laplace type problem, which can be noted in relations 16.4. An equivalent functional is possible to define, which leads to the calculation of F by the finite element method, by means of discretization of the cross section. Flexion-torsion coupling: When, due to the loads applied on the beam, there exists simultaneously bending and torsion of the beam, the approach of the previous chapter is always valid. Keeping the definitions in Sections 15.1.1 and 15.2 for the degrees of freedom u, v, qx, qy, one arrives at the following displacement field:

Ï dq Ô u x = u – y q z + z q y + j ---------x + h x dx Ô Ìu = v – zq + h x y Ô y Ôu = w + yq + h x z Ó z

The torsion being uniform, the equilibrium relations in 15.19 become more restrictive and can be reduced to:

dT dT dN ---------x = 0; ---------y = 0; ---------z = 0 dx dx dx dM dM dM ----------x = 0; ----------z + T y = 0; ----------y – T z = 0 dx dx dx

3

4

(16.5)

Except if the considered application requires the calculation of the shear stresses in a cross section. One has to solve an analogous problem for the homogeneous beams, when one desires to calculate the torsional Saint-Venant stiffness: J =

© 2003 by CRC Press LLC

∂F

∂F

– z ------- + y ÚD ÊË y ------∂z ∂y

2

+ z 2ˆ dS . ¯

TX846_Frame_C16 Page 316 Monday, November 18, 2002 12:32 PM

Taking into account six degrees of freedom also leads to six constitutive 5 relations. One finds : du N x = · ESÒ ------dx dq · GS Ò dv T y = ------------- Ê ------ – q z – z c ---------xˆ (*) dx ¯ k y Ë dx dq · GS Ò dw T z = ------------- Ê -------- + q y + y c ---------xˆ (*) dx ¯ k z Ë dx dq M x = · GJ Ò ---------x – z c T y + y c T z dx dq M y = · EI yÒ --------y dx dq M z = · EI zÒ ---------z dx

5

(16.6)

In each of the relations marked with (*), there appears a supplementary coupling term connected to the existence of a third coefficient denoted as kyz. The complete form is then: dq dv k y T y + k yz T z = · GSÒ Ê ------ – q z – z c --------x-ˆ Ë dx dx ¯ dq dw k yz T y + k z T z = · GSÒ Ê -------- + q y + y c --------xˆ Ë dx dx ¯ This secondary coupling has been neglected in the indicated form.

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 317 Monday, November 18, 2002 12:33 PM

17 FLEXURE OF THICK COMPOSITE PLATES The mechanical behavior of a laminated plate as studied in Chapter 12 involves the definition of stress resultants Nx, Ny, Txy and moment resultants Mx, My, Mxy. These resultants are obtained from the membrane stresses sx, sy, txy. The other stress components, sz, txz, tyz have not been taken into account until now. In this chapter we note how these stresses exist and have influence on the mechanical behavior of the laminate. We will also examine the configurations of plates for which the influence of these stresses are significant (for example, plates with relatively high thicknesses, justifying the title given for this chapter). This study is based on the previous definition of the displacement parameters based on integral displacement forms, and constitutes an approach analogous (and also original) to that used in Chapter 15 for the description of the bending of composite beams.

17.1 PRELIMINARY REMARKS 17.1.1 Transverse Normal Stress sz The plate is situated as in Chapter 12 from which the name of transverse normal stress sz. Such stress appears due to the application of a transverse load (concentrated or distributed) which will cause bending of the plate. A very local concentration of load in a very small zone cannot be examined with the theory of plates, which is not able to provide spatial distribution of the stresses in the neighborhood of the point of load application. This phenomenon is complex even in three-dimensional numerical modeling. Therefore, what will be presented will not be valid in the immediate surroundings of a very local transverse load (for example, an insert). A distributed load gives rise to the stresses sz with small amplitude as compared with the stresses sx and sy. This is the reason why sz is often neglected.

17.1.2 Transverse Shear Stresses txz and tyz Due to the assumption of perfect bonding between the plies, the stress vector remains continuous across an interfacial element with normal vector n = z , between two consecutive plies of the laminate. Then txz and tyz remain continuous at the

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 318 Monday, November 18, 2002 12:33 PM

interfaces between plies (see Section 15.1.2). In addition, the upper face and lower face of the laminate are assumed to be free of tangential forces. The thickness of the laminate is denoted as h. One then has:

txz = tyz = 0 for z = ±h/2 Assume stress and moment resultants to be constant in a given zone of the laminate: Nx, Ny, Txy, My, Mx, Mxy constants "(x, y) Then, by inversion of Equation 12.20, for example, one notes that the following global strain 2

2

2

2

2

eox, eoy, goxy, ∂ w0 /∂x , ∂ w0 /∂y , 2∂ w0 /∂ x∂ y are constant in the zone under consideration. The local strains of Equation 12.12 then depend only on the coordinate z of the laminate. This is the same for the membrane stresses sx, sy, txy. With the above consideration, local equilibrium can be written as (in the absence of body forces):

∂s x ∂t xy ∂t xz --------- + ---------- + ---------- = 0 ∂x ∂y ∂z ∂t xy ∂s y ∂t yz --------- + -------- + ---------- = 0 ∂x ∂y ∂z

(17.1)

The transverse shear stresses then appear to be constant across the thickness of a ply. Being continuous at the interface and nil at the location z = ± h/2, they are nil in all the thickness of the laminate. From this, these stresses do not play an important role in all cases: they do not always exist, their existence being related to variable stresses and moment resultants. When they exist and depending on the composition of the laminate, they can have influence on the deformation in bending, and on the interlaminar adhesion (between layers). We will assume that these stresses exist, associated with the hypotheses of the following paragraph.

17.1.3 Hypotheses The plate has midplane symmetry. The plies are orthotropic, the orthotropic axes coinciding with the x, y, z 1 axes of the laminate. The stress sz is negligible.

1

For example, this is the case for a laminate made of layers of balanced fabric at 0∞, 90∞, or 45∞, –45∞, for unidirectional layers at 0∞ and 90∞, or for mats. Instead of this hypothesis, one can also adopt the less restrictive hypothesis of a balanced laminate. In this case the following calculations are much more involved, without appreciable gain on the enlargement of the field of applications examined in Section 17.6.3.

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 319 Monday, November 18, 2002 12:33 PM

Remarks: For each ply having orthotropic axes x, y, z, the constitutive Equation 13.3 can be written as, taking into account the simplification sz # 0: Ï ¸ Ï ¸ n 1 --- – ----yx- 0 0 0 Ô sx Ô Ô ex Ô Ex Ey Ô Ô Ô Ô n xy 1 Ô ey Ô Ô sy Ô --0 0 0 – ---Ey Ô Ô Ô Ô Ex Ô Ô Ô Ô 1 Ì g xy ˝ = 0 ------ 0 0 G 0 Ì t xy ˝ xy Ô Ô Ô Ô Ôg Ô Ô Ô 1 - 0 Ô t xz Ô 0 0 0 ----Ô xz Ô G xz Ô Ô Ô Ô 1 Ôt Ô Ô g yz Ô 0 0 0 0 ----yz G yz Ó Ó ˛ ˛ or under inverse form Ï sx ¸ E 11 Ô Ô Ô sy Ô E 21 Ô Ô t = Ì xy ˝ 0 Ô Ô 0 Ô t xz Ô Ôt Ô 0 Ó yz ˛

E 12 E 22 0 0 0

0 0 E 33 = G xy 0 0

0 0 0 0

0 0 0 E 44 = G xz 0

E 55 = G yz

Ï ex ¸ Ô Ô Ô ey Ô Ô Ô Ì g xy ˝ Ô Ô Ô g xz Ô Ôg Ô Ó yz ˛

(17.2)

where: Ex n yx E x Ey - ; E 12 = ----------------------- ; E 22 = ----------------------E 11 = ----------------------1 – n xy n yx 1 – n xy n yx 1 – n xy n yx The transverse shear is at the origin of distortions as illustrated in Figure 17.1 for the shear stress tyz. As a consequence, the displacements due to flexion discussed in Section 12.2.1 can be adapted as shown in Figure 17.2.

Figure 17.1 Distortion of Section due to Transverse Shear tyz

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 320 Monday, November 18, 2002 12:33 PM

Figure 17.2 Flexural Displacements

In this figure, (a) represents a section before and after bending and (b) shows the evolution of the section as a rigid displacement (parameters v0, w0, and qx) to which are associated increments hy and hz in the plane y,z. Note: Due to the existence of midplane symmetry, the antisymmetric manner with respect to z, these increments are small, but they cannot be neglected a priori. (At this stage, we do not have a definition for the equivalent rotation, noted as qx in b). This justifies the interest in the definition of the displacement field relating these increments. A supplementary interest rests in the possibility, during the study, to look after the necessary approximations more closely to lead to a useful 2 technical formulation.

17.2 DISPLACEMENT FIELD The elastic displacement at each point of the laminate has the components u(x, y, z), v (x, y, z) and w (x, y, z). With simplified description of Paragraph 12.2.1, one sees in Figure 17.2 (b), average translations denoted as v0 and w0, and a rotation of the section denoted as qx, to which one superimposes the supplementary displacements hy and hz. We will define these averages in integral forms as follows: Translation along x direction: By definition, this is u0 such that: 1 u 0 = --h

Ú

h/2

– h/2

u ( x, y, z ) dz

Rotation about the y axis: By definition, this is qy(x,y) such that : 3

qy =

2 3

Ú

h/2

– h/2

E 11 E 12 ˆ Ê -------- + --------- u ( x, y, z ) ¥ z dz Ë EI 11 EI 12¯

Approximations that do not appear neatly in the specialized literature. Such a definition of the “average rotation” q y will be fundamental in the following to ensure the energetic coherence of the formulation for the transverse shears (see Section 17.6.6).

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 321 Monday, November 18, 2002 12:33 PM

1 4 -. where one has reused the notations of Section 12.1.6 for the terms ---EI ij The longitudinal displacement u(x, y, z) then takes the form:

u ( x, y, z ) = u 0 ( x, y ) + z q y ( x, y ) + h x ( x, y, z ) with: h/2

E 11 E 12 ˆ Ê -------- + --------- h x z dz = 0 Ë – h/2 EI 11 EI 12¯

Ú

In effect, one can obtain starting from this expression:

Ú

h/2

– h/2

u dz = h ¥ u o + q y

Ú

h/2

– h/2

z dz +

Ú

h/2

– h/2

h x dz 5

the integrals disappearing due to antisymmetry in z : h/2

E 11 E 12 ˆ Ê -------- + --------- uz dz = u o Ë – h/2 EI 11 EI 12¯

Ú

… + qy +

h/2

E 11 E 12 ˆ Ê -------- + --------- z dzº Ë – h/2 EI 11 EI 12¯

Ú

h/2

E 11 E 12 ˆ Ê -------- + --------- h x z dz Ë – h/2 EI 11 EI 12¯

Ú

In the second member, the first integral disappears due to midplane symmetry. In addition, taking into account the definition of qy written above, the second integral is also nil. Translation along the y direction: This is v0(x,y) such that: 1 v 0 = --h

Ú

h/2

– h/2

v ( x, y, z ) dz

Rotation about the x axis: This is qx such that:

qx = –

Ú

h/2

– h/2

E 22 E 12 ˆ Ê -------- + --------- v ( x, y, z ) ¥ z dz Ë EI 22 EI 12¯

The longitudinal displacement v(x,y,z) then takes the form: v ( x, y ) = v 0 ( x, y ) – z q x ( x, y ) + h y ( x, y, z ) 4

Recall that (Section 12.1.6): th

1 ----- = [ C ] –1 , EI 5

n ply

where

Â

C ij =

st

3

3

k z k – z k-1ˆ E ij Ê ------------------Ë 3 ¯

k=I ply

The coefficient of qy is 1 because one can note that:

- + ---------ˆ z dz Ú–h/2 ÊË -------EI 11 EI 12¯ h/2

E 11

© 2003 by CRC Press LLC

E 12

2

2 C 11 C 12 C 12 C 11 C 22 - + --------- = ---------------------------= -------- – ---------------------------- = 1 2 2 EI 11 EI 12 C 11 C 22 – C 12 C 11 C 22 – C 12

TX846_Frame_C17 Page 322 Monday, November 18, 2002 12:33 PM

with:

Ú

( h/2 )

– h/2

E 22 E 12 ˆ Ê -------- + --------- h z dz = 0 Ë EI 22 EI 12¯ y

Translation along the z direction: This is w0(x,y) such that: 1 w 0 ( x, y ) = --h

Ú

( h/2 )

– h/2

w ( x, y, z ) dz

The vertical displacement takes the form: w ( x, y, z ) = w 0 ( x, y ) + h z ( x, y, z ) In summary, one obtains for the elastic displacement field: u = u 0 + z q y + h x ( x, y, z ) v = v 0 – z q x + h y ( x, y, z ) w = w0

(17.3)

+ h z ( x, y, z )

h x , h y , h z antisymmetric in z. h/2

E 11 E 12 ˆ Ê -------- + --------- h x z dz = Ë – h/2 EI 11 EI 12¯

Ú

(17.4)

h/2

E 22 E 12 ˆ Ê -------- + --------- h y z dz = 0 Ë – h/2 EI 22 EI 12¯

Ú

(17.5)

17.3 STRAINS One deduces from the previous displacements the strains:

∂q ∂h e x = e 0x + z --------y + ---------x ∂x ∂x ∂q ∂h e y = e 0y – z --------x + --------y ∂y ∂y ∂h ∂h ∂q ∂q g xy = g 0xy + z ÊË --------y – --------xˆ¯ + ---------x + --------y ∂y ∂x ∂y ∂x ∂w ∂h ∂h g xz = ---------0 + q y + ---------x + ---------z ∂x ∂z ∂x ∂w ∂h ∂h g yz = ---------0 – q x + --------y + ---------z ∂y ∂z ∂y

17.4 CONSTITUTIVE RELATIONS 17.4.1 Membrane Equations Recall the method that was already used in Section 12.1.1.

© 2003 by CRC Press LLC

(17.6)

TX846_Frame_C17 Page 323 Monday, November 18, 2002 12:33 PM

stress resultant N x = Ú –h/2 s x dx: h/2

Nx =

∂q ∂h E 11 Ê e 0x + z --------y + ---------xˆ dz + Ë ∂x ∂x ¯ – h/2

Ú

h/2

∂ N x = A 11 e 0x + A 12 e 0y + -----∂x

[ 17.2 ] et [ 17.6 ] : 6

from

Ú

h/2

– h/2

∂q ∂h E 12 Ê e 0y – z --------x + --------yˆ dz Ë ∂y ∂y ¯

∂ E 11 h x dz + -----∂y – h/2

Ú

h/2

Ú

h/2

– h/2

E 12 h y dz

stress resultant N y = Ú –h/2 s y dz: h/2

N y = A 21 e 0x + A 22 e 0y stress resultant T xy = Ú –h/2 t xy dz: h/2

T xy =

∂h ∂h ∂q ∂q E 33 Ê g oxy + z Ê --------y – --------xˆ + ---------x + --------yˆ dz Ë Ë ¯ ∂y ∂x ¯ ∂y ∂x – h/2

Ú

h/2

T xy = A 33 g oxy In summary, one finds again the relations already established in Chapter 12 (Equations 12.5) as: Ï Nx ¸ A 11 A 12 0 Ô Ô Ì N y ˝ = A 21 A 22 0 Ô Ô 0 0 A 33 Ó T xy ˛

Ï e ox ¸ Ô Ô Ì e oy ˝ Ô Ô Ó g oxy ˛

or, in inverse form, by using the notations in Equation 12.9: Ï e ox ¸ Ï Nx ¸ – n yx /E y 0 1/E x Ô Ô 1Ô Ô 1 –1 --e N ¥ = h [ A ] = Ì oy ˝ 1/E y 0 h ÌÔ y Ô˝ h – n xy /E x Ô Ô g T Ó oxy ˛ Ó xy ˛ 0 0 1/G xy

Ï Nx ¸ Ô Ô Ì Ny ˝ Ô Ô Ó T xy ˛

(17.7)

17.4.2 Bending Behavior One has again the already known moment resultants (see Section 12.2.1). Moment resultant M y = Ú –h/2 s x z dz: with [17.2] and [17.5]: h/2

My =

∂h 2 ∂q E 11 Ê z e ox + z --------y + z ---------xˆ dz … Ë ∂x ∂x ¯ – h/2

Ú

h/2

º+

∂h 2 ∂q E 12 Ê z e oy – z --------x + z --------yˆ dz Ë ∂y ∂y ¯ – h/2

Ú

h/2

∂q ∂q ∂ M y = C 11 --------y + C 12 ¥ – --------x + -----∂x ∂y ∂x 6

∂ E 11 h x z dz + -----y ∂ – h/2

Ú

h/2

Ú

h/2

– h/2

E 12 h y z dz

The simplifications are due to the antisymmetry of the integrated functions (midplane symmetry).

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 324 Monday, November 18, 2002 12:33 PM

In the last two terms there appear the nonzero integrals of even functions. If one neglects the contribution of the rates of variation along the x and y direction, respectively, of these terms, the previous equation 7 is reduced to

∂q ∂q M y = C 11 --------y + C 12 ¥ – --------x ∂x ∂y Moment resultant M x = – –Mx =

Ú

h/2

– h/2

s y z dz :

∂h 2 ∂q E 12 Ê z e ox + z --------y + z ---------xˆ dzº Ë ∂x ∂x ¯ – h/2 h/2

Ú

Ú

º+

h/2

– h/2

∂h 2 ∂q E 22 Ê z e oy – z --------x + z --------yˆ dz Ë ∂y ∂y ¯

which is reduced to:

∂q ∂q ∂ – M x = C 12 --------y + C 22 ¥ – --------x + -----∂x ∂y ∂x

∂ E 12 h x z dz + -----∂y – h/2

Ú

h/2

Ú

h/2

– h/2

E 22 h y z dz 7

and in neglecting the contribution of the last two terms :

∂q ∂q – M x = C 12 --------y + C 22 ¥ – --------x ∂x ∂y Moment resultant M xy = – – M xy =

Ú

h/2

– h/2

t xy z dz

∂h ∂h ∂q 2 ∂q E 33 Ê z g oxy + z Ê --------y – --------xˆ + z ---------x + z --------yˆ dz Ë Ë ¯ ∂ y ∂x ¯ ∂ y ∂ x – h/2

Ú

h/2

which is reduced to:

∂q ∂q ∂ – M xy = C 33 Ê --------y – --------xˆ + -----Ë ∂y ∂x ¯ ∂y

∂ E 33 h x z dz + -----∂x – h/2

Ú

h/2

Ú

h/2

– h/2

E 33 h y z dz

and in neglecting the contribution of the variations of the differences hx 7 and hy :

∂q ∂q – M xy = C 33 Ê --------y – --------xˆ Ë ∂y ∂x ¯ 7

The existence of such approximation does not appear if one neglects a priori the increments hx, hy, hz in Equation 17.3.

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 325 Monday, November 18, 2002 12:33 PM

In summary, one finds again a form analogous to Equation 12.16 (with C13 = C23 = 0 due to the orientation of the plies (see Hypotheses in Section 17.1.3): ∂q

Ï --------y ¸ ∂x Ô Ô Ô Ô ∂q x – -------Ì ˝ ∂y Ô Ô ∂q Ô Ô Ê ∂q -y – --------xˆ Ó Ë ------∂y ∂x ¯ ˛

C 11 C 12 0 Ï My ¸ Ô Ô Ô Ô Ì – M x ˝ = C 21 C 22 0 Ô Ô Ô –M Ô 0 0 C 33 Ó xy ˛

(17.8)

Or in the inverse form, by reusing the notations of Section 12.1.6. ∂q

Ï --------y ¸ ∂x Ô Ô Ô ∂q x Ô Ì – -------˝ = ∂y Ô Ô ∂q Ô Ô Ê ∂q -y – --------xˆ Ó Ë ------∂y ∂x ¯ ˛

1 --------EI 11

1 --------EI 12

1 --------EI 21

1 --------EI 22

0

0

0 Ï My ¸ Ô Ô Ô Ô 0 Ì –Mx ˝ Ô Ô 1 -------- Ô – M xy Ô C Ó ˛

(17.9)

33

17.4.3 Transverse Shear Equation We define here new stress resultants starting from the transverse shear stresses, which are denoted as transverse shear stress resultants: Shear stress resultant Q x = Ú –h/2 t xz dz Using Equations 17.2 and 17.6: h/2

Qx =

∂w ∂h ∂h G xz Ê ---------0 + q y + ---------x + ---------zˆ dz Ë ∂x ∂z ∂x ¯ – h/2 h/2

Ú

in setting · hG xzÒ =

Ú

h/2

G xz dz

– h/2

yields

∂w Q x = · hG xzÒ Ê ---------0 + q yˆ + Ë ∂x ¯

dh G xz ---------x dz ∂z – h/2

Ú

h/2

(17.10)

where one can note the presence of the integral of an even function: Shear stress resultant Q y = Ú –h/2 t yz dz h/2

Qy =

© 2003 by CRC Press LLC

∂w ∂h ∂h G yz Ê ---------0 – q x + --------y + ---------zˆ dz Ë ∂y ∂z ∂y ¯ – h/2

Ú

h/2

TX846_Frame_C17 Page 326 Monday, November 18, 2002 12:33 PM

in setting · hG yzÒ =

Ú

h/2

G yz dz

– h/2

yields

∂h G yz --------y dz ∂z – h/2

∂w Q y = · hG yzÒ Ê ---------0 – q xˆ + Ë ∂y ¯

Ú

h/2

(17.11)

17.5 EQUILIBRIUM EQUATIONS These are the same for the plates in general, no matter what are their compositions and are, therefore, classical. One recalls here only the equilibrium equations for bending.

17.5.1 Transverse Equilibrium ∂t

∂t

∂s

zx zy - + --------- + ---------z + f z = 0 local equilibrium relation --------∂x ∂y ∂z In integrating across the thickness, one reveals the transverse shear stresses Qx and Qy:

∂ Qx ∂ Qy --------- + --------- + [ s z ] h/2 – h/2 + ∂x ∂y

Ú

h/2

– h/2

f z dz = 0

Then denoted by pz, the transverse stress density:

∂ Qx ∂ Qy --------- + --------- + p z = 0 ∂x ∂y

17.5.2 Equilibrium in Bending ∂s

∂t

∂t

xy xz -x + --------- + --------- + fx = 0 local equilibrium relation -------∂x ∂y ∂z After multiplication with z, the integration over the thickness leads to

∂ M ∂ M xy ----------y – -----------+ ∂x ∂y

Ú

h/2

– h/2

∂ ------ ( z t ) – t xz dz + ∂ z xz

∂ M ∂ M xy h/2 ----------y – ----------- – Q x + [ z t xz ] –h/2 + ∂x ∂y

Ú

h/2

– h/2

Ú

h/2

– h/2

z f x dz = 0

zf x dz = 0

In neglecting the moment density:

∂ M ∂ M xy ----------y – ----------- – Qx = 0 ∂x ∂y ∂t

∂s

(17.12)

∂t

yx yz - + ---------y + --------- + fy = 0 local equilibrium relation --------∂x ∂y ∂z An analogous calculation leads to

∂ M xy ∂ M x ------------ + ---------- + Q y = 0 ∂x ∂y

© 2003 by CRC Press LLC

(17.13)

TX846_Frame_C17 Page 327 Monday, November 18, 2002 12:33 PM

17.6 TECHNICAL FORMULATION FOR BENDING One can note in the preceding that midplane symmetry always leads to the decoupling of the membrane behavior from the bending behavior. As a consequence, in what follows, one will consider uniquely the stresses due to bending (one will make Nx = Ny = Txy = 0). In addition to the hypotheses in Section 17.1.3, one will neglect, for the calculation of the stresses, the variations of increments {hx, hy, hz} as 8 functions of x and y.

17.6.1 Plane Stresses Due to Bending One can write successively for a ply number k: k

k

s x = E 11 e x + E 12 e y Then with [17.6]:

∂q ∂h ∂q ∂h k k s x = E 11 ÊË e ox + z --------y + ---------xˆ¯ + E 12 ÊË e oy – z --------x + --------yˆ¯ ∂x ∂x ∂y ∂y and with [17.7] and [17.9]: N x n yx M M k s x = E 11 -------- – --------N y + z Ê --------y- – --------x-ˆ º Ë hE x hE y EI 11 EI 12¯

n xy Ny M M k º + E 12 - N x + -------– -------+ z Ê --------y- – --------x-ˆ Ë hE x hE y EI 12 EI 22¯ k

k

E 11 E 12 ˆ - + --------- M y + z s x = z ÊË -------EI 11 EI 12¯ k

k

k

E 11 E 12 ˆ Ê -------- + --------- ¥ – M x Ë EI 12 EI 22¯

(17.14)

k

s y = E 12 e x + E 22 e y An analogous calculation leads to k

k

k

k

E 12 E 22 ˆ E 12 E 22 ˆ - + --------- M y + z Ê -------- + --------- ¥ – M x s y = z ÊË -------¯ Ë EI 11 EI 12 EI 12 EI 22¯ k

(17.15)

t xy = E 33 g xy = G xy g xy Then with Equation 17.6: k

∂h ∂h ∂q ∂q k t xy = G xy ÊË g oxy + z ÊË --------y – --------xˆ¯ + ---------x + --------yˆ¯ ∂y ∂x ∂y ∂x 8

This simplification constitutes here the extension to plates of the generalized Navier-Bernoulli principle for beams (see Section 15.1.5).

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 328 Monday, November 18, 2002 12:33 PM

and with Equations 17.7 and 17.9 and Txy = 0: k

G xy -M t xy = – z -------C 33 xy

(17.16)

17.6.2 Transverse Shear Stresses in Bending

k

t xz = E 44 g xz = G xz g xz from [ 17.2 ] k

and with Equation 17.6 and neglecting the variation ∂hz /∂ x: k ∂w k ∂h t xz = G xz ÊË ---------0 + q yˆ¯ + G xz ---------x ∂x ∂z

k

(17.17)

t yz = E 55 g yz = G yz g yz k

which leads in an analogous manner to k ∂w k ∂h t yz = G yz ÊË ---------0 – q xˆ¯ + G yz --------y ∂z ∂y

(17.18)

Knowledge of the transverse shears, then, requires the previous calculation of the warping increments hx and hy.

17.6.3 Characterization of the Bending, Warping Increments hx and hy Warping hx (x, y, z): Starting from the first equation of local equilibrium:

∂t xz ∂s ∂t xy ---------- = – ---------x – --------∂z ∂x ∂y Then with Equations 17.14, 17.16, and 17.17: G xy ∂ M xy E 11 E 12 ˆ ∂ M x E 11 E 12 ˆ ∂ M y k ∂ hx - + --------- ---------- + z Ê -------- + --------- ---------- + z ------- -----------= – z Ê -------G xz ----------2 Ë ¯ Ë ¯ C 33 ∂ y ∂z EI 11 EI 12 ∂ x EI 12 EI 22 ∂ x 2

k

k

k

k

k

Taking into account the equilibrium Equation 17.12, one can rewrite E 11 E 12 ˆ E 11 E 12 ˆ ∂ M x º k ∂ hx - + --------- Q x + z Ê -------- + --------- ---------= – z Ê -------G xz ----------2 Ë ¯ Ë ∂z EI 11 EI 12 EI 12 EI 22¯ ∂ x 2

k

k

k

Ê G xy E k11 E k12 ˆ ∂ M xy º + z Á -------- – --------- – ---------˜ -----------Ë C 33 EI 11 EI 12¯ ∂ y

k

k

(17.19)

Warping hy (x, y, z): In an analogous manner, starting from the second equation of the local equilibrium:

∂t yz ∂s ∂t yx --------- = – --------y – --------∂z ∂y ∂x

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 329 Monday, November 18, 2002 12:33 PM

Then with Equations 17.15, 17.16, and 17.18: 2 Ê E k12 E k22 ˆ ∂ M y Ê E k12 E k22 ˆ ∂ M x k ∂ hy ----------------------= – + z z + G yz ---------Á ˜ Á --------- + ---------˜ ---------- º 2 ∂z Ë EI 11 EI 12¯ ∂ y Ë EI 12 EI 22¯ ∂ y xy ∂ M xy º + zG ------- -----------C 33 ∂ x k

Taking into account the equilibrium Equation 17.13, one can rewrite E 12 E 22 ˆ ∂ M y E 12 E 22 ˆ º k ∂ hx - = – z Ê -------- + --------- ---------- – z Ê -------- + --------- Q y G yz ---------2 Ë ¯ Ë ∂z EI 11 EI 12 ∂ y EI 12 EI 22¯ 2

k

k

k

k

Ê G xy E k12 E k22 ˆ ∂ M xy - – --------- – ---------˜ -----------º + z Á ------Ë C 33 EI 12 EI 22¯ ∂ x k

(17.20)

17.6.3.1 Particular Cases Equations 17.19 and 17.20 simplify in the following particular cases: Homogeneous orthotropic plate: Then from relations 17.2, 17.8, and 17.9: k

k

E 11 = E 11 ; E 12 = E 12 ; E

k 22

= E 22

C 22 12 E 22 1 - ¥ -----3- ; --------- = ----------------------------- = -----------------------------2 2 C 11 C 22 – C 12 EI 11 E 11 E 22 – E 12 h E 11 1 12 --------- = ----------------------------- ¥ -----32 EI 22 E 11 E 22 – E 12 h C 12 – E 12 1 12 --------- = – ---------------------------- = ---------------------------- ¥ -----3- ; 2 2 C 11 C 22 – C 12 EI 12 E 11 E 22 – E 12 h

1 1 12 ------- = -------- ¥ -----3C 33 G xy h

Then Equation 17.19 and Equation 17.20 reduce to

∂ hx 12 G xz ----------= – z ¥ -----3- ¥ Q x 2 h ∂z 2

∂ h 12 G yz ----------2-y = – z ¥ -----3- ¥ Q y h ∂z 2

(17.21)

Cylindrical bending about x or y axis of a multilayered plate characterized by identical Poisson coefficient in the x,y plane of the plate as: "k: n xy = n xy ; n yx = n yx k

© 2003 by CRC Press LLC

k

TX846_Frame_C17 Page 330 Monday, November 18, 2002 12:33 PM

9

Then for any two plies k and m, one has (see Equations 17.2) : k

k

k

E 12 E 22 E 11 ------- = ------- = ------- = a km m m m E 11 E 12 E 22 then: C ij =

Ú

n

h/2

k ij

– h/2

th

k=I 1

= E ij

Ú

z1

z0

1Ï C ij = E ij Ì Ó

Ú

2

z dz + E ij 2

z1

z0

Ú

st

z2

ply

Ï k Ì E ij Ó

¸ 2 z dz ˝ z k-1 ˛

Ú

zk

z dz º + E ij n

2

z1

z dz + a 12 2

ply

Â

E z dz = 2

Ú

z2

Ú

zn

2

z dz

z n-1

z dz º + a n-1, n 2

z1

3 ¸ 1 ah 2 z dz ˝ = E ij ¥ --------12 z n-1 ˛

Ú

zn

where a is a nondimensional coefficient. One then has 1

C 22 12 EI 22 1 --------- = ---------------------------- = ----------------------------------¥ ---------3 ; 2 1 1 1 2 C 11 C 22 – C 12 a h EI 11 E 11 E 22 – ( E 12 ) 1

12 EI 11 1 ---------- = ----------------------------------¥ ---------3 1 1 1 2 a h EI 22 E 11 E 22 – ( E 12 ) 1

12 EI 12 1 ---------- = ----------------------------------¥ ---------3 1 1 1 2 EI 12 E 11 E 22 – ( E 12 ) a h In [17.19], we have the simplification : k

k

1

k

k

1

- E 11 E 12 + E 12 E 11 12 E 11 E 12 - ¥ ---------3 -------- + --------- = --------------------------------------------1 1 1 2 ah EI 12 EI 22 E 11 E 22 – ( E 12 ) 1

1

1

1

a k1 ( – E 11 E 12 + E 12 E 11 ) 12 - ¥ ---------3 = 0 = -----------------------------------------------------1 1 1 2 ah E 11 E 22 – ( E 12 ) as well as an analogous simplification in Equation 17.20: k

k

E 12 E 22 -------- + --------- = 0 EI 11 EI 12 10

Equations 17.19 and 17.20 simplify as follows : 9 10

Recall the relation nyx Ex = nxy Ey (see Equation 9.4). In the first case in Equation 17.22, Mxy = Qy = 0 and Equation 17.20 disappears. In the second case, Mxy = Qy = 0 and Equation 17.19 disappears.

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 331 Monday, November 18, 2002 12:33 PM

1. cylindrical bending about y axis E 11 E 12 ˆ k ∂ hx - + --------- Q x = – z Ê -------G xz ----------2 Ë ∂z EI 11 EI 12¯ 2. cylindrical bending about x axis 2

k

k

(17.22)

E 22 E 12 ˆ k ∂ h - + --------- Q y G yz ----------2-y = – z Ê -------Ë ∂z EI 22 EI 12¯ 2

k

k

The case of a multilayer plate such that for any two plies k and m one 11 has in the plane of the plate : k

E ij -----m- = a km E ij

"i and j = 1, 2, 3

Then Equations 17.19 and 17.20 reduce to

∂ hx E 11 E 12 ˆ - + --------- Q x G ----------= – z Ê -------2 Ë ∂z EI 11 EI 12¯ 2

k

k

k xz

(17.23)

∂ h E 22 E 12 ˆ - + --------- Q y G ----------2-y = – z Ê -------Ë ∂z EI 22 EI 12¯ 2

k

k

k yz

The preceding particular cases constitute a severe restriction among the variety of practical laminations. Nevertheless we will conserve in the following the simplified forms of Equations 17.21, 17.22, and 17.23 because they well show the direct connection between the warpings hx and hy and the transverse shear forces Qx and Qy, respectively.

17.6.3.2 Consequences Setting hx and hy in the forms: ¸ Qx ¥ g(z ) Ô h x ( x, y, z ) = ----------------· hG xzÒ Ô ˝ Qy - ¥ p ( z ) ÔÔ h y ( x, y, z ) = ---------------· hG yzÒ ˛

(17.24)

The constitutive Equations 17.10 and 17.11 are written as: h/2 ∂w Qx dg Q x = · hG xzÒ Ê ---------0 + q yˆ + ----------------G ------ dz Ë ∂x ¯ · hG xzÒ –h/2 xz dz

Ú

11

E

k

G

k

- = a km . Such a limiting case is rare in practice, because it imposes in particular: ----33m- = -----xy m E 33

© 2003 by CRC Press LLC

G xy

TX846_Frame_C17 Page 332 Monday, November 18, 2002 12:33 PM

then by setting : 1 k x = Ê 1 – ----------------Ë · hG xzÒ

h/2

dg G xz ------ dzˆ d z ¯ – h/2

Ú

· hG xzÒ Ê ∂ w 0 --------- + q yˆ Q x = ----------------¯ kx Ë ∂ x Qy ∂w Q y = · hG yzÒ Ê ---------0 – q xˆ + ---------------Ë ∂y ¯ · hG yzÒ then by setting :

Ú

h/2

– h/2

1 k y = Ê 1 – ----------------Ë · hG yzÒ

Ú

(17.25)

dp G yz ------ dz dz

h/2

– h/2

dp G yz ------ dzˆ dz ¯

· hG yzÒ Ê ∂ w 0 - --------- – q xˆ Q y = ---------------¯ ky Ë ∂ y

(17.26)

There appear two transverse shear coefficients kx and ky which require the knowledge of the functions g(z) and p(z) for their calculations.

17.6.4 Warping Functions Boundary conditions: We have assumed that the upper and lower faces of the plate were free of any shear. Then the transverse shear in Equations 17.17 and 17.18 leads to Q x dg ∂ w0 ˆ + ----------------------- = 0 for z = ±h /2 Ê --------Ë ∂ y- + qy¯ · hGxzÒ dz

then with Equation 17.25: dg k x + ------ = 0 dz

for

z = ±h /2

Q y dp ∂ w0 ˆ – ----------------- ------ = 0 for z = ±h /2 Ê --------Ë ∂ y- – qy¯ · hGyzÒ dz

then with [17.26]: dp k y + ------ = 0 dz

for

z = ±h /2

Continuity at the interfaces: The continuity of the transverse shear at the interfaces between layers results from the assumed perfect bonding between two plies (see Paragraph 15.1.2). One then has at the interface between two consecutive plies k and k + 1:

t xz = t xz ; t yz = t yz k

© 2003 by CRC Press LLC

k+1

k

k+1

TX846_Frame_C17 Page 333 Monday, November 18, 2002 12:33 PM

then with Equations 17.17, 17.18 and Equations 17.25, 17.26: dg dg k+1ˆ k k+1 G xz Ê k x + --------kˆ = G xz Ê k x + -----------Ë ¯ Ë dz dz ¯ dp dp k+1ˆ k k+1 G yz Ê k y + --------kˆ = G yz Ê k y + -----------Ë ¯ Ë dz dz ¯ Formulation of the warping functions: Let us substitute to g(z) and p(z) the functions g0(z) and p0(z) such that: g0 ( z ) = g ( z ) + z ¥ k x ; p0 ( z ) = p ( z ) + z ¥ k y g0(z) and p0(z) are called the warping functions. Then the boundary conditions and the interface conditions simplify, and Equations 17.23 allow one to formulate the problems that permit a simple calculation of warping functions g0(z) and p0(z). One obtains · hG xzÒ Ê E 11 E 12 ˆ d g0 Ï ------------------ + --------k Ô dz 2 = – z ¥ ----------------G xz Ë EI 11 EI 12¯ Ô Ô dg Ì --------0 = 0 for z = ±h /2 Ô dz Ô k+1 dg 0k+1 0k Ô G k dg - for z = z k = G xz -------------Ó xz ---------dz dz

(17.27)

p0 · hG yzÒ Ê E 22 E 12 ˆ Ïd - --------- + --------= – z ¥ ---------------2 k Ô ---------G yz Ë EI 22 EI 12¯ Ô dz Ô dp Ì --------0 = 0 for z = ±h /2 Ô dz Ô dp 0k k+1 dp 0k+1 Ô G k ---------- for z = z k Ó yz dz- = G yz -------------dz

(17.28)

2

k

2

k

k

k

The antisymmetric functions g0 and p0 are then defined in a unique manner.

17.6.5 Consequences Form of the transverse shear stresses: Equations 17.17 and 17.18 then take the simple forms: k

G xz dg 0 --------; t xz = Q x ¥ ----------------· hG xzÒ dz

© 2003 by CRC Press LLC

k

G yz dp 0 - -------t yz = Q y ¥ ---------------· hG yzÒ dz

(17.29)

TX846_Frame_C17 Page 334 Monday, November 18, 2002 12:33 PM

Transverse shear coefficients: One obtains these coefficients from the Equation 17.5: h/2 E 11 E 12 ˆ Ú –h/2 Ê --------+ --------h z dz = 0 Ë EI11 EI12¯ x

here is : Qx E 11 E 12 ˆ Ê -------- + --------- ¥ ----------------( g 0 – k xz ) z dz = 0 Ë ¯ · hG – h/2 EI 11 xzÒ EI 12 h/2

Ú

noting that : 2

C 11 C 12 – C 12 C 11 C 12 E 11 E 12 ˆ 2 Ê -------- + --------- z dz = -------- + --------- = ---------------------------- = 1. 2 Ë – h/2 EI 11 C 11 C 12 – C 12 EI 12¯ EI 11 EI 12

Ú

h/2

One obtains : kx =

h/2

E 11 E 12 ˆ Ê -------- + --------- g 0 z dz Ë – h/2 EI EI ¯

Ú

11

(17.30)

12

E 22 E 12 - + -------- ) h y z dz = 0 Ú –h/2 ( -------h/2

EI 22

EI 12

here is : Qy E ˆ Ê -E--22 - ( p – k yz ) z dz = 0 -- + ---12 -- ¥ ---------------Ë ¯ · hG yzÒ 0 – h/2 EI 22 EI 12

Ú

h/2

leading to: ky =

h/2

E 22 E 12 ˆ Ê -------- + --------- p 0 z dz Ë – h/2 EI 22 EI 12¯

Ú

(17.31)

In summary, in the absence of body forces (inertia forces, example), the bending behavior uncoupled from the membrane behavior of a thick laminated plate can be simplified in a few particular cases noted below. The characteristic relations are summarized in the following table.

Bending Behavior (no in-plane stress resultants) or or

homogeneous orthotropic plate/orthotropic axes : x, y, z Laminated plate/midplane symmetry/orthotropic axes of plies: x,y,z/same Poisson ratios vxy and vyx for all plies/cylindrical bending about x or y axis. Laminated plate/midplane symmetry/orthotropic axes of plies: x,y,z/elastic constants are proportional from one ply to another Equilibrium relation: ∂Q ∂Q ∂ M xy ∂ M x ∂ M ∂ M xy ----------x + ----------y + p z = 0; ----------y – ----------- + ---------- + Q y = 0 - – Q x = 0; ----------∂x ∂y ∂x ∂y ∂x ∂y

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 335 Monday, November 18, 2002 12:33 PM

Constitutive relations: Ï My ¸ C 11 C 12 0 0 0 Ô Ô Ô Ô Ô Ô Ô –Mx Ô C 21 C 22 0 0 0 Ô Ô Ô Ô Ì – M xy ˝ = 0 0 C 33 0 0 Ô Ô Ô Ô · hG xzÒ Ô Qx Ô 0 0 0 0 -----------------kx Ô Ô Ô Ô · hG yzÒ Ô Q Ô -----------------0 0 0 0 y ky Ó ˛

∂q

Ï --------y ¸ Ô ∂x Ô Ô ∂q x Ô Ô – -------Ô ∂y Ô Ô Ô ∂q y ∂q x Ô – -------- ˝ Ì -------Ô ∂y ∂x Ô Ô ∂ w0 Ô - + qy Ô Ô --------∂x Ô Ô Ô ∂ w0 Ô --------– q x ˛ Ó ∂y

with [C]

–1

1 = ----EI

Stresses stresses within the ply :

sx: cf. [17.14];

sy: cf. [17.15];

txy: cf. [17.16] (17.32)

transverse shear stresses k

k

G xz dg 0 - --------- ; t xz = Q x ----------------· hG xzÒ dz

G yz dh 0 - --------t yz = Q y ----------------· hG yzÒ dz

Warping functions g0 (z) is the solution of the problem: Ï 2 k k g0 · hG xzÒ Ê E 11 E 12 ˆ Ôd - Á --------- + ---------˜ k Ô ----------2- = – z ----------------G xz Ë EI 11 EI 12¯ Ô dz Ô dg 0 Ì -------Ô dz- = 0 for z = ± h/2 Ô Ô k dg 0k dg 0k+1 - = G k+1 for z = z k Ô G xz ---------xz ---------------dz dz Ó

p0 (z) is the solution of the problem:

Ï 2 k k p0 · hG yzÒ Ê E 22 E 12 ˆ Ôd -----------------------------------------˜ = – z + Á k 2 Ô G yz Ë EI 22 EI 12¯ Ô dz Ô dp 0 Ì -------Ô dz- = 0 for z = ± h/2 Ô Ô k dp 0k dp 0k+1 - = G k+1 for z = z k Ô G yz ----------yz ---------------dz dz Ó

Transverse shear coefficients kx and ky: They are given by the formula:

kx =

h/2

E 11 E 12 ˆ Ê -------- + --------- g 0 z dz; Ë – h/2 EI 11 EI 12¯

Ú

© 2003 by CRC Press LLC

ky =

h/2

E 22 E 12 ˆ Ê -------- + --------- p 0 z dz Ë – h/2 EI 22 EI 12¯

Ú

TX846_Frame_C17 Page 336 Monday, November 18, 2002 12:33 PM

17.6.6 Interpretation in Terms of Energy We will limit ourselves to the surface energy density due to transverse shear stresses as: 1 W t = --2

h/2

1 ( t xz g xz + t yz g yz ) dz = --2 – h/2

Ú

t xz t yz ˆ Ê ------- + -------- dz Ë G G yz¯ – h/2 xz

Ú

2

h/2

2

Substituting Equation 17.29, one obtains 1 W t = --2

G xz Ê dg 0ˆ 2 1 2 -2 -------- dz + --Q x ------------------Ë ¯ d z 2 – h/2 · hG xzÒ

Ú

h/2

G yz Ê dp 0ˆ 2 2 -------- dz Q y ------------------2 – h/2 · hG yzÒ Ë dz ¯

Ú

h/2

The first integral can be rewritten as: 2

1 Qx --- --------------------2 2 · hG xzÒ

2 dg d d g0 G xz ------ Ê g 0 --------0ˆ – g 0 ---------dz 2 dz Ë dz ¯ – h/2 dz

Ú

h/2

or, taking into account Equation 17.27: dg 1 Qx Ï --- --------------------2 Ì G xz g 0 --------0 dz 2 · hG xzÒ Ó 2

h/2 – h/2

+ · hG xzÒ

¸ E 11 E 12 ˆ Ê -------- + --------- g 0 z dz ˝ Ë ¯ – h/2 EI 11 EI 12 ˛

Ú

h/2

where one recognizes Equation 17.30 of the transverse shear coefficient kx, The first integral is reduced to 2

Qx 1 --- k x ----------------2 · hG xzÒ Following a similar approach for the second integral and taking into account Equations 17.28 and 17.31 for the transverse shear coefficient ky, the surface energy due to transverse shear takes the form: 2

2

Qx Qy 1 1 + --- k ---------------W t = --- k x ----------------2 · hG xzÒ 2 y · hG yzÒ

17.7 EXAMPLES Examples for plates in bending are shown in details in Part Four of this book, in Chapter 18, “Applications.” We give here a few useful elements to treat these examples.

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 337 Monday, November 18, 2002 12:33 PM

17.7.1 Homogeneous Orthotropic Plate Warping functions: Equation 17.27 becomes k

E 11 = E

k

11

; E 12 = E 12 ; E

k 22

12

= E 22 ; G xz = G xz k

2 2 Ê E 11 E 22 12 d g0 12ˆ E 12 12 ----------------------------- -----3-˜ = – z ¥ -----2----------2 = – zh Á --------------------------------– 3 2 2 dz h Ë E 11 E 22 – E 12 h E 11 E 22 – E 12 h ¯

dg --------0 = 0 for z = ±h /2 dz then

12

2 2 dg 0 3 z 3 4z -------- = --- Ê 1 – 4 -----2ˆ ; g 0 = --- z Ê 1 – --- -----2ˆ dz 2Ë 2 Ë 3h ¯ h¯

Transverse shear stresses and shear coefficients: One deduces from Equation 17.32: 2 Q 3 z t xz = ------x ¥ --- ÊË 1 – 4 -----2ˆ¯ h 2 h

12 k x = -----3h

h/2

(17.33)

2

3Ê 4z --- 1 – --- -----2ˆ z 2 dz Ë 3h ¯ – h/2 2

Ú

6 k x = --5

(17.34)

In an analogous manner starting from Equation 17.28: p0 ( z ) = g0 ( z ) then: 2 Q 3 z t yz = ------y ¥ --- ÊË 1 – 4 -----2ˆ¯ h 2 h

(17.35)

6 k y = --5

(17.36)

Remark: In Application 18.3.7 (Chapter 18), one treats the case of a thick homogeneous orthotropic plate in cylindrical bending about the y axis. The plate supports a uniformly distributed load. One can consider there the strong influence of transverse shear in bending. Two characteristics of the plate then apply directly on the deflection:

12

g0 is, as g, antisymmetric in z (see Equation 17.4).

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 338 Monday, November 18, 2002 12:33 PM

Figure 17.3 Sandwich Plate

The relative thickness h/a, where a is the length of the bent side of the plate The ratio Ex/Gxz (for certain combinations of fiber/matrix, this ratio becomes large compared with unity; for example, for unidirectional)

17.7.2 Sandwich Plate The plate consists of two orthotropic materials: Material (1) for the skins Material (2) for the core (see Figure 17.3) Assuming the proportionality of elastic coefficients for the two materials leads to (see Section 17.6.3): then C ij =

Ú

h/2

➀

E ij z dz = E ij 2

– h/2

3

Ú

– H 2 /2

– H 1 /2

3

➁

z dz + E ij 2

Ú

H 2 /2

2

➀

z dz + E ij

– H 2 /2

3

➀ H 1 – H 2ˆ ➁ H - + E ij -------2 C ij = E ij Ê ------------------Ë 12 ¯ 12

H1 – H2 H aH aH ➀ - + a 12 -------2 C ij = E ij ¥ -----------1 with -----------1 = ------------------12 12 12 12 3

3

3

3

3

one deduces from there: ➀

C 11 12 E 11 1 - ¥ ----------3 --------- = ----------------------------- = -----------------------------------2 ➀ ➀ ➀ 2 C 11 C 22 – C 12 EI 11 E 11 E 22 – ( E 12 ) a H 1 ➀

– C 12 12 1 – E 12 - ¥ ----------3 --------- = ----------------------------- = ----------------------------------2 ➀ ➀ ➀ 2 C 11 C 22 – C 12 EI 12 E 11 E 22 – ( E 12 ) a H 1

© 2003 by CRC Press LLC

Ú

H 1 /2 H 2 /2

2

z dz

TX846_Frame_C17 Page 339 Monday, November 18, 2002 12:33 PM

17.7.2.1 Warping Functions 13

From the above one can write in Equation 17.27 : k

k

k

k

Ex E 12 E 11 E 12 ˆ Ê --------3 - + --------- = ------➀x- ¥ ----------3 = ---------------------------------------------3 3 Ë EI 11 EI 12¯ ( H – H2 ) ➀ ➁ H2 1 E x a H1 - + E x --E x -----------------12 12 In addition : ➀

➀

· hG xzÒ = G xz ( H 1 – H 2 ) + G xz H 2 Equation 17.27 then can be written as: ➀

➁

Ex G xz ( H 1 – H 2 ) + G xz H 2 g0 Ïd - ¥ 12 ----------------------------------------------------= – z ¥ ------k ➀ 3 3 ➁ 3 2 Ô ---------E dz G ( H – H ) + E H xz x 1 2 x 2 Ô Ô dg Ì --------0 = 0 for z = ± H 1 /2 Ô dz Ô Ô G dg -0 continuous for z = ±H 2 /2 Ó xz ------dz 2

k

In Equation 17.28, one obtains an analogous formulation. In effect, one can write k

k

k

k

Ey E 12 E 22 E 12 ˆ Ê -------- + --------- = -----➀-y ¥ ---------3 = --------------------------------------------3 3 3 Ë EI 22 EI 12¯ ( H – H2 ) ➀ ➁ H2 1 Ey a h --+ E E y -----------------y 12 12 The problem [17.28] is then written as: ➀

➁

E G yz ( H 1 – H 2 ) + G yz H 2 p0 Ïd = – z ¥ -------ky- ¥ 12 ----------------------------------------------------➀ 3 3 ➁ 3 2 Ô ---------dz G yz Ey ( H1 – H2 ) + Ey H2 Ô Ô dp Ì --------0 = 0 z = ±H 1 /2 Ô dz Ô dp 0 Ô G -------Ó yz dz continuous for z = ±H 2 /2 2

k

Remark: These problems are identical to that which allows the calculation of the warping function for the bending of a sandwich beam, and one can consider it in Chapter 18, application 18.3.5. One can then carry out the same steps of calculation. The results obtained are shown below. 13

See Equations 17.2.

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 340 Monday, November 18, 2002 12:33 PM

17.7.2.2 Transverse Shear Stresses Stress txz: E x Ê -----2- – z2ˆ + E x Ê -----1- – -------2 ˆ Ë4 ¯ Ë4 4¯ = Q x ¥ 6 ¥ -----------------------------------------------------------➀ 3 3 ➁ 3 Ex ( H1 – H2 ) + Ex H2 ➁

H H – ------2 £ z £ ------2 ; t xz 2 2

2

H

➀

H

2

H

2

(17.37)

2

➀ H1 x 4

E ( ---- – z ) H H2 ------ £ z £ ------1 : t xz = Q x ¥ 6 ¥ -------------------------------------------------➀ 3 3 ➁ 3 2 2 E x ( H1 – H2 ) + Ex H2 2

Stress tyz: ➁ H

2

➀ H

2

H

2

E y ( ---4-2 – z2 ) + E y ( ---4-1 – ---4-2 ) H2 H2 – ------ £ z £ ------ ; t yz = Q y ¥ 6 ¥ ---------------------------------------------------------➀ 3 3 ➁ 3 2 2 Ey ( H1 – H2 ) + Ey H2 2

➀ H1 y 4

(17.38)

E ( ---- – z ) H H ------2 £ z £ ------1 ; t yz = Q y ¥ 6 ¥ -------------------------------------------------➀ 3 3 ➁ 3 2 2 E y ( H1 – H2 ) + Ey H2 2

17.7.2.3 Transverse Shear Coefficients ➁

Ï Ex 3 ➀ 2 Ê 4 ➁ ax -H 2 E x H 1 + --- E x – E ➀x ˆ H 22 º - ------k x = --------------------------------------------------------➀ 3 3 ➁ 3 Ì ➁ Ë5 ¯ 8 [ E x ( H 1 – H 2 ) + E x H 2 ] Ó G xz ➀ 2

➀

¸ Ex ) Ê 4 5 H2 3b x E x ( H 1 – H 2 ) … + (------------ --- H + ------ – H 21 H 32ˆ ˝ + ------------------------------------------------➀ Ë5 1 ➀ 3 3 ➁ 3 ¯ 5 G xz ˛ Ex ( H1 – H2 ) + Ex H2 5

➀

with

2

2

➁

G xz ( H 1 – H 2 ) + G xz H 2 a x = 12 ¥ ----------------------------------------------------➀ 3 3 ➁ 3 Ex ( H1 – H2 ) + Ex H2

(17.39)

➀ 2 ➀ ➁ ➀ ˆ a Ex Ï H2 2 Ex ˆ ¸ 2 Ê G xz 2 G xz Ê ----------------˜ H 1 – ------– 1 b x = -----x- H 2 ------– + H Á Á ˜ Ì 1 2 ➁ ➁ 16 G ➀xz Ó 3 3 E ➀x ¯ ˝˛ G xz Ë Ë G xz ¯

ky is given by an expression formally identical to that in which the index x is replaced by y. In Application 18.3.8 we treat the case of a rectangular sandwich plate in cylindrical bending, clamped on one side and subjected to a uniform linear force on another. The plate is free on the other sides. One shows the influence of transverse shear on the deflection. This influence increases when: The mechanical characteristics (moduli) of the core are weaker than those of the skins. The relative thickness of the core is important (thin skins). The relative thickness of the plate is large (thick plate).

© 2003 by CRC Press LLC

TX846_Frame_C18a Page 341 Monday, November 18, 2002 12:40 PM

PART IV APPLICATIONS We have grouped in this last part of the book exercises and examples for applications. These have various objectives and different degrees of difficulties. Leaving aside (except for special cases) the cases that are too academic, we will concern ourselves with applications of concrete nature, with an emphasis on the numerical aspect of the results. A few of these applications should be used as validation tests for numerical models.

© 2003 by CRC Press LLC

TX846_Frame_C18a Page 343 Monday, November 18, 2002 12:40 PM

18 APPLICATIONS 18.1 LEVEL 1 18.1.1 Simply Supported Sandwich Beam Problem Statement: 1. The following figure represents a beam made of duralumin that is supported at two points. It is subjected to a transverse load of F = 50 daN. Calculate the deflection—denoted as D —of the beam under the action of the force F.

2. We separate the beam of duralumin into two parts with equal thickness ep = 2.5 mm, by imaginarily cutting the beam at its midplane. Each half is bonded to a parallel pipe made of polyurethane foam, making the skins of a sandwich beam having essentially the same mass as the initial beam (in neglecting the mass of the foam and the glue). The beam is resting on the same supports and is subjected to the same load F. Calculate the deflection caused by F, denoted by D¢. Compare with the value of D found in Part 1. (Take the shear modulus of the foam to be: Gc = 20 MPa.)

Solution: 1. We will use the classical formula that gives the deflection at the center of the beam on two supports: F D = ----------48EI

© 2003 by CRC Press LLC

3

with

bh I = -------12

TX846_Frame_C18a Page 344 Monday, November 18, 2002 12:40 PM

For duralumin (see Section 1.6): E = 75,000 MPa. One finds D = 16.7 mm 2. Denoting by W the elastic energy due to flexure, one has

Ú

W =

beam

2

1 M --- ----------- dx + 2 · EI Ò

Ú

beam

1

1 k --- ------------T 2 dx 2 · GSÒ

2

with : k 1 ------------ # --------------------------------------· GSÒ G c ( e c + 2e p ) ¥ b ∂W

Using Castigliano theorem, one has D¢ = -------∂F then: D¢ =

Ú

beam

M dM ----------- -------- dx + · EI Ò dF

Ú

beam

dT k ------------T ------ dx · GSÒ dF

0 £ x £ /2:

M = Fx/2; F M = --- ( – x ); 2

/2 £ x £ : 1 Ï D¢ = ----------- Ì · EI Ò Ó

Ú

/2

0

Fx x ------ ¥ --- dx + 2 2

k Ï º + ------------· GS Ò ÌÓ

Ú

/2

0

T = –F /2 T = F /2

¸ F ( – x) --- ( – x ) ----------------- dx º ˝ 2 /2 2 ˛

Ú

F dx – --- ¥ – ------ + 2 2

F dx ¸ --- ¥ ------ ˝ 2 ˛ /2 2

Ú

3

F k F D¢ = ------------------ + ------ -----------48 · EI Ò 4 · GSÒ Approximate calculation: ( ec + ep ) ec b - + E c ¥ ------· EI Ò # E p ¥ e p ¥ b ¥ --------------------12 2 2

3

then: · EI Ò = 7090 MKS + 7.8 MKS

negligible

1 2

with

E c = 60 MPa ( cf. 1.6 )

To establish this relation, see Chapter 15, Equation 15.17. See calculation of this coefficient in 18.2.1, and more precise calculation in 18.3.5.

© 2003 by CRC Press LLC

TX846_Frame_C18a Page 345 Monday, November 18, 2002 12:40 PM

one obtains for D¢: D¢ = 0.18 mm + 1.04 mm bending moment

shear

D¢ = 1.22 mm Comparing with the deflection D found in Part 1 above: D 14 ----- = -----D¢ 1

Remarks: The sandwich configuration has allowed us to divide the deflection by 14 without significant augmentation of the mass: with adhesive film thickness 3 0.2 mm and a specific mass of 40 kg/m for the foam, one obtains a total mass of the sandwich: m = 700 g (duralumin) + 50 g (foam) + 48 g (adhesive) This corresponds to an increase of 14% with respect to the case of the full beam in Question 1. The deflection due to the shear energy term is close to 6 times more important than that due to the bending moment only. In the case of the full beam in question 1, this term is negligible. In effect one has: k = 1.2 for a homogeneous beam of rectangular section, then: k ------- = 8.27 ¥ 10 –8 GS (with G = 29,000 MPa, Section 1.6). The contribution to the deflection D of the shear force is then: k

dT

- T ------ dx = 0.02 mm > 1. The displacement of configuration (c) is much larger than the others. This will create problems when operating the arm. 2. The deflections are identical for configurations (a) and (c) if Ex ˆ 1 1 2 --- = --- Ê --- + ----------3 8 Ë 3 2G xy¯ then: E -------x- = 4 G xy

© 2003 by CRC Press LLC

TX846_Frame_C18a Page 395 Monday, November 18, 2002 12:40 PM

3. In looking for the modulus Gxy to be as high as possible, one reads on Tables 5.4 and 5.5 (Section 5.4.2.) a ratio Ex /Gxy = 3.9 (4) for the composition:

4. The maximum value of the longitudinal modulus of elasticity observed on Table 5.4 is E¢x = 134,000 MPa This corresponds to a shear modulus (Table 5.5): G¢xy = 4,200 MPa The same deflection as the previous one for the configuration (c) can be obtained by 3 3 E¢x ˆ F 2 F -------------- Ê --- + ------------ = ----------8E¢x I¢ Ë 3 2G¢xy ¯ 3E x I

then: 3 E¢x ˆ 3E 2 I¢ p r e¢ --- = ------------ = 3.5 = ---------x- Ê --- + -----------3 Ë I 8E¢x 3 2G¢x y ¯ pr e e¢ ---- = 3.5 e

The tube with thickness e¢ and modulus Ex¢ will be more stiff for configuration (a) but will have a mass multiplied by 3.5 to keep the stiffness of configuration (c). 5. Configurations (a) and (c) are the more deformable. One then has to write 3E x I Ê F ˆ F ----- = ---------- ≥ --3 Ë D¯ min Dy with = 15 m; I = pr e; r = 0.15 m; (F/D)min = 10 N/m; Ex = 75,407 MPa 3

4

e ≥ 14 mm

© 2003 by CRC Press LLC

TX846_Frame_C18a Page 396 Monday, November 18, 2002 12:40 PM

The ply thickness being 0.13 mm, one obtains 108 layers oriented as follows:

6. The specific mass of the laminate is indicated in Section 3.3.3, as r = 1530 3 kg/m. The distributed mass of the arm is then: m ----- = 2 p re ¥ r = 20.2 kg/m with the angular acceleration indicated in Figure 18.8, one obtains the following inertial load:

We then deduce from there: The deflection at the end due to the concentrated mass: 3

100 D concent. = -------------3E x I 19

The deflection at the end due to distributed load : 4

11 0.81 D distributed = --------- ¥ ---------------Ex I 120 from which we can obtain a total deflection: 3

3

100 100 D total = -------------- ( 1 + 0.033 ) # -------------3E x I 3E x I The rigidity (F/Dtotal) appears to be well related essentially to the concentrated inertial load at the extremity of the arm. 19

---------- [ 2 – 3 ( X/ ) + ( X/ ) ] Result obtained from the differential equation: EI x d v/dX = – 0.81 6

© 2003 by CRC Press LLC

2

2

2

3

TX846_Frame_C18b Page 397 Monday, November 18, 2002 12:43 PM

18.2 LEVEL 2 18.2.1 Sandwich Beam: Simplified Calculation of the Shear Coefficient Problem Statement: Represented below is the cross section of a sandwich beam. The thickness of the skins is small compared with that of the core. Under the action of a shear load T, 20 the shear stresses in the section are assumed to vary in a piecewise-linear fashion along the y direction. The constitutive materials, denoted as 1 and 2, are assumed to be isotropic, or transversely isotropic. The shear moduli are denoted as G1 for material 1 (skin) and G2 for material 2 (core). The beam has a width of unity. 1. Calculate the shear coefficient k for flexure in the plane x,y.

2. Give a simplified expression for the case—current in the applications— where G1 >> G2 with the notations for the thicknesses: H1 – H2 e p = ------------------; 2

ec = H2

Solution: 1. Let W be the strain energy due to shear stresses. One has (Equation 15.17): 2

1 dW 1 kT --------- = --- ------------- = --2 dx 2 · GS Ò

Ú

section

t xy ------ dy Gi 2

In the upper skin, one has H 1 – 2y t xy = -----------------¥ to H1 – H2

20

This representation of the shear stresses is only approximate. One will find in Application 18.3.5 the results concerning a more precise distribution of these stresses. In fact, the approximate representation of the shear proposed here is better approximated than the skins of the sandwich structure will have a small thickness as compared to that of the core.

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 398 Monday, November 18, 2002 12:43 PM

On the other hand in the core: txy = t0 T =

Then with:

Ú

t xy ( dy ¥ 1 )

section

One deduces from there the maximum shear stress to: 2 t o = T ¥ ------------------H1 + H2 Strain energy: dW 1 t xy --------- = --- -----dy = dx 2 Gi

Ú

2

Ú

H 2 /2

o

t -----o- dy + G2 2

t ( H 1 – 2y ) -----o- ------------------------dy 2 G H 2 /2 1 ( H1 – H2 )

Ú

H 1 /2

2

2

After calculation: 1 --2

Ú

2 t xy t H H 1 – H 2ˆ H H 1 – H 2ˆ 2T ------ dy = ----o- Ê ------2 + -----------------= --------------------------2 Ê ------2 + -----------------Ë 3G 1 ¯ 3G 1 ¯ Gi 2 Ë G2 ( H1 + H2 ) G2 2

2

one then has 2 2 H H 1 – H 2ˆ 2T 1 kT --- ------------- = --------------------------2 Ê ------2 + -----------------Ë 3G 1 ¯ 2 · GS Ò ( H1 + H2 ) G2

Then: 4 · GS Ò H H 1 – H 2ˆ k = --------------------------2 Ê ------2 + -----------------3G 1 ¯ ( H1 + H2 ) Ë G2 with (Equation 15.16): GS = G1 (H1 – H2) + G2 H2: 4 [ G 1 ( H 1 – H 2 ) + G 2 H 2 ] Ê H 2 H 1 – H 2ˆ - ------ + -----------------k = --------------------------------------------------------2 Ë G2 3G 1 ¯ ( H1 + H2 ) 2. Case where G2 30 N/mm applied.

18.2.11 Determination of the Elastic Characteristics of a Carbon/Epoxy Unidirectional Layer from Tensile Test Problem Statement: Consider a unidirectional plate of carbon/epoxy, from which one cuts the two samples shown below. They are tested in a testing machine. One measures the strains using strain gages arranged as shown. The strains obtained under different loads are linearized. One shows their values corresponding to a uniform tensile stress sx equal to 20 MPa. Calculate the elastic constants of the unidirectional layer subject to in-plane loading.

Solution: One can use the Equation 11.5: Sample No. 1: The axes x and y are ,coincident with the axes and t (q = 0). From which:

s s 20 e 1x = -----x = -----x Æ E = ------------------- = 139,860 MPa Ex E 143 E-6 n n xy e 1y = – ------ ¥ s x = – -----t- ¥ s x Æ n t = 0.25 E Ex

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 436 Monday, November 18, 2002 12:43 PM

Sample No. 2: The axes x and y make an angle of q = 20∞ with the axes 40 l and t, from which : Ï c4 s4 s n ¸ 2 2 1 e 2x = -----x = Ì ----- + ---- + c s ÊË ------- – 2 -----t-ˆ¯ ˝ ¥ s x Ex E ˛ E E G t t Ó Ïn n xy 1 ¸ 1 1 - ¥ s x = – Ì -----t- ( c 4 + s 4 ) – c 2 s 2 Ê ----- + ---- – -------ˆ ˝ ¥ s x e 2y = – -----Ë ¯ Ex E E G E t t ˛ Ó leading to 1 0.1325 Ï ------- + ---------------- = 2.69 E-4 Et Ô G t Ì 1 1 Ô ------ – ---- = 1.144 E-4 Ó G t E t from which: Et = 7320 MPa; Gt = 3980 MPa In summary: E = 139 ,860 MPa E t = 7 320 MPa

n t = 0.25;

n t = 0.013

G t = 3980 MPa

18.2.12 Sailboat Shell in Glass/Polyester Consider a siding of a laminated shell for a sailboat made of glass/polyester. It is made up of a stack of layers of balanced fabric and glass mat. The reinforcements, in “E” glass, are in the following form: Balanced fabric: Vf = 20%, mass of the glass per square meter: mof = 500 g. Mat: Vf = 15%, mass of glass per square meter: mof = 300 g.

Problem Statement: 1. Calculate: (a) The thickness of one layer of fabric of glass/polyester. (b) The thickness of a layer of mat of glass/polyester. 2. Given the composition of the laminated siding as follows: [M/F/M/F]s (M ´ Mat; F ´ Fabric) 40

n Et

n E

One has -----t- = -----t- See Exercise 18.1.2

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 437 Monday, November 18, 2002 12:43 PM

Figure 18.9

Figure 18.10

what is the total thickness, denoted as h, of the laminated siding? 3. Elastic characteristics of a fabric layer: One considers a layer of balanced fabric to be equivalent to two series of unidirectional plies crossed at 90∞, each series possessing half of the total thickness of the fabric layer (see Figure 18.9). The elastic characteristics of these unidirectional plies are as follows: E = 18,000 MPa; Et = 4900 MPa; Gt = 1850 MPa; nt = 0.3. Calculate the elastic characteristics (moduli, Poisson coefficients) of a layer of fabric in axes C,T. 4. The layers of mat are considered as isotropic in their planes, with the elastic characteristics: EMat = 8350 MPa; n Mat = 0.3. Figure 18.10 represents one planar portion of the laminated siding. All the fabric plies are oriented at 0∞ – 90∞. Calculate the global elastic characteristics (moduli, Poisson coefficients) of the siding working in its plane. Remark: Tests done on samples made of this material indicate a modulus of elasticity along the x direction to be equal to 9200 MPa. What can be said about this? 5. Rupture: The rupture strengths, considered to be equal in tension and in compression, are as follows:

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 438 Monday, November 18, 2002 12:43 PM

Fabric layer: along C or T: srupture fabric = 139 MPa. Mat layer: srupture Mat = 113 MPa. (a) Calculate the maximum stress sox leading to first ply failure of the siding. What are the layers that fracture? (b) Apply the maximum stress sox. In the previous layers that fractured, the glass fibers are supposed all broken. What happens to the laminate?

Solution: 1. The thickness of a layer denoted as h is such that (see Section 3.2.4): m of h = ---------Vf rf The specific mass of “E” glass is (see Section 1.6): r = 2600 kg/m , from which: 3

hfabric = 0.96 mm; hMat = 0.77 mm. 2. The siding is constituted of the following stacking sequence:

The total thickness is h = 0.77 ¥ 4 + 0.96 ¥ 3 = 5.96 mm. 3. Elastic characteristics of a fabric layer: The moduli and Poisson coefficients can be evaluated starting from the simplified relations of Section 3.4.2. One obtains, with k = 0.5 (balanced fabric): EC = ET = 11,450 MPa GCT = 1850 MPa; nCT = nTC = 0.128 A more precise calculation of these characteristics requires to establish the matrix –1 h[A] of Section 12.1.2. (Equation (12.9)). We calculate at first --h1- [ A ] (Equation 12.8): 0∞ 90∞ 1 --- A ij = ( E ij ) ( 0.5 ) + ( E ij ) ( 0.5 ) h

The terms E ij are given by the Equation 11.8. One will have, for example: 1 1 E + Et --- A 11 = ( E ) ( 0.5 ) + ( E t ) ( 0.5 ) = --- --------------------h 2 1 – n t n t

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 439 Monday, November 18, 2002 12:43 PM

with E n t = n t -----t ; E One obtains 11,737 1507 0 1507 11,737 0 ( MPa ) 0 0 1850

1 --- [ A ] = h

1 ---------------11,540

h[A ]

-1

0.128 = – --------------11,540

0.128 – --------------11,540

0

1 ---------------11,540

0

0

1 -----------1 850

0 from which:

E C = E T = 11,540 MPa G CT = 1850 MPa

n CT = n TC = 0.128 (The difference between the values obtained above is small). 4. Elastic characteristics of the siding: These are deduced from the matrix -1 h[A] (Equation 12.9) calculated for all the laminate. We calculate at first

1 --- [ A ] (Equation h

12.8):

fabric Mat 1 --- A ij = ( E ij ) ( p fabric ) + ( E ij ) ( p Mat ) h

with p

fabric

3 ¥ 0.96 = ---------------------- = 0.483; 5.96 fabric

E 11

fabric

E 12

fabric

= E 22

p

Mat

EC = E C = ---------------2 1 – n CT

= n CT E C ;

E Mat Mat Mat -; E 11 = E 22 = ----------------2 1 – n Mat

fabric

E 33

= G CT

n Mat E Mat Mat E 12 = -----------------2 1 – n Mat

E Mat Mat E 33 = G Mat = -------------------------2 ( 1 + n Mat )

© 2003 by CRC Press LLC

= 0.517. (see Equation 11.8)

TX846_Frame_C18b Page 440 Monday, November 18, 2002 12:43 PM

We obtain 10,410 2149 0

1 --- [ A ] = h

2149 0 10,410 0 [ MPa ] 0 2554

1 -----------9966

h[A ]

–1

= – 0.206 ------------9966 0

------------– 0.206 9966

0

1 -----------9966

0

0

1 -----------2554

then: E x = E y = 9966 MPa G xy = 2554 MPa

n xy = n yx = 0.206 Remark: The real modulus (measured) 9200 MPa is a bit smaller than the one calculated. In effect, due to the curvature of fibers from weaving, a fabric layer is softer than the stacking of unidirectionals that are crossed at 90∞. However, the approximation obtained by calculation is suitable (difference < 10%). 5. Fracture of the siding: (a) One subjects the siding to a stress sox. The strains of this siding are given by the Equation 12.9 as: Ï e ox Ô Ì e oy Ô Ó g oxy

Ï s ¸ ox Ô –1 Ô ˝ = h[A ] Ì 0 Ô Ô Ó 0 ˛

¸ Ï s ox /9966 Ô Ô = ˝ Ì – 0.206 s ox / 9966 Ô Ô 0 ˛ Ó

¸ Ô ˝ Ô ˛

These strains give rise to the following stresses: In the layers of fabric (see results from Question 3): Ï sC Ô Ì sT Ô Ó t CT

¸ Ï 11,737 Ô Ô ˝ = Ì 1507 Ô Ô 0 ˛ Ó

1507 11,737 0

0 0 1850

¸Ï s ox /9966 ÔÔ ˝Ì – 0.206 s ox /9966 ÔÔ 0 ˛Ó

Ï 1.15 s ox Ô ◊◊◊ = Ì -0.09 s ox Ô 0 Ó

© 2003 by CRC Press LLC

¸ Ô ˝ Ô ˛

¸ Ô ˝◊◊◊ Ô ˛

TX846_Frame_C18b Page 441 Monday, November 18, 2002 12:43 PM

The Hill–Tsai criterion in these layers is satisfied for a stress sox such that: 1.15 s oxˆ Ê – 0.09 s oxˆ – 0.09 ¥ 1.15 s ox Ê -----------------+ ---------------------- – -------------------------------------- = 1 2 Ë 139 ¯ Ë 139 ¯ 139 2

2

2

as:

sox = 116 MPa Mat

In the layers of Mat, with the values of the coefficients E ij of Question 4, we have Ï sx ¸ Ï s ox /9 966 Ô Ô Mat Ô Ì s y ˝ = [ E ] Ì – 0.206 s ox /9 966 Ô Ô Ô 0 Ó t xy ˛ Ó

¸ Ï 0.86 s ox Ô Ô ˝ = Ì 0.087 s ox Ô Ô 0 ˛ Ó

¸ Ô ˝ Ô ˛

The Hill–Tsai criterion in the mat layers is satisfied for a stress sox such that : 41

0.86 s oxˆ Ê 0.087 s oxˆ 0.86 ¥ 0.087 s ox Ê -----------------+ --------------------- – ------------------------------------- = 1 2 Ë 113 ¯ Ë 113 ¯ 113 2

2

2

then:

s ox = 138 MPa The fabric layers are the first to fail, for a stress of

sox max = 116 MPa (b) This stress being applied, the rupture of the fabric layers translates into the rupture of the glass fibers. The stress resultant corresponding to this constraint as: Nx = sox max ¥ h = 116 ¥ 5.96 = 691 N/mm is then completely taken up by the layers of Mat. The stress in these layers is then: Nx 691 - = ------------------- = 224 MPa s ox Mat = ----------------4 ¥ h Mat 4 ¥ 0.77

41

A mat layer does not have transverse isotropy in the axes y, z (or x,z). The Hill-Tsai expression is then modified. We use however the Equation 14.6 here (see remark 39 at the bottom of page in Application 18.2.10).

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 442 Monday, November 18, 2002 12:43 PM

It exceeds the rupture strength of the Mat (113 MPa). Then this latter layer fractures. The siding is then completely broken under the stress:

sox max = 116 MPa

18.2.13 Determination of the In-Plane Shear Modulus of a Balanced Fabric Ply Problem Statement: Consider a sample cut from a laminated panel made of identical layers of balanced fabric, all oriented along the axes C (warp direction) and T (fill direction) in the following figure. The sample is in a state of simple tension in its plane along the x axis as shown in the figure.

sox π 0;

soy = toxy = 0

Two strain gages are bonded (see figure). These are denoted as 1 and 2:

From gage 1, one reads a strain eox. From gage 2, one reads a strain eoy. 1. Noting that goxy = 0, give the expression for the distortion gCT in the axes C and T as a function of eox and eoy. 2. Give the expression for the stress tCT in the axes C and T as a function of sox. 3. Deduce from the previous answer the shear modulus GCT as a function of eox, eoy, and sox.

Solution: 1. Equation 11.7 allows one to write Ï Ô eC Ô Ì eT Ô Ô g CT Ó

© 2003 by CRC Press LLC

¸ Ï Ô Ô c2 Ô Ô ˝ = Ì s2 Ô Ô Ô Ô 2cs ˛ Ó

s

2

c

2

– 2cs

¸Ï ÔÔ e ox ÔÔ ˝Ì e cs ÔÔ oy 2 2 ( c – s ) ÔÔ g oxy ˛Ó – cs

¸ Ô Ô ˝ Ô Ô ˛

TX846_Frame_C18b Page 443 Monday, November 18, 2002 12:43 PM

Here, we have a balanced laminate with midplane symmetry, loaded in its axes x,y. Then (Equation 12.9): goxy = 0, from which: 1 1 g CT = 2cs e ox – 2cs e oy with c = ------- ; s = – ------2 2 g CT = – e ox + e oy 2. According to Equation 11.4: Ï Ô sC Ô Ì sT Ô Ô t CT Ó

¸ Ï Ô Ô c2 Ô Ô ˝ = Ì s2 Ô Ô Ô Ô sc ˛ Ó

s

2

c

¸Ï ÔÔ s ox ÔÔ 2cs ˝Ì 0 ÔÔ 2 2 ( c – s ) ÔÔ 0 ˛Ó – 2cs

2

– sc

¸ Ô Ô ˝ Ô Ô ˛

then:

s ox t CT = sc s ox = – ------2 3. The constitutive behavior of the fabric in its axes can be written, starting from the Equation 11.5, as: Ï eC Ô Ô Ì eT Ô Ô Ó g CT

¸ Ô Ô ˝ = Ô Ô ˛

Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

1 ----Ec

n CT – ------Ec

CT – -------

n Ec

1 ----Ec

0

0

¸ Ô Ô Ô Ô 0 ˝ Ô Ô 1 --------- Ô G CT Ô ˛

0

Ï sC Ô Ô = Ì sT Ô Ô Ó t CT

¸ Ô Ô ˝ Ô Ô ˛

t CT g CT = -------G CT From which:

s ox G CT = --------------------------2 ( e ox – e oy )

18.2.14 Quasi-Isotropic Laminate Problem Statement: Consider a laminate made up of a number of identical unidirectional plies, with midplane symmetry and the following composition:

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 444 Monday, November 18, 2002 12:43 PM

The elastic characteristics of a ply in its axes and t are denoted as: E, Et, Gt, nt, nt One examines the behavior of this laminate under in-plane loading, following the law (Equation 12.9): Ï e ox Ô Ì e oy Ô Ó g oxy

¸ Ï s ox Ô –1 Ô ˝ = h [ A ] Ì s oy Ô Ô ˛ Ó t oxy

¸ Ô ˝ Ô ˛

1. Calculate the coefficients of the matrix --h1- [ A ] . 2. By inversion, deduce from there the elastic moduli of the laminate. 3. What comment can one make? Deduce from there the law for the behavior of the laminate under in-plane loading in the axes (X,Y) derived from the (x, y) axes by a rotation angle q.

Solution: 1. Coefficients

1 --- A ij h

are given by the Equation 12.8 as: 1 1 --- A ij = --- E 0∞ + E 90∞ + E +45∞ + E –45∞ ij ij ij h 4 ij 0∞

The stiffness coefficients E ij are obtained from the behavior of a ply (Equation 11.8). In using this relation for q = 0∞, 90∞, +45∞, –45∞, one obtains 1 1 1 3 --- A 11 = --- A 22 = --- --- ( E + E t ) + n t E + 2G t h h 4 2 1 1 1 --- A 12 = --- --- ( E + E t ) + 3 n t E – 2G t 4 2 h 1 1 1 --- A 33 = --- --- ( E + E t ) – n t E + 2G t 4 2 h 1 1 --- A 13 = --- A 23 = 0 h h where one recalls that: E =

© 2003 by CRC Press LLC

E -----------------------; 1 – n t n t

Et =

Et ----------------------1 – n t n t

TX846_Frame_C18b Page 445 Monday, November 18, 2002 12:43 PM

The matrix

1 --- [ A ] reduces h

to A 11 1 --- A 21 h 0

A 12 A 11 0

0 0 A 33

2. From the above, the modulus of elasticity of the laminate in directions x and y, and the associated Poisson coefficient are 1 --- A 11 1 h -; --- = -----------------------------2 2 1 E -----2 ( A 11 – A 12 ) h

1 --- A 12 n h – --- = – -----------------------------2 2 1 E -----2 ( A 11 – A 12 ) h

One obtains after calculation: [ 2 ( E + E t ) + 4 n t E ] [ E + E t – 2 n t E + 4G t ] E = ------------------------------------------------------------------------------------------------------------------3 4 --2- ( E + E t ) + n t E + 2G t

n =

1 --- ( E + E t ) + 3 n t E – 2G t 2 ---------------------------------------------------------------3 --- ( E + E t ) + n t E + 2G t 2

The shear modulus is written as: 1 1 G = --- --- ( E + E t ) – n t E + 2G t 4 2 3. One can remark that: E G = -------------------2(1 + n ) This leads to an isotropic elastic behavior of the laminate in its plane. As a result, in all coordinate systems (X,Y) derived from (x,y) by any rotation angle, the constitutive behavior of the laminate is unchanged and is written as: Ï e Ô X Ô Ì eY Ô Ô g Ó XY

© 2003 by CRC Press LLC

¸ n 1 --- – --Ô E E Ô 1 --˝ = – --EnE Ô Ô 0 0 ˛

Ï s Ô X Ô 0 = Ì sY Ô 1 Ô t ---G Ó XY 0

¸ Ô Ô ˝ Ô Ô ˛

TX846_Frame_C18b Page 446 Monday, November 18, 2002 12:43 PM

Remark: This result generalizes to other groups of orientations for plies such as:

p 2p 0, --- , ------ ; 3 3

p 2p 3p 4p 0, --- , ------, ------, -----5 5 5 5

and so on. More generally, a laminate made up of n orientations (a whole number n > 2), having the values of --np- ( p – 1 ), with p = 1,…, n and with the same proportion of plies along each orientation as (1/n) is elastically isotropic. One shows also that 42 for all these laminates, E and n are invariable.

18.2.15 Orthotropic Plate in Pure Torsion Problem Statement: Consider a square plate (a ¥ a) of unidirectional glass/epoxy (Vf = 60%), thickness h, welded at the center of its lower face on a support. It is subjected to a uniform 43 and constant torsional moment density mo (N mm/mm) along its perimeter. The directions , t of the unidirectional form an angle q with the axes x,y of the plate (see figure).

1. Assuming that all stress resultants in the plate are zero (except the torsional moment), determine the bending displacement at all points of the midplane. 2. Determine the state of stresses in the axes (x, y) then in the axes (,t) of the unidirectional layer. 3. Numerical application: q = 45∞; a = 1 m; h = 5 mm; mo = –10 N mm/mm. 42

43

For more details, see Bibliography at the end of the book: “Stiffness isotropy and resistance quasi-isotropy of laminates with periodic orientations.” The practical importance of such a load is very limited. It is better to consider this example as a means to validate a computer program using finite elements. It is one of the “patches” issued from the work “Computer programs for composite structures: Examples of reference for validation” (see Bibliography at the end of the book).

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 447 Monday, November 18, 2002 12:43 PM

Solution: 1. In the constitutive Equation 12.16, one has C ij = E ij

3

h/2

h 2 z dz = E ij -----12 – h/2

Ú

then: 3

h [ C ] = ------ [ E ] 12 where [ E ] is the matrix shown in details in Equation 11.8. By inverting the Equation 12.16 and noting that: [C] where

1 --E

–1

12 –1 12 1 = -----3- [ E ] = -----3- --h h E

is the matrix shown in details in Equation 11.5, one has Ï Ô Ô Ô Ô Ô Ì Ô Ô Ô Ô Ô Ó

¸ 2 ∂ wo Ô Ô – -----------2 Ô ∂x Ô 2 ∂ w o Ô˝ – -----------2 Ô ∂y Ô Ô 2 ∂ wo Ô - Ô – 2 -----------∂x∂y ˛

Ï My 12 1 Ô = -----3- --- Ì – M x h E Ô Ó – M xy

¸ Ô ˝ Ô ˛

[1]

44

Assuming the unit stress resultants all to be zero except Mxy, Nx = Ny = Txy = Mx = My = 0;

one has

Mxy = mo

There remains (see Equation 11.5):

∂ wo 12 h xy ----------- = -----3- ------- mo ; 2 h G xy ∂x 2

∂ wo 12 m xy ----------- = -----3- ------- mo ; 2 h G xy ∂y 2

∂ w 12 1 2 ------------o- = -----3- -------- m o ∂x∂y h G xy 2

Therefore one can write wo(x, y) in the form: 12 m 2 2 w o = -----3- -------o- ( Ax + By + Cxy + Dx + Ey + F ) G xy h

44

With this hypothesis, equations of equilibrium, constitutive equation, and boundary conditions are verified.

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 448 Monday, November 18, 2002 12:43 PM

At the center of the plate: wo = 0;

∂ wo ---------∂x

=

∂ wo ---------∂y

= 0

from which: D = E = F = 0. And by identification with the second derivatives: 2A = hxy; 2B = mxy; 2C = 1 The out-of-plane displacement takes the form: 6m o - ( h xy x 2 + m xy y 2 + xy ) w o = ------------3 h G xy

[2]

2. State of stresses: The strain field in the axes of the plate is written as (Equation 12.12, taking into account [1]): Ï Ô ex Ô Ô Ì ey Ô Ô Ô g xy Ó

Ï

¸ Ô Ô Ô Ô Ô Ô Ô Ô ¥ = z Ì ˝ Ô Ô Ô Ô Ô Ô Ô Ô ˛ Ó

¸ 2 Ô ∂ wo Ô – -----------2 ∂ x ÔÔ Ô 2 ∂ wo ˝ – -----------Ô 2 ∂y Ô Ô 2 ∂ wo Ô – 2 ------------- Ô ∂x∂y ˛

Ï Ô 0 Ô 12 1 Ô = z ¥ -----3- --- Ì 0 h E Ô Ô Ô –mo Ó

¸ Ô Ô Ô ˝ Ô Ô Ô ˛

from which one can write the stresses in the axes (x, y) using Equation 11.8: Ï sx ¸ Ï ex Ô Ô Ô Ì sy ˝ = [ E ] Ì ey Ô Ô Ô Ó t xy ˛ Ó g xy

¸ Ï 0 Ô 1 Ô 12 ˝ = z ¥ -----3- [ E ] --E- Ì 0 h Ô Ô ˛ Ó –mo

¸ Ï 0 Ô 12 Ô ˝ = z ¥ -----3- Ì 0 h Ô Ô ˛ Ó –mo

¸ Ô ˝ Ô ˛

then:

s x = 0;

s y = 0;

12 t xy = – z ¥ -----3- m o h

Stresses in the axes of the unidirectional: These are obtained by using 45 the Equation 11.4, which is

s = – 2cs t xy s t = 2cs t xy t t = ( c – s ) t xy 2

45

2

24 = z ¥ c s ¥ -----3- m o h 24 = – z ¥ cs ¥ -----3- m o h 12 2 2 = – z ( c – s ) ¥ -----3- m o h

Note that here the angle q = ( · x ) since the Equation 11.4 is written with q = ( x · ) .

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 449 Monday, November 18, 2002 12:43 PM

3. Numerical application: One has (Section 3.3.3) for the glass/epoxy: E = 45,000 MPa; Gt = 4500 MPa;

Et = 12,000 MPa;

nt = 0.3 (nt = 0.08)

from which (Equation 11.5 with q = –45∞):

h xy m xy 0.1375 ------- = ------- = – ---------------G xy G xy 4500 and wo takes the form: 1 2 w o = – -------------- [ xy – 0.1375 ( x 2 + y ) ] 9 375 The deformed configuration is shown in the figure below:

The stresses (in MPa) are written as:

sx = sy = 0;

txy = 0.96 ¥ z (mm).

s = –st = 0.96 ¥ z (mm);

tt = 0

18.2.16 Plate Made by Resin Transfer Molding (R.T.M.) Problem Statement: First part: A roll of mat of carbon fibers has the following characteristics: Areal mass density: mof = 30 g/m 3 Specific mass: rf = 1,750 kg/m

© 2003 by CRC Press LLC

2

TX846_Frame_C18b Page 450 Monday, November 18, 2002 12:43 PM

One deposits 21 layers of this mat over a plate in a rectangular mold. The mold is then closed and sealed, as shown in the figure below:

R1 and R2 represent two valves. R2 is closed, R1 is open. The mold is vacuumed. R2 is open, R1 is open. Polyester resin is filled into the cavity of the mold. Then resin begins to flow out through valve R1. R1 and R2 are closed. The mold is then heated, and the resin polymerizes. After demolding, one obtains a plate of mat/polyester. 1. Calculate the fiber volume fraction Vf (%). 2. Calculate the modulus of elasticity along the longitudinal and transverse directions, denoted respectively as E and Et, of a unidirectional of carbon/ polyester, that would have the same amount of fiber volume fraction. The following is given Ef = 230,000 MPa;

Eft = 15,000 MPa (Section 3.3.1, Table 3.3)

Eresin = 4000 MPa (Section 1.6) 3. Starting from the relation in Section 3.5.1 giving the modulus of elasticity of mat (which is assumed to be isotropic in the plane of the plate), deduce from there the value of Emat. Assume that nmat = 0.3. Second part: One polymerizes on each face of the previous plate two plies of preimpregnated carbon/epoxy unidirectionals with Vf = 60%. (see characteristics given in Section 3.3.3). Each ply has a thickness of 0.13 mm. The four plies (two above, two below) are oriented in the same direction denoted as x (or 0∞). The midplane of the laminated plate coincides with axes x and y.

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 451 Monday, November 18, 2002 12:43 PM

1. Write numerically for the unidirectional and for the mat the constitutive relation in the x, y axes in the form: Ï sx ¸ Ï ex Ô Ô Ô Ì sy ˝ = [ E ] Ì ey Ô Ô Ô Ó t xy ˛ Ó g xy

¸ Ô ˝ Ô ˛

2. Calculate in the axes x, y the coefficients of the in-plane constitutive relation of the laminated plate (matrix [A], Section 12.1.1). Deduce from there the moduli of elasticity and the Poisson coefficients of the plate. 3. Calculate in the axes x, y the coefficients for the bending behavior of the laminated plate (matrix [C], Section 12.1.4). Deduce from there the apparent bending moduli along the directions x and y. 4. This laminated plate is submitted to a tensile stress resultant along the x direction denoted as Nx (N/mm). The tensile rupture strength of mat is 100 MPa. Calculate the value of the stress resultant Nx that leads to firstply failure of the laminate. In which component (unidirectional or mat) will this failure occur? This component is supposed to be completely broken (i.e., its mechanical characteristics are reduced to zero). What then is the state of stress in the other component? Make a conclusion.

Solution: First part: 1. Fiber volume fraction of carbon: vol. fibers V f = ---------------------------------total volume If s is the rectangular surface at the base of the mold, the volume of a layer of mat is m s -------ofrf from which, for 21 layers: 21 ¥ s ¥ m of § r f - = 12% V f = -------------------------------------3 s ¥ 3 ¥ 10 2. Moduli of elasticity (see Section 3.3.1): One has E = E f V f + E m V m = 31,120 MPa 1 - = 4386 MPa E t = E m ----------------------Em V m + -----V f E ft

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 452 Monday, November 18, 2002 12:43 PM

3. One has (see Section 3.5.1) 3 5 E mat = --- E + --- E t = 14,410 MPa 8 8 Second part: 1. Constitutive behavior: Unidirectional: Ï e Ô x Ô Ì ey Ô Ô g Ó xy

¸ Ô Ô ˝ = Ô Ô ˛

Ê 1 Á -------------------Á 134,000 Á 0.25 Á – ------------------Á 134,000 Á Á 0 Ë

ˆÏ ˜Ô ˜ ˜Ô 0 ˜Ì ˜Ô 1 ˜˜ Ô -----------4200 ¯ Ó

0.25 – ------------------134,000

0

1 -----------7000

0

s x ¸Ô Ô sy ˝ Ô t xy Ô˛

After inversion: Ï sx ¸ 134,440 Ô Ô = Ì sy ˝ 1756 Ô Ô 0 Ó t xy ˛

1756 7023 0

0 0 4200

Ï ex Ô Ì ey Ô Ó g xy

¸ Ô ˝ Ô ˛

Mat: Ï e Ô x Ô Ì ey Ô Ô g Ó xy

1 ¸ ----------------14,410 Ô Ô 0.3 ˝ = – ---------------14,410 Ô Ô 0 ˛

0.3 – ---------------14,410

0

1 ----------------14,410

0

0

2 ( 1 + 0.3 ) --------------------------14,410

Ï s ¸ Ô x Ô Ô Ô Ì sy ˝ Ô Ô Ô t Ô Ó xy ˛

After inversion: Ï sx ¸ 15,835 Ô Ô = Ì sy ˝ 4750 Ô Ô 0 Ó t xy ˛

4750 15,835 0

0 0 5542

2. Membrane behavior of the laminated plate: n

A ij =

Â

ply n∞1

© 2003 by CRC Press LLC

(k) (k)

E ij e

Ï ex Ô Ì ey Ô Ó g xy

¸ Ô ˝ Ô ˛

TX846_Frame_C18b Page 453 Monday, November 18, 2002 12:43 PM

A11 = 134,440 ¥ 4 ¥ 0.13 + 15,835 ¥ 3 = 117,408 (MPa mm) A22 = 7023 ¥ 4 ¥ 0.13 + 15,835 ¥ 3 = 51,151 (MPa mm) A12 = 1756 ¥ 4 ¥ 0.13 + 4,750 ¥ 3 = 15,163 (MPa mm) A13 = A23 = 0 A33 = 4200 ¥ 4 ¥ 0.13 + 5542 ¥ 3 = 18,810 (MPa mm). From this, and with a total thickness of the plate of h = 3 + 4 ¥ 0.13 = 3.52 mm we have

[A] =

117,408 15,163 0 1 ----------------32,078

h[A ]

–1

0.3 = – ---------------32,078

15,163 51,151 0

0 ; 0 18,810

0.13 – ---------------13,975

0

1 ----------------13,975

0

0

1 -----------5344

0

then for the moduli of elasticity of the plate: E x = 31,078 MPa;

n xy = 0.3;

E y = 13,975 MPa;

G xy = 5344 MPa

n yx = 0.13

3. Bending behavior of the laminated plate: n

C ij =

Â

ply n∞1

© 2003 by CRC Press LLC

3

3

( k ) z k – z k-1ˆ E ij Ê ------------------Ë 3 ¯

TX846_Frame_C18b Page 454 Monday, November 18, 2002 12:43 PM

3

3

3

1.5 1.76 – 1.5 3 C 11 = 134,440 ¥ ---------------------------- ¥ 2 + 15,835 ¥ --------- ¥ 2 = 221,763 MPa ¥ mm 3 3 3

3

3

3

3

3

3

3

3

1.5 1.76 – 1.5 C 22 = 7023 ¥ ---------------------------- ¥ 2 + 15,835 ¥ --------- ¥ 2 = 3 3

45,352 MPa ¥ mm

1.5 1.76 – 1.5 C 12 = 1756 ¥ ---------------------------- ¥ 2 + 4 750 ¥ --------- ¥ 2 = 3 3 C 13 = C 23 = 0

3

13,119 MPa ¥ mm

1.5 1.76 – 1.5 C 33 = 4200 ¥ ---------------------------- ¥ 2 + 5 542 ¥ --------- ¥ 2 = 3 3

18,284 MPa ¥ mm

3

3

from which (see Section 12.1.6):

1 -------------------217,968

[C]

–1

1 = – ------------------753,509

1 – ------------------753,509

0

1 ----------------44,576

0

0

1 ----------------18,284

0

=

1 --------EI 11

1 --------EI 12

0

1 --------EI 21

1 --------EI 22

0

0

0

1 --------EI 33

Apparent bending modulus in the x direction: 1 1 --------- = -----------------3 Æ E fx = 59,972 MPa h EI 11 E fx ¥ ----12 The apparent bending modulus in the y direction: 1 1 --------- = -----------------3 Æ E fy = 12,264 MPa h EI 22 E fy ¥ ----12 4. Rupture: For a stress resultant Nx, the plate is deformed in its plane according to the relation: Ï ex Ô Ì ey Ô Ó g xy

Ï N ¸ ¸ x Ô Ô –1 Ô ˝ = [A] Ì 0 ˝ Ô Ô Ô Ó 0 ˛ ˛ -1

then with the values found for [A] :

ex = 8.856 ¥ 10

© 2003 by CRC Press LLC

-6

¥ Nx; ey = –2.66 ¥ 10

-6

¥ Nx; gxy = 0

TX846_Frame_C18b Page 455 Monday, November 18, 2002 12:43 PM

One then has for the stresses: In the unidirectional layer:

s = sx = 134,440 ex + 1756 ey = 1.183 Nx st = sy = 1756 ex + 7023 ey = –0.003 Nx tt = txy = 0. In the mat layer:

sx = 15,835 ex + 4750 ey = 0.128 Nx sy = 4750 ex + 15,835 ey = 5.5 ¥ 10

-5

¥ Nx

txy = 0 From which the failure criteria are (see Section 14.2.3) In the unidirectional layer: ( 1.183N x ) ( – 0.003N x ) 1.183 ¥ – 0.003N x -------------------------- + ----------------------------- – ------------------------------------------> a made of unidirectional glass/ resin (see figure). It is supported at two opposite sides and is loaded by a constant transverse pressure of qo.

1. Calculate the deflection due to bending at the midline of the plate located at x = a/2 (maximum deflection). 2. Indicate the numerical values of the contributions from the bending moment and from transverse shear using the following: Ex = 40,000 MPa; Gxz = 400 MPa; nxy = 0.3; nyx = 0.075; qo = –1 MPa; a = 150 mm; h = 15 mm. Comment.

Solution: 1. For the cylindrical bending considered, Equation 17.32 allows one to write dQ x ---------- = – q 0 ; dx

dM y ---------- = Q x ; dx

d qy M y = C 11 --------; dx

Elimination of Qx, My and qy leads to 4

q d wo -----------= ------o4 C 11 dx © 2003 by CRC Press LLC

hG xz Ê dw o - ---------- + q yˆ Q x = ----------¯ k x Ë dx

TX846_Frame_C18c Page 494 Monday, November 18, 2002 12:45 PM

then: 3 2 q x4 x x w o = ------o- Ê ------ + A ----- + B ----- + Cx + Dˆ ¯ C 11 Ë 24 6 2

The boundary conditions are written as: x = 0 ¸w = 0; ˝ 0 x=a ˛

2 kx dq d wo - q 0 – -----------M y = 0 fi --------y = ----------= 0 2 dx hG xz dx

After calculation of the constants A, B, C, D, one obtains for the deflection at x = a/2: ¸ 1 a h 2E 4 12 ( 1 – n xy n yx ) Ï 5 - Ì --------- + k x Ê ---ˆ -------x- ----------------------------------- ˝ w 0 Ê ---ˆ = q 0 a ---------------------------------3 Ë 2¯ Ë ¯ G ( – n n ) 384 96 1 a xz xy yx ˛ Ex h Ó The calculation of kx was done in Section 17.7.1 for this type of plate. One has (see Equation 17.34) kx = 6/5 = 1.2 from which: 2 ¸ Ex 1 a 4 12 ( 1 – n xy n yx ) Ï 5 Ê --h-ˆ -------------- ----------------------------------- ˝ + w 0 Ê ---ˆ = q 0 a ---------------------------------Ì 3 Ë a¯ G xz 80 ( 1 – n xy n yx ) Ë 2¯ Ex h Ó 384 ˛

The first term in the brackets represents the contribution from the bending moment, and the second term represents that due to transverse shear. 2. Numerical values: wo(a/2) = –0.5727 mm – 0.5625 mm (moment)

(transverse shear)

wo(a/2) = –1.13525 mm Note that 49.5% of this deflection is due to transverse shear. One can see from the above expression for wo(a/2) that the influence of transverse shear on the bending deflection increases with the value of the relative thickness h/a (here, © 2003 by CRC Press LLC

TX846_Frame_C18c Page 495 Monday, November 18, 2002 12:45 PM

h/a = 1/10 corresponds to a thick plate). One also notes the influence of the ratio 48 Ex /Gxz.

18.3.8 Bending of a Sandwich Plate Problem Statement: A rectangular sandwich plate (a ¥ b) is fixed on side b, and loaded along the opposite side by a constant distributed load fo (N/mm). The two other sides are free (see figure).

The plate consists of two identical orthotropic skins of material 1, and an orthotropic core made of material 2. The orthotropic axes are parallel to the axes x,y,z. 1. Calculate the deflection of the midplane at the extremity x = a of the x axis, assuming cylindrical bending about y axis for the plate. 2. Numerical application: Given fo = –10 N/mm a = b = 1000 mm H1 = 2H2 = 100 mm Material 1: (1) Ex = 40,000 MPa (1) Gxz = 4000 MPa Material 2: (2) Ex = 40 MPa (2) Gxz = 15 MPa For each of the materials nxy = 0.3 nyx = 0.075

48

This example of thick plate in bending constitutes a test case for the evaluation of computer programs using finite elements. For complementary information on this topic, see bibliography, “Computer programs for Composite Structures: Reference examples and Validation.”

© 2003 by CRC Press LLC

TX846_Frame_C18c Page 496 Monday, November 18, 2002 12:45 PM

(a) Calculate the deflection at the extremity x = a and show the contributions from the bending moment and from the transverse shear. (b) Calculate the transverse shear stress txz: On the midplane of the plate. At the interface between the core and the upper skin. At the midthickness of the upper skin.

Solution: 1. In the case of cylindrical bending, Equation 17.32 allows one to write dQ x ---------- = 0; dx

d qy M y = C 11 --------; dx

dM y ---------- = Q x ; dx

· hG xzÒ Ê dw 0 ---------- + q yˆ Q x = ----------------¯ k x Ë dx

Then Qx = fo, and elimination of Qx, My, and qy leads to 3

fo d wo ----------- = -----3 C 11 dx then: 2 fo Ê x3 x w o = – ------ ----- + A ----- + Bx + Cˆ ¯ 2 C 11 Ë 6

The boundary conditions are written as: fo dw – ----------o = 0 x = 0 : w 0 = 0 et q y = 0 fi k x ----------------· hG xzÒ dx 2 dq d wo - = 0 x = a : M y = 0 fi --------y = – ----------2 dx dx

After calculation of the constants A, B, C, one obtains the deflection at x = a: 3

fo a fo a - + k x ----------------w o ( a ) = ---------3C 11 · hG xzÒ with (see Equation 12.16): 3

3

3

➀ H 1 – H 2ˆ ➁H C 11 = E 11 Ê -----------------+ E 11 ------2 Ë 12 ¯ 12

and according to Equation 17.2: ➀

C 11 © 2003 by CRC Press LLC

➁

E x ( H1 – H2 ) + E x H2 = --------------------------------------------------12 ( 1 – n xy n yx ) 3

3

3

TX846_Frame_C18c Page 497 Monday, November 18, 2002 12:45 PM

According to Equation 17.10: ➀

➁

· hG xzÒ = G xz ( H 1 – H 2 ) + G xz H 2 from which one obtains 4 ( 1 – n xy n yx )f o a kx fo a w o ( a ) = --------------------------------------------------+ ----------------------------------------------------➀ 3 3 ➁ 3 ➀ ➁ E x ( H 1 – H 2 ) + E x H 2 G xz ( H 1 – H 2 ) + G xz H 2 3

The calculation of kx was carried out in Section 17.7.2 for this type of plate. It was given by Equation 17.39. 2. Numerical application: (a) Deflection: Equation 17.39 gives kx = 110.8 from which: wo(a) = –1.177 mm + (–5.519 mm) (moment)

(transverse shear)

wo(a) = –6.636 mm Note that 83% of this deflection is due to transverse shear, and this happens in spite of very thick skins. This important influence is due to the very large value compared with unity (110.8) of the transverse shear coefficient and due to the fact that the plate is thick (H1/a = 1/10). (b) Transverse shear stress txz (see Section 17.7.2): Midplane: (z = 0): txz = 0.1286 MPa Interface (z = H2 /2): txz = 0.12855 MPa Midthickness of the upper layer: z = (H1 + H2)/4: txz = 0.075 MPa

18.3.9 Bending Vibration of a Sandwich Beam

49

Problem Statement: Consider a sandwich beam of length and width d simply supported at its ends (see figure). It consists of two identical skins of material 1 (glass/resin) and a core 49

This application constitutes a test case for the validation of computer programs using finite elements, see in the bibiography, “Programs for the calculation of Composite Structures, Reference examples and Validation.”

© 2003 by CRC Press LLC

TX846_Frame_C18c Page 498 Monday, November 18, 2002 12:45 PM

of material 2 (foam). These materials are transversely isotropic in the plane y, z.

The elastic characteristics are denoted as: ➀

➀

➁

➁

E x , G xy , E x , G xy Specific masses are r1 and r2. 1. Write the equation for the resonant frequencies for bending vibration in the plane of symmetry (x, y) of this beam. 2. Numerical application: Given: ➀

Ex

= 40,000 MPa; ➁

Ex

= 40 MPa;

r1 = 2,000 kg/m

➀

G xy = 4,000 MPa; ➁

G xy = 15 MPa;

H1 = 2H2 = 100 mm;

3

r2 = 50 kg/m

= 1000 mm;

3

d = 100 mm

Calculate the first five frequencies in bending vibration.

Solution: 1. Equation for the vibration frequencies: At first one establishes the differential equation for the dynamic displacement n (x, t) starting from the Equation 15.18, noting that for the example considered, the elastic center and the center of gravity of section are the same (decoupling between bending vibration and longitudinal vibrations). 2 ∂ Ty ∂ qz ∂ n ∂M --------- = · r S Ò --------2- ; ---------z + T y = · r I zÒ ---------2 ∂x ∂ x ∂t ∂t 2

· GS Ò ∂ n T y = ------------- Ê ------- – q zˆ ; ¯ k Ë∂ x

∂q M z = · EI zÒ --------z ∂x

Elimination of Ty, Mz, qz between these four relations leads to the equation for n (x, t): 4 4 2 · r I zÒ · r S Ò ∂ 4 n ∂ n · r I zÒ ∂ n · r SÒ ∂ n --------4- – ------------- ( 1 + a ) --------------------------------------------------------- --------- = 0 + + k 2 2 · GSÒ · EI zÒ ∂ t 4 · EI zÒ · EI zÒ ∂ t 2 ∂x ∂x ∂ t

© 2003 by CRC Press LLC

TX846_Frame_C18c Page 499 Monday, November 18, 2002 12:45 PM

with · r SÒ · EI zÒ -¥k a = ------------------------· GSÒ · r I zÒ In assuming that the solution takes the form n (x, t) = no(x) ¥ cos(wt + j) one can rewrite the differential equation that defines the modal deformation vo(x) in the following nondimensional form: 4

2

d no d no 1 ---------- + w 2 ( 1 + a ) ---------- + w 2 Ê a w 2 – -----2ˆ n o = 0 4 2 Ë ¯ dx dx r in which

n · r I zÒ 2 2 · r I zÒ 2 x 2 - w ; r = ----------------2 x = --- ; n o = -----o ; w = ----------- · EI zÒ · r SÒ After writing the characteristic equation, the reduced modal deformation takes the form: v o = AchX 1 x + BshX 1 x + C cos X 2 x + D sin X 2 x

[1]

where: 2

X1

2

X2

2 w (1 + a) 1 2 2 1 – a = + ------------------------ + w w ÊË ------------ˆ¯ + -----2 2 2 r 2

[2]

The boundary conditions corresponding to simply supported ends are written as: x = 0 or : n = 0; or:

∂q M z = · EI zÒ --------z = 0 "t ∂x d n ----------2-o + a w 2 n o = 0 dx 2

x = 0 or 1 : n o = 0;

These four conditions allow one to obtain with [1] a linear and homogeneous system in A,B,C,D. By setting the determinant equal to zero, one obtains an equation for vibrations which reduces to sin X2 = 0 Then the solution can be written as: X2 = np, (n = 1, 2, 3,…) © 2003 by CRC Press LLC

[3]

TX846_Frame_C18c Page 500 Monday, November 18, 2002 12:45 PM

2. With the numerical values indicated in the Problem Statement, one can calculate the shear coefficient k, the literal expression for which has been established in Application 18.3.5. One finds k = 110.8. The frequencies can be written starting from the circular frequencies w1, w2, w3,… extracted from equation [3], where X2 takes the form [2].

w f i = ------i ( H z ) 2p one obtains:

50

f 1 = 64.476 Hz ; f 4 = 265.383 Hz ;

50

f 2 = 131.918 Hz ;

f 3 = 198.734 Hz

f 5 = 331.963 Hz.

One keeps voluntarily the nonsignificant decimal, for the purpose of comparison with values obtained from numerical models.

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 503 Thursday, July 11, 2002 5:42 PM

APPENDIX 1 STRESSES IN THE PLIES OF A LAMINATE OF CARBON/EPOXY LOADED IN ITS PLANE The tables in this appendix give for each ply in the laminate the stresses along the principal orthotropic directions of the ply, denoted as and t. These stresses are denoted as σ , σ t, τ t. The laminate is successively subjected to three cases of simple loading:

σ x = 1 MPa: normal stress along the 0° direction. σ y = 1 MPa: normal stress along the 90° direction. τ xy = 1 MPa: shear stress.

CHARACTERISTICS OF EACH PLY Vf = 60% fiber volume fraction. Thickness of each ply: 0.13 mm. Moduli: Modulus along the fiber direction: E = 134,000 MPa. Modulus along the transverse direction: Et = 7000 MPa. Shear modulus: Gt = 4200 MPa. Poisson coefficient: νt = 0.25. Fracture strength: Tension along the longitudinal direction: σ rupture = 1270 MPa. Compression along the longitudinal direction: σ rupture = 1130 MPa. Tension along the transverse direction: σ t rupture = 42 MPa. Compression along the transverse direction: σ t rupture = 141 MPa. Shear strength: τ t rupture = 63 MPa.

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 504 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 505 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 506 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 507 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 508 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 509 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 510 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 511 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 512 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 513 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 514 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 515 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 517 Thursday, July 11, 2002 5:42 PM

APPENDIX 2 BUCKLING OF ORTHOTROPIC STRUCTURES The problems related to the stability of orthotropic plates and shells are not treated in this book. However, we give in the following a few figures that allow one to estimate the order of magnitude of loads that can lead to buckling due to compression or due to shear in orthotropic panels and tubes.

Rectangular Panels 1

The following plates allow one to calculate the critical stress resultants in compression and in shear for different support conditions.

1

See Sections 5.2.4 or 12.1.1. for the definition of the stress resultants. See relations [12.16] for the definition of the constants C11, C22, C12, C33 that appear in the plates.

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 518 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 519 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 520 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 521 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 522 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 523 Thursday, July 11, 2002 5:42 PM

Buckling of Orthotropic Tubes Buckling in bending creating ovalization of the tube: Bending leads to ovalisation of the cross section. The moment of inertia which affects the rigidity in bending decreases (this is the unstable process). The phenomenon is known as the “Brazier effect.”

2 2 2 Ex × Ey M critical = ---------- π r 0 e ---------------------1 – v xy v yx 9 bending © 2003 by CRC Press LLC

1/2

TX846_Frame_Appendix Page 524 Thursday, July 11, 2002 5:42 PM

Buckling due to external pressure: The notations in the above figure are kept. L is the length of the tube or the container that is subject to buckling. p critical

Ey E 1/4 r e 5/2 - × -----x × ----0 × ---- = 0.83 × ----------------------------1 – 0.1E x /E y E y L r 0

Buckling due to torsion:

The critical stress resultant in torsion is given by:

π e T xy = ----- -------3 2 12 critical r0 L 2

9

1/4

3

5

Ex Ey -5 × -----------------------------( 1 – ν xy ν yx )

1/8

Buckling due to axial compression: This aspect is not considered here, because the occurrence of elastic instability is strongly influenced by the presence of geometric imperfections in the orthotropic cylinder

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 525 Thursday, July 11, 2002 5:42 PM

BIBLIOGRAPHY Les matériaux composites, J. Weiss, C. Bord, Vol. 1 and 2, Publications of the Ministry of Industry and Research of Centre d’Études Techniques des Industries Mécanique. Les matériaux composites. G. Hellard, P. Lafon, Conference, Dec. 1984. Manufacturer’s documentation. Vetrotex—Saint Gobain, skis Dynastar, Ciba Geigy. Calcul des structures en matériaux composites. J.J. Barrau, S. Laroze, Eyrolles-Masson, Paris 1987. Calcul des structures en matériaux composites, F. Joubert, R. Harry, Mechanical Engineering Laboratory—I.U.T. « A »/C.O.D.E.M.A.C., Bordeaux 1985. Matériaux composites pour structures d’aeronefs, J. Rouchon, École Nationale Supérieure d’Ingénieurs de construction Aéronautiques, Toulouse, 1980. Les applications des composites dans le domaine aéronautique, G. Hellard, G. Hilaire, M. Tores, Aerospatiale publication. Fabrication des avions et missiles, M.P. Guibert, Dunod, Paris, 1960. Techniques de l’Ingénieur—Plastiques—A.3250—K. Gamski. Fibres de verre, d’aramide et de carbone, des renforts sur mesure pour composites, R. Kleinholz, G. Molinier, Vetrotex journal, No. 59, 1986. Résistance des constructions—matériaux composites—G. Hellard, École Nationale Supérieure d’Ingénieurs de Construction Aéronautiques, Toulouse, 1983. Initiation aux matériaux composites et à leurs techniques de fabrication— Avions Marcel Dassault—Bréguet Aviation—Edition No. 1, Toulouse. Manuel de techniques de collage, G. Fauner, W. Hendlich, eds. Soproge S.A., Paris, 1984. Recherches sur la théorie des assemblages collés, O. Volkersen—La Construction Métallique, No. 4, 1965. L’Aéronautique et L’Astronautique, No. 107, 4, 1984. Matériaux et structures composites ou l’adaptation aux besoins, P. Lamicq, 7th French Congress in Mechanics, Bordeaux, 1985. Publication of specialized press : Air et Cosmos; Aviation magazine; “ça m’intéresse;” Science et vie; Dassault-Bréguet Information; Aérospatiale Information; Vétrotex actualités; Aspects des résines Ciba Geigy; Interavia Revue Aérospatiale. Introduction aux matériaux composites, R. Naslain, Vol. 2, Matrices métalliques et céramiques, Ed. of C.N.R.S. and of Institute of Composite Materials.

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 526 Thursday, July 11, 2002 5:42 PM

Matériaux composites à matrice organique, G. Chrétien, Technique et documentation Lavoisier, Paris, 1986. Guide pratique des matériaux composites, M. Geier, D. Duedal, Technique et documentation Lavoisier, Paris 1985. La flexion—torsion dynamique des poutres composites, M. Carrier, J.M. Cieaux, Université Toulouse III—I.U.T. “A,” 1987. Proceedings of the 4th Journées Nationales sur les composites, Ed., Pluralis, Paris, 1984. Proceedings of the 5th Journées Nationales sur les composites, C. Bathias, D. Menkes, A.M.A.C., Ed. Pluralis, Paris, 1986. Transverse shear deformation in bending of composite beams of any cross section shapes, D. Gay, Mechanics of structured media, Part B : pp. 155– 171, Elsevier Scientific Publishing Company, 1981. Homogèneisation en torsion d’une poutre composite, J.J. Barrau, O. Chambard, M. Nuc, D. Gay-Tendances actuelles en calcul des structures, Bastia 1985. Les système ressorts-composites, L. De Goncourt, K.H. Sayers, Composites, No. 3, May/June 1988, pp. 145–150. Composites de grande diffusion, A. Jardon, M. Costes, European conference on Composite Materials, London, July 1987. Conception des véhicles spatiaux, D. Marty, Masson Ed., Paris, 1986. Effets des microfissures de résine sur les propriétés des composites aéronautiques en kevlar/époxyde-F. Turris, H.Y. Loken, R.F. Pinzelli, Composites No. 2, March/April 1988, pp. 35–40. Conduits PVDF renforcés. Contraintes thermiques et mécanismes de rupture, B. Échalier, P. Bleut, F. Lefebvre, C. Tournut, Composites, No. 3, May/ June 1987, pp. 183–188. Structure coques—Équations générales et stabilité, J. Barbe, E.N.S.A.E., 1983. Comment utiliser au meilleur coût les matériaux composites. M. Reyne, Ed. de l’Usine Nouvelle, Paris, 1986. Fibres de carbone revêtues de nickel, E.D. Kaufman, Composites No. 3, May/June 1988. FRANCE—COMPOSITES. French suppliers for the fabrication of organic composites, CEPP, 25 Rue Dagorno, 75012 Paris. Matériaux composites—Teknea, Marseille, 1989. Manuel de calcul des composites verre/résine, Manera, Massot, Morel, Verchery, Pluralis, 1988. Phénomènes interfaciaux dans les composites à matrice thermoplastique: Application au FIT, M. Guigon, A. Kloster, Annales des composites 1989, 1–2, pp. 83–90. Développement d’une nouvelle technologie pour fabriquer des poteaux, E. Pfletschinger-Composites No. 3, May/June 1987, pp. 67–72. Conception et dimensionnement du volet extérieur en fibres de carbone du CN 235, J.L. Duquesne, M. Gonzales, ENSICA, June 1990. Les plastiques, M. Reyne, Ed. Hermès, Paris, 1990. Impact and Residual Fatigue Behavior of ARALL, W.S. Johnson, Advances in Composites Materials and Structures, ASME-AMD, Vol. 82, 1989. © 2003 by CRC Press LLC

TX846_Frame_Appendix Page 527 Thursday, July 11, 2002 5:42 PM

Elastic Analysis and Engineering Design formulae for bonded joints—D.A. Bigwood, A.D. Grocombe, International Journal of Adhesion and Adhesive, Vol. 9, No. 4, Oct. 1989, pp. 229–242. Conception et essais de tubes composites hautes performances, P. Odru, C. Sparks, J. Schmitt, J.F. Puch, Matériaux-Mécanique-Électricité, No. 433, Feb/Mar 1990, pp. 4–6. Metal laminates—A family of Advanced Materials, M.L. Verbruggen, J.W. Gunnik, Plastics/Metals/Ceramics, SAMPE European chapter, Bâle, May 1990, pp. 455–465. General buckling curves for specially orthotropic rectangular plates, E.J. Brunnelle, G.A. Oyibo, AIAA Journal, Vol. 21, No. 8, Aug. 1983, pp. 1150– 1154. Technologie des composites, M. Reyne, Ed. Hermès, Paris, 1990. Interaction effects in fibre composites, V.R. Riley, Polymer Conference Series, University of Utah, June 1970. Progiciels de calcul de structures composites; Exemples de réference et de validation, Coordonnateur G. Matheron, ed. Hermès, Paris, 1995. Isotropie de Rigidité et quasi-isotropie de résistance des stratifiés à orientation périodiques, D. Gay, F. Joubert, Revue des composites et des matériaux avancés, Vol. 4, No. 2, 1994, pp. 241–261. Les composites, M. Reyne, Presses Universitaires de France, Paris, 1995.

© 2003 by CRC Press LLC

© 2003 by CRC Press LLC

COMPOSITE MATERIALS DESIGN AND APPLICATIONS

Daniel Gay Suong V. Hoa Stephen W. Tsai

CRC PR E S S Boca Raton London New York Washington, D.C.

© 2003 by CRC Press LLC

TX846 disclaimer Page iv Friday, November 8, 2002 8:38 AM

Library of Congress Cataloging-in-Publication Data Gay, Daniel, 1942[Matériaux composites. English] Composite materials / by Daniel Gay ; translated by Suong V. Hoa, Stephen W. Tsai. p. cm. Translation of: Matériaux composites. 4th ed. Includes bibliographical references and index. ISBN 1-58716-084-6 (alk. paper) 1. Composite materials. I. Title. TA418.9.C6 G39 2002 620.1′18—dc21

2002073794 CIP

This book contains information obtained from authentic and highly regarded sources. Reprinted material is quoted with permission, and sources are indicated. A wide variety of references are listed. Reasonable efforts have been made to publish reliable data and information, but the author and the publisher cannot assume responsibility for the validity of all materials or for the consequences of their use. Neither this book nor any part may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopying, microÞlming, and recording, or by any information storage or retrieval system, without prior permission in writing from the publisher. The consent of CRC Press LLC does not extend to copying for general distribution, for promotion, for creating new works, or for resale. SpeciÞc permission must be obtained in writing from CRC Press LLC for such copying. Direct all inquiries to CRC Press LLC, 2000 N.W. Corporate Blvd., Boca Raton, Florida 33431. Trademark Notice: Product or corporate names may be trademarks or registered trademarks, and are used only for identiÞcation and explanation, without intent to infringe.

Visit the CRC Press Web site at www.crcpress.com © 2003 by CRC Press LLC French editions published by Editions Hermès, Paris, 1997 No claim to original U.S. Government works International Standard Book Number 1-58716-084-6 Library of Congress Card Number 2002073794 Printed in the United States of America 1 2 3 4 5 6 7 8 9 0 Printed on acid-free paper

© 2003 by CRC Press LLC

TX846_Frame_FM Page v Thursday, July 11, 2002 5:38 PM

PREFACE The economic importance of composite materials is now well known. There are strong indications everywhere that this importance will be increasing in the future. Composite materials now occupy an established position in the aerospace industry. They are also used for many components in the automotive industry and civil infrastructures now have their reinforcements made of composite materials. There is a large range of manufacturing processes for the production of low-cost composites. There is a need by engineers working in composites for a practical source of reference for the design and application of composites. This book fills that need. In the educational sector, composite materials now are taught at many universities around the world. Usually the topic covered is laminate theory. Composites Design courses also exist in a few universities and institutes. The demand from students and also practitioners of composites for knowledge and training in design of composites is increasing. However a good design book has not been available. The content of these design courses concentrates mostly on analysis while applications still remain at the specimen level. This book, initially written by Daniel Gay in French, has been distributed widely in France and in French speaking countries. The authors are of the opinion that having the book in the English language would facilitate the training and dissemination of knowledge to the regions where composites are used the most. The book has been translated to English with modifications and updates. The book consists of four main parts, with increasing levels of complexity. Each part can be studied independently from the other parts. The first part presents an introduction to composite materials, the fabrication processes, the properties of a single ply, sandwich materials, conceptual design, assembly, and applications of composites in the aerospace and other areas. This part can be used by itself to form a part of a course on advanced materials and associated designs. The second part presents the mechanics of composite materials. This consists of discussion on elastic anisotropic properties, the directional dependence of different properties, and mechanical properties of thin laminates. This part can be used by itself to teach students and engineers on the mechanics of composite materials. The third part presents the orthotropic coefficients that may be conveniently used for design. The Hill–Tsai failure criterion, bending of composite beams, torsion of composite beams, and bending of thick composite plates. This part requires knowledge of strength of materials. Information presented here is more theoretical than in preceding parts. Its main objective is to contribute to a better interpretation of the behavior of composite components.

© 2003 by CRC Press LLC

TX846_Frame_FM Page vi Thursday, July 11, 2002 5:38 PM

The fourth part provides numerous (41) numerical examples on the use and design of composites. There are three levels of examples. Level 1 deals with the determination of mechanical properties of composite structures in different forms such as plates, tubes, or composite components made using different processes such as hand-lay-up or filament winding. Level 2 deals with thermoelastic properties of different laminates. Failure analysis is also carried out. Level 3 deals with bonding of cylinders made of composites, buckling of composite sandwich beams, flexural shear in sandwich beams, vibrations of composite This volume can be used to teach students at the first year graduate level as well as the final year undergraduate level. It is also useful for practical engineers who want to learn, on the job, the guidelines for the use of composites in their applications. The authors hope that this volume can make significant contribution to the training of future engineers who utilize composites. Suong V. Hoa Montreal, Quebec, Canada Daniel Gay Toulouse, France Stephen Tsai Stanford, California July 2002

© 2003 by CRC Press LLC

TX846_Frame_FM Page vii Thursday, July 11, 2002 5:38 PM

CONTENTS PART I: PRINCIPLES OF CONSTRUCTION 1

Composite Materials, Interest, and Properties 1.1 What Is Composite Material? 1.2 Fibers and Matrix 1.2.1 Fibers 1.2.2 Matrix Materials 1.3 What Can Be Made Using Composite Materials? 1.4 Typical Examples of Interest on the Use of Composite Materials 1.5 Examples on Replacing Conventional Solutions with Composites 1.6 Principal Physical Properties

2

Fabrication Processes 2.1 Molding Processes 2.1.1 Contact Molding 2.1.2 Compression Molding 2.1.3 Molding with Vacuum 2.1.4 Resin Injection Molding 2.1.5 Molding by Injection of Premixed 2.1.6 Molding by Foam Injection 2.1.7 Molding of Components of Revolution 2.2 Other Forming Processes 2.2.1 Sheet Forming 2.2.2 Profile Forming 2.2.3 Stamp Forming 2.2.4 Preforming by Three-Dimensional Assembly 2.2.5 Cutting of Fabric and Trimming of Laminates 2.3 Practical Hints on Manufacturing Processes 2.3.1 Acronyms 2.3.2 Cost Comparison

3

Ply Properties 3.1 Isotropy and Anisotropy 3.1.1 Isotropic Materials 3.1.2 Anisotropic Material 3.2 Characteristics of the Reinforcement–Matrix Mixture 3.2.1 Fiber Mass Fraction 3.2.2 Fiber Volume Fraction 3.2.3 Mass Density of a Ply 3.2.4 Ply Thickness

© 2003 by CRC Press LLC

TX846_Frame_FM Page viii Thursday, July 11, 2002 5:38 PM

3.3 Unidirectional Ply 3.3.1 Elastic Modulus 3.3.2 Ultimate Strength of a Ply 3.3.3 Examples 3.3.4 Examples of “High Performance” Unidirectional Plies 3.4 Woven Fabrics 3.4.1 Forms of Woven Fabric 3.4.2 Elastic Modulus of Fabric Layer 3.4.3 Examples of Balanced Fabrics/Epoxy 3.5 Mats and Reinforced Matrices 3.5.1 Mats 3.5.2 Summary Example of Glass/Epoxy Layers 3.5.3 Spherical Fillers 3.5.4 Other Reinforcements 3.6 Multidimensional Fabrics 3.7 Metal Matrix Composites 3.8 Tests

4

Sandwich Structures 4.1 What Is a Sandwich Structure? 4.2 Simplified Flexure 4.2.1 Stresses 4.2.2 Displacements 4.3 A Few Special Aspects 4.3.1 Comparison of Mass Based on Equivalent Flexural Rigidity (EI) 4.3.2 Buckling of Sandwich Structures 4.3.3 Other Types of Damage 4.4 Fabrication and Design Problems 4.4.1 Honeycomb: An Example of Core Material 4.4.2 Processing Aspects 4.4.3 Insertion of Attachment Pieces 4.4.4 Repair of Laminated Facings 4.5 Nondestructive Quality Control

5

Conception and Design 5.1 Design of a Composite Piece 5.1.1 Guidelines for Values for Predesign 5.2 The Laminate 5.2.1 Unidirectional Layers and Fabrics 5.2.2 Importance of Ply Orientation 5.2.3 Code to Represent a Laminate 5.2.4 Arrangement of Plies 5.3 Failure of Laminates 5.3.1 Damages 5.3.2 Most Frequently Used Criterion: Hill–Tsai Failure Criterion 5.4 Sizing of the Laminate 5.4.1 Modulus of Elasticity. Deformation of a Laminate 5.4.2 Case of Simple Loading 5.4.3 Case of Complex Loading—Approximate Orientation Distribution of a Laminate 5.4.4 Case of Complex Loading: Optimum Composition of a Laminate 5.4.5 Practical Remarks: Particularities of the Behavior of Laminates

© 2003 by CRC Press LLC

TX846_Frame_FM Page ix Thursday, July 11, 2002 5:38 PM

6

Joining and Assembly 6.1 Riveting and Bolting 6.1.1 Principal Modes of Failure in Bolted Joints for Composite Materials 6.1.2 Recommended Values 6.1.3 Riveting 6.1.4 Bolting 6.2 Bonding 6.2.1 Adhesives Used 6.2.2 Geometry of the Bonded Joints 6.2.3 Sizing of Bonded Surfaces 6.2.4 Examples of Bonding 6.3 Inserts

7

Composite Materials and Aerospace Construction 7.1 Aircraft 7.1.1 Composite Components in Aircraft 7.1.2 Characteristics of Composites 7.1.3 A Few Remarks 7.1.4 Specific Aspects of Structural Resistance 7.1.5 Large Carriers 7.1.6 Regional Jets 7.1.7 Light Aircraft 7.1.8 Fighter Aircraft 7.1.9 Architecture of Composite Parts in Aircraft 7.1.10 Elements of Braking 7.1.11 The Future 7.2 Helicopters 7.2.1 The Situation 7.2.2 Composite Zones 7.2.3 Blades 7.2.4 Yoke Rotor 7.2.5 Other Composite Working Components 7.3 Propeller Blades for Airplanes 7.4 Turbine Blades in Composites 7.5 Space Applications 7.5.1 Satellites 7.5.2 Pressure Vessels 7.5.3 Nozzles 7.5.4 Other Composite Components

8

Composite Materials for Other Applications 8.1 Composite Materials and the Manufacturing of Automobiles 8.1.1 Introduction 8.1.2 Evaluation and Evolution 8.1.3 Research and Development 8.2 Composites in Naval Construction 8.2.1 Competition 8.2.2 Ships 8.3 Sports and Recreation 8.3.1 Skis 8.3.2 Bicycles

© 2003 by CRC Press LLC

TX846_Frame_FM Page x Thursday, July 11, 2002 5:38 PM

8.4 Other 8.4.1 8.4.2 8.4.3 8.4.4 8.4.5 8.4.6

Applications Wind Turbines Compressed Gas Bottles Buggy Chassis Tubes for Off-Shore Installations Biomechanics Applications Telepherique Cabin

PART II: MECHANICAL BEHAVIOR OF LAMINATED MATERIALS 9

Anisotropic Elastic Media 9.1 Review of Notations 9.1.1 Continuum Mechanics 9.1.2 Number of Distinct ϕijk Terms 9.2 Orthotropic Materials 9.3 Transversely Isotropic Materials

10

Elastic Constants of Unidirectional Composites 10.1 10.2 10.3 10.4 10.5

11

Longitudinal Modulus E Poisson Coefficient Transverse Modulus Et Shear Modulus Gt Thermoelastic Properties 10.5.1 Isotropic Material: Recall 10.5.2 Case of Unidirectional Composite 10.5.3 Thermomechanical Behavior of a Unidirectional Layer

Elastic Constants of a Ply Along an Arbitrary Direction 11.1 Compliance Coefficients 11.2 Stiffness Coefficients 11.3 Case of Thermomechanical Loading 11.3.1 Compliance Coefficients 11.3.2 Stiffness Coefficients

12

Mechanical Behavior of Thin Laminated Plates 12.1 Laminate with Midplane Symmetry 12.1.1 Membrane Behavior 12.1.2 Apparent Moduli of the Laminate 12.1.3 Consequence: Practical Determination of a Laminate Subject to Membrane Loading 12.1.4 Flexure Behavior 12.1.5 Consequence: Practical Determination for a Laminate Subject to Flexure 12.1.6 Simplified Calculation for Flexure 12.1.7 Case of Thermomechanical Loading 12.2 Laminate without Midplane Symmetry 12.2.1 Coupled Membrane–Flexure Behavior 12.2.2 Case of Thermomechanical Loading

PART III: JUSTIFICATIONS, COMPOSITE BEAMS, AND THICK PLATES 13

Elastic Coefficients 13.1 Elastic Coefficients in an Orthotropic Material 13.2 Elastic Coefficients for a Transversely Isotropic Material 13.2.1 Rotation about an Orthotropic Transverse Axis 13.3 Case of a Ply

© 2003 by CRC Press LLC

TX846_Frame_FM Page xi Thursday, July 11, 2002 5:38 PM

14

The Hill–Tsai Failure Criterion 14.1 Isotropic Material: Von Mises Criterion 14.2 Orthotropic Material: Hill–Tsai Criterion 14.2.1 Preliminary Remarks 14.2.2 Case of a Transversely Isotropic Material 14.2.3 Case of a Unidirectional Ply Under In-Plane Loading 14.3 Variation of Resistance of a Unidirectional Ply with Respect to the Direction of Loading 14.3.1 Tension and Compression Resistance 14.3.2 Shear Strength

15

Composite Beams in Flexure 15.1 Flexure of Symmetric Beams with Isotropic Phases 15.1.1 Degrees of Freedom 15.1.2 Perfect Bonding between the Phases 15.1.3 Equilibrium Relations 15.1.4 Constitutive Relations 15.1.5 Technical Formulation 15.1.6 Energy Interpretation 15.1.7 Extension to the Dynamic Case 15.2 Case of Any Cross Section (Asymmetric)

16

Composite Beams in Torsion 16.1 Uniform Torsion 16.1.1 Torsional Degree of Freedom 16.1.2 Constitutive Relation 16.1.3 Determination of the Function Φ( y, z) 16.1.4 Energy Interpretation 16.2 Location of the Torsion Center

17

Flexure of Thick Composite Plates 17.1 Preliminary Remarks 17.1.1 Transverse Normal Stress σz 17.1.2 Transverse Shear Stresses τxz and τyz 17.1.3 Hypotheses 17.2 Displacement Field 17.3 Strains 17.4 Constitutive Relations 17.4.1 Membrane Equations 17.4.2 Bending Behavior 17.4.3 Transverse Shear Equation 17.5 Equilibrium Equations 17.5.1 Transverse Equilibrium 17.5.2 Equilibrium in Bending 17.6 Technical Formulation for Bending 17.6.1 Plane Stresses Due to Bending 17.6.2 Transverse Shear Stresses in Bending 17.6.3 Characterization of the Bending, Warping Increments ηx and ηy 17.6.4 Warping Functions 17.6.5 Consequences 17.6.6 Interpretation in Terms of Energy 17.7 Examples 17.7.1 Homogeneous Orthotropic Plate 17.7.2 Sandwich Plate

© 2003 by CRC Press LLC

TX846_Frame_FM Page xii Thursday, July 11, 2002 5:38 PM

PART IV: APPLICATIONS 18

Applications 18.1 Level 1 18.1.1 18.1.2 18.1.3 18.1.4 18.1.5 18.1.6 18.1.7 18.1.8 18.1.9 18.1.10 18.1.11 18.1.12 18.1.13 18.1.14 18.1.15 18.2 Level 2 18.2.1 18.2.2 18.2.3 18.2.4 18.2.5 18.2.6 18.2.7 18.2.8 18.2.9 18.2.10 18.2.11 18.2.12 18.2.13 18.2.14 18.2.15 18.2.16 18.2.17 18.3 Level 3 18.3.1 18.3.2 18.3.3 18.3.4 18.3.5 18.3.6 18.3.7 18.3.8 18.3.9

© 2003 by CRC Press LLC

Simply Supported Sandwich Beam Poisson Coefficient of a Unidirectional Layer Helicopter Blade Transmission Shaft for Trucks Flywheel in Carbon/Epoxy Wing Tip Made of Carbon/Epoxy Carbon Fiber Coated with Nickel Tube Made of Glass/Epoxy under Pressure Filament Wound Vessel, Winding Angle Filament Wound Reservoir, Taking the Heads into Account Determination of the Volume Fraction of Fibers by Pyrolysis Lever Arm Made of Carbon/PEEK Unidirectional and Short Fibers Telegraphic Mast in Glass/Resin Unidirectional Ply of HR Carbon Manipulator Arm of Space Shuttle Sandwich Beam: Simplified Calculation of the Shear Coefficient Procedure for Calculation of a Laminate Kevlar/Epoxy Laminates: Evolution of Stiffness Depending on the Direction of the Load Residual Thermal Stresses due to Curing of the Laminate Thermoelastic Behavior of a Tube Made of Filament-Wound Glass/Polyester Polymeric Tube Loaded by Thermal Load and Creep First Ply Fracture of a Laminate—Ultimate Rupture Optimum Laminate for Isotropic Stress State Laminate Made of Identical Layers of Balanced Fabric Wing Spar in Carbon/Epoxy Determination of the Elastic Characteristics of a Carbon/Epoxy Unidirectional Layer from Tensile Test Sailboat Shell in Glass/Polyester Determination of the In-Plane Shear Modulus of a Balanced Fabric Ply Quasi-Isotropic Laminate Orthotropic Plate in Pure Torsion Plate Made by Resin Transfer Molding (R.T.M.) Thermoelastic Behavior of a Balanced Fabric Ply Cylindrical Bonding Double Bonded Joint Composite Beam with Two Layers Buckling of a Sandwich Beam Shear Due to Bending in a Sandwich Beam Column Made of Stretched Polymer Cylindrical Bending of a Thick Orthotropic Plate under Uniform Loading Bending of a Sandwich Plate Bending Vibration of a Sandwich Beam

TX846_Frame_FM Page xiii Thursday, July 11, 2002 5:38 PM

APPENDICES, BIBLIOGRAPHY, AND INDEX Appendix 1 Stresses in the Plies of a Laminate of Carbon/Epoxy Loaded in Its Plane Characteristics of Each Ply

Appendix 2 Buckling of Orthotropic Structures Rectangular Panels Buckling of Orthotropic Tubes

Bibliography

© 2003 by CRC Press LLC

TX846_Frame_C01 Page 1 Monday, November 18, 2002 10:34 AM

PART I PRINCIPLES OF CONSTRUCTION

© 2003 by CRC Press LLC

TX846_Frame_C01 Page 3 Monday, November 18, 2002 10:34 AM

1 COMPOSITE MATERIALS, INTEREST, AND PROPERTIES 1.1 WHAT IS COMPOSITE MATERIAL? As the term indicates, composite material reveals a material that is different from common heterogeneous materials. Currently composite materials refers to materials having strong fibers—continuous or noncontinuous—surrounded by a weaker matrix material. The matrix serves to distribute the fibers and also to transmit the load to the fibers. Notes: Composite materials are not new. They have been used since antiquity. Wood and cob have been everyday composites. Composites have also been used to optimize the performance of some conventional weapons. For example: In the Mongolian arcs, the compressed parts are made of corn, and the stretched parts are made of wood and cow tendons glued together. Japanese swords or sabers have their blades made of steel and soft iron: the steel part is stratified like a sheet of paste, with orientation of defects 1 and impurities in the long direction (see Figure 1.1), then formed into a U shape into which the soft iron is placed. The sword then has good resistance for flexure and impact. One can see in this period the beginning of the distinction between the common composites used universally and the high performance composites. The composite material as obtained is Very heterogeneous. Very “anisotropic.” This notion of “anisotropy” will be illustrated later in Section 3.1 and also in Chapter 9. Simply put this means that the mechanical properties of the material depend on the direction.

1

15

In folding a sheet of steel over itself 15 times, one obtains 2

© 2003 by CRC Press LLC

= 32,768 layers.

TX846_Frame_C01 Page 4 Monday, November 18, 2002 10:34 AM

Figure 1.1 Effect of the Orientation of Impurities

1.2 FIBERS AND MATRIX The bonding between fibers and matrix is created during the manufacturing phase of the composite material. This has fundamental influence on the mechanical properties of the composite material.

1.2.1 Fibers Fibers consist of thousands of filaments, each filament having a diameter of between 5 and 15 micrometers, allowing them to be producible using textile 2 machines; for example, in the case of glass fiber, one can obtain two semiproducts as shown in Figure 1.2. These fibers are sold in the following forms: Short fibers, with lengths of a few centimeters or fractions of millimeters are felts, mats, and short fibers used in injection molding. Long fibers, which are cut during time of fabrication of the composite material, are used as is or woven. Principal fiber materials are

Glass Aramid or Kevlar‚ (very light) Carbon (high modulus or high strength) Boron (high modulus or high strength) Silicon carbide (high temperature resistant)

In forming fiber reinforcement, the assembly of fibers to make fiber forms for the fabrication of composite material can take the following forms:

2

One wants to have fibers as thin as possible because their rupture strength decreases as their diameter increases, and very small fiber diameters allow for effective radius of curvature in fiber bending to be on the order of half a millimeter. However, exception is made for boron fibers (diameter in the order of 100 microns), which are formed around a tungsten filament (diameter = 12 microns). Their minimum radius of curvature is 4 mm. Then, except for particular cases, weaving is not possible.

© 2003 by CRC Press LLC

TX846_Frame_C01 Page 5 Monday, November 18, 2002 10:34 AM

Figure 1.2 Different Fiber Forms

Unidimensional: unidirectional tows, yarns, or tapes Bidimensional: woven or nonwoven fabrics (felts or mats) Tridimensional: fabrics (sometimes called multidimensional fabrics) with fibers oriented along many directions (>2) Before the formation of the reinforcements, the fibers are subjected to a surface treatment to Decrease the abrasion action of fibers when passing through the forming machines. Improve the adhesion with the matrix material. Other types of reinforcements, full or empty spheres (microspheres) or powders (see Section 3.5.3), are also used.

1.2.1.1 Relative Importance of Different Fibers in Applications Figure 1.3 allows one to judge the relative importance in terms of the amount of fibers used in the fabrication of composites. One can immediately notice the industrial importance of fiber glass (produced in large quantities). Carbon and Kevlar fibers are reserved for high performance components. Following are a few notes on the fibers: Glass fiber: The filaments are obtained by pulling the glass (silicon + sodium carbonate and calcium carbonate; T > 1000∞C) through the small orifices of a plate made of platinum alloy. Kevlar fiber: This is an aramid fiber, yellowish color, made by DuPont de Nemours (USA). These are aromatic polyamides obtained by synthesis at -10∞C, then fibrillated and drawn to obtain high modulus of elasticity. Carbon fiber: Filaments of polyacrylonitrile or pitch (obtained from residues of the petroleum products) are oxidized at high temperatures (300∞C), then heated further to 1500∞C in a nitrogen atmosphere. Then only the hexagonal © 2003 by CRC Press LLC

TX846_Frame_C01 Page 6 Monday, November 18, 2002 10:34 AM

Figure 1.3 Relative Sale Volume of Different Fibers

Figure 1.4 Structure of Carbon Fiber

carbon chains, as shown in Figure 1.4, remain. Black and bright filaments are obtained. High modulus of elasticity is obtained by drawing at high temperature. Boron fiber: Tungsten filament (diameter 12 mm) serves to catalyze the reaction between boron chloride and hydrogen at 1200∞C. The boron fibers obtained have a diameter of about 100 mm (the growth speed is about 1 micron per second). Silicon carbide: The principle of fabrication is analogous to that of boron fiber: chemical vapor deposition (1200∞C) of methyl trichlorosilane mixed with hydrogen. The principal physical–mechanical properties of the fibers are indicated in Table 1.3. Note the very significant disparity of the prices per unit weight. © 2003 by CRC Press LLC

TX846_Frame_C01 Page 7 Monday, November 18, 2002 10:34 AM

1.2.2 Matrix Materials The matrix materials include the following: Polymeric matrix: thermoplastic resins (polypropylene, polyphenylene sulfone, polyamide, polyetheretherketone, etc.) and thermoset resins (polyesters, phenolics, melamines, silicones, polyurethanes, epoxies). Their principal physical properties are indicated in the Table 1.4. Mineral matrix: silicon carbide, carbon. They can be used at high temperatures (see Sections 2.2.4, 3.6, 7.1.10, 7.5). Metallic matrix: aluminum alloys, titanium alloys, oriented eutectics.

1.3 WHAT CAN BE MADE USING COMPOSITE MATERIALS? The range of applications is very large. A few examples are shown below. Electrical, Electronics Insulation for electrical construction Supports for circuit breakers Supports for printed circuits Armors, boxes, covers Antennas, radomes Tops of television towers Cable tracks Windmills Buildings and Public Works Housing cells Chimneys Concrete molds Various covers (domes, windows, etc.) Swimming pools Facade panels Profiles Partitions, doors, furniture, bathrooms Road Transports Body components Complete body Wheels, shields, radiator grills, Transmission shafts Suspension springs Bottles for compressed petroleum gas Chassis Suspension arms Casings Cabins, seats Highway tankers, isothermal trucks Trailers © 2003 by CRC Press LLC

TX846_Frame_C01 Page 8 Monday, November 18, 2002 10:34 AM

Rail transports: Fronts of power units Wagons Doors, seats, interior panels Ventilation housings Marine Transports: Hovercrafts Rescue crafts Patrol boats Trawlers Landing gears Anti-mine ships Racing boats Pleasure boats Canoes Cable transports: Telepherique cabins Telecabins Air transports All composite passenger aircrafts All composite gliders Many aircraft components: radomes, leading edges, ailerons, vertical stabilizers Helicopter blades, propellers Transmission shafts Aircraft brake discs Space Transports Rocket boosters Reservoirs Nozzles Shields for atmosphere reentrance General mechanical applications Gears Bearings Housings, casings Jack body Robot arms Fly wheels Weaving machine rods Pipes Components of drawing table Compressed gas bottles Tubes for offshore platforms Pneumatics for radial frames Sports and Recreation Tennis and squash rackets Fishing poles Skis © 2003 by CRC Press LLC

TX846_Frame_C01 Page 9 Monday, November 18, 2002 10:34 AM

Poles used in jumping Sails Surf boards, Roller skates Bows and arrows Javelins Protection helmets Bicycle frames Golf clubs Oars

1.4 TYPICAL EXAMPLES OF INTEREST ON THE USE OF COMPOSITE MATERIALS In the domain of commercial aircraft, one can compare the concerns of manufacturers with the principal characteristic properties of composite materials. The concerns of the manufacturers are performance and economy. The characteristics of composite components include the following: Weight saving leads to fuel saving, increase in payload, or increase in range which improves performances. Good fatigue resistance leads to enhanced life which involves saving in the long-term cost of the product. Good corrosion resistance means fewer requirements for inspection which results in saving on maintenance cost. Moreover, taking into account the cost of the composite solution as compared with the conventional solution, one can state that composites fit the demand of aircraft manufacturers.

1.5 EXAMPLES ON REPLACING CONVENTIONAL SOLUTIONS WITH COMPOSITES Table 1.1 shows a few significant cases illustrating the improvement on price and performance that can be obtained after replacement of a conventional solution with a composite solution.

1.6 PRINCIPAL PHYSICAL PROPERTIES Tables 1.2 through 1.5 take into account the properties of only individual components, reinforcements, or matrices. The characteristics of composite materials resulting from the combination of reinforcement and matrix depend on The proportions of reinforcements and matrix (see Section 3.2) The form of the reinforcement (see Section 3.2) The fabrication process © 2003 by CRC Press LLC

TX846_Frame_C01 Page 10 Monday, November 18, 2002 10:34 AM

Table 1.1 Properties of Commonly Used Resins Application 3

65 m reservoir for chemicals Smoke stack for chemical plant Nitric acid vapor washer Helicopter stabilizer Helicopter winch support Helicopter motor hub X–Y table for fabrication of integrated circuits Drum for drawing table Head of welding robot Weaving machine rod Aircraft floor

Price of Previous Construction

Stainless steel + installation: 1. Steel: 1. Stainless steel: 1. Light alloys + steel (16 kg): 1. Welded steel (16 kg): 1. (Mass: 1): 1. Cast aluminum: Rate of fabrication: 30 plates/hr Speed of drawing: 15 to 30 cm/sec Aluminum: Mass = 6 kg Aluminum: Rate = 250 shots/minute (Mass = 1): 1.

Price of Composite Construction

0.53 0.51 0.33 Carbon/epoxy (9 kg): 0.45 Carbon/epoxy (11 kg): 1.2 Carbon/Kevlar/epoxy (mass: 0.8): 0.4 Carbon/epoxy honeycomb sandwich: 55 plates/hr Kevlar/epoxy: 40 to 80 cm/sec Carbon/epoxy: Mass = 3 kg Carbon/epoxy: Rate = 350 shots/minute Carbon/Kevlar/epoxy (mass: 0.8): 1.7

These characteristics may be observed in Figure 1.5, which shows the tensile strength for different fiber fractions and different forms of reinforcement for the case of glass/resin composite, and Figure 1.6, which gives an interesting view on the specific resistance of the principal composites as a function of temperature. (The specific strength is defined as the strength divided by the density srupt/r.) Other remarkable properties of these materials include the following: Composite materials do not yield (their elastic limits correspond to the rupture limit; see Section 5.4.5). Composite materials are very fatigue resistant (see Section 5.1). Composite materials age subject to humidity (epoxy resin can absorb water by diffusion up to 6% of its mass; the composite of reinforcement/resin can absorb up to 2%) and heat. Composite materials do not corrode, except in the case of contact “aluminum with carbon fibers” in which case galvanic phenomenon creates rapid corrosion. Composite materials are not sensitive to the common chemicals used in engines: grease, oils, hydraulic liquids, paints and solvents, petroleum. However, paint thinners attack the epoxy resins. Composite materials have medium to low level impact resistance (inferior to that of metallic materials). Composite materials have excellent fire resistance as compared with the light alloys with identical thicknesses. However, the smokes emitted from the combustion of certain matrices can be toxic. © 2003 by CRC Press LLC

Density r 3 (kg/m )

Elastic Modulus E (MPa)

Shear Modulus G (MPa)

Poisson Ratio n

Steels

7800

205,000

79,000

0.3

Aluminum Alloy 2024 Titanium Alloy TA 6V Copper

2800

75,000

29,000

4400

105,000

8800

125,000

Nickel

8900

220,000

Beryllium

1840

294,000

Silicon

2200

95,000

Metals and Alloys

Tensile Strength sult (Mpa)

Elongation (%)

Coefficient of Thermal Expansion at -1 20∞C a (∞C ) -5

1.8 to 10

1.3 ¥ 10

0.3

400 to 1600 450

10

2.2 ¥ 10

40,300

0.3

1200

14

0.8 ¥ 10

48,000

0.3

200 to 500 500 to 850 200

0.05

-5

-5

-5

1.7 ¥ 10

-5

1.2 ¥ 10 5

Coefficient of Thermal Conductivity at 20∞C l(W/m∞C)

Heat Capacity c(J/kg˚C)

20 to 100

400 to 800

800

140

1000

350

17

540

700

380

390

650

70

500

900

150 (20˚C) 90 (800˚C) 1.4 (20˚C) 3 (1200˚C)

1750 (20˚C) 3000 (800˚C) 750 (20˚C) 1200(500˚C)

900

Useful Temperature Limit Tmax (˚C)

1300

TX846_Frame_C01 Page 11 Monday, November 18, 2002 10:34 AM

© 2003 by CRC Press LLC

Table 1.2 Properties of Commonly Used Metals and Alloys and Silicon

Tensile Fiber Modulus of Shear Diameter Density Elasticity Modulus Poisson Strength Elongation 3 Reinforcements d(mm) r(kg/m ) E(Mpa) G(Mpa) Ratio n sUlt (Mpa) E(%)

“R” glass, high performance “E” glass, common applications Kevlar 49 “HT” graphite, high strength “HM” graphite, high modulus Boron Aluminum Aluminum silicate Silicon carbide Polyethylene

Useful Coefficient of Coefficient Thermal of Thermal Heat Temperature Price Expansion Conductivity Capacity Limit Tmax 1993 -1 l(W/M∞C) c(J/kg˚C) a (∞C ) (∞C) ($/kg) -5

0.2

3200

4

0.3 ¥ 10

30,000

0.25

2500

3.5

0.5 ¥ 10

130,000 230,000

12,000 50,000

0.4 0.3

2900 3200

2.3 1.3

-0.2 ¥ 10 -5 0.02 ¥ 10

1800

390,000

20,000

0.35

2500

0.6

0.08 ¥ 10

100 20

2600 3700

400,000 380,000

3400 1400

0.8 0.4

0.4 ¥ 10

10

2600

200,000

3000

1.5

14

2550

200,000

2800

1.3

960

100,000

3000

10

2500

86,000

16

2600

74,000

12 7

1450 1750

6.5

-5

-5

-5

1

800

700

14

1

800

700

2

0.03 200 (20∞C) 60 (800∞C)

1400 800

>1500

70 70

200 (20∞C) 60 (800∞C)

800

>1500

140

900

500 >1000

500

50 (20∞C) 7 (800∞C)

1300

600

-5

-5

0.5 ¥ 10

150

TX846_Frame_C01 Page 12 Monday, November 18, 2002 10:34 AM

© 2003 by CRC Press LLC

Table 1.3 Properties of Commonly Used Reinforcements

Resins

Tensile Density Elastic Shear r Modulus Modulus Poisson Strength Elongation 3 (kg/m ) E(Mpa) G(Mpa) Ratio n sUlt (Mpa) E%

Coefficient of Thermal Expansion -1 a (∞C )

Thermosets

Epoxy

1200

4500

1600

0.4

130

Phenolic Polyester Polycarbonate Vinylester Silicone Urethane

1300 1200 1200 1150 1100 1100

1100 1400

0.4 0.4 0.35

70 80 60 75 35 30

Polyimide

1400

3000 4000 2400 3300 2200 700 to 7000 4000 to 19,000

0.5

1100

0.35

70

2 (100˚C) 6 (200˚C) 2.5 2.5 4

900

1200

1300

4000

1100 1350

2000 3000

1250 1300

3500 4000

0.4

0.35

1 8 6 5

¥ ¥ ¥ ¥

-5

10 -5 10 -5 10 -5 10

0.2

1000

90 to 200

0.3 0.2

1000 1400 1200

120 to 200 60 to 200 120 >100 100 to 350 100

100 1

Thermoplastics

Polypropylene (pp) Polyphenylene sulfone (pps) Polyamide (pa) Polyether sulfone (pes) Polyetherimide (pei) Polyether-etherketone (peek)

-5

11 ¥ 10

Coefficient Useful of Thermal Temperature Price Heat Conductivity Capacity Limit Tmax 1993 l (W/m∞C) C(J/kg∞C) (∞C) ($/kg)

-5

8 ¥ 10

0.2

-5

30

20 to 400

9 ¥ 10

65

100

5 ¥ 10

70 85

200 60

8 ¥ 10 -5 6 ¥ 10

105 90

60 50

6 ¥ 10 -5 5 ¥ 10

1000

250 to 300

330

70 to 140

-5

2.4 4 4

130 to 250

-5

-5

6 to 20

1200

0.2 0.3

170 180

6 25

200 140 to 250

20 96

TX846_Frame_C01 Page 13 Monday, November 18, 2002 10:34 AM

© 2003 by CRC Press LLC

Table 1.4 Properties of Commonly Used Resins

Cores

Balsa

Compressive Modulus Shear Strength Density of Elasticity Modulus Poisson Elongation 3 r(Kg/M ) E(Mpa) G(Mpa) Ratio n sUlt(Mpa) E%

100 to 190 30 to 70

Polyurethane foam Polystyrene 30 to 45 foam Honeycombs Impregnated carton Impregnated glass fabric Aluminum 15 to 130 Steel Nomex®

25 to 50

2000 to 6000 25 to 60

100 to 250

8 to 18 0.4

20 to 30

0.4

50 to 350 100 to 600 130 to 910 550 to 1250 10 to 40

Coefficient of Thermal Expansion -1 a(∞C )

Coefficient Useful of Thermal Temperature Price Heat Conductivity Capacity Limit 1993 Tmax (∞C) l(W/M∞C) C(J/Kg∞C) ($/Kg)

0.05

11 75

0.25 to 1.25

0.2 to 8

0.2 to 2.5

75

TX846_Frame_C01 Page 14 Monday, November 18, 2002 10:34 AM

© 2003 by CRC Press LLC

Table 1.5 Properties of Commonly Used Core Materials

TX846_Frame_C01 Page 15 Monday, November 18, 2002 10:34 AM

Figure 1.5 Tensile Strength of Glass/Resin Composites

Figure 1.6 Specific Strength of Different Composites

© 2003 by CRC Press LLC

TX846_Frame_C02 Page 17 Monday, November 18, 2002 10:40 AM

2 FABRICATION PROCESSES The mixture of reinforcement/resin does not really become a composite material until the last phase of the fabrication, that is, when the matrix is hardened. After this phase, it would be impossible to modify the material, as in the way one would like to modify the structure of a metal alloy using heat treatment, for example. In the case of polymer matrix composites, this has to be polymerized, for example, polyester resin. During the solidification process, it passes from the liquid state to the solid state by copolymerization with a monomer that is mixed with the resin. The phenomenon leads to hardening. This can be done using either a chemical (accelerator) or heat. The following pages will describe the principal processes for the formation of composite parts.

2.1 MOLDING PROCESSES The flow chart in Figure 2.1 shows the steps found in all molding processes. Forming by molding processes varies depending on the nature of the part, the number of parts, and the cost. The mold material can be made of metal, polymer, wood, or plaster.

2.1.1 Contact Molding Contact molding (see Figure 2.2) is open molding (there is only one mold, either male or female). The layers of fibers impregnated with resin (and accelerator) are placed on the mold. Compaction is done using a roller to squeeze out the air pockets. The duration for resin setting varies, depending on the amount of accelerator, from a few minutes to a few hours. One can also obtain parts of large dimensions at the rate of about 2 to 4 parts per day per mold.

2.1.2 Compression Molding With compression molding (see Figure 2.3), the countermold will close the mold after the impregnated reinforcements have been placed on the mold. The whole assembly is placed in a press that can apply a pressure of 1 to 2 bars. The polymerization takes place either at ambient temperature or higher. The process is good for average volume production: one can obtain several dozen parts a day (up to 200 with heating). This has application for automotive and aerospace parts. © 2003 by CRC Press LLC

TX846_Frame_C02 Page 18 Monday, November 18, 2002 10:40 AM

Figure 2.1 Steps in Molding Process

Figure 2.2 Contact Molding

Figure 2.3 Compression Molding © 2003 by CRC Press LLC

TX846_Frame_C02 Page 19 Monday, November 18, 2002 10:40 AM

Figure 2.4 Vacuum Molding

Figure 2.5 Electron Beam or X-ray Molding

2.1.3 Molding with Vacuum This process of molding with vacuum is still called depression molding or bag molding. As in the case of contact molding described previously, one uses an open mold on top of which the impregnated reinforcements are placed. In the case of sandwich materials, the cores are also used (see Chapter 4). One sheet of soft plastic is used for sealing (this is adhesively bonded to the perimeter of the mold). Vacuum is applied under the piece of plastic (see Figure 2.4). The piece is then compacted due to the action of atmospheric pressure, and the air bubbles are eliminated. Porous fabrics absorb excess resin. The whole material is polymerized by an oven or by an autoclave under pressure (7 bars in the case of carbon/epoxy to obtain better mechanical properties), or with heat, or with electron beam, or x-rays; see Figure 2.5). This process has applications for aircraft structures, with the rate of a few parts per day (2 to 4). © 2003 by CRC Press LLC

TX846_Frame_C02 Page 20 Monday, November 18, 2002 10:40 AM

Figure 2.6 Resin Injection Molding

Figure 2.7 Injection of Premixed

Figure 2.8 Injection of Thermoplastic Premixed

2.1.4

Resin Injection Molding

With resin injection molding (see Figure 2.6), the reinforcements (mats, fabrics) are put in place between the mold and countermold. The resin (polyester or phenolic) is injected. The mold pressure is low. This process can produce up to 30 pieces per day. The investment is less costly and has application in automobile bodies.

2.1.5

Molding by Injection of Premixed

The process of molding by injection of premixed allows automation of the fabrication cycle (rate of production up to 300 pieces per day). Thermoset resins: Can be used to make components of auto body. The schematic of the process is shown in Figure 2.7. Thermoplastic resins: Can be used to make mechanical components with high temperature resistance, as shown in Figure 2.8. © 2003 by CRC Press LLC

TX846_Frame_C02 Page 21 Monday, November 18, 2002 10:40 AM

Figure 2.9 Foam Injection

Figure 2.10 Centrifugal Molding

2.1.6 Molding by Foam Injection Molding by foam injection (see Figure 2.9) allows the processing of pieces of fairly large dimensions made of polyurethane foam reinforced with glass fibers. These pieces remain stable over time, with good surface conditions, and have satisfactory mechanical and thermal properties.

2.1.7 Molding of Components of Revolution The process of centrifugal molding (see Figure 2.10) is used for the fabrication of tubes. It allows homogeneous distribution of resin with good surface conditions, including the internal surface of the tube. The length of the tube depends on the length of the mold. Rate of production varies with the diameter and length of the tubes (up to 500 kg of composite per day). The process of filament winding (see Figure 2.11) can be integrated into a continuous chain of production and can fabricate tubes of long length. The rate of production can be up to 500 kg of composite per day. These can be used to make missile tubes, torpillas, containers, or tubes for transporting petroleum. For pieces which must revolve around their midpoint, winding can be done on a mandrel. This can then be removed and cured in an autoclave (see Figure 2.12). The fiber volume fraction is high (up to 85%). This process is used to fabricate components of high internal pressure, such as reservoirs and propulsion nozzles. © 2003 by CRC Press LLC

TX846_Frame_C02 Page 22 Monday, November 18, 2002 10:40 AM

Figure 2.11 Filament Winding

Figure 2.12 Filament Winding on Complex Mandrel

Figure 2.13 Sheet Forming

2.2 OTHER FORMING PROCESSES 2.2.1 Sheet Forming This procedure of sheet forming (see Figure 2.13) allows the production of plane or corrugated sheets by corrugation or ribs. © 2003 by CRC Press LLC

TX846_Frame_C02 Page 23 Monday, November 18, 2002 10:40 AM

Figure 2.14 Profile Forming

Figure 2.15 Stamp Forming

2.2.2. Profile Forming The piece shown in Figure 2.14 is made by pultrusion. This process makes possible the fabrication of continuous open or closed profiles. The fiber content is important for high mechanical properties. The rate of production varies between 0.5 and 3 m/ minute, depending on the nature of the profile.

2.2.3 Stamp Forming Stamp forming (see Figure 2.15) is only applicable to thermoplastic composites. One uses preformed plates, which are heated, stamped, and then cooled down.

2.2.4 Preforming by Three-Dimensional Assembly Example: Carbon/carbon: The carbon reinforcement is assembled by depositing the woven tows along several directions in space. Subsequently the empty space between the tows is filled by “impregnation.” The following two techniques are used: Impregnation using liquid: Pitch is used under a pressure of 1000 bars, followed by carbonization. Impregnation using gas: This involves chemical vapor deposition using a hot gaseous hydrocarbon atmosphere. Example: Silicon/silicon. The reinforcement is composed of filaments of silicon ceramics. The silicon matrix is deposited in the form of liquid solution of colloidal silicon, followed by drying under high pressure and high temperature (2000 bars, 2000∞C). The preforms are then machined. The phases of development © 2003 by CRC Press LLC

TX846_Frame_C02 Page 24 Monday, November 18, 2002 10:40 AM

of these composites, such as the densification (formation of the matrix) are long and delicate. These make the products very onerous. Applications include missile and launcher nozzles, brake disks, ablative tiles for reentry body of spacecraft into the atmosphere.

2.2.5 Cutting of Fabric and Trimming of Laminates Some components need a large number of fabric layers (many dozens, can be hundreds). For the small and medium series, it can be quite expensive to operate manually for following the form of a cut. respect the orientation specified by the design (see Chapter 5). minimizing waste. There is a tendency to produce a cut or a drape automatically with the following characteristics: a programmed movement of the cutting machine a rapid cutting machine, such as an orientable vibrating cutting knife or a laser beam with the diameter of about 0.2 mm and a cutting speed varying from 15 to 40 meters/minute, depending on the power of the laser and the thickness of the part. Example: With a draping machine MAD Forest-Line (FRA), the draping is done in two steps by means of two distinct installations: A cutting machine that produces a roller to which the cut pieces are attached (cassettes) A depositing machine which uses the cassette of cut pieces to perform the draping. The two operations are shown schematically in Figure 2.16.

2.3 PRACTICAL HINTS ON MANUFACTURING PROCESSES 2.3.1 Acronyms To describe the modes of fabricating the composite pieces, the professionals use many abbreviations. Each is detailed below, with reference to the paragraph number where the process is explained. B.M.C.: “Bulk Molding Compound.” Matrix: resins. Reinforcement: cut fibers; additional fillers (powder). Pressure: 5–10 MPa. Temperature: 120– 150∞C. Centrifugation: Matrix: resins. Reinforcement: cut fibers, mat, fabrics; see Section 2.1.7. © 2003 by CRC Press LLC

TX846_Frame_C02 Page 25 Monday, November 18, 2002 10:40 AM

Figure 2.16 Draping Process

Contact molding: Matrix: resins. Reinforcement: mat, fabrics; see Section 2.1.1. Filament winding: Matrix: resins. Reinforcement: continuous fibers; see Section 2.1.7. Compression molding: Matrix: resins. Reinforcement: fabrics or unidirectionals; see Section 2.1.2. Autoclave molding: Matrix: resins. Reinforcement: fabrics or unidirectionals; under pressure in an autoclave; see Section 2.1.3. Pultrusion: Matrix: resins. Reinforcement: mat, fabrics, continuous fibers; see Section 2.2.2. R-RIM: “Reinforced–Reaction Injection Molding” (there is expansion in the mold). Pressure: 0.5 MPa. Temperature: 50–60∞ C; see Section 2.1.6. S-RIM: “Structural Reaction Injection Molding” (components for structure, particularly in automobiles). Similar to R-RIM, injection of liquid thermoset resins consists of two highly reactive constituents. RTM: “Resin Transfer Molding.” Matrix: resins.. Reinforcement: Preforms of cut fibers or fabrics. Pressure: low (in vacuum or 0.1–0.3 MPa). Temperature: 80∞C. SMC: “Sheet Molding Compound.” Matrix: liquid resin with addition of magnesia. Reinforcement: mat, unidirectionals. Pressure: 5–10 MPa. Temperature: 120–150∞C. © 2003 by CRC Press LLC

TX846_Frame_C02 Page 26 Monday, November 18, 2002 10:40 AM

26 Composite Materials: Design and Applications

Figure 2.17 Cost Comparison for Different Processes

© 2003 by CRC Press LLC

TX846_Frame_C02 Page 27 Monday, November 18, 2002 10:40 AM

RTP: “Reinforced Thermoplastics.” Matrix: thermoplastic resins. Reinforcement: cut fibers. Pressure: 50 to 150 MPa. Temperature: 120–150∞C. RST: “Reinforced Stamped Thermoplastics.” Pressure: 15–20 MPa. Initial temperature: ª200∞C; see Section 2.2.3. ZMC: Matrix: resin. Reinforcement: cut fibers. Pressure: 30–50 MPa. Temperature: 120–150∞C. TMC: Similar to “SMC” but with higher amount of glass fibers (a few millimeters in thickness). XMC: Similar to “SMC” but with specific orientation of the fibers.

2.3.2 Cost Comparison The diagram in Figure 2.17 allows the comparison of the cost to fabricate composite products. One needs to note the important difference between the cost of composites produced in large volume and the cost of high performance composites.

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 29 Monday, November 18, 2002 12:05 PM

3 PLY PROPERTIES It is of fundamental importance for the designer to understand and to know precisely the geometric and mechanical characteristics of the “fiber + matrix” mixture which is the basic structure of the composite parts. The description of these characteristics is the object of this chapter.

3.1 ISOTROPY AND ANISOTROPY When one studies the mechanical behavior of elastic bodies under load (elasticity theory), one has to consider the following: An elastic body subjected to str esses deforms in a reversible manner. At each point within the body, one can identify the principal planes on which there are only normal stresses. The normal directions on these planes are called the principal stress directions. A small sphere of material surrounding a point of the body becomes an ellipsoid after loading. The spatial position of the ellipsoid relative to the principal stress directions enables us to characterize whether the material under study is isotr opic or anisotropic. Figure 3.1 illustrates this phenomenon. Figure 3.2 illustrates the deformation of an isotropic sample and an anisotropic sample. In the latter case, the oblique lines represent the preferred directions along which one would place the fibers of reinforcement. One can consider that a longitudinal loading applied to an isotropic plate would create an extension in the longitudinal direction and a contraction in the transverse direction. The same loading applied to an anisotropic plate creates an angular distortion, in addition to the longitudinal extension and transversal contraction. In the simple case of plane stress, one can obtain the elastic constants using stress–strain relations.

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 30 Monday, November 18, 2002 12:05 PM

Figure 3.1 Schematic of Deformation

Figure 3.2 Comparison between Deformation of an Isotropic and Anisotropic Plate

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 31 Monday, November 18, 2002 12:05 PM

Figure 3.3 Stress–Strain Behavior in an Isotropic Material

3.1.1 Isotropic Materials The following relations are valid for a material that is elastic and isotropic.

One can write the stress–strain relation (see Figure 3.3) in matrix form as

Ï ex Ô Ì ey Ô Ó g xy

1

1 n --- – --- 0 E E ¸ Ô n 1 ˝ = – --- --- 0 E E Ô ˛ 1 0 0 ---G

1

Ï sx ¸ Ô Ô Ì sy ˝ Ô Ô Ó t xy ˛

In these equations, ex,ey,gxy are also the small strains that are obtained in a classical manner from the displacements ux and uy as: ex = ∂ux /∂x; ey = ∂uy /∂ y; gxy = ∂ux /∂y + ∂uy /∂x.

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 32 Monday, November 18, 2002 12:05 PM

Figure 3.4 Deformation in an Anisotropic Material

There are three elastic constants: E, n, G. There exists a relation among them as: E G = -------------------2(1 + n ) The above relation shows that a material that is isotropic and elastic can be characterized by two independent elastic constants: E and n.

3.1.2 Anisotropic Material The matrix equation for anisotropic material (see Figure 3.4) is

Ï ex Ô Ì ey Ô Ó g xy

© 2003 by CRC Press LLC

1 ----Ex

¸ Ô n xy ˝ = – -----Ex Ô ˛ 0

n yx – -----Ey 1 ----Ey 0

0

Ï sx ¸ Ô Ô 0 Ì sy ˝ Ô Ô Ó t xy ˛ 1 -------G xy

TX846_Frame_C03 Page 33 Monday, November 18, 2002 12:05 PM

2

Note that the stress–strain matrix above is symmetric. The number of distinct elastic constants is five: Two moduli of elasticity: Ex and Ey, Two Poisson coefficients: nyx and nxy, and One shear modulus: Gxy. In fact there are only four independent elastic constants: Ex, Ey, Gxy, and nyx (or nxy). The fifth elastic constant can be obtained from the others using the symmetry relation: 3

E n xy = n yx -----x Ey

3.2 CHARACTERISTICS OF THE REINFORCEMENT–MATRIX MIXTURE We denote as ply the semi-product “reinforcement + resin” in a quasi-bidimen4 sional form. This can be A tape of unidirectional fiber + matrix, A fabric + matrix, or A mat + matrix. These are examined more below.

3.2.1 Fiber Mass Fraction Fiber mass fraction is defined as Mass of fibers M f = ----------------------------------Total mass In consequence, the mass of matrix is Mass of matrix M m = ------------------------------------Total mass with Mm = 1 – Mf

2 3 4

To know more about the development on this point, refer to Section 9.2 and Exercise 18.1.2. Refer to Section 13.2. Such condition exists in the commercial products. These are called preimpregnated or SMC (sheet molding compound). One can also find non-preformed mixtures of short fibers and resin. These are called premix or BMC (bulk molding compound).

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 34 Monday, November 18, 2002 12:05 PM

Table 3.1 Common Fiber Volume Fractions in Different Processes Molding Process

Fiber Volume Fraction

Contact Molding Compression Molding Filament Winding Vacuum Molding

30% 40% 60%–85% 50%–80%

3.2.2 Fiber Volume Fraction Fiber volume fraction is defined as Volume of fiber V f = ---------------------------------------Total volume As a result, the volume of matrix is given as Volume of matrix V m = --------------------------------------------Total volume 5

with

Vm = 1 – Vf Note that one can convert from mass fraction to volume fraction and vice versa. If rf and rm are the specific mass of the fiber and matrix, respectively, we have Mf --rf

V f = ----------------Mf Mm --- + ----r r f

Vf rf M f = -----------------------------Vf rf + Vm rm

m

Depending on the method of fabrication, the common fiber volume fractions are as shown in Table 3.1.

3.2.3 Mass Density of a Ply The mass density of a ply can be calculated as total mass r = -------------------------------total volume 5

In reality, the mixture of fiber/matrix also includes a small volume of voids, characterized by the porosity of the composite. One has then Vm + Vf + Vp = 1, in which Vp denotes the percentage of “volume of void/total volume.” Vp is usually much less than 1 (See Exercise 18.1.11).

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 35 Monday, November 18, 2002 12:05 PM

Table 3.2 Ply Thicknesses of Some Common Composites

E glass R glass Kevlar H.R. Carbon

Mf

H

34% 68% 65% 68%

0.125 mm 0.175 mm 0.13 mm 0.13 mm

The above equation can also be expanded as mass of fiber mass of matrix r = --------------------------------- + ------------------------------------total volume total volume volume of matrix volume of fiber = ---------------------------------------- r f + -------------------------------------------- r m total volume total volume or

r = r f V f + r mV m

3.2.4 Ply Thickness The ply thickness is defined as the number of grams of mass of fiber mof per 2 m of area. The ply thickness, denoted as h, is such that: m of 2 h ¥ 1 ( m ) = total volume = total volume ¥ ------------------------------------------fiber volume ¥ r f or m of h = --------Vf rf One can also express the thickness in terms of mass fraction of fibers rather than in terms of volume fraction. 1 1–M 1 h = m of ---- + ------ Ê ---------------fˆ rf rm Ë Mf ¯ Table 3.2 shows a few examples of ply thicknesses.

3.3 UNIDIRECTIONAL PLY 3.3.1 Elastic Modulus The mechanical characteristics of the fiber/matrix mixture can be obtained based on the characteristics of each of the constituents. In the literatur e, there are theoretical as well as semi-empirical relations. As such, the results from these relations may not always agree with experimental values. One of the reasons is

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 36 Monday, November 18, 2002 12:05 PM

Table 3.3 Fiber Elastic Modulus Kevlar

Carbon H.R.

Carbon H.M.

fiber longitudinal modulus in direction Ef (MPa)

74,000

130,000

230,000

390,000

fiber transverse modulus in t direction (MPa) Eft

74,000

5400

15,000

6000

fiber shear modulus (Mpa) Gft

30,000

12,000

50,000

20,000

fiber Poisson ratio vft

0.25

0.4

0.3

0.35

Ï Ô Ô Ô Ô Ô Ì Ô Ô Ô Ô Ô Ó

Glass E

Isotropic

Anisotropic

because the fibers themselves exhibit some degree of anisotropy. In Table 3.3, one can see small values of the elastic modulus in the transverse direction for 6 Kevlar and carbon fibers, whereas glass fiber is isotropic. With the definitions in the previous paragraph, one can use the following relations to characterize the unidirectional ply: Modulus of elasticity along the direction of the fiber El is given by

7

E = EfVf + EmVm or E = Ef Vf + Em ( 1 – Vf ) In practice, this modulus depends essentially on the longitudinal modulus of the fiber, Ef, because Em > E m .

Figure 3.12 Elastic Modulus of Glass/Epoxy Layers

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 46 Monday, November 18, 2002 12:05 PM

Figure 3.13 Tensile Strength of Glass/epoxy Layers

The composite (matrix + filler) is isotropic, with elastic properties E, G, n given by the following relations: Defining:

1 – n mˆ V f Em - 1 + 3 Ê -------------------------------K = -------------------------Ë 1 + n m¯ ( 1 – V f ) 3 (1 – 2 nm ) 9KG E ª ----------------3K + G Em 15 1 – n m ˆ V f - 1 + ------ Ê ----------------------------------G ª ----------------------2 (1 + nm ) 2 Ë 4 – 5 n m¯ ( 1 – V f ) 1 3K – 2G n ª --- ÊË --------------------ˆ¯ 2 3K + G

3.5.4 Other Reinforcements One may also use reinforcements in the form of crushed fibers, flakes (see Figure 3.15), or powders made of the following: Glass Graphite Metals

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 47 Monday, November 18, 2002 12:05 PM

Figure 3.14 Spherical Fillers

Figure 3.15 Form of Flakes

Figure 3.16 Mica Flakes Arrangement

Aluminum Mica (L ª 100 mm) Talc (L ª 10 mm) Immersed in a resin with stratified fibers, mica flakes have the arrangement as shown in the Figure 3.16. One can observe that the modulus of the resin is 13 increased as Ln ( 1 + u ) E = 1 – ------------------------- ¥ E mica V mica + E m V m ; u

13

L G m V mica - ¥ -----------u = -- ---------e E mica V m

For more details, see “Interaction Effects in Fiber Composites,” which is listed in the Bibliography at the end of the book.

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 48 Monday, November 18, 2002 12:05 PM

Figure 3.17 Cross Section with and without Mica

Figure 3.18 4D Architecture

The average properties of mica are Emica = 170,000 MPa and rmica = 2,800 kg/m . 3

Figure 3.17 shows the increase resistance against the microfracture of the resin.

3.6 MULTIDIMENSIONAL FABRICS An example of “4D” architecture of carbon reinforcement from the European society of propulsion (FRA) has the reinforcement assembled according to preestablished directions (see Figure 3.18). The fiber volume fraction is on the order 14 of 30%. The matrix comes to fill the voids between the fibers. The principal advantages of these types of composites are The supplementary connection (as compared with the bidimensional plies) makes the composites safe from delamination. The mechanical resistance is conserved—and even improved—at high temperatures (up to 3,000∞C for carbon/carbon). The coefficient of expansion remains small. They are resistant against thermal shock. 14

See Section 2.2.4.

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 49 Monday, November 18, 2002 12:05 PM

Table 3.7 Properties of Three-Dimensional Carbon/Carbon

Aerolor 41 3

Specific mass (kg/m ) Longitudinal tensile fracture strength (MPa) Longitudinal compressive fracture strength (MPa) Tensile strength in z direction (MPa) Compressive strength in z direction (MPa) Shear strength in z plane (MPa) Longitudinal elastic modulus E (MPa) Elastic modulus Ez (MPa) Shear modulus Gz (MPa) Shear modulus G (MPa) Poisson ratio uz Poisson ratio u Thermal expansion coefficient -1 a(∞C ) at 1000∞C at 2,500∞C Thermal expansion coefficient -1 az(∞C ) at 1000∞C at 2,500∞C Coefficient of thermal conductivity (W/m ¥ ∞C)

16

17

Septcarb 4

1700 to 2000 40 to 100 80 to 200

1500 to 2000 95 and increasing, up to 2000∞C 65

>10 80 to 200

3 120

20 to 40 30,000

10 16,000

-6

-6

0.7 ¥ 10 ; 3 ¥ 10 -6

-6

6 ¥ 10 ; 6 ¥ 10

5000 2200 5700 0.17 0.035 -6 -6 3 ¥ 10 ; 4 ¥ 10 -6

-6

7 ¥ 10 ; 9 ¥ 10

300

There is a high coefficient of thermal conductivity. They have small density. The silicon/silicon is transparent to radio-electric waves. Table 3.7 gives the characteristics of two composites made of tridimensional carbon/carbon. The mechanical properties are the same along all directions noted 15 16 17 by in the following figure. The composite is transversely isotropic.

15 16 17

This notion is shown in detail in Section 13.2. Product of the Aerolor company (FRA). Product of European company in propulsion (FRA).

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 50 Monday, November 18, 2002 12:05 PM

Figure 3.19 Layers of ARALL and GLARE

Figure 3.20 Sic Whisker

3.7 METAL MATRIX COMPOSITES There are a number of products in development or in experimental stage including: Matrices: aluminum, magnesium, titanium (see also Section 7.4) and Reinforcements (fibers): aramid, carbon, boron, silicon carbide (SiC) Example: ARALL (Aluminum Reinforced Aramid) and GLARE (Aluminum 18 Reinforced Glass). The essential advantage is better impact damage tolerance because of better resistance to failure due to thin metallic layers and resistance against the crack propagation from one layer to the other (see Figure 3.19). Example: Short silicon carbide fibers (whiskers)/aluminum. This is a socalled “incompatible” composite because the big difference between the thermomechanical properties of the constituents leads to high stress concentrations and debonding between the fibers and the matrix (see Figure 3.20). This has good applications at high temperatures. The diameter of the whisker is about 20 mm. Slenderness ratio L/∆ ª 5 and fiber volume fraction Vf ª 0.3. Example: Boron/aluminum. This is used in aerospace applications (see Section 7.5.4). The technique to obtain these materials is shown schematically in Figure 3.21. This composite can be used continuously at temperatures on the order of 300∞C, while maintaining notable mechanical properties (see Section 1.6 for the properties of boron).

18

®

AKZO Fibers/DELFT University (Holland). Structural Laminates Company/New Kensington (USA).

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 51 Monday, November 18, 2002 12:05 PM

Figure 3.21 Boron/Aluminum Composite

Some characteristics of unidirectional plies made of aluminum matrix (6061) include:

Fiber volume fraction Vf (%) 3 Specific mass (kg/m ) Longitudinal tensile strength (MPa) Longitudinal compressive strength (MPa) Longitudinal elastic modulus (MPa)

HR Carbon

Aluminum

Silicon Carbide

50 2300 800 600 200,000

50 3100 550 3100 190,000

50 2700 1400 3000 140,000

3.8 TESTS The relations cited on the previous pages for the calculation of the modulus and Poisson coefficients of the composites only allow obtaining an order of magnitude for the mechanical properties. Some of these relations are not quite accurate, particularly for the shear modulus. Also, these properties are very sensitive to the fabrication conditions. It is necessary for the design engineer to have the results provided by the suppliers of the reinforcement and the matrix materials or to better the results obtained by tests in the labs. Some of these tests have been standardized, for example, tensile tests, flexure tests, and impact tests. A tensile test (NF T 51–034, ASTM D 3039) on the specimen in Figure 3.22, instrumented with electrical strain gage, allows the measurement of the strength and the elongation to fracture. A delamination test (NF T 57–104) on a specimen which has a small span for bending (see Figure 3.23). It fails by delamination under the effect of interlaminar shear stress. One can obtain the interlaminar shear 19 strength. There are other tests, not yet standardized, that are very useful for the fabrication of high performance composites, for example, for control of the fiber volume fraction. In fact, during the phase of polymerization under pressure of a polymer matrix composite, the resin gets absorbed into an absorbing fabric, in variable quantity depending on the cycle of pressure and temperature. In consequence, 19

This is a simplified way that little reflects the complexity of the state of real stress due to the presence of very close concentrated loads.

© 2003 by CRC Press LLC

TX846_Frame_C03 Page 52 Monday, November 18, 2002 12:05 PM

Figure 3.22 Tensile Test

Figure 3.23 Short Beam Shear Test

Figure 3.24 Variation In Stiffness During Curing

the fiber volume fraction Vf varies, and as a result, the dimensional characteristics of the piece (thickness) also vary. To deal with this problem, one may want to evaluate by test the optimal moment for the application of pr essure, by the measurement of the flexural rigidity of a specimen as a function of time of fabrication (see Figure 3.24).

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 53 Monday, November 18, 2002 12:07 PM

4 SANDWICH STRUCTURES Sandwich structures occupy a large proportion of composite materials design. They appear in almost all applications. Historically they were the first light and 1 high-performance structures. In the majority of cases, one has to design them for a specific purpose. Sandwich structures usually appear in industry as semifinished products. In this chapter we will discuss the principal properties of sandwich structures.

4.1 WHAT IS A SANDWICH STRUCTURE? A sandwich structure results from the assembly by bonding—or welding—of two thin facings or skins on a lighter core that is used to keep the two skins separated (see Figure 4.1). Their properties are astonishing. They have Very light weight. As a comparison, the mass per unit area of the dome 2 of the Saint Peter’s Basilica in Rome (45 meter diameter) is 2,600 kg/m , whereas the mass per surface area of the same dome made of steel/ 2 polyurethane foam sandwich (Hanover) is only 33 kg/m . Very high flexural rigidity. Separation of the surface skins increases flexural rigidity. Excellent thermal insulation characteristics. However, be careful: Sandwich materials are not dampening (no acoustic insulation). Fire resistance is not good for certain core types. The risk of buckling is greater than for classical structures. The facing materials are diverse, and the core materials are as light as possible. One can denote couples of compatible materials to for m the sandwich (see Figure 4.2). Be careful: Polyester resins attack polystyrene foams. 1

See Section 7.1.

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 54 Monday, November 18, 2002 12:07 PM

Figure 4.1 Sandwich Structure (10 £ Ec/Ep £ 100)

Figure 4.2 Constituents of Sandwich Materials

The assembly of the facings to the core is carried out using bonding adhesives. In some exceptional cases, the facings are welded to the core. The quality of the bond is fundamental for the performance and life duration of the piece. In practice we have 0.025 mm £ adhesive thickness £ 0.2 mm

4.2 SIMPLIFIED FLEXURE 4.2.1 Stresses Figure 4.3 shows in a simple manner the main stresses that arise due to the 2 application of bending on a sandwich beam. The beam is clamped at its left end, and a force T is applied at its right end. Isolating and magnifying one elementary segment of the beam, on a cross section, one can observe the shear stress resultant T and the moment resultant M. The shear stress resultant T causes shear stresses t and the moment resultant causes normal stresses s. 2

For more details on these stresses, see Chapters 15 and 17, and also Applications 18.3.5 and 18.3.8.

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 55 Monday, November 18, 2002 12:07 PM

Figure 4.3 Bending Representation

Figure 4.4 Stresses in Sandwich Structure

To evaluate t and s, one makes the following simplifications: The normal stresses are assumed to occur in the facings only, and they are uniform across the thickness of the facings. The shear stresses are assumed to occur in the core only, and they are 3 uniform in the core. One then obtains immediately the expressions for t and s for a beam of unit width and thin facings shown in Figure 4.4.

4.2.2 Displacements In the following example, the displacement D is determined for a sandwich beam subjected to bending as a consequence of Deformation due to normal stresses s and Deformation created by shear stresses t (see Figure 4.5). 3

See Section 17.7.2 and the Applications 18.2.1 and 18.3.5 for a better approach.

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 56 Monday, November 18, 2002 12:07 PM

Figure 4.5 Bending Deflection

To evaluate D, one can, among other methods, use the Castigliano theorem 4

2

1 k 1 M 2 W = --- ----------- dx + --- ------------T dx 2 · GSÒ 2 · EIÒ

Ú

elastic energy

Ú

contribution from bending

D

deflection

∂W = -------∂F

contribution from shear

energy load

5

where the following notations are used for a beam of unit width: M = Moment resultant T = Shear stress resultant Ep = Modulus of elasticity of the material of the facings Gc = Shear modulus of the core material ( ec + ep ) -; · EI Ò #E p e p ¥ 1 ¥ --------------------2 2

k/ · GS Ò = 1/G c ( e c + 2e p ) ¥ 1.

Example: A cantilever sandwich structure treated as a sandwich beam (see Figure 4.6). Elastic energy is shown by 1 W = --2

2 2 1 F ( – x) ------------------------ dx + --2 · EI Ò 0

Ú

2

k

dx Ú ------------F · GSÒ 2

0

3

k F W = ----- Ê -------------- + ------------ˆ 2 Ë 3 · EIÒ · GSÒ ¯ 4

5

See Equation 15.16 that allows one to treat this sandwich beam like a homogeneous beam. One can also use the classical strength of materials approach. See Application 18.2.1 or Chapter 15.

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 57 Monday, November 18, 2002 12:07 PM

Figure 4.6 Cantilever Beam

where · EI Ò = 475 ¥ 10 ; 2

· GSÒ ------------ = 650 ¥ 10 2 k

The end displacement D can be written as ∂W D = -------∂F Then for an applied load of 1 Newton D = 0.7 ¥ 10 Flexure

–2

mm/N + 1.54 ¥ 10

–2

mm/N

Shear

Remark: Part of the displacement D due to shear appears to be higher than that due to bending, whereas in the case of classical homogeneous beams, the shear displacement is very small and usually neglected. Thus, this is a specific property of sandwich structures that strongly influences the estimation of the bending displacements.

4.3 A FEW SPECIAL ASPECTS 4.3.1 Comparison of Mass Based on Equivalent Flexural Rigidity (EI) Figure 4.7 allows the comparison of different sandwich structures having the same flexural rigidity ·EI Ò. Following the discussion in the previous section, this accounts for only a part of the total flexural deformation. © 2003 by CRC Press LLC

TX846_Frame_C04 Page 58 Monday, November 18, 2002 12:07 PM

Figure 4.7 Comparison of Plates Having Similar Flexural Rigidity EI

Figure 4.8 Buckling of Sandwich Structure

4.3.2 Buckling of Sandwich Structures The compression resistance of all or part of a sandwich structure is limited by the so-called critical values of the applied load, above which the deformations become large and uncontrollable. This phenomenon is called buckling of the structure (see Figure 4.8). Depending on the type of loading, one can distinguish different types of buckling which can be global or local.

4.3.2.1 Global Buckling 6

Depending on the supports, the critical buckling load Fc is given by p · EI Ò F cr = K -------------------------------------2 2 · EI Ò + p -------------kK · GS Ò 2

6

See Application 18.3.4.

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 59 Monday, November 18, 2002 12:07 PM

Figure 4.9 Local Buckling of Facings

Figure 4.10 Damage by Local Buckling

4.3.2.2 Local Buckling of the Facings The facings are subject to buckling due to the low stiffness of the core. Depending on the type of loading, one can find the modes of deformation as shown in Figure 4.9. The critical compression stress is given in the equation below where nc is the Poisson coefficient of the core. 2 1/3

s cr = a ¥ (E p ¥ E c ) with

2 – 1 /3

a = 3 { 12 ( 3 – v c ) ( 1 + v c ) } 2

The critical load to cause local damage by local buckling of a facing and the types of damage are shown in Figure 4.10.

4.3.3 Other Types of Damage Local crushing: This is the crushing of the core material at the location of the load application (see figure below).

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 60 Monday, November 18, 2002 12:07 PM

Compression rupture: In this case (see figure below), note that the weak com7 pression resistance of Kevlar fibers leads to a compression strength about two times less than for sandwich panels made using glass fibers.

4.4 FABRICATION AND DESIGN PROBLEMS 4.4.1 Honeycomb: An Example of Core Material These well-known materials are made of hexagonal cells that are regularly spaced. Such geometry can be obtained using a technique that is relatively simple. Many thin sheets are partially bonded. Starting from stacked bonded sheets, they are expanded as shown in Figure 4.11. The honeycomb material can be metal (light alloy, steel) or nonmetal (carton impregnated with phenolic resin, polyamide sheets, or impregnated glass fabrics). Metallic honeycombs are less expensive and more resistant. Nonmetallic honeycombs are not sensitive to corrosion and are good thermal insulators. The following table shows the mechanical and geometric characteristics of a few current honeycombs, using the notations of Figure 4.11. Table 4.1 Properties of Some Honeycomb

Dia. (D): inscribed circle (mm) Thickness e (mm) 3 Specific mass (kg/m ) Shear strength txz rup (MPa) Shear modulus: Gxz (MPa) # 1.5 Gmat(e/D) Shear strength tyz rup (MPa) Shear modulus: Gyz (MPa) Compression strength: sz rup (MPa) a

Bonded Sheets of a Polyamide: Nomex

Light Alloy AG3

Light Alloy 2024

6; 8; 12

4

6

64 1.7 58

0.85 24 2.8

Nomex® is a product of Du Pont de Nemours.

7

See Section 3.3.3.

© 2003 by CRC Press LLC

0.05 80 3.2 520

2 250 4.4

0.04 46 1.5 280

0.9 140 2

TX846_Frame_C04 Page 61 Monday, November 18, 2002 12:07 PM

Figure 4.11 Honeycomb

Figure 4.12 Processing of Honeycomb

Figure 4.13 Deformation of Honeycomb

4.4.2

Processing Aspects

The processing of the honeycomb is done with a diamond disk (peripheral speed in the order of 30 m/s). The honeycomb is kept on the table of the machine by an aluminum sheet to which it is bonded. Below the aluminum sheet, a depression anchors it to the table (see Figure 4.12). One can also deform the honeycomb. It is important to constrain it carefully, because the deformation behavior is complex. For example, a piece of honeycomb 8 under cylindrical bending shows two curvatures as illustrated in Figure 4.13. 8

This phenomenon is due to the Poisson effect, particularly sensitive here (see Section 12.1.4).

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 62 Monday, November 18, 2002 12:07 PM

Figure 4.14 Over-Expansion of Honeycomb

Figure 4.15 Curvature of Honeycomb

Figure 4.16 Processing of a Sandwich Piece of a Structural Part

The processing can be facilitated using the method of overexpansion which modifies the configuration of the cells as shown in Figure 4.14. At limit of curvature, R is the radius of the contour, and e is the thickness of the sheets which consitute the honeycombs (see Figure 4.15). Nomex honeycombs (sheets of bonded polyamide) must be processed at high temperature. The schematic for the processing of a structural part of sandwich honeycomb is as in Figure 4.16. For moderate loadings (for example, bulkheads), it is possible to fold a sandwich panel following the schematic in Figure 4.17. © 2003 by CRC Press LLC

TX846_Frame_C04 Page 63 Monday, November 18, 2002 12:07 PM

Figure 4.17 Folding of Honeycomb

Figure 4.18 Incorporation of Inserts

4.4.3 Insertion of Attachment Pieces When it is necessary to transmit local loadings, depending on the intensity of these loads, it is convenient to distribute these over one or many inserts, as 9 indicated in Figure 4.18. The filling resin of epoxy type, shown in Figure 4.18, can be lightened by incorporation of phenolic microspheres with resulting density 3 for the lightened resin of 700 to 900 kg/m and crush strength # 35 MPa (see Figure 4.19).

4.4.4 Repair of Laminated Facings For sandwich materials of the type “honeycombs/laminates,” the repair of local damage is relatively easy. It consists of patching the plies of the laminate. The configuration of the repair zone appears as in Figure 4.20.

4.5 NONDESTRUCTIVE QUALITY CONTROL Apart from using the classical methods for controlling the surface defects, which allows the repair of external delaminations of laminated facings, using the following techniques allows the identification and repair of internal defects due to fabrication or due to damages in service. These defects can entail imper fect bonding, delaminations, and inclusions. Principal nondestructive detection methods are illustrated in Figure 4.21.

9

See Sections 6.2.4 and 6.3.

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 64 Monday, November 18, 2002 12:07 PM

Figure 4.19 Some Links for Sandwich Structures

Figure 4.20 Honeycomb Repair

When a composite structure (for example, a reservoir under pressure) is subjected to loading, many microcracks can occur within the piece. Microcracking in the resin, fiber fracture, and disbond between fiber and matrix can exist even within the admissible loading range. These ruptures create acoustic waves that propagate to the surface of the piece. They can be detected and analyzed using acoustic emission sensors (see Figure 4.22). The number of peaks as well as the duration and the amplitude of the signal can be used to indicate the integrity of the piece. In addition, the accumulated number of peaks may be used to predict the fracture of the piece (i.e., the change of slope of the curve in Figure 4.23). © 2003 by CRC Press LLC

TX846_Frame_C04 Page 65 Monday, November 18, 2002 12:07 PM

Figure 4.21 Principal Nondestructive Testing Methods

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 66 Monday, November 18, 2002 12:07 PM

Figure 4.21 (Continued).

© 2003 by CRC Press LLC

TX846_Frame_C04 Page 67 Monday, November 18, 2002 12:07 PM

Figure 4.22 Acoustic Emission Technique

Figure 4.23 Plotting of AE Events

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 69 Monday, November 18, 2002 12:09 PM

5 CONCEPTION AND DESIGN A different paradigm: As every mechanical part, a composite part has to withstand loadings. In addition, the conception process has to extend over a range much larger than for a component made of “pre-established” material. In fact, For isotropic materials, the classical process of conception consists of selection of an existing material and then design of the piece. For a component made of composites, the designer “creates” the material based on the functional requirements. The designer chooses the reinforcement, the matrix, and the process for curing. Following that the designer must define the component architecture, i.e., the arrangement and dimensions of plies, the representation of these on the designs, etc. These subjects are covered in this chapter.

5.1 DESIGN OF A COMPOSITE PIECE The following characteristic properties always have to be kept in mind by the designer: Fiber orientation enables the optimization of the mechanical behavior along a specific direction. The material is elastic up to rupture. It cannot yield by local plastic deformation as can classical metallic materials. Fatigue resistance is excellent.

A Very Good Fatigue Resistance The specific fatigue resistance is expressed by the ratio (s/r), with r being the specific mass. For composite materials, this specific resistance is three times higher than for aluminum alloys and two times higher than that of high strength steel and titanium alloys because the fatigue resistance is equal to 90% of the static fracture strength for a composite, instead of 35% for aluminum alloys and 50% 1 for steels and titanium alloys (see Figure 5.1). 1

See Section 5.4.4.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 70 Monday, November 18, 2002 12:09 PM

Figure 5.1 Comparison of Fatigue Behavior Between Composite and Aluminum

The percent elongation is not the same as that for metals (attention should be paid to the metal/composite joints). Complex forms can be easily molded. It is possible to reduce the number of parts and to limit the amount of processing work. One must adapt the classical techniques of attachments and take into account their induced problems: fragility, delustering, fatigue, thermal stresses.

5.1.1 Guidelines for Values for Predesign Figure 5.2 shows a comparison between different materials, which can help in the choice of composite in the predesign phase. Figure 5.3 allows the comparison of principal specific properties of fibers which make up the plies. The specific modulus and specific strength are presented in the spirit of lightweight structural materials. The safety factors are defined to take care of uncertainties on

The The The The The

magnitude of mechanical characteristics of reinforcement and matrix stress concentrations imperfection of the hypotheses for calculation fabrication process aging of materials

The orders of magnitude of safety factors are as follows:

High volume composites: Static loading Intermittent loading over long term: Cyclic loading: Impact loading: High performance composites:

© 2003 by CRC Press LLC

short duration: long duration:

2 4 4 5 10 1.3 to 1.8

TX846_Frame_C05 Page 71 Monday, November 18, 2002 12:09 PM

Figure 5.2 Comparison of Characteristics of Different Materials

Figure 5.3 Specific Characteristics of Different Fibers

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 72 Monday, November 18, 2002 12:09 PM

Figure 5.4 Unidirectional Layer

5.2 THE LAMINATE Recall that laminates result in the superposition of many layers, or plies, or sheets, made of unidirectional layers, fabrics or mats, with proper orientations in each ply. This is the operation of hand-lay-up.

5.2.1 Unidirectional Layers and Fabrics Unidirectional layers are as shown in Figure 5.4. The advantages of unidirectional layers are: They have high rigidity (maximum number of fibers in one direction). The ply can be used to wrap over long distance. Then the load transmission of the fibers is continuous over large distance. They have less waste. The disadvantages of unidirectional layers are The time for wrapping is long. One cannot cover complex shapes using wrapping. Example: Carbon/epoxy unidirectionals: Width 300 or 1000 mm, preimpregnated with resin; usable over a few years when stored at cold temperature (–18∞C). Fabrics can be found in rolls in dry form or impregnated with resin (Figure 5.5). The advantages of fabrics are Reduced wrapping time Possibility to shape complex form using the deformation of the fabric Possibility to combine different types of fibers in the same fabric The disadvantages of fabrics are Lower modulus and strength than the case of unidirectionals Larger amount of waste material after cutting Requirement of joints when wrapping large parts

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 73 Monday, November 18, 2002 12:09 PM

Figure 5.5 A Fabric Layer

5.2.2 Importance of Ply Orientation One of the fundamental advantages of laminates is their ability to adapt and control the orientation of fibers so that the material can best resist loadings. It is therefore important to know how the plies contribute to the laminate resistance, taking into account their relative orientation with respect to the loading direction. Figures 5.6 through 5.9 show the favorable situations and those that should be avoided. Recall the Mohr circle:

cf. for example the stress state below and the associated Mohr circle

In Figure 5.7, the Mohr circle for stresses shows that the 45∞ fibers support the compression, s1 = -t (t is the arithmetic value of shear stress), while the resin supports the tension, s2 = t , with low fracture limit. The fibers in Figure 5.8 support the tension, s1 = t, whereas the resin supports the compression, s2 = -t. In Figure 5.9, one has deposited the fibers at 45∞ and –45∞. Taking into account the previous remarks, one observes that the 45∞ fibers can support the tension s1 = t, whereas the -45∞ fibers can support the compression, s2 = -t. The resin is less loaded than previously.

5.2.3 Code to Represent a Laminate 5.2.3.1 Normalized Orientation Considering the working mode of the plies as discussed in the previous section, the most frequently used orientations are represented as in Figure 5.10. The direction called “0∞” corresponds to either the main loading direction, a preferred direction of the piece under consideration, or the axis of the chosen coordinates. Note: One also finds in real applications plies with orientations ±30∞ and ±60∞.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 74 Monday, November 18, 2002 12:09 PM

Figure 5.6 Effect of Ply Orientation

Figure 5.7 Bad Design

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 75 Monday, November 18, 2002 12:09 PM

Figure 5.8 Mediocre Design

Figure 5.9 Good Design

Figure 5.10 Common Orientations

5.2.3.2 Middle Plane By definition the middle plane is the one that separates two half-thicknesses of the laminate. In Figure 5.11, the middle plane is the plane x–y. On this plane, z = 0.

5.2.3.3 Description of Plies The description of plies is done by beginning with the lowest ply on the side z < 0 and proceeding to the uppermost ply of the side z > 0. In so doing, Each ply is noted by its orientation. The successive plies are separated by a slash “/”.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 76 Monday, November 18, 2002 12:09 PM

Figure 5.11 Laminate and its Middle Plane x–y 2

One must avoid the grouping of too many plies of the same orientation. However, when this occurs, an index number is used to indicate the number of these identical plies.

5.2.3.4 Midplane Symmetry One notes that a laminate has midplane symmetry or is symmetric when the stacking of the plies on both sides starting from the middle plane is identical. Example:

Example:

2

This is to limit the interlaminar stresses (see Section 5.4.4 and Chapter 17). This precaution applies also to the fabrics (for example, no more than four consecutive fabric layers of carbon/ epoxy along one direction).

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 77 Monday, November 18, 2002 12:09 PM

Figure 5.12 Effect of Laminate Lay-up on Deformation

5.2.3.4.1 What Is the Need of Midplane Symmetry For the construction of laminated pieces, the successive impregnated plies are stacked at ambient temperature, then they are placed within an autoclave for curing. At high temperature, the extension of the whole laminate takes place without warping. However, during cooling, the plies have a tendency to contract differently depending on their orientations. From this, thermal residual stresses occur. When midplane symmetry is utilized, it imposes the symmetry on these stresses and prevents the deformations of the whole part, for example, warping as shown in Figure 5.12.

5.2.3.5 Particular Cases of Balanced Fabrics Some laminates are made partially or totally of layers of balanced fabric. One then needs to describe on the drawing the composition of the laminate. Example:

The previous laminate, made up of three layers of balanced fabric, has midplane symmetry. In effect, if one considers one woven fabric layer as equivalent to two 3 series of unidirectional layers crossed at 90∞, it also has midplane symmetry. 3

If this hypothesis is to be verified for a plain weave or a taffeta (see Section 3.4.1), and even for a ribbed twill, it becomes worse as long as the pitch of the weaving machine increases (pitch of the plain weave: 2; ribbed twill: 3; 4-harness satin: 4; 5-harness satin: 5; etc.). If one supposes that this pitch is increasing towards infinity, then the woven fabric becomes the superposition of two unidirectional layers crossed at 90∞. It then does not possess midplane symmetry any more. This property can be observed on a unique ply of 5-harness satin of carbon/epoxy as it is cured in an autoclave, which deforms (curved surface) on demolding (see Application 18.2.17).

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 78 Monday, November 18, 2002 12:09 PM

Figure 5.13 Laminate with Balanced Fabrics; Representation 1

As indicated in Section 3.4.2, one can consider the resulting laminate in two 4 different ways : (a) Each layer of fabric is replaced by two identical plies crossed at 90∞, each with thickness equal to half the thickness e of the fabric layer and each with known elastic properties. This representation is convenient for the determination of the elastic properties of the laminate. One then has the equivalencies shown in Figure 5.13. (b) Each layer of fabric is replaced by one anisotropic ply with thickness e for which one knows the elastic properties and failure strengths. This representation is useful for the determination of the rupture stress of the laminate. One then has the equivalencies shown in Figure 5.14.

5.2.3.6 Technological Minimum Generally one uses a minimum amount of plies (from 5 to 10%) for each direction: 5 0∞, 90∞, 45∞, -45∞. The minimum thickness of a laminate should be of the order of one millimeter, for example, eight unidirectional layers, or three to four layers of balanced fabric of carbon/epoxy.

5.2.4 Arrangement of Plies The proportion and the number of plies to place along each of the directions — 0∞, 90∞, 45∞, -45∞—take into account the mechanical loading that is applied to the laminate at the location under consideration. A current case consists of loading 4 5

See Exercises 18.2.9 and 18.2.10. Apart from space applications, where thicknesses are very small, the skins of sandwich plates are laminates which do not have separately midplane symmetry.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 79 Monday, November 18, 2002 12:09 PM

Figure 5.14 Laminate with Balanced Fabrics; Representation 2

Figure 5.15 Stresses and Stress Resultants 6

of the laminate in its plane. This is called membrane loading. The mechanical loadings can take the form of stresses (sx, sy, txy in Figure 5.15a) or stress resultants (Nx, Ny, Txy in Figure 5.15b). The stress resultants are the products of the stresses with the thickness h of the laminate. Generally, three criteria should be considered by the designer for the ply configuration: 1. Support the loading without deterioration of the laminate 2. Limit the deformation of the loaded piece 3. Minimize the weight of the material used These criteria do not always work together. For example, searching for minimum thickness might not be compatible with high rigidity. Searching for high rigidity 6

The laminate can also work in bending. This is studied in Chapters 12 and 17.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 80 Monday, November 18, 2002 12:09 PM

Figure 5.16 Example of Representation

might not be compatible with minimum weight. One will see in Section 5.4 guidelines for proportions values that allows a laminate with minimum laminate thickness to support specified mechanical loading without damage,. Once a laminate is defined (number of layers and orientations), one must respect the following conditions (without forgetting the technological minimum indicated at the end of the previous paragraph) as much as possible: 90∞ plies placed on the surface, then 45∞ and -45∞ plies, when the predominant stress resultant is oriented along the 0∞ direction No more than 4 consecutive plies along the same direction

5.2.4.1 Example of Representation The plies are progressively terminated to obtain a gradual change in thickness (maximum 2 plies for each 6 mm interval). The symbols for the composition of the laminate are shown on plan view (see Figure 5.16).

5.2.4.2 The Case of Sandwich Structure The description of the sandwich material is done as in Figure 5.17.

5.3 FAILURE OF LAMINATES 5.3.1 Damages Figure 5.18 shows schematically different types of failure leading to damage of a laminate. The main modes of damage, when the loads exceed the critical limits, are illustrated in Figure 5.19.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 81 Monday, November 18, 2002 12:09 PM

Figure 5.17 Description of a Sandwich Material

Figure 5.18 Different Modes of Failure

Figure 5.19 Modes of Damage

One cannot be satisfied with the classical maximum stress criterion Figure 5.20 shows a unidirectional laminate loaded successively in two different manners. In the two cases, the maximum normal stress has the same value denoted

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 82 Monday, November 18, 2002 12:09 PM

Figure 5.20 Stresses and Fiber Orientation

as s. In the loading case (a), the unidirectional specimen will rupture when

s > srupture along This is the maximum stress criterion. In the loading case (b), the maximum normal stress occurs in a direction that is different from that of the fibers (one can obtain this by tracing the Mohr’s circle as discussed previously). We have seen (Section 3.3.2) that the rupture resistance decreases. It is weaker than the situation of case (a). The unidirectional laminate therefore ruptures when

s < srupture along This phenomenon is more evident if the unidirectional laminate is loaded in a direction transverse to the fibers t. In this case, the laminate rupture resistance is that of the matrix, which is much less than that of the fibers. Taking into consideration the evolution of the rupture resistance with the loading direction, one can not use a simple maximum stress criterion as for the classical metallic materials.

5.3.2 Most Frequently Used Criterion: Hill–Tsai Failure Criterion

7

One can apply this criterion successively to each ply of the laminate, that is for each one of the orientations 0∞, 90∞, ±45∞ that have been considered. As has been discussed in Chapter 3, the axes of a unidirectional ply are denoted as for the direction along the fibers, and t for the transverse direction. The stresses are denoted as s in the fiber direction, st in the direction transverse to the fibers, and tt for the shear stress (see figure below). One denotes the Hill–Tsai number (see Figure 5.21) the number a such that If a < 1: no ply rupture occurs. If a ≥ 1: rupture occurs in the ply considered. Generally, this deterioration is due to the rupture of the resin. The mechanical properties of a broken ply become almost negligible, except for those along the fiber direction (modulus of elasticity and rupture resistance) 7

For more detailed study of this criterion, see Chapter 14.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 83 Monday, November 18, 2002 12:09 PM

Figure 5.21 Hill–Tsai Number

5.3.2.1 Notes Attention: The rupture resistance srupture does not have the same value in tension and in compression (see, for example, Section 3.3.3). It is therefore useful to place in the denominators of the previous Hill–Tsai expression the rupture resistance values corresponding to the mode of loading (tension or compression) that appear in the numerator. Using this criterion, when one detects the rupture of one of the plies (more precisely the rupture of the plies along one of the four orientations), this does not necessarily lead to the rupture of the whole laminate. In most cases, the degraded laminate continues to resist the applied stress resultants. In increasing these stress resultants, one can detect which orientation can produce new rupture. This may—or may not—lead to complete rupture of the laminate. If complete rupture does not occur, one can still increase 8 the admissible stress resultants. In this way one can use a multiplication factor on the initial critical loading to indicate the ratio between the first ply rupture and the ultimate rupture. As a consequence of the previous remark it appears possible to work with a laminate that is partially degraded. It is up to the designer to consider the finality of the application, to decide whether the partially degraded laminate can be used. One can make a parallel–in a gross way–with the situation of classical metallic alloys as represented in Figure 5.22.

5.3.2.2 How to Determine s, st, tt in Each Ply Consider for example the laminate shown in Figure 5.23, consisting of identical plies. The following characteristics are known:

8

See Exercise 18.2.7.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 84 Monday, November 18, 2002 12:09 PM

Figure 5.22 Comparison of Behavior until Failure Between Metal and Laminated Material

Figure 5.23 Average Stresses

the mechanical properties of the basic ply the proportions (percentages) of plies in each of the directions (0∞, 90∞, 45∞, -45∞) the global values of the applied stresses, here, for example, sx and txy One considers this case of loading as consisting of the superposition of two simple loading cases: sx only, and then txy only. For each of these cases of elementary loadings, one looks for the stresses s, st, tt in each ply. Manual calculation is 9 usually too long. It should be replaced by using a computer. Appendix 1 has tables for stress values for carbon/epoxy plies with 60% fiber volume fraction. Subsequently, one finds, always for each ply, the sum of the stresses s , st, and tt, respectively, due to each of the simple loadings sx and txy. It is then possible to calculate the Hill–Tsai number to verify the integrity of each of the plies. In the Application 18.1.6, there is an example to determine the thickness of a laminate subject to this type of combined loading.

9

The procedure for this calculation is described in Section 12.1.3.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 85 Monday, November 18, 2002 12:09 PM

5.4 SIZING OF THE LAMINATE 5.4.1 Modulus of Elasticity. Deformation of a Laminate For the varied proportions of plies in the 0∞, 90∞, ±45∞, the tables that follow allow the determination of the deformation of a laminated plate subject to the applied stresses. For this one uses a stress–strain relation similar to that described in Section 3.1 for an anisotropic plate, which is repeated below:

Ex, Ey, Gxy, nxy, nyx are the modulus of elasticity and Poisson ratios of the laminate, and ex, ey, gxy are normal and shear strains in the plane xy. Example: What are the elastic moduli and thermal expansion coefficients for a glass/epoxy laminate (Vf = 60%) with the following ply configuration?

10

Answer: Table 5.14 indicates the following values for this laminate: Ex = 33,100 MPa Ey = 17,190 MPa (this value is obtained by permuting the proportions of 0∞ and 90∞) nxy = 0.34 nyx = 0.17 Table 5.15) shows Gxy = 6,980 MPa. One then obtains the strains ex, ey, gxy, when the stresses are known, using the matrix relation mentioned above. -5 For the coefficient of thermal expansion, Table 5.14 shows: ax = 0.64 ¥ 10 -5 and ay = 1.21 ¥ 10 by permuting the proportions of 0∞ and 90∞.

10

Recall (Sections 3.1 and 3.2) that uxy/Ex = uyx/Ey .

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 86 Monday, November 18, 2002 12:09 PM

5.4.2 Case of Simple Loading The laminate is subjected to only one single stress: sx or sy or txy. Depending on the percentages of the plies in the four directions, one would like to know the order of magnitude of the stresses that can cause first ply failure in the laminate.

Tables 5.1 through 5.15 indicate the maximum stresses as well as the elastic characteristics and the coefficients of thermal expansion for the laminates having the following characteristics: Materials include carbon, Kevlar, glass/epoxy with Vf = 60% fiber volume fraction. All have identical plies (same unidirectionals, same thickness). The laminate is balanced (same number of 45∞ and -45∞ plies). The midplane symmetry is realized. The percentages of plies along the 4 directions 0∞, 90∞, ±45∞ vary in increments of 10%. Calculation of the maximum stresses sx max, sy max, txy max is done based on the Hill–Tsai 11 failure criterion. Example of how to use the tables:

Which maximum tensile stress along the 0∞ direction can be applied to a Kevlar/ epoxy laminate containing 60% fiber volume with the orientation distribution as shown in the above figure? Answer: Table 5.6 indicates the maximum stress in the 0∞ direction (or x). For the percentages given, one has:

sx max(tension) = 308 MPa 11

See Application 18.2.2.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 87 Monday, November 18, 2002 12:09 PM

Table 5.1 Carbon/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Maximum stress sx max (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

Example:

Which maximum compression stress along the 90∞direction (or y) can be applied to a carbon/epoxy laminate containing 60% fiber volume fraction with the orientation distribution as shown in the above figure?

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 88 Monday, November 18, 2002 12:09 PM

Table 5.2 Carbon/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Maximum stress symax (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

Answer: Table 5.2 shows the maximum stresses in the 90∞ direction. For this configuration, one has

symax = s13/67/10/10 = s10/60/15/15 + Ds = 744 + Ds 0∞

Denoting p and p one has

90∞

as the proportions of the plies along the 0∞ and 90∞ directions,

∂s ∂s 0∞ - ¥ Dp 90∞ D s = --------¥ Dp + ---------0∞ 90∞ ∂p ∂p

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 89 Monday, November 18, 2002 12:09 PM

Table 5.3 Carbon/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Maximum stress txymax (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

One obtains by linear interpolation: 3 7 D s = ( 747 – 744 ) ¥ ------ + ( 846 – 744 ) ¥ ------ = 72 MPa 10 10 Therefore,

sy max = 744 + 72 = 816 MPa Remark: The plates that show the maximum stresses are not usable for the balanced fabrics. In effect, the compression strength values of a layer of balanced

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 90 Monday, November 18, 2002 12:09 PM

Table 5.4 Carbon/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Modulus Ex (MPa), Poisson ratio uxy and coefficient of thermal expansion ax as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

fabric are smaller than what is obtained when one superimposes the unidirectional 12 plies crossed at 0∞ and 90∞ in equal quantities in these two directions.

5.4.3 Case of Complex Loading—Approximate Orientation Distribution of a Laminate When the normal and tangential loadings are applied simultaneously onto the laminate, the previous tables are not valid because they were established for the 12

Also see remarks in Section 3.4.2.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 91 Monday, November 18, 2002 12:09 PM

Table 5.5 Carbon/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Shear modulus Gxy (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

cases of simple stress states. However, one can still use them to effectively obtain 13 a first estimate of the proportions of plies along the four orientations. The principle is as follows: Consider the case of complex loading and replacing the stresses with the stress resultants Nx, Ny, Txy which were defined in Section 5.2.4. In general these stress resultants constitute the initial numerical data that are given by some previous studies. One then can assume that each one of the three stress resultants is associated with an appropriate orientation of the plies following the remarks made in Section 5.2.2. 13

Attention: What follows is for the determination of proportions, and not thicknesses.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 92 Monday, November 18, 2002 12:09 PM

Table 5.6 Kevlar/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Maximum stress sxmax (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞,-45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

Using this hypothesis, Nx, assumed to be supported by the 0∞ plies (or along x), requires a thickness ex for these plies such that: Nx e x = -----------------s rupture where s rupture is the rupture stress of a unidirectional ply in the long direction. In the same manner, Ny is supposed to be supported by the 90∞ plies (or along y), and requires a thickness for these plies of Ny e y = -----------------s rupture

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 93 Monday, November 18, 2002 12:09 PM

Table 5.7 Kevlar/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Maximum stress symax (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

Finally, Txy is assumed to be supported by the ±45∞ plies and requires a thickness for these plies of T xy e xy = ------------t rupture where trupture is the maximum stress that a ±45∞ laminate can support.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 94 Monday, November 18, 2002 12:09 PM

Table 5.8 Kevlar/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Maximum stress txy max (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

One then can retain for the complete laminate the proportions indicated below.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 95 Monday, November 18, 2002 12:09 PM

Table 5.9 Kevlar/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Longitudinal modulus Ex (MPa), Poisson ratio uxy and coefficient of thermal expansion ax as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

Example: Determine the composition of a laminate made up of unidirectional plies of carbon/epoxy (Vf = 60%) to support the stress resultants Nx = -800 N/mm, Ny = -900 N/mm, Txy = -300 N/mm. The compression strength s rupture is 1,130 MPa (see Section 3.3.3, or Table 5.1 for 100% of 0∞ plies). Then: 800 900 e x = ------------ = 0.71 mm; e y = ------------ = 0.8 mm 1130 1130

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 96 Monday, November 18, 2002 12:09 PM

Table 5.10 Kevlar/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Shear modulus Gxy (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

The optimum shear strength trupture is given in Table 5.3 for 100% ±45∞, then:

trupture = 397 MPa from which: 340 e xy = --------- = 0.86 mm 397

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 97 Monday, November 18, 2002 12:09 PM

Table 5.11 0.13 mm

Glass/Epoxy Laminate: Vf = 60%, Ply Thickness =

Maximum stress s x max (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

One obtains for the proportions at ex - = 0.3 0∞: --------------------------e x + e y + e xy ey - = 0.34 90∞: --------------------------e x + e y + e xy e xy - = 0.36 ± 45∞: --------------------------e x + e y + e xy

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 98 Monday, November 18, 2002 12:09 PM

Table 5.12 0.13 mm

Glass/Epoxy Laminate: Vf = 60%, Ply Thickness =

Maximum stress sy max (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

One can then retain for the composition of the laminate the following approximate values:

Remark: The thicknesses ex, ey, exy evaluated above only serve to determine the proportions. After that, they should not be kept. In effect each orientation really

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 99 Monday, November 18, 2002 12:09 PM

Table 5.13 0.13 mm

Glass/Epoxy Laminate: Vf = 60%, Ply Thickness =

Maximum stress txy max (MPa) as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

supports a part of each stress resultant. For example, the 0∞ plies cover the major part of stress resultant Nx, but they also support a part of stress resultant Ny and a part of stress resultant Txy. This then results in a more unfavorable situation for each orientation as compared with what has been assumed previously. The minimum necessary thickness of the laminate will in fact be larger than the previous result (ex + ey + exy ), which therefore appears to be dangerously optimistic. The practical determination of the minimum thickness of the laminate is determined based on the Hill–Tsai failure criterion, as indicated at the end of Section 5.3.2, and explained in details in Application 18.1.6. Also, with the same stress resultants and proportions as in the previous example, one finds a minimum thickness of 2.64 mm (see Application 18.1.6, in Chapter 18), whereas the previous sum (ex + ey + exy) gives a thickness of 2.37 mm, 10% lower than the required minimum thickness (2.64 mm).

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 100 Monday, November 18, 2002 12:09 PM

Table 5.14 Glass/Epoxy Laminate: Vf = 60%, Ply Thickness = 0.13 mm

Longitudinal modulus Ex (MPa), Poisson ratio uxy , and coefficient of thermal expansion a x as a function of the ply percentages in the directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply: see Section 3.3.3)

5.4.4 Case of Complex Loading: Optimum Composition of a Laminate Estimation of the proportions in the previous paragraph does not lead to an optimum laminate in general. An optimum laminate is the one with the smallest thickness among all laminates of different compositions that can support the given combined stress resultants Nx, Ny, Txy. 14 Tables 5.15 through 5.19, based on Hill-Tsai criterion, give the optimum compositions of laminates based on unidirectionals of carbon/epoxy for the various 14

See Section 5.3.2.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 101 Monday, November 18, 2002 12:09 PM

Table 5.15 0.13 mm

Glass/Epoxy Laminates. Vf = 60%. Ply Thickness =

Shear modulus Gxy as a function of percentages of plies in directions 0∞, 90∞, +45∞, -45∞. (More information on modulus and strength of a basic ply, see Section 3.3.3).

stress resultants Nx, Ny, Txy. The indicated compositions correspond to laminates that are capable of supporting the specified stress resultants and at the same time keeping a minimum thickness. One can see this number, in millimeters, within the circles, when the arithmetic sum of the stress resultants is equal to 100 N/mm. Also represented in the tables are The direction along which the first ply failure will occur. The multiplication factor for the stress resultants in order to go from first ply failure to ultimate fracture of the laminate. The two compositions that are closest to the optimum composition, obtained by varying the indicated composition along the direction of the arrows.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 102 Monday, November 18, 2002 12:09 PM

First, the arrows in increasing solid line or decreasing solid line denote the increase or decrease of 5% in terms of the proportions marked. Next, the arrows in increasing broken line or decreasing broken line denote the increase or decrease of 5% in terms of the proportions marked. Example: Given the stress resultants: Nx = 720 N/mm;

Ny = 0;

Txy = 80 N/mm

one can then deduce values of the reduced stress resultants: N x = 720/ ( 720 + 80 ) = 0.9;

N y = 0;

Txy = 80/ ( 720 + 80 ) = 0.1

One then uses Table 5.16 (all stress resultants are positive), where one can obtain for these values of reduced stress resultants the following figure:

This can be interpreted as follows: Optimal composition of the laminate 70% of 0∞ plies (along x direction) 10% of 90∞ plies 10% of plies in 45∞, 10% of plies in –45∞ Critical thickness of the laminate: 0.156 mm when the arithmetic sum of the 3 stress resultants is equal to 100 N/mm. For this thickness, the first ply failure occurs in the 90∞ plies. However, one can continue to load this laminate until it reaches 1.33 times the critical load, as: Nx = 1.33 ¥ 720 = 957 N/mm;

Ny = 0

Txy = 1.33 ¥ 80 = 106 N/mm At this point, there is complete rupture of the laminate. Returning to our example, the arithmetic sum of the stress resultants is equal to 720 + 80 = 800 N/mm. Then, the thickness of the laminate has to be more than: 8 ¥ 0.156 = 1.25 mm Neighboring compositions: The second smallest thickness in the vicinity is obtained by modifying the indicated composition in the direction specified by the arrows in solid line, as

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 103 Monday, November 18, 2002 12:09 PM

Table 5.16 Optimum Composition of a Carbon/Epoxy Laminate

Vf = 0.6, 10% minimum in each direction of 0∞, 90∞, +45∞, -45∞. (Ply characteristics: see Appendix 1 or Section 3.3.3).

One then obtains (not shown on the plate) a thickness of 0.160 mm (increase of 2.5% relative to the previous value) and a multiplication factor for the loading equal to 1.35. Continuing in the direction of increasing thickness, the third smallest thickness in the immediate vicinity is obtained by modifying the indicated composition in the direction specified by the arrows in broken line, as:

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 104 Monday, November 18, 2002 12:09 PM

Table 5.17 Optimum Composition of a Carbon/Epoxy Laminate

Vf = 0.6, 10% minimum in each direction of 0∞, 90∞, +45∞, -45∞. (Ply characteristics: see Appendix 1 or Section 3.3.3).

One then obtains a thickness (not shown on the plate) of 0.165 mm (increase of 6%) and a multiplication factor of 1.3 for the load. Example: Given the stress resultants Nx = 600 N/mm; Ny = -300 N /mm; Txy = 100 N/mm The corresponding reduced stress resultants are N x = .6; N y = – .3 ; T xy = 0.1 N/mm One obtains from Table 5.18:

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 105 Monday, November 18, 2002 12:09 PM

Table 5.18 Optimum Composition of a Carbon/Epoxy Laminate

Vf = 0.6, 10% minimum in each direction of 0∞, 90∞, +45∞, -45∞. (Ply characteristics: see Appendix 1 or Section 3.3.3).

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 106 Monday, November 18, 2002 12:09 PM

Table 5.19 Optimum Composition of a Carbon/Epoxy Laminate

Vf = 0.6, 10% minimum in each direction of 0∞, 90∞, +45∞, -45∞. (Ply characteristics: see Appendix 1 or Section 3.3.3).

where Critical thickness is 10 ¥ 0.152 = 1.52 mm These are the 90∞ plies that fail first. Complete rupture of the laminate occurs when: Nx = 1.29 ¥ 600 = 774 N/mm Ny = 1.29 ¥ -300 = -387 N/mm Txy = 1.29 ¥ 100 = 129 N/mm

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 107 Monday, November 18, 2002 12:09 PM

The closest critical thicknesses (in increasing order) are obtained with the following successive compositions:

Remarks: A few loading cases can lead to several distinct optimum compositions, but with identical thicknesses. For example the reduced stress resultants: N x = N y = 0.5; T xy = 0 This is a case of isotropic loading, the Mohr circle is reduced to one point (see figure below).

Table 5.16 indicates

One obtains in this case a unique critical thickness of 0.161 mm (corresponding 15 to a sum Nx + Ny = 100 N/mm) independent of the proportion p. The isotropic composition (25%, 25%, 25%, 25%) in the directions 0∞, 90∞, +45∞, –45∞, which appears intuitive, can in fact be replaced by compositions that present the values of modulus of elasticity that are varied and adaptable to the designer in the 16 directions 0∞, 90∞ 45∞, or -45∞, or even a, a + p /2 with a certain a. 15 16

See Section 18.2.8. See Section 5.4.2, Table 5.4.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 108 Monday, November 18, 2002 12:09 PM

In some loading cases, one finds from the table only arrows in a solid line. For example, for the following reduced stress resultants: N x = 0.3;

N y = 0;

T xy = 0.7

one finds from Table 5.16 the following figure:

The three neighboring optimum compositions in increasing order are

(The thicknesses of 0.255 mm and 0.262 mm are not indicated on the plate). The third composition, characterized by an increase in thickness of 0.252 to 0.262 mm, or 6%, leads to an increase in modulus of elasticity in the x (0∞) by 36% (see Section 5.4.2, Table 5.4). One can note finally that for the majority of cases, the optimum compositions 17 indicated in Tables 5.16 to 5.19 are not easy to postulate using intuition.

5.4.5 Practical Remarks: Particularities of the Behavior of Laminates 18

The fabrics are able to cover the left surfaces due to pushing action in warp and fill directions. The radii of the mold must not be too small. This concerns particularly the inner radius Ri as shown in Figure 5.24. The graph gives an idea for the minimum value required for the inner and outer radii. The thickness of a polymerized ply is not more than 0.8 to 0.85 times that of a ply before polymerization. This value of the final thickness must also take into account a margin of uncertainty on the order of 15%. When one unidirectional sheet does not cover the whole surface required to constitute a ply, it is necessary to take precautions when cutting the different pieces of the sheet. A few examples of wrapping are given in Figure 5.25. The unidirectional sheets do not fit well into sharp corners in the fiber direction. The schematic in Figure 5.26 shows the dispositions to accommodate sudden changes in draping directions. 17 18

See Exercise 18.1.6. It is more difficult for the plain weave than for the satins, due to the mode of weaving (See Section 3.4.1).

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 109 Monday, November 18, 2002 12:09 PM

Figure 5.24 Minimum Required for Inner and Outer Radii of Mold

Figure 5.25 Recommended Arrangement for Cutting

Figure 5.26 Method to Lay up at Corner

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 110 Monday, November 18, 2002 12:09 PM

Figure 5.27 Corner Situations

Figure 5.28a Three Plies in Separate Positions

Delaminations: When the plies making up the laminate separate from each other, it is called delamination. Many causes are susceptible to provoke this deterioration: An impact that does not leave apparent traces on the surface and can lead to internal delaminations. A mode of loading leads to the disbond of the plies (tension over the interface) as shown in Figure 5.27. Shear stresses at the interfaces between different plies, very near the edges of the laminates, which one can make evident as follows (with a three-ply laminate): 1. Consider the three plies in Figure 5.28(a), separated. Under the effect of loading (right-hand-side figure), they are deformed independently and do not fit with each other when they are put together. 2. Now the plies constitute a balanced laminate. Under the same loading, they deform together, without distorsion, as shown in Figure 5.28(b). 3. This is because interlaminar stresses occur on the bonded faces. One can show that these stresses are located very close to the edges of the laminate, as illustrated in Figure 5.28(c).

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 111 Monday, November 18, 2002 12:09 PM

Figure 5.28b Three Plies, Together

Figure 5.28c Stresses at Free Edge

A complex state of stresses at the interface, due to local buckling, for example (see Figure 5.29). Practical as well as theoretical studies of these interlaminar stresses are difficult, and the phenomenon is still not well understood.

Why is Fatigue Resistance so Good? Paradox: Glass is a very brittle material (no plastic deformation). The resin is also often a brittle material. (for example, epoxy). However, the association of reinforcement/matrix constituted of these two materials opposes to the propagation of cracks and makes the resultant composite to endure fatigue remarkably. Explanation: When the cracks propagate, for example, in the unidirectional layer shown schematically in Figure 5.30 in the form of alternating of fibers and

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 112 Monday, November 18, 2002 12:09 PM

Figure 5.29 Delamination Due to Buckling at Interface

Figure 5.30 Crack Propagation in Composites

resin, the initial stress concentration at the end of the crack leads to failure in the resin. The fibers, then debonded, benefit from a relaxation of the stresses. There is no more stress concentrations as in a homogeneous material. Laminated tubes can be obtained by winding of filaments, rubans of unidi19 rectionals or fabrics. In a first approximation, one can estimate the strains and stresses in flexure and in torsion from the relations in Figure 5.31 in which Ex and Gxy are the moduli of elasticity in the tangent plane x,y. I and Io are respectively the quadratic moment of inertia and polar moment of inertia (Io = 2I). Y is the coordinate of a point in the section (in the undeformed position) in the X, Y, Z coordinates. r is the average radius of the tube.

19

For a complete study of the flexure and torsion of the composite beams, See Section 15 and 16.

© 2003 by CRC Press LLC

TX846_Frame_C05 Page 113 Monday, November 18, 2002 12:09 PM

Figure 5.31 Composite Tube Relations

© 2003 by CRC Press LLC

6 JOINING AND ASSEMBLY We have seen previously how to design a laminate to support loads. A second fundamental aspect of the design of a composite piece consists of the design for the attachment of the composite to the rest of the structure. Here we will examine the assembly problems involving riveting, bolting, and bonding: of a composite part to another composite part and of a composite part to a metallic part.

6.1 RIVETING AND BOLTING In all mechanical components, the introduction of holes gives stress concentration factors. Specifically in composite pieces, the introduction of holes (for molded-in holes or holes made by drilling) induces weakening of the fracture resistance in comparison with the region without holes by a factor of 40 to 60% in tension 15% in compression Example: Figure 6.1 presents the process of degradation before rupture of a glass/epoxy laminate containing a free hole, under uniaxial stress. Causes of hole degradation: Stress concentration factors: The equilibrium diagrams shown in Figure 6.2 demonstrate the increase in stress concentration in the case of a laminate. For the case of slight (and usually neglected) press-fit of the rivet, the stresses shown in these figures are:

s ¢M > s in a region where:

slocal rupture < slaminate rupture

© 2003 by CRC Press LLC

Figure 6.1 Cracks in a Laminate with Hole when Load Increases

Figure 6.2 Stress Concentration Factors

with the maximum stress s ¢M in the laminate given as: Ï E ¸ E sM¢ = s ¢ ¥ Ì 1 + 2 ÊË -----x – n xyˆ¯ + -------x- ˝ G E xy ˛ y Ó where

Ex and Ey are the moduli of elasticity in the 0∞ and 90∞ directions Gxy is the shear modulus nxy is the Poisson ratio

© 2003 by CRC Press LLC

Figure 6.3 Weakened Zones Due to Presence of Holes

Bearing due to lateral pressure: This is the contact pressure between the shaft of the assembly device (rivet or bolt) and the wall of the hole. When this pressure is excessive, it leads to mushrooming and delamination of the laminate. In consequence: The resistance of a hole occupied by the rivet or bolt is weaker than that of an empty hole: decrease on order of 40%). Fracture of fibers during the hole cutting process, or the misalignment of fibers if the hole is made before polymerization: Figure 6.3 illustrates the correlation between the weakened zones consecutive to rupture of fibers and the “overstressed” zones.

6.1.1 Principal Modes of Failure in Bolted Joints for Composite Materials These are represented in Figure 6.4.

6.1.2 Recommended Values Pitch, edge distance, thickness (see Figure 6.5) Orientation of plies: Recommendation for percentages of plies near the holes (see Figure 6.6). © 2003 by CRC Press LLC

Figure 6.4

Different Types of Bolt Joint Failures

Condition of nonbearing pressure: In Figure 6.7, F and T designate the normal and shear loads respectively, that are applied on the assembly over a width equal to one pitch distance. The equivalent bearing pressure which leads to the crushing of the wall of the hole of diameter Ø, is F/(Ø ¥ e). It must remain smaller than an admissible maximum, as: F ------ £ s carbon: s admissible bearing = 500 MPa f e admissible bearing pressure glass: t admissible bearing = 300 MPa © 2003 by CRC Press LLC

Figure 6.5 Recommended Pitch, Edge Distance, and Thickness

Figure 6.6 Recommended Orientation

Figure 6.7 Normal and Shear Loads on Assembly

Evaluation of the admissible stresses: The principle of calculation consists of magnifying the stresses that are given by elementary considerations, 1 by means of the empirical coefficients of magnification : 1

When one takes into account the aging of the piece, an additional 10% is applied to the maximum stresses.

© 2003 by CRC Press LLC

Due to the presence of the hole and Due to pressure of contact or bearing on the wall of the hole (rivet, bolt). With the notations of Figure 6.7, one has: F 1 F s magnified = --- ÊË --- + 0.2 ------ˆ¯ a S fe tension: a = 0.6 compression: a = 0.8 1 T t magnified = ------- --0.7 S One must also verify that these stresses are admissible (that is, they do not lead to the fracture of the ply) by using the method of verification of fracture described in Paragraph 5.3.2.

6.1.3 Riveting The relative specifics and recommendations for riveting the composite parts can be presented as follows: Do not hit the rivets as this can lead to poor resistance to impact of the laminates. Pay attention to the risk of “bolt lifting” of the bolt heads due to small thickness of the laminates. Note the necessity to assure the galvanic compatibility between the rivet and the laminates to be assembled. Riveting accompanied by bonding of the surfaces to be assembled provides a gain in the mechanical resistance on the order of 20 to 30%. On the other hand, the disassembly of the joint becomes impossible, and the weight is increased. Characteristics of rivets for composites are shown in Figure 6.8.

6.1.4 Bolting Examine a current example that requires a bolted joint. 2

Example: Junction of a panel by bolted joint (simple case) : Consider a sandwich panel fixed to a support component that is subjected to simple loadings that can be represented by a shear load and a bending moment (see Figure 6.9). One expects an attachment using bolt. As shown in the schematics of Figure 6.10, even if the bolt is not tightened, it is able to act to equilibrate the bending moment. However, action of the shear load will separate the facings. 2

A more complete case on the fixation of the panel is examined in the application in Paragraph 18.1.6.

© 2003 by CRC Press LLC

Figure 6.8 Different Types of Riveting

Figure 6.9 Junction of a Panel using Bolted Joint

© 2003 by CRC Press LLC

Figure 6.10 Local behavior without Bolt Tightening

Figure 6.11 Bolt tightening Reduces the Possibility of Damage

It is the tightening of the bolt that will lead to a distribution of contact pressure between the support component and the facings. The sum of the forces due to this contact pressure will balance out the shear load, while suppressing the risk of separating the facings (see Figure 6.11). The tightening of the bolt is therefore indispensable. However, the laminated facings being fragile cannot admit high contact pressures that are localized under the bolt head and under the nut. This leads to the insertion of metallic washers as shown in Figure 6.12. The bolting accompanied by bonding of the surfaces provides a gain in mechanical resistance on the order of 20 to 30%. On the other hand, the joint cannot be disassembled, and there is an increase in weight.

6.2 BONDING Remember briefly that this assembly technique consists of the adhesion by molecular attraction between two parties to be bonded and an adhesive that must be able to transfer the loads. One can cite the principal advantages of this mode of joining: © 2003 by CRC Press LLC

Figure 6.12 Configuration for Bolted Joints

Figure 6.13 Curing of Adhesive

distribution of stresses over an important surface possibility to optimize the geometry and dimensions of bonding light weight of the assembly insulation and sealing properties of adhesive

6.2.1 Adhesives Used The adhesives used include:

epoxies polyesters polyurethanes methacrylates

In all cases, the mechanism of curing is shown schematically in Figure 6.13. The adhesives are resistand simultaneously to high temperatures (>180∞C) humidity a number of chemical agents © 2003 by CRC Press LLC

Figure 6.14 Stresses in Bolted Joint

Figure 6.15 Fracture Modes in a Bonded Joint

The pieces to be assembled have to be surface treated. This consists of three steps: degreasing surface cleaning protection of cleaned surface The case of metal–laminate bond: The differences in physical properties of the constituents requires that the adhesive must compensate for the differences in thermal dilatations elongation under stress The schematic in Figure 6.14 indicates in an exaggerated manner the deformed configuration of a double bonded joint. This shows the role of the adhesive and the gradual transmission of the load from the central piece to the external support. Fracture of a bonded assembly can take dif ferent forms, as indicated in Figure 6.15.

6.2.2 Geometry of the Bonded Joints One must, as much as possible, envisage the joint geometries that allow the following specifications: the adhesive joint must work in shear in its plane tensile stresses in the joint must be avoided Consequently, the transmission of the loads will be dependent on the geometries, as shown in Figure 6.16. A double sided joint with increasing thickness is shown in Figure 6.17. Transmission of couples is shown in Figure 6.18. © 2003 by CRC Press LLC

Figure 6.16 Different Designs for Bonded Joints

Figure 6.17 Double Sided Lap Joint

6.2.3 Sizing of Bonded Surfaces The resistance of the adhesive is characterized by its shear strength trupture. This resistance varies with the process of bonding (cold bonding or hot bonding). For epoxy adhesive, one can cite the following values: Cold bonding: (Araldite): Adhesive thickness = 0.2 mm

trupture = 10 MPa at 20∞C = 3 MPa at 80∞C © 2003 by CRC Press LLC

Figure 6.18 Design for the Transmission of Couples

Figure 6.19 Curing Cycle of Epoxy Adhesive

Hot bonding: Polymerization temperature is between 120∞C and 180∞C:

t rupture = 15 to 30 MPa from 20∞C to 100∞C The diagram in Figure 6.19 shows, for example, the cycle of polymerization of an epoxy adhesive “REDUX 914.” Denoting ec for the thickness of the adhesive joint, one has for an order of magnitude: 0.1 mm £ ec £ 0.3 mm when the joints are very thick, one adds adhesive glass powder or cut fibers. © 2003 by CRC Press LLC

Figure 6.20 Scarf Joint

Figure 6.21 Configurations of Parallel Joint

Figure 6.22 Stresses in Adhesive

Scarf joint: This joint (see Figure 6.20) allows one to obtain a sufficient bonding surface, with weak tensile stress. Parallel joint: As illustrated in Section 6.2.2, there is bending in the bonded parts. The geometric configurations are varied (see Figure 6.21). When one isolates the bonded zone, the stress variation is shown in the figure on the right-hand side of Figure 6.22 (the bond width is assumed to be equal to unity) The stresses in the adhesive (Figure 6.22) consists essentially of a shear stress t and a normal stress called “peel stress” s. © 2003 by CRC Press LLC

Figure 6.23 Maximum Shear Stress

These stresses present maximum values sM and tM very close to the edges of the adhesive. These maxima can be approached by superposition of the partial maxima created by each of the resultants N, T, Mf, by means of the following expressions in which Ec is the modulus of the adhesive, and E1 and E2 are the moduli along the horizontal direction of the bonded parts 1 and 2. One can also write: Gc -; a 1 = -------------E1 e1 ec

Gc -; a 2 = -------------E2 e2 ec

12E c -; b 1 = -------------3 E1 e1 ec

12E c b 2 = -------------3 E2 e2 ec

Maximum shear stresses are illustrated in Figure 6.23 Maximum peel stress is shown in Figure 6.24.

Remarks: The resultants N, T, Mf are evaluated per unit width of the bond. When several resultants coexist, one obtains the total maximum shear stress by superposition of the partial maxima of shear stresses and the maximum peel stress by superposition of the partial maxima of peel stresses. When the lower piece is also subjected to the resultants, the previously obtained relations are usable, by means of permuting the indices 1 and 2, and by changing the sign of the second member © 2003 by CRC Press LLC

Figure 6.24 Maximum Peel Stress 3

Limits for the relations

a b 0.6 £ -----1 and -----1 £ 2 a2 b2 ( a1 + a2 ) ¥ ≥ 9 2

( b1 + b2 ) ¥ ≥ 4 ¥ 6 4

4

Example: For the simple lap joint below, one has (with the notations used previously)

e1 + e2 - + e cˆ N = F ; M f = F ¥ Ê -------------Ë 2 ¯

t M = t M( N ) + t M( M ) ; s M = s M( M ) f

f

This is valuable if a1, a2, b1, b2 respect the limits of utilization written above. Collar (see Figure 6.25) 4 Cylindrical sleeve (see Figure 6.26)

3

4

For more details, see Bibliography: “Elastic Analysis and Engineering Design Formulae for Bonded Joints.” For different thicknesses and different materials to be assembled, see Exercise 18.3.1.

© 2003 by CRC Press LLC

Figure 6.25 Shear Stresses in Simple Collar

Figure 6.26 Shear Stresses in Cylindrical Sleeve

Figure 6.27 Ply Orientation in Bonded Laminates

In a laminate, orientation of the plies that are in contact with the joint influences strongly the failure by fiber–resin decohesion. This can be easily understood through Figure 6.27. A tensile load in plies that are in contact with the adhesive requires that fiber orientation in these plies must be along the direction of the load. © 2003 by CRC Press LLC

Figure 6.28 An example of Laminate Bonding

Figure 6.29 Bonding of Sandwich Facings

6.2.4 Examples of Bonding Laminates One notes in Figure 6.28 the use of steps that gradually decrease the thickness of titanium piece. Note also that the design allows one to separate the str ess concentration effects localized at the beginning of each step. Sandwiches (see Figure 6.29) The bonding at the borders of sandwich panels must be done in a simple manner (especially for the preparation of the core) and with the best possible contact for the bonded parts, similar to the cases shown in Figure 6.30.

6.3 INSERTS It seems necessary to include in composite parts reinforcement pieces, or “inserts,” which may be used to attach to the surrounding structure. The inserts decrease the transmitted stresses to admissible values for the composite part. The case of sandwich pieces: One frequently finds the metallic inserts following the schematics in Figure 6.31. © 2003 by CRC Press LLC

Figure 6.30 Different Sandwich Facing Designs

Figure 6.31 Inserts in Sandwich Construction

The case of pieces under uniaxial loads: Tensile load (see Figure 6.32) Compression load (see Figure 6.33) Tension–compression load (see Figure 6.34) Arrangement that allows the increase of the bonded surfaces is shown in Figure 6.35.

© 2003 by CRC Press LLC

Figure 6.32 Composite Piece Under Tensile Load

Figure 6.33 Composite Piece under Compression Load

Figure 6.34 Composite Piece under Tension-compression Load

Figure 6.35 Arrangement to Increase Bond Surface

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 135 Monday, November 18, 2002 12:17 PM

7 COMPOSITE MATERIALS AND AEROSPACE CONSTRUCTION Aeronautical constructors have been looking for light weight and robustness from composites since the earlier times. As a brief history: In 1938, the Morane 406 plane (FRA) utilized sandwich panels with wood core covered with light alloy skins. In 1943, composites made of hemp fiber and phenolic resin were used on the Spitfire (U.K.) airplane. Glass/resin has been used since 1950, with honeycombs. This allows the construction of the fairings with complex forms. Boron/epoxy was introduced around 1960, with moderate development since that time. Carbon/epoxy has been used since 1970. Kevlar/epoxy has been used since 1972. Experiences have proved that the use of composites allows one to obtain weight reduction varying from 10% to 50%, with equal performance, together with a cost reduction of 10% to 20%, compared with making the same piece with conventional metallic materials.

7.1 AIRCRAFT 7.1.1 Composite Components in Aircraft Currently a large variety of composite components are used in aircrafts. Following the more or less important role that composites play to assure the integrity of the aircraft, one can cite the following: Primary structure components (integrity of which is vital for the aircraft): © 2003 by CRC Press LLC

TX846_Frame_C07 Page 136 Monday, November 18, 2002 12:17 PM

Wing box Empennage box Fuselage The control components: Ailerons Control components for direction and elevation High lift devices Spoilers Exterior components: Fairings “Karmans” Storage room doors Landing gear trap doors Radomes, front cauls Interior components: Floors Partitions, bulkheads Doors, etc. Example: The vertical stabilizer of the Tristar transporter (Lockheed Company, USA) With classical construction, it consists of 175 elements assembled by 40,000 rivets. With composite construction, it consists only with 18 elements assembled by 5,000 rivets.

7.1.2 Characteristics of Composites One can indicate the qualities and weak points of the principal composites used. These serve to justify their use in the corresponding components.

7.1.2.1 Glass/Epoxy, Kevlar/Epoxy These are used in fairings, storage room doors, landing gear trap doors, karmans, radomes, front cauls, leading edges, floors, and passenger compartments. Pluses: 1 High rupture strength Very good fatigue resistance Minuses: High elastic elongation Maximum operating temperature around 80∞C Nonconducting material 1

See Section 3.3.3.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 137 Monday, November 18, 2002 12:17 PM

7.1.2.2 Carbon/Epoxy This is used in wing box, horizontal stabilizers, fuselage, ailerons, wings, spoilers (air brakes) vertical stabilizers, traps, and struts. Pluses: High rupture resistance Very good fatigue strength Very good heat and electricity conductor High operating temperature (limited by the resin) No dilatation until 600∞C Smaller specific mass than that of glass/epoxy Minuses: More delicate fabrication Impact resistance two or three times less than that of glass/epoxy Material susceptible to lightning

7.1.2.3 Boron/Epoxy This is used for vertical stabilizer boxes and horizontal stabilizer boxes. Pluses: High rupture resistance High rigidity Very good compatibility with epoxy resins Good fatigue resistance Minuses: 2 Higher density than previous composites Delicate fabrication and forming High cost

7.1.2.4 Honeycombs Honeycombs are used for forming the core of components made of sandwich structures. Pluses: Low specific mass Very high specific modulus and specific strength Very good fatigue resistance Minuses: Susceptible to corrosion Difficult to detect defects

2

See Section 3.3.3.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 138 Monday, November 18, 2002 12:17 PM

7.1.3 A Few Remarks The construction using only glass fibers is less and less favored in comparison with a combination of Kevlar fi bers and carbon fibers for weight saving reasons:

If one would like to have maximum strength, use Kevlar. If one would like to have maximum rigidity, use carbon. Kevlar fibers possess excellent vibration damping resistance. Due to bird impacts, freezing rain, impact from other particles (sand, dirt), one usually avoids the use of composites in the leading edges without 3 metallic protection.

Carbon/epoxy composite is a good electrical conductor and susceptible to lightning, with the following consequences: Damages at the point of impact: delamination, burning of resin Risk of lightning in attachments (bolts) The necessity to conduct to the mass for the electrical circuits situated under the composite element Remedies consist of the following: Glass fabric in conjunction with a very thin sheet of aluminum (20 mm) The use of a protective aluminum film (aluminum flam spray) Temperature is an important parameter that limits the usage of epoxy resins. A few experimental components have been made of bismaleimide resins (ther4 mosets that soften at temperatures higher than 350 ∞C rather than 210 ∞C for epoxies). One other remedy would be to use a thermoplastic resin with high 5 temperature resistance such as poly-ether-ether-ketone “peek” that softens at 380∞C. Laminates made of carbon/peek are more expensive than products made of carbon/epoxy. However, they present good performance at higher operating temperatures (continuously at 130∞C and periodically at 160 ∞C) and have the following additional advantages: Superior impact resistance Negligible moisture absorption Very low smoke generation in case of fire

3

4

5

The impacts can create internal damages that are invisible from the outside. This can also happen on the wing panels (for example, drop of tools on the panels during fabrication or during maintenance work). The mechanical properties of the thermoset resins diminish when the temperature reaches the “glass transition temperature.” See Section 1.6 for the physical properties.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 139 Monday, November 18, 2002 12:17 PM

Figure 7.1 Temperature Cycle and Load Cycle for Components of an Aircraft

7.1.4 Specific Aspects of Structural Resistance One must apply to composite components the technique called fail safe in aerodynamics, which consists of foreseeing the mode of rupture (delamination, for example) and acting in such a manner that this does not lead to the destruction of the component during the period between inspections. Composite components are repairable. Methods of reparation are analogous to 6 those for laminates made of unidirectionals or fabrics. Considering the very important reduction of the number of rivets used as compared with the conventional construction, one obtains a smother surface, which can lead to better aerodynamic performance. One also considers that the attack of the environment and the cycles of fatigue over the years do not lead to significant deterioration of the composite pieces (shown in Figure 7.1 are two types of fatigue cycles for the components of aircraft structure). The failure aspect subject to a moderate impact is more problematic with the structures made of composite materials, because the energy absorbed by plastic deformation does not exist. For the cabins, one uses phenolic resins. These have good fire resistance, with low smoke emission. For the same reason, one prefers replacing Kevlar fibers with a combination of glass/carbon (lighter than glass alone and less expensive than carbon alone). It is possible to benefit from anisotropy of the laminates for the control 7 of dynamic and aeroelastic behavior of the wing structures.

7.1.5 Large Carriers The following examples give an idea on the evolution of use of composites in aircrafts over two decades: Example: Aerospatiale (FRA); Airbus Industry (EU) (Figure 7.2) Example: Boeing (USA) (Figure 7.3) 6 7

See Section 4.4.4. See Section 7.1.8.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 140 Monday, November 18, 2002 12:17 PM

Figure 7.2 Evolution of Mass of Composites in Aircraft

Figure 7.3 Use of Composite in Boeing Aircraft

How to evaluate the gains: In theory: For example, a study was made by Lockheed Company (USA) for the design of a large carrier having the following principal characteristics: payload 68 tons, range 8300 km. This study gives the following significant results: for an aircraft made using conventional metallic construction: total mass at take-off: 363 tons mass of the structure: 175 tons for an aircraft made using “maximum” composite construction: total mass at take-off: 245 tons mass of the structure: 96 tons. Such a difference can be explained by the cascading consequences that can be illustrated as in Figure 7.4. In practice: In reality, introduction of composites in the aircrafts is limited to certain parts of the structures. It is done case by case and in a progressive manner during the life of the aircraft (re-evaluation operation). One is then led to consider the different notions: © 2003 by CRC Press LLC

TX846_Frame_C07 Page 141 Monday, November 18, 2002 12:17 PM

Figure 7.4 Cascading Effect in Mass Reduction

Notion of the exchange rate is the cost for a kilogram saved when one substitutes a classical metallic piece with a piece made mainly with composite. For the substitution light alloy—carbon/epoxy—this cost is on the order of $160 (1984) per kilogram when the piece is calculated in terms of rigidity (similar deformation for the same load). It is amortized over a period of at least one year for the gain in “paying passenger.” Notion of gain in paying passenger is the gain in terms of the number of passengers, of freight, or in fuel cost; for example, for a large carrier: An aircraft of 150 tons, with 250 passengers consists of 60 tons of structure. A progressive introduction of 1600 kg of high performance composite materials leads to a gain of 16 more passengers along with their luggage. A reduction of 1 kg mass leads to the reduction of fuel consumption of around 120 liters per year. Why are the reductions of mass (average about 20%) not more spectacular? Consider the example of a vertical stabilizer. The distribution of mass of a composite vertical stabilizer can be presented as follows:

Facings in carbon/epoxy: 30% of total mass Honeycombs, adhesives: 35% of total mass Attachments: 25% of total mass Connections between carbon/epoxy components and attachments: overlayers of carbon/epoxy Allowance for the aging of the carbon/epoxy: overdimensions of the facings (the stresses are magnified about 10% more for a subsonic aircraft and 13% for a supersonic aircraft) In consequence, the global gain of mass in comparison with a classical metallic construction for the vertical stabilizer is not more than an order of about 15%. Example: European aircraft Airbus A-310–300 (Figure 7.5). © 2003 by CRC Press LLC

TX846_Frame_C07 Page 142 Monday, November 18, 2002 12:17 PM

Figure 7.5 Composite Components in an Airbus A-310

Total mass: 180 tons Mass of structure: 44.7 tons Mass of composites: 6.2 tons Mass of high performance composites: 1.1 tons Reduction of mass of structure: 1.4 tons Percentage of composites: 13.8% of mass of structure. A reduction of mass of the structure of 1 kg augments the range of the aircraft by 1 nautical mile.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 143 Monday, November 18, 2002 12:17 PM

Figure 7.6 Composite Components in an Airbus A-320

Example: European aircraft Airbus A-320 (Figure 7.6).

Total mass: 72 tons Empty mass: 40 tons Mass of structure: 21 tons Mass of composite materials: 4.5 tons, corresponding to a reduction of mass of the structure of 1.1 tons. The percent of composite mass is 21.5% of the mass of the structure. A few other characteristics: Length: 37.6 m; breadth: 34 m; 150 to 176 passengers transported from 3,500 to 5,500 km; maximum cruising speed: 868 km/h Example: European aircraft Airbus A-340 Total mass: 253.5 tons Mass of structure: 76 tons Mass of composites: 11 tons, corresponding to a reduction of structure mass of 3 tons Percentage of composites: 14.5% of the mass of the structure Example: Future supersonic aircraft ATSF (Figure 7.7), Aerospatiale (FRA) and British Aerospace (UK). Principal characteristics defined at the stage before the project Transport of 200 passengers over a distance of 12,000 km Cruising speed between Mach 2 (2,200 km/hr) and Mach 2.4 (2,600 km/hr) © 2003 by CRC Press LLC

TX846_Frame_C07 Page 144 Monday, November 18, 2002 12:17 PM

Figure 7.7 Composite Components in a Future Supersonic Aircraft

Economically viable for a single type of aircraft on the market (enlarged international cooperation)

7.1.6 Regional Jets Example: Regional transport aircraft ATR 72, ATR (FRA–ITA) (Figure 7.8): Total mass: 20 tons Percentage of composite materials more than 25% of the mass of the structure Transports 66 passengers over a distance of 2,600 kilometers Interior equipment: Facings of panels for portholes and ceiling, baggage compartment, bulkheads, toilets, storing armors in glass-carbon/phenolic resins/NOMEX honeycomb; decoration by a film of “TEDLAR” © 2003 by CRC Press LLC

TX846_Frame_C07 Page 145 Monday, November 18, 2002 12:17 PM

Figure 7.8 Composite Components in the Regional Transport Aircraft ATR 72

Figure 7.9 Business Aircraft Falcon 10

Example: Business aircraft Falcon 10 (Figure 7.9). Aircrafts (AMD–BA) (FRA). The principal wing box (primary structure) is constructed in ribbed panels of carbon/epoxy; it has been flying experimentally since 1985. Mass of wing box: 339 kg Reduction of mass in comparison with conventional metallic construction: 80 kg (20%) The connection between the wing and the fuselage and the attachment between the landing gears and the wing box are made using metallic pieces. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 146 Monday, November 18, 2002 12:17 PM

Figure 7.10 Propulsive Propeller Configuration

7.1.7

Light Aircraft

These are the aircrafts for tourism and for the gliders. The new generation of these aircrafts is characterized by A large utilization of composites A renewal in aerodynamic solutions Remarks: In addition to the problems to be resolved by the manufacturers (small manufacturers for the most part), comes the preparation of the dossiers of certification including composite primary structures. The useful reduction of masses, the range of flight, and the cruising speed, due to the utilization of composites, are amplified more clearly in these types of aircrafts. Example: Back propeller aircraft. The principle of this is illustrated in Figure 7.10, with the advantages and drawbacks. The modification of the mass distribution, due to the displacement of the motor, requires a propeller shaft (foreseen to be in carbon/epoxy) and a wing shifted to the back. One can propose the “all composite” solution as follows: The solution “long shaft.” Sup’air airplane Centrair (FRA); Figure 7.11 The solution of shifted wing and additional duck wing: Beech Starship aircraft (USA); Figure 7.12: Eight to ten passengers: 650 km/hr with low fuel consumption Structure in carbon/epoxy Mass of the wings: 800 kg (reduction of 35% in comparison with a metallic solution) Mass of fuselage (structure): 240 kg Mass of the composite: about 70% of the mass of the structure © 2003 by CRC Press LLC

TX846_Frame_C07 Page 147 Monday, November 18, 2002 12:17 PM

Figure 7.11 An All-composite Airplane

Figure 7.12 Beech Starship Aircraft

Example: The modern glider planes. These are made entirely of composites. Figure 7.13 shows a plane made of glass/epoxy: Two-seater glider plane: Marianne Centrair (FRA): Mass: 440 kg © 2003 by CRC Press LLC

TX846_Frame_C07 Page 148 Monday, November 18, 2002 12:17 PM

Figure 7.13 The Marianne Centrair Airplane

Wings: 2 parts bonded Fuselage: 2 parts bonded

7.1.8 Fighter Aircraft For this type of aircraft, there is a progressive replacement of metallic elements by composite elements. Beyond specific characteristics already mentioned previously for the large aircrafts, here the composite components have to assure the necessary rigidity for the wing box to conserve the ability of command in a domain of flight larger than for the case of large civil aircrafts. For the flight with electrical commands, the use of composites allows for an evolution of the aerodynamic design for better maneuverability. In the near future, 25 to 40% of the structure of the fighter aircrafts will be made of composite materials. Example: European airplane Alphajet (Figure 7.14). Example: Airplane Mirage 2000 A.M.D.–B.A. (FRA; Figure 7.15). Mass of composite materials: 65 kg (On this aircraft there are boron/epoxy composite components.) Characteristics of boron: The diameter of the fiber varies between 0.1 mm and 0.2 mm depending on the demand of the customer. The radius of curvature, in fact, cannot be less than 4 or 5 mm. One finds for the sheets: width is 1 m, 80 filaments/cm, length: 3.5 m. 8 for the fabrics: patented process; the warp direction consists of textile filaments, the fill direction consists of boron filaments. Example: Airplane F-18 Hornet, M.D. Douglas/Northrop (USA; Figure 7.16). Example: Airplane X-29 Grumman (USA; Figure 7.17). Example: Airplane Rafale A.M.D.–B.A. (FRA; Figure 7.18). Note that on this airplane there is a very large usage of high performance composites (carbon/ epoxy and Kevlar/epoxy). Mass of composite materials is 1,110 kg, leading to a 9 25% reduction in the mass of the structure. Figure 7.18 shows the main components using composites. 8 9

Patent Avions M. Dassault-Bréguet Aviation/Brochier. This is to compare with the number for Mirage 2000 airplane presented previously.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 149 Monday, November 18, 2002 12:17 PM

Figure 7.14 Alphajet Plane

Figure 7.15 Mirage Airplane

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 150 Monday, November 18, 2002 12:17 PM

Figure 7.16 F-18 Hornet Airplane

Figure 7.17 X-29 Grumman Airplane

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 151 Monday, November 18, 2002 12:17 PM

Figure 7.18 Rafale Airplane

7.1.9 Architecture of Composite Parts in Aircraft 7.1.9.1 Sandwich Design Sandwich with transverse honeycomb: Following the nature of the component, one uses two methods of fabrication: Multisteps in which the facings of the sandwich piece are polymerized separately and then are placed on the core having an adhesive film. After that the assembly is polymerized following the method represented in 10 Section 4.4.2, where eventually polymerization is done in an autoclave. Monostep in which, after the honeycomb core is formed, the facings are placed directly on this core. The assembly is polymerized using the same method as for the multistep method. Example: Wing box (Figure 7.19). 10

See also Section 2.1.3.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 152 Monday, November 18, 2002 12:17 PM

Figure 7.19 Wing Box

Figure 7.20 Horizontal Empennage of a Fighting Aircraft

The honeycomb core assures the rigidity of the component. However, the mass of the piece depends on the thickness of the core. Example: Horizontal empennage of a fighting aircraft (Figure 7.20). Remarks: One avoids drilling holes in boron/epoxy pieces as much as possible. This operation is onerous and requires ultrasonic technique with diamond tools. There is a problem with corrosion of metallic honeycomb. The corrosion is due to the progressive condensation of water in the cavities. This is combined with the mechanical and thermal stresses (fatigue) in the structure. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 153 Monday, November 18, 2002 12:17 PM

Figure 7.21 Sandwich Construction for Panels

Figure 7.22 High Lift Devices Flap

Remedies include Covering the honeycomb core surface with a resin film Introducing an inorganic inhibitor at the potential points of attack to prevent the reaction with water Sandwich construction for panels: When the thickness of the piece becomes large (on the order of 150 mm), the facings are stiffened separately by using a honeycomb core, following the arrangements shown in Figure 7.21. When the piece is of large size (long), the requirement of “nondeformation” can require the interposition of intermediate “ribs.” Each component (facings, ribs) is polymerized in the assembled state, following the technique of monostep described above. Example: High lift devices flap (Figure 7.22) Sandwich for the reinforcement of spars and ribs: One can increase the rigidity in flexure and in torsion by introducing honeycombs, as represented in Figure 7.23. Stiffened panels: Currently one can find the ribbed panels in metallic construction. The ribs can be added, or monolithic, meaning that they are formed as part of the same piece when the panel is made. One observes in parallel here with the same technique in ribbed panels in composites. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 154 Monday, November 18, 2002 12:17 PM

Figure 7.23 Sandwich for Spars and Ribs

Figure 7.24 Stiffeners Form

Figure 7.25 Wing Box

Added stiffeners: The composite stiffeners can have the forms shown in Figure 7.24. Example: Wing box (Figure 7.25). Monolithic stiffeners: These are cured at the same time with the facings. These can support higher loads than the previous case, but with higher cost. The mode of fabrication is shown schematically in Figure 7.26 for the so-called “omega” ribs. One uses cores, which are made partly by thermoexpandable silicone. One also uses hollow silicone cores stiffened by compressed air, or cores that melt at temperature on the order of 170∞C, which is slightly higher than the polymerization temperature of the piece. Example: Flanged plates (Figure 7.27) Example: Stabilizer panel (European aircraft Airbus A-300; see Figure 7.28). The carbon/epoxy ribs are obtained by combining the autoclave pressure and 11 the thermal dilatation of detachable metallic light alloy modules. The steps of the process are shown schematically in Figure 7.28: 11

See Section 1.6 for the coefficients of thermal expansion as compared between light alloy and carbon.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 155 Monday, November 18, 2002 12:17 PM

Figure 7.26 Monolithic Stiffeners

Figure 7.27 Flanged Plate

Example: Wing tip (Airplane ATR 72, ATR (FRA-ITA). This is a primary wing piece (its failure will bring about the failure of the airplane). It consists of two carbon/epoxy panels with monolithic ribs, two spars in carbon/epoxy, and 18 metallic flanges in light alloy folded sheets, as shown schematically in Figure 7.29. Mass of box: 260 kg (reduction of 65 kg as compared with a metallic solution). Remarks: Lightning protection of such a structure requires specific precautions such as: Incorporation of a conducting fabric made of bronze wires on all external surfaces Installation of lightening conductors along the spars Protection of the connections Example: Air brakes (European airplane Airbus A-320; Figure 7.30).

7.1.10

Elements of Braking

Different from the brakes for ground vehicles, the brakes for aircrafts are characterized by successively distinct phases of isolated operations over time. These repeat themselves in almost identical conditions from one landing to the next. These are © 2003 by CRC Press LLC

TX846_Frame_C07 Page 156 Monday, November 18, 2002 12:17 PM

Figure 7.28 Stabilizer Panel

Figure 7.29 Wing Tip on ATR 72 Airplane

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 157 Monday, November 18, 2002 12:17 PM

Figure 7.30 Air Brakes on Airbus A-320

“heat absorption” brakes, which are activated for only a few seconds (about 20 seconds). The subsequent cooling of these brakes happens progressively afterwards. The heat coming from the transformation of kinetic energy is stored in the components participating in the friction phenomenon, which serve as “heat sinks.” These components must have the following characteristics: Being able to create a high braking moment which remains stable as the temperature increases Being able to support a very important “thermal shock,” on the order of 6 10 joules per kg mass of the component Being refractory and retaining a good dimensional stability Being able to retain their mechanical properties at high temperature Having as low mass as possible The corresponding brakes are of “disk” type. The materials that can be used to make these friction disks are compared in Figure 7.31. One can see the interest in using three-dimensional composite materials in carbon/carbon, which have the following characteristics: Their dynamic friction coefficient is stable with respect to the temperature, varying from 0.25 to 0.3. They resist thermal shock and are refractory until 1600∞C. 12 They retain their mechanical properties at high temperature. 3 They are light weight (specific mass of 1900 kg/m ). Example: Disk brakes in carbon/carbon (Figure 7.32) “Aerolor” (FRA). Example: Supersonic transport aircraft Concorde (FRA-U.K.). The gain in paying passenger due to this type of brakes represents six passengers and their luggage, or 600 kg. 12

See order of magnitude of the mechanical properties in Section 3.6.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 158 Monday, November 18, 2002 12:17 PM

Figure 7.31 Airbrake Materials

Such types of brakes can also be developed for rapid trains, as well as for racing cars and motorcycles.

7.1.11 The Future One can cite as the principal objectives for the airplane manufacturers: Obtain with composite materials a minimum mass reduction of 20% as compared with the metallic solution using the new light alloys aluminum/ lithium. This implies the improvement in the performance of fibers and matrices. Improvement on the manufacturing process. The graph in Figure 7.33 shows that significant efforts remain to be done to reduce the labor cost in the manufacturing of high performance composite components. Apart from improvement such as automatic draping or electron beam curing or by x-ray, other more classical techniques described in Chapter 2 have actually been adapted for the fabrication of aircrafts or their components. One can mention RTM process (see Section 2.3.1), for example, tail cone of airplane Airbus A-321. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 159 Monday, November 18, 2002 12:17 PM

Figure 7.32 Disk Brakes in Carbon/carbon

Figure 7.33 Different Costs in Composite Solution © 2003 by CRC Press LLC

TX846_Frame_C07 Page 160 Monday, November 18, 2002 12:17 PM

Figure 7.34 Evolution of Percent of Composite Materials in Aircraft Structure

Figure 7.35 Relative Mass of Principal Materials Used in Aircraft Structures

High pressure injection (see Section 2.1.5) with short fibers or with particles. Thermoforming (see Sections 2.3.1 and 2.2.3) for the small pieces. Compression molding (see Sections 2.3.1 and 2.1.2). One can see in Figure 7.34 that about 20% of the mass of the structure of civil aircrafts should integrate composite materials. Figure 7.35 shows the evolution foreseen for the relative mass of the principal materials used for aircraft structures.

7.2 HELICOPTERS 7.2.1 The Situation This category of aircraft is less advanced than the airplanes in terms of technological evolution towards “perfection” as shown in the graph in Figure 7.36. In fact, taking into account the possibilities of specific mass reduction for this type of aircraft, one can see in the graph in Figure 7.37 the increasing trend in the strong integration of composites, with higher percentages as compared with the case of airplanes. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 161 Monday, November 18, 2002 12:17 PM

Figure 7.36 Degree of Technological Evolution

Figure 7.37 Evolution of Composites Mass on Helicopters

Example: Evolution of the mass of composite materials on the helicopters of Aerospatiale (FRA). In comparison with conventional metallic construction, one can mention the following mass reduction:\. 15% on the secondary structures Up to 50% in the working pieces, such as the elements of transmission of power and control

7.2.2 Composite Zones Figure 7.38 shows the composite components in a helicopter.

7.2.3 Blades The blades are the essential elements of the aircraft. They consist principally of the following: An envelope or a box that assures an aerodynamic profile and a stiffener for torsion (the blade does not twist under aerodynamic forces, at least for the actual generation of aircrafts). © 2003 by CRC Press LLC

TX846_Frame_C07 Page 162 Monday, November 18, 2002 12:17 PM

Figure 7.38 Composite Components in a Helicopter

A spar which resists the centrifugal tension on the blade as well as the flexure caused by the lift and drag loads. It is made of glass/epoxy (“R” glass, more resistant and less sensitive to aging by humidity). A rear edge that stiffens the blade in flexure in the direction of the drag. A filler material (foam or honeycomb) that prevents the deformation of the profile. Figure 7.39 shows the different parts of the blade.

7.2.3.1 Advantages The list of advantages obtained with this type of design is impressive: The blade is molded (molding by assembly of two half shells under pressure). This solution allows one to obtain an optimized profile (variable chord and thickness, nonsymmetric profile, nonlinear twist). The stiffeners for fluttering and for torsion can be controlled thanks to judicious usage of composite materials.

7.2.3.2 Consequences The payload is augmented. The mass reduction attains 400 kg for the aircraft Superpuma Aesrospatiale (FRA). The cruising speed is increased for the same power. The gain is 32 km/h at 1500 m altitude as compared with a previous helicopter. The cost of fabrication is reduced by 50% in comparison with conventional metallic solution. The cost of operation is reduced. The life of the blade is practically unlimited. None of the load in the range of flight of the aircraft can lead to the fatigue damage. It is quasiindestructible, even when testing the specimens. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 163 Monday, November 18, 2002 12:17 PM

Figure 7.39 Helicopter Blade 13

Increased security: the blade has the fail safe character. An impact (projectile, collision) causes a local deterioration which does not lead to the fall of the aircraft. 14 The blade is repairable with a relatively simple process. The blade is not sensitive to corrosion. Remarks: The blade as conceived can be ultralight. However, light weight cannot be below a value that assures a minimum inertia that is indispensable for the good operation of the rotor.

7.2.4 Yoke Rotor This is the mechanical assembly that allows The rotation of the blades The small amplitude angular displacements of the blades during rotation

13 14

See Section 7.1.4. See Section 4.4.4.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 164 Monday, November 18, 2002 12:17 PM

Pitch control, that is, the control of the aerodynamic incidence of the profiles of the blades To assure all these functions, the previous classical metallic rotors were very complex. They consisted of many pieces —in particular the ball bearings —and numerous points of lubrication. In fact, the maintenance was very costly. The modern rotors—first developed by Aerospatiale (FRA)—substitute for these classical articulations the degrees of freedom starting from the elastic deformation: Composites made of metal/elastomer Laminates Example: The yoke “Starflex” Aerospatiale (FRA). As its name indicates, this yoke has the form of a star with flexible arms (see Figure 7.40) obtained by draping a large amount of balanced glass/epoxy fabric and molding under heat and pressure. The different degrees of freedom necessary for the operation as cited above are made possible by the capabilities as shown in Figure 7.41:

Figure 7.40 The Starflex Yoke

Figure 7.41 Details of the Starflex Yoke System © 2003 by CRC Press LLC

TX846_Frame_C07 Page 165 Monday, November 18, 2002 12:17 PM

The elastic arm assures angular displacement called “lift fluttering.” The elastic ball and socket allows for the rotation noted as pitch on the figure. This translates into a variation in the incidence of the profile. The elastomer bearing allows for fluttering of the blade in the plane of the figure, called “drag fluttering.” Consequences include the following: A spectacular decrease in the number of components. (One goes from 377 pieces for a classical metallic solution with 30 bearings to 70 pieces for a composite solution without any bearings.) There is a corresponding mass reduction of 40 kg. There is a reduced cost of fabrication. The maintenance is reduced in considerable proportion, lowering significantly the hourly cost of the flight. There is increased security (more viability of the mechanical assembly).

7.2.4.1 Evolution of the Yoke Rotors Example: The yoke “Triflex” Aerospatiale (FRA). The elastic deformation of the arms (see Figure 7.42) is sufficient to assure the displacements in lift, drag, and the variable incidence (pitch). The liaison arm/yoke and arm/joints of the blades are delicate works.

Figure 7.42 Triflex Yoke © 2003 by CRC Press LLC

TX846_Frame_C07 Page 166 Monday, November 18, 2002 12:17 PM

Figure 7.43 Spheriflex Yoke

Figure 7.44 Pitch Lever

Example: The yoke “Spheriflex” Aerospatiale (FRA). This is so called because only the elastic ball-and-socket allows the various angular displacements: flapping and pitching. The foot of the blade is modified as a consequence (see Figure 7.43). The number of components becomes extremely reduced, with a minimum volume (less than the volume of the previous solutions).

7.2.5 Other Composite Working Components Most of these are made of carbon/epoxy. The parts already in service or in development include

The rotor mast The plate for the cyclical control of the pitch The struts for the control of the pitch The levers for the pitch (see Figure 7.44) where the composite design leads to a reduction of mass of 45% as compared with the metallic solution 15 Lever winch gallows The stabilizer 15

See Section 1.5.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 167 Monday, November 18, 2002 12:17 PM

Example: Aircraft Dauphin Aerospatiale (FRA). Stabilizer in light alloy

231 parts 5900 rivets Mass = 1 Global cost = 1

Stabilizer in carbon/epoxy

88 parts 0 rivets Mass = 0.78 Global cost = 0.66

In the case of the military helicopters: Utilization of composite materials reduces the “radar signature” of the helicopter. The damages by the projectiles on the blades, yokes, and command struts evolve more slowly in the composite parts and allow the aircraft to be able to return to its base (except for the case of a projectile shell break with a diameter larger than 20 mm). 16 The “crash” resistance is less for a composite structure as compared with conventional structure.

7.3 PROPELLER BLADES FOR AIRPLANES The design using composites for the propeller blades for airplanes is analogous to that for the helicopter blades. They consist essentially of a torsion box of composite with a spar made of metal or composites. Example: Propeller blade Hamilton Standard (USA) for the motor “14 SF” for 17 the airplane ATR 42 (Figure 7.45). Example: Propeller blade Ratier-Figeac (FRA) for the motor of the plane TRANSALL (FRA–GER). The adoption of a spar in unidirectional glass and a torsion box in carbon leads to a particular weight reduction, when the diameters of the rotors become important, as indicated in Figure 7.46, which has the following characteristics: Diameter of the 4-bladed rotor: 5.5 m Mass of a composite blade: 51 kg Mass reduction as compared with a metallic blade: 53 kg (mass of a metallic blade: 104 kg) Total mass reduction (2 ¥ 4 blades): 430 kg The centrifugal inertia force at the foot of the blade decreases from 105,000 daN to 30,000 daN. This is taken up by the glass fibers in the spar which are bonded to a steel piece having the form of a tulip and addition of circumferential hoop winding of rovings to allow for the “fail safe” design. If there is bonding rupture, the blade is retained on its base by the hoop windings. The construction of the Ratier-Figeac propeller blade is shown schematically in Figure 7.47. 16 17

See Section 7.1.4. See Section 7.1.6.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 168 Monday, November 18, 2002 12:17 PM

Figure 7.45 Propeller Blade, Hamilton Standard

Figure 7.46 Mass Saving in Using Composites for Blades

Example: Airplane with rocking rotors XV-15 BELL (USA; Figure 7.48), propellers Dowty Rotol Ltd. (U.K.), which has the following characteristics:

Rotor diameter: 7.6 m Chord at foot of blade: 0.5 m Mass of composites: 70% of the mass of the structure. Wing: stiffened panels in carbon/epoxy.

The new generation of the propellers (called “rapid” or “transonic”) is destined to propel commercial airplanes with a speed close to that obtained with the jets (Mach 0.8 to 0.85, or more than 850 km/h). Interest in such propellers rests in a propulsion efficiency higher than that of modern jets (with double flux) at high speeds, as shown in Figure 7.49. For good aerodynamic and acoustic behavior, the propellers are characterized by low thickness, a large “chord” and a strong curvature which gives them the form of an oriental saber. The complexity of the geometry combined with important speeds of rotation (more than 4000 revolutions per minute) requires the composite construction. Example: Propeller “Propfan” Hamilton Standard (USA; Figure 7.50). Made of two rotors in “counter-rotation,” this is designed to propel the middle range airplanes. The method of fabrication is the same as the more classical propellers mentioned above: a spar made with light metal alloy forged and machined. A filling foam is molded around the spar to give the form of the torsion box in glass/epoxy. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 169 Monday, November 18, 2002 12:17 PM

Figure 7.47 Ratier-Figeac Propeller Blade

Figure 7.48 Rocking Rotor in Bell XV-15 Plane © 2003 by CRC Press LLC

TX846_Frame_C07 Page 170 Monday, November 18, 2002 12:17 PM

Figure 7.49 Propulsion Efficiency of Propellers

Figure 7.50 Profan Propeller

Example: Transonic propeller “Charme” ONERA (FRA; Figure 7.51). The number of blades is high (12) to reduce the load in each blade. The blades are made of carbon/epoxy bonded to the titanium foot of the blades.

7.4 TURBINE BLADES IN COMPOSITES Research to increase the efficiency of aeronautical motors leads to the increase of Air compression ratios, which reach the values on the order of 45. Temperatures of the gases in the turbines. The fixed or mobile blades in the release stages have to operate with a gas temperature on the order of 1500∞C. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 171 Monday, November 18, 2002 12:17 PM

Figure 7.51 The Transonic Propeller “Charme”

Among the materials experimented with in view of increasing the operating temperature are the “oriented eutectics.” These are composed of two distinct phases: A superalloy phase with nickel base A carbon phase The solidification of this alloy is directed with a solidification front (interface between the liquid and the solid). The carbon phase is developed in the form of fibers with diameters on the order of microns and of infinite length, and parallel to the direction of displacement of the solidification front. One then obtains a unidirectional composite metal/metal. The advantages and disadvantages of these types of materials can be summarized as follows: Pluses: It is possible to obtain directly, using solidification, pieces with the form of the turbine blades. There can be a gain of 30∞C on the maximum operating temperature of actual blades. Minuses: The growing speed of the composite is low: 2 cm/hour. The proportion of fibers is low (5% to 10%) and cannot be controlled because it is constrained by the composition of the eutectic. The material is sensitive to thermal fatigue due to the run–stop operating cycles of the turbine. Fracture resistance at temperatures above 900∞C is weaker than that for super alloys in actual service.

7.5 SPACE APPLICATIONS There is no doubt that for launchers, space shuttles, and satellites the reduction of mass is most critical. Each kilogram reduction on the launcher for the European rocket Ariane E.S.A. (EU) gives a gain in payload of 30,000 US dollars. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 172 Monday, November 18, 2002 12:17 PM

7.5.1 Satellites The structural part of the satellites is essentially constituted of an assembly of tubes and plates. Principally the structure has to Resist average and fluctuating accelerations of the launch, counted as number 2 of times the acceleration of gravity (g = 9.81 m/sec ), up to 5 ¥ g continuously and 5 ¥ g maximum amplitude in sinusoidal fluctuation, for frequencies up to 40 Hz. (In order to avoid resonance, the structure has to be very rigid. It is the rigidity that appears like the factor that controls the dimensions.) Be quasi-insensitive to temperature variations (such as in the case of precision optical instruments: telescope, high-resolution camera). Here, carbon is used for the tubular structure (very low coefficient of expansion, on the -7 18 order of 10 ). The primary structures of satellites can include sandwich plates, with the following characteristics: 19

Light alloy honeycomb cores (not Nomex because of gas emission in space). Facings (skins) made of laminates, without mirror symmetry for maximum lightness. The thickness of the skin is on the order of 0.1 mm. When 20 demolding, they are very deformed. These are then bonded onto the aluminum core. One then obtains a sandwich plate that is globally balanced. Example: Camera V.H.R. (Visible high-resolution) SPOT (FRA), which is the upper part of the satellite shown in Figure 7.52. In the case of the spatial structures, among the foreseen solutions for the construction of tubular space stations, one can experiment on tubes made of extruded carbon with junctions of half-shell made of carbon.

7.5.2 Pressure Vessels The pressure vessels contain the combustibles, fuel or “powder,” for the propulsion. These can be made by winding impregnated unidirectional ribbons over a mandrel with a particular form. The mandrel must be resistant to shrinkage after 21 polymerization and should be designed to be extractable (see Figure 7.53). The efficiency of a filament-wound pressure vessel is defined as: p ( burst pressure ) efficiency ratio = ------------------------------------------------r g ( specific weight ) ( meters ) and has the units of length, for example: Efficiency of glass/epoxy: 25 km. Efficiency of Kevlar/epoxy: 35 km. which explains the predominant use of Kevlar/epoxy in these applications. 18 19 20 21

See See See See

Section Section Section Section

1.6. 1.6. 5.2.3. 2.1.7.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 173 Monday, November 18, 2002 12:17 PM

Figure 7.52 Camera V.H.R Spot

Figure 7.53 Filament-wound Pressure Vessel © 2003 by CRC Press LLC

TX846_Frame_C07 Page 174 Monday, November 18, 2002 12:17 PM

Figure 7.54 Filament Winding for Mono-block Part

Figure 7.55 Evolution of the Structure of Nozzles

For some applications, the principle of filament winding allows one to obtain vessels and tubes at the same winding session (see Figure 7.54).

7.5.3 Nozzles The propulsion nozzles of solid propergol (powder) have operating temperatures up to 3000∞C during several dozens of seconds, with pressures varying between 22 a few bars and several dozens of bars. The material making up the internal liner disappears progressively by decomposition, melting, vaporization, and sublimation. This is the phenomenon of ablation. The materials that can play such a role have to possess A strong resistance to ablation at a high operating temperature A low specific mass A strong resistance to mechanical and thermal shock Figure 7.55 shows the evolution of the structure of these nozzles until the advent of the three-dimensional carbon/epoxy composite materials with the mechanical characteristics indicated in Section 3.6. 22

1 bar = 0.1 MPa.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 175 Monday, November 18, 2002 12:17 PM

Figure 7.56 Sepcarb Material for Propulsion Nozzles

Figure 7.57 Nozzles in Rosette Form

Example: Material “Sepcarb” European company for propulsion (FRA; 23 6 Figure 7.56). The quantity of heat before ablation can reach 84 ¥ 10 joules per kilogram of material. For example the motor for peak operation of the European launcher Ariane, with the divergent nozzle made of carbon/epoxy, has the following characteristics: A mass reduction of 50% in comparison with previous nozzle constructions A gain of the launch force of 10% thanks to higher elongation Example: Divergent nozzle with “rosette” layering. Figure 7.57 shows the difference in constitution of this type of nozzle and a nozzle with classical concentric stratification, with a few orders of dimensional amplitude. To compare with the concentric stratification, this design: allows more convenient machining (more precise work of the lathe tool). is more resistant to delamination. 23

See Section 3.6.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 176 Monday, November 18, 2002 12:17 PM

7.5.4 Other Composite Components 7.5.4.1 For Thermal Protection One can distinguish two modes on entrance into the atmosphere during the return of the space vehicles: Rapid entrance with strong incidence: This is the case of the ballistic missiles and manned capsules. The heat flux is very high (on the order 2 of 10,000 kW/m ) with relatively short time of entrance. One can use, depending on the particular case: 24 Heat sinks in carbon/carbon or in beryllium (for case of the ballistic missiles). Ablative materials (see above for the case of the nozzles) for the manned capsules. Slow entrance with weak incidence: This is the case of hypersonic planes or “space shuttles.” The duration of the entrance is on the order of 2000 seconds. The heat fluxes are weaker but can attain hundreds of kilowatts per square meters of the structure at the beginning of the entrance (80 km altitude), for example: 2 500 kW/m at the leading edge 2 100 to 200 kW/m on the under part The entrance temperatures reach 1700∞C, or 2000∞C at the nose of the shuttle. There are several types of thermal protection, depending on the zones of the equipment and the reutilization of the facing: 25

Heat sinks associated with insulation Reflective thermal barrier (lining of the vehicle reflects the heat flux it receives) Ablative facing (The transformation of the facing by fusion, vaporization, sublimation, chemical decomposition absorbs the heat, and the vaporized gases cool the remaining layer, decreasing also the convective thermal flux.) The areal masses of these devices are related to the limiting admissible temperatures of the structure immediately below (see Figure 7.58). Example: NASA space shuttle (USA), which has an empty mass of 70 tons. Depending on the zones, one uses the linings made of composites of carbon/ carbon or silicon/silicon and pieces of structure (horizontal members, cross members) in boron/aluminum. The useful temperature of the latter is 300∞C for continuous use and up to 600∞C for peak applications. 26 The under part is protected by composite “tiles” in silicon/silicon ceramic that constitutes a reflective thermal barrier. The tiles are separated from the structure of light alloy or laminated boron/aluminum by a sandwich of felt and nonflammable 24 25 26

See Section 7.1.10. See Section 3.7. See Sections 2.2.4 and 3.6.

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 177 Monday, November 18, 2002 12:17 PM

Figure 7.58 Areal Mass for Thermal Protection

nylon/silicon/“NOMEX” honeycomb. There are about 30,000 tiles. Their installation is shown in Figure 7.59. Example: Space shuttle Hermes (EU), which has an empty mass of 8.5 tons. The tiles are replaced by thousands of pieces made of carbon/carbon, silicon/ silicon (see Figure 7.60). The pieces have to be reused for thirty landings.

7.5.4.2 For Energy Storage On board satellites and space stations, systems using the composite flywheels for the supply of electric power and for the control of attitude provide a mass reduction of 25% as compared with conventional storage methods using batteries and gyroscopic means (specific power on the order of 5 kW per kilogram of the device). In addition, in the Strategic Defense Initiative program (USA), the devices of flywheels can deliver high levels of specific powers on the order of 100 kW per kilogram of the device. The peripheral speeds can attain 1400 m/sec (filament-wound flywheels in carbon), and the speeds of rotation from 40,000 to 60,000 rpm. Example: Development of an energy storage module (USA; Figure 7.61). 3

Total mass: 200 kg (occupied volume: 0.15 m ) Specific energy: 230 kJ/kg (total energy # 46,000 kJ) Peripheric speed: 1100 m/sec Figure 7.62 shows different solutions for the construction of carbon/epoxy flywheels. © 2003 by CRC Press LLC

TX846_Frame_C07 Page 178 Monday, November 18, 2002 12:17 PM

Figure 7.59 NASA Space Shuttle

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 179 Monday, November 18, 2002 12:17 PM

Figure 7.60 Space Shuttle Hermes

© 2003 by CRC Press LLC

TX846_Frame_C07 Page 180 Monday, November 18, 2002 12:17 PM

Figure 7.61 Flywheel Energy Storage

Figure 7.62 Different Flywheel Designs

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 181 Monday, November 18, 2002 12:22 PM

8 COMPOSITE MATERIALS FOR OTHER APPLICATIONS We have given in Chapter 1 an idea on the diversity of the products which can 1 be made using composite materials. In this chapter we examine a few of these products, which form a good part in the evolution of these materials, excluding the aerospace sector presented in the previous chapter.

8.1 COMPOSITE MATERIALS AND THE MANUFACTURING OF AUTOMOBILES 8.1.1 Introduction Composite materials have been introduced progressively in automobiles, following polymer materials, a few of which have been used as matrices. It is interesting to examine the relative masses of different materials which are used in the construction of automobiles. This is shown in the graph in Figure 8.1. Even though the relative mass of polymer-based materials appears low, one needs to take into account that the specific mass of steel is about 4 times greater than that of polymers. This explains the higher percentage in terms of volume for the polymers. Among the polymers, the relative distribution can be shown as in Figure 8.2. The materials called “plastics” include those so-called “reinforced plastics” for composite pieces that do not have very high performance. The graph in Figure 8.3 gives an idea for the distribution by zone of the “plastic” pieces in an automobile and also shows the evolution in time. One can see the increasing importance of high-performance parts.

8.1.2 Evaluation and Evolution A few dates on the introduction of composite parts (fibers + matrix) include: The antiques as shown in Figure 8.4 1968: wheel rims in glass/epoxy in automobile S.M.Citroen (FRA) 1970: shock absorber shield made of glass/polyester in automobile R5 Renault (FRA) 1

See Section 1.3.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 182 Monday, November 18, 2002 12:22 PM

Figure 8.1 Use of Different Materials in Automobiles

Figure 8.2 Mass Distribution Among Polymer Materials

Consequences of the introduction of composite pieces in automobiles are now well-known. They allow a number of advantages. One can find several common points with aeronautic construction. There are also disadvantages that are more specific to automobiles. Advantages include Lightening of the vehicles: A reduction of mass of 1 kg induces a final reduction of 1.5 kg, taking into account the consecutive lightening of the mechanical components.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 183 Monday, November 18, 2002 12:22 PM

Figure 8.3 Distribution of “Plastic” Components in an Automobile

Figure 8.4 Composite Pieces in Antique Cars

Cost reduction: This is due to the reduction of the number of pieces required for a certain component and to noise reduction and isolation. The better corrosion resistance of the composite pieces. Significant disadvantages are It is difficult, for fabrication in large volume, to obtain as good a surface finish as that of painted sheet metals. For the car body, the painting process and the treatment of the surfaces require high temperature exposure.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 184 Monday, November 18, 2002 12:22 PM

How to Evaluate the Gains: In theory: These are the experimental vehicles; Ford, Peugeot (1979). As compared with the metallic pieces, composite parts have obtained mass reduction of 20% to 30% on the pieces for the body. 40% to 60% on the mechanical pieces Example: Ford vehicle, which has a mass in metallic construction of 617 kg and a mass in composite construction of 300 kg for a global gain of 52%. It is convenient to consider this case as “technological prowess” far from the priority of economic constraints. In practice: Over the past years, an increasing number of pieces made of glass fibers/organic matrices have been introduced. The following list contains pieces that are in actual service or in development. Components for the body Motor cap Hood cover Hatchback door Fenders Roofs Opening roof Doors Shock absorber Interior components Seat frames Side panel and central consoles Holders Components under the hood Headlight supports Oil tanks Direction columns Cover for cylinder heads Cover for distributor Transmission shafts Motor and gearbox parts Components for the structure Chassis parts Leaf springs Floor elements Figure 8.5 shows the importance of the volumes actually occupied by the composites in an automobile. Example: Automobile BX Citroen (FRA)1983 with a total mass of 885 kg. Many of the molded pieces made of glass/resin composites as shown in Figure 8.6 are now commonly used by the automobile manufacturers. We note in particular the two elements below, the importance and large volume production of which (rate of production of more than 1000 pieces per day), indicate a significant penetration of composites in the manufacturing of automobiles.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 185 Monday, November 18, 2002 12:22 PM

Figure 8.5 Composite Pieces in an Automobile

The hood is made of glass/polyester molded at high temperature in a press 2 (20,000 kN) with the deposition of a gel coat during molding to assure the quality of the surface. The following comparison is eloquent: 2

See Section 2.1.1.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 186 Monday, November 18, 2002 12:22 PM

Figure 8.6

Composite Pieces in BX Citroen

Figure 8.7 Automobile Alpine V6, Renault

Conventional metallic construction (GS Citroen): 7 elements Composite construction: 1 element Mass gain: 7.8 kg or 46%. The rear window frame is made of injection molded glass/polyester (23,000 kN press). The mechanical characteristics obtained with this method (fracture resistance, modulus, impact resistance) are in the vicinity of those obtained by compression molding. One obtains a single piece that can support the rear glass piece, the aerodynamic details, the hinges, and the lower part of the trunk. The advantages over the classical construction are great: Classical construction (GS Citroen): 27 elements Composite construction: 7 elements Mass reduction: 1.7 kg or 16% Example: Automobile Alpine V6 Turbo, Renault (FRA), 1986 (Figure 8.7). The entire body in glass/polyester composites is not obtained by molding according to

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 187 Monday, November 18, 2002 12:22 PM

3

the technique used for the previous model A 310 (contact molding). It is made by bonding around fifty elements in glass/polyester on a tubular chassis. The panels are made by molding using a press at low pressure and temperature (6 minutes at 45∞C). 4 Contouring is done using a high-speed water jet. Structural bonding is done on a frame at 60 ∞C. Robots control it. The classical mechanical nuts and bolts are replaced by 15 kg of adhesives. Significant advantages include the following: There is reduction in fabrication time: 80 hours versus 120 hours for the construction of the previous model A 310. Excellent fatigue resistance is realized: (mileage > 300,000 km). There is good filter for noise from mechanical sources. The flexibility in the method of fabrication: The tooling in the press is interchangeable in order to produce small series of different pieces on the same press. This process is well adapted to a low rate of fabrication (10 cars per day). Mass reduction—as compared with the technique used in the previous model, which itself was using composites—is 100 kg. 3 For a cylinder size of 2500 cm (power of 147 kW or 240 CV), it is one of the most rapid series of vehicles ever produced in France previously (250 km/h) with a remarkable ratio of quality/price as compared with other competing European vehicles (Germany in particular). Example: Racing car “F.1” Ferrari (ITA) (Figure 8.8). This car body is a sandwich made of NOMEX honeycomb/carbon/epoxy. In addition, a crossing tube made of carbon/epoxy transmits to the chassis aerodynamic effects that act on the rear flap. This is attached to the chassis by light alloy parts, bonded to the composite part with structural araldite epoxy adhesive. There is weight reduction compared with previous metallic solution, and one also sees very good fatigue resistance, which is important in regard to mechanical vibrations.

8.1.3 Research and Development A number of working pieces—traditionally made of metallic alloys—of road vehicles have been designed and constructed in composite materials, and they have actually been tested and commercialized:

8.1.3.1 Chassis Components Research and Development work has been concerned with the spars, floors, front structures, rear structures, and also the complete structure. Principal advantage: Reduction in the number of parts and thus in the cost. Secondary advantage: Mass reduction (beams for truck chassis in Kevlar/ carbon/epoxy lead to a mass reduction of 38%—46 kg versus 74 kg for metal). 3 4

See Section 2.1.1. See Section 2.2.5.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 188 Monday, November 18, 2002 12:22 PM

Figure 8.8 Ferrari F.1 Racing Car

Figure 8.9 Front Face of 405 Peugeot

The problems involved are numerous: How to assemble the pieces. What will be the mechanical behavior when subjected to strong impacts? How is the rate of production to be augmented? The actual fabrication methods are too slow (decrease in the cycle time by using automation). Example: The superior cross beam or “front face” of the automobile 405 Peugeot (FRA). This component (see Figure 8.9) is subjected to repeated load cycles in tension, flexure, and torsion. It also supports several dozens of

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 189 Monday, November 18, 2002 12:22 PM

Figure 8.10 Comparison Between Metallic and Composite Springs

components and equipment that form the front face of the vehicle. Characteristics include: Part molded in glass/polyester (Vf = 42%) 5 Fabrication process: SMC : Press 15,000 N Rate of production: 1200 pieces/day Machining/drilling (70 holes); installation of inserts (30) and components made by laser, numerical machining, and robots

8.1.3.2 Suspension Components Springs: One of the principal characteristics of the unidirectionals (namely 6 glass/resin) is their capacity to accumulate elastic energy. Herein lies the interest in making composite springs. In theory, a glass/resin spring is capable of storing 5 to 7 times more elastic energy than a steel spring of the same mass. Other advantages include: The composite springs are “nonbreakable.” Damage only translates into a minor modification of the behavior of the component. It is possible to integrate many functions in one particular system, leading to a reduction in the number of parts, an optimal occupation of space, and an improvement in road behavior. The mass reduction is important (see Figure 8.10) The disadvantages: It is difficult to adapt the product to the requirements of the production. It is not sufficient to demonstrate the technical feasibility; one must optimize the three-criteria product-process-production rate (rates of production of 5 6

S.M.C. process: See Section 2.1.3 and 3.2. See Section 3.3.2, comparison of load-elongation diagrams for a metal and a unidirectional.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 190 Monday, November 18, 2002 12:22 PM

Figure 8.11 Leaf Spring

Figure 8.12 Combination of Functions

several thousands of parts per day in the automotive industry, to be made using a few processes, i.e., filament winding, compression molding, pultrusion, and 7 pultrusion-forming). The current development and commercialization efforts deal with leaf springs and torsion beam springs. Example: Single leaf spring (see Figure 8.11). A spring made of many metallic leaves is replaced by a single leaf spring made of composite in glass/epoxy. Many vehicles are sold with this type of spring, for example, Rover –GB; Nissan–JAP; General Motors–USA; Renault–FRA). Example: Multifunctional system (Bertin–FRA). This prototype for the front suspension of the automobile combines the different functions of spring, rolling return, and wheel guide (see Figure 8.12). Example: Stabilizing system. This is used for the connection between an automobile and a caravan (Bertin/Tunesi–FRA). The combined functions are shown schematically in Figure 8.13. The mass is divided by 4.5 in comparison with an “all metal” solution. Example: The automobile suspension triangle has two parts (FRA) that are bonded to make a box (see Figure 8.14).

8.1.3.3 Mechanical Pieces Motor: The parts shown schematically in Figure 8.15 are in the experimental stage or in service in thermal motors. For pieces that have to operate at high temperatures, one should use the high temperature material system

7

See Chapter 2.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 191 Monday, November 18, 2002 12:22 PM

Figure 8.13 Stabilizing System

Figure 8.14 Composite Suspension Triangle 8

glass/polyamide (up to 300∞C). One can also mention the pump blades and the synchronizers in speed boxes made of glass/polyamide. 9 Composite transmission shafts : These are used in Competition vehicles (rallies), allowing high speed of rotation with low inertia Small and large trucks Figure 8.16 shows how the low mass density associated with high rigidity in flexure allows the elimination of the intermediate bearing (this induces also a supplementary reduction in mass and cost). 8

9

The polyamide resin is said to be “thermally stable;” that is, it can maintain its mechanical properties at high temperatures (up to 500∞C for one hour). See Application 18.1.4.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 192 Monday, November 18, 2002 12:22 PM

Figure 8.15 Composite Mechanical Components

Figure 8.16 Composite Shafts

For the transmission shafts equipped with supports, one obtains the following advantages: Reduction of mass of 30% to 60% in comparison with the transmission shafts with universal cardan joints

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 193 Monday, November 18, 2002 12:22 PM

Figure 8.17 Composite-metal Shaft Bonding

Reduction in mechanical vibrations Decrease in acoustic vibration level (in particular the “peak”) Good resistance against chemical agents Very good fatigue resistance

Lateral transmission shafts are used for vehicles with front drive. They are used to eliminate the homokinetic joints that are actually used. They are made of a weak matrix material and wound fibers that allow the freedom of flexure for the transmission shaft.

8.2 COMPOSITES IN NAVAL CONSTRUCTION 8.2.1 Competition 8.2.1.2 Multishell Sail Boats In the past years there has been a spectacular development in the sailboat competition, with significant research activities on the improvement of the qualities of the boats, and the design of sail boats called “multishells” with large dimensions, made of high performance composites, characterized by Low mass leading to reduced “water drafts” 10 New and more performing “riggings” Resistance against intense fatigue loadings, namely for the joint mechanisms between the shells Example: Catamaran Elf Aquitaine (FRA) 1983 (see Figure 8.18). This is a large boat (20 m) in high performance composite materials. It has the following principal characteristics: A mast-sail constituted of two half-shells in carbon/epoxy, 24 meters long Connecting arms for shells with “x” shape that work in flexure to take up the difference in pitching between the two shells

10

There is a record speed of 34 knots with a class C catamaran (7.6 m in length).

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 194 Monday, November 18, 2002 12:22 PM

Figure 8.18 Elf Aquitaine Catamaran

A total fully equipped mass of 5.3 tons, corresponding to a mass reduction of 50% as compared with a construction in light alloy Example: Competition skiff WM (FRA) 1995 (see Figure 8.19). Example: Surf board 1995 (see Figure 8.20).

8.2.2 Ships In the defense domain, there are composite boats of large dimensions (>50 m): escort-patrollers are expected to be 90 m in length. Example: Anti-mine ocean liner BAMO (FRA). The Catamaran shell is 52 m in length, 15 m in width, and molded in 8 parts. It has 250 tons of glass/polyester composites in monolithic and sandwich construction with balsa core for the bridges and walls (see Figure 8.21).

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 195 Monday, November 18, 2002 12:22 PM

Figure 8.19 Competition Skiff

Figure 8.20 Surf Board

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 196 Monday, November 18, 2002 12:22 PM

Figure 8.21 Anti-mine Ocean Liner

8.3 SPORTS AND RECREATION 8.3.1 Skis Initially made of monolithic wood, the ski has evolved toward composite solutions in which each phase — each in itself a composite material — fulfills a determined function. Figure 8.22 illustrates a transverse cross section of a ski of a previous generation: steel for the elasticity of the element, wood to dampen the vibration, interspersed aluminum for its better adherence to wood. Among the essential mechanical characteristics, the manufacturer has to master the following:

Flexibility in flexure Ski stiffness in torsion (for turning) Elastic limit Fracture limit

One must also note the large diversities of the quality of The snow and the slopes (operating conditions) The skiers (different levels) Taking into account the above specifications requires the manufacturers to provide a large variety of skis. The principal components include The structure is the part of the ski that assures the essential functions as mentioned previously. It may require a piece—or an assembly of several pieces—along the longitudinal direction of the ski, and the cross section

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 197 Monday, November 18, 2002 12:22 PM

Figure 8.22 Cross Section of an Antique Ski

Figure 8.23 Different Ski Cross Section Forms

Figure 8.24 Section of Ski Dynastar

area may take the form shown in Figure 8.23. In fact, other elements can be added to these requirements, which will allow one to control separately stiffness in flexure and stiffness in torsion. The ratio of these two stiffnesses will determine the behavior of the ski, particularly during turning. For this, one uses mainly the following materials: Glass/epoxy Carbon/epoxy Kevlar/epoxy Honeycombs Zicral (AU 2 ZN) Steel alloy Example: Skis Dynastar (FRA): The real appearance of a section is complex, as shown in Figure 8.24, on which one can recognize the “omega,” the box, and the sandwich structures described previously. The filling contributes little to the mechanical characteristics of the whole structure (10% to 15%), but it constitutes the big part in the total volume

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 198 Monday, November 18, 2002 12:22 PM

Figure 8.25 Composite Bicycle

(70 to 80%). Its specific mass has to be as small as possible. The filling can be of Wood, which is sensitive to humidity, with scatter in mechanical characteristics and specific mass depending on the lots Polyurethane foam, with weak mechanical characteristics Acrylic foam, which is very onerous The covers and the edges are in glass/phenol or in glass/granix. The upper edges are in zicral, the lower edges are in steel. The synthetic inner soles have high specific mass.

8.3.2 Bicycles Initially reserved only for competition, numerous variations with frames and wheels made of carbon/epoxy can now be found (see Figure 8.25).

8.4 OTHER APPLICATIONS 8.4.1 Wind Turbines The renewed interest in wind turbines has been caused by the use of composites in the fabrication of the blades. These can be of large dimensions (lengths exceeding 24 meters). Example: Figure 8.26 gives an idea of the size of a wind turbine that develops a maximum power of 33 kW. The blades in glass/epoxy are made here by vacuum 11 forming using two half-shells assemblies by epoxy adhesive bonding. The blades can also be done by filament winding, a process well suited for the construction of torsion box (Figure 8.27). Nevertheless, for longer lengths, the

11

See Section 2.1.3.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 199 Monday, November 18, 2002 12:22 PM

Figure 8.26 Wind Turbines

Figure 8.27 Filament Winding for Wind Turbine

flexure of the blade varies during winding (difference in flexural rigidity in one neutral plane from the other). One can mention also the composite propeller blades for the cooling blowers, 12 which borrow the technology of the aircraft propellers, which have a speed of rotation larger than for the wind turbines. 12

See Section 7.3.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 200 Monday, November 18, 2002 12:22 PM

Figure 8.28 Composite Gas Bottles

8.4.2 Compressed Gas Bottles These are made using filament-wound glass/epoxy or Kevlar/epoxy (see Figure 8.28) reinforcing a thin envelope in light alloy which is used for sealing purposes. The pressure can reach 350 bars in operating conditions (rupture at more than 1,000 bars). The ratio (gas volume/bottle mass) is multiplied by 4 in comparison with the steel solution. Applications include Very light breathing apparatus (for scuba diving) Reservoirs for gaseous fuels Accessories for missiles

8.4.3 Buggy Chassis These are made using glass/epoxy. They are very resilient and can help reduce noise. They are very light with a reduced number of pieces in comparison with the metallic solution. They also offer very good fatigue endurance, as has already 13 been described above for glass/epoxy. Other advantages include the possibility of integration of the “spring” function in the structure of the chassis and increase in the “critical” speed from which a proper mode of vibration can develop in the suspension (see Figure 8.29).

8.4.4 Tubes for Off-Shore Installations These are used in deep waters. The weight of the metallic tubes —or risers— increases proportionally with the depth and can attain high values (one third of the limit stress for a depth of 1000 m). This gives rise to interest in using tubes made of glass/carbon/resin, which are three to four times lighter than tubes made of steel. Example: Production tubes for a cable-held platform. The platform is held with cables toward the bottom (see Figure 8.30). A large number of production 13

See Section 5.4.4.

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 201 Monday, November 18, 2002 12:22 PM

Figure 8.29 M.B.B. Buggy

Figure 8.30 Riser Tubes

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 202 Monday, November 18, 2002 12:22 PM

tubes connect the underwater bottom to the platform. They are subjected to the static and dynamic loadings (due to underwater currents) as: Tension Flexure Circumferential extension and contraction due to external and internal pressures Characteristics: Safety factor as compared with complete rupture: 2 to 3. The micro cracks in the resin require internal and external sealings using elastomers.

8.4.5 Biomechanics Applications The carbon/carbon composites (see Section 3.6) have the rare properties of not provoking fibrous outgrowth when in contact with the blood stream; they are socalled thrombo resistant. In addition, the following qualities also favor their implantation in the human body:

Chemical resistance and inertness Mechanical and fatigue resistance Controllable flexibility due to the nature of composite materials Low specific mass Transparency to different rays Possible sterilization at very high temperatures

The principal applications (to be expanded) for the moment are

Hip and knee implants (in development) Osteosynthesis plates Dental implants Implant apparatus

8.4.6 Telepherique Cabin A substitution using composites on the classical solution for the telepherique cars made of metals gives, at equal mass, a notable augmentation of the useful payload. Example: Company Ingenex/telepherique of Argentieres (FRA): Increasing capacity while keeping existing installations, that is cables—pylons—motorization. Previous metallic telepherique: useful payload 45 passengers New composite telepherique, carbon/Kevlar/epoxy (Figure 8.31): useful load 70 passengers (with the same mass as the previous construction) Augmentation of capacity: 55%

© 2003 by CRC Press LLC

TX846_Frame_C08 Page 203 Monday, November 18, 2002 12:22 PM

Cost comparison: renewal of all installation with the metallic solution ($11 million) Renewal of two telepherique cabins with the composite solution ($1.1 million): cost divided by 10

Figure 8.31 Telepherique Cabin

© 2003 by CRC Press LLC

TX846_Frame_C09 Page 205 Monday, November 18, 2002 12:24 PM

PART II MECHANICAL BEHAVIOR OF LAMINATED MATERIALS We have introduced in the previous part the anisotropic properties of composite 1 materials from a qualitative point of view, and we have indicated the characteristic elastic constants for the behavior of an anisotropic layer in its plane. We have also mentioned the relations that allow one to predict the mechanical behavior of a fiber/matrix combination from the properties of the individual 2 3 constituents. In Chapter 5, we have also given the elements necessary for the sizing of the laminates made of carbon/epoxy, Kevlar/epoxy, and glass/epoxy, in terms of strength and deformation. This second part is dedicated to the justification and application of these properties and results. It requires a detailed study of the behavior of anisotropic composite layers and of the stacking that makes up the laminate. It is useful to note that the basics of the mechanics of continuous media—namely, the state of stress and strain at a point—already described in great details in many texts on mechanics of materials, are supposed to be known.

1 2 3

See Section 3.1. See Section 3.3.1. See Section 5.2/5.3.

© 2003 by CRC Press LLC

TX846_Frame_C09 Page 207 Monday, November 18, 2002 12:24 PM

9 ANISOTROPIC ELASTIC MEDIA 9.1 REVIEW OF NOTATIONS 9.1.1 Continuum Mechanics We consider the following classical notions and notations of the mechanics of continuous media: State of stress at a point: This is defined by a second order tensor with the symbol Â. The 3 by 3 matrix associated with this tensor is symmetric. In this matrix, there are six distinct terms, which are denoted as sij:

s11 ; s22 ; s33 ; s23 ; s13 ; s12 State of strain at a point: This is defined as a second order tensor e. The 3 by 3 matrix for this tensor is symmetric. It consists of six distinct terms denoted as eij:

e11; e22; e33; e23; e13; e12 Linear elastic medium: The strains are linear and homogeneous functions of the stresses. The corresponding relations are:

e ij = j ijk ¥ s k

1

Homogeneous medium: In this case, the matrix terms jijkl characterizing the elastic behavior of the medium are not point functions. They are the same at all points in the considered medium.

1

For example:

e11 = j1111 s11 + j1112 s12 + j1113 s13 + j1121 s21 + j1122 s22 + j1123 s23 + j1131 s31 + j1132 s32 + j1133 s33.

© 2003 by CRC Press LLC

TX846_Frame_C09 Page 208 Monday, November 18, 2002 12:24 PM

9.1.2 Number of Distinct jijk Terms The above stress–strain relation can be written in matrix form as:

Due to the symmetry of the stresses ( s k = s k ), the corresponding coefficients are the same, i.e., j ijk = j ijk . Due to the symmetry of the strains (eij = eji), the corresponding coefficients are the same, i.e., j ijk = j jik . In other words, the knowledge of only the coefficients of the 6 ¥ 6 matrix written above is required. In addition, application of the theorem of virtual work on the stresses 2 shows that the coefficients jijk are symmetric, meaning: j ijk = j kij . Therefore, the 6 ¥ 6 matrix mentioned previously is symmetric. The number of distinct coefficients is: 6(6 + 1 ) -------------------- = 21 coefficients 2 2

Consider two simple stress states: • State No. 1: One single stress, (sk)1, which causes the strain: (eij)1 = jijk (sk)1 • State No. 2: One single stress, (spq)2, which causes the strain: (emn)2 = jmnpq (spq)2 One can write that the work of the stress in state No. 1 on the strain in state No. 2 is equal to the work of the stress in state No. 2 on the strain in state No. 1, as: ( s k ) 1 ¥ ( e k ) 2 = ( s pq ) 2 ¥ ( e pq ) 1 which means: ( s k ) 1 ¥ j kpq ¥ ( s pq ) 2 = ( s pq ) 2 ¥ j pqk ¥ ( s k ) 1 from which one has:

© 2003 by CRC Press LLC

jkpq = jpqk

TX846_Frame_C09 Page 209 Monday, November 18, 2002 12:24 PM

In summary: stress reciprocity: j ijk = j ijk strain definition: j ijk = j jik

(9.1)

symmetry: j ijk = j kij There remain 21 distinct coefficients j ijk The previous stress–strain relation can then be written as: Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

e 11 e 22 e 33 e 23 e 13 e 12

¸ j 1111 Ô Ô j 2211 Ô Ô j 3311 ˝ = j 2311 Ô Ô j 1311 Ô Ô j 1211 ˛

j 1122 j 2222 j 3322 j 2322 j 1322 j 1222

j 1133 j 2233 j 3333 j 2333 j 1333 j 1233

2 j 1123 2 j 2223 2 j 3323 2 j 2323 2 j 1323 2 j 1223

2 j 1113 2 j 2213 2 j 3313 2 j 2313 2 j 1313 2 j 1213

2 j 1112 2 j 2212 2 j 3312 2 j 2312 2 j 1312 2 j 1212

Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

s 11 s 22 s 33 s 23 s 13 s 12

¸ Ô Ô Ô Ô ˝ Ô Ô Ô Ô ˛

The matrix above does not have the general symmetry as in the general form (9 ¥ 9) presented previously. (Note the coefficients 2 in this matrix). One can get around this inconvenience by doubling the terms e23, e13, e12, introducing the shear strains:

g 23 = 2 e 23 ;

g 13 = 2 e 13 ;

g 12 = 2 e 12

from which the stress–strain behavior can then be written in a symmetric form as:

Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

e 11 e 22 e 33 2 e 23 2 e 13 2 e 12

¸ j 1111 j 1122 j 1133 Ô Ô j 2211 j 2222 j 2233 Ô Ô j 3311 j 3322 j 3333 = ˝ 2 j 2311 2 j 2322 2 j 2333 Ô g 23 Ô g 2 j 1311 2 j 1322 2 j 1333 Ô 13 Ô g 12 2 j 1211 2 j 1222 2 j 1233 ˛

2 j 1123 2 j 2223 2 j 3323 4 j 2323 4 j 1323 4 j 1223

2 j 1113 2 j 2213 2 j 3313 4 j 2313 4 j 1313 4 j 1213

2 j 1112 2 j 2212 2 j 3312 4 j 2312 4 j 1312 4 j 1212

Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

s 11 s 22 s 33 s 23 s 13 s 12

¸ Ô Ô Ô Ô ˝ Ô Ô Ô Ô ˛

(9.2)

9.2 ORTHOTROPIC MATERIALS Definition: An orthotropic material is a homogeneous linear elastic material having two planes of symmetry at every point in terms of mechanical properties, these two planes being perpendicular to each other.

© 2003 by CRC Press LLC

TX846_Frame_C09 Page 210 Monday, November 18, 2002 12:24 PM

3

Then one can show that the number of independent elastic constants is nine. The constitutive relation expressed in the so-called “orthotropic” axes, defined by three axes constructed on the two orthogonal planes and their intersection line, can be written in the following form, called the engineering notation because it utilizes the elastic modulus and Poisson ratios:

Ï Ô Ô Ô Ô Ô Ô Ô Ô Ì Ô Ô Ô Ô Ô Ô Ô Ô Ó

¸ e 11 Ô Ô Ô e 22 Ô Ô Ô Ô e 33 Ô ˝ Ô g 23 Ô Ô Ô g 13 Ô Ô Ô g 12 Ô ˛

n 21 n 31 – ------ – -----E2 E3 n 12 n 32 1 – ------ ----- – -----E2 E1 E3 n 13 n 23 1 – ------ – ------ ----E3 E1 E2 1 ----E1

0

0

0

0

0

0

0

0

0

Ï 0 Ô Ô Ô 0 0 0 Ô Ô Ô 0 0 0 ÔÔ Ì Ô 1 0 Ô -------- 0 G 23 Ô Ô 1 0 ------- 0 Ô Ô G 13 1 Ô 0 0 -------- Ô G 12 Ó 0

0

s 11 ¸ Ô Ô Ô s 22 Ô Ô Ô s 33 Ô Ô ˝ Ô s 23 Ô Ô Ô s 13 Ô Ô Ô Ô s 12 ˛

(9.3)

where E1, E2, E3 are the longitudinal elastic moduli. G23, G13, G12 are the shear moduli. n12, n13, n23, n21, n31, n32 are the Poisson ratios. In addition, the symmetry of the stress–strain matrix above leads to the following relations:

n 21 n 12 ------ = ------; E2 E1

n 31 n 13 ------ = ------; E3 E1

n 32 n 23 ------ = ------E3 E2

(9.4)

9.3 TRANSVERSELY ISOTROPIC MATERIALS Definition: A transversely isotropic material is a homogeneous linear elastic material such that any plane including a preferred axis, is a plane of mechanical symmetry. 4 One can show that the constitutive relation has five independent elastic constants. For the fiber/matrix composite shown in Figure 9.1 the preferred axis is . The fibers are distributed uniformly in the direction along . All directions perpendicular to the fibers characterize the transverse direction t. 3 4

Proof is shown in Section 13.1. Proof is shown in Section 13.2.

© 2003 by CRC Press LLC

TX846_Frame_C09 Page 211 Monday, November 18, 2002 12:24 PM

Figure 9.1 Transversely Isotropic Unidirectional

The engineering stress–strain relation has the form: Ï Ô Ô Ô Ô Ô Ô Ô Ô Ì Ô Ô Ô Ô Ô Ô Ô Ô Ó

Ï n n 1 e ¸ ----- – -----t- – -----t0 0 0 Ô Ô E E E t t Ô Ô Ô Ô n n 1 e tt Ô – -----t- ---– ----t 0 0 0 Ô Et E Et Ô Ô Ô Ô n t nt 1 Ô e t¢t¢ Ô --0 0 0 – ----– --Ô Ô E E E t t ˝ = Ì Ô Ô 2 ( 1 + nt ) g tt¢ Ô --------------------- 0 0 0 0 0 Ô Et Ô Ô Ô Ô 1 0 0 0 0 g t¢ Ô ------- 0 Ô G t Ô Ô Ô 1 Ô 0 0 0 0 0 ------- Ô g t Ô G t Ó ˛

s ¸ Ô Ô Ô s tt Ô Ô Ô s t¢t¢ Ô Ô ˝ Ô t tt¢ Ô Ô Ô t t¢ Ô Ô Ô Ô t t ˛

(9.5)

Remarks: The independent elastic constants are

Young modulus along the direction: E. Young modulus along any transverse direction t: Et. Shear modulus in the plane , t: Gt. Poisson coefficients: nt and nt.

The symmetry of the coefficients of the constitutive relation leads to

n n ------t = -----t- E Et One may also note that the shear modulus in the plane t, t¢ can be written as: Et --------------------2 (1 + nt ) This equation is classic for isotropic materials.

© 2003 by CRC Press LLC

TX846_Frame_C10 Page 213 Monday, November 18, 2002 12:25 PM

10 ELASTIC CONSTANTS OF UNIDIRECTIONAL COMPOSITES In this chapter we examine a distinct combination of two materials (matrix and fiber), with simple geometry and loading conditions, in order to estimate the elastic properties of the equivalent material, i.e., of the composite.

10.1 LONGITUDINAL MODULUS E The two materials are shown schematically in Figure 10.1 where m stands for matrix. f stands for fiber. Hypothesis: The two materials are bonded together. More precisely, one makes the following assumptions: Both the matrix m and the fiber f have the same longitudinal strain el. The interface between the two materials allows the z normal strains in the two materials to be different.

ez π ez m

f

The state of stresses resulting from a force F can therefore be written as:

s 0 0 SÆ 0 0 0 m 0 0 0 m

s 0 0 SÆ 0 0 0 f 0 0 0 f

and the corresponding state of strains:

e 0 0 e Æ 0 et 0 m 0 0 ez m

© 2003 by CRC Press LLC

e 0 0 e Æ 0 et 0 f 0 0 ez f

TX846_Frame_C10 Page 214 Monday, November 18, 2002 12:25 PM

Figure 10.1 Longitudinal Modulus E

Each material is assumed to be linear elastic and isotropic, with the following stress–strain relation: 1+n n e = ------------ S – --- trace ( S )I E E

(10.1)

in which e represents the strain tensor, S represents the stress tensor, and I the unity tensor. E and n are the elastic constants of the considered material. For the composite (m + f ), one uses Equation 9.5 with restriction to the plane l,t. It reduces to:

Ï e ¸ Ô Ô Ì et ˝ = Ô Ô Ó g t ˛

1 ----E

n – -----tEt

n – -----tE

1 ---Et

0

0

0

Ï s ¸ Ô Ô 0 Ì st ˝ Ô Ô 1 Ó t t ˛

------G t

The stress s(m+f ) can be written as (see Figure 10.1 above): em ef F F - + s --------------s = --- = ------------------------------ = s --------------( em + ef ) ¥ 1 em + ef em + ef S m + f

m

f 1

which can be written in terms of the volume fractions of the fiber and the matrix as

s m + f

1

See Section 3.2.2.

© 2003 by CRC Press LLC

=

s Vm + s Vf m

f

TX846_Frame_C10 Page 215 Monday, November 18, 2002 12:25 PM

Expressing the stresses in terms of the strains for each material yields E e = Em e Vm + Ef e Vf then: E = Em Vm + Ef Vf

(10.2)

Note: Among the real phenomena that are not taken into account in the expression of El is the lack of perfect straightness of the fibers in the matrix. Also, the modulus El depends on the sign of the stress (tension or compression). In rigorous consideration, the material is “bimodulus.” Example: Unidirectional layers with 60% fiber volume fraction (Vf = 0.60) with epoxy matrix:

E tension (MPa) E compression (MPa)

Kevlar

“HR” Carbon

“HM” Carbon

85,000 80,300

134,000 134,000

180,000 160,000

10.2 POISSON COEFFICIENT Considering again the loading defined in the previous paragraph, the transverse strain for the matrix m and fiber f can be written as:

n e t = – --- s = – ne E and for the composite (m + f ):

n = -----t- ¥ s E m + f m + f et

= – n t e

The strain in the transverse direction can also be written as:

et m + f

et

m + f

De D ( em + ef ) De m - V m + --------f V f - = --------= -----------------------em + ef em ef = et Vm + et Vf m

f

Because e has the same value in m and f: – n t e = – n m e V m - n f e V f

n t = n m V m + n f V f © 2003 by CRC Press LLC

(10.3)

TX846_Frame_C10 Page 216 Monday, November 18, 2002 12:25 PM

10.3 TRANSVERSE MODULUS Et To evaluate the modulus along the transverse direction E, the two materials are shown in the Figure 10.2. In addition, one uses the following simplifications: Hypothesis: At the interface between the two materials, assume the following: Freedom of movement in the l direction allows for different strains in the two materials:

e π e m

f

Freedom of movement in the z direction allows for different strains in the two materials:

ez π ez m

f

Then, the state of stress created by a load F (see Figure 10.2), can be reduced for each material to the following: 0 0 0 S Æ 0 st 0 0 0 0

Figure 10.2 Transverse Modulus Et © 2003 by CRC Press LLC

TX846_Frame_C10 Page 217 Monday, November 18, 2002 12:25 PM

The strains can be written as:

e 0 0 e Æ 0 et 0 0 0 ez m or f Then for the composite (m + f ), one has 1 e t = ---- s t Et On the other hand, using direct calculation leads to (see Figure 10.2) D ( em + ef ) - = et Vm + et Vf e t = -----------------------em + ef m f then: 1 1 1 ---- s = ------ s t V m + ---- s t V f Et t Em Ef

Vm Vf 1 ---- = ------ + ----Em Ef Et

or

1 E t = E m ----------------------------------Em -V ( 1 – V f ) + ----E f

(10.4)

f

Remarks: Due to the above simplifications that allow the possibility for relative sliding along the l and z directions at the interface, the transverse modulus Et above may not be accurate. One finds in the technical literature many more complex formulae giving Et. However, none can provide guaranteed good result. Taking into consideration the load applied (see Figure 10.2),: the modulus Ef that appears in Equation 10.4 is the modulus of elasticity of the fiber in a direction that is perpendicular to the fiber axis. This modulus can be very different from the modulus along the axis of the fiber, due to the 2 anisotropy that exists in fibers. 2

This point was discussed in Paragraph 3.3.1.

© 2003 by CRC Press LLC

TX846_Frame_C10 Page 218 Monday, November 18, 2002 12:25 PM

10.4 SHEAR MODULUS Gt Load application that can be used to evaluate the shear modulus Gt is shown schematically in the Figure 10.3, both with the angular deformations that are produced. The state of stress, identical for both the matrix and fiber material, can be written as: 0 t t 0 S Æ t t 0 0 0 0 0 The corresponding strains can be written as: 0 e t 0 e Æ e t 0 0 m or f 0 0 0 Using the constitutive equation, one has

t t 1+n e t = ------------ t t = -----2G E then:

t t g t = ----G Also, from Figure 10.3, one has

g t m + f

Figure 10.3 Shear modulus Gt © 2003 by CRC Press LLC

( e m + e f ) = g t e m + g t e f m

f

TX846_Frame_C10 Page 219 Monday, November 18, 2002 12:25 PM

which can be rewritten as: = g t V m + g t V f m + f m f

g t

t t t t t t ------ = ------ V m + -----V G t Gm Gf f V V 1 ------- = ------m- + -----f Gm Gf G t 1 G t = G m ----------------------------------Gm - Vf ( 1 – V f ) + -----G

3

(10.5)

f

10.5 THERMOELASTIC PROPERTIES 10.5.1 Isotropic Material: Recall When the influence of temperature is taken into consideration, Hooke’s law for the case of no temperature influence: 1+n n e = ------------ S – --- trace ( S )I E E is replaced by the Hooke–Duhamel law: 1+n n e = ------------ S – --- trace ( S ) I + a DT I E E where

10.5.2

(10.6)

e = Strain tensor S = Stress tensor I = Unity tensor E, n = Elastic constants for the considered material 4 a = Coefficient of thermal expansion DT = Change in temperature with respect to a reference temperature at which the stresses and strains are nil

Case of Unidirectional Composite

The coefficient of thermal expansion of the matrix is usually much larger (more 4 than ten times) than that of the fiber. In Figure 10.4, one can imagine that even in the absence of mechanical loading, a change in temperature DT will produce a 3 4

A few values of the shear modulus Gf are shown in Section 3.3.1. See Section 1.6, “Principal Physical Properties.”

© 2003 by CRC Press LLC

TX846_Frame_C10 Page 220 Monday, November 18, 2002 12:25 PM

Figure 10.4 Unidirectional Composite

longitudinal strain in the composite. This longitudinal strain has a value that is intermediate between the strain of the fiber alone and that of the matrix alone. Then, in the composite one finds internal stresses along the direction l (along the direction t, the fiber and matrix can expand differently). One then has: For the stresses:

s 0 0 SÆ 0 0 0 m 0 0 0 m

s 0 0 SÆ 0 0 0 f 0 0 0 f

For the strains:

e 0 0 e Æ 0 et 0 m 0 0 ez m

e 0 0 e Æ 0 et 0 f 0 0 ez f

10.5.2.1 Coefficient of Thermal Expansion along the Direction l One has for the fiber and the matrix, respectively:

s s e = ------ m + a m DT = e = ----- f + a f DT Em Ef f m The external equilibrium can be written as (see Figure 10.4):

s ¥ em + s ¥ ef = 0 m f © 2003 by CRC Press LLC

TX846_Frame_C10 Page 221 Monday, November 18, 2002 12:25 PM

where, taking into account the equality of the strains: em 1 s ------ m + a m DT = – s ¥ ----¥ ---- + a f DT Em ef Ef m ( a f – a m )DT ( a f – a m )DT ----------------------------= s = ----------------------------em Vm 1 1 1 1 ------ + ----- ¥ --------- + ------ ¥ ---ef Vf Em Em Ef Ef m V represents the volume fraction. The longitudinal strain can then be written as: ( a f E f V f + a m E m V m ) ( DT ) e = e = -----------------------------------------------------------------Ef Vf + Em Vm m f It is also the longitudinal strain that is created only by the effect of temperature:

e

= a DT

m + f where a is the longitudinal coefficient of thermal expansion. One can then equate the above expressions to obtain:

af Ef Vf + am Em Vm a = -----------------------------------------------Ef Vf + Em Vm

(10.7)

10.5.2.2 Coefficient of Thermal Expansion along the Transverse Direction t The global thermal strain can be written as (see Figure 10.4): ef D ( em + ef ) em - = e t --------------- + e t --------------= -----------------------em + ef em + ef em + ef m + f m f

et

then:

et m + f

= et ¥ Vm + et ¥ Vf m

f 5

Using the Hooke and Duhamel law (Equation 10.6) :

n Vm - s + a m DTˆ V m + Ê – ----f s + a f DTˆ V f = Ê – -----Ë Em ¯ Ë Ef ¯ m m + f f et

5

For the Poisson coefficients of common fibers, see Section 3.3.1.

© 2003 by CRC Press LLC

TX846_Frame_C10 Page 222 Monday, November 18, 2002 12:25 PM

Using the expressions for stresses obtained before, one obtains:

et m + f

Ï ¸ ( nf Em – nm Ef ) = Ì ( a m V m + a f V f ) + ---------------------------------V m Vf ( a f – a m ) ˝DT E V + E V m m f f Ó ˛

The quantity between the brackets represent the coefficient of thermal expansion along the transverse direction t, at, which can be written as: ( nf Em – nm Ef ) - ¥ ( af – am ) a t = a m V m + a f V f + --------------------------------E Em ------ + ------fV V f

(10.8)

m

10.5.3 Thermomechanical Behavior of a Unidirectional Layer Under the combined effect of the stresses and temperature, the global thermomechanical strains of a unidirectional layer can be obtained using the following relation: 1 -----

E Ï e ¸ Ô Ô v Ì e t ˝ = – -----tE Ô Ô Ó g t ˛ 0

n

t – ----E t

1 ---Et

0

0

Ï a ¸ Ï s ¸ Ô Ô Ô Ô 0 Ì s t ˝ + DT Ì a t ˝ Ô Ô Ô Ô Ó0˛ 1 Ó t t ˛

(10.9)

------G t

in which the coefficients E, Et, vt, Gt, a and at have the values given by the Equations 10.2 to 10.8, respectively.

© 2003 by CRC Press LLC

TX846_Frame_C11 Page 223 Monday, November 18, 2002 12:26 PM

11 ELASTIC CONSTANTS OF A PLY ALONG AN ARBITRARY DIRECTION To study the behavior of a laminate made up of many plies with different orientations, it is necessary to know the behavior of each of the plies in directions that are different from the principal material directions of the ply. We propose to determine the elastic constants for this ply behavior using relatively simple calculations.

11.1 COMPLIANCE COEFFICIENTS 1

The ply is already defined in Chapter 3. Let , t and z be the orthotropic axes 2 of a ply shown in the Figure 11.1. For a thin laminate made up by a superposition of many plies, we assume that the stresses szz are zero. It is then possible, for an orthotropic material, to write the stress–strain relation in the plane ,t starting from Equation 9.3 or 9.5 in the form: n

l t - – -----Ï e ¸ Ï ---Et Ô Ô Ô E Ô Ô Ô nt l ---Ì e t ˝ = Ì – -----Et E Ô Ô Ô Ô Ô Ô 0 0 Ó g t ˛ Ó

0 ¸Ï s ¸ ÔÔ Ô ÔÔ Ô 0 ˝Ì s t ˝ ÔÔ Ô l Ô -------- ÔÔ G t ˛Ó t t ˛

(11.1)

Problem: How can one transform this relation expressed in the coordinates ,t into a relation expressed in coordinates x,y inclined at an angle of q with the ,t 3 coordinates (see Figure 11.1). First recall the following: 1 2 3

See Section 3.2. The orthotropic axes 1,2,3 in Equation 9.3 are now called l,t,z, respectively. What follows is treated more globally and completely in Section 13.2.2.

© 2003 by CRC Press LLC

TX846_Frame_C11 Page 224 Monday, November 18, 2002 12:26 PM

Figure 11.1 Orthotropic Axes and Arbitrary Direction in the Plane of a Ply

Recall 1: The stress s acting on a surface with a normal vector n is given by { σ } = [ σ ij ] { n }

(11.2) column matrix of stress components σ

stress matrix

column matrix of direction cosines n

Recall 2: The coordinates of the same vector V in axes x,y as well as ,t, such that ( x . ) = cos q, are V = V + Vt t = Vx x + Vy y with the relation: Ï V x ¸ Ï c s ¸Ï V ¸ Ì ˝ = Ì ˝Ì ˝ Ó V y ˛ Ó – s c ˛Ó V t ˛

Ê c = cos q ˆ Ë c = sin q ¯

(11.3)

In axes ,t the stress acting on the surface with a normal x can be expressed as follows, using Equation 11.2 above: Ïc ¸ { s /x } ,t = [ s ij ] ,t { x } ,t = [ s ij ] ,t Ì ˝ Ós ˛ where {s/x} is the stress vector and [sij] is the stress matrix and in axes x,y, following Equation 11.3:

{ s /x } x,y =

© 2003 by CRC Press LLC

Ïc ¸ [ s ij ] ,t Ì ˝ –s c Ós ˛ c

s

TX846_Frame_C11 Page 225 Monday, November 18, 2002 12:26 PM

In a similar manner, the stresses acting on the surface with the normal y are written in the x,y axes as:

{ s /y } x,y =

Ï –s ¸ [ s ij ] ,t Ì ˝ c Óc˛

c

s

–s

Therefore, the matrix of stresses in the x,y axes is: c

{ s ij } x,y = [ s /x , s /y ] =

s

–s c

[ s ij ] ,t

c –s s

c

in setting:

c

[P] =

s

–s c

and observing that the matrix [P] is orthogonal ( [P] = [P] ), one has –1

t

4

[ s ij ] , t = [ P ] [ s ij ] x, y [ P ] t

t

where [P] is the transpose of matrix [P]. This expression can be developed to become

s t t s x t xy c s = c –s s c t xy s y – s c t t s t One can also rearrange the equation to be Ï s ¸ Ô Ô Ì st ˝ = Ô Ô Ó t t ˛

2

s

2

2

c s

sc

c

2

– sc

Ï sx ¸ Ô Ô 2cs Ì sy ˝ Ô Ô 2 2 ( c – s ) Ó t xy ˛ – 2cs

Then: [ s ] ,t = [ T ] [ s ] x,y 4

One has: sx,y = Ps,t P; st P = Psxy; Ps,t = sx,y P; s,t = Psx,yP.

© 2003 by CRC Press LLC

t

t

t

t

(11.4)

TX846_Frame_C11 Page 226 Monday, November 18, 2002 12:26 PM

5

with

c [T ] =

s

2

s

2

2

– 2sc

2

2sc

c

sc

(c – s ) 2

– sc

2

In a similar manner, the strain components can be transformed as: 2 2 Ï ex ¸ c s Ô Ô 2 Ì ey ˝ = s c2 Ô Ô – cs cs Ó e xy ˛

Ï e ¸ Ô Ô – 2cs Ì e t ˝ Ô 2 2 Ô ( c – s ) Ó e t ˛ 2cs

or: 2 Ï ex ¸ s c Ô Ô 2 2 s Ì ey ˝ = c Ô Ô Ó g xy ˛ – 2cs 2cs 2

Ï e ¸ Ô Ô Ì et ˝ – cs Ô Ô 2 2 ( c – s ) Ó g t ˛ cs

Ïe ¸ Ïe ¸ Ì ˝ = [T ¢]Ì ˝ Ó g ˛x,y Ó g ˛,t

then: with:

c [T ¢] =

s

2

2

s

2

cs

2

– cs

c

– 2cs 2cs

(c – s ) 2

2

The stress–strain Equation 11.1 can then be expressed in the axes x,y since we have written:

Ïe ¸ Ïe ¸ Ïe ¸ Ì ˝ = [T ¢]Ì ˝ ; Ì ˝ = Ó g ˛x,y Ó g ˛,t Ó g ˛,t

1 ----E

– n t ---------Et

– n t ---------E

1 ---Et

0

5

0

0 0 { s } ,t ; { s } ,t = [ T ] { s } x,y 1 -------G t

This [T ] matrix is readily established if one knows the relation that allows one to express the components of a tensor in one system in terms of the components of the same tensor in m m m another system. Here this relation is: s IJ = cos I cos J smn with cos I = cos(m,I ); see Section 13.1.

© 2003 by CRC Press LLC

TX846_Frame_C11 Page 227 Monday, November 18, 2002 12:26 PM

where after substitution: n t -------E t

1 ----E

n

[ T ¢ ] – ------t E

0

1 ---Et

0

Ï sx ¸ Ô Ô Ô Ô 0 [ T ] Ì sy ˝ Ô Ô Ô Ô 1 -------Ó t xy ˛ G t 0

Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

Ï ex ¸ Ô Ô Ô Ô Ì ey ˝ = Ô Ô Ô Ô Ó g xy ˛

new matrix of elastic coefficients in x,y axes

When all calculations are performed, one obtains the following constitutive relation, written in the coordinates x,y that make an angle q with the axes ,t. The elastic moduli and Poisson coefficients appear in these relations. One can also see the 6 existence of the coupling coefficients h and m, which demonstrates that a normal 7 stress can produce a distortion. Ï ex ¸ Ô Ô Ô Ô Ì ey ˝ = Ô Ô Ô Ô Ó g xy ˛

yx – ------E y

h xy -------G xy

xy – ------E x

1 --Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

n

1 --Ex

n

Ï sx ¸ Ô Ô Ô Ô Ì sy ˝ Ô Ô Ô Ô Ó t xy ˛

with: 1 E x ( q ) = ---------------------------------------------------------4 4 n tˆ 2 2 1 c s ----- + ---- + c s Ê -------- – 2 -----Et Et ¯ E Ë Gt 1 E y ( q ) = ---------------------------------------------------------4 4 n tˆ 2 2 1 s c ----- + ----- + c s Ê -------- – 2 -----Et Et ¯ E Ë Gt

(11.5)

1 -2 G xy ( q ) = ----------------------------------------------------------------------n tˆ ( c 2 – s 2 ) 2 2Ê 1 1 ------------------------------4c s E + E + 2 E + G Ë t t¯ t

6

7

n yx ------(q) Ey

=

n t 4 -----(c Et

h xy -------(q) G xy

Ï c2 s2 n t 2 2 1 ˆ¸ - – ---- + ( c – s ) Ê -----– ---------= – 2cs Ì ---E Et Ë Et 2Gt¯ ˝ Ó ˛

m xy -------(q) G xy

Ï s2 c2 n t 2 2 1 ˆ¸ - – ----- – ( c – s ) Ê -----– ---------= – 2cs Ì ---E Et Ë Et 2Gt¯ ˝ Ó ˛

4 2 2 1 1 1 - + ---- – ------ˆ + s ) – c s Ê ---Ë E Et Gt¯

Recall that the matrix of elastic coefficients is symmetric, meaning in particular: hxy /Gxy = hx /Ex and mxy /Gxy = my /Ey. See example described in Section 3.1.

© 2003 by CRC Press LLC

TX846_Frame_C11 Page 228 Monday, November 18, 2002 12:26 PM

11.2 STIFFNESS COEFFICIENTS When one inverts Equation 11.1 written in the coordinate axes l,t of a ply, one obtains n E

------------------Ï s ¸ ( 1 – n t n tl ) Ô Ô n t E t Ô Ô Ì s t ˝ = (-------------------1 – n t n t ) Ô Ô Ô Ô 0 Ó t t ˛

E

0 Ï e ¸ Ô Ô Ô Ô 0 Ì et ˝ Ô Ô Ô Ô G t Ó g t ˛

t --------------------

( 1 – n t n t ) Et -------------------( 1 – n t n t )

0

where the “stiffness” coefficients appear, as opposed to the Equation 11.1 where the “compliance” coefficients appear. To simplify the writing, one can denote Ï sl ¸ E Ô Ô Ì s t ˝ = n t E t Ô Ô 0 Ó t t ˛

0 Ï e ¸ Ô Ô 0 Ì et ˝ Ô Ô G t Ó g t ˛

n t E Et 0

(11.6)

An identical procedure can be followed to arrive at the stress–strain relation: c s

2

2

– cs

s

2

c

2

Ï s ¸ Ô Ô – 2cs Ì s t ˝: Ô Ô 2 2 ( c – s ) Ó t t ˛ 2cs

cs

Ï Ô Ô Ô Ì Ô Ô Ô Ó

Ï sx ¸ Ô Ô Ì sy ˝ = Ô Ô Ó t xy ˛

[ T1 ] (11.7) 2

s

2

2

c

2

c s

2cs

– 2c s

–c s cs (c – s ) 2

2

Ï ex ¸ Ô Ô Ì ey ˝ Ô Ô Ó g xy ˛

Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

Ï e ¸ Ô Ô Ì et ˝ = Ô Ô Ó g t ˛

[ T 1¢ ] Recall that axes x,y are derived from the axes ,t by a rotation q about the third axis z. Substituting Equations 11.7 into 11.6, one obtains Ï sx ¸ E Ô Ô Ì s y ˝ = [ T 1 ] n t E t Ô Ô 0 Ó t xy ˛

n t E Et 0

Ï ex ¸ Ô Ô 0 [ T 1¢ ] Ì e y ˝ Ô Ô G t Ó g xy ˛ 0

which can be rewritten as: Ï sx ¸ E 11 E 12 E 13 Ô Ô Ì s y ˝ = E 21 E 22 E 23 Ô Ô Ó t xy ˛ E 31 E 32 E 33

© 2003 by CRC Press LLC

Ï ex ¸ Ô Ô Ì ey ˝ Ô Ô Ó g xy ˛

TX846_Frame_C11 Page 229 Monday, November 18, 2002 12:26 PM

Once the calculations are performed, one obtains the following expressions for the stiffness coefficients E ij , where c = cosq and s = sinq.

Ï sx ¸ E 11 E 12 E 13 Ô Ô s = Ì y˝ E 21 E 22 E 23 Ô Ô t Ó xy ˛ E 31 E 32 E 33

Ï ex ¸ Ô Ô Ì ey ˝ Ô Ô Ó g xy ˛

with: E 11 ( q ) = c E + s E t + 2c s ( n t E + 2G t ) 4

4

2 2

E 22 ( q ) = s E + c E t + 2c s ( n t E + 2G t ) 4

4

2 2

2 2

E 33 ( q ) = c s ( E + E t – 2 n t E ) + ( c – s ) G t 2 2

2

(11.8)

E 12 ( q ) = c s ( E + Et – 4G t ) + ( c + s ) n t E 2 2

4

4

E 13 ( q ) = – cs { c E – s E t – ( c – s ) ( n t E + 2G t ) } 2

2

2

2

E 23 ( q ) = – cs { s E – c E t + ( c – s ) ( n t E + 2G t ) } 2

2

2

2

expressions in which: E = E / ( 1 – n t n t ) : E t = E t / ( 1 – n t n t ) The rate of variation of stiffness coefficients E ij as functions of the angle q is repre sented in Figure 11.2 for a ply characterized by moduli E and Et with very different 8 values, for example the case of unidirectional layers of fiber/resin.

11.3 CASE OF THERMOMECHANICAL LOADING 11.3.1 Compliance Coefficients 9

When considering the temperature variations, one must substitute the stress–strain Equation 11.1 with Equation 10.9: Ï e ¸ Ô Ô Ô Ô Ì et ˝ = Ô Ô Ô Ô Ó g t ˛ 8 9

1 ----E

n

n

t – -----E t

t – -----E

1 ---Et

0

0

0 Ï s ¸ Ï a ¸ Ô Ô Ô Ô Ô Ô Ô Ô 0 Ì s t ˝ + DT Ì a t ˝ Ô Ô Ô Ô Ô Ô Ô 1 Ô -------Ó0˛ G t Ó t t ˛

See characteristics of the fiber/resin unidirectionals in Paragraph 3.3.3. See Section 10.5.

© 2003 by CRC Press LLC

TX846_Frame_C11 Page 230 Monday, November 18, 2002 12:26 PM

Figure 11.2 Variation of Stiffness Coefficients for a Misaligned Ply

in which a and a t are the coefficients of thermal expansion of the unidirectional layer along the longitudinal direction and transverse direction t, respectively. Following the same procedure as in Section 11.1 with the same notations, one can write

Ïe ¸ Ïe ¸ Ì ˝ = [ T ¢ ] Ì ˝ ; { s } ,t = [ T ] { s } x,y Ó g ˛x,y Ó g ˛,t

© 2003 by CRC Press LLC

TX846_Frame_C11 Page 231 Monday, November 18, 2002 12:26 PM

Then, upon substituting, Ï ex ¸ Ô Ô Ô Ô Ì ey ˝ = [ T ¢ ] Ô Ô Ô Ô Ó g xy ˛

1 ----E

n

n

t – -----E

0

t

t – -----E

1 ---Et

0

0

0

1 -------G t

Ï a ¸ Ï sx ¸ Ô Ô Ô Ô Ô Ô Ô Ô [ T ] Ì s y ˝ + DT [ T ¢ ] Ì a t ˝ Ô Ô Ô Ô Ô Ô Ô Ô Ó0˛ Ó t xy ˛

One finds again in the first part of the second term a matrix of compliance coefficients, the terms of which are described in details in Equation 11.5. The second part of the second term is written as: 2

s

2

2

c

2

– 2 cs

2cs

c DT

s

Ï a ¸ Ï c a + s at ¸ Ô Ô Ô Ô – c s Ì a t ˝ = DT Ì s 2 a + c 2 a t ˝ Ô Ô Ô Ô 2 2 Ó 2cs ( a t – a ) ˛ (c – s ) Ó 0 ˛ 2

cs

2

Therefore, the thermomechanical relation for a unidirectional layer written in the axes x.y, different from the ,t coordinates, can be summarized as follows:

h xy -------G xy

n

1 yx ----- – ------Ï ex ¸ Ex Ey Ô Ô Ô Ô n xy 1 ----Ì e y ˝ = – ------Ey Ex Ô Ô hx my Ô Ô ---------Ó g xy ˛ Ex Ey

m xy -------G xy 1 -------G xy

Ï sx ¸ Ô Ô Ô Ô Ì s y ˝ + DT Ô Ô Ô Ô Ó t xy ˛

Ï ax ¸ Ô Ô Ô Ô Ì ay ˝ Ô Ô Ô Ô Ó a xy ˛

E x , E y ,G xy , n xy , n yx , h xy , m xy are given by the relations [11.5]

ax = c a + s at 2

2

ay = s a + c at 2

2

a xy = 2cs ( a t – a ) c = cos q ; s = sin q

© 2003 by CRC Press LLC

(11.9)

TX846_Frame_C11 Page 232 Monday, November 18, 2002 12:26 PM

11.3.2 Stiffness Coefficients Inverting Equation 10.9 gives

E

n E

t -------------------- -------------------- 0 Ï s ¸ ( 1 – n t n t ) ( 1 – n t n t ) Ô Ô Ô Ô n t E t Et - -------------------- 0 Ì s t ˝ = -------------------( 1 – n t n t ) ( 1 – n t n t ) Ô Ô Ô Ô Ó t t ˛ G t 0 0

Ï e ¸ Ô Ô Ô Ô Ì e t ˝º Ô Ô Ô Ô Ó g t ˛ n E

E

t Ï --------------------------------------- ¸ Ô ( 1 – nt nt ) a + ( 1 – nt nt ) a t Ô Ô Ô º – DT Ì nt Et Et ˝ --------------------------------------a + a l t Ô ( 1 – nt nt ) ( 1 – n t n t ) Ô Ô Ô 0 Ó ˛

Following the procedure of Section 11.2, with the same notations, one can write: Ïe ¸ Ïe ¸ { s } x,y = [ T l ] { s } ,t ; Ì ˝ = [ T 1¢ ] Ì ˝ Ó g ˛,t Ó g ˛x,y where after substitution: Ï E a + n t E a t ¸ Ï sx ¸ Ï ex ¸ E n t E 0 Ô Ô Ô Ô Ô Ô Ì s y ˝ = [ T l ] n t E t Et 0 [ T 1¢ ] Ì e y ˝ – DT [ T l ] Ì n t E t a + E t a t ˝ Ô Ô Ô Ô Ô Ô 0 0 0 G t Ó ˛ Ó t xy ˛ Ó g xy ˛ One finds again, in the first part of the second term, the matrix detailed in Equation 11.8. The second part of the second term can be developed as follows:

c – DT

s

2

2

– cs

s

2

c

2

cs

2cs Ï E a + n t E a t ¸ Ô Ô – 2c s Ì n t E t a + E t a t ˝ = º Ô Ô 2 2 0 ˛ (c – s ) Ó Ï c E ( a + n t a t ) + s E t ( n t a + a t ) ¸ Ô Ô º – DT Ì s 2 E ( a + n t a t ) + c 2 E t ( n t a + a t ) ˝ Ô Ô Ó cs [ E t ( n t a + a t ) – E ( a + n t a t ) ] ˛ 2

© 2003 by CRC Press LLC

2

TX846_Frame_C11 Page 233 Monday, November 18, 2002 12:26 PM

Therefore, the thermomechanical behavior of a unidirectional layer in the coordinate axes x,y can be written in the following form, in terms of the properties in the ,t coordinates.

Ï sx ¸ E 11 E 12 E 13 Ô Ô Ì s y ˝ = E 21 E 22 E 23 Ô Ô Ó t xy ˛ E 31 E 32 E 33

Ï ex ¸ Ô Ô Ì e y ˝ – DT Ô Ô Ó g xy ˛

Ï a E1 ¸ Ô Ô Ì a E2 ˝ Ô Ô Ó a E3 ˛

E 11 E 22 E 33 E 12 E 13 E 23 are given by the relations [11.8]

a E 1 = c E ( a + n t a t ) + s E t ( n t a + a t ) 2

2

a E 2 = s E ( a + n t a t ) + c E t ( n t a + a t ) 2

2

a E 3 = cs [ E t ( n t a + a t ) – E ( a + n t a t ) ] c = cos q ; s = sin q E = E / ( 1 – n t n t ) E t = E t / ( 1 – n t n t )

© 2003 by CRC Press LLC

(11.10)

TX846_Frame_C12 Page 235 Monday, November 18, 2002 12:27 PM

12 MECHANICAL BEHAVIOR OF THIN LAMINATED PLATES 1

The definition of a laminate was given in Chapter 5. In the same chapter the practical calculation methods for the laminate was also described. We propose here to justify these methods, meaning to study the behavior of the laminate when it is subjected to a combination of loadings. This study is necessary if one wants 2 to have correct design with strains or stresses within their admissible values.

12.1 LAMINATE WITH MIDPLANE SYMMETRY 12.1.1

Membrane Behavior 3

We consider in the following a laminate with midplane symmetry. The total thickness of the laminate is denoted as h. It consists of n plies. Ply number k has a thickness denoted as ek (see Figure 12.1). Plane x, y is the plane of symmetry.

12.1.1.1 Loadings The laminate is subjected to loadings in its plane. The stress resultants are denoted as Nx, Ny, Txy = Tyx. These are the membrane stress resultants.They are defined as: Nx: Stress resultant in the x direction over a unit width along the y direction. th

Nx =

Ú

n ply

h/2 – h/2

s x dz =

Â

( sx )k ¥ ek

(12.1)

st

k=1 ply

Ny: Stress resultant along the y direction over a unit width along the x direction. th

Ny =

1 2 3

Ú

h/2 – h/2

n ply

s y dz =

Â

( sy )k ¥ ek

(12.2)

st

k=1 ply

See Section 5.2. The problem of buckling of the laminates is not the scope of this chapter. See Appendix 2. See Section 5.2.3.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 236 Monday, November 18, 2002 12:27 PM

Figure 12.1 Definition of Laminate and Membrane Loading

Txy (or Tyx ): Membrane shear stress resultant over a unit width along the y direction (or respectively along the x direction): th

T xy =

Ú

n ply

h/2 – h/2

Â

t xy dz =

( t xy ) k ¥ e k

(12.3)

st

k=1 ply

12.1.1.2 Displacement Field The elastic displacement at each point of the laminate is assumed to be two dimensional, in the x, y plane of the laminate. It has the components: uo , vo. The nonzero strains can be written as:

e ox = ∂ u 0 / ∂ x e oy = ∂ v 0 / ∂ y g oxy = ∂ u 0 / ∂ y + ∂ v 0 / ∂ x It was shown in the previous chapter (Equation 11.8) that one can express, in a given coordinate system, the stresses in a ply as functions of the strains. Then the stress resultant Nx defined in Equation 12.1 can be written as follows: th

n ply

Nx =

Â

k

k

k

{ E 11 e ox + E 12 e oy + E 13 g oxy }e k

st

k=1 ply

then: N x = A 11 e ox + A 12 e oy + A 13 g oxy © 2003 by CRC Press LLC

TX846_Frame_C12 Page 237 Monday, November 18, 2002 12:27 PM

with: th

th

n ply

A 11 =

Â

th

n ply

Â

k 11 k

E e ; A 12 =

st

n ply k 12 k

E e ; A 13 =

st

k=1 ply

Â

k

E 13 e k

st

k=1 ply

k=1 ply

In an analogous manner, one obtains for the Equation 12.2: N y = A 21 e ox + A 22 e oy + A 23 g oxy with: th

n ply

Â

A 2j =

k

E 2j e k

st

k=1 ply

and for the shear stress resultant Txy one can write, starting from Equation 12.3: T xy = A 31 e ox + A 32 e oy + A 33 g oxy with: th

n ply

Â

A 3j =

k

E 3j e k

st

k=1 ply

Therefore, it is possible to express the stress resultants in the following matrix form: Ï Nx ¸ A 11 A 12 A 13 Ô Ô N = Ì y˝ A 21 A 22 A 23 Ô Ô T A 31 A 32 A 33 Ó xy ˛ with:

Ï e ox ¸ Ô Ô Ì e oy ˝ Ô Ô Ó g oxy ˛

4

(12.4)

th

n ply

A ij =

Â

k

E ij e k = A ji

st

k=1 ply

Remarks: One observes from the above expressions that coefficients Aij are independent of the stacking order of the plies. One can also see that the normal stress resultants Nx or Ny create angular distortions. This coupling will disappear if the laminate is balanced. This means that apart from the midplane symmetry, there are as many and identical plies that make with the x axis an angle +q as those that make 4

The developments of E ij are given in Equation 11.8.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 238 Monday, November 18, 2002 12:27 PM

with the x axis an angle -q. In effect, the coefficients E 13 and E 23 are 6 antisymmetric in q and, therefore, cancel each other out for the pairs of plies at ±q when one calculates the terms A13 and A23. The result is then: 5

A 13 = A 23 = 0 and the stress–strain relation for the laminate is reduced to Ï Nx ¸ A 11 A 12 0 Ô Ô N = Ì y˝ A 12 A 22 0 Ô Ô 0 0 A 33 Ó T xy ˛

Ï e ox ¸ Ô Ô Ì e oy ˝ Ô Ô Ó g oxy ˛

(12.5)

It is possible to substitute the stress resultants Nx, Ny, Txy with the global average stresses (which are fictitious):

s ox = N x /h s oy = N y /h

(12.6)

t oxy = T xy /h One then deduces from Equation 12.4 the average membrane stress–strain behavior of a laminate as: Ï s ox ¸ A 11 A 12 A 13 Ô Ô 1 -s = Ì oy ˝ h A 21 A 22 A 23 Ô Ô t A 31 A 32 A 33 Ó oxy ˛

Ï e ox ¸ Ô Ô Ì e oy ˝ Ô Ô Ó g oxy ˛

(12.7)

One can also note that according to Equation 12.4 the terms of the matrix 1 ---[A] above can be written as: h th

1 --- ¥ A ij = h

n ply

Â st

e k E ij ¥ ----k h

k=1 ply

Then the ratios ek /h can be rearranged to obtain the proportions of plies having the same orientation. In case where these proportions have already been fixed—and therefore their numerical values are known—it becomes possible to calculate the terms --h1-Aij without knowing the thickness. For example, if the selected orientak tions are 0∞, 90∞, +45∞, -45∞, and by denoting p (%) as the percentages of the plies along the different orientations, one has: 1 --- ¥ A ij = E ij0∞ ¥ p 0∞ + E ij90∞ ¥ p 90∞ + E ij+45∞ ¥ p +45∞ + E ij-45∞ ¥ p -45∞ h 5 6

See Figure 12.1 and figure in the Equation 11.8. The expressions developed for E ij are given in Equation 11.8.

© 2003 by CRC Press LLC

(12.8)

TX846_Frame_C12 Page 239 Monday, November 18, 2002 12:27 PM

Figure 12.2 Practical Determination of a Laminate Subject to Membrane Loading

12.1.2 Apparent Moduli of the Laminate Inversion of Equation 12.7 above allows one to obtain what can be called as apparent moduli and coupling coefficients associated with the membrane behavior in the plane x,y. These coefficients appear in the following relation: Ï e ox ¸ Ï s ox ¸ Ô Ô Ô Ô Ô Ô Ô –1 Ô Ì e oy ˝ = h [ A ] Ì s oy ˝ = Ô Ô Ô Ô Ô Ô Ô Ô Ó g oxy ˛ Ó t oxy ˛

1 ----Ex

yx –n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï s ox ¸ Ô Ô Ô Ô Ì s oy ˝ Ô Ô Ô Ô Ó t oxy ˛

(12.9)

12.1.3 Consequence: Practical Determination of a Laminate Subject to Membrane Loading Given: The stress resultants are given and denoted as: Nx, Ny, Txy. Using the values of these stress resultants, one can estimate the ply 7 proportions in the four orientations. Assume in Figure 12.2 that the plies are identical (same material and same thickness). The problem is to determine The apparent elastic moduli of the laminate and the associated coupling coefficients, in order to estimate strains under loading The minimum thickness for the laminate in order to avoid rupture of one of the plies in the laminate

7

See Section 5.4.3.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 240 Monday, November 18, 2002 12:27 PM

12.1.3.1 Principle of Calculation Apparent moduli of the laminate: The matrix --h1-[A] evaluated using Equation 12.8 can be inverted, and one obtains Equation 12.9 as: Ï e ox ¸ Ô Ô Ô Ô Ì e oy ˝ = Ô Ô Ô Ô Ó g oxy ˛

1 ----Ex

yx –n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï s ox ¸ Ô Ô Ô Ô Ì s oy ˝ Ô Ô Ô Ô Ó t oxy ˛

We have already determined the apparent moduli and the coupling coefficients of the laminate. Nonrupture of the laminate: Let s, st, and tt be the stresses in the orthotropic axes , t of one of the plies making up the laminate that is subjected to the loadings Nx, Ny, Txy. Let h be the thickness of the laminate (unknown at the moment) so that the rupture limit of the ply using the Hill–Tsai failure criterion is just reached. 8 One then has for this ply :

s s t s s t t t -----2 + -----2 – ---------- = 1 + ----2 2 s st s t t 2

2

2

rupture rupture rupture rupture

Multiplying the two parts of this equation with the square of thickness h: ( s h ) ( s t h ) ( s h ) ( s t h ) ( t t h ) --------------- + -------------- – --------------------------- = h2 - + --------------2 2 2 2 s st t t s 2

rupture

2

rupture

2

rupture

(12.10)

rupture

To obtain the values (s h), (sth), (tt h), one has to multiply with h the global stresses sox, soy, toxy that are applied on the laminate, to become (soxh), (soy h), (toxy h) which are the known stress resultants: N x = ( s ox h ); N y = ( s oy h ); T xy = ( t oxy h ) Then, for a ply, the calculation of the Hill–Tsai criterion can be done by substituting for the unknown global stresses the known stress resultants Nx, Ny, Txy. This leads to the calculation of the thickness h so that the ply under consideration does not fracture. In this way, each ply number k leads to a laminate thickness value denoted as hk. The final thickness to be retained will the one with the highest value. 8

For the Hill–Tsai failure criterion, see Section 5.2.3 and detailed explanation in Chapter 14.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 241 Monday, November 18, 2002 12:27 PM

12.1.3.2 Calculation Procedure 1. Complete calculation: The ply proportions are given, the matrix --h1- [A] of the Equation 12.7 is known, and then—after inversion—we obtain the 9 elastic moduli of the laminate (Equation 12.9). Multiplying 12.9 with the thickness h (unknown) of the laminate: 1 ----Ï h e ox ¸ Ex Ô Ô Ô Ô xy Ì h e oy ˝ = –n------Ex Ô Ô Ô Ô hx -----Ó h g oxy ˛ E

yx –n------Ey

h xy -------G xy

1 ----Ey

m xy -------G xy

my

1 -------G xy

----

Ey

x

Ï Nx ¸ Ô Ô Ô Ô Ì Ny ˝ Ô Ô Ô Ô Ó T xy ˛

Then introducing a multiplication factor of h for the stresses in the ply—or the group of plies—corresponding to the orientation k (see Equation 11.8): E 11 Ï h sx ¸ Ô Ô Ì h s y ˝ = E 21 Ô Ô E 31 Ó h t xy ˛ ply n∞k

E 12 E 22 E 32

E 13 Ï h e ox ¸ Ô Ô E 23 Ì h e oy ˝ Ô Ô E 33 Ó h g oxy ˛

ply n∞k

laminate

and in the orthotropic coordinates of the ply (see Equation 11.4): 2 2 Ï h s ¸ s – 2cs c Ô Ô 2 2 h s = Ì t˝ c 2cs s Ô Ô 2 2 h t Ó t ˛ sc – sc ( c – s )

Ï h sx ¸ Ô Ô Ì h sy ˝ Ô Ô Ó h t xy ˛

ply n∞k

ply n∞k

ply n∞k

c = cos q ; s = sin q

Saturation of the Hill–Tsai criterion leads then to Equation 12.10 where the above known stress resultants values appear in the numerator as: ( h s ) ( h s t ) ( h s ) ( h s t ) ( h t t ) --------------- + -------------- – --------------------------- = h2 ¥ 1 - + ------------2 2 2 2 s st t t s 2

rupture

2

2

rupture

rupture

rupture

After having written an analogous expression for each orientation k of the plies, one retains for the final value of the laminate thickness, the maximum value found for h. 9

One can read directly these moduli in Tables 5.1 to 5.15 of Section 5.4.2 for balanced laminates of carbon, Kevlar, and glass/epoxy with Vf = 60% fiber volume fraction.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 242 Monday, November 18, 2002 12:27 PM

(2) Simplified calculation: One can write more rapidly the Equation 12.10 if one knows at the beginning for each orientation the stresses due to a global uniaxial state of unit stress applied on the laminate: first s ¢ox = 1 (for example, 1 MPa), then s ¢¢oy = 1 MPa, then t ¢¢¢ oxy = 1 MPa. Assume first that the state of stress is given as: ¢ = 1 ( MPa ) s ox

s ox ¢ = 0 t ¢oxy = 0 Inverting the Equation 12.9 leads to Ï e o¢ x Ô Ô Ì e o¢ y Ô Ô ¢ Ó g oxy

¸ Ô Ô ˝ = Ô Ô ˛

1 ----Ex

yx –n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï 1 MPa ¸ Ô Ô Ô Ô Ì 0 ˝ Ô Ô Ô Ô Ó 0 ˛

which can be considered as “unitary strains” of the laminate. These allow the calculation of the stresses in each ply by means of Equations 11.8 and then 11.4, successively, as: Ï s ¢x Ô Ì s ¢y Ô Ó t x¢ y

E 11 ¸ Ô ˝ = E 21 Ô E 31 ˛

ply n∞k

E 12 E 22 E 32

E 13 Ï e o¢ x Ô E 23 Ì e o¢ y Ô E 33 Ó g o¢ xy

ply n∞k

¸ Ô ˝ Ô ˛

laminate

and in the orthotropic coordinates of the ply (Equation 11.4): Ï s ¢ Ô Ì s ¢t Ô Ó t ¢ t

2 2 ¸ s – 2cs c Ô 2 2 = ˝ c 2cs s Ô 2 2 ˛ sc – sc ( c – s )

ply n∞k

ply n∞k

Ï s ¢x Ô Ì s ¢y Ô Ó t ¢x y

¸ Ô ˝ Ô ˛

c = cos q s = sin q

ply n∞k

Consider then the state of stresses:

s ox ≤ = 0 s oy ≤ = 1 ( MPa ) ≤ = 0 t oxy Following the same procedure, one can calculate s ¢¢ , s ¢¢t , and t ¢¢t in the orthotropic axes of each ply for a global stress on the laminate that is reduced to s ¢¢oy = 1 MPa. © 2003 by CRC Press LLC

TX846_Frame_C12 Page 243 Monday, November 18, 2002 12:27 PM

Finally consider the state of stresses: ¢¢¢ = 0 s ox ¢¢¢ = 0 s oy ¢¢¢ = 1 ( MPa ) t oxy Following the same procedure, one obtains s ¢¢ , s ¢¢t , and t ¢¢t in the orthotropic axes of each ply for a global stress applied on the laminate, and that is reduced ¢¢ = 1 MPa.10 to t oxy 11 It is then easy to determine by simple rule of proportion (or multiplication) the quantities (s h), (sth), and (tt h) in each ply, corresponding to loadings that are no longer unitary, but equal successively to N x = ( s ox h ) then: N y = ( s oy h ) then: T xy = ( t oxy h ) Subsequently, the principle of superposition allows one to determine (sh)total (sth)total and (tth)total when one applies simultaneously Nx, Ny, and Txy. From these it is possible to write the modified Hill–Tsai expression in the form of Equation 12.10, which will provide the thickness for the laminate needed to avoid the fracture of the ply under consideration. If hk is the laminate thickness obtained from the ply number k, after having gone over all the plies, one will retain for the final thickness h the thickness of highest value found as: h = sup {hk}

12

Remark: The principle of calculation is conserved when the plies have different thicknesses with any orientations. It then becomes indispensable to program the procedure, or to use existing computer programs. Then one can propose a complete composition for the laminate and verify that the solution is satisfactory regarding the criterion mentioned previously (deformation and fracture). This is 10

11

This calculation can be easily programmed on a computer: cf. Application 18.2.2 “Program for Calculation of a Laminate.” One will find in Appendix 1 at the end of the book the values s, st, tt obtained for the particular case of a carbon/epoxy laminate with ply orientations of 0∞, 90∞, +45∞, -45∞. These values are given in Plates 1 to 12. For example, one has the following:

s ox ¢ = 1 MPa Æ s ¢ , s t¢, t t¢ s ox ( MPa ) then: 12

Æ s , s t , t t

s ox s s ox s ¢ -------- = ----- fi s = s ¢ ¥ -------, - ¥ Nx and h s = -----1 1 ¢ ¢ s ox s

This method to determine the thickness is illustrated by an example: See Application 18.1.6.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 244 Monday, November 18, 2002 12:27 PM

Figure 12.3 Bending of the Laminate

facilitated by using the user friendly aspect of the program, allowing rapid return of the solution.

12.1.4

Flexure Behavior

In the previous paragraph, we have limited discussion to loadings consisting of Nx, Ny, and Txy applying in the midplane of the laminate. We will now examine the cases that can cause deformation outside of the plane of the laminate. The laminate considered is—as before—supposed to have midplane symmetry.

12.1.4.1 Displacement Fields Hypothesis: Assume that a line perpendicular to the midplane of laminate before deformation (see Figure 12.3) remains perpendicular to the midplane surface after deformation. Consequence: If one denotes as before uo and vo the components of the displacement in the midplane and wo as the displacement out of the plane (see Figure 12.3), the displacement of any point at a position z in the laminate (in the nondeformed configuration) can be written as

∂ w0 Ï u = u o – z -------Ô ∂x Ô w0 Ì v = v – z ∂-------o Ô ∂y Ô Ów = w o

(12.11)

One can then deduce the nonzero strains: 2 Ï ∂ w0 Ô e x = e ox – z ----------2 Ô ∂x Ô 2 Ô ∂ w0 Ì e y = e oy – z ----------2 Ô ∂y Ô 2 Ô ∂ w0 Ô g xy = g oxy – z ¥ 2 ------------∂x∂y Ó

© 2003 by CRC Press LLC

(12.12)

TX846_Frame_C12 Page 245 Monday, November 18, 2002 12:27 PM

Figure 12.4 Moment Resultants

12.1.4.2 Loadings In addition to the membrane stress resultants Nx, Ny, Txy in the previous paragraphs, one can add the moment resultants along the x and y directions (see Figure 12.4). As in the case of the membrane stress resultants, the moment resultants serve to synthesize the cohesive forces that appear by sectioning, following classical method that is common for all structures (beams, plates, etc.). One can interpret 13 these as the unit moments of the cohesive forces. They are written as: My: Moment resultant along the y axis, due to the stresses sx, over a unit width along the y direction. My =

Ú

h/2 – h /2

s x z dz

(12.13)

Mx: Moment resultant along the x direction, due to the stress sy, over a unit width along the x direction. Mx = –

Ú

h/2 – h /2

s y z dz

(12.14)

Mxy: (or –Myx): Twisting moment along the x axis (or y axis), due to the shear stress txy over a unit width along the y direction (or x direction): M xy = – 13

Ú

h/2 – h /2

t xy z dz

(12.15)

The expression of My can be written in integral form as:

Ú–h /2 sx z dz

My =

Ú–h /2 zz Ÿ sx xdz

Mx =

Ú–h /2 zz Ÿ sy ydz

. x = – Ú–h /2 s y z dz

M xy =

Ú–h /2 zz Ÿ txy ydz

. x = – Ú–h /2 t xy z dz

h/2

.y =

h/2

also: h/2

h/2

Finally:

© 2003 by CRC Press LLC

h/2

h/2

TX846_Frame_C12 Page 246 Monday, November 18, 2002 12:27 PM

Taking Equation 11.8 into consideration, which allows one to express, in a certain coordinate system, the stresses in a ply as functions of strains, the moment resultant My (Equation 12.13) can be written as: th

n ply

Ï

Â ÌÓ Ú

My =

zk z k-1

st

k=1 ply

¸ ( E 11k e x + E 12k e y + E 13k g xy )z dz ˝ ˛

which, when using Equation 12.12 becomes th

n ply

My =

Ï Ì Ó

Ï kÊ ∂ w oˆ º 2 ∂ w oˆ - + E 12k Ê z e oy – z 2 ----------E z e ox – z ----------z k-1 Ì 11 Ë 2 ¯ 2 Ë ∂x ∂y ¯ Ó 2

Â Ú st

k=1 ply

zk

2

¸ ∂ w oˆ ¸ º + E 13k Ê z g oxy – z 2 2 -----------dz ˝ Ë ∂ x ∂ y¯ ˝˛ ˛ 2

Due to midplane symmetry, every integral of the form:

Ú

zk z k-1

E lj z dz

in the above expression is accompanied by an integral of the form:

Ú

– z k-1 –zk

E lj z dz

that is opposite in sign. Integrals of this type disappear and there remains th

n ply

My =

Â st

k=1 ply

Ï k ( z k – z k-1 ) ∂ w o k ( z k – z k-1 ) ∂ w o … ------------------------- ----------------------------------- ----------- + E 12 – Ì E 11 2 2 3 3 ∂x ∂y Ó 3

3

3

2

3

2

k ( z k – z k-1 ) ∂ w o ¸ … + E 13 ------------------------- 2 ------------- ˝ 3 ∂x∂y ˛ 3

3

which can be written as: 2 2 ∂ w ∂ wo ∂ wo – M y = -C 11 ----------C ----------- – C 13 2 ------------o12 2 2 ∂ x∂y ∂x ∂y 2

with th

n ply

C 1j =

Â st

k=1 ply

© 2003 by CRC Press LLC

( z k – z k-1 ) E 1jk -----------------------3 3

3

2

TX846_Frame_C12 Page 247 Monday, November 18, 2002 12:27 PM

Proceeding in an analogous manner with Mx and Mxy (Equations 12.14 and 12.15), one obtains the following matrix form: Ï ∂ w ¸ C 13 Ô – ------------2o- Ô ∂x Ô Ô Ô ∂ 2w Ô C 23 Ì – -------------o- ˝ Ô ∂ y2 Ô Ô Ô C 33 Ô ∂ 2 wo Ô Ó – 2 -----------∂x∂y ˛ 2

C 11 Ï My ¸ Ô Ô Ô Ô Ì – M x ˝ = C 21 Ô Ô Ô Ô C 31 Ó – M xy ˛

C 12 C 22 C 32

(12.16)

with : th

n ply

C ij =

Â st

( z k – z k-1 ) E ijk -----------------------3 3

3

k=1 ply

Remarks: One can observe that in Equation 12.16 the coefficients Cij depend on the stacking sequence of the plies. Does a laminated plate bend under membrane loadings? Using the displacement field due to flexure to express, for example, the stress resultant Nx (Equation 12.11), one has th

n ply

Nx =

Ï Ì Ó

Ï kÊ ∂ w oˆ ∂ w oˆ … k Ê - + E 12 E e – z ----------e oy – z ----------z k – 1 Ì 11 Ë ox 2 ¯ 2 Ë ∂x ∂y ¯ Ó 2

Â Ú st

k=1 ply

zk

2

¸ ∂ w ¸ k Ê … + E 13 g – z ¥ 2 ------------o-ˆ¯ ˝ dz ˝ Ë oxy ∂x∂y ˛ ˛ 2

Making use of the remark mentioned above, the midplane symmetry causes the disappearance of integrals of the type:

Ú

zk z k-1

E ljk z dz

As a consequence, one finds again the Equation 12.4 as: N 1 = A 11 e ox + A 12 e oy + A 13 g oxy As a result of the midplane symmetry, the membrane behavior is independent of the flexural behavior. Even in the case of balanced laminate (as many plies oriented at angle q as the number of plies oriented at an angle -q), terms C13 and C23 in Equation 12.16 are not zero. This modifies the deformed bending configuration compared with the isotropic case (see Figure 12.5). © 2003 by CRC Press LLC

TX846_Frame_C12 Page 248 Monday, November 18, 2002 12:27 PM

Figure 12.5 Bending Configurations of a Plate

The terms C13 and C23 disappear only in the following cases: The plies are oriented uniquely in the 0∞ and 90∞. Then the product 14 cosq ¥ sinq is zero and : k k E 13 = E 23 = 0

"k

The laminate [0/90/45/-45] is constituted mainly with balanced fabric layers (in each fabric layer, the fibers along the warp and fill directions 15 are, by first approximation at the same z location), or mats layers. The stresses in the different plies are obtained from the Equations 11.8. For example, in the ply number k, one has: k k k s x = E 11 e x + E 12 e y + E 13 g xy

and taking into consideration Equations 12.12 for the strains: k k k k ∂ wo º ----------s x = [ E 11 e ox + E 12 e oy + E 13 g oxy ] – z E 11 2 ∂x 2

∂ w k ∂ wo k º + E 12 ----------- + E 13 ¥ 2 ------------o2 ∂ x∂y ∂y 2

2

one can resume by:

s x = s xmembrane + s xflexure Along the thickness of the laminate, the stress sx can be considered as the sum of two parts: a constant part and a linearly varying part, as seen in Figure 12.6. One can also observe analogous forms for the stresses sy and txy .

14 15

See Equations 11.8 See Section 5.2.3.5, Particular Cases of Balanced Fabrics.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 249 Monday, November 18, 2002 12:27 PM

Figure 12.6 Total Normal Stress in a Laminate

12.1.5 Consequence: Practical Determination for a Laminate Subject to Flexure Given: The moment resultants are known. Using these resultants, one is led to estimate proportions of plies along 16 the four orientations (or more, eventually) and to predict the stacking sequence. Principle for the calculation: Nonrupture of laminate: Following a procedure analogous to that described in Section 12.1.3, it is possible to calculate the stresses s, st, tt along the orthotropic axes of each of the plies. This allows the control of their integrity using the Hill–Tsai failure criterion. This requires the use of a computer program which can allow the adjustment of the composition of the laminate. Flexure deformation: The determination of the deformed configuration of the laminate under flexure poses the same problem as with the isotropic plates: outside of a few cases of academic interest, it is necessary to use 17 a computer program based on the finite element method.

12.1.6 Simplified Calculation for Flexure It is possible, for a first estimate, to perform simplified calculations by considering that 2 ∂ wo ----------the moment M is related uniquely to the curvature and the moment Mx to the y 2 2 ∂x wo curvature ∂-----------. One then can determine experimentally: 2 ∂y

1. The apparent failure stresses in flexure An experiment on a sample can provide the value for the moment at failure, denoted by Mrupture on Figure 12.7 (per unit width of the sample). Analogy with 16 17

See Section 5.2. These elements are constituted on the basis presented above and can include the effects which were not taken into account previously: in particular, the transverse shear stresses in flexure due to the transverse shear stress resultants (consult this subject in Chapter 17).

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 250 Monday, November 18, 2002 12:27 PM

Figure 12.7 Bending Failure

Figure 12.8 Homogeneous and Laminated Beams

the flexure of beams leads to: M rupture ¥ h/2 6 then: s rupture = M rupture ¥ -----2 s rupture = ------------------------------3 h /12 h 2. Apparent flexure moduli These are obtained starting from the comparison of relations between the “composite” and “homogeneous.” One recalls on Figure 12.8(a) the relation between the moment and curvature for a homogeneous beam with unit width, obtained 18 by integration of the local behavior : 3 s M h ¥ 1 d wo - = – ------f e x = -----x Æ -------------- ¥ ----------2 E 12 E dx 2

If one notes that Equation 12.16, recalled as: Ï My ¸ Ï –∂ wo / ∂ x ¸ Ô Ô Ô Ô 2 2 Ì –Mx ˝ = [ C ] Ì –∂ wo / ∂ y ˝ Ô Ô Ô Ô Ó – M xy ˛ Ó – 2 ¥ ∂ 2 w / ∂ x dy ˛ 2

2

o

18

∂u

dw o

2

d wo

sx

- = – z ----- which can be integrated into Recall that e x = ------ with u = –z ---------- ; then z ----------2 ∂x dx E dx the thickness.

© 2003 by CRC Press LLC

2

TX846_Frame_C12 Page 251 Monday, November 18, 2002 12:27 PM

can be inverted, and noting:

[C]

-1

1/EI 11

1/EI 12

1/EI 13

= 1/EI 21

1/EI 22

1/EI 23

1/EI 31

1/EI 32

1/EI 33

one obtains:

∂ wo –1 1 1 ----------- = --------- ¥ M y + --------- ¥ M x + --------- ¥ M xy 2 ∂x EI 11 EI 12 EI 13 2

The identification of the behavior noted in Figure 12.8(a), on the one hand, with only the first term of the moment My in the equation in Figure 12.8(b), on the other hand, that is: h ¥1 EI 11 ∫ E -------------12 3

leads to an approximate equation of an equivalent modulus E that one can interpret as the flexure modulus along the x direction of the homogeneous material: 12 E flexure = -----3- ¥ EI 11 h ( along x ) Note: When the plies of the laminate are oriented uniquely along the 0∞ and 90∞ directions, or when the laminate [0/90/45/–45] is constituted uniquely of balanced fabrics and of mats, excluding the unidirectional layers, then one has in the matrix [C]: C 13 = C 23 = 0 then: 2

EI 11

C 12 = C 11 – ------C 22

12.1.7 Case of Thermomechanical Loading 12.1.7.1 Membrane Behavior When one considers variation in temperature, which is assumed to be identical in all plies of the laminate, the stresses are given by the modified Equations 11.10. Following the procedure of Section 12.2, with the same hypotheses and notations, the stress resultant Nx (Equation 12.1) becomes th

th

n ply

Nx =

Â st

k=1 ply

n ply

{E

k 11

e ox + E

k 12

e oy + E

k 13

g oxy }e k – DT

Â st

k=1 ply

then: N x = A 11 e ox + A 12 e oy + A 13 g oxy – DT · a EhÒ x © 2003 by CRC Press LLC

a E1 ¥ ek k

TX846_Frame_C12 Page 252 Monday, November 18, 2002 12:27 PM

with: th

th

n ply

A 1j =

Â

n ply

E

k 1j

e k ; · a EhÒ x =

st

Â

a E1 ek k

st

k=1 ply

k=1 ply

Following the same procedure for Ny and Txy, the stress resultants are expressed as: Ï Nx ¸ A 11 A 12 A 13 Ô Ô N = Ì y˝ A 21 A 22 A 23 Ô Ô A 31 A 32 A 33 Ó T xy ˛

Ï e ox ¸ Ï · a EhÒ x ¸ Ô Ô Ô Ô Ì e oy ˝ – DT Ì · a EhÒ y ˝ Ô Ô Ô Ô Ó g oxy ˛ Ó · a EhÒ xy ˛

with : th

n ply

A ij =

Â

E ijk ¥ e k = A ji

cf. [ 11.8 ]

st

k=1 ply

¸ Ô · a EhÒ x = a E ¥ ek Ô Ô st k=1 ply Ô th Ô n ply Ô k · a EhÒ y = a E2 ¥ ek ˝ Ô st k=1 ply Ô th Ô n ply Ô k · a EhÒ xy = a E3 ¥ ek Ô Ô st k=1 ply ˛ th

(12.17)

n ply

Â

k 1

Â

cf. [ 11.10 ]

Â

Inversion of the above relation allows one to show the apparent moduli of the laminate (see Paragraph 12.1.2) and thermal membrane strains: Ï e ox ¸ Ï s ox ¸ Ï · a EhÒ x ¸ Ô Ô Ô Ô –1 Ô –1 Ô Ì e oy ˝ = h [ A ] Ì s oy ˝ + DT [ A ] Ì · a EhÒ y ˝ Ô Ô Ô Ô Ô Ô Ó g oxy ˛ Ó t oxy ˛ Ó · a EhÒ xy ˛ or with Equation 12.9: Ï e ox ¸ Ô Ô Ô Ô Ì e oy ˝ = Ô Ô Ô Ô Ó g oxy ˛ © 2003 by CRC Press LLC

1 ----Ex

yx –n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï s ox ¸ Ï · a EhÒ x ¸ Ô Ô Ô Ô Ô Ô Ô –1 Ô Ì s oy ˝ + DT [ A ] Ì · a EhÒ y ˝ Ô Ô Ô Ô Ô Ô Ô Ô Ó t oxy ˛ Ó · a EhÒ xy ˛

TX846_Frame_C12 Page 253 Monday, November 18, 2002 12:27 PM

which can be rewritten as: Ï e ox ¸ Ï s ox ¸ Ï --1- · a EhÒ ¸ x Ô Ô Ô Ô Ô Ôh Ô Ô Ô Ô –1 Ô –1 Ô 1 Ì e oy ˝ = h [ A ] Ì s oy ˝ + DT ¥ h [ A ] Ì --h- · a EhÒ y ˝ Ô Ô Ô Ô Ô Ô Ô Ô Ô Ô Ô --1- · a EhÒ Ô xy ˛ Ó g oxy ˛ Ó t oxy ˛ Óh

Remarks: Evaluation of terms (1/h)·aEhÒx, (1/h)·aEhÒy, and (1/h)·aEhÒxy only requires the knowledge of the proportions of plies along the different orientations 19 and not their thicknesses. -1 The matrix h[A] , already mentioned in Section 12.1.2, contains the global moduli of the laminate. One can then write (see Equation 12.9): Ï e ox ¸ Ô Ô Ô Ô Ì e oy ˝ = Ô Ô Ô Ô Ó g oxy ˛

1 ----Ex

yx –n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï s ox ¸ Ô Ô Ô Ô Ì s oy ˝ + DT Ô Ô Ô Ô Ó t oxy ˛

1 ----Ex

yx n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï --1- · a EhÒ ¸ x Ô Ôh Ô1 Ô Ì --h- · a EhÒ y ˝ Ô Ô Ô --1- · a EhÒ Ô xy ˛ Óh

The last term of the above equation allows one to show the global expansion coefficients of the laminate, which are denoted as aox, aoy, and aoxy, as below: Ï a ox ¸ Ô Ô Ô Ô Ì a oy ˝ = Ô Ô Ô Ô Ó a oxy ˛

1 ----Ex

yx –n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï --1- · a EhÒ ¸ x Ô Ôh Ô1 Ô Ì --h- · a EhÒ y ˝ Ô Ô Ô --1- · a EhÒ Ô xy ˛ Óh

(12.18)

In summary, the membrane thermomechanical behavior of a laminate with midplane symmetry can be written as: Ï e ox ¸ Ô Ô Ô Ô Ì e oy ˝ = Ô Ô Ô Ô Ó g oxy ˛

19

1 ----Ex

yx –n------Ey

h xy -------G xy

xy –n------Ex

1 ----Ey

m xy -------G xy

hx -----Ex

my ----Ey

1 -------G xy

Ï s ox ¸ Ô Ô Ô Ô Ì s oy ˝ + DT Ô Ô Ô Ô Ó t oxy ˛

Ï a ox ¸ Ô Ô Ô Ô Ì a oy ˝ Ô Ô Ô Ô Ó a oxy ˛

See Application18.2 “Residual Thermal Stresses due to Curing of the Laminate.”

© 2003 by CRC Press LLC

(12.19)

TX846_Frame_C12 Page 254 Monday, November 18, 2002 12:27 PM

This is an equation in which aox, aoy, and aoxy are given by Equations 12.17 and 20 12.18.

12.1.7.2 Flexure Behavior Following the procedure in Section 12.14 with the same notations, the moment resultant My (Equation 12.13) becomes, using the modified Equations 11.10: th

n ply

My =

Ï

Â ÌÓ Ú

zk zk – 1

st

k=1 ply

¸ k k ( E 11 e x + E 12 e y + E 13 g xy )z dz ˝ ˛ th

n ply

– DT

Â ÊË Ú

zk zk – 1

st

k a E 1 ¥ z dzˆ¯

k=1 ply

The plate is assumed to have midplane symmetry, then each integral of the form – z k-1 Úzk-1 a E1 z dz is associated with another integral such that Ú–zk a E1 z dz is equal and opposite in sign. There remains the following expression, with the notations of Section 12.1.4: zk

∂ w0 ∂ w0 ∂ w - – C 12 ----------- – C 13 ¥ 2 ------------0M y = – C 11 ----------2 2 ∂ x∂y ∂x ∂y 2

2

2

Due to the midplane symmetry, the behavior in flexure 12.16 is not modified when the laminate is subjected to thermomechanical loading.

Remark: In the preceding discussion, it is assumed that the temperature field is uniform across the thickness of the laminate.

12.2 LAMINATE WITHOUT MIDPLANE SYMMETRY 12.2.1 Coupled Membrane–Flexure Behavior If one considers again the calculations of Section 12.1.4 without midplane symmetry, one can see the presence of new integrals as: 2

zk

2

k k z k – z k-1ˆ E ij z dz = E ij Ê ------------------Ë 2 ¯ z k-1

Ú

for the ply k. When the summation over all plies is taken, these integrals lead to nonzero terms with the form: th

n ply

B ij =

Â st

2

2

k z k – z k-1ˆ E ij Ê ------------------Ë 2 ¯

k=1 ply 20

One indicates in Tables 5.4, 5.9, and 5.14 of Section 5.4 the values of expansion coefficients of the laminates made of carbon, Kevlar, and glass/epoxy with Vf = 60% fiber volume fraction.

© 2003 by CRC Press LLC

TX846_Frame_C12 Page 255 Monday, November 18, 2002 12:27 PM

Then one has for the development of My (see Section 12.1.4):

∂ w0 ∂ w0 ∂ w - – C 12 ----------- – C 13 ¥ 2 ------------0- + B 11 e ox + B 12 e oy + B 13 g oxy M y = – C 11 ----------2 2 ∂ x∂y ∂x ∂y 2

2

2

In this expression appears the coupling between bending and membrane behavior. In a similar manner, the stress resultant Nx which was developed in Section 12.1.4 is rewritten as: 2 ∂ w0 ∂ w ∂ w0 - – B 13 ¥ 2 ------------0- – B 12 ----------N x = A 11 e ox + A 12 e oy + A 13 g oxy – B 11 ----------2 2 ∂ x∂y ∂y ∂x 2

2

where one can find the coupling as mentioned previously. Developing along the same manner the resultants Mx, Mxy, Ny, and Txy, one can regroup the obtained relations. Therefore, the global relation for the behavior can be written as: Ï Nx ¸ Ô Ô Ô Ny Ô Ô Ô Ô T xy Ô Ì ˝ = Ô My Ô Ô –M Ô x Ô Ô Ô –M Ô Ó xy ˛

A

B

B

C

e ox Ï ¸ Ô Ô e oy Ô Ô Ô Ô g oxy Ô Ô Ì –∂ 2 w / ∂ x2 ˝ 0 Ô Ô Ô 2 2 Ô Ô –∂ w0 / ∂ y Ô Ô Ô 2 Ó –2 ∂ w0 / ∂ x ∂ y ˛

(12.20)

with : th

th

n ply

n ply

Â

A ij =

E e k ; B ij =

st

st

k=1 ply

2

2

k z k – z k-1ˆ E ij Ê ------------------Ë 2 ¯

k=1 ply

th

n ply

C ij =

Â

k ij

Â st

3

3

k z k – z k-1ˆ E ij Ê ------------------Ë 3 ¯

k=1 ply

12.2.2 Case of Thermomechanical Loading Using the expression developed for moment resultant My as shown in Section 12.1.7.2, one can find the following form of integrals for each ply k: zk

2

2

z k – z k-1ˆ a E ¥ z dz = a E ÊË ------------------2 ¯ z k-1

Ú

k 1

k 1

after summing over all plies of the laminate, it appears a nonzero term of the form: th

n ply

· a Eh Ò x = 2

Â st

k=1 ply

© 2003 by CRC Press LLC

2

2

k z k – z k-1ˆ a E 1 ÊË ------------------2 ¯

TX846_Frame_C12 Page 256 Monday, November 18, 2002 12:27 PM

A similar development for other resultants lead to the following relation for thermomechanical behavior: Ï Nx ¸ Ô Ô Ô Ny Ô Ô Ô Ô T xy Ô Ì ˝ = Ô My Ô Ô –M Ô x Ô Ô Ô –M Ô Ó xy ˛

A

B

B

C

A ij =

with:

Â

e ox Ï · a EhÒ x ¸ Ï ¸ Ô Ô Ô Ô e oy Ô · a EhÒ y Ô Ô Ô Ô Ô Ô Ô g oxy Ô · a EhÒ xy Ô Ô Ô ˝ Ì – ∂ 2 w / ∂ x 2 ˝ – DT Ì 2 0 Ô · a Eh Ò x Ô Ô Ô Ô Ô Ô 2 2 Ô 2 Ô · a Eh Ò y Ô Ô –∂ w0 / ∂ y Ô Ô Ô Ô Ô 2 2 Ó · a Eh Ò xy ˛ Ó –2 ∂ w0 / ∂ x ∂ y ˛ k

E ij e k ;

B ij =

k

Â k

C ij =

2

2

k z k – z k-1ˆ E ij Ê ------------------Ë 2 ¯ 3 k

(12.21)

3 k-1

-ˆ Â E ÊË ------------------3 ¯ k ij

z –z

k

· a EhÒ x =

Â aE

k 1

ek ;

· a EhÒ y =

k

· a Eh Ò x = 2

Â k

Â aE

k 2

ek ;

· a EhÒ xy =

k

k ( z k – z k-1 ) -; a E 1 -----------------------2 2

k 3

k

2

· a Eh Ò y = 2

Â k

· a Eh Ò xy = 2

k ( z k – z k-1 ) -; a E 2 -----------------------2

Â k

© 2003 by CRC Press LLC

Â aE

2

2

k ( z k – z k-1 ) a E 3 -----------------------2 2

2

ek

TX846_Frame_C13 Page 257 Monday, November 18, 2002 12:29 PM

PART III JUSTIFICATIONS, COMPOSITE BEAMS, AND THICK PLATES We regroup in Part III elements that are less utilized than those in the previous parts. Nevertheless they are of fundamental interest for a better understanding of the principles for calculation of composite components. In the first two chapters, we focused on anisotropic properties and fracture strength of orthotropic materials, and then more particularly on transversely isotropic ones. The following two chapters allow us to consider that composite components in the form of beams can be “homogenized.” This means that their study is analogous to the study of homogeneous beams that are common in the literature. Finally, the last chapter in this part describes with a similar procedure the behavior of thick composite plates subject to transverse loadings.

© 2003 by CRC Press LLC

TX846_Frame_C13 Page 259 Monday, November 18, 2002 12:29 PM

13 ELASTIC COEFFICIENTS The definition of a linear elastic anisotropic medium was given in Chapter 9. We have also given, without justification, the behavior relations characterizing the particular case of orthotropic materials. Now we propose to examine more closely the elastic constants which appear in stress–strain relations for these materials. In the case of transversely isotropic materials, we will study also the manner in which the constants evolve.

13.1 ELASTIC COEFFICIENTS IN AN ORTHOTROPIC MATERIAL Recall: Consider the relation for elastic behavior written in Paragraph 9.1.1 in the form:

e mn = j mnpq ¥ s pq Recall that the components jmnpq of a tensor expressed in the coordinate system 1,2,3 are written as FIJKL in a coordinate system I,II,II using the relation: F IJKL = cos I cos J cos K cos L j mnpq m

n

p

q

(13.1)

in which: cos I = cos ( m, I ) m

1

By definition, for mechanical behavior, an orthotropic medium has at any point two orthogonal planes of symmetry. Consider here two coordinate systems 1,2,3 and I,II,III, constructed on these planes and their intersection. One plane can be obtained from the other by a 180∞ rotation about the 3 axis as shown in Figure 13.1. One can deduce

[ cos I ] = m

1

See Section 9.2.

© 2003 by CRC Press LLC

–1 0 0 0 –1 0 0 0 1

TX846_Frame_C13 Page 260 Monday, November 18, 2002 12:29 PM

Figure 13.1 Orthotropic Medium

Application of Relation 13.1 above leads to = j 1 1 1 1 ; F I I II II

FI I I I

= j 1 1 2 2 ; F I I III III

= j1 1 3 3

F II II II II = j 2 2 2 2 ; F II II III III = j 2 2 3 3 ; F III III III III = j 3 3 3 3 F II III II III = j 2 3 2 3 ; F I III I III = j 1 3 1 3 ; F I II I II

= j1 2 1 2

and: F I I II III = – j 1 1 2 3 ; However, because the mechanical properties in the coordinates 1,2,3 and I,II,III are identical, one has F I I II III = j 1 1 2 3 from this: F I I II III = j 1 1 2 3 = – j 1 1 2 3 = 0 In an analogous manner:

j II II II III = 0; F III III II III = 0 F I I I III = 0; F II II I III = 0; F III III I III = 0 F II III I II = 0; F I III I II = 0 finally: F I I I II

= j 1 1 1 2 ; F II II I II = j 2 2 1 2 ; F III III I II = j 3 3 12

F II III I III = j 2 3 1 3 © 2003 by CRC Press LLC

TX846_Frame_C13 Page 261 Monday, November 18, 2002 12:29 PM

Until now, we have taken into account the symmetry with respect to plane 1,3. Consider now the coordinates 1,2,3 and I’, II’, III’ (see Figure 13.1), which can be obtained from each other by a 180∞ rotation about the 2 axis (symmetry with respect to plane 1,2). One has [ cos I ] = m

–1 0 0

0 0 1 0 0 –1

The same procedure as above will lead to F I¢I¢I¢II¢

= – j 1 1 1 2 = j 1 1 1 2 = 0; F II¢II¢I¢II¢ = – j 2 2 1 2 = j 2 2 1 2 = 0

F III¢III¢I¢II¢ = – j 3 3 1 2 = j 3 3 1 2 = 0; F II¢III¢I¢III¢ = – j 2 3 1 3 = j 2 3 1 3 = 0 Considering the symmetry of the coefficients jmnpq indicated in Relation 9.1, we have written here the only nonzero terms. For the mechanical behavior, one obtains by simplification of Equation 9.2:

2

Ï e 11 ¸ j1 1 1 1 j1 1 2 2 j1 1 3 3 0 0 0 Ô Ô Ô e 22 Ô j2 2 1 1 j2 2 2 2 j2 2 3 3 0 0 0 Ô Ô Ô e 33 Ô j3 3 1 1 j3 3 2 2 j3 3 3 3 0 0 0 Ì ˝ = g 0 0 0 0 0 4 j2 3 2 3 Ô 23 Ô Ôg Ô 0 0 0 0 0 4 j1 3 1 3 Ô 13 Ô Ôg Ô j 0 0 0 0 0 4 1 2 12 Ó 12 ˛

Ï s 11 ¸ Ô Ô Ô s 22 Ô Ô Ô Ô s 33 Ô Ì ˝ Ô t 23 Ô Ôt Ô Ô 13 Ô Ôt Ô Ó 12 ˛

(13.2)

There remain then only nine distinct elastic coefficients, which can be written in the form of Young’s moduli and Poisson ratios as: Ïe ¸ Ô 11 Ô Ô Ô Ô e 22 Ô Ô Ô Ô Ô Ô e 33 Ô Ì ˝ = Ôg Ô Ô 23 Ô Ô Ô Ô g 13 Ô Ô Ô Ôg Ô Ó 12 ˛

2

1 – n 21 – n 31 ----- --------- ---------E3 E1 E2 – n 12 1 ---------- ----E1 E2

– n 32 ---------E3

– n 13 – n 23 ---------- ---------E1 E2

1 ----E3

0

0

0

0

0

0

0

0

0

0 0 0 ÏÔ s 11 ¸Ô Ô Ô 0 0 0 Ô s 22 Ô Ô Ô Ô Ô 0 0 0 Ô s 33 Ô Ì ˝ 1 -------- 0 0 Ô t 23 Ô G 23 Ô Ô Ô Ô 1 - 0 Ô t 13 Ô 0 ------G 13 Ô Ô 1 Ô - t 12 Ô 0 0 ------˛ G Ó 12

Recall the symmetry relations: jijkl = jijlk; jijkl = jjikl; jijkl = jklij.

© 2003 by CRC Press LLC

(13.3)

TX846_Frame_C13 Page 262 Monday, November 18, 2002 12:29 PM

Figure 13.2 Transversely Isotropic Material

13.2 ELASTIC COEFFICIENTS FOR A TRANSVERSELY ISOTROPIC MATERIAL 3

Recall: By definition, a transversely isotropic material (Figure 13.2) is such that any plane including a preferred axis is a plane of mechanical symmetry. We have already noted that this is a particular case of orthotropic materials. Therefore, the 4 only nonzero elastic constants are shown in Figure 13.2. The preferred direction is axis 1 in Figure 13.2. Considering that the coordinates 1,2,3 and I,II,III can be obtained from each other by a rotation of q. One then has 1 0 0 m [ cos I ] = 0 c – s with c = cos q s = sin q 0 s c From the definition of material, the matrix of elastic coefficients has to remain invariant in this rotation. The Relation 13.1 allows one to write • FI I I I = j1 1 1 1 • F I I II II = j 1 1 2 2 c + j 1 1 3 3 s = j 1 1 2 2 2

3 4

2

See Section 9.3. Using the symmetries in Equation 9.1 and also using the discussion of the previous paragraph.

© 2003 by CRC Press LLC

TX846_Frame_C13 Page 263 Monday, November 18, 2002 12:29 PM

then:

j1 1 2 2 ( c – 1 ) + j1 1 3 3 s = 0 2

2

j1 1 2 2 = j1 1 3 3 4 2 2 2 2 2 2 • F II II II II = j 2 2 2 2 c + j 2 2 3 3 s c + j 2 3 2 3 s c + j 2 3 3 2 s c º

º + j3 2 2 3 s2 c2 + j3 2 3 2 s2 c2 + j3 3 2 2 s2 c2 + j3 3 3 3 s4 and: F II II II II = j 2 2 2 2 Then, taking into account the symmetries, we obtain the relation:

j 2 2 2 2 ( c – 1 ) + j 3 3 3 3 s + 2s c ( j 2 2 3 3 + 2 j 2 3 2 3 ) = 0 4

4

2 2

(a)

4 2 2 2 2 2 2 • F III III III III = j 2 2 2 2 s + j 2 2 3 3 s c + j 2 3 2 3 s c + j 2 3 3 2 s c º

º + j3 2 3 2 s2 c2 + j3 2 3 2 s2 c2 + j3 3 2 2 s2 c2 + j3 3 3 3 s4 and: F III III III III = j 3 3 3 3 then taking in account symmetry, we have:

j 2 2 2 2 s + j 3 3 3 3 ( c – 1 ) + 2s c ( j 2 2 3 3 + 2 j 2 3 2 3 ) = 0 4

4

2 2

(b)

Examining member by member the difference of relations shown in (a) and (b) above, one obtains:

j2 2 2 2 = j3 3 3 3 Replacing in (a):

j 2 2 2 2 ( c + s – 1 ) + 2s c ( j 2 2 3 3 + 2 j 2 3 2 3 ) = 0 4

4

2 2

– 2 s c j 2 2 2 2 + 2s c ( j 2 2 3 3 + 2 j 2 3 2 3 ) = 0 2 2

2 2

2 j2 3 2 3 = j2 2 2 2 – j2 2 3 3 • F I III I III = j 1 2 1 2 s + j 1 3 1 3 c = j 1 3 1 3 2

© 2003 by CRC Press LLC

2

TX846_Frame_C13 Page 264 Monday, November 18, 2002 12:29 PM

then

j1 2 1 2 s + j1 3 1 3 ( c – 1 ) = 0 2

2

j1 2 1 2 = j1 3 1 3 We have written four relations for the nine coefficients; there remain five distinct elastic coefficients. Equation 13.2 is reduced to Ï e 11 ¸ j1 1 1 1 j1 1 2 2 j1 1 2 2 0 0 0 Ô Ô Ô e 22 Ô j2 2 1 1 j2 2 2 2 j2 2 3 3 0 0 0 Ô Ô e Ô 33 Ô j2 2 1 1 j3 3 2 2 j2 2 2 2 0 0 0 Ì ˝ = 0 0 0 0 0 2 ( j2 2 2 2 – j2 2 3 3 ) Ô g 23 Ô Ôg Ô 0 0 0 0 0 4 j1 2 1 2 Ô 13 Ô Ôg Ô 0 0 0 0 0 4 j1 2 1 2 Ó 12 ˛

Ï s 11 ¸ Ô Ô Ô s 22 Ô Ô Ô Ô s 33 Ô Ì ˝ (13.4) Ô t 23 Ô Ôt Ô Ô 13 Ô Ôt Ô Ó 12 ˛

or in the form of Young’s moduli and Poisson ratios: Ï e 11 ¸ Ô Ô Ô Ô Ô e 22 Ô Ô Ô Ôe Ô Ô 33 Ô Ì ˝ = Ô g 23 Ô Ô Ô Ô Ô Ô g 13 Ô Ô Ô Ôg Ô Ó 12 ˛

13.2.1

1 ----E1

– n 21 ---------E2

– n 21 ---------E2

0

0

– n 12 ---------E1

1 ----E2

–n -----E2

0

0

– n 12 ---------E1

–n -----E2

1 ----E2

0

0 0

0

0

0

2(1 + n) -------------------E2

0

0

0

0

1 -------G 12

0

0

0

0

0

0 ÏÔ s 11 ¸Ô Ô Ô 0 Ô s 22 Ô Ô Ô Ô Ô 0 Ô s 33 Ô Ì ˝ 0 Ô t 23 Ô Ô Ô Ô Ô 0 Ô t 13 Ô Ô Ô 1 -------- Ô t 12 Ô ˛ G Ó

(13.5)

12

Rotation about an Orthotropic Transverse Axis

13.2.1.1 Problem How can one transform the elastic coefficients of the previous constitutive equation 5 when writing them in coordinate axes x,y,z other than the orthotropic axes ,t,z ? The coordinate axes x,y,z are obtained from the orthotropic axes by a rotation q about the z axis, as shown in Figure 13.3. Recall Relation 13.1, which allows the calculation of components FIJKL in the coordinate axes x,y,z as functions of the components jmnpq in the coordinate axes ,t,z to be: F IJKL = cos I cos J cos K cos L ¥ j mnpq m

( axes x, y, z ) 5

n

p

q

( axes , t, z )

The orthotropic axes 1,2,3 of Equation 13.5 are therefore denoted as ,t,z.

© 2003 by CRC Press LLC

TX846_Frame_C13 Page 265 Monday, November 18, 2002 12:29 PM

Figure 13.3 Rotation above an Orthotropic Transverse Axis

with (see Figure 13.3):

[cos I ] = m

cos ( , x ) cos ( t, x ) cos ( z, x )

cos ( , y ) cos ( t, y ) cos ( z, y )

c –s 0 cos ( , z ) = s c 0 cos ( t, z ) 0 0 1 cos ( z, z )

Noting that the only nonzero coefficients jmnpq are those that appear in Equation 13.4, one obtains: • FI I I I = c j1 1 1 1 + c s j1 1 2 2 + c s j1 2 1 2 + c s j1 2 2 1 º 4

2 2

2 2

2 2

º + c2 s2 j2 1 1 2 + c2 s2 j2 1 2 1 + c2 s2 j2 2 1 1 + s4 j2 2 2 2 • F I I I I = c j 1 1 1 1 + s j 2 2 2 2 + 2c s ( j 1 1 2 2 + 2 j 1 2 1 2 ) 4

4

2 2

Expressing this coefficient as a function of the “technical” constants which appear in Equation 13.5, one obtains: 4 4 n s c 2 2 1 F I I I I = ----- + ---- + s c Ê ------- – 2 -----t-ˆ Ë E Et Et ¯ G t

• F I I II II = c s j 1 1 1 1 + c j 1 1 2 2 – c s j 1 2 1 2 – c s j 1 2 2 1 º 2 2

4

2 2

2 2

º – s2 c2 j2 1 1 2 – s2 c2 j2 1 2 1 + s4 j2 2 1 1 + s2 c2 j2 2 2 2 • F I I II II = ( c + s ) j 1 1 2 2 + c s ( j 1 1 1 1 + j 2 2 2 2 – 4c s j 1 2 1 2 ) 4

4

2 2

2 2

or in the “technical” form:

n 1 1 4 4 2 2 1 F I I II II = – -----t- ( c + s ) + c s Ê ----- + ---- – -------ˆ Ë E E t G t¯ Et • F I I III III = c j 1 1 3 3 + s j 2 2 3 3 and as 2

2

j1 1 3 3 = j1 1 2 26

F I I III III = c j 1 1 2 2 + s j 2 2 3 3 2

6

2

Because this is a transversely isotropic material; see Equations 9.2 and 13.4.

© 2003 by CRC Press LLC

TX846_Frame_C13 Page 266 Monday, November 18, 2002 12:29 PM

or in the “technical” form: 2n 2n F I I III III = – Ê c -----t- + s ----ˆ Ë Et E t¯

• F I I II III = 0 • F I I I III = 0 • F I I I II = – c s j 1 1 1 1 + c s j 1 1 2 2 + c s j 1 2 1 2 – cs j 1 2 2 1 + sc j 2 1 1 2 º 3

3

3

3

3

… – s3 c j2 1 2 1 – s3 c j2 2 1 1 + s3 c j2 2 2 2 F I I I II = – sc { c j 1 1 1 1 – s j 2 2 2 2 – ( c – s ) ( j 1 1 2 2 + 2 j 1 2 1 2 ) } 2

2

2

2

or in the “technical” form: Ï c2 s2 n 1 ¸ 2 2 F I I I II = – cs Ì ----- – ---- + ( c – s ) Ê -----t- – -----------ˆ ˝ Ë E t 2G t¯ ˛ Ó E Et • F II II II II = s j 1 1 1 1 + s c j 1 1 2 2 + s c j 1 2 1 2 + s c j 1 2 2 1 º 4

2 2

2 2

2 2

º + s c j2 1 1 2 + s c j2 1 2 1 + s c j2 2 1 1 + c j2 2 2 2 2 2

2 2

2 2

4

F II II II II = s j 1 1 1 1 + c j 2 2 2 2 + s c ( 4 j 1 2 1 2 + 2 j 1 1 2 2 ) 4

4

2 2

or in “technical” form: 4 4 n c s 2 2 1 F II II II II = ----- + ---- + s c Ê ------- – 2 -----t-ˆ Ë G t E Et Et ¯

• F II II III III = s j 1 1 3 3 + c j 2 2 3 3 and as j 1 1 3 3 = j 1 1 2 2 7 2

2

F II II III III = s j 1 1 2 2 + c j 2 2 3 3 2

2

or in “technical” form: 2n 2n F II II III III = – Ê s -----t- + c ----ˆ Ë Et E t¯

• F II II II III = 0 • F II II I III = 0 • F II II I II = – s c j 1 1 1 1 + s c j 1 1 2 2 – sc j 1 2 1 2 + s c j 1 2 2 1 º 3

3

3

3

… ( – sc 3 j 2 1 1 2 + s 3 c j 2 1 2 1 – sc 3 j 2 2 1 1 + c 3 s j 2 2 2 2 ) F II II I II = – sc { s j 1 1 1 1 + c j 2 2 2 2 + ( c – s ) ( j 1 1 2 2 + 2 j 1 2 1 2 ) } 2

7

See Equations 9.2 and 13.4.

© 2003 by CRC Press LLC

2

2

2

TX846_Frame_C13 Page 267 Monday, November 18, 2002 12:29 PM

or in “technical” form: Ï s2 c2 n 1 ¸ 2 2 F II II I II = – cs Ì ----- – ---- – ( c – s ) Ê -----t- – -----------ˆ ˝ Ë ¯ E E E 2G t t t ˛ Ó • F III III III III = j 3 3 3 3 in “technical” form: 1 F III III III III = ---Et • F III III II III = 0 • F III III I III = 0 • F III III I II = – sc j 3 3 1 1 + sc j 3 3 2 2 and as j 3 3 1 1 = j 1 1 2 2 8 F III III I II = – sc j 1 1 2 2 + sc j 2 2 3 3 in “technical” form:

n – n tˆ F III III I II = – sc Ê --------------Ë Et ¯ • F II III II III = s j 1 3 1 3 + c j 2 3 2 3 2

2

8

we know that for a transversely isotropic material, one has:

j1 3 1 3 = j1 2 1 2

and

2 j2 3 2 3 = j2 2 2 2 – j2 2 3 3

then: 2 2 j2 2 2 2 – j2 2 3 3 ˆ F II III II III = s j 1 2 1 2 + c Ê ---------------------------------Ë ¯ 2

in “technical” form: c (1 + n) s F II III II III = ----------- + ---------------------4G t 2E t 2

2

• F II III I III = – sc j 1 3 13 + sc j 2 3 2 3 is still:

8

1 F II III I III = – sc Ê j 2 1 2 1 – --- ( j 2 2 22 – j 2 2 3 3 )ˆ Ë ¯ 2 8

See Equations 9.2 and 13.4.

© 2003 by CRC Press LLC

TX846_Frame_C13 Page 268 Monday, November 18, 2002 12:29 PM

or in “technical” form: 1 (1 + n) F II III I III = – sc Ê ----------- – -----------------ˆ Ë 4G t 2E t ¯ • F III II I II = 0 • F I III I III = c j 1 3 1 3 + s j 2 3 2 3 is still: 2

2

2 2 ( j2 2 2 2 – j2 2 3 3 ) F I III I III = c j 1 2 12 + s ------------------------------------2

or in “technical” form: c 2(1 + n) F I III I III = ----------- + s ----------------4G t 2E t 2

• F I III I II = 0 • F I II I II = s c j 1 1 1 1 – s c j 1 1 2 2 + c j 1 2 1 2 – s c j 1 2 2 1 º 2 2

2 2

4

2 2

º – s2 c2 j2 1 1 2 + s4 j2 1 2 1 – s2 c2 j2 2 1 1 + s2 c2 j2 2 2 2 2 2

F I II I II = s c ( j 1 1 1 1 + j 2 2 2 2 – 2 j 1 1 2 2 ) + ( c – s ) j 1 2 1 2 2 2

2

or in “technical” form:

n ¸ 1 2 2Ï 1 2 2 2 1 F I II I II = s c Ì ----- + ---- + 2 -----t- ˝ + ( c – s ) ----------Et ˛ 4G t Ó E Et All the nonzero coefficients F IJKL found above allow one to write the constitutive 9 relation in the form : Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

e xx e yy e zz g yz g xz g xy

¸ F I I II II F I I III III 0 0 2F I I I II FI I I I Ô Ô F II II I I F II II II II F II II III III 0 0 2F II II I II Ô Ô F III III I I F III III II II F III III III III 0 0 2F III III I II ˝ = 0 0 0 4F II III II III 4F II III I III 0 Ô Ô 0 0 0 0 4F I III II III 4F I III I III Ô Ô 0 0 4F I II I II 2F I II I I 2F I II II II 2F I II III III ˛

Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

s xx s yy s zz t yz t xz t xy

¸ Ô Ô Ô Ô ˝ Ô Ô Ô Ô ˛

(13.6) 9

This is deduced from the general Equation 9.2.

© 2003 by CRC Press LLC

TX846_Frame_C13 Page 269 Monday, November 18, 2002 12:29 PM

13.2.1.2 Technical Form In analogy with the technical form of Equation 13.5, which was written in orthotropic axes, one can write the constitutive equation in terms of equivalent moduli and Poisson coefficients, as: Ï Ô Ô Ô Ô Ô Ô Ì Ô Ô Ô Ô Ô Ô Ó

e xx ¸ Ô Ô e yy Ô Ô e zz ÔÔ ˝ = g yz Ô Ô Ô g xz Ô Ô Ô g xy ˛

1 ----Ex – n xy ---------Ex

– n yx – n zx ---------- ---------Ey Ez

0

0

– n zy ---------Ez

0

0

1 ----Ez

0

0

1 ----Ey

– n xz – n yz ---------- ---------Ex Ey

0

0

0

1 -------G yz

x xz ------G xz

0

0

0

x yz ------G yz

1 -------G xz

hx ----Ex

my ----Ey

z ----zEz

0

0

h xy ------G xy

Ï Ô m xy Ô -------- Ô G xy Ô z xy Ô ------G xy Ô Ì 0 Ô Ô Ô 0 Ô Ô 1 Ô -------- Ó G xy

s xx ¸ Ô Ô s yy Ô Ô Ô s zz Ô ˝ t yz Ô Ô Ô t xz Ô Ô Ô t xy ˛

(13.7)

In this equation, there are coupling terms characterized by the coefficients hxy , mxy , zxy , and xxy , which are not similar to the Poisson coefficients. The values of elastic constants in Relation 13.7 are deduced immediately from the technical forms obtained above for the coefficients FIJKL. These constants are detailed below. One obtains subsequently the elastic modulus and Poisson coefficients in the x,y,z coordinates.

n c s 1 1 ----- = ----- + ---- + s 2 c 2 Ê ------- – 2 -----t-ˆ Ë Ex E Et Et ¯ G t 4

4

4 4 n s c 1 1 ----- = ----- + ---- + s 2 c 2 Ê ------- – 2 -----t-ˆ Ë G t Ey E Et Et ¯

1 1 ----- = ---Et Ez

1 E x ( q ) = --------------------------------------------------------4 4 ➡ 2 n tˆ c s 2 2 1 ----- + ---- + s c Ê ------– ---------Ë G t E t ¯ E Et ➡

➡

n n yx 4 4 – ------ = – -----t- ( c + s ) º Et Ey 1 1 1 º + c 2 s 2 Ê ---- + ---- – -------ˆ Ë E E t G t¯

➡

1 E y ( q ) = --------------------------------------------------------4 4 s c 2 n tˆ 2 2Ê 1 ----- + ----- + s c ------- – ---------Ë G t E t ¯ E Et E z ( q ) = E t ( "q )

n yx n ------ ( q ) = -----t- ( c 4 + s 4 ) º Ey Et 1 1 1 º – c 2 s 2 Ê ---- + ---- – -------ˆ Ë E E t G t¯

n zx 2n 2n – ------ = – Ê c -----t- + s ----ˆ Ë Et E t¯ Ez

➡

n zy 2n 2n – ------ = – Ê s -----t- + c ----ˆ Ë E E t¯ Ez t

➡

2(1 + n ) s 1 -------- = c 2 -------------------- + ------G t Et G yz

2 ➡ G yz ( q ) = ---------------------------s 2 2(1 + n)

2

© 2003 by CRC Press LLC

n zx ( q ) = c n t + s n 2

2

n zy ( q ) = s n t + c n 2

2

1

c -------------------Et

+ -----G t

TX846_Frame_C13 Page 270 Monday, November 18, 2002 12:29 PM

1 2(1 + n ) c -------- = s 2 -------------------- + ------G t G xz Et 2

1

2 ➡ G xz ( q ) = ------------------------c 2 2(1 + n) s -------------------- + ------Et G t

2 2 2 1 n 1 1 1 (c – s ) -------- = 4c 2 s 2 Ê ----- + ---- + 2 -----t-ˆ + ---------------------- ➡ G xy ( q ) = ---------------------------------------------------------------------2 2 2 n 2 2 1 (c – s ) 1 Ë E Et G xy Et ¯ G t - + 2 -----t-ˆ + ---------------------4c s Ê E----+ --Et ¯ G t Ë Et

Ï c2 s2 h xy ------- = – 2cs Ì ----- – ---- º G xy Ó E Et

Ï s2 c2 m xy ------- = – 2cs Ì ----- – ---- º G xy Ó E Et

;

n t 1 ¸ º + ( c – s ) Ê ----- – -----------ˆ Ë E t 2G t¯ ˝ ˛ 2

n t 1 ¸ º – ( c 2 – s 2 ) Ê ----- – -----------ˆ Ë E t 2G t¯ ˝ ˛

2

z xy ( n – n t ) ------- = – 2cs ------------------Et G xy

z xz 1 2(1 + n ) ------- = – cs Ê ------- – --------------------ˆ Ë G t G xz Et ¯

;

(13.8)

13.3 CASE OF A PLY One can observe from Equation 13.7 that the stress–strain relations in the plane x,y appear decoupled in the case when szz = 0. We suppose that this applies for the plies making a thin laminate. Each ply will be characterized in its plane by 10 the following relations which are extracted from relations 13.5 and 13.7: In the orthotropic axes ,t: Ï e ¸ Ô Ô Ô Ô Ì et ˝ = Ô Ô Ô Ô Óg t ˛

1 ----E

– n t --------Et

– n t --------E

1 ---Et

0

0

0 ÏÔs ¸Ô Ô Ô 0 Ì st ˝ Ô Ô 1 Ô Ô ------- t G t Ó t ˛

(13.9)

In the x,y axes, making an angle q with the orthotropic axes:

10

The orthotropic axes of Equation 13.5 are denoted as l,t,z for a ply (see Section 3.3.1).

© 2003 by CRC Press LLC

TX846_Frame_C13 Page 271 Monday, November 18, 2002 12:29 PM

Ï e xx ¸ Ô Ô Ôe Ô Ì yy ˝ = Ô Ô Ôg Ô Ó xy ˛

1 ----Ex

yx – -----E

h xy ------G xy

– n xy ---------Ex

1 ----Ey

m xy ------G xy

hx ----Ex

my ----Ey

1 -------G xy

n

y

Ï s xx ¸ Ô Ô Ôs Ô Ì yy ˝ Ô Ô Ôt Ô Ó xy ˛

For the constants, the values were shown in detail in 13.8.

© 2003 by CRC Press LLC

(13.10)

TX846_Frame_C14 Page 273 Monday, November 18, 2002 12:30 PM

14 THE HILL–TSAI FAILURE CRITERION

There are many failure criteria for orthotropic materials. The most commonly used 1 for design calculations is the so-called “Hill-Tsai” criterion. This criterion can be interpreted as analogous to the Von Mises criterion which is applicable to isotropic material in elastic deformation. We will review at the beginning the principal aspects of the Von Mises criterion.

14.1 ISOTROPIC MATERIAL: VON MISES CRITERION The material is elastic and isotropic. In Figure 14.1, one denotes by I,II,III the principal directions of the stress tensor S for a given point. The corresponding matrix is

sI 0 0 0 s II 0 0 0 s III The general form of the deformation energy dW for an elementary volume dV surrounding the point considered can be written as: 1 dW total = --2

ÂÂs i

ij

e ij dV

j

which can be reduced to 1 dW total = --- ( s I e I + s II e II + s III e III ) dV 2 1

See failure of composite materials in Section 5.3.2.

© 2003 by CRC Press LLC

TX846_Frame_C14 Page 274 Monday, November 18, 2002 12:30 PM

Figure 14.1 Principal Directions for the Stress Tensor

eI eII eIII are the principal strains that one can express as functions of stresses using the constitutive Equation 10.1 as: 1+n n e = ------------ S – --- trace ( S )I E E This leads to: 1Ï1 + n 2 n 2 2 2¸ Ê dW --------- ˆ = --- Ì ------------ ( s I + s II + s III ) – --- ( s I + s II + s III ) ˝ Ë dV ¯ total E 2Ó E ˛ (Note that (dW/dV) represents energy per unit volume). The total elastic deformation above is due to the dilatation and distortion of the material. The Von Mises criterion postulates that the material resists to a state of isotropic (or spherical) stress, but will plastify when the distortion energy per unit volume reaches a critical value. One notes that: dW dW Ê dW --------- ˆ = Ê --------- ˆ – Ê --------- ˆ Ë dV ¯ total Ë dV ¯ spherical stress Ë dV ¯ distorsion The isotropic portion of the stress state here is written as: a state of isotropic dilatation (Equation 10.1):

s I + s II + s III --------------------------------. 3

1 + n s I + s II + s IIIˆ n - – --- ( s I + s II + s III ) e = ------------ ÊË ------------------------------¯ E 3 E then: ¸ s I + s II + s IIIˆ 1Ï Ê dW - ¥ e˝ --------- ˆ = --- Ì 3 ¥ Ê ------------------------------Ë ¯ Ë dV ¯ spherical stress 3 2Ó ˛ ¸ 1 Ï 1 + n ( s I + s II + s III ) n Ê dW - – --- ( s I + s II + s III ) 2 ˝ --------- ˆ = --- Ì ------------ -------------------------------------Ë dV ¯ spherical stress 3 E 2Ó E ˛ 2

© 2003 by CRC Press LLC

It creates

TX846_Frame_C14 Page 275 Monday, November 18, 2002 12:30 PM

One obtains then by replacing: 1Ï1 + n 2 n 2 2 2 Ê dW --------- ˆ = --- Ì ------------ ( s I + s II + s III ) – --- ( s I + s II + s III ) º Ë dV ¯ distorsion E 2Ó E ¸ 1 + n ( s I + s II + s III ) n º – ----------- --------------------------------------- + --- ( s I + s II + s III ) 2 ˝ 3 E E ˛ 2

2 ( s I + s II + s III ) ¸ 1 Ï 2 dW 2 2 -˝ then: Ê --------- ˆ = ------- Ì ( s I + s II + s III ) – -------------------------------------Ë dV ¯ distorsion 4G Ó 3 ˛

(14.1)

One can rewrite as following the quantity in brackets: 2 2 --- { s I + s 2II + s 2III – s I s II – s II s III – s III s I } 3 2 --- { ( s I + s II + s III ) 2 – 3 ( s I s II + s II s III + s III s I ) } 3 1 2 Ê dW --------- ˆ = ------- { ( s I + s II + s III ) º Ë dV ¯ distorsion 6G º – 3 ( s I s II + s II s III + s III s I ) }

(14.2)

Remarks: If one denotes as n the direction making the same angle with each of the principal directions (following Figure 14.1), one observes on the face with the normal n, a stress s such that: s = S(n) that is: Ï sI / 3 ¸ Ô Ô {s } = Ì s II / 3 ˝ Ô Ô Ó s III / 3 ˛ which can be decomposed as: A normal stress: sn = s ◊ n

s I + s II + s III s n = -----------------------------3

then:

The above consists of the average or isotropic part of the stress tensor.

2

A shear stress:

t = 2

s – sn 2

2

Recall the expression sI + sII + sIII that constitutes the first scalar invariant of the stress tensor.

© 2003 by CRC Press LLC

TX846_Frame_C14 Page 276 Monday, November 18, 2002 12:30 PM

then:

s I + s II + s IIIˆ 2 ¸ 1Ï 2 2 2 2 - ˝ t = --- Ì s I + s II + s III – ÊË ------------------------------¯ 3 3Ó ˛ which can be compared with Equation 14.1. Thus, 1 3 2 Ê dW --------- ˆ = ------- Ê --- t ˆ Ë dV ¯ distorsion 2G Ë 2 ¯ The shear stress t also appears as the shear characteristic of the distortion energy. One recognizes in Equation 14.2 the presence of the first and second scalar invariants of the stress tensor independent of the coordinate system. In coordinate axes other than the principal directions, the second invariant can be written as: ( s 11 s 22 – t 12 ) + ( s 22 s 33 – t 23 ) + ( s 33 s 11 – t 31 ) 2

2

2

One then has for any coordinate system: 1 2 Ê dW --------- ˆ = ------- { ( s 11 + s 22 + s 33 ) º Ë dV ¯ distorsion 6G º – 3 ( ( s 11 s 22 – t 212 ) + ( s 22 s 33 – t 223 ) + ( s 33 s 11 – t 231 ) ) } then: 1 2 2 Ê dW --------- ˆ = ---------- { ( s 11 – s 22 ) + ( s 22 – s 33 ) º Ë dV ¯ distorsion 12G º + ( s 33 – s 11 ) 2 + 6 ( t 212 + t 223 + t 231 ) } The elastic domain (where the distortion energy is below a certain critical value) can then be characterized by the condition: 2 2 2 a { ( s 11 – s 22 ) + ( s 22 – s 33 ) + ( s 33 – s 11 ) º

º + 6 ( t 212 + t 223 + t 231 ) } < 1

(14.3)

To determine the constant, a uniaxial test is sufficient; in effect if one denotes by se the elastic limit obtained from a tension–compression test, one has: a ¥ 2 se = 1 2

then: a = 1/2 s e

2

© 2003 by CRC Press LLC

TX846_Frame_C14 Page 277 Monday, November 18, 2002 12:30 PM

Figure 14.2 Principal Axes for an Orthotropic Ply

14.2 ORTHOTROPIC MATERIAL: HILL–TSAI CRITERION 14.2.1 Preliminary Remarks A parallel with the Von Mises criterion can be seen with the following remarks: For an orthotropic material, the principal directions for the stresses do not coincide with the orthotropic directions, unlike the isotropic case. A uniaxial test is not enough to determine all the terms of the equation for the criterion because the mechanical behavior changes with the direction of loading. For the fiber/resin composites, the elastic limit corresponds with the rupture limit. The rupture strengths are very different when loading is applied along the l direction or along the t direction. The rupture strengths are different in tension as compared with in compression. One can then write in the orthotropic coordinates ,t,z — shown in Figure 14.2 — an expression similar to Equation 14.3, as: a ( s – s t ) + b ( s t – s z ) + c ( s z – s ) + d t z + e t tz + f t t £ 1 2

2

2

2

2

2

(14.4)

14.2.2 Case of a Transversely Isotropic Material In the following, we will limit ourselves, for the purpose of simplification, to the 3 case of a transversely isotropic material. The constants a, b, c, d, e, f in Equation 14.4 above will be determined using the results of the following tests: Test along the longitudinal direction : 1 a + c = ------2s rupture 3

For an orthotropic material, the procedure is identical.

© 2003 by CRC Press LLC

TX846_Frame_C14 Page 278 Monday, November 18, 2002 12:30 PM

Test along the transverse direction t: 1 a + b = ------2 s t rupture Test along the transverse direction z: due to transverse isotropy:

1 b + c = ------2 s t rupture then:

1 a = c = ---------22 s rupture 1 1 – ---------2 b = ------2 s t rupture 2 s

rupture

Shear tests:

1 t t Æ f = -----2t t rupture

1 t tz Æ e = -----2t tz rupture 1 t Æ d = -----2t t rupture

z

due to transverse isotropy. Replacing in Equation 14.4:

1 ---------2 2 s

{ ( s – st ) + ( s – sz ) } º 2

2

rupture

t tz 1 1 1 ˆ 2 º – Ê ---------------------- ( t 2t + t 2z ) + -------------------£1 - – ------------------ ( s t – s z ) + ------------------2 2 2 Ë 2 s2 ¯ t t rupture t tz rupture s t rupture rupture 2

© 2003 by CRC Press LLC

TX846_Frame_C14 Page 279 Monday, November 18, 2002 12:30 PM

4

and in developing :

s st + sz s 2 1 ------------------- + ------------------ – ------------------- – ------------------ ˆº - ( s t + s z ) + s z s t Ê ------------------2 2 2 2 Ë s2 ¯ s rupture s t rupture s rupture s rupture t rupture 2

2

2

t tz t + t z º + t-------------------- £1 + ------------------2 2 t t rupture t tz rupture 2

2

2

(14.5)

Remark: For the case of a “three-dimensional” orthotropic material, an analogous reasoning to the previous presentation leads to a more general criterion, which can be written as:

s st sz 1 1 1 ˆ ------------- + ------------- – ------------+ -----------s st º + -----------– Ê ------------2 2 2 2 2 2 Ë s rupt. s t rupt. s z rupt. s rupt. s t rupt. s z rupt.¯ 2

2

2

1 1 1 1 1 ˆ 1 ˆ º – Ê ------------ + ------------– ------------s t s z – ÊË ------------+ ------------– ------------ sz s º 2 2 2 2 2 Ë s2 ¯ ¯ s s s s s t rupt. z rupt. z rupt. rupt. rupt. t rupt.

tt t tz tz º + ------------- + ------------- + --------------£1 2 2 2 t t rupt. t tz rupt. t z rupt. 2

2

2

14.2.3 Case of a Unidirectional Ply Under In-Plane Loading When the stress state is plane-stress, in the plane defined by the axes ,t (see Figure 14.2), one has

s z = t z = t tz = 0 Equation 14.5 is simplified, and one obtains what is called “the Hill–Tsai criterion” for a ply subject to stresses within its plane:

s st s st tt ------------------ + ----------------- – ------------------ + ------------------ 0) and Equations 14.7, s rupture will be the limit stress in compression, and st rupture the limit stress in tension for 0∞ £ q £ 90∞.

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 283 Monday, November 18, 2002 12:30 PM

15 COMPOSITE BEAMS IN FLEXURE Due to their slenderness, a number of composite elements (mechanical components or structural pieces) can be considered as beams. A few typical examples are shown schematically in Figure 15.1. The study of the behavior under loading of these elements (evaluation of stresses and displacements) becomes a very complex problem when one gets into three-dimensional aspects. In this chapter, we propose a monodimensional approach to the problem in an original method. It consists of the definition of displacements corresponding to the traditional stress and moment resultants for the applied loads. This leads to a homogenized formulation for the flexure—and for torsion. This means that the equilibrium and behavior relations are formally identical to those that characterize the behavior of classical homogeneous beams. Utilization of these relations for the calculation of stresses and displacements then leads to expressions that are analogous to the common beams. We will limit ourselves to the composite beams with constant characteristics (geometry, materials) in any cross section, made of different materials—which we call phases —that are assumed to be perfectly bonded to each other. To clarify the procedure and for better simplicity in the calculations, we will limit ourselves in this chapter to the case of composite beams with isotropic phases. The extension to the transversely isotropic materials is immediate. When the phases are orthotropic, with eventually orthotropic directions that are changing from one point to another in the section, the study will be analogous, with a 1 much more involved formulation.

15.1 FLEXURE OF SYMMETRIC BEAMS WITH ISOTROPIC PHASES In the following, D symbolizes the domain occupied by the cross section, in the y,z plane. The external frontier is denoted as ∂D. One distinguishes also (see Figure 15.2) the internal frontiers which limit the phases, denoted by lij for two contiguous phases i and j. The area of the phase i is denoted as Si; its moduli of elasticity are denoted by Ei and Gi. The elastic displacement at any point of the beam has the components: ux (x, y,z); uy (x,y,z); uz (x,y,z). The beam is bending in the plane of symmetry x,y under external loads which are also symmetric with respect to this plane. 1

The only restrictive condition lies in the fact that one of the orthotropic directions is supposed to remain parallel to the longitudinal axis of the beam.

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 284 Monday, November 18, 2002 12:30 PM

Figure 15.1 Composite Beams

Figure 15.2 Composite Beam, with Plane of Symmetry

15.1.1 Degrees of Freedom 15.1.1.1 Equivalent Stiffness One writes in condensed form the following integrals taken over the total cross 2 section : · ESÒ =

Ú

=

E i dS or

D

ÂE S

i i

i

number of phases

· EI zÒ =

Ú

ÂE I

=

2

E i y dS or

D

i zi

i

number of phases

· GSÒ =

Ú

D

G i dS or

=

ÂG S

i i

i

number of phases

2

Izi is the quadratic moment of the Phase i with respect with z axis.

© 2003 by CRC Press LLC

(15.1)

TX846_Frame_C15 Page 285 Monday, November 18, 2002 12:30 PM

15.1.1.2 Longitudinal Displacement By definition, longitudinal displacement is denoted by u(x) and written as: 1 u ( x ) = -----------· ESÒ

Ú

D

E i u x ( x, y, z )dS

which consists of a mean displacement u(x) and an incremental displacement Dux as: u x ( x, y, z ) = u ( x ) + Du x ( x, y, z ) where one notes that:

Ú

D

E i Du x dS = 0

(15.2)

15.1.1.3 Rotations of the Sections By definition, this is the fictitious rotation—or equivalent—given by the following expression: –1 q z ( x ) = ------------· EI zÒ

Ú

E i u x ( x, y, z ) ¥ y dS

Ú

E i y dS +

D

Or, with the above: –1 Ï q z ( x ) = ------------- Ì u ( x ) · EI zÒ Ó

D

¸ E i Du x ( x, y, z )y dS ˝ D ˛

Ú

15.1.1.4 Elastic Center Origin 0 of the coordinate y is chosen such that the following integral is zero:

Ú

D

E i y dS = 0

We call elastic center the corresponding point 0 that is located as in the expression above. Then Dux takes the form: Du x ( x, y, z ) = – y q z ( x ) + h x ( x, y, z ) 3

with :

Ú

D

E i h x y dS

and

Ú

D

E i h x dS = 0

(*)

The displacement ux (x,y,z) can then take the form: u x ( x, y, z ) = u ( x ) – y q z ( x ) + h x ( x, y, z ). 3

In what follows, the second property is the consequence of Equation 15.2.

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 286 Monday, November 18, 2002 12:30 PM

15.1.1.5 Transverse Displacement along y Direction By definition, this is v(x) that is given by the following expression: 1 v ( x ) = -----------· GSÒ

Ú

D

G i u y ( x, y, z )dS

It follows from this definition that: u y ( x, y, z ) = v ( x ) + h y ( x, y, z ) where one notes that:

Ú

G i h y dS = 0.

D

15.1.1.6 Transverse Displacement along z Direction By definition, this is w(x) given by 1 w ( x ) = -----------· GSÒ

Ú

D

G i u z ( x, y, z )dS

It follows from this definition and from the existence of the plane of symmetry x,y of the beam a zero average transverse displacement, as: w(x) = 0. u z ( x, y, z ) = 0 + h z ( x, y, z ),

with

Ú

D

G i h z dS = 0.

In summary, we obtain the following elastic displacement field: Ê u x = u ( x ) – y q z ( x ) + h x ( x, y, z ) Á u = v(x ) + h y ( x, y, z ) Á y Ë uz = h z ( x, y, z )

(15.3)

The origin of the axes is the elastic center such that:

Ú

D

E i y dS = 0

(15.4)

The three-dimensional incremental displacements hx, hy, hz with respect to the unidimensional approximation u, v, qz verify the following:

Ú E h dS = Ú Ú G h dS = 0 Ú G h dS = 0 i

x

D

D

i

y

i

z

D

D

© 2003 by CRC Press LLC

E i y h x dS = 0 (15.5)

TX846_Frame_C15 Page 287 Monday, November 18, 2002 12:30 PM

Remarks: hx represents the longitudinal distortion of a cross section, that is, the quantity that this section displaces out of the plane which characterizes it if it moves truly as a rigid plane body. hy and hz represent the displacements that characterize the variations of the form of the cross section in its initial plane.

15.1.2 Perfect Bonding between the Phases 15.1.2.1 Displacements The bonding is assumed to be perfect. Then the displacements are continuous when crossing through the interface between two phases in contact. For two phases in contact i and j, one has: ux i

= ux j

uy i

= uy j

uz i

= uz j

15.1.2.2 Strains For the phases i and j in Figure 15.3, in the plane of an elemental interface with a normal vector of n, the relations between the strain tensors e are: x ◊ e(x) i = x ◊ e(x) j t ◊ e(x) i = t ◊ e(x) j t ◊ e( t ) i = t ◊ e( t ) j which can also be written as:

e xx = e xx i j – e xy n z + e xz n y = – e xy n z + e xz n y i

i

j

j

e yy n – 2 e yz n y n z + e zz n = e yy n – 2 e yz n y n z + e zz n y 2 z

i © 2003 by CRC Press LLC

2 y

i

i

2 z

j

2

j

j

TX846_Frame_C15 Page 288 Monday, November 18, 2002 12:30 PM

Figure 15.3 Interface between Two Phases

15.1.2.3 Stresses The stress vector s = S ( n ), where S represents the stress tensor, remains continuous across an element of the interface with normal n as:

t xy n y + t xz n z = t xy n y + t xz n z i

i

j

j

s yy n y + t yz n z = s yy n y + t yz n z i i j j t yz n y + s zz n z = t yz n y + s zz n z i

i

j

(15.6)

j

15.1.3 Equilibrium Relations Starting from the local equilibrium, in the absence of body forces, we have

∂s ij --------- = 0 ∂ xj By integrating over the cross section: d -----dx

Ú

D

s xx dS +

∂ t xzˆ xy Ê ∂t --------- + --------- dS = 0 Ë ∂y ∂z ¯ D

Ú

where the normal stress resultant Nx appears as: Nx =

Ú

D

s xx dS .

Then, transforming the second integral to an integral over the frontier ∂D of D : 4

dN ---------x + dx 4

∂t xy

∂t xz

Ú

∂D

( t xy n y + t xz n z )dG = 0

- + ------ )dS = Ú ∂ D ( t xy n y + t xz n z )d G is made possible due to the contiNote that equality Ú D ( -----∂y ∂z nuity of the expression (txy ny + txz nz) across the interfaces between the different phases (see Equation 15.6).

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 289 Monday, November 18, 2002 12:30 PM

in which ny and nz are the cosines of the outward normal n , and d G represents element of frontier ∂D. If one assumes the absence of shear stresses applied over the lateral surface of the beam, then txy ny + txz nz = 0 along the external frontier ∂D. Then for longitudinal equilibrium we have5 dN ---------x = 0 dx d -----dx

Ú

D

t xy dS +

∂t yzˆ yy Ê ∂s ---------- dS = 0 + --------Ë ∂y ∂z ¯ D

Ú

where one recognizes the shear stress resultant: Ty =

Ú

D

t xy dS.

Then transforming the second integral into an integral over the external frontier 6 ∂D of the domain D of the cross section :

∂T --------y + ∂x

Ú

( s yy n y + t yz n z )d G = 0

∂D

if one remarks that:

Ú

∂D

(s yy n y + t yz n z )d G =

Ú

∂D

y ◊ S ( n )d G = y ◊

Ú

∂D

s dG = p y ( N/m )

which is the transverse density of loading on the lateral surface of the beam, transverse equilibrium can be written as: dT y --------- + p y = 0 dx d -----dx

5

Ú

D

– y s xx dS +

∂t xy ∂ t xzˆ - + ---------- dS = 0 – y Ê --------Ë ∂y ∂z ¯ D

Ú

We have neglected the body forces which appear in the local equation of equilibrium in the form of a function fx. If these exist (inertia forces, centrifugal forces, or vibration inertia, for dN - + p x = 0 in which p x = Ú D f x dS represents the example), one obtains for the equilibrium: -----dx longitudinal load density. ∂s ∂t - ) dS = Ú ∂D ( s yy n y + t yz n z )d G is made possible due to the Note that the equality Ú D ( ------+ -----∂y ∂z x

6

yy

yz

continuity of the expression (syy ny + tyz nz ) across the frontier lines between different phases (see Equation 15.6).

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 290 Monday, November 18, 2002 12:30 PM

where appears the moment resultant: Mz =

Ú

D

– y s xx dS.

7

Then transforming the second integral : dM ----------z + dx

Ú

∂D

– y ( t xy n y + t xz n z ) dG +

Ú

D

t xy dS = 0

where one notes that:

Ú

∂D

– y ( t xy n y + t xz n z ) dG =

Ú

∂D

– yx ◊ S ( n )dG º =

Ú

∂D

– y ( s ◊ x ) dG = m z ( mN/m )

which can be called a density moment on the beam. Then one obtains the equilibrium relation: dM ----------z + T y + m z = 0 dx The case where a density moment could exist in statics is practically nil, we therefore assume that mz = 0. In summary, one obtains for the equations of equilibrium: dN ---------x = 0 dx dT y --------- + p y = 0 dx dM ----------z + T y = 0 dx

(15.7)

15.1.4 Constitutive Relations Taking into account the isotropic nature of the different phases, the constitutive relation can be written in tensor form for Phase i as: 1 + ni ni – ----tr ( S )I e = -------------S Ei Ei

7

( I = unity tensor)

Analogous note for the continuity of the expression (txy ny + txz nz) across the lines of internal interfaces (Equation 15.6).

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 291 Monday, November 18, 2002 12:30 PM

One deduces, in integrating over the domain occupied by the cross section of the beam:

Ú

D

Ú

e xx E i dS =

D

s xx dS –

Ú

D

n i ( s yy + s zz )dS

Taking into account the form of the displacements in Equation 15.3, one can write

Ú

D

e xx E i dS =

∂u dq ---------x E i dS = – ---------z ∂ x dx D

Ú

∂ E i dS + -----x ∂ D

du yE i dS + ------dx D

Ú

Ú

Ú

D

E i h x dS

which leads, with the notation in Equation 15.1, to the relation: du N x = · ESÒ ------- + dx

Ú

D

Ú

– y e xx E i dS =

D

Ú

D

– y s xx dS +

n i ( s yy + s zz )dS

Ú

D

(15.8)

n i y( s yy + s zz ) dS

Taking into account the form of the displacements in Equation 15.3 one can write dq – y e xx E i dS = ---------z dx D

du 2 E i y dS – ------dx D

Ú

Ú

∂ E i y dS – -----∂x D

Ú

Ú

E i y h x dS

D

This leads, with the notation in Equation 15.1, to the relation: dq M z = · EI zÒ ---------z – dx

Ú

D

Ú

D

n i y ( s yy + s zz ) dS

2 e xy G i dS =

Ú

D

t xy dS

(15.9)

Taking into account the form of the displacements in Equation 15.3, one can write

Ú

D

2 e xy G i dS =

u x ∂u yˆ Ê ∂-------- + -------- G i dS = – q z Ë ∂x ¯ D ∂y

Ú

º+

∂h dv G i ---------x dS + -----∂y dx D

Ú

G i dS º

D

∂ G i dS + -----∂x D

Ú

Ú

Ú

D

h y G i dS

which gives with the notation in Equation 15.1, the relation: dv T y = · GSÒ Ê ------ – q zˆ + Ë dx ¯ © 2003 by CRC Press LLC

∂h Gi ---------x dS ∂y D

Ú

(15.10)

TX846_Frame_C15 Page 292 Monday, November 18, 2002 12:30 PM

15.1.5 Technical Formulation 15.1.5.1 Simplifications We extend to the composite beams the simplifications made for the homogeneous beams as: 1. syy and szz ---------z (Equation 15.9) and N x # < ES > ------- (Equation 15.8): dx dx Mz Nx - y + E i ----------s xx = – E i -----------· EI zÒ · ESÒ bending

(15.11)

extension

Remark: The continuity (exx )i = (e xx )j at the interface between the Phases i and j leads to 10

( s xx ) i ( s xx ) -------------- = --------------j Ei Ej

8

9

10

This hypothesis is better verified by the fact that the Poisson coefficients of the different phases have similar values. This hypothesis is known in the literature for the homogeneous beams as the generalized “Navier–Bernoulli” hypothesis. See Section 15.1.2.

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 293 Monday, November 18, 2002 12:30 PM

Figure 15.4 Normal and Bending Stresses

which shows the discontinuity of normal stresses due to the difference in the longitudinal moduli, as illustrated in Figure 15.4.

15.1.5.3 Shear Stress Expression 15.1.5.3.1 Characterization of Warping Starting from the local equilibrium described by the relation:

∂s ij --------- = 0 ∂ xj we study the flexure shear stress in the plane of the cross section, noted as:

t = t xy y + t xy z Taking into consideration Equations 15.11 and 15.7, and the simplification 2, at the beginning of Section 15.1.5.1, one can write E i dN x E i dM z ∂t xy ∂ t xz Ei ∂s xx ---------- + ---------- = – ---------- ----------y – ----------- --------- = – ------------ = ------------T ¥ y ∂y ∂z · EI zÒ dx · ESÒ dx ∂x · EI zÒ y and with the displacement field in Equation 15.3:

∂h ∂h Ei -¥y G i Ê ----------2-x + ----------2-xˆ = – T y -----------Ë ∂y ¯ · EI zÒ ∂z 2

2

Putting hx in the form: Ty ¥ g ( y,z ) h x = -----------·GS Ò © 2003 by CRC Press LLC

(15.12)

TX846_Frame_C15 Page 294 Monday, November 18, 2002 12:30 PM

leads to E · GSÒ 2 — g = – -----i ------------- ¥ y G i · EI zÒ

(15.13)

and Equation 15.10 becomes dv T y = · GSÒ Ê ------ – q zˆ + Ë dx ¯ 1 T y Ê1 – -----------Ë · GSÒ

Ty ∂ g ------ dS G i -----------· GS Ò ∂y D

Ú

∂g dv G i ------ dSˆ = · GSÒ Ê ------ – q zˆ ¯ Ë ¯ ∂ y dx D

Ú

or: · GSÒ dv T y = ------------ Ê ------ – q zˆ ¯ k Ë dx

(15.14)

In the above relation appears a k coefficient which is analogous to the shear coefficient for homogeneous beams.

15.1.5.3.2 External Limit Condition We have supposed that the lateral surface of the beam is free from shear. This gives, along the external contour ∂D of the cross section, the relation:

t ◊ n = t xy n y + t xz n z = 0, and, with the displacement field in Equation 15.3 and the simplifications described above: dv Ê -----– q zˆ n y + grad h x ◊ n = 0 Ë dx ¯ Introducing the function g(y,z) (Equation 15.12) and with 15.14, one obtains

∂g grad g ◊ n = ------- = – kn y ∂n Substituting the function g(y,z) with the function go (y,z) such that: g o ( y,z ) = g ( y,z ) + k ¥ y © 2003 by CRC Press LLC

(15.15)

TX846_Frame_C15 Page 295 Monday, November 18, 2002 12:30 PM

one verifies that go is solution of the problem: E · GSÒ Ï — 2 g o = – -----i ------------ ¥ y in domain D G i · EI zÒ Ô Ì go Ô ∂------Ó ∂ n- = 0 on the boundary ∂ D We denote go(y,z) as the longitudinal warping function for the cross section.

15.1.5.3.3 Conditions at the Interfaces The continuity conditions already described in Section 15.1.2 lead for the warping function, at the interface between two phases i and j, g oi = g oj

t xyi n y + t xzi n z = t xyj n y + t xzj n z then:

∂g ∂g G i --------oi- = G j --------oj∂n ∂n

15.1.5.3.4 Uniqueness of the Solution This is given by Equation 15.5 which is interpreted here as:

Ú

D

E i g o dS = 0

15.1.5.3.5 Form of the Shear Stresses One can easily verify the following expressions: Ty ∂ go -------t xy = G i -----------· GSÒ ∂ y Ty ∂ go -------t xz = G i -----------· GSÒ ∂ z then again: Ty t = G i ------------grad go · GSÒ

15.1.5.3.6 Shear Coefficient for the Section The shear coefficient for the section is obtained starting from the Equation 15.5:

Ú

D

© 2003 by CRC Press LLC

E i h x dS = 0

TX846_Frame_C15 Page 296 Monday, November 18, 2002 12:30 PM

This necessitates the knowledge of the warping function go. Then the above relation can be rewritten as: Ty E i -----------( g – k ¥ y ) ¥ y dS = 0 · GS Ò o D

Ú which leads to:

1 k = ------------· EI zÒ

Ú

E i g o ydS

D

In summary, in the absence of body forces (inertia forces for example), the bending of a composite beam in its plane of symmetry can be characterized by a homogenized formulation — equivalent to a classical homogeneous beam solution—in the following manner:

• Elastic center 0: it is such that

Ú

D

E i ydS = 0

• Equivalent stiffnesses: (15.16) · ESÒ =

ÂE S ; i i

i

· EI zÒ =

ÂE I

i zi

i

;

· GSÒ ------------ = k

Â i

1 G i S i ¥ --k

• Equilibrium relations: (stress resultants calculated at elastic center) dT dN x --------- = 0; --------y + p y = 0; dx dx • Constitutive relations: du N x = · ESÒ ------- ; dx

© 2003 by CRC Press LLC

dM ----------z + T y = 0 dx

· GSÒ dv T y = ------------ Ê ------ – q zˆ ; ¯ k Ë dx

dq M z = · EI zÒ ---------z dx

TX846_Frame_C15 Page 297 Monday, November 18, 2002 12:30 PM

(Contd.)

Stresses: Mz Nx - y + E i ----------s xx = – E i -----------· EI zÒ · ESÒ

normal stresses

Ty ∂ go -------- ¸ t xy = G i -----------· GSÒ ∂ y Ô Gi gradg o ˝ t = ------------T · GS Ò y Ty ∂ go Ô t xz = G i ------------ -------- ˛ · GSÒ ∂ z

shear stresses

• longitudinal warping function go(y, z): it is the solution to the problem Ï ∂ 2g ∂ 2g Ô ----------o + ----------o = Ô ∂ y2 ∂ z2 Ì ∂ go Ô -------- = Ô ∂n Ó

E · GSÒ – -----i ------------- y in domain D of the section. G i · EI zÒ

(15.16)

0 on the boundary ∂ D

with internal continuity: ¸ Ô ∂ g oi ∂ g oj ˝ along internal boundaries ij G i --------- = G j --------- Ô ∂n ∂n ˛ g oi = g oj

and the uniqueness condition:

Ú

D

E i g o dS = 0

Shear coefficient k: it is given by the formula: 1 k = ------------· EI zÒ

Ú

E i g o y dS

D

15.1.6 Energy Interpretation 15.1.6.1 Energy Due to Normal Stresses sxx Denoting by dWs as the deformation energy of an elementary portion of a beam with length dx due to the application of normal stresses sxx, one has Ï1 1 dW s = --- s xx e xx dV = Ì --2 Ó2

Ú

© 2003 by CRC Press LLC

s xx ¸ -------- dS ˝dx D Ei ˛

Ú

2

TX846_Frame_C15 Page 298 Monday, November 18, 2002 12:30 PM

Taking into account Equation 15.11 for the normal stresses: dW 1 ----------s- = --dx 2 1 = --2

2 Ei Ei 1 - M z y + ----------- N x dS ---- – -----------· EI zÒ · ESÒ D Ei

Ú

2

Mz 2 1 -2 y dS + --E i -------------2 D · EI zÒ

Ú

2

Nx -2 dS º E i ------------D · ESÒ

Ú

Mz Nx -y dS E i -----------------------· EI zÒ · ESÒ D

Ú

º+

(the above expression simplifies due to the definition of the elastic center 0 in 15.16); therefore: 2

2

dW 1 Mz 1 Nx ----------s- = --- ------------ + --- ----------dx 2 · EI zÒ 2 · ESÒ

15.1.6.2 Energy Due to Shear Stresses t Denoting dWt as the deformation energy of an elementary portion of a beam with length dx due to the application of shear stresses t , one has: 1 dW t = --2

1Ï 2 ( t xy e xy + t xz e xz )dV = --- Ì 2Ó D

Ú

¸ 1 2 2 ----- ( t xy + t xz )dS ˝ dx G D i ˛

Ú

then, taking into account the form of the shear stresses in 15.16: dW 1 -----------t = --dx 2

T y Ï Ê ∂ g oˆ 2 Ê ∂ g oˆ 2 ¸ -2 Ì -------- + -------- ˝ dS G i -------------D · GSÒ Ó Ë ∂ y ¯ Ë ∂ y ¯ ˛ 2

Ú

2

dW t 1 Ty ----------- = --- -------------dx 2 · GSÒ 2

Ï∂ ¸ ∂g ∂g ∂ 2 G i Ì ------ Ê g o --------oˆ + ------ Ê g o --------oˆ – g o ◊ — g o ˝ dS Ë ¯ Ë ¯ ∂y ∂z ∂z D Ó ∂y ˛

Ú

11

with the value from 15.16 of the Laplacian of the warping function go : dW t 1 Ty Ï ----------- = --- -------------dx 2 · GSÒ 2 ÌÓ 2

11

∂ go

E · GSÒ Gi g o -----i ------------- ydS + G D i · EI zÒ

Ú

∂ go

∂ go

¸ ∂g G i g o --------o dG ˝ ∂ n ∂D ˛

Ú

∂ The equality Ú D G i { ∂---∂-y ( g o ----is made possible due the continuity of ) + ∂---z- ( g o ----) } dS = Ú ∂D G i g o -----dG ∂n ∂y ∂y g the quantities G i g o ∂----at the interfaces lij (See Section 15.1.5.3.3, “Conditions at the Interfaces”). o

∂n

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 299 Monday, November 18, 2002 12:30 PM

One knows in the above the expression of the shear coefficient k for the section (see 15.16). Then: 2

dW t 1 Ty ----------- = --- k -----------dx 2 · GSÒ In summary, the strain energy density can be written as: 2

2

2

1 Mz 1 Ty dW 1 N x - + --- k -------------------- = --- ------------ + --- -----------dx 2 · ESÒ 2 · EI zÒ 2 · GSÒ

(15.17)

Remarks: Note the analogy between this expression and that for the strain energy of a classical homogeneous beam, which should be written here as: 2

2

2

dW 1N 1M 1 T --------- = --- -----x- + --- ------z- + --- k ------ydx 2 ES 2 EI z 2 GS As a practical consequence of this homogenization, it becomes possible to determine the equivalent characteristics which are necessary for the entry of data into a computer program utilizing finite elements of classical homogeneous beams. The problem then comes to the numerical evaluation of the following values: Equivalent moduli: Eequivalent, Gequivalent, (or nequivalent) Geometric characteristics: Sequivalent, Iz

, and k

equivalent

By taking Sequivalent = S (real area of the cross section), one can easily verify that: E

· ESÒ · GSÒ G = ------------ ; = -----------equivalent S S · EI zÒ 1 · ESÒ n = -----------------; = --- ------------ – 1 equivalent E 2 · GSÒ

equivalent

Iz

equivalent

equivalent

15.1.7 Extension to the Dynamic Case The equilibrium relations of Section 15.1.3. were written in the absence of body forces. In vibratory motions, these body forces exist in the form of inertia forces. One then has

∂s ij --------- – r ü i = 0 ∂ xj © 2003 by CRC Press LLC

TX846_Frame_C15 Page 300 Monday, November 18, 2002 12:30 PM

Following the main steps of the calculations in Section 15.1.3, for a beam under 12 free vibration, one obtains: 2 ∂ Nx ∂ --------- = -------2 ∂x ∂t

Ú

r i u x dS

D

which leads, with Equation 15.3, to the following expression: 2 ∂ Nx ∂q ∂u --------- = · r S Ò --------2- – y G · r S Ò ---------2-z ∂x ∂t ∂t 2

in which we denote ·r S Ò =

Ú

D

r i dS

y G ·r S Ò =

and

Ú

D

r i y dS.

yG appears here as the ordinate of the mass center (center of gravity) of the section. One has neglected the secondary coupling due to hx: 2 ∂T ∂ --------y = -------2 ∂x ∂t

Ú

r i u y dS

D

with Equation 15.3 and neglecting the secondary coupling due to hx: 2 ∂T ∂v --------y = · r SÒ -------2∂x ∂t 2 ∂ Mz ∂ ---------- + T y = -------2 ∂x ∂t

Ú

D

– y r i u x dS

with Equation 15.3, posing · r I zÒ = Ú D r i y dS , and neglecting the secondary coupling due to hx: 2

2 ∂ Mz ∂q ∂u ---------- + T y = · r I zÒ ---------2-z – yG · r SÒ --------2∂x ∂t ∂t 2

The above relations are to be joined with the constitutive relations in 15.16. However one must note these constitutive relations were written in the absence of body forces. Nevertheless, we will consider them to be valid, with the condition that the concerned frequencies are not too high. Generally this case corresponds to the mechanical frequencies, and one denotes this as the “quasi static” domain. 12

One removes all the forces and moments on the beam except inertial forces and moments.

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 301 Monday, November 18, 2002 12:30 PM

In summary, in dynamic regime, one has to replace the equilibrium relations and the constitutive behavior which appear in 15.16 with the following relations: • Governing equations (stress resultants calculated at elastic center): 2 ∂ Nx ∂q ∂u --------- = · r S Ò --------2- – y G · r S Ò ---------2-z ∂x ∂t ∂t 2

2 ∂ Tx ∂v -------- = ·r S Ò -------2∂x ∂t

(15.18)

2 ∂ Mz ∂q ∂u ---------- + T y = · r I z Ò ---------2-z – y G · r S Ò --------2∂x ∂t ∂t 2

with · r SÒ =

Âr S ; i i

Âr I

· r I zÒ =

i zi

i

;

y G · r SÒ =

i

Ú

D

r i y dS

• Constitutive relations:

∂u N x = · ESÒ ------; ∂x

· GSÒ ∂ v T y = ------------ Ê ------ – q zˆ ; ¯ k Ë ∂x

∂q M z = · EI zÒ --------z ∂x

Remark: We note in the above relations a nonclassical coupling between the longitudinal oscillations u(x,t) and flexural oscillations. This coupling disappears 13 if the elastic center is mixed with the center of gravity.

15.2 CASE OF ANY CROSS SECTION (ASYMMETRIC) Now, the cross section of the beam does not present any particular symmetry (see Figure 15.5). One can consider for this general case the procedure adopted in the previous paragraph for beams with symmetry. One notes the supplementary equivalent stiffness: ·EI y Ò =

Ú

D

E i z dS = 2

Â EI

i yi i number of phases

It also appears an equivalent rotation qy(x) defined by the expression: 1 q y ( x ) = ------------· EI y Ò

Ú

D

E i u x ( x, y,z ) ¥ z dS

Then, from the definitions of qy, u, and qz (Section 15.1.1): 1 q y ( x ) = ------------· EI y Ò 13

See Chapter 18, Application 18.3.9.

© 2003 by CRC Press LLC

Ú

D

E i { u – y q z + h ox } ¥ z dS

TX846_Frame_C15 Page 302 Monday, November 18, 2002 12:30 PM

Figure 15.5 Composite Beam with any Cross Section

this expression simplifies if one chooses the origin of the coordinate z such that:

Ú

D

E i z dS = 0;

Ú

D

E i yz dS = 0

These relations, joined with the condition already established in the previous paragraph: Ú D E i y ds = 0 , allow one to define the position of the elastic center 0 of the section, as well as the orientation of the axes y and z that we will call the principal axes of the section. Then, in summary: elastic center:

Ú E y dS = 0 Ú E z dS = 0 Ú E yz dS = 0 i

D

i

D

principal axes:

i

D

One can then rewrite the contribution hox to the longitudinal displacement ux , which appeared above, in the form:

h ox ( x, y, z ) = z ¥ q y + h x ( x, y, z ) and one verifies that, by definition of the degree of freedom q y:

Ú

D

E i h x z dS = 0

The displacement ux (x, y, z) then takes the form: u x ( x, y, z ) = u ( x ) – y q z ( x ) + z q y ( x ) + h x ( x, y, z ) In addition, due to the disappearance of symmetry in the section, the transverse displacement w(x) (Section 15.1.1.6) is not zero. © 2003 by CRC Press LLC

TX846_Frame_C15 Page 303 Monday, November 18, 2002 12:30 PM

We then obtain for the elastic displacement field: ux = u (x ) – y qz + z qy + hx uy = v (x ) + hy uz = w ( x ) + hz The three-dimensional incremental displacements hx, hy,hz verify (see Section 15.1.1.6):

Ú

D

Ú

E i h x dS =

D

E i h x y dS =

Ú Ú

D

D

Ú

D

E i h x z dS = 0

G i h y dS = 0 G i h z dS = 0

Starting from the above and following the same procedure as in the previous paragraph, successively for the bending in the plane x,y, with identical results, then in the plane x,z, we obtain results summarized in the following relations:

• degree of freedom: u(x ) v ( x ); q y ( x )

along x: along y:

along z: w ( x ); q z ( x ) • elastic center: it is such that:

Ú

D

Ú

E i ydS =

D

E i z dS = 0

• principal axes: they are such that:

Ú

D

E i yz dS = 0

• equivalent stiffnesses: · ESÒ =

ÂE S

i i

i

· EI zÒ =

ÂE I

i zi

;

· EI yÒ =

i

· GSÒ ------------ = ky

© 2003 by CRC Press LLC

i yi

i

Â G S ¥ ----; k 1

i i

i

ÂE I

y

· GSÒ ------------ = kz

Â G S ¥ ----k1

i i

i

z

(Continued)

TX846_Frame_C15 Page 304 Monday, November 18, 2002 12:30 PM

(Contd.) • equilibrium relations: (stress resultants calculated at elastic center) dN ---------x = 0 dx dT dT y --------- + p y = 0; ---------z + p z = 0 dx dx dM z dM ---------- + T y = 0; ----------y – T z = 0 dx dx • constitutive relations: du N x = · ESÒ ------dx · GSÒ dv T y = ------------ Ê ------ – q zˆ ; ¯ k y Ë dx dq M z = · EI zÒ ---------z ; dx • normal stresses:

· GSÒ dw T z = ------------ Ê ------- + q yˆ ¯ k z Ë dx

14

(15.19)

dq M y = · EI yÒ --------y dx

Mz My Nx - y + E i ------------ z + E i ----------s xx = – E i -----------· EI zÒ · EI yÒ · ESÒ • shear stresses: Gi Ê ∂ go ∂h T y -------- + T z --------oˆ t xy = -----------Ë · GSÒ ∂y ∂y ¯ Gi Ê ∂ go ∂h T y -------- + T z --------oˆ t xz = -----------Ë · GSÒ ∂z ∂z ¯ then Gi t = ------------ ( T y grad g o + T z grad h o ) (Continued) · GSÒ

14

Remark: As already mentioned in Section 15.1.6 for a beam with a plane of symmetry, it is possible to evaluate the equivalent characteristics that one has to introduce in data form in order to utilize computer programs for the calculation by 14

· GSÒ dv

- ( ---- – q z ) it comes to a form such as: In fact, in place of the constitutive relation Ty = -------k y dx dv --- – q z ) where appears a coupling coefficient kyz. This means that a unique k y Ty + k yz Tz = · GSÒ ( dz shear resultant Tz leads to flexure in the x,y plane. This secondary effect has been neglected · GSÒ dw - + q y ). - ( ---here. Analogous remark yields for the constitutive relation T z = -------dx k z

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 305 Monday, November 18, 2002 12:30 PM

• Longitudinal warping functions: function go(y,z): It is the solution to the problem Ï ∂2 g ∂2 g E i · GSÒ Ô ----------o + ----------o = – ---- ------------- y in domain D of the section G i · EI zÒ Ô ∂ y2 ∂ z2 Ì ∂ go Ô -------- = 0 on the boundary ∂D Ô ∂n Ó with internal continuity: ¸ Ô ∂ g oi ∂ g oj ˝along internal boundaries ij G i --------- = G j --------- Ô ∂n ∂n ˛ g oi = g oj

and the uniqueness condition:

Ú

D

E i g o dS = 0

function ho(y,z): It is the solution to the problem : Ï ∂2 h ∂2 h E i · GSÒ Ô ----------o + ----------o = – ---- ------------- z in domain D of the section 2 G Ô ∂ y2 i · EI yÒ ∂z Ì ∂ ho Ô -------- = 0 on the boundary ∂D Ô ∂n Ó with internal continuity: ¸ Ô ∂ h oi ∂ h oj ˝along internal boundaries ij G i ---------- = G j ---------- Ô ∂n ∂n ˛ h oi = h oj

and the uniqueness condition:

Ú

D

E i h o dS = 0

• Shear coefficients coefficient k y : it is given by the formula: coefficient k z : it is given by the formula:

1 k y = ------------· EI zÒ

Ú

E i g o y dS

1 k z = ------------· EI yÒ

Ú

E i h o z dS

D

D

• Strain energy 2

2

2

2

2

Ty Tz 1 Mz 1 My 1 1 dW 1 N x - + --- ------------ + --- k y -------------------- = --- ------------ + --- -----------+ --- k z -----------dx 2 · ESÒ 2 · EI zÒ 2 · EI zÒ 2 · GSÒ 2 · GSÒ

© 2003 by CRC Press LLC

TX846_Frame_C15 Page 306 Monday, November 18, 2002 12:30 PM

15

finite elements for the classical beams. The characteristics Eequivalent, Gequivalent, Iz equivalent, Iy equivalent, can be obtained right away. On the contrary, the calculation of the shear coefficients ky and kz is not direct. At first it is necessary to know the values of the functions go and ho, solutions in the domain occupied by the cross section of Poisson type problem, as one can take note in the preceding table. The nature of these problems makes it possible for each of the functions go and ho to write an equivalent functional which allows the calculation of the function considered by means of discretization of the cross section using finite elements.

15

It is convenient to note that a computer program based on elements of homogeneous beams cannot provide correct values for the stresses in a cross section, because these stresses are of particular formulation for composite beams (see 15.16).

© 2003 by CRC Press LLC

TX846_Frame_C16 Page 307 Monday, November 18, 2002 12:32 PM

16 COMPOSITE BEAMS IN TORSION As in the previous chapter, we consider here the composite beams made of isotropic phases. Extension to transversely isotropic phases is straightforward. The study of orthotropic phases with one principal direction parallel to the axis of the beam, the other two principal directions in the plane of a cross section, does not present fundamental difficulties.

16.1 UNIFORM TORSION We will keep the conventions and notations of the previous chapter. On Figure 16.1, 0 is the elastic center, x, y, and z are the principal axes. The beam is slender and uniformly twisted, this means that every cross section is subjected to a pure and constant torsion moment, along the x axis, denoted as Mx. Then, under the application of this moment, each line in the beam, initially parallel to the x axis, becomes a helicoid curve, including (in the absence of symmetry in the cross section) the line which, initially, was coinciding with the elastic x axis itself. The only line which remains rectilinear is cutting the plane of all sections at a point which will be called torsion center and denoted as C, with coordinates yC and zC in the principal axes (see Figure 16.1).

16.1.1 Torsional Degree of Freedom By definition, this is the rotation of each section about the x axis, denoted as qx. The torsional moment Mx being constant, the angle qx evolves along the x axis in such a manner that, for any pair of cross sections spaced with a distance dx, one can observe a same increment of rotation dqx; then: 1

d qx --------- = constant dx 1

Here it is not necessary to define the rotation qx by means of an integral of displacements, as in the previous chapter relating to flexure. In effect, we will see in the following that the displacement field associated with this pure rotation of the sections leads to the exact solution of the problem in the elastic domain (at least for the case of uniform warping).

© 2003 by CRC Press LLC

TX846_Frame_C16 Page 308 Monday, November 18, 2002 12:32 PM

Figure 16.1 Elastic Center (O), Torsion Center (C), and Principal Axes

From this it comes that the angle of rotation of the sections varies linearly along the longitudinal axis x. As a consequence, we assume a priori the components of the displacement field ux, uy, uz, to be written as: dq u x = ---------x ¥ j ( y, z ) dx uy = –( z – z c ) qx

(16.1)

uz = ( y – y c ) qx where the function denoted as j (y, z) is characteristic of the cross section shape and of the materials that constitute the section. This is called the warping function for torsion.

16.1.2 Constitutive Relation With the displacement field in Equation 16.1 the only nonzero strains are written as: d q ∂j g xy = ---------x ÊË ------ – ( z – z c )ˆ¯ dx ∂y d q ∂j g xz = ---------x ÊË ------ + ( y – y c )ˆ¯ dx ∂z The only nonzero stresses are then the shear stresses txy and txz. The torsional moment can be deduced by integration over the domain of the straight section as: Mx =

dq ( y t xz – z t xy ) dS = ---------x dx D

Ú

Ï Gi Ì y D Ó

Ú

∂j Ê ----- – y cˆ º Ë ∂z ¯

¸ ∂j º – z Ê ----- + z cˆ + y 2 + z 2 ˝ dS Ë∂ y ¯ ˛ © 2003 by CRC Press LLC

TX846_Frame_C16 Page 309 Monday, November 18, 2002 12:32 PM

Substituting to the function j (y, z) the function F(y,z) such that: F ( y, z ) = j ( y, z ) + yz c – zy c

(16.2)

it becomes: dq M x = ---------x ¥ dx

∂F ∂F 2 2 G i Ê y -------- – z -------- + y + z ˆ dS Ë ¯ ∂ z ∂ y D

Ú

In this expression, it is possible to define an equivalent stiffness in torsion with the form: · GJ Ò =

Ú

D

∂F ∂F 2 2 G i Ê y -------- – z -------- + y + z ˆ dS Ë ∂z ¯ ∂y

(16.3)

One obtains then for the constitutive relation:

∂q M x = · GJ Ò --------x ∂x

16.1.3 Determination of the Function F(y,z) 16.1.3.1 Local Equilibrium Local equilibrium is written as:

∂t xy ∂t xz --------- + --------- = 0 ∂y ∂z then with the displacement field in Equation 16.1: 2

— j =0 and with form 16.2 of the function F: 2

— F =0

16.1.3.2 Conditions at the External Boundary The lateral surface being free of stresses, one can write along the external boundary ∂D:

t . n = 0. With the displacement field in Equation 16.1: Ï ∂f ¸ Ï ∂f ¸ - – ( z – z c ) ˝n y + Ì ------ + ( y – y c ) ˝ n z = 0 Ì ----Ó ∂y ˛ Ó ∂z ˛ © 2003 by CRC Press LLC

TX846_Frame_C16 Page 310 Monday, November 18, 2002 12:32 PM

then again:

∂F ∂F -------n y + -------n z = zn y – yn z ∂y ∂z

16.1.3.3 Conditions at the Internal Boundaries The continuity conditions of Section 15.1.2 are verified for uy and uz. At an interfacial line lij between two phases i and j, the continuity of ux leads to Fi = Fj The continuity relations in Equation 15.6 lead to the continuity of (txy ny + txz nz) when crossing the lines lij, that produces the continuity of

∂F ∂F G i Ê ---------i – zˆ n y + G i Ê ---------i + yˆ n z Ë ∂z ¯ Ë ∂y ¯

16.1.3.4 Uniqueness of the Function F If one superimposes torsion and bending, by using the degrees of freedom for flexure defined in the previous chapter, the displacement component ux becomes: dq u x = u – y q z + z q y + ---------x j + h x dx The longitudinal displacement u(x) has to respond to its definition (Section 15.1.1), meaning 1 u = -----------· ESÒ

Ú

E i u x dS

D

1 Ï u = ------------ Ì u · ESÒ Ó

Ú

E i dS – q z

Ú

q º+d ---------x dx

E i j dS +

D

Ú

D

D

E i y dS + q y

Ú

E i z dS º

D

¸ E i h x dS ˝ D ˛

Ú

This requires that:

Ú

D

E i j dS = 0

Then, taking into account the form in Equation 16.2 of F and the properties of the elastic center:

Ú

D

© 2003 by CRC Press LLC

E i F dS = 0

TX846_Frame_C16 Page 311 Monday, November 18, 2002 12:32 PM

In summary, the function F(y,z) is the solution of the problem: Ï —2 F = 0 Ô Ì ∂F - = zn y – yn z Ô ------Ó ∂n

in domain D of the section on the external boundary ∂D

with the internal continuity: Fi = Fj

¸ Ô along the internal ∂ Fi ∂ Fj ˝ Ê ˆ Ê ˆ G i --------- – ( zn y + yn z ) = G j --------- – ( zn y + yn z ) Ô boundaries ij Ë ∂n ¯ Ë ∂n ¯ ˛ and the condition of uniqueness:

Ú

D

E i F dS = 0

16.1.4 Energy Interpretation The strain energy of an elementary segment of a beam with thickness dx is written as: Ï1 1 dW = --- 2 ( t xy e xy + t xz e xz ) dV = Ì --2 Ó2

Ú

¸ 2 2 G i ( g xy + g xz ) dS ˝ dx D ˛

Ú

then, taking into account the displacement field in Equation 16.1: dW 1 dq --------- = --- Ê ---------xˆ dx 2 Ë dx ¯

2

2 2 Ï ∂F ¸ ∂F G i Ì Ê ------- – zˆ + Ê ------- + yˆ ˝ dS ¯ Ë ¯ Ë ∂z D Ó ∂y ˛

Ú

2

which can be rewritten as : 2 dW 1 dq Ï --------- = --- Ê ---------xˆ Ì dx 2 Ë dx ¯ Ó

º+

2

Ï ∂F ∂F 2 2¸ G i Ì y ------- – z ------- + y + z ˝ dS – ∂y D Ó ∂z ˛

Ú

Ú G F— F dSº 2

i

D

Ï ∂F ¸ ¸ ∂F G i F Ì Ê ------- – zˆ n y + Ê ------- + yˆ n z ˝ d G ˝ Ë ¯ Ë ¯ ∂z ∂D Ó ∂y ˛ ˛

Ú

In effect, one has, for example: 2 2 ¸ Fˆ ∂F ∂F ∂F ∂ F ∂ Ï ∂F Ê ∂------ – z ------- = ------- Ê ------- – zˆ = ------ Ì F Ê ------- – zˆ ˝ – F --------2Ë ∂y ¯ ¯ ¯ ∂y Ó Ë ∂y ∂y ∂y Ë ∂y ∂y ˛

© 2003 by CRC Press LLC

TX846_Frame_C16 Page 312 Monday, November 18, 2002 12:32 PM

where we note the presence of the stiffness in torsion ·GJ Ò defined by Equation 16.3. Thus, dq 2 dW 1 --------- = --- · GJ Ò Ê ---------xˆ Ë dx ¯ dx 2

2

1 Mx or = --- -----------2 · GJ Ò

16.2 LOCATION OF THE TORSION CENTER Consider the cantilever beam that is clamped at its left end as shown schematically in Figure 16.2, and more particularly the segment limited by the cross sections denoted by D0 and D1. In the section D1,0 is the elastic center and C is the torsion center the position of which we wish to determine. With this objective, we will apply on the cross section D1 the two following successive loadings: Loading No. 1: One applies on the torsion center C of the cross section D1 a force F situated in the plane of the section. Loading No. 2: One applies on the same cross section D1 a torsional moment denoted as Mx (see Figure 16.2). When one applies these two loads successively, the final state is independent of the order of the application. As a consequence for the external forces acting on the isolated segment (D0 D1), the work corresponding to loading No. 1 on the displacements created by loading No. 2 is equal to the work corresponding to loading No. 2 on the displacements created by loading No. 1. This can be written in the following form: W

(loading 1¥ displacement 2)

=W

(loading 2¥ displacement 1)

Now we evaluate these works: a) W (loading 1 ¥ displacement 2) On D0: F creates the bending moments Mz and My, thus a normal stress distribution given in the principal axes by Equation 15.17 as: Mz My - ¥ y + E i ------------¥z ( s xx ) 1 = – E i -----------· EI zÒ · EI yÒ

Figure 16.2 Cantilever Beam with Two Successive Loadings © 2003 by CRC Press LLC

TX846_Frame_C16 Page 313 Monday, November 18, 2002 12:32 PM

Then, taking into account the displacement field in Equation 16.1, the work done on D0 is

Ú

D

( s xx ) 1 ¥ ( u x ) 2 dS =

Ï ¸ dq Mz My - ¥ y + E i ------------ ¥ z ˝ ---------x j dS Ì – E i -----------· EI Ò · EI Ò DÓ z y ˛ dx

Ú

dq = ---------x dx

Ï ¸ Mz My - ¥ y + E i ------------ ¥ z ˝( F – yz c + zy c )dS Ì – E i -----------· EI zÒ · EI yÒ DÓ ˛

Ú

On D1: The torsion center C does not move in the plane of the cross section during torsion. The work done by the force F in the displacement field of torsion is nil. b) W (loading 2 ¥ displacement 1) Force F as applied to the torsion center C does not lead to the rotation of the cross sections around the longitudinal axis x. From this the torsional moment Mx does not work on the bending displacement field due to F . The equality of the two works is then written as: dq ---------x dx

Ï ¸ Mz My - ¥ y + E i ------------ ¥ z ˝( F – yz c + zy c )dS = 0 Ì – E i -----------· EI zÒ · EI yÒ DÓ ˛

Ú

then: Mz -----------· EI zÒ

Ú

D

( E i y F – E i y z c + E i yzy c )dS º

My º + -----------· EI yÒ

2

Ú

D

( E i z F + E i z y c – E i yzz c ) ds = 0 2

This relation has to be verified when the force applied at C varies in magnitude and direction in the plane of the section. One can deduce fr om there that the relation is valid no matter what the values of Mz and My are. Both the above integrals are then nil. One extracts from this property the coordinates of the torsion center: 1 y c = – ------------· EI yÒ

Ú

1 z c = ------------· EI zÒ

D

D

Ú

E i z F dS

E i y F dS

In summary, the uniform torsion of a cylindrical composite beam made of perfectly bonded isotropic phases can be characterized by a homogenized © 2003 by CRC Press LLC

TX846_Frame_C16 Page 314 Monday, November 18, 2002 12:32 PM

formulation — equivalent to that of a classical homogeneous beam — in the following manner:

• degree of freedom: about x axis: q x • elastic center 0: it is such that

ÚD Ei y dS

• principal axes: they are such that

=

ÚD Ei z dS

ÚD Ei yz dS

= 0

= 0

• equivalent stiffnesses: · EI z Ò =

Â Ei Izi

;

· EI yÒ =

Â Ei Iyi i

i

∂F ∂F 2 2 · GJ Ò = Ú G i Ê y -------- – z -------- + y + z ˆ dS Ë ∂z ¯ ∂y D • torsion center: coordinates in principal axes: 1 y c = – ------------- Ú E i z F dS · EI yÒ D 1 z c = -------------- Ú E i y F dS · EI z Ò D dM • equilibrium relation: ----------x = 0 dx

( M x = constant )

dq • constitutive relation: M x = · GJ Ò ---------x dx d qx ∂ F • shear stresses t xy = G i --------- ÊË -------- – zˆ¯ dx ∂y dq ∂ F t xz = G i ---------x ÊË -------- + yˆ¯ dx ∂z • function F(y, z): it is the solution to the problem: Ï ∂2 F ∂2 F Ô --------- + --------- = 0 in domain D of the section. Ô ∂ y2 ∂ z2 Ì Ô ∂F = zn y – yn z on the external boundary ∂D. Ô ------∂n Ó with internal continuity: Fi = Fj

¸ Ô along internal ∂ Fi ∂ Fj ˝ Ê ˆ Ê ˆ G i --------- – zn y + yn z = G j --------- – zn y + yn z Ô boundaries ij Ë ∂n ¯ Ë ∂n ¯ ˛ and the uniqueness condition: Ú E i F dS = 0 D

• strain energy density 2

1 Mx dW --------- = --- -----------2 · GJ Ò dx

© 2003 by CRC Press LLC

(16.4)

TX846_Frame_C16 Page 315 Monday, November 18, 2002 12:32 PM

Remarks: A finite element computer program for the classical homogeneous beams 3 is usable with the condition that the equivalent rigidity in torsion ·GJ Ò can be available. This requires the numerical calculation of the function 4 F. The latter is the solution of a Laplace type problem, which can be noted in relations 16.4. An equivalent functional is possible to define, which leads to the calculation of F by the finite element method, by means of discretization of the cross section. Flexion-torsion coupling: When, due to the loads applied on the beam, there exists simultaneously bending and torsion of the beam, the approach of the previous chapter is always valid. Keeping the definitions in Sections 15.1.1 and 15.2 for the degrees of freedom u, v, qx, qy, one arrives at the following displacement field:

Ï dq Ô u x = u – y q z + z q y + j ---------x + h x dx Ô Ìu = v – zq + h x y Ô y Ôu = w + yq + h x z Ó z

The torsion being uniform, the equilibrium relations in 15.19 become more restrictive and can be reduced to:

dT dT dN ---------x = 0; ---------y = 0; ---------z = 0 dx dx dx dM dM dM ----------x = 0; ----------z + T y = 0; ----------y – T z = 0 dx dx dx

3

4

(16.5)

Except if the considered application requires the calculation of the shear stresses in a cross section. One has to solve an analogous problem for the homogeneous beams, when one desires to calculate the torsional Saint-Venant stiffness: J =

© 2003 by CRC Press LLC

∂F

∂F

– z ------- + y ÚD ÊË y ------∂z ∂y

2

+ z 2ˆ dS . ¯

TX846_Frame_C16 Page 316 Monday, November 18, 2002 12:32 PM

Taking into account six degrees of freedom also leads to six constitutive 5 relations. One finds : du N x = · ESÒ ------dx dq · GS Ò dv T y = ------------- Ê ------ – q z – z c ---------xˆ (*) dx ¯ k y Ë dx dq · GS Ò dw T z = ------------- Ê -------- + q y + y c ---------xˆ (*) dx ¯ k z Ë dx dq M x = · GJ Ò ---------x – z c T y + y c T z dx dq M y = · EI yÒ --------y dx dq M z = · EI zÒ ---------z dx

5

(16.6)

In each of the relations marked with (*), there appears a supplementary coupling term connected to the existence of a third coefficient denoted as kyz. The complete form is then: dq dv k y T y + k yz T z = · GSÒ Ê ------ – q z – z c --------x-ˆ Ë dx dx ¯ dq dw k yz T y + k z T z = · GSÒ Ê -------- + q y + y c --------xˆ Ë dx dx ¯ This secondary coupling has been neglected in the indicated form.

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 317 Monday, November 18, 2002 12:33 PM

17 FLEXURE OF THICK COMPOSITE PLATES The mechanical behavior of a laminated plate as studied in Chapter 12 involves the definition of stress resultants Nx, Ny, Txy and moment resultants Mx, My, Mxy. These resultants are obtained from the membrane stresses sx, sy, txy. The other stress components, sz, txz, tyz have not been taken into account until now. In this chapter we note how these stresses exist and have influence on the mechanical behavior of the laminate. We will also examine the configurations of plates for which the influence of these stresses are significant (for example, plates with relatively high thicknesses, justifying the title given for this chapter). This study is based on the previous definition of the displacement parameters based on integral displacement forms, and constitutes an approach analogous (and also original) to that used in Chapter 15 for the description of the bending of composite beams.

17.1 PRELIMINARY REMARKS 17.1.1 Transverse Normal Stress sz The plate is situated as in Chapter 12 from which the name of transverse normal stress sz. Such stress appears due to the application of a transverse load (concentrated or distributed) which will cause bending of the plate. A very local concentration of load in a very small zone cannot be examined with the theory of plates, which is not able to provide spatial distribution of the stresses in the neighborhood of the point of load application. This phenomenon is complex even in three-dimensional numerical modeling. Therefore, what will be presented will not be valid in the immediate surroundings of a very local transverse load (for example, an insert). A distributed load gives rise to the stresses sz with small amplitude as compared with the stresses sx and sy. This is the reason why sz is often neglected.

17.1.2 Transverse Shear Stresses txz and tyz Due to the assumption of perfect bonding between the plies, the stress vector remains continuous across an interfacial element with normal vector n = z , between two consecutive plies of the laminate. Then txz and tyz remain continuous at the

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 318 Monday, November 18, 2002 12:33 PM

interfaces between plies (see Section 15.1.2). In addition, the upper face and lower face of the laminate are assumed to be free of tangential forces. The thickness of the laminate is denoted as h. One then has:

txz = tyz = 0 for z = ±h/2 Assume stress and moment resultants to be constant in a given zone of the laminate: Nx, Ny, Txy, My, Mx, Mxy constants "(x, y) Then, by inversion of Equation 12.20, for example, one notes that the following global strain 2

2

2

2

2

eox, eoy, goxy, ∂ w0 /∂x , ∂ w0 /∂y , 2∂ w0 /∂ x∂ y are constant in the zone under consideration. The local strains of Equation 12.12 then depend only on the coordinate z of the laminate. This is the same for the membrane stresses sx, sy, txy. With the above consideration, local equilibrium can be written as (in the absence of body forces):

∂s x ∂t xy ∂t xz --------- + ---------- + ---------- = 0 ∂x ∂y ∂z ∂t xy ∂s y ∂t yz --------- + -------- + ---------- = 0 ∂x ∂y ∂z

(17.1)

The transverse shear stresses then appear to be constant across the thickness of a ply. Being continuous at the interface and nil at the location z = ± h/2, they are nil in all the thickness of the laminate. From this, these stresses do not play an important role in all cases: they do not always exist, their existence being related to variable stresses and moment resultants. When they exist and depending on the composition of the laminate, they can have influence on the deformation in bending, and on the interlaminar adhesion (between layers). We will assume that these stresses exist, associated with the hypotheses of the following paragraph.

17.1.3 Hypotheses The plate has midplane symmetry. The plies are orthotropic, the orthotropic axes coinciding with the x, y, z 1 axes of the laminate. The stress sz is negligible.

1

For example, this is the case for a laminate made of layers of balanced fabric at 0∞, 90∞, or 45∞, –45∞, for unidirectional layers at 0∞ and 90∞, or for mats. Instead of this hypothesis, one can also adopt the less restrictive hypothesis of a balanced laminate. In this case the following calculations are much more involved, without appreciable gain on the enlargement of the field of applications examined in Section 17.6.3.

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 319 Monday, November 18, 2002 12:33 PM

Remarks: For each ply having orthotropic axes x, y, z, the constitutive Equation 13.3 can be written as, taking into account the simplification sz # 0: Ï ¸ Ï ¸ n 1 --- – ----yx- 0 0 0 Ô sx Ô Ô ex Ô Ex Ey Ô Ô Ô Ô n xy 1 Ô ey Ô Ô sy Ô --0 0 0 – ---Ey Ô Ô Ô Ô Ex Ô Ô Ô Ô 1 Ì g xy ˝ = 0 ------ 0 0 G 0 Ì t xy ˝ xy Ô Ô Ô Ô Ôg Ô Ô Ô 1 - 0 Ô t xz Ô 0 0 0 ----Ô xz Ô G xz Ô Ô Ô Ô 1 Ôt Ô Ô g yz Ô 0 0 0 0 ----yz G yz Ó Ó ˛ ˛ or under inverse form Ï sx ¸ E 11 Ô Ô Ô sy Ô E 21 Ô Ô t = Ì xy ˝ 0 Ô Ô 0 Ô t xz Ô Ôt Ô 0 Ó yz ˛

E 12 E 22 0 0 0

0 0 E 33 = G xy 0 0

0 0 0 0

0 0 0 E 44 = G xz 0

E 55 = G yz

Ï ex ¸ Ô Ô Ô ey Ô Ô Ô Ì g xy ˝ Ô Ô Ô g xz Ô Ôg Ô Ó yz ˛

(17.2)

where: Ex n yx E x Ey - ; E 12 = ----------------------- ; E 22 = ----------------------E 11 = ----------------------1 – n xy n yx 1 – n xy n yx 1 – n xy n yx The transverse shear is at the origin of distortions as illustrated in Figure 17.1 for the shear stress tyz. As a consequence, the displacements due to flexion discussed in Section 12.2.1 can be adapted as shown in Figure 17.2.

Figure 17.1 Distortion of Section due to Transverse Shear tyz

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 320 Monday, November 18, 2002 12:33 PM

Figure 17.2 Flexural Displacements

In this figure, (a) represents a section before and after bending and (b) shows the evolution of the section as a rigid displacement (parameters v0, w0, and qx) to which are associated increments hy and hz in the plane y,z. Note: Due to the existence of midplane symmetry, the antisymmetric manner with respect to z, these increments are small, but they cannot be neglected a priori. (At this stage, we do not have a definition for the equivalent rotation, noted as qx in b). This justifies the interest in the definition of the displacement field relating these increments. A supplementary interest rests in the possibility, during the study, to look after the necessary approximations more closely to lead to a useful 2 technical formulation.

17.2 DISPLACEMENT FIELD The elastic displacement at each point of the laminate has the components u(x, y, z), v (x, y, z) and w (x, y, z). With simplified description of Paragraph 12.2.1, one sees in Figure 17.2 (b), average translations denoted as v0 and w0, and a rotation of the section denoted as qx, to which one superimposes the supplementary displacements hy and hz. We will define these averages in integral forms as follows: Translation along x direction: By definition, this is u0 such that: 1 u 0 = --h

Ú

h/2

– h/2

u ( x, y, z ) dz

Rotation about the y axis: By definition, this is qy(x,y) such that : 3

qy =

2 3

Ú

h/2

– h/2

E 11 E 12 ˆ Ê -------- + --------- u ( x, y, z ) ¥ z dz Ë EI 11 EI 12¯

Approximations that do not appear neatly in the specialized literature. Such a definition of the “average rotation” q y will be fundamental in the following to ensure the energetic coherence of the formulation for the transverse shears (see Section 17.6.6).

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 321 Monday, November 18, 2002 12:33 PM

1 4 -. where one has reused the notations of Section 12.1.6 for the terms ---EI ij The longitudinal displacement u(x, y, z) then takes the form:

u ( x, y, z ) = u 0 ( x, y ) + z q y ( x, y ) + h x ( x, y, z ) with: h/2

E 11 E 12 ˆ Ê -------- + --------- h x z dz = 0 Ë – h/2 EI 11 EI 12¯

Ú

In effect, one can obtain starting from this expression:

Ú

h/2

– h/2

u dz = h ¥ u o + q y

Ú

h/2

– h/2

z dz +

Ú

h/2

– h/2

h x dz 5

the integrals disappearing due to antisymmetry in z : h/2

E 11 E 12 ˆ Ê -------- + --------- uz dz = u o Ë – h/2 EI 11 EI 12¯

Ú

… + qy +

h/2

E 11 E 12 ˆ Ê -------- + --------- z dzº Ë – h/2 EI 11 EI 12¯

Ú

h/2

E 11 E 12 ˆ Ê -------- + --------- h x z dz Ë – h/2 EI 11 EI 12¯

Ú

In the second member, the first integral disappears due to midplane symmetry. In addition, taking into account the definition of qy written above, the second integral is also nil. Translation along the y direction: This is v0(x,y) such that: 1 v 0 = --h

Ú

h/2

– h/2

v ( x, y, z ) dz

Rotation about the x axis: This is qx such that:

qx = –

Ú

h/2

– h/2

E 22 E 12 ˆ Ê -------- + --------- v ( x, y, z ) ¥ z dz Ë EI 22 EI 12¯

The longitudinal displacement v(x,y,z) then takes the form: v ( x, y ) = v 0 ( x, y ) – z q x ( x, y ) + h y ( x, y, z ) 4

Recall that (Section 12.1.6): th

1 ----- = [ C ] –1 , EI 5

n ply

where

Â

C ij =

st

3

3

k z k – z k-1ˆ E ij Ê ------------------Ë 3 ¯

k=I ply

The coefficient of qy is 1 because one can note that:

- + ---------ˆ z dz Ú–h/2 ÊË -------EI 11 EI 12¯ h/2

E 11

© 2003 by CRC Press LLC

E 12

2

2 C 11 C 12 C 12 C 11 C 22 - + --------- = ---------------------------= -------- – ---------------------------- = 1 2 2 EI 11 EI 12 C 11 C 22 – C 12 C 11 C 22 – C 12

TX846_Frame_C17 Page 322 Monday, November 18, 2002 12:33 PM

with:

Ú

( h/2 )

– h/2

E 22 E 12 ˆ Ê -------- + --------- h z dz = 0 Ë EI 22 EI 12¯ y

Translation along the z direction: This is w0(x,y) such that: 1 w 0 ( x, y ) = --h

Ú

( h/2 )

– h/2

w ( x, y, z ) dz

The vertical displacement takes the form: w ( x, y, z ) = w 0 ( x, y ) + h z ( x, y, z ) In summary, one obtains for the elastic displacement field: u = u 0 + z q y + h x ( x, y, z ) v = v 0 – z q x + h y ( x, y, z ) w = w0

(17.3)

+ h z ( x, y, z )

h x , h y , h z antisymmetric in z. h/2

E 11 E 12 ˆ Ê -------- + --------- h x z dz = Ë – h/2 EI 11 EI 12¯

Ú

(17.4)

h/2

E 22 E 12 ˆ Ê -------- + --------- h y z dz = 0 Ë – h/2 EI 22 EI 12¯

Ú

(17.5)

17.3 STRAINS One deduces from the previous displacements the strains:

∂q ∂h e x = e 0x + z --------y + ---------x ∂x ∂x ∂q ∂h e y = e 0y – z --------x + --------y ∂y ∂y ∂h ∂h ∂q ∂q g xy = g 0xy + z ÊË --------y – --------xˆ¯ + ---------x + --------y ∂y ∂x ∂y ∂x ∂w ∂h ∂h g xz = ---------0 + q y + ---------x + ---------z ∂x ∂z ∂x ∂w ∂h ∂h g yz = ---------0 – q x + --------y + ---------z ∂y ∂z ∂y

17.4 CONSTITUTIVE RELATIONS 17.4.1 Membrane Equations Recall the method that was already used in Section 12.1.1.

© 2003 by CRC Press LLC

(17.6)

TX846_Frame_C17 Page 323 Monday, November 18, 2002 12:33 PM

stress resultant N x = Ú –h/2 s x dx: h/2

Nx =

∂q ∂h E 11 Ê e 0x + z --------y + ---------xˆ dz + Ë ∂x ∂x ¯ – h/2

Ú

h/2

∂ N x = A 11 e 0x + A 12 e 0y + -----∂x

[ 17.2 ] et [ 17.6 ] : 6

from

Ú

h/2

– h/2

∂q ∂h E 12 Ê e 0y – z --------x + --------yˆ dz Ë ∂y ∂y ¯

∂ E 11 h x dz + -----∂y – h/2

Ú

h/2

Ú

h/2

– h/2

E 12 h y dz

stress resultant N y = Ú –h/2 s y dz: h/2

N y = A 21 e 0x + A 22 e 0y stress resultant T xy = Ú –h/2 t xy dz: h/2

T xy =

∂h ∂h ∂q ∂q E 33 Ê g oxy + z Ê --------y – --------xˆ + ---------x + --------yˆ dz Ë Ë ¯ ∂y ∂x ¯ ∂y ∂x – h/2

Ú

h/2

T xy = A 33 g oxy In summary, one finds again the relations already established in Chapter 12 (Equations 12.5) as: Ï Nx ¸ A 11 A 12 0 Ô Ô Ì N y ˝ = A 21 A 22 0 Ô Ô 0 0 A 33 Ó T xy ˛

Ï e ox ¸ Ô Ô Ì e oy ˝ Ô Ô Ó g oxy ˛

or, in inverse form, by using the notations in Equation 12.9: Ï e ox ¸ Ï Nx ¸ – n yx /E y 0 1/E x Ô Ô 1Ô Ô 1 –1 --e N ¥ = h [ A ] = Ì oy ˝ 1/E y 0 h ÌÔ y Ô˝ h – n xy /E x Ô Ô g T Ó oxy ˛ Ó xy ˛ 0 0 1/G xy

Ï Nx ¸ Ô Ô Ì Ny ˝ Ô Ô Ó T xy ˛

(17.7)

17.4.2 Bending Behavior One has again the already known moment resultants (see Section 12.2.1). Moment resultant M y = Ú –h/2 s x z dz: with [17.2] and [17.5]: h/2

My =

∂h 2 ∂q E 11 Ê z e ox + z --------y + z ---------xˆ dz … Ë ∂x ∂x ¯ – h/2

Ú

h/2

º+

∂h 2 ∂q E 12 Ê z e oy – z --------x + z --------yˆ dz Ë ∂y ∂y ¯ – h/2

Ú

h/2

∂q ∂q ∂ M y = C 11 --------y + C 12 ¥ – --------x + -----∂x ∂y ∂x 6

∂ E 11 h x z dz + -----y ∂ – h/2

Ú

h/2

Ú

h/2

– h/2

E 12 h y z dz

The simplifications are due to the antisymmetry of the integrated functions (midplane symmetry).

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 324 Monday, November 18, 2002 12:33 PM

In the last two terms there appear the nonzero integrals of even functions. If one neglects the contribution of the rates of variation along the x and y direction, respectively, of these terms, the previous equation 7 is reduced to

∂q ∂q M y = C 11 --------y + C 12 ¥ – --------x ∂x ∂y Moment resultant M x = – –Mx =

Ú

h/2

– h/2

s y z dz :

∂h 2 ∂q E 12 Ê z e ox + z --------y + z ---------xˆ dzº Ë ∂x ∂x ¯ – h/2 h/2

Ú

Ú

º+

h/2

– h/2

∂h 2 ∂q E 22 Ê z e oy – z --------x + z --------yˆ dz Ë ∂y ∂y ¯

which is reduced to:

∂q ∂q ∂ – M x = C 12 --------y + C 22 ¥ – --------x + -----∂x ∂y ∂x

∂ E 12 h x z dz + -----∂y – h/2

Ú

h/2

Ú

h/2

– h/2

E 22 h y z dz 7

and in neglecting the contribution of the last two terms :

∂q ∂q – M x = C 12 --------y + C 22 ¥ – --------x ∂x ∂y Moment resultant M xy = – – M xy =

Ú

h/2

– h/2

t xy z dz

∂h ∂h ∂q 2 ∂q E 33 Ê z g oxy + z Ê --------y – --------xˆ + z ---------x + z --------yˆ dz Ë Ë ¯ ∂ y ∂x ¯ ∂ y ∂ x – h/2

Ú

h/2

which is reduced to:

∂q ∂q ∂ – M xy = C 33 Ê --------y – --------xˆ + -----Ë ∂y ∂x ¯ ∂y

∂ E 33 h x z dz + -----∂x – h/2

Ú

h/2

Ú

h/2

– h/2

E 33 h y z dz

and in neglecting the contribution of the variations of the differences hx 7 and hy :

∂q ∂q – M xy = C 33 Ê --------y – --------xˆ Ë ∂y ∂x ¯ 7

The existence of such approximation does not appear if one neglects a priori the increments hx, hy, hz in Equation 17.3.

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 325 Monday, November 18, 2002 12:33 PM

In summary, one finds again a form analogous to Equation 12.16 (with C13 = C23 = 0 due to the orientation of the plies (see Hypotheses in Section 17.1.3): ∂q

Ï --------y ¸ ∂x Ô Ô Ô Ô ∂q x – -------Ì ˝ ∂y Ô Ô ∂q Ô Ô Ê ∂q -y – --------xˆ Ó Ë ------∂y ∂x ¯ ˛

C 11 C 12 0 Ï My ¸ Ô Ô Ô Ô Ì – M x ˝ = C 21 C 22 0 Ô Ô Ô –M Ô 0 0 C 33 Ó xy ˛

(17.8)

Or in the inverse form, by reusing the notations of Section 12.1.6. ∂q

Ï --------y ¸ ∂x Ô Ô Ô ∂q x Ô Ì – -------˝ = ∂y Ô Ô ∂q Ô Ô Ê ∂q -y – --------xˆ Ó Ë ------∂y ∂x ¯ ˛

1 --------EI 11

1 --------EI 12

1 --------EI 21

1 --------EI 22

0

0

0 Ï My ¸ Ô Ô Ô Ô 0 Ì –Mx ˝ Ô Ô 1 -------- Ô – M xy Ô C Ó ˛

(17.9)

33

17.4.3 Transverse Shear Equation We define here new stress resultants starting from the transverse shear stresses, which are denoted as transverse shear stress resultants: Shear stress resultant Q x = Ú –h/2 t xz dz Using Equations 17.2 and 17.6: h/2

Qx =

∂w ∂h ∂h G xz Ê ---------0 + q y + ---------x + ---------zˆ dz Ë ∂x ∂z ∂x ¯ – h/2 h/2

Ú

in setting · hG xzÒ =

Ú

h/2

G xz dz

– h/2

yields

∂w Q x = · hG xzÒ Ê ---------0 + q yˆ + Ë ∂x ¯

dh G xz ---------x dz ∂z – h/2

Ú

h/2

(17.10)

where one can note the presence of the integral of an even function: Shear stress resultant Q y = Ú –h/2 t yz dz h/2

Qy =

© 2003 by CRC Press LLC

∂w ∂h ∂h G yz Ê ---------0 – q x + --------y + ---------zˆ dz Ë ∂y ∂z ∂y ¯ – h/2

Ú

h/2

TX846_Frame_C17 Page 326 Monday, November 18, 2002 12:33 PM

in setting · hG yzÒ =

Ú

h/2

G yz dz

– h/2

yields

∂h G yz --------y dz ∂z – h/2

∂w Q y = · hG yzÒ Ê ---------0 – q xˆ + Ë ∂y ¯

Ú

h/2

(17.11)

17.5 EQUILIBRIUM EQUATIONS These are the same for the plates in general, no matter what are their compositions and are, therefore, classical. One recalls here only the equilibrium equations for bending.

17.5.1 Transverse Equilibrium ∂t

∂t

∂s

zx zy - + --------- + ---------z + f z = 0 local equilibrium relation --------∂x ∂y ∂z In integrating across the thickness, one reveals the transverse shear stresses Qx and Qy:

∂ Qx ∂ Qy --------- + --------- + [ s z ] h/2 – h/2 + ∂x ∂y

Ú

h/2

– h/2

f z dz = 0

Then denoted by pz, the transverse stress density:

∂ Qx ∂ Qy --------- + --------- + p z = 0 ∂x ∂y

17.5.2 Equilibrium in Bending ∂s

∂t

∂t

xy xz -x + --------- + --------- + fx = 0 local equilibrium relation -------∂x ∂y ∂z After multiplication with z, the integration over the thickness leads to

∂ M ∂ M xy ----------y – -----------+ ∂x ∂y

Ú

h/2

– h/2

∂ ------ ( z t ) – t xz dz + ∂ z xz

∂ M ∂ M xy h/2 ----------y – ----------- – Q x + [ z t xz ] –h/2 + ∂x ∂y

Ú

h/2

– h/2

Ú

h/2

– h/2

z f x dz = 0

zf x dz = 0

In neglecting the moment density:

∂ M ∂ M xy ----------y – ----------- – Qx = 0 ∂x ∂y ∂t

∂s

(17.12)

∂t

yx yz - + ---------y + --------- + fy = 0 local equilibrium relation --------∂x ∂y ∂z An analogous calculation leads to

∂ M xy ∂ M x ------------ + ---------- + Q y = 0 ∂x ∂y

© 2003 by CRC Press LLC

(17.13)

TX846_Frame_C17 Page 327 Monday, November 18, 2002 12:33 PM

17.6 TECHNICAL FORMULATION FOR BENDING One can note in the preceding that midplane symmetry always leads to the decoupling of the membrane behavior from the bending behavior. As a consequence, in what follows, one will consider uniquely the stresses due to bending (one will make Nx = Ny = Txy = 0). In addition to the hypotheses in Section 17.1.3, one will neglect, for the calculation of the stresses, the variations of increments {hx, hy, hz} as 8 functions of x and y.

17.6.1 Plane Stresses Due to Bending One can write successively for a ply number k: k

k

s x = E 11 e x + E 12 e y Then with [17.6]:

∂q ∂h ∂q ∂h k k s x = E 11 ÊË e ox + z --------y + ---------xˆ¯ + E 12 ÊË e oy – z --------x + --------yˆ¯ ∂x ∂x ∂y ∂y and with [17.7] and [17.9]: N x n yx M M k s x = E 11 -------- – --------N y + z Ê --------y- – --------x-ˆ º Ë hE x hE y EI 11 EI 12¯

n xy Ny M M k º + E 12 - N x + -------– -------+ z Ê --------y- – --------x-ˆ Ë hE x hE y EI 12 EI 22¯ k

k

E 11 E 12 ˆ - + --------- M y + z s x = z ÊË -------EI 11 EI 12¯ k

k

k

E 11 E 12 ˆ Ê -------- + --------- ¥ – M x Ë EI 12 EI 22¯

(17.14)

k

s y = E 12 e x + E 22 e y An analogous calculation leads to k

k

k

k

E 12 E 22 ˆ E 12 E 22 ˆ - + --------- M y + z Ê -------- + --------- ¥ – M x s y = z ÊË -------¯ Ë EI 11 EI 12 EI 12 EI 22¯ k

(17.15)

t xy = E 33 g xy = G xy g xy Then with Equation 17.6: k

∂h ∂h ∂q ∂q k t xy = G xy ÊË g oxy + z ÊË --------y – --------xˆ¯ + ---------x + --------yˆ¯ ∂y ∂x ∂y ∂x 8

This simplification constitutes here the extension to plates of the generalized Navier-Bernoulli principle for beams (see Section 15.1.5).

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 328 Monday, November 18, 2002 12:33 PM

and with Equations 17.7 and 17.9 and Txy = 0: k

G xy -M t xy = – z -------C 33 xy

(17.16)

17.6.2 Transverse Shear Stresses in Bending

k

t xz = E 44 g xz = G xz g xz from [ 17.2 ] k

and with Equation 17.6 and neglecting the variation ∂hz /∂ x: k ∂w k ∂h t xz = G xz ÊË ---------0 + q yˆ¯ + G xz ---------x ∂x ∂z

k

(17.17)

t yz = E 55 g yz = G yz g yz k

which leads in an analogous manner to k ∂w k ∂h t yz = G yz ÊË ---------0 – q xˆ¯ + G yz --------y ∂z ∂y

(17.18)

Knowledge of the transverse shears, then, requires the previous calculation of the warping increments hx and hy.

17.6.3 Characterization of the Bending, Warping Increments hx and hy Warping hx (x, y, z): Starting from the first equation of local equilibrium:

∂t xz ∂s ∂t xy ---------- = – ---------x – --------∂z ∂x ∂y Then with Equations 17.14, 17.16, and 17.17: G xy ∂ M xy E 11 E 12 ˆ ∂ M x E 11 E 12 ˆ ∂ M y k ∂ hx - + --------- ---------- + z Ê -------- + --------- ---------- + z ------- -----------= – z Ê -------G xz ----------2 Ë ¯ Ë ¯ C 33 ∂ y ∂z EI 11 EI 12 ∂ x EI 12 EI 22 ∂ x 2

k

k

k

k

k

Taking into account the equilibrium Equation 17.12, one can rewrite E 11 E 12 ˆ E 11 E 12 ˆ ∂ M x º k ∂ hx - + --------- Q x + z Ê -------- + --------- ---------= – z Ê -------G xz ----------2 Ë ¯ Ë ∂z EI 11 EI 12 EI 12 EI 22¯ ∂ x 2

k

k

k

Ê G xy E k11 E k12 ˆ ∂ M xy º + z Á -------- – --------- – ---------˜ -----------Ë C 33 EI 11 EI 12¯ ∂ y

k

k

(17.19)

Warping hy (x, y, z): In an analogous manner, starting from the second equation of the local equilibrium:

∂t yz ∂s ∂t yx --------- = – --------y – --------∂z ∂y ∂x

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 329 Monday, November 18, 2002 12:33 PM

Then with Equations 17.15, 17.16, and 17.18: 2 Ê E k12 E k22 ˆ ∂ M y Ê E k12 E k22 ˆ ∂ M x k ∂ hy ----------------------= – + z z + G yz ---------Á ˜ Á --------- + ---------˜ ---------- º 2 ∂z Ë EI 11 EI 12¯ ∂ y Ë EI 12 EI 22¯ ∂ y xy ∂ M xy º + zG ------- -----------C 33 ∂ x k

Taking into account the equilibrium Equation 17.13, one can rewrite E 12 E 22 ˆ ∂ M y E 12 E 22 ˆ º k ∂ hx - = – z Ê -------- + --------- ---------- – z Ê -------- + --------- Q y G yz ---------2 Ë ¯ Ë ∂z EI 11 EI 12 ∂ y EI 12 EI 22¯ 2

k

k

k

k

Ê G xy E k12 E k22 ˆ ∂ M xy - – --------- – ---------˜ -----------º + z Á ------Ë C 33 EI 12 EI 22¯ ∂ x k

(17.20)

17.6.3.1 Particular Cases Equations 17.19 and 17.20 simplify in the following particular cases: Homogeneous orthotropic plate: Then from relations 17.2, 17.8, and 17.9: k

k

E 11 = E 11 ; E 12 = E 12 ; E

k 22

= E 22

C 22 12 E 22 1 - ¥ -----3- ; --------- = ----------------------------- = -----------------------------2 2 C 11 C 22 – C 12 EI 11 E 11 E 22 – E 12 h E 11 1 12 --------- = ----------------------------- ¥ -----32 EI 22 E 11 E 22 – E 12 h C 12 – E 12 1 12 --------- = – ---------------------------- = ---------------------------- ¥ -----3- ; 2 2 C 11 C 22 – C 12 EI 12 E 11 E 22 – E 12 h

1 1 12 ------- = -------- ¥ -----3C 33 G xy h

Then Equation 17.19 and Equation 17.20 reduce to

∂ hx 12 G xz ----------= – z ¥ -----3- ¥ Q x 2 h ∂z 2

∂ h 12 G yz ----------2-y = – z ¥ -----3- ¥ Q y h ∂z 2

(17.21)

Cylindrical bending about x or y axis of a multilayered plate characterized by identical Poisson coefficient in the x,y plane of the plate as: "k: n xy = n xy ; n yx = n yx k

© 2003 by CRC Press LLC

k

TX846_Frame_C17 Page 330 Monday, November 18, 2002 12:33 PM

9

Then for any two plies k and m, one has (see Equations 17.2) : k

k

k

E 12 E 22 E 11 ------- = ------- = ------- = a km m m m E 11 E 12 E 22 then: C ij =

Ú

n

h/2

k ij

– h/2

th

k=I 1

= E ij

Ú

z1

z0

1Ï C ij = E ij Ì Ó

Ú

2

z dz + E ij 2

z1

z0

Ú

st

z2

ply

Ï k Ì E ij Ó

¸ 2 z dz ˝ z k-1 ˛

Ú

zk

z dz º + E ij n

2

z1

z dz + a 12 2

ply

Â

E z dz = 2

Ú

z2

Ú

zn

2

z dz

z n-1

z dz º + a n-1, n 2

z1

3 ¸ 1 ah 2 z dz ˝ = E ij ¥ --------12 z n-1 ˛

Ú

zn

where a is a nondimensional coefficient. One then has 1

C 22 12 EI 22 1 --------- = ---------------------------- = ----------------------------------¥ ---------3 ; 2 1 1 1 2 C 11 C 22 – C 12 a h EI 11 E 11 E 22 – ( E 12 ) 1

12 EI 11 1 ---------- = ----------------------------------¥ ---------3 1 1 1 2 a h EI 22 E 11 E 22 – ( E 12 ) 1

12 EI 12 1 ---------- = ----------------------------------¥ ---------3 1 1 1 2 EI 12 E 11 E 22 – ( E 12 ) a h In [17.19], we have the simplification : k

k

1

k

k

1

- E 11 E 12 + E 12 E 11 12 E 11 E 12 - ¥ ---------3 -------- + --------- = --------------------------------------------1 1 1 2 ah EI 12 EI 22 E 11 E 22 – ( E 12 ) 1

1

1

1

a k1 ( – E 11 E 12 + E 12 E 11 ) 12 - ¥ ---------3 = 0 = -----------------------------------------------------1 1 1 2 ah E 11 E 22 – ( E 12 ) as well as an analogous simplification in Equation 17.20: k

k

E 12 E 22 -------- + --------- = 0 EI 11 EI 12 10

Equations 17.19 and 17.20 simplify as follows : 9 10

Recall the relation nyx Ex = nxy Ey (see Equation 9.4). In the first case in Equation 17.22, Mxy = Qy = 0 and Equation 17.20 disappears. In the second case, Mxy = Qy = 0 and Equation 17.19 disappears.

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 331 Monday, November 18, 2002 12:33 PM

1. cylindrical bending about y axis E 11 E 12 ˆ k ∂ hx - + --------- Q x = – z Ê -------G xz ----------2 Ë ∂z EI 11 EI 12¯ 2. cylindrical bending about x axis 2

k

k

(17.22)

E 22 E 12 ˆ k ∂ h - + --------- Q y G yz ----------2-y = – z Ê -------Ë ∂z EI 22 EI 12¯ 2

k

k

The case of a multilayer plate such that for any two plies k and m one 11 has in the plane of the plate : k

E ij -----m- = a km E ij

"i and j = 1, 2, 3

Then Equations 17.19 and 17.20 reduce to

∂ hx E 11 E 12 ˆ - + --------- Q x G ----------= – z Ê -------2 Ë ∂z EI 11 EI 12¯ 2

k

k

k xz

(17.23)

∂ h E 22 E 12 ˆ - + --------- Q y G ----------2-y = – z Ê -------Ë ∂z EI 22 EI 12¯ 2

k

k

k yz

The preceding particular cases constitute a severe restriction among the variety of practical laminations. Nevertheless we will conserve in the following the simplified forms of Equations 17.21, 17.22, and 17.23 because they well show the direct connection between the warpings hx and hy and the transverse shear forces Qx and Qy, respectively.

17.6.3.2 Consequences Setting hx and hy in the forms: ¸ Qx ¥ g(z ) Ô h x ( x, y, z ) = ----------------· hG xzÒ Ô ˝ Qy - ¥ p ( z ) ÔÔ h y ( x, y, z ) = ---------------· hG yzÒ ˛

(17.24)

The constitutive Equations 17.10 and 17.11 are written as: h/2 ∂w Qx dg Q x = · hG xzÒ Ê ---------0 + q yˆ + ----------------G ------ dz Ë ∂x ¯ · hG xzÒ –h/2 xz dz

Ú

11

E

k

G

k

- = a km . Such a limiting case is rare in practice, because it imposes in particular: ----33m- = -----xy m E 33

© 2003 by CRC Press LLC

G xy

TX846_Frame_C17 Page 332 Monday, November 18, 2002 12:33 PM

then by setting : 1 k x = Ê 1 – ----------------Ë · hG xzÒ

h/2

dg G xz ------ dzˆ d z ¯ – h/2

Ú

· hG xzÒ Ê ∂ w 0 --------- + q yˆ Q x = ----------------¯ kx Ë ∂ x Qy ∂w Q y = · hG yzÒ Ê ---------0 – q xˆ + ---------------Ë ∂y ¯ · hG yzÒ then by setting :

Ú

h/2

– h/2

1 k y = Ê 1 – ----------------Ë · hG yzÒ

Ú

(17.25)

dp G yz ------ dz dz

h/2

– h/2

dp G yz ------ dzˆ dz ¯

· hG yzÒ Ê ∂ w 0 - --------- – q xˆ Q y = ---------------¯ ky Ë ∂ y

(17.26)

There appear two transverse shear coefficients kx and ky which require the knowledge of the functions g(z) and p(z) for their calculations.

17.6.4 Warping Functions Boundary conditions: We have assumed that the upper and lower faces of the plate were free of any shear. Then the transverse shear in Equations 17.17 and 17.18 leads to Q x dg ∂ w0 ˆ + ----------------------- = 0 for z = ±h /2 Ê --------Ë ∂ y- + qy¯ · hGxzÒ dz

then with Equation 17.25: dg k x + ------ = 0 dz

for

z = ±h /2

Q y dp ∂ w0 ˆ – ----------------- ------ = 0 for z = ±h /2 Ê --------Ë ∂ y- – qy¯ · hGyzÒ dz

then with [17.26]: dp k y + ------ = 0 dz

for

z = ±h /2

Continuity at the interfaces: The continuity of the transverse shear at the interfaces between layers results from the assumed perfect bonding between two plies (see Paragraph 15.1.2). One then has at the interface between two consecutive plies k and k + 1:

t xz = t xz ; t yz = t yz k

© 2003 by CRC Press LLC

k+1

k

k+1

TX846_Frame_C17 Page 333 Monday, November 18, 2002 12:33 PM

then with Equations 17.17, 17.18 and Equations 17.25, 17.26: dg dg k+1ˆ k k+1 G xz Ê k x + --------kˆ = G xz Ê k x + -----------Ë ¯ Ë dz dz ¯ dp dp k+1ˆ k k+1 G yz Ê k y + --------kˆ = G yz Ê k y + -----------Ë ¯ Ë dz dz ¯ Formulation of the warping functions: Let us substitute to g(z) and p(z) the functions g0(z) and p0(z) such that: g0 ( z ) = g ( z ) + z ¥ k x ; p0 ( z ) = p ( z ) + z ¥ k y g0(z) and p0(z) are called the warping functions. Then the boundary conditions and the interface conditions simplify, and Equations 17.23 allow one to formulate the problems that permit a simple calculation of warping functions g0(z) and p0(z). One obtains · hG xzÒ Ê E 11 E 12 ˆ d g0 Ï ------------------ + --------k Ô dz 2 = – z ¥ ----------------G xz Ë EI 11 EI 12¯ Ô Ô dg Ì --------0 = 0 for z = ±h /2 Ô dz Ô k+1 dg 0k+1 0k Ô G k dg - for z = z k = G xz -------------Ó xz ---------dz dz

(17.27)

p0 · hG yzÒ Ê E 22 E 12 ˆ Ïd - --------- + --------= – z ¥ ---------------2 k Ô ---------G yz Ë EI 22 EI 12¯ Ô dz Ô dp Ì --------0 = 0 for z = ±h /2 Ô dz Ô dp 0k k+1 dp 0k+1 Ô G k ---------- for z = z k Ó yz dz- = G yz -------------dz

(17.28)

2

k

2

k

k

k

The antisymmetric functions g0 and p0 are then defined in a unique manner.

17.6.5 Consequences Form of the transverse shear stresses: Equations 17.17 and 17.18 then take the simple forms: k

G xz dg 0 --------; t xz = Q x ¥ ----------------· hG xzÒ dz

© 2003 by CRC Press LLC

k

G yz dp 0 - -------t yz = Q y ¥ ---------------· hG yzÒ dz

(17.29)

TX846_Frame_C17 Page 334 Monday, November 18, 2002 12:33 PM

Transverse shear coefficients: One obtains these coefficients from the Equation 17.5: h/2 E 11 E 12 ˆ Ú –h/2 Ê --------+ --------h z dz = 0 Ë EI11 EI12¯ x

here is : Qx E 11 E 12 ˆ Ê -------- + --------- ¥ ----------------( g 0 – k xz ) z dz = 0 Ë ¯ · hG – h/2 EI 11 xzÒ EI 12 h/2

Ú

noting that : 2

C 11 C 12 – C 12 C 11 C 12 E 11 E 12 ˆ 2 Ê -------- + --------- z dz = -------- + --------- = ---------------------------- = 1. 2 Ë – h/2 EI 11 C 11 C 12 – C 12 EI 12¯ EI 11 EI 12

Ú

h/2

One obtains : kx =

h/2

E 11 E 12 ˆ Ê -------- + --------- g 0 z dz Ë – h/2 EI EI ¯

Ú

11

(17.30)

12

E 22 E 12 - + -------- ) h y z dz = 0 Ú –h/2 ( -------h/2

EI 22

EI 12

here is : Qy E ˆ Ê -E--22 - ( p – k yz ) z dz = 0 -- + ---12 -- ¥ ---------------Ë ¯ · hG yzÒ 0 – h/2 EI 22 EI 12

Ú

h/2

leading to: ky =

h/2

E 22 E 12 ˆ Ê -------- + --------- p 0 z dz Ë – h/2 EI 22 EI 12¯

Ú

(17.31)

In summary, in the absence of body forces (inertia forces, example), the bending behavior uncoupled from the membrane behavior of a thick laminated plate can be simplified in a few particular cases noted below. The characteristic relations are summarized in the following table.

Bending Behavior (no in-plane stress resultants) or or

homogeneous orthotropic plate/orthotropic axes : x, y, z Laminated plate/midplane symmetry/orthotropic axes of plies: x,y,z/same Poisson ratios vxy and vyx for all plies/cylindrical bending about x or y axis. Laminated plate/midplane symmetry/orthotropic axes of plies: x,y,z/elastic constants are proportional from one ply to another Equilibrium relation: ∂Q ∂Q ∂ M xy ∂ M x ∂ M ∂ M xy ----------x + ----------y + p z = 0; ----------y – ----------- + ---------- + Q y = 0 - – Q x = 0; ----------∂x ∂y ∂x ∂y ∂x ∂y

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 335 Monday, November 18, 2002 12:33 PM

Constitutive relations: Ï My ¸ C 11 C 12 0 0 0 Ô Ô Ô Ô Ô Ô Ô –Mx Ô C 21 C 22 0 0 0 Ô Ô Ô Ô Ì – M xy ˝ = 0 0 C 33 0 0 Ô Ô Ô Ô · hG xzÒ Ô Qx Ô 0 0 0 0 -----------------kx Ô Ô Ô Ô · hG yzÒ Ô Q Ô -----------------0 0 0 0 y ky Ó ˛

∂q

Ï --------y ¸ Ô ∂x Ô Ô ∂q x Ô Ô – -------Ô ∂y Ô Ô Ô ∂q y ∂q x Ô – -------- ˝ Ì -------Ô ∂y ∂x Ô Ô ∂ w0 Ô - + qy Ô Ô --------∂x Ô Ô Ô ∂ w0 Ô --------– q x ˛ Ó ∂y

with [C]

–1

1 = ----EI

Stresses stresses within the ply :

sx: cf. [17.14];

sy: cf. [17.15];

txy: cf. [17.16] (17.32)

transverse shear stresses k

k

G xz dg 0 - --------- ; t xz = Q x ----------------· hG xzÒ dz

G yz dh 0 - --------t yz = Q y ----------------· hG yzÒ dz

Warping functions g0 (z) is the solution of the problem: Ï 2 k k g0 · hG xzÒ Ê E 11 E 12 ˆ Ôd - Á --------- + ---------˜ k Ô ----------2- = – z ----------------G xz Ë EI 11 EI 12¯ Ô dz Ô dg 0 Ì -------Ô dz- = 0 for z = ± h/2 Ô Ô k dg 0k dg 0k+1 - = G k+1 for z = z k Ô G xz ---------xz ---------------dz dz Ó

p0 (z) is the solution of the problem:

Ï 2 k k p0 · hG yzÒ Ê E 22 E 12 ˆ Ôd -----------------------------------------˜ = – z + Á k 2 Ô G yz Ë EI 22 EI 12¯ Ô dz Ô dp 0 Ì -------Ô dz- = 0 for z = ± h/2 Ô Ô k dp 0k dp 0k+1 - = G k+1 for z = z k Ô G yz ----------yz ---------------dz dz Ó

Transverse shear coefficients kx and ky: They are given by the formula:

kx =

h/2

E 11 E 12 ˆ Ê -------- + --------- g 0 z dz; Ë – h/2 EI 11 EI 12¯

Ú

© 2003 by CRC Press LLC

ky =

h/2

E 22 E 12 ˆ Ê -------- + --------- p 0 z dz Ë – h/2 EI 22 EI 12¯

Ú

TX846_Frame_C17 Page 336 Monday, November 18, 2002 12:33 PM

17.6.6 Interpretation in Terms of Energy We will limit ourselves to the surface energy density due to transverse shear stresses as: 1 W t = --2

h/2

1 ( t xz g xz + t yz g yz ) dz = --2 – h/2

Ú

t xz t yz ˆ Ê ------- + -------- dz Ë G G yz¯ – h/2 xz

Ú

2

h/2

2

Substituting Equation 17.29, one obtains 1 W t = --2

G xz Ê dg 0ˆ 2 1 2 -2 -------- dz + --Q x ------------------Ë ¯ d z 2 – h/2 · hG xzÒ

Ú

h/2

G yz Ê dp 0ˆ 2 2 -------- dz Q y ------------------2 – h/2 · hG yzÒ Ë dz ¯

Ú

h/2

The first integral can be rewritten as: 2

1 Qx --- --------------------2 2 · hG xzÒ

2 dg d d g0 G xz ------ Ê g 0 --------0ˆ – g 0 ---------dz 2 dz Ë dz ¯ – h/2 dz

Ú

h/2

or, taking into account Equation 17.27: dg 1 Qx Ï --- --------------------2 Ì G xz g 0 --------0 dz 2 · hG xzÒ Ó 2

h/2 – h/2

+ · hG xzÒ

¸ E 11 E 12 ˆ Ê -------- + --------- g 0 z dz ˝ Ë ¯ – h/2 EI 11 EI 12 ˛

Ú

h/2

where one recognizes Equation 17.30 of the transverse shear coefficient kx, The first integral is reduced to 2

Qx 1 --- k x ----------------2 · hG xzÒ Following a similar approach for the second integral and taking into account Equations 17.28 and 17.31 for the transverse shear coefficient ky, the surface energy due to transverse shear takes the form: 2

2

Qx Qy 1 1 + --- k ---------------W t = --- k x ----------------2 · hG xzÒ 2 y · hG yzÒ

17.7 EXAMPLES Examples for plates in bending are shown in details in Part Four of this book, in Chapter 18, “Applications.” We give here a few useful elements to treat these examples.

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 337 Monday, November 18, 2002 12:33 PM

17.7.1 Homogeneous Orthotropic Plate Warping functions: Equation 17.27 becomes k

E 11 = E

k

11

; E 12 = E 12 ; E

k 22

12

= E 22 ; G xz = G xz k

2 2 Ê E 11 E 22 12 d g0 12ˆ E 12 12 ----------------------------- -----3-˜ = – z ¥ -----2----------2 = – zh Á --------------------------------– 3 2 2 dz h Ë E 11 E 22 – E 12 h E 11 E 22 – E 12 h ¯

dg --------0 = 0 for z = ±h /2 dz then

12

2 2 dg 0 3 z 3 4z -------- = --- Ê 1 – 4 -----2ˆ ; g 0 = --- z Ê 1 – --- -----2ˆ dz 2Ë 2 Ë 3h ¯ h¯

Transverse shear stresses and shear coefficients: One deduces from Equation 17.32: 2 Q 3 z t xz = ------x ¥ --- ÊË 1 – 4 -----2ˆ¯ h 2 h

12 k x = -----3h

h/2

(17.33)

2

3Ê 4z --- 1 – --- -----2ˆ z 2 dz Ë 3h ¯ – h/2 2

Ú

6 k x = --5

(17.34)

In an analogous manner starting from Equation 17.28: p0 ( z ) = g0 ( z ) then: 2 Q 3 z t yz = ------y ¥ --- ÊË 1 – 4 -----2ˆ¯ h 2 h

(17.35)

6 k y = --5

(17.36)

Remark: In Application 18.3.7 (Chapter 18), one treats the case of a thick homogeneous orthotropic plate in cylindrical bending about the y axis. The plate supports a uniformly distributed load. One can consider there the strong influence of transverse shear in bending. Two characteristics of the plate then apply directly on the deflection:

12

g0 is, as g, antisymmetric in z (see Equation 17.4).

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 338 Monday, November 18, 2002 12:33 PM

Figure 17.3 Sandwich Plate

The relative thickness h/a, where a is the length of the bent side of the plate The ratio Ex/Gxz (for certain combinations of fiber/matrix, this ratio becomes large compared with unity; for example, for unidirectional)

17.7.2 Sandwich Plate The plate consists of two orthotropic materials: Material (1) for the skins Material (2) for the core (see Figure 17.3) Assuming the proportionality of elastic coefficients for the two materials leads to (see Section 17.6.3): then C ij =

Ú

h/2

➀

E ij z dz = E ij 2

– h/2

3

Ú

– H 2 /2

– H 1 /2

3

➁

z dz + E ij 2

Ú

H 2 /2

2

➀

z dz + E ij

– H 2 /2

3

➀ H 1 – H 2ˆ ➁ H - + E ij -------2 C ij = E ij Ê ------------------Ë 12 ¯ 12

H1 – H2 H aH aH ➀ - + a 12 -------2 C ij = E ij ¥ -----------1 with -----------1 = ------------------12 12 12 12 3

3

3

3

3

one deduces from there: ➀

C 11 12 E 11 1 - ¥ ----------3 --------- = ----------------------------- = -----------------------------------2 ➀ ➀ ➀ 2 C 11 C 22 – C 12 EI 11 E 11 E 22 – ( E 12 ) a H 1 ➀

– C 12 12 1 – E 12 - ¥ ----------3 --------- = ----------------------------- = ----------------------------------2 ➀ ➀ ➀ 2 C 11 C 22 – C 12 EI 12 E 11 E 22 – ( E 12 ) a H 1

© 2003 by CRC Press LLC

Ú

H 1 /2 H 2 /2

2

z dz

TX846_Frame_C17 Page 339 Monday, November 18, 2002 12:33 PM

17.7.2.1 Warping Functions 13

From the above one can write in Equation 17.27 : k

k

k

k

Ex E 12 E 11 E 12 ˆ Ê --------3 - + --------- = ------➀x- ¥ ----------3 = ---------------------------------------------3 3 Ë EI 11 EI 12¯ ( H – H2 ) ➀ ➁ H2 1 E x a H1 - + E x --E x -----------------12 12 In addition : ➀

➀

· hG xzÒ = G xz ( H 1 – H 2 ) + G xz H 2 Equation 17.27 then can be written as: ➀

➁

Ex G xz ( H 1 – H 2 ) + G xz H 2 g0 Ïd - ¥ 12 ----------------------------------------------------= – z ¥ ------k ➀ 3 3 ➁ 3 2 Ô ---------E dz G ( H – H ) + E H xz x 1 2 x 2 Ô Ô dg Ì --------0 = 0 for z = ± H 1 /2 Ô dz Ô Ô G dg -0 continuous for z = ±H 2 /2 Ó xz ------dz 2

k

In Equation 17.28, one obtains an analogous formulation. In effect, one can write k

k

k

k

Ey E 12 E 22 E 12 ˆ Ê -------- + --------- = -----➀-y ¥ ---------3 = --------------------------------------------3 3 3 Ë EI 22 EI 12¯ ( H – H2 ) ➀ ➁ H2 1 Ey a h --+ E E y -----------------y 12 12 The problem [17.28] is then written as: ➀

➁

E G yz ( H 1 – H 2 ) + G yz H 2 p0 Ïd = – z ¥ -------ky- ¥ 12 ----------------------------------------------------➀ 3 3 ➁ 3 2 Ô ---------dz G yz Ey ( H1 – H2 ) + Ey H2 Ô Ô dp Ì --------0 = 0 z = ±H 1 /2 Ô dz Ô dp 0 Ô G -------Ó yz dz continuous for z = ±H 2 /2 2

k

Remark: These problems are identical to that which allows the calculation of the warping function for the bending of a sandwich beam, and one can consider it in Chapter 18, application 18.3.5. One can then carry out the same steps of calculation. The results obtained are shown below. 13

See Equations 17.2.

© 2003 by CRC Press LLC

TX846_Frame_C17 Page 340 Monday, November 18, 2002 12:33 PM

17.7.2.2 Transverse Shear Stresses Stress txz: E x Ê -----2- – z2ˆ + E x Ê -----1- – -------2 ˆ Ë4 ¯ Ë4 4¯ = Q x ¥ 6 ¥ -----------------------------------------------------------➀ 3 3 ➁ 3 Ex ( H1 – H2 ) + Ex H2 ➁

H H – ------2 £ z £ ------2 ; t xz 2 2

2

H

➀

H

2

H

2

(17.37)

2

➀ H1 x 4

E ( ---- – z ) H H2 ------ £ z £ ------1 : t xz = Q x ¥ 6 ¥ -------------------------------------------------➀ 3 3 ➁ 3 2 2 E x ( H1 – H2 ) + Ex H2 2

Stress tyz: ➁ H

2

➀ H

2

H

2

E y ( ---4-2 – z2 ) + E y ( ---4-1 – ---4-2 ) H2 H2 – ------ £ z £ ------ ; t yz = Q y ¥ 6 ¥ ---------------------------------------------------------➀ 3 3 ➁ 3 2 2 Ey ( H1 – H2 ) + Ey H2 2

➀ H1 y 4

(17.38)

E ( ---- – z ) H H ------2 £ z £ ------1 ; t yz = Q y ¥ 6 ¥ -------------------------------------------------➀ 3 3 ➁ 3 2 2 E y ( H1 – H2 ) + Ey H2 2

17.7.2.3 Transverse Shear Coefficients ➁

Ï Ex 3 ➀ 2 Ê 4 ➁ ax -H 2 E x H 1 + --- E x – E ➀x ˆ H 22 º - ------k x = --------------------------------------------------------➀ 3 3 ➁ 3 Ì ➁ Ë5 ¯ 8 [ E x ( H 1 – H 2 ) + E x H 2 ] Ó G xz ➀ 2

➀

¸ Ex ) Ê 4 5 H2 3b x E x ( H 1 – H 2 ) … + (------------ --- H + ------ – H 21 H 32ˆ ˝ + ------------------------------------------------➀ Ë5 1 ➀ 3 3 ➁ 3 ¯ 5 G xz ˛ Ex ( H1 – H2 ) + Ex H2 5

➀

with

2

2

➁

G xz ( H 1 – H 2 ) + G xz H 2 a x = 12 ¥ ----------------------------------------------------➀ 3 3 ➁ 3 Ex ( H1 – H2 ) + Ex H2

(17.39)

➀ 2 ➀ ➁ ➀ ˆ a Ex Ï H2 2 Ex ˆ ¸ 2 Ê G xz 2 G xz Ê ----------------˜ H 1 – ------– 1 b x = -----x- H 2 ------– + H Á Á ˜ Ì 1 2 ➁ ➁ 16 G ➀xz Ó 3 3 E ➀x ¯ ˝˛ G xz Ë Ë G xz ¯

ky is given by an expression formally identical to that in which the index x is replaced by y. In Application 18.3.8 we treat the case of a rectangular sandwich plate in cylindrical bending, clamped on one side and subjected to a uniform linear force on another. The plate is free on the other sides. One shows the influence of transverse shear on the deflection. This influence increases when: The mechanical characteristics (moduli) of the core are weaker than those of the skins. The relative thickness of the core is important (thin skins). The relative thickness of the plate is large (thick plate).

© 2003 by CRC Press LLC

TX846_Frame_C18a Page 341 Monday, November 18, 2002 12:40 PM

PART IV APPLICATIONS We have grouped in this last part of the book exercises and examples for applications. These have various objectives and different degrees of difficulties. Leaving aside (except for special cases) the cases that are too academic, we will concern ourselves with applications of concrete nature, with an emphasis on the numerical aspect of the results. A few of these applications should be used as validation tests for numerical models.

© 2003 by CRC Press LLC

TX846_Frame_C18a Page 343 Monday, November 18, 2002 12:40 PM

18 APPLICATIONS 18.1 LEVEL 1 18.1.1 Simply Supported Sandwich Beam Problem Statement: 1. The following figure represents a beam made of duralumin that is supported at two points. It is subjected to a transverse load of F = 50 daN. Calculate the deflection—denoted as D —of the beam under the action of the force F.

2. We separate the beam of duralumin into two parts with equal thickness ep = 2.5 mm, by imaginarily cutting the beam at its midplane. Each half is bonded to a parallel pipe made of polyurethane foam, making the skins of a sandwich beam having essentially the same mass as the initial beam (in neglecting the mass of the foam and the glue). The beam is resting on the same supports and is subjected to the same load F. Calculate the deflection caused by F, denoted by D¢. Compare with the value of D found in Part 1. (Take the shear modulus of the foam to be: Gc = 20 MPa.)

Solution: 1. We will use the classical formula that gives the deflection at the center of the beam on two supports: F D = ----------48EI

© 2003 by CRC Press LLC

3

with

bh I = -------12

TX846_Frame_C18a Page 344 Monday, November 18, 2002 12:40 PM

For duralumin (see Section 1.6): E = 75,000 MPa. One finds D = 16.7 mm 2. Denoting by W the elastic energy due to flexure, one has

Ú

W =

beam

2

1 M --- ----------- dx + 2 · EI Ò

Ú

beam

1

1 k --- ------------T 2 dx 2 · GSÒ

2

with : k 1 ------------ # --------------------------------------· GSÒ G c ( e c + 2e p ) ¥ b ∂W

Using Castigliano theorem, one has D¢ = -------∂F then: D¢ =

Ú

beam

M dM ----------- -------- dx + · EI Ò dF

Ú

beam

dT k ------------T ------ dx · GSÒ dF

0 £ x £ /2:

M = Fx/2; F M = --- ( – x ); 2

/2 £ x £ : 1 Ï D¢ = ----------- Ì · EI Ò Ó

Ú

/2

0

Fx x ------ ¥ --- dx + 2 2

k Ï º + ------------· GS Ò ÌÓ

Ú

/2

0

T = –F /2 T = F /2

¸ F ( – x) --- ( – x ) ----------------- dx º ˝ 2 /2 2 ˛

Ú

F dx – --- ¥ – ------ + 2 2

F dx ¸ --- ¥ ------ ˝ 2 ˛ /2 2

Ú

3

F k F D¢ = ------------------ + ------ -----------48 · EI Ò 4 · GSÒ Approximate calculation: ( ec + ep ) ec b - + E c ¥ ------· EI Ò # E p ¥ e p ¥ b ¥ --------------------12 2 2

3

then: · EI Ò = 7090 MKS + 7.8 MKS

negligible

1 2

with

E c = 60 MPa ( cf. 1.6 )

To establish this relation, see Chapter 15, Equation 15.17. See calculation of this coefficient in 18.2.1, and more precise calculation in 18.3.5.

© 2003 by CRC Press LLC

TX846_Frame_C18a Page 345 Monday, November 18, 2002 12:40 PM

one obtains for D¢: D¢ = 0.18 mm + 1.04 mm bending moment

shear

D¢ = 1.22 mm Comparing with the deflection D found in Part 1 above: D 14 ----- = -----D¢ 1

Remarks: The sandwich configuration has allowed us to divide the deflection by 14 without significant augmentation of the mass: with adhesive film thickness 3 0.2 mm and a specific mass of 40 kg/m for the foam, one obtains a total mass of the sandwich: m = 700 g (duralumin) + 50 g (foam) + 48 g (adhesive) This corresponds to an increase of 14% with respect to the case of the full beam in Question 1. The deflection due to the shear energy term is close to 6 times more important than that due to the bending moment only. In the case of the full beam in question 1, this term is negligible. In effect one has: k = 1.2 for a homogeneous beam of rectangular section, then: k ------- = 8.27 ¥ 10 –8 GS (with G = 29,000 MPa, Section 1.6). The contribution to the deflection D of the shear force is then: k

dT

- T ------ dx = 0.02 mm > 1. The displacement of configuration (c) is much larger than the others. This will create problems when operating the arm. 2. The deflections are identical for configurations (a) and (c) if Ex ˆ 1 1 2 --- = --- Ê --- + ----------3 8 Ë 3 2G xy¯ then: E -------x- = 4 G xy

© 2003 by CRC Press LLC

TX846_Frame_C18a Page 395 Monday, November 18, 2002 12:40 PM

3. In looking for the modulus Gxy to be as high as possible, one reads on Tables 5.4 and 5.5 (Section 5.4.2.) a ratio Ex /Gxy = 3.9 (4) for the composition:

4. The maximum value of the longitudinal modulus of elasticity observed on Table 5.4 is E¢x = 134,000 MPa This corresponds to a shear modulus (Table 5.5): G¢xy = 4,200 MPa The same deflection as the previous one for the configuration (c) can be obtained by 3 3 E¢x ˆ F 2 F -------------- Ê --- + ------------ = ----------8E¢x I¢ Ë 3 2G¢xy ¯ 3E x I

then: 3 E¢x ˆ 3E 2 I¢ p r e¢ --- = ------------ = 3.5 = ---------x- Ê --- + -----------3 Ë I 8E¢x 3 2G¢x y ¯ pr e e¢ ---- = 3.5 e

The tube with thickness e¢ and modulus Ex¢ will be more stiff for configuration (a) but will have a mass multiplied by 3.5 to keep the stiffness of configuration (c). 5. Configurations (a) and (c) are the more deformable. One then has to write 3E x I Ê F ˆ F ----- = ---------- ≥ --3 Ë D¯ min Dy with = 15 m; I = pr e; r = 0.15 m; (F/D)min = 10 N/m; Ex = 75,407 MPa 3

4

e ≥ 14 mm

© 2003 by CRC Press LLC

TX846_Frame_C18a Page 396 Monday, November 18, 2002 12:40 PM

The ply thickness being 0.13 mm, one obtains 108 layers oriented as follows:

6. The specific mass of the laminate is indicated in Section 3.3.3, as r = 1530 3 kg/m. The distributed mass of the arm is then: m ----- = 2 p re ¥ r = 20.2 kg/m with the angular acceleration indicated in Figure 18.8, one obtains the following inertial load:

We then deduce from there: The deflection at the end due to the concentrated mass: 3

100 D concent. = -------------3E x I 19

The deflection at the end due to distributed load : 4

11 0.81 D distributed = --------- ¥ ---------------Ex I 120 from which we can obtain a total deflection: 3

3

100 100 D total = -------------- ( 1 + 0.033 ) # -------------3E x I 3E x I The rigidity (F/Dtotal) appears to be well related essentially to the concentrated inertial load at the extremity of the arm. 19

---------- [ 2 – 3 ( X/ ) + ( X/ ) ] Result obtained from the differential equation: EI x d v/dX = – 0.81 6

© 2003 by CRC Press LLC

2

2

2

3

TX846_Frame_C18b Page 397 Monday, November 18, 2002 12:43 PM

18.2 LEVEL 2 18.2.1 Sandwich Beam: Simplified Calculation of the Shear Coefficient Problem Statement: Represented below is the cross section of a sandwich beam. The thickness of the skins is small compared with that of the core. Under the action of a shear load T, 20 the shear stresses in the section are assumed to vary in a piecewise-linear fashion along the y direction. The constitutive materials, denoted as 1 and 2, are assumed to be isotropic, or transversely isotropic. The shear moduli are denoted as G1 for material 1 (skin) and G2 for material 2 (core). The beam has a width of unity. 1. Calculate the shear coefficient k for flexure in the plane x,y.

2. Give a simplified expression for the case—current in the applications— where G1 >> G2 with the notations for the thicknesses: H1 – H2 e p = ------------------; 2

ec = H2

Solution: 1. Let W be the strain energy due to shear stresses. One has (Equation 15.17): 2

1 dW 1 kT --------- = --- ------------- = --2 dx 2 · GS Ò

Ú

section

t xy ------ dy Gi 2

In the upper skin, one has H 1 – 2y t xy = -----------------¥ to H1 – H2

20

This representation of the shear stresses is only approximate. One will find in Application 18.3.5 the results concerning a more precise distribution of these stresses. In fact, the approximate representation of the shear proposed here is better approximated than the skins of the sandwich structure will have a small thickness as compared to that of the core.

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 398 Monday, November 18, 2002 12:43 PM

On the other hand in the core: txy = t0 T =

Then with:

Ú

t xy ( dy ¥ 1 )

section

One deduces from there the maximum shear stress to: 2 t o = T ¥ ------------------H1 + H2 Strain energy: dW 1 t xy --------- = --- -----dy = dx 2 Gi

Ú

2

Ú

H 2 /2

o

t -----o- dy + G2 2

t ( H 1 – 2y ) -----o- ------------------------dy 2 G H 2 /2 1 ( H1 – H2 )

Ú

H 1 /2

2

2

After calculation: 1 --2

Ú

2 t xy t H H 1 – H 2ˆ H H 1 – H 2ˆ 2T ------ dy = ----o- Ê ------2 + -----------------= --------------------------2 Ê ------2 + -----------------Ë 3G 1 ¯ 3G 1 ¯ Gi 2 Ë G2 ( H1 + H2 ) G2 2

2

one then has 2 2 H H 1 – H 2ˆ 2T 1 kT --- ------------- = --------------------------2 Ê ------2 + -----------------Ë 3G 1 ¯ 2 · GS Ò ( H1 + H2 ) G2

Then: 4 · GS Ò H H 1 – H 2ˆ k = --------------------------2 Ê ------2 + -----------------3G 1 ¯ ( H1 + H2 ) Ë G2 with (Equation 15.16): GS = G1 (H1 – H2) + G2 H2: 4 [ G 1 ( H 1 – H 2 ) + G 2 H 2 ] Ê H 2 H 1 – H 2ˆ - ------ + -----------------k = --------------------------------------------------------2 Ë G2 3G 1 ¯ ( H1 + H2 ) 2. Case where G2 30 N/mm applied.

18.2.11 Determination of the Elastic Characteristics of a Carbon/Epoxy Unidirectional Layer from Tensile Test Problem Statement: Consider a unidirectional plate of carbon/epoxy, from which one cuts the two samples shown below. They are tested in a testing machine. One measures the strains using strain gages arranged as shown. The strains obtained under different loads are linearized. One shows their values corresponding to a uniform tensile stress sx equal to 20 MPa. Calculate the elastic constants of the unidirectional layer subject to in-plane loading.

Solution: One can use the Equation 11.5: Sample No. 1: The axes x and y are ,coincident with the axes and t (q = 0). From which:

s s 20 e 1x = -----x = -----x Æ E = ------------------- = 139,860 MPa Ex E 143 E-6 n n xy e 1y = – ------ ¥ s x = – -----t- ¥ s x Æ n t = 0.25 E Ex

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 436 Monday, November 18, 2002 12:43 PM

Sample No. 2: The axes x and y make an angle of q = 20∞ with the axes 40 l and t, from which : Ï c4 s4 s n ¸ 2 2 1 e 2x = -----x = Ì ----- + ---- + c s ÊË ------- – 2 -----t-ˆ¯ ˝ ¥ s x Ex E ˛ E E G t t Ó Ïn n xy 1 ¸ 1 1 - ¥ s x = – Ì -----t- ( c 4 + s 4 ) – c 2 s 2 Ê ----- + ---- – -------ˆ ˝ ¥ s x e 2y = – -----Ë ¯ Ex E E G E t t ˛ Ó leading to 1 0.1325 Ï ------- + ---------------- = 2.69 E-4 Et Ô G t Ì 1 1 Ô ------ – ---- = 1.144 E-4 Ó G t E t from which: Et = 7320 MPa; Gt = 3980 MPa In summary: E = 139 ,860 MPa E t = 7 320 MPa

n t = 0.25;

n t = 0.013

G t = 3980 MPa

18.2.12 Sailboat Shell in Glass/Polyester Consider a siding of a laminated shell for a sailboat made of glass/polyester. It is made up of a stack of layers of balanced fabric and glass mat. The reinforcements, in “E” glass, are in the following form: Balanced fabric: Vf = 20%, mass of the glass per square meter: mof = 500 g. Mat: Vf = 15%, mass of glass per square meter: mof = 300 g.

Problem Statement: 1. Calculate: (a) The thickness of one layer of fabric of glass/polyester. (b) The thickness of a layer of mat of glass/polyester. 2. Given the composition of the laminated siding as follows: [M/F/M/F]s (M ´ Mat; F ´ Fabric) 40

n Et

n E

One has -----t- = -----t- See Exercise 18.1.2

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 437 Monday, November 18, 2002 12:43 PM

Figure 18.9

Figure 18.10

what is the total thickness, denoted as h, of the laminated siding? 3. Elastic characteristics of a fabric layer: One considers a layer of balanced fabric to be equivalent to two series of unidirectional plies crossed at 90∞, each series possessing half of the total thickness of the fabric layer (see Figure 18.9). The elastic characteristics of these unidirectional plies are as follows: E = 18,000 MPa; Et = 4900 MPa; Gt = 1850 MPa; nt = 0.3. Calculate the elastic characteristics (moduli, Poisson coefficients) of a layer of fabric in axes C,T. 4. The layers of mat are considered as isotropic in their planes, with the elastic characteristics: EMat = 8350 MPa; n Mat = 0.3. Figure 18.10 represents one planar portion of the laminated siding. All the fabric plies are oriented at 0∞ – 90∞. Calculate the global elastic characteristics (moduli, Poisson coefficients) of the siding working in its plane. Remark: Tests done on samples made of this material indicate a modulus of elasticity along the x direction to be equal to 9200 MPa. What can be said about this? 5. Rupture: The rupture strengths, considered to be equal in tension and in compression, are as follows:

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 438 Monday, November 18, 2002 12:43 PM

Fabric layer: along C or T: srupture fabric = 139 MPa. Mat layer: srupture Mat = 113 MPa. (a) Calculate the maximum stress sox leading to first ply failure of the siding. What are the layers that fracture? (b) Apply the maximum stress sox. In the previous layers that fractured, the glass fibers are supposed all broken. What happens to the laminate?

Solution: 1. The thickness of a layer denoted as h is such that (see Section 3.2.4): m of h = ---------Vf rf The specific mass of “E” glass is (see Section 1.6): r = 2600 kg/m , from which: 3

hfabric = 0.96 mm; hMat = 0.77 mm. 2. The siding is constituted of the following stacking sequence:

The total thickness is h = 0.77 ¥ 4 + 0.96 ¥ 3 = 5.96 mm. 3. Elastic characteristics of a fabric layer: The moduli and Poisson coefficients can be evaluated starting from the simplified relations of Section 3.4.2. One obtains, with k = 0.5 (balanced fabric): EC = ET = 11,450 MPa GCT = 1850 MPa; nCT = nTC = 0.128 A more precise calculation of these characteristics requires to establish the matrix –1 h[A] of Section 12.1.2. (Equation (12.9)). We calculate at first --h1- [ A ] (Equation 12.8): 0∞ 90∞ 1 --- A ij = ( E ij ) ( 0.5 ) + ( E ij ) ( 0.5 ) h

The terms E ij are given by the Equation 11.8. One will have, for example: 1 1 E + Et --- A 11 = ( E ) ( 0.5 ) + ( E t ) ( 0.5 ) = --- --------------------h 2 1 – n t n t

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 439 Monday, November 18, 2002 12:43 PM

with E n t = n t -----t ; E One obtains 11,737 1507 0 1507 11,737 0 ( MPa ) 0 0 1850

1 --- [ A ] = h

1 ---------------11,540

h[A ]

-1

0.128 = – --------------11,540

0.128 – --------------11,540

0

1 ---------------11,540

0

0

1 -----------1 850

0 from which:

E C = E T = 11,540 MPa G CT = 1850 MPa

n CT = n TC = 0.128 (The difference between the values obtained above is small). 4. Elastic characteristics of the siding: These are deduced from the matrix -1 h[A] (Equation 12.9) calculated for all the laminate. We calculate at first

1 --- [ A ] (Equation h

12.8):

fabric Mat 1 --- A ij = ( E ij ) ( p fabric ) + ( E ij ) ( p Mat ) h

with p

fabric

3 ¥ 0.96 = ---------------------- = 0.483; 5.96 fabric

E 11

fabric

E 12

fabric

= E 22

p

Mat

EC = E C = ---------------2 1 – n CT

= n CT E C ;

E Mat Mat Mat -; E 11 = E 22 = ----------------2 1 – n Mat

fabric

E 33

= G CT

n Mat E Mat Mat E 12 = -----------------2 1 – n Mat

E Mat Mat E 33 = G Mat = -------------------------2 ( 1 + n Mat )

© 2003 by CRC Press LLC

= 0.517. (see Equation 11.8)

TX846_Frame_C18b Page 440 Monday, November 18, 2002 12:43 PM

We obtain 10,410 2149 0

1 --- [ A ] = h

2149 0 10,410 0 [ MPa ] 0 2554

1 -----------9966

h[A ]

–1

= – 0.206 ------------9966 0

------------– 0.206 9966

0

1 -----------9966

0

0

1 -----------2554

then: E x = E y = 9966 MPa G xy = 2554 MPa

n xy = n yx = 0.206 Remark: The real modulus (measured) 9200 MPa is a bit smaller than the one calculated. In effect, due to the curvature of fibers from weaving, a fabric layer is softer than the stacking of unidirectionals that are crossed at 90∞. However, the approximation obtained by calculation is suitable (difference < 10%). 5. Fracture of the siding: (a) One subjects the siding to a stress sox. The strains of this siding are given by the Equation 12.9 as: Ï e ox Ô Ì e oy Ô Ó g oxy

Ï s ¸ ox Ô –1 Ô ˝ = h[A ] Ì 0 Ô Ô Ó 0 ˛

¸ Ï s ox /9966 Ô Ô = ˝ Ì – 0.206 s ox / 9966 Ô Ô 0 ˛ Ó

¸ Ô ˝ Ô ˛

These strains give rise to the following stresses: In the layers of fabric (see results from Question 3): Ï sC Ô Ì sT Ô Ó t CT

¸ Ï 11,737 Ô Ô ˝ = Ì 1507 Ô Ô 0 ˛ Ó

1507 11,737 0

0 0 1850

¸Ï s ox /9966 ÔÔ ˝Ì – 0.206 s ox /9966 ÔÔ 0 ˛Ó

Ï 1.15 s ox Ô ◊◊◊ = Ì -0.09 s ox Ô 0 Ó

© 2003 by CRC Press LLC

¸ Ô ˝ Ô ˛

¸ Ô ˝◊◊◊ Ô ˛

TX846_Frame_C18b Page 441 Monday, November 18, 2002 12:43 PM

The Hill–Tsai criterion in these layers is satisfied for a stress sox such that: 1.15 s oxˆ Ê – 0.09 s oxˆ – 0.09 ¥ 1.15 s ox Ê -----------------+ ---------------------- – -------------------------------------- = 1 2 Ë 139 ¯ Ë 139 ¯ 139 2

2

2

as:

sox = 116 MPa Mat

In the layers of Mat, with the values of the coefficients E ij of Question 4, we have Ï sx ¸ Ï s ox /9 966 Ô Ô Mat Ô Ì s y ˝ = [ E ] Ì – 0.206 s ox /9 966 Ô Ô Ô 0 Ó t xy ˛ Ó

¸ Ï 0.86 s ox Ô Ô ˝ = Ì 0.087 s ox Ô Ô 0 ˛ Ó

¸ Ô ˝ Ô ˛

The Hill–Tsai criterion in the mat layers is satisfied for a stress sox such that : 41

0.86 s oxˆ Ê 0.087 s oxˆ 0.86 ¥ 0.087 s ox Ê -----------------+ --------------------- – ------------------------------------- = 1 2 Ë 113 ¯ Ë 113 ¯ 113 2

2

2

then:

s ox = 138 MPa The fabric layers are the first to fail, for a stress of

sox max = 116 MPa (b) This stress being applied, the rupture of the fabric layers translates into the rupture of the glass fibers. The stress resultant corresponding to this constraint as: Nx = sox max ¥ h = 116 ¥ 5.96 = 691 N/mm is then completely taken up by the layers of Mat. The stress in these layers is then: Nx 691 - = ------------------- = 224 MPa s ox Mat = ----------------4 ¥ h Mat 4 ¥ 0.77

41

A mat layer does not have transverse isotropy in the axes y, z (or x,z). The Hill-Tsai expression is then modified. We use however the Equation 14.6 here (see remark 39 at the bottom of page in Application 18.2.10).

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 442 Monday, November 18, 2002 12:43 PM

It exceeds the rupture strength of the Mat (113 MPa). Then this latter layer fractures. The siding is then completely broken under the stress:

sox max = 116 MPa

18.2.13 Determination of the In-Plane Shear Modulus of a Balanced Fabric Ply Problem Statement: Consider a sample cut from a laminated panel made of identical layers of balanced fabric, all oriented along the axes C (warp direction) and T (fill direction) in the following figure. The sample is in a state of simple tension in its plane along the x axis as shown in the figure.

sox π 0;

soy = toxy = 0

Two strain gages are bonded (see figure). These are denoted as 1 and 2:

From gage 1, one reads a strain eox. From gage 2, one reads a strain eoy. 1. Noting that goxy = 0, give the expression for the distortion gCT in the axes C and T as a function of eox and eoy. 2. Give the expression for the stress tCT in the axes C and T as a function of sox. 3. Deduce from the previous answer the shear modulus GCT as a function of eox, eoy, and sox.

Solution: 1. Equation 11.7 allows one to write Ï Ô eC Ô Ì eT Ô Ô g CT Ó

© 2003 by CRC Press LLC

¸ Ï Ô Ô c2 Ô Ô ˝ = Ì s2 Ô Ô Ô Ô 2cs ˛ Ó

s

2

c

2

– 2cs

¸Ï ÔÔ e ox ÔÔ ˝Ì e cs ÔÔ oy 2 2 ( c – s ) ÔÔ g oxy ˛Ó – cs

¸ Ô Ô ˝ Ô Ô ˛

TX846_Frame_C18b Page 443 Monday, November 18, 2002 12:43 PM

Here, we have a balanced laminate with midplane symmetry, loaded in its axes x,y. Then (Equation 12.9): goxy = 0, from which: 1 1 g CT = 2cs e ox – 2cs e oy with c = ------- ; s = – ------2 2 g CT = – e ox + e oy 2. According to Equation 11.4: Ï Ô sC Ô Ì sT Ô Ô t CT Ó

¸ Ï Ô Ô c2 Ô Ô ˝ = Ì s2 Ô Ô Ô Ô sc ˛ Ó

s

2

c

¸Ï ÔÔ s ox ÔÔ 2cs ˝Ì 0 ÔÔ 2 2 ( c – s ) ÔÔ 0 ˛Ó – 2cs

2

– sc

¸ Ô Ô ˝ Ô Ô ˛

then:

s ox t CT = sc s ox = – ------2 3. The constitutive behavior of the fabric in its axes can be written, starting from the Equation 11.5, as: Ï eC Ô Ô Ì eT Ô Ô Ó g CT

¸ Ô Ô ˝ = Ô Ô ˛

Ï Ô Ô Ô Ô Ì Ô Ô Ô Ô Ó

1 ----Ec

n CT – ------Ec

CT – -------

n Ec

1 ----Ec

0

0

¸ Ô Ô Ô Ô 0 ˝ Ô Ô 1 --------- Ô G CT Ô ˛

0

Ï sC Ô Ô = Ì sT Ô Ô Ó t CT

¸ Ô Ô ˝ Ô Ô ˛

t CT g CT = -------G CT From which:

s ox G CT = --------------------------2 ( e ox – e oy )

18.2.14 Quasi-Isotropic Laminate Problem Statement: Consider a laminate made up of a number of identical unidirectional plies, with midplane symmetry and the following composition:

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 444 Monday, November 18, 2002 12:43 PM

The elastic characteristics of a ply in its axes and t are denoted as: E, Et, Gt, nt, nt One examines the behavior of this laminate under in-plane loading, following the law (Equation 12.9): Ï e ox Ô Ì e oy Ô Ó g oxy

¸ Ï s ox Ô –1 Ô ˝ = h [ A ] Ì s oy Ô Ô ˛ Ó t oxy

¸ Ô ˝ Ô ˛

1. Calculate the coefficients of the matrix --h1- [ A ] . 2. By inversion, deduce from there the elastic moduli of the laminate. 3. What comment can one make? Deduce from there the law for the behavior of the laminate under in-plane loading in the axes (X,Y) derived from the (x, y) axes by a rotation angle q.

Solution: 1. Coefficients

1 --- A ij h

are given by the Equation 12.8 as: 1 1 --- A ij = --- E 0∞ + E 90∞ + E +45∞ + E –45∞ ij ij ij h 4 ij 0∞

The stiffness coefficients E ij are obtained from the behavior of a ply (Equation 11.8). In using this relation for q = 0∞, 90∞, +45∞, –45∞, one obtains 1 1 1 3 --- A 11 = --- A 22 = --- --- ( E + E t ) + n t E + 2G t h h 4 2 1 1 1 --- A 12 = --- --- ( E + E t ) + 3 n t E – 2G t 4 2 h 1 1 1 --- A 33 = --- --- ( E + E t ) – n t E + 2G t 4 2 h 1 1 --- A 13 = --- A 23 = 0 h h where one recalls that: E =

© 2003 by CRC Press LLC

E -----------------------; 1 – n t n t

Et =

Et ----------------------1 – n t n t

TX846_Frame_C18b Page 445 Monday, November 18, 2002 12:43 PM

The matrix

1 --- [ A ] reduces h

to A 11 1 --- A 21 h 0

A 12 A 11 0

0 0 A 33

2. From the above, the modulus of elasticity of the laminate in directions x and y, and the associated Poisson coefficient are 1 --- A 11 1 h -; --- = -----------------------------2 2 1 E -----2 ( A 11 – A 12 ) h

1 --- A 12 n h – --- = – -----------------------------2 2 1 E -----2 ( A 11 – A 12 ) h

One obtains after calculation: [ 2 ( E + E t ) + 4 n t E ] [ E + E t – 2 n t E + 4G t ] E = ------------------------------------------------------------------------------------------------------------------3 4 --2- ( E + E t ) + n t E + 2G t

n =

1 --- ( E + E t ) + 3 n t E – 2G t 2 ---------------------------------------------------------------3 --- ( E + E t ) + n t E + 2G t 2

The shear modulus is written as: 1 1 G = --- --- ( E + E t ) – n t E + 2G t 4 2 3. One can remark that: E G = -------------------2(1 + n ) This leads to an isotropic elastic behavior of the laminate in its plane. As a result, in all coordinate systems (X,Y) derived from (x,y) by any rotation angle, the constitutive behavior of the laminate is unchanged and is written as: Ï e Ô X Ô Ì eY Ô Ô g Ó XY

© 2003 by CRC Press LLC

¸ n 1 --- – --Ô E E Ô 1 --˝ = – --EnE Ô Ô 0 0 ˛

Ï s Ô X Ô 0 = Ì sY Ô 1 Ô t ---G Ó XY 0

¸ Ô Ô ˝ Ô Ô ˛

TX846_Frame_C18b Page 446 Monday, November 18, 2002 12:43 PM

Remark: This result generalizes to other groups of orientations for plies such as:

p 2p 0, --- , ------ ; 3 3

p 2p 3p 4p 0, --- , ------, ------, -----5 5 5 5

and so on. More generally, a laminate made up of n orientations (a whole number n > 2), having the values of --np- ( p – 1 ), with p = 1,…, n and with the same proportion of plies along each orientation as (1/n) is elastically isotropic. One shows also that 42 for all these laminates, E and n are invariable.

18.2.15 Orthotropic Plate in Pure Torsion Problem Statement: Consider a square plate (a ¥ a) of unidirectional glass/epoxy (Vf = 60%), thickness h, welded at the center of its lower face on a support. It is subjected to a uniform 43 and constant torsional moment density mo (N mm/mm) along its perimeter. The directions , t of the unidirectional form an angle q with the axes x,y of the plate (see figure).

1. Assuming that all stress resultants in the plate are zero (except the torsional moment), determine the bending displacement at all points of the midplane. 2. Determine the state of stresses in the axes (x, y) then in the axes (,t) of the unidirectional layer. 3. Numerical application: q = 45∞; a = 1 m; h = 5 mm; mo = –10 N mm/mm. 42

43

For more details, see Bibliography at the end of the book: “Stiffness isotropy and resistance quasi-isotropy of laminates with periodic orientations.” The practical importance of such a load is very limited. It is better to consider this example as a means to validate a computer program using finite elements. It is one of the “patches” issued from the work “Computer programs for composite structures: Examples of reference for validation” (see Bibliography at the end of the book).

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 447 Monday, November 18, 2002 12:43 PM

Solution: 1. In the constitutive Equation 12.16, one has C ij = E ij

3

h/2

h 2 z dz = E ij -----12 – h/2

Ú

then: 3

h [ C ] = ------ [ E ] 12 where [ E ] is the matrix shown in details in Equation 11.8. By inverting the Equation 12.16 and noting that: [C] where

1 --E

–1

12 –1 12 1 = -----3- [ E ] = -----3- --h h E

is the matrix shown in details in Equation 11.5, one has Ï Ô Ô Ô Ô Ô Ì Ô Ô Ô Ô Ô Ó

¸ 2 ∂ wo Ô Ô – -----------2 Ô ∂x Ô 2 ∂ w o Ô˝ – -----------2 Ô ∂y Ô Ô 2 ∂ wo Ô - Ô – 2 -----------∂x∂y ˛

Ï My 12 1 Ô = -----3- --- Ì – M x h E Ô Ó – M xy

¸ Ô ˝ Ô ˛

[1]

44

Assuming the unit stress resultants all to be zero except Mxy, Nx = Ny = Txy = Mx = My = 0;

one has

Mxy = mo

There remains (see Equation 11.5):

∂ wo 12 h xy ----------- = -----3- ------- mo ; 2 h G xy ∂x 2

∂ wo 12 m xy ----------- = -----3- ------- mo ; 2 h G xy ∂y 2

∂ w 12 1 2 ------------o- = -----3- -------- m o ∂x∂y h G xy 2

Therefore one can write wo(x, y) in the form: 12 m 2 2 w o = -----3- -------o- ( Ax + By + Cxy + Dx + Ey + F ) G xy h

44

With this hypothesis, equations of equilibrium, constitutive equation, and boundary conditions are verified.

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 448 Monday, November 18, 2002 12:43 PM

At the center of the plate: wo = 0;

∂ wo ---------∂x

=

∂ wo ---------∂y

= 0

from which: D = E = F = 0. And by identification with the second derivatives: 2A = hxy; 2B = mxy; 2C = 1 The out-of-plane displacement takes the form: 6m o - ( h xy x 2 + m xy y 2 + xy ) w o = ------------3 h G xy

[2]

2. State of stresses: The strain field in the axes of the plate is written as (Equation 12.12, taking into account [1]): Ï Ô ex Ô Ô Ì ey Ô Ô Ô g xy Ó

Ï

¸ Ô Ô Ô Ô Ô Ô Ô Ô ¥ = z Ì ˝ Ô Ô Ô Ô Ô Ô Ô Ô ˛ Ó

¸ 2 Ô ∂ wo Ô – -----------2 ∂ x ÔÔ Ô 2 ∂ wo ˝ – -----------Ô 2 ∂y Ô Ô 2 ∂ wo Ô – 2 ------------- Ô ∂x∂y ˛

Ï Ô 0 Ô 12 1 Ô = z ¥ -----3- --- Ì 0 h E Ô Ô Ô –mo Ó

¸ Ô Ô Ô ˝ Ô Ô Ô ˛

from which one can write the stresses in the axes (x, y) using Equation 11.8: Ï sx ¸ Ï ex Ô Ô Ô Ì sy ˝ = [ E ] Ì ey Ô Ô Ô Ó t xy ˛ Ó g xy

¸ Ï 0 Ô 1 Ô 12 ˝ = z ¥ -----3- [ E ] --E- Ì 0 h Ô Ô ˛ Ó –mo

¸ Ï 0 Ô 12 Ô ˝ = z ¥ -----3- Ì 0 h Ô Ô ˛ Ó –mo

¸ Ô ˝ Ô ˛

then:

s x = 0;

s y = 0;

12 t xy = – z ¥ -----3- m o h

Stresses in the axes of the unidirectional: These are obtained by using 45 the Equation 11.4, which is

s = – 2cs t xy s t = 2cs t xy t t = ( c – s ) t xy 2

45

2

24 = z ¥ c s ¥ -----3- m o h 24 = – z ¥ cs ¥ -----3- m o h 12 2 2 = – z ( c – s ) ¥ -----3- m o h

Note that here the angle q = ( · x ) since the Equation 11.4 is written with q = ( x · ) .

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 449 Monday, November 18, 2002 12:43 PM

3. Numerical application: One has (Section 3.3.3) for the glass/epoxy: E = 45,000 MPa; Gt = 4500 MPa;

Et = 12,000 MPa;

nt = 0.3 (nt = 0.08)

from which (Equation 11.5 with q = –45∞):

h xy m xy 0.1375 ------- = ------- = – ---------------G xy G xy 4500 and wo takes the form: 1 2 w o = – -------------- [ xy – 0.1375 ( x 2 + y ) ] 9 375 The deformed configuration is shown in the figure below:

The stresses (in MPa) are written as:

sx = sy = 0;

txy = 0.96 ¥ z (mm).

s = –st = 0.96 ¥ z (mm);

tt = 0

18.2.16 Plate Made by Resin Transfer Molding (R.T.M.) Problem Statement: First part: A roll of mat of carbon fibers has the following characteristics: Areal mass density: mof = 30 g/m 3 Specific mass: rf = 1,750 kg/m

© 2003 by CRC Press LLC

2

TX846_Frame_C18b Page 450 Monday, November 18, 2002 12:43 PM

One deposits 21 layers of this mat over a plate in a rectangular mold. The mold is then closed and sealed, as shown in the figure below:

R1 and R2 represent two valves. R2 is closed, R1 is open. The mold is vacuumed. R2 is open, R1 is open. Polyester resin is filled into the cavity of the mold. Then resin begins to flow out through valve R1. R1 and R2 are closed. The mold is then heated, and the resin polymerizes. After demolding, one obtains a plate of mat/polyester. 1. Calculate the fiber volume fraction Vf (%). 2. Calculate the modulus of elasticity along the longitudinal and transverse directions, denoted respectively as E and Et, of a unidirectional of carbon/ polyester, that would have the same amount of fiber volume fraction. The following is given Ef = 230,000 MPa;

Eft = 15,000 MPa (Section 3.3.1, Table 3.3)

Eresin = 4000 MPa (Section 1.6) 3. Starting from the relation in Section 3.5.1 giving the modulus of elasticity of mat (which is assumed to be isotropic in the plane of the plate), deduce from there the value of Emat. Assume that nmat = 0.3. Second part: One polymerizes on each face of the previous plate two plies of preimpregnated carbon/epoxy unidirectionals with Vf = 60%. (see characteristics given in Section 3.3.3). Each ply has a thickness of 0.13 mm. The four plies (two above, two below) are oriented in the same direction denoted as x (or 0∞). The midplane of the laminated plate coincides with axes x and y.

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 451 Monday, November 18, 2002 12:43 PM

1. Write numerically for the unidirectional and for the mat the constitutive relation in the x, y axes in the form: Ï sx ¸ Ï ex Ô Ô Ô Ì sy ˝ = [ E ] Ì ey Ô Ô Ô Ó t xy ˛ Ó g xy

¸ Ô ˝ Ô ˛

2. Calculate in the axes x, y the coefficients of the in-plane constitutive relation of the laminated plate (matrix [A], Section 12.1.1). Deduce from there the moduli of elasticity and the Poisson coefficients of the plate. 3. Calculate in the axes x, y the coefficients for the bending behavior of the laminated plate (matrix [C], Section 12.1.4). Deduce from there the apparent bending moduli along the directions x and y. 4. This laminated plate is submitted to a tensile stress resultant along the x direction denoted as Nx (N/mm). The tensile rupture strength of mat is 100 MPa. Calculate the value of the stress resultant Nx that leads to firstply failure of the laminate. In which component (unidirectional or mat) will this failure occur? This component is supposed to be completely broken (i.e., its mechanical characteristics are reduced to zero). What then is the state of stress in the other component? Make a conclusion.

Solution: First part: 1. Fiber volume fraction of carbon: vol. fibers V f = ---------------------------------total volume If s is the rectangular surface at the base of the mold, the volume of a layer of mat is m s -------ofrf from which, for 21 layers: 21 ¥ s ¥ m of § r f - = 12% V f = -------------------------------------3 s ¥ 3 ¥ 10 2. Moduli of elasticity (see Section 3.3.1): One has E = E f V f + E m V m = 31,120 MPa 1 - = 4386 MPa E t = E m ----------------------Em V m + -----V f E ft

© 2003 by CRC Press LLC

TX846_Frame_C18b Page 452 Monday, November 18, 2002 12:43 PM

3. One has (see Section 3.5.1) 3 5 E mat = --- E + --- E t = 14,410 MPa 8 8 Second part: 1. Constitutive behavior: Unidirectional: Ï e Ô x Ô Ì ey Ô Ô g Ó xy

¸ Ô Ô ˝ = Ô Ô ˛

Ê 1 Á -------------------Á 134,000 Á 0.25 Á – ------------------Á 134,000 Á Á 0 Ë

ˆÏ ˜Ô ˜ ˜Ô 0 ˜Ì ˜Ô 1 ˜˜ Ô -----------4200 ¯ Ó

0.25 – ------------------134,000

0

1 -----------7000

0

s x ¸Ô Ô sy ˝ Ô t xy Ô˛

After inversion: Ï sx ¸ 134,440 Ô Ô = Ì sy ˝ 1756 Ô Ô 0 Ó t xy ˛

1756 7023 0

0 0 4200

Ï ex Ô Ì ey Ô Ó g xy

¸ Ô ˝ Ô ˛

Mat: Ï e Ô x Ô Ì ey Ô Ô g Ó xy

1 ¸ ----------------14,410 Ô Ô 0.3 ˝ = – ---------------14,410 Ô Ô 0 ˛

0.3 – ---------------14,410

0

1 ----------------14,410

0

0

2 ( 1 + 0.3 ) --------------------------14,410

Ï s ¸ Ô x Ô Ô Ô Ì sy ˝ Ô Ô Ô t Ô Ó xy ˛

After inversion: Ï sx ¸ 15,835 Ô Ô = Ì sy ˝ 4750 Ô Ô 0 Ó t xy ˛

4750 15,835 0

0 0 5542

2. Membrane behavior of the laminated plate: n

A ij =

Â

ply n∞1

© 2003 by CRC Press LLC

(k) (k)

E ij e

Ï ex Ô Ì ey Ô Ó g xy

¸ Ô ˝ Ô ˛

TX846_Frame_C18b Page 453 Monday, November 18, 2002 12:43 PM

A11 = 134,440 ¥ 4 ¥ 0.13 + 15,835 ¥ 3 = 117,408 (MPa mm) A22 = 7023 ¥ 4 ¥ 0.13 + 15,835 ¥ 3 = 51,151 (MPa mm) A12 = 1756 ¥ 4 ¥ 0.13 + 4,750 ¥ 3 = 15,163 (MPa mm) A13 = A23 = 0 A33 = 4200 ¥ 4 ¥ 0.13 + 5542 ¥ 3 = 18,810 (MPa mm). From this, and with a total thickness of the plate of h = 3 + 4 ¥ 0.13 = 3.52 mm we have

[A] =

117,408 15,163 0 1 ----------------32,078

h[A ]

–1

0.3 = – ---------------32,078

15,163 51,151 0

0 ; 0 18,810

0.13 – ---------------13,975

0

1 ----------------13,975

0

0

1 -----------5344

0

then for the moduli of elasticity of the plate: E x = 31,078 MPa;

n xy = 0.3;

E y = 13,975 MPa;

G xy = 5344 MPa

n yx = 0.13

3. Bending behavior of the laminated plate: n

C ij =

Â

ply n∞1

© 2003 by CRC Press LLC

3

3

( k ) z k – z k-1ˆ E ij Ê ------------------Ë 3 ¯

TX846_Frame_C18b Page 454 Monday, November 18, 2002 12:43 PM

3

3

3

1.5 1.76 – 1.5 3 C 11 = 134,440 ¥ ---------------------------- ¥ 2 + 15,835 ¥ --------- ¥ 2 = 221,763 MPa ¥ mm 3 3 3

3

3

3

3

3

3

3

3

1.5 1.76 – 1.5 C 22 = 7023 ¥ ---------------------------- ¥ 2 + 15,835 ¥ --------- ¥ 2 = 3 3

45,352 MPa ¥ mm

1.5 1.76 – 1.5 C 12 = 1756 ¥ ---------------------------- ¥ 2 + 4 750 ¥ --------- ¥ 2 = 3 3 C 13 = C 23 = 0

3

13,119 MPa ¥ mm

1.5 1.76 – 1.5 C 33 = 4200 ¥ ---------------------------- ¥ 2 + 5 542 ¥ --------- ¥ 2 = 3 3

18,284 MPa ¥ mm

3

3

from which (see Section 12.1.6):

1 -------------------217,968

[C]

–1

1 = – ------------------753,509

1 – ------------------753,509

0

1 ----------------44,576

0

0

1 ----------------18,284

0

=

1 --------EI 11

1 --------EI 12

0

1 --------EI 21

1 --------EI 22

0

0

0

1 --------EI 33

Apparent bending modulus in the x direction: 1 1 --------- = -----------------3 Æ E fx = 59,972 MPa h EI 11 E fx ¥ ----12 The apparent bending modulus in the y direction: 1 1 --------- = -----------------3 Æ E fy = 12,264 MPa h EI 22 E fy ¥ ----12 4. Rupture: For a stress resultant Nx, the plate is deformed in its plane according to the relation: Ï ex Ô Ì ey Ô Ó g xy

Ï N ¸ ¸ x Ô Ô –1 Ô ˝ = [A] Ì 0 ˝ Ô Ô Ô Ó 0 ˛ ˛ -1

then with the values found for [A] :

ex = 8.856 ¥ 10

© 2003 by CRC Press LLC

-6

¥ Nx; ey = –2.66 ¥ 10

-6

¥ Nx; gxy = 0

TX846_Frame_C18b Page 455 Monday, November 18, 2002 12:43 PM

One then has for the stresses: In the unidirectional layer:

s = sx = 134,440 ex + 1756 ey = 1.183 Nx st = sy = 1756 ex + 7023 ey = –0.003 Nx tt = txy = 0. In the mat layer:

sx = 15,835 ex + 4750 ey = 0.128 Nx sy = 4750 ex + 15,835 ey = 5.5 ¥ 10

-5

¥ Nx

txy = 0 From which the failure criteria are (see Section 14.2.3) In the unidirectional layer: ( 1.183N x ) ( – 0.003N x ) 1.183 ¥ – 0.003N x -------------------------- + ----------------------------- – ------------------------------------------> a made of unidirectional glass/ resin (see figure). It is supported at two opposite sides and is loaded by a constant transverse pressure of qo.

1. Calculate the deflection due to bending at the midline of the plate located at x = a/2 (maximum deflection). 2. Indicate the numerical values of the contributions from the bending moment and from transverse shear using the following: Ex = 40,000 MPa; Gxz = 400 MPa; nxy = 0.3; nyx = 0.075; qo = –1 MPa; a = 150 mm; h = 15 mm. Comment.

Solution: 1. For the cylindrical bending considered, Equation 17.32 allows one to write dQ x ---------- = – q 0 ; dx

dM y ---------- = Q x ; dx

d qy M y = C 11 --------; dx

Elimination of Qx, My and qy leads to 4

q d wo -----------= ------o4 C 11 dx © 2003 by CRC Press LLC

hG xz Ê dw o - ---------- + q yˆ Q x = ----------¯ k x Ë dx

TX846_Frame_C18c Page 494 Monday, November 18, 2002 12:45 PM

then: 3 2 q x4 x x w o = ------o- Ê ------ + A ----- + B ----- + Cx + Dˆ ¯ C 11 Ë 24 6 2

The boundary conditions are written as: x = 0 ¸w = 0; ˝ 0 x=a ˛

2 kx dq d wo - q 0 – -----------M y = 0 fi --------y = ----------= 0 2 dx hG xz dx

After calculation of the constants A, B, C, D, one obtains for the deflection at x = a/2: ¸ 1 a h 2E 4 12 ( 1 – n xy n yx ) Ï 5 - Ì --------- + k x Ê ---ˆ -------x- ----------------------------------- ˝ w 0 Ê ---ˆ = q 0 a ---------------------------------3 Ë 2¯ Ë ¯ G ( – n n ) 384 96 1 a xz xy yx ˛ Ex h Ó The calculation of kx was done in Section 17.7.1 for this type of plate. One has (see Equation 17.34) kx = 6/5 = 1.2 from which: 2 ¸ Ex 1 a 4 12 ( 1 – n xy n yx ) Ï 5 Ê --h-ˆ -------------- ----------------------------------- ˝ + w 0 Ê ---ˆ = q 0 a ---------------------------------Ì 3 Ë a¯ G xz 80 ( 1 – n xy n yx ) Ë 2¯ Ex h Ó 384 ˛

The first term in the brackets represents the contribution from the bending moment, and the second term represents that due to transverse shear. 2. Numerical values: wo(a/2) = –0.5727 mm – 0.5625 mm (moment)

(transverse shear)

wo(a/2) = –1.13525 mm Note that 49.5% of this deflection is due to transverse shear. One can see from the above expression for wo(a/2) that the influence of transverse shear on the bending deflection increases with the value of the relative thickness h/a (here, © 2003 by CRC Press LLC

TX846_Frame_C18c Page 495 Monday, November 18, 2002 12:45 PM

h/a = 1/10 corresponds to a thick plate). One also notes the influence of the ratio 48 Ex /Gxz.

18.3.8 Bending of a Sandwich Plate Problem Statement: A rectangular sandwich plate (a ¥ b) is fixed on side b, and loaded along the opposite side by a constant distributed load fo (N/mm). The two other sides are free (see figure).

The plate consists of two identical orthotropic skins of material 1, and an orthotropic core made of material 2. The orthotropic axes are parallel to the axes x,y,z. 1. Calculate the deflection of the midplane at the extremity x = a of the x axis, assuming cylindrical bending about y axis for the plate. 2. Numerical application: Given fo = –10 N/mm a = b = 1000 mm H1 = 2H2 = 100 mm Material 1: (1) Ex = 40,000 MPa (1) Gxz = 4000 MPa Material 2: (2) Ex = 40 MPa (2) Gxz = 15 MPa For each of the materials nxy = 0.3 nyx = 0.075

48

This example of thick plate in bending constitutes a test case for the evaluation of computer programs using finite elements. For complementary information on this topic, see bibliography, “Computer programs for Composite Structures: Reference examples and Validation.”

© 2003 by CRC Press LLC

TX846_Frame_C18c Page 496 Monday, November 18, 2002 12:45 PM

(a) Calculate the deflection at the extremity x = a and show the contributions from the bending moment and from the transverse shear. (b) Calculate the transverse shear stress txz: On the midplane of the plate. At the interface between the core and the upper skin. At the midthickness of the upper skin.

Solution: 1. In the case of cylindrical bending, Equation 17.32 allows one to write dQ x ---------- = 0; dx

d qy M y = C 11 --------; dx

dM y ---------- = Q x ; dx

· hG xzÒ Ê dw 0 ---------- + q yˆ Q x = ----------------¯ k x Ë dx

Then Qx = fo, and elimination of Qx, My, and qy leads to 3

fo d wo ----------- = -----3 C 11 dx then: 2 fo Ê x3 x w o = – ------ ----- + A ----- + Bx + Cˆ ¯ 2 C 11 Ë 6

The boundary conditions are written as: fo dw – ----------o = 0 x = 0 : w 0 = 0 et q y = 0 fi k x ----------------· hG xzÒ dx 2 dq d wo - = 0 x = a : M y = 0 fi --------y = – ----------2 dx dx

After calculation of the constants A, B, C, one obtains the deflection at x = a: 3

fo a fo a - + k x ----------------w o ( a ) = ---------3C 11 · hG xzÒ with (see Equation 12.16): 3

3

3

➀ H 1 – H 2ˆ ➁H C 11 = E 11 Ê -----------------+ E 11 ------2 Ë 12 ¯ 12

and according to Equation 17.2: ➀

C 11 © 2003 by CRC Press LLC

➁

E x ( H1 – H2 ) + E x H2 = --------------------------------------------------12 ( 1 – n xy n yx ) 3

3

3

TX846_Frame_C18c Page 497 Monday, November 18, 2002 12:45 PM

According to Equation 17.10: ➀

➁

· hG xzÒ = G xz ( H 1 – H 2 ) + G xz H 2 from which one obtains 4 ( 1 – n xy n yx )f o a kx fo a w o ( a ) = --------------------------------------------------+ ----------------------------------------------------➀ 3 3 ➁ 3 ➀ ➁ E x ( H 1 – H 2 ) + E x H 2 G xz ( H 1 – H 2 ) + G xz H 2 3

The calculation of kx was carried out in Section 17.7.2 for this type of plate. It was given by Equation 17.39. 2. Numerical application: (a) Deflection: Equation 17.39 gives kx = 110.8 from which: wo(a) = –1.177 mm + (–5.519 mm) (moment)

(transverse shear)

wo(a) = –6.636 mm Note that 83% of this deflection is due to transverse shear, and this happens in spite of very thick skins. This important influence is due to the very large value compared with unity (110.8) of the transverse shear coefficient and due to the fact that the plate is thick (H1/a = 1/10). (b) Transverse shear stress txz (see Section 17.7.2): Midplane: (z = 0): txz = 0.1286 MPa Interface (z = H2 /2): txz = 0.12855 MPa Midthickness of the upper layer: z = (H1 + H2)/4: txz = 0.075 MPa

18.3.9 Bending Vibration of a Sandwich Beam

49

Problem Statement: Consider a sandwich beam of length and width d simply supported at its ends (see figure). It consists of two identical skins of material 1 (glass/resin) and a core 49

This application constitutes a test case for the validation of computer programs using finite elements, see in the bibiography, “Programs for the calculation of Composite Structures, Reference examples and Validation.”

© 2003 by CRC Press LLC

TX846_Frame_C18c Page 498 Monday, November 18, 2002 12:45 PM

of material 2 (foam). These materials are transversely isotropic in the plane y, z.

The elastic characteristics are denoted as: ➀

➀

➁

➁

E x , G xy , E x , G xy Specific masses are r1 and r2. 1. Write the equation for the resonant frequencies for bending vibration in the plane of symmetry (x, y) of this beam. 2. Numerical application: Given: ➀

Ex

= 40,000 MPa; ➁

Ex

= 40 MPa;

r1 = 2,000 kg/m

➀

G xy = 4,000 MPa; ➁

G xy = 15 MPa;

H1 = 2H2 = 100 mm;

3

r2 = 50 kg/m

= 1000 mm;

3

d = 100 mm

Calculate the first five frequencies in bending vibration.

Solution: 1. Equation for the vibration frequencies: At first one establishes the differential equation for the dynamic displacement n (x, t) starting from the Equation 15.18, noting that for the example considered, the elastic center and the center of gravity of section are the same (decoupling between bending vibration and longitudinal vibrations). 2 ∂ Ty ∂ qz ∂ n ∂M --------- = · r S Ò --------2- ; ---------z + T y = · r I zÒ ---------2 ∂x ∂ x ∂t ∂t 2

· GS Ò ∂ n T y = ------------- Ê ------- – q zˆ ; ¯ k Ë∂ x

∂q M z = · EI zÒ --------z ∂x

Elimination of Ty, Mz, qz between these four relations leads to the equation for n (x, t): 4 4 2 · r I zÒ · r S Ò ∂ 4 n ∂ n · r I zÒ ∂ n · r SÒ ∂ n --------4- – ------------- ( 1 + a ) --------------------------------------------------------- --------- = 0 + + k 2 2 · GSÒ · EI zÒ ∂ t 4 · EI zÒ · EI zÒ ∂ t 2 ∂x ∂x ∂ t

© 2003 by CRC Press LLC

TX846_Frame_C18c Page 499 Monday, November 18, 2002 12:45 PM

with · r SÒ · EI zÒ -¥k a = ------------------------· GSÒ · r I zÒ In assuming that the solution takes the form n (x, t) = no(x) ¥ cos(wt + j) one can rewrite the differential equation that defines the modal deformation vo(x) in the following nondimensional form: 4

2

d no d no 1 ---------- + w 2 ( 1 + a ) ---------- + w 2 Ê a w 2 – -----2ˆ n o = 0 4 2 Ë ¯ dx dx r in which

n · r I zÒ 2 2 · r I zÒ 2 x 2 - w ; r = ----------------2 x = --- ; n o = -----o ; w = ----------- · EI zÒ · r SÒ After writing the characteristic equation, the reduced modal deformation takes the form: v o = AchX 1 x + BshX 1 x + C cos X 2 x + D sin X 2 x

[1]

where: 2

X1

2

X2

2 w (1 + a) 1 2 2 1 – a = + ------------------------ + w w ÊË ------------ˆ¯ + -----2 2 2 r 2

[2]

The boundary conditions corresponding to simply supported ends are written as: x = 0 or : n = 0; or:

∂q M z = · EI zÒ --------z = 0 "t ∂x d n ----------2-o + a w 2 n o = 0 dx 2

x = 0 or 1 : n o = 0;

These four conditions allow one to obtain with [1] a linear and homogeneous system in A,B,C,D. By setting the determinant equal to zero, one obtains an equation for vibrations which reduces to sin X2 = 0 Then the solution can be written as: X2 = np, (n = 1, 2, 3,…) © 2003 by CRC Press LLC

[3]

TX846_Frame_C18c Page 500 Monday, November 18, 2002 12:45 PM

2. With the numerical values indicated in the Problem Statement, one can calculate the shear coefficient k, the literal expression for which has been established in Application 18.3.5. One finds k = 110.8. The frequencies can be written starting from the circular frequencies w1, w2, w3,… extracted from equation [3], where X2 takes the form [2].

w f i = ------i ( H z ) 2p one obtains:

50

f 1 = 64.476 Hz ; f 4 = 265.383 Hz ;

50

f 2 = 131.918 Hz ;

f 3 = 198.734 Hz

f 5 = 331.963 Hz.

One keeps voluntarily the nonsignificant decimal, for the purpose of comparison with values obtained from numerical models.

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 503 Thursday, July 11, 2002 5:42 PM

APPENDIX 1 STRESSES IN THE PLIES OF A LAMINATE OF CARBON/EPOXY LOADED IN ITS PLANE The tables in this appendix give for each ply in the laminate the stresses along the principal orthotropic directions of the ply, denoted as and t. These stresses are denoted as σ , σ t, τ t. The laminate is successively subjected to three cases of simple loading:

σ x = 1 MPa: normal stress along the 0° direction. σ y = 1 MPa: normal stress along the 90° direction. τ xy = 1 MPa: shear stress.

CHARACTERISTICS OF EACH PLY Vf = 60% fiber volume fraction. Thickness of each ply: 0.13 mm. Moduli: Modulus along the fiber direction: E = 134,000 MPa. Modulus along the transverse direction: Et = 7000 MPa. Shear modulus: Gt = 4200 MPa. Poisson coefficient: νt = 0.25. Fracture strength: Tension along the longitudinal direction: σ rupture = 1270 MPa. Compression along the longitudinal direction: σ rupture = 1130 MPa. Tension along the transverse direction: σ t rupture = 42 MPa. Compression along the transverse direction: σ t rupture = 141 MPa. Shear strength: τ t rupture = 63 MPa.

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 504 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 505 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 506 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 507 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 508 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 509 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 510 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 511 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 512 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 513 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 514 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 515 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 517 Thursday, July 11, 2002 5:42 PM

APPENDIX 2 BUCKLING OF ORTHOTROPIC STRUCTURES The problems related to the stability of orthotropic plates and shells are not treated in this book. However, we give in the following a few figures that allow one to estimate the order of magnitude of loads that can lead to buckling due to compression or due to shear in orthotropic panels and tubes.

Rectangular Panels 1

The following plates allow one to calculate the critical stress resultants in compression and in shear for different support conditions.

1

See Sections 5.2.4 or 12.1.1. for the definition of the stress resultants. See relations [12.16] for the definition of the constants C11, C22, C12, C33 that appear in the plates.

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 518 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 519 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 520 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 521 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 522 Thursday, July 11, 2002 5:42 PM

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 523 Thursday, July 11, 2002 5:42 PM

Buckling of Orthotropic Tubes Buckling in bending creating ovalization of the tube: Bending leads to ovalisation of the cross section. The moment of inertia which affects the rigidity in bending decreases (this is the unstable process). The phenomenon is known as the “Brazier effect.”

2 2 2 Ex × Ey M critical = ---------- π r 0 e ---------------------1 – v xy v yx 9 bending © 2003 by CRC Press LLC

1/2

TX846_Frame_Appendix Page 524 Thursday, July 11, 2002 5:42 PM

Buckling due to external pressure: The notations in the above figure are kept. L is the length of the tube or the container that is subject to buckling. p critical

Ey E 1/4 r e 5/2 - × -----x × ----0 × ---- = 0.83 × ----------------------------1 – 0.1E x /E y E y L r 0

Buckling due to torsion:

The critical stress resultant in torsion is given by:

π e T xy = ----- -------3 2 12 critical r0 L 2

9

1/4

3

5

Ex Ey -5 × -----------------------------( 1 – ν xy ν yx )

1/8

Buckling due to axial compression: This aspect is not considered here, because the occurrence of elastic instability is strongly influenced by the presence of geometric imperfections in the orthotropic cylinder

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 525 Thursday, July 11, 2002 5:42 PM

BIBLIOGRAPHY Les matériaux composites, J. Weiss, C. Bord, Vol. 1 and 2, Publications of the Ministry of Industry and Research of Centre d’Études Techniques des Industries Mécanique. Les matériaux composites. G. Hellard, P. Lafon, Conference, Dec. 1984. Manufacturer’s documentation. Vetrotex—Saint Gobain, skis Dynastar, Ciba Geigy. Calcul des structures en matériaux composites. J.J. Barrau, S. Laroze, Eyrolles-Masson, Paris 1987. Calcul des structures en matériaux composites, F. Joubert, R. Harry, Mechanical Engineering Laboratory—I.U.T. « A »/C.O.D.E.M.A.C., Bordeaux 1985. Matériaux composites pour structures d’aeronefs, J. Rouchon, École Nationale Supérieure d’Ingénieurs de construction Aéronautiques, Toulouse, 1980. Les applications des composites dans le domaine aéronautique, G. Hellard, G. Hilaire, M. Tores, Aerospatiale publication. Fabrication des avions et missiles, M.P. Guibert, Dunod, Paris, 1960. Techniques de l’Ingénieur—Plastiques—A.3250—K. Gamski. Fibres de verre, d’aramide et de carbone, des renforts sur mesure pour composites, R. Kleinholz, G. Molinier, Vetrotex journal, No. 59, 1986. Résistance des constructions—matériaux composites—G. Hellard, École Nationale Supérieure d’Ingénieurs de Construction Aéronautiques, Toulouse, 1983. Initiation aux matériaux composites et à leurs techniques de fabrication— Avions Marcel Dassault—Bréguet Aviation—Edition No. 1, Toulouse. Manuel de techniques de collage, G. Fauner, W. Hendlich, eds. Soproge S.A., Paris, 1984. Recherches sur la théorie des assemblages collés, O. Volkersen—La Construction Métallique, No. 4, 1965. L’Aéronautique et L’Astronautique, No. 107, 4, 1984. Matériaux et structures composites ou l’adaptation aux besoins, P. Lamicq, 7th French Congress in Mechanics, Bordeaux, 1985. Publication of specialized press : Air et Cosmos; Aviation magazine; “ça m’intéresse;” Science et vie; Dassault-Bréguet Information; Aérospatiale Information; Vétrotex actualités; Aspects des résines Ciba Geigy; Interavia Revue Aérospatiale. Introduction aux matériaux composites, R. Naslain, Vol. 2, Matrices métalliques et céramiques, Ed. of C.N.R.S. and of Institute of Composite Materials.

© 2003 by CRC Press LLC

TX846_Frame_Appendix Page 526 Thursday, July 11, 2002 5:42 PM

Matériaux composites à matrice organique, G. Chrétien, Technique et documentation Lavoisier, Paris, 1986. Guide pratique des matériaux composites, M. Geier, D. Duedal, Technique et documentation Lavoisier, Paris 1985. La flexion—torsion dynamique des poutres composites, M. Carrier, J.M. Cieaux, Université Toulouse III—I.U.T. “A,” 1987. Proceedings of the 4th Journées Nationales sur les composites, Ed., Pluralis, Paris, 1984. Proceedings of the 5th Journées Nationales sur les composites, C. Bathias, D. Menkes, A.M.A.C., Ed. Pluralis, Paris, 1986. Transverse shear deformation in bending of composite beams of any cross section shapes, D. Gay, Mechanics of structured media, Part B : pp. 155– 171, Elsevier Scientific Publishing Company, 1981. Homogèneisation en torsion d’une poutre composite, J.J. Barrau, O. Chambard, M. Nuc, D. Gay-Tendances actuelles en calcul des structures, Bastia 1985. Les système ressorts-composites, L. De Goncourt, K.H. Sayers, Composites, No. 3, May/June 1988, pp. 145–150. Composites de grande diffusion, A. Jardon, M. Costes, European conference on Composite Materials, London, July 1987. Conception des véhicles spatiaux, D. Marty, Masson Ed., Paris, 1986. Effets des microfissures de résine sur les propriétés des composites aéronautiques en kevlar/époxyde-F. Turris, H.Y. Loken, R.F. Pinzelli, Composites No. 2, March/April 1988, pp. 35–40. Conduits PVDF renforcés. Contraintes thermiques et mécanismes de rupture, B. Échalier, P. Bleut, F. Lefebvre, C. Tournut, Composites, No. 3, May/ June 1987, pp. 183–188. Structure coques—Équations générales et stabilité, J. Barbe, E.N.S.A.E., 1983. Comment utiliser au meilleur coût les matériaux composites. M. Reyne, Ed. de l’Usine Nouvelle, Paris, 1986. Fibres de carbone revêtues de nickel, E.D. Kaufman, Composites No. 3, May/June 1988. FRANCE—COMPOSITES. French suppliers for the fabrication of organic composites, CEPP, 25 Rue Dagorno, 75012 Paris. Matériaux composites—Teknea, Marseille, 1989. Manuel de calcul des composites verre/résine, Manera, Massot, Morel, Verchery, Pluralis, 1988. Phénomènes interfaciaux dans les composites à matrice thermoplastique: Application au FIT, M. Guigon, A. Kloster, Annales des composites 1989, 1–2, pp. 83–90. Développement d’une nouvelle technologie pour fabriquer des poteaux, E. Pfletschinger-Composites No. 3, May/June 1987, pp. 67–72. Conception et dimensionnement du volet extérieur en fibres de carbone du CN 235, J.L. Duquesne, M. Gonzales, ENSICA, June 1990. Les plastiques, M. Reyne, Ed. Hermès, Paris, 1990. Impact and Residual Fatigue Behavior of ARALL, W.S. Johnson, Advances in Composites Materials and Structures, ASME-AMD, Vol. 82, 1989. © 2003 by CRC Press LLC

TX846_Frame_Appendix Page 527 Thursday, July 11, 2002 5:42 PM

Elastic Analysis and Engineering Design formulae for bonded joints—D.A. Bigwood, A.D. Grocombe, International Journal of Adhesion and Adhesive, Vol. 9, No. 4, Oct. 1989, pp. 229–242. Conception et essais de tubes composites hautes performances, P. Odru, C. Sparks, J. Schmitt, J.F. Puch, Matériaux-Mécanique-Électricité, No. 433, Feb/Mar 1990, pp. 4–6. Metal laminates—A family of Advanced Materials, M.L. Verbruggen, J.W. Gunnik, Plastics/Metals/Ceramics, SAMPE European chapter, Bâle, May 1990, pp. 455–465. General buckling curves for specially orthotropic rectangular plates, E.J. Brunnelle, G.A. Oyibo, AIAA Journal, Vol. 21, No. 8, Aug. 1983, pp. 1150– 1154. Technologie des composites, M. Reyne, Ed. Hermès, Paris, 1990. Interaction effects in fibre composites, V.R. Riley, Polymer Conference Series, University of Utah, June 1970. Progiciels de calcul de structures composites; Exemples de réference et de validation, Coordonnateur G. Matheron, ed. Hermès, Paris, 1995. Isotropie de Rigidité et quasi-isotropie de résistance des stratifiés à orientation périodiques, D. Gay, F. Joubert, Revue des composites et des matériaux avancés, Vol. 4, No. 2, 1994, pp. 241–261. Les composites, M. Reyne, Presses Universitaires de France, Paris, 1995.

© 2003 by CRC Press LLC

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close